The 3rd edition of this successful textbook contains ample material for a comprehensive upperlevel undergraduate or beg
1,647 113 45MB
English Pages 989 [998] Year 2015
Graduate Texts in Physics
Marius Grundmann
The Physics of Semiconductors An Introduction Including Nanophysics and Applications Third Edition
Graduate Texts in Physics Series editors Kurt H. Becker, Brooklyn, USA Sadri Hassani, Normal, USA Bill Munro, Kanagawa, Japan Richard Needs, Cambridge, UK William T. Rhodes, Boca Raton, USA Susan Scott, Acton, Australia H. Eugene Stanley, Boston, USA Martin Stutzmann, Garching, Germany Andreas Wipf, Jena, Germany
Graduate Texts in Physics Graduate Texts in Physics publishes core learning/teaching material for graduateand advancedlevel undergraduate courses on topics of current and emerging ﬁelds within physics, both pure and applied. These textbooks serve students at the MS or PhDlevel and their instructors as comprehensive sources of principles, deﬁnitions, derivations, experiments and applications (as relevant) for their mastery and teaching, respectively. International in scope and relevance, the textbooks correspond to course syllabi sufﬁciently to serve as required reading. Their didactic style, comprehensiveness and coverage of fundamental material also make them suitable as introductions or references for scientists entering, or requiring timely knowledge of, a research ﬁeld.
More information about this series at http://www.springer.com/series/8431
Marius Grundmann
The Physics of Semiconductors An Introduction Including Nanophysics and Applications Third Edition
123
Marius Grundmann Institut für Experimentelle Physik II Universität Leipzig Leipzig Germany
ISSN 18684513 Graduate Texts in Physics ISBN 9783319238791 DOI 10.1007/9783319238807
ISSN 18684521
(electronic)
ISBN 9783319238807
(eBook)
Library of Congress Control Number: 2015954622 Springer Cham Heidelberg New York Dordrecht London © Springer International Publishing Switzerland 2006, 2010, 2016 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, express or implied, with respect to the material contained herein or for any errors or omissions that may have been made. Printed on acidfree paper Springer International Publishing AG Switzerland is part of Springer Science+Business Media (www.springer.com)
To Michelle, Sophia Charlotte and Isabella Rose
Preface
Semiconductor electronics is commonplace in every household. Semiconductor devices have enabled economically reasonable ﬁberbased optical communication, optical storage, and highfrequency ampliﬁcation and have recently revolutionized photography, display technology, and lighting. By now solar energy harvesting with photovoltaics contributes a signiﬁcant portion to the energy mix. Along with these tremendous technological developments, semiconductors have changed the way we work, communicate, entertain, and think. The technological progress of semiconductor materials and devices is evolving continuously with a large worldwide effort in human and monetary capital. For students, semiconductors offer a rich and exciting ﬁeld with a great tradition, offering diverse fundamental and applied topics [1] and a bright future. This book introduces students to semiconductor physics and semiconductor devices. It brings them to the point where they can specialize and enter supervised laboratory research. It is based on the twosemester semiconductor physics course taught at Universität Leipzig in its Master of Science physics curriculum. Since the book can be followed with little or no preexisting knowledge in solidstate physics and quantum mechanics, it is also suitable for undergraduate students. For the interested reader several additional topics are included in the book that can be covered in subsequent, more specialized courses. The material is selected to provide a balance between aspects of solidstate and semiconductor physics, the concepts of various semiconductor devices and modern applications in electronics and photonics. The ﬁrst semester contains the fundamentals of semiconductor physics (Part I, Chaps. 1–10) and selected topics from Part II (Chaps. 11–20). Besides important aspects of solidstate physics such as crystal structure, lattice vibrations, and band structure, semiconductor speciﬁcs such as technologically relevant materials and their properties, doping and electronic defects, recombination, surfaces, and heteroand nanostructures are discussed. Semiconductors with electric polarization and magnetization are introduced. The emphasis is put on inorganic semiconductors, but a brief introduction to organic semiconductors is given in Chap. 17. Dielectric structures (Chap. 19) serve as mirrors, cavities, and microcavities and are a vital
vii
viii
Preface
part of many semiconductor devices. Other chapters give introduction to carbonbased nanostructures and transparent conductive oxides (TCOs). The third part (Part III, Chaps. 21–24) is dedicated to semiconductor applications and devices that are taught in the second semester of the course. After a general and detailed discussion of various diode types, their applications in electrical circuits, photodetectors, solar cells, lightemitting diodes, and lasers are treated. Finally, bipolar and ﬁeldeffect transistors including thinﬁlm transistors are discussed. In the present text of the third edition, a few errors and misprints of the second edition have been corrected. Several topics have been extended and are treated in more depth, e.g., double donors and double acceptors, negativeU centers, Boltzmann transport equation, ionic conductivity, hopping conductivity, impact ionization, thermopower, polarons, intraband transitions, amorphous semiconductors, disorder effects, heteroepitaxy on mismatched, curved and patterned substrates, and noise. A chapter on semiconductor surfaces has been added. The list of references has been augmented by almost 400 quotations with respect to the list in the second edition. All references now include title and complete page numbers. The references have been selected to (i) cover important historical and milestone papers, (ii) direct to reviews and topical books for further reading and (iii) give access to current literature and uptodate research. In Fig. 1, the original papers within the more than 1800 references in this book are shown by year. Roughly three phases of semiconductor physics and technology can be seen. Before the realization of the ﬁrst transistor in 1947, only a few publications are noteworthy. Then an intense phase of understanding the physics of semiconductors and developing semiconductor technology and devices based on bulk semiconductors (mostly Ge, Si, GaAs) followed. At the end of the 1970s, a new era began with the advent of quantum wells and heterostructures, and later nanostructures (nanotubes, nanowires, and quantum dots) and new materials (e.g., organic semiconductors, nitrides or graphene). Also several very recent references to emerging topics such as 2D materials, topological insulators or novel amorphous semiconductors are given.
100
References
hetero nano organic bulk
10
pretransistor
1 1880
1900
1920
1940
1960
Year
Fig. 1 Histogram of references in this book
1980
2000
2020
Preface
ix
I would like to thank many colleagues for their various contributions to this book, in alphabetical order (if no afﬁliation is given, at the time at Universität Leipzig): Gabriele Benndorf, Klaus Bente, Rolf Böttcher, Matthias Brandt, Christian Czekalla, Christof Peter Dietrich, Pablo Esquinazi, Heiko Frenzel, Volker Gottschalch, Helena Franke (née Hilmer), Axel Hoffmann (TU Berlin), Alois Krosty (OttovonGuericke Universität Magdeburg), Michael Lorenz, Stefan Müller, Thomas Nobis, Rainer Pickenhain, HansJoachim Queisser (MaxPlanckInstitut für Festkörperforschung, Stuttgart), Bernd Rauschenbach (LeibnizInstitut für Oberflächenmodiﬁzierung, Leipzig), Bernd Rheinländer, Heidemarie Schmidt, Mathias Schmidt, Rüdiger SchmidtGrund, Matthias Schubert, Jan Sellmann, Oliver Stier (TU Berlin), Chris Sturm, Florian Tendille (CNRSCRHEA), Gerald Wagner, Eicke Weber (UC Berkeley), Holger von Wenckstern, Michael Ziese, and Gregor Zimmermann. This book has beneﬁtted from their comments, proof reading, experimental data, and graphic material. Also, numerous helpful comments from my students on my lectures and previous editions of this book are gratefully acknowledged. I am also indebted to many other colleagues, in particular to (in alphabetical order) Gerhard Abstreiter, Zhores Alferov, Martin Allen, Levon Asryan, Günther Bauer, Manfred Bayer, Friedhelm Bechstedt, Dieter Bimberg, Otto Breitenstein, Len Brillson, Fernando Briones, Immanuel Brosery , JeanMichel Chauveau, Jürgen Christen, Philippe De Mierry, Steve Durbin, Laurence Eaves, Klaus Ellmer, Guy Feuillet, Elvira Fortunato, Ulrich Göseley , Alfred Forchel, Manus Hayne, Frank Heinrichsdorff, Fritz Hennebergery , Detlev Heitmann, Robert Heitzy , Evamarie HeyHawkins, Detlef Hommel, Evgeni Kaidashev, Eli Kapon, Nils Kirstaedter, Claus Klingshirn, Fred Kochy , Jörg Kotthaus, Nikolai Ledentsov, Peter Littlewood, Dave Look, Axel Lorke, Anupam Madhukar, Ingrid Mertig, Bruno Meyery , David Mowbray, Hisao Nakashima, Jörg Neugebauer, Michael Oestreich, Louis Piper, MatsErik Pistol, Fred Pollaky , Volker Riede, Bernd Rosenow, Hiroyuki Sakaki, Lars Samuelson, Darrell Schlom, Vitali Shchukin, Maurice Skolnick, Robert Suris, Volker Türck, Konrad Ungery , Victor Ustinov, Leonid Vorob’jev, Richard Warburton, Alexander Weber, Peter Werner, Wolf Widdra, Ulrike Woggon, Roland Zimmermann, Arthur Zrenner, Alex Zunger, and Jesús ZúñigaPérez, with whom I have worked closely, had enjoyable discussions with and who have posed questions that stimulated me. It is my distinct privilege and joy that this list becomes longer as I pursue studies in semiconductor physics but sadly the number of ysymbols increases too rapidly from edition to edition. Leipzig
Marius Grundmann
Contents
1
Introduction . . . . . . . . . . . . . . . . . . . . . 1.1 Timetable and Key Achievements . 1.2 Nobel Prize Winners . . . . . . . . . . 1.3 General Information . . . . . . . . . .
Part I
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
1 2 12 21
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
Fundamentals
2
Bonds. . . . . . . . . . . . . . . . . . . . . . . . 2.1 Introduction . . . . . . . . . . . . . . 2.2 Covalent Bonds . . . . . . . . . . . 2.2.1 ElectronPair Bond . . 2.2.2 sp3 Bonds. . . . . . . . . 2.2.3 sp2 Bonds. . . . . . . . . 2.3 Ionic Bonds . . . . . . . . . . . . . . 2.4 Mixed Bonds . . . . . . . . . . . . . 2.5 Metallic Bonding . . . . . . . . . . 2.6 vanderWaals Bonds. . . . . . . . 2.7 Hamilton Operator of the Solid .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
25 25 25 26 26 29 32 33 36 37 38
3
Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Introduction . . . . . . . . . . . . . . . . . . . . . 3.2 Crystal Structure . . . . . . . . . . . . . . . . . . 3.3 Lattice . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.1 Unit Cell . . . . . . . . . . . . . . . . 3.3.2 Point Group . . . . . . . . . . . . . . 3.3.3 Space Group . . . . . . . . . . . . . . 3.3.4 2D Bravais Lattices . . . . . . . . . 3.3.5 3D Bravais Lattices . . . . . . . . . 3.3.6 Polycrystalline Semiconductors . 3.3.7 Amorphous Semiconductors . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
41 41 42 43 43 43 45 46 46 51 51
xi
xii
Contents
3.4
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
53 53 53 54 55 56 57 59 61 61 61 62 63 64 66 66 67 70 72 72 74 77 77 77
Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Point Defects . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.1 Point Defect Types . . . . . . . . . . . . . . . 4.2.2 Thermodynamics . . . . . . . . . . . . . . . . . 4.2.3 Diffusion . . . . . . . . . . . . . . . . . . . . . . 4.2.4 Dopant Distribution . . . . . . . . . . . . . . . 4.2.5 Large Concentration Effects . . . . . . . . . 4.3 Dislocations . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.1 Dislocation Types . . . . . . . . . . . . . . . . 4.3.2 Visualization of Dislocations by Etching 4.3.3 Impurity Hardening . . . . . . . . . . . . . . . 4.4 Extended Defects . . . . . . . . . . . . . . . . . . . . . . . 4.4.1 Microcracks. . . . . . . . . . . . . . . . . . . . 4.4.2 Stacking Faults . . . . . . . . . . . . . . . . . . 4.4.3 Grain Boundaries . . . . . . . . . . . . . . . . 4.4.4 Antiphase and Inversion Domains . . . . . 4.5 Disorder. . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
81 81 81 81 83 85 88 92 96 96 100 101 103 103 103 105 106 110
3.5 3.6
3.7
4
Important Crystal Structures . . . . . . . . . 3.4.1 Rocksalt Structure . . . . . . . . . 3.4.2 CsCl Structure . . . . . . . . . . . 3.4.3 Diamond Structure. . . . . . . . . 3.4.4 Zincblende Structure . . . . . . . 3.4.5 Wurtzite Structure . . . . . . . . . 3.4.6 Chalcopyrite Structure . . . . . . 3.4.7 Spinel Structure. . . . . . . . . . . 3.4.8 Fluorite Structure. . . . . . . . . . 3.4.9 Delafossite Structure . . . . . . . 3.4.10 Perovskite Structure . . . . . . . . 3.4.11 NiAs Structure . . . . . . . . . . . 3.4.12 Further Structures . . . . . . . . . Polytypism . . . . . . . . . . . . . . . . . . . . . Reciprocal Lattice . . . . . . . . . . . . . . . . 3.6.1 Reciprocal Lattice Vectors . . . 3.6.2 Miller Indices . . . . . . . . . . . . 3.6.3 Brillouin Zone . . . . . . . . . . . Alloys . . . . . . . . . . . . . . . . . . . . . . . . 3.7.1 Random Alloys . . . . . . . . . . . 3.7.2 Phase Diagram . . . . . . . . . . . 3.7.3 Virtual Crystal Approximation 3.7.4 Lattice Parameter. . . . . . . . . . 3.7.5 Ordering. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . .
Contents
5
6
xiii
Mechanical Properties. . . . . . . . . . . . . . . . . . . . . . . . . . 5.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Lattice Vibrations . . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 Monoatomic Linear Chain . . . . . . . . . . . 5.2.2 Diatomic Linear Chain . . . . . . . . . . . . . . 5.2.3 Lattice Vibrations of a ThreeDimensional Crystal . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.4 Density of States . . . . . . . . . . . . . . . . . . 5.2.5 Phonons . . . . . . . . . . . . . . . . . . . . . . . . 5.2.6 Localized Vibrational Modes . . . . . . . . . 5.2.7 Phonons in Alloys . . . . . . . . . . . . . . . . . 5.2.8 Disorder . . . . . . . . . . . . . . . . . . . . . . . . 5.2.9 Electric Field Created by Optical Phonons 5.3 Elasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.1 Thermal Expansion . . . . . . . . . . . . . . . . 5.3.2 Stress–Strain Relation . . . . . . . . . . . . . . 5.3.3 Biaxial Strain . . . . . . . . . . . . . . . . . . . . 5.3.4 ThreeDimensional Strain . . . . . . . . . . . . 5.3.5 Substrate Bending . . . . . . . . . . . . . . . . . 5.3.6 Scrolling . . . . . . . . . . . . . . . . . . . . . . . 5.4 Plasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.1 Critical Thickness . . . . . . . . . . . . . . . . . 5.4.2 Cleaving. . . . . . . . . . . . . . . . . . . . . . . . 5.4.3 Wafer Breakage . . . . . . . . . . . . . . . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
111 111 111 112 115
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
118 121 123 124 127 128 129 132 132 133 137 139 141 143 145 145 150 151
Band Structure . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . 6.2 Electrons in a Periodic Potential . . . . . . . . . 6.2.1 Bloch’s Theorem . . . . . . . . . . . . . 6.2.2 FreeElectron Dispersion . . . . . . . 6.2.3 NonVanishing Potential. . . . . . . . 6.2.4 Kramer’s Degeneracy. . . . . . . . . . 6.2.5 Symmetry Considerations . . . . . . . 6.3 Band Structures of Selected Semiconductors. 6.3.1 Silicon . . . . . . . . . . . . . . . . . . . . 6.3.2 Germanium. . . . . . . . . . . . . . . . . 6.3.3 GaAs . . . . . . . . . . . . . . . . . . . . . 6.3.4 GaP . . . . . . . . . . . . . . . . . . . . . . 6.3.5 GaN . . . . . . . . . . . . . . . . . . . . . 6.3.6 Lead Salts . . . . . . . . . . . . . . . . . 6.3.7 MgO, ZnO, CdO . . . . . . . . . . . . . 6.3.8 Chalcopyrites . . . . . . . . . . . . . . . 6.3.9 Spinels. . . . . . . . . . . . . . . . . . . . 6.3.10 Delafossites . . . . . . . . . . . . . . . . 6.3.11 Perovskites . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
153 153 154 154 155 156 159 160 162 163 163 163 163 163 163 164 165 166 166 167
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
xiv
Contents
6.4 6.5 6.6 6.7 6.8 6.9
6.10
6.11
6.12
7
Systematics of Semiconductor Band Gaps . . Alloy Semiconductors . . . . . . . . . . . . . . . . Amorphous Semiconductors . . . . . . . . . . . . Temperature Dependence of the Band Gap. . Isotope Dependence of the Band Gap . . . . . Electron Dispersion . . . . . . . . . . . . . . . . . . 6.9.1 Equation of Electron Motion. . . . . 6.9.2 Effective Mass of Electrons . . . . . 6.9.3 Nonparabolicity of Electron Mass . Holes. . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.10.1 Hole Concept . . . . . . . . . . . . . . . 6.10.2 Hole Dispersion Relation . . . . . . . 6.10.3 ValenceBand Fine Structure. . . . . 6.10.4 Band Inversion . . . . . . . . . . . . . . Strain Effects on the Band Structure . . . . . . 6.11.1 Strain Effect on Band Edges . . . . . 6.11.2 Strain Effect on Effective Masses . 6.11.3 Interaction with a Localized Level . Density of States. . . . . . . . . . . . . . . . . . . . 6.12.1 General Band Structure . . . . . . . . 6.12.2 Amorphous Semiconductors . . . . . 6.12.3 FreeElectron Gas . . . . . . . . . . . .
Electronic Defect States. . . . . . . . . . . 7.1 Introduction . . . . . . . . . . . . . . 7.2 Carrier Concentration. . . . . . . . 7.3 Intrinsic Conduction . . . . . . . . 7.4 Doping . . . . . . . . . . . . . . . . . 7.4.1 Concept . . . . . . . . . . 7.4.2 Doping Principles . . . 7.5 Shallow Defects . . . . . . . . . . . 7.5.1 Donors. . . . . . . . . . . 7.5.2 Acceptors . . . . . . . . . 7.5.3 Compensation . . . . . . 7.5.4 Multiple Impurities . . 7.5.5 Amphoteric Impurities 7.5.6 Autodoping . . . . . . . 7.5.7 High Doping. . . . . . . 7.6 QuasiFermi Levels . . . . . . . . . 7.7 Deep Levels . . . . . . . . . . . . . . 7.7.1 Charge States . . . . . . 7.7.2 Double Donors . . . . . 7.7.3 Double Acceptors . . . 7.7.4 Jahn–Teller Effect . . . 7.7.5 NegativeU Center. . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
168 170 173 174 176 177 177 178 181 183 183 184 188 189 190 191 193 194 195 195 196 199
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .
203 203 204 207 209 209 210 211 211 220 223 226 228 229 230 234 235 236 238 240 241 242
Contents
xv
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
. . . . . .
245 247 247 249 251 251
8
Transport. . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1 Introduction . . . . . . . . . . . . . . . . . . . . . . 8.2 Conductivity. . . . . . . . . . . . . . . . . . . . . . 8.3 LowField Transport . . . . . . . . . . . . . . . . 8.3.1 Mobility . . . . . . . . . . . . . . . . . . 8.3.2 Microscopic Scattering Processes. 8.3.3 Ionized Impurity Scattering. . . . . 8.3.4 Deformation Potential Scattering . 8.3.5 Piezoelectric Potential Scattering . 8.3.6 Polar Optical Scattering . . . . . . . 8.3.7 Dislocation Scattering . . . . . . . . 8.3.8 Grain Boundary Scattering . . . . . 8.3.9 Temperature Dependence . . . . . . 8.3.10 Doping Dependence. . . . . . . . . . 8.3.11 Piezoresistivity . . . . . . . . . . . . . 8.4 HighField Transport . . . . . . . . . . . . . . . . 8.4.1 DriftSaturation Velocity . . . . . . 8.4.2 Negative Differential Resistivity . 8.4.3 Velocity Overshoot . . . . . . . . . . 8.4.4 Impact Ionization. . . . . . . . . . . . 8.5 HighFrequency Transport . . . . . . . . . . . . 8.6 Polarons. . . . . . . . . . . . . . . . . . . . . . . . . 8.6.1 Large Polarons . . . . . . . . . . . . . 8.6.2 Small Polarons . . . . . . . . . . . . . 8.7 Hopping Transport . . . . . . . . . . . . . . . . . 8.8 Transport in Amorphous Semiconductors . . 8.9 Ionic Transport . . . . . . . . . . . . . . . . . . . . 8.10 Diffusion . . . . . . . . . . . . . . . . . . . . . . . . 8.11 Continuity Equation . . . . . . . . . . . . . . . . 8.12 Heat Conduction . . . . . . . . . . . . . . . . . . . 8.13 Coupled Heat and Charge Transport . . . . . 8.13.1 Thermopower and Seebeck Effect 8.13.2 Peltier Effect. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
255 255 256 258 258 259 260 261 262 262 263 263 264 266 267 268 269 269 270 271 275 275 275 277 278 280 281 282 284 284 286 286 289
9
Optical Properties . . . . . . . . . . . . . . . 9.1 Spectral Regions and Overview 9.2 Complex Dielectric Function . . 9.3 Reflection and Diffraction . . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
291 291 292 293
7.8
7.7.6 DX Center . . . . . . . . . . . . . . . 7.7.7 EL2 Defect. . . . . . . . . . . . . . . 7.7.8 Semiinsulating Semiconductors 7.7.9 Isoelectronic Impurities . . . . . . 7.7.10 Surface States . . . . . . . . . . . . . Hydrogen in Semiconductors . . . . . . . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
xvi
Contents
9.4 9.5 9.6
9.7
9.8
9.9
Absorption . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Electron–Photon Interaction . . . . . . . . . . . . . . . . . Band–Band Transitions . . . . . . . . . . . . . . . . . . . . 9.6.1 Joint Density of States . . . . . . . . . . . . . . 9.6.2 Direct Transitions . . . . . . . . . . . . . . . . . 9.6.3 Indirect Transitions . . . . . . . . . . . . . . . . 9.6.4 Urbach Tail . . . . . . . . . . . . . . . . . . . . . 9.6.5 Amorphous Semiconductors . . . . . . . . . . 9.6.6 Excitons . . . . . . . . . . . . . . . . . . . . . . . . 9.6.7 Phonon Broadening . . . . . . . . . . . . . . . . 9.6.8 Exciton Polariton. . . . . . . . . . . . . . . . . . 9.6.9 BoundExciton Absorption . . . . . . . . . . . 9.6.10 Biexcitons . . . . . . . . . . . . . . . . . . . . . . 9.6.11 Trions . . . . . . . . . . . . . . . . . . . . . . . . . 9.6.12 Band Gap Renormalization . . . . . . . . . . . 9.6.13 Electron–Hole Droplets . . . . . . . . . . . . . 9.6.14 TwoPhoton Absorption . . . . . . . . . . . . . Impurity Absorption . . . . . . . . . . . . . . . . . . . . . . 9.7.1 Shallow Levels . . . . . . . . . . . . . . . . . . . 9.7.2 Deep Levels . . . . . . . . . . . . . . . . . . . . . Absorption in the Presence of Free Charge Carriers. 9.8.1 FreeCarrier Absorption . . . . . . . . . . . . . 9.8.2 Burstein–Moss Shift . . . . . . . . . . . . . . . 9.8.3 InterValenceband Transitions . . . . . . . . . 9.8.4 InterValley Transitions . . . . . . . . . . . . . 9.8.5 IntraBand Transitions . . . . . . . . . . . . . . Lattice Absorption. . . . . . . . . . . . . . . . . . . . . . . . 9.9.1 Dielectric Constant . . . . . . . . . . . . . . . . 9.9.2 Reststrahlenbande . . . . . . . . . . . . . . . . . 9.9.3 Polaritons . . . . . . . . . . . . . . . . . . . . . . . 9.9.4 Phonon–Plasmon Coupling . . . . . . . . . . .
10 Recombination . . . . . . . . . . . . . . . . . . . . 10.1 Introduction . . . . . . . . . . . . . . . . . 10.2 Band–Band Recombination . . . . . . 10.2.1 Spontaneous Emission . . . 10.2.2 Absorption . . . . . . . . . . . 10.2.3 Stimulated Emission . . . . 10.2.4 Net Recombination Rate. . 10.2.5 Recombination Dynamics . 10.2.6 Lasing . . . . . . . . . . . . . . 10.3 Exciton Recombination . . . . . . . . . 10.3.1 Free Excitons . . . . . . . . . 10.3.2 Bound Excitons. . . . . . . . 10.3.3 Alloy Broadening . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
295 297 299 299 300 304 307 308 309 313 313 317 319 319 320 321 322 323 323 326 328 328 332 334 335 336 337 337 338 339 340
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
. . . . . . . . . . . . .
343 343 344 344 346 347 347 349 350 351 351 351 358
Contents
xvii
10.4 10.5 10.6 10.7 10.8 10.9
10.10 10.11
10.12
10.13
Part II
Phonon Replica . . . . . . . . . . . . . . . . . SelfAbsorption. . . . . . . . . . . . . . . . . . Donor–Acceptor Pair Transitions. . . . . . InnerImpurity Recombination . . . . . . . Auger Recombination . . . . . . . . . . . . . Band–Impurity Recombination . . . . . . . 10.9.1 Shockley–Read–Hall Kinetics . 10.9.2 Multilevel Traps . . . . . . . . . . ABC Model . . . . . . . . . . . . . . . . . . . . Field Effect . . . . . . . . . . . . . . . . . . . . 10.11.1 Thermally Activated Emission. 10.11.2 Direct Tunneling . . . . . . . . . . 10.11.3 Assisted Tunneling . . . . . . . . Recombination at Extended Defects. . . . 10.12.1 Surfaces . . . . . . . . . . . . . . . . 10.12.2 Grain Boundaries . . . . . . . . . 10.12.3 Dislocations . . . . . . . . . . . . . ExcessCarrier Profiles. . . . . . . . . . . . . 10.13.1 Generation at Surface. . . . . . . 10.13.2 Generation in the Bulk . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . .
362 365 366 367 368 370 370 374 374 375 375 376 376 377 377 378 378 379 379 380
Selected Topics
11 Surfaces . . . . . . . . . . . . . . . . . . . . . . . . 11.1 Introduction . . . . . . . . . . . . . . . . 11.2 Surface Crystallography . . . . . . . . 11.3 Surface Energy . . . . . . . . . . . . . . 11.4 Surface Reconstruction . . . . . . . . 11.5 Surface Morphology . . . . . . . . . . 11.6 Surface Physical Properties. . . . . . 11.6.1 Surface Phonons . . . . . . 11.6.2 Surface Plasmons . . . . . 11.6.3 Electronic Surface States
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
. . . . . . . . . .
385 385 386 387 388 390 392 392 393 395
12 Heterostructures . . . . . . . . . . . . . . . . . . . 12.1 Introduction . . . . . . . . . . . . . . . . . 12.2 Heteroepitaxy . . . . . . . . . . . . . . . . 12.2.1 Growth Methods . . . . . . . 12.2.2 Substrates . . . . . . . . . . . . 12.2.3 Growth Modes . . . . . . . . 12.2.4 Heterosubstrates . . . . . . . 12.2.5 Patterned Substrates . . . . . 12.2.6 Pseudomorphic Structures. 12.2.7 Plastic Relaxation . . . . . . 12.2.8 Surfactants . . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
399 399 400 400 400 403 405 410 412 413 414
xviii
Contents
12.3
12.4
12.5 12.6
Energy Levels in Heterostructures . . . . . . . . . . . . . . . . . . 12.3.1 Band Lineup in Heterostructures . . . . . . . . . . . . 12.3.2 Quantum Wells . . . . . . . . . . . . . . . . . . . . . . . . 12.3.3 Superlattices . . . . . . . . . . . . . . . . . . . . . . . . . . 12.3.4 Single Heterointerface Between Doped Materials. Recombination in Quantum Wells . . . . . . . . . . . . . . . . . . 12.4.1 Thickness Dependence . . . . . . . . . . . . . . . . . . . 12.4.2 Broadening Effects . . . . . . . . . . . . . . . . . . . . . 12.4.3 Quantum Confined Stark Effect. . . . . . . . . . . . . Isotope Superlattices . . . . . . . . . . . . . . . . . . . . . . . . . . . Wafer Bonding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
13 External Fields . . . . . . . . . . . . . . . . . . . . . . . . 13.1 Electric Fields. . . . . . . . . . . . . . . . . . . . 13.1.1 Bulk Material . . . . . . . . . . . . . 13.1.2 Quantum Wells . . . . . . . . . . . . 13.2 Magnetic Fields . . . . . . . . . . . . . . . . . . 13.2.1 Hall Effect . . . . . . . . . . . . . . . 13.2.2 FreeCarrier Absorption . . . . . . 13.2.3 Energy Levels in Bulk Crystals . 13.2.4 Energy Levels in a 2DEG. . . . . 13.2.5 Shubnikov–de Haas Oscillations 13.3 Quantum Hall Effect . . . . . . . . . . . . . . . 13.3.1 Integral QHE . . . . . . . . . . . . . 13.3.2 Fractional QHE . . . . . . . . . . . . 13.3.3 Weiss Oscillations . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
415 415 417 424 424 427 427 428 431 433 433
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
. . . . . . . . . . . . . .
437 437 437 439 441 441 448 449 451 452 453 455 458 460
14 Nanostructures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.2 Quantum Wires. . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.2.1 VGroove Quantum Wires . . . . . . . . . . . . . 14.2.2 CleavedEdge Overgrowth Quantum Wires . . 14.2.3 Nanowhiskers . . . . . . . . . . . . . . . . . . . . . . 14.2.4 Nanobelts . . . . . . . . . . . . . . . . . . . . . . . . . 14.2.5 Quantization in TwoDimensional Potential Wells . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3 Quantum Dots . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.1 Quantization in ThreeDimensional Potential Wells . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.2 Electrical and Transport Properties. . . . . . . . 14.3.3 SelfAssembled Preparation . . . . . . . . . . . . 14.3.4 Optical Properties . . . . . . . . . . . . . . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
461 461 462 462 465 465 467
..... .....
468 471
. . . .
. . . .
471 473 477 482
15 Polarized Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.2 Spontaneous Polarization . . . . . . . . . . . . . . . . . . . . . . . . . .
489 489 489
. . . .
. . . .
. . . .
Contents
15.3
15.4
xix
Ferroelectricity . . . . . . . . . . . . . . . . . . . . . . . . 15.3.1 Materials . . . . . . . . . . . . . . . . . . . . . 15.3.2 Soft Phonon Mode . . . . . . . . . . . . . . 15.3.3 Phase Transition . . . . . . . . . . . . . . . . 15.3.4 Domains. . . . . . . . . . . . . . . . . . . . . . 15.3.5 Optical Properties . . . . . . . . . . . . . . . Piezoelectricity . . . . . . . . . . . . . . . . . . . . . . . . 15.4.1 Piezoelectric Effect . . . . . . . . . . . . . . 15.4.2 Zincblende Crystals . . . . . . . . . . . . . . 15.4.3 Wurtzite Crystals. . . . . . . . . . . . . . . . 15.4.4 Piezoelectric Effects in Nanostructures .
16 Magnetic Semiconductors . . . . . . . . . . . 16.1 Introduction . . . . . . . . . . . . . . . . 16.2 Magnetic Semiconductors. . . . . . . 16.3 Diluted Magnetic Semiconductors . 16.4 Spintronics . . . . . . . . . . . . . . . . . 16.4.1 Spin Transistor . . . . . . . 16.4.2 Spin LED. . . . . . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
490 492 492 493 496 497 498 498 498 499 503
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
505 505 505 507 511 512 512
17 Organic Semiconductors . . . . . . . . . . . . . . . . . . . . 17.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . 17.2 Materials . . . . . . . . . . . . . . . . . . . . . . . . . . 17.2.1 Small Organic Molecules, Polymers. 17.2.2 Organic Semiconductor Crystals . . . 17.3 Electronic Structure . . . . . . . . . . . . . . . . . . . 17.4 Doping . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.5 Transport Properties . . . . . . . . . . . . . . . . . . 17.6 Optical Properties . . . . . . . . . . . . . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
515 515 515 515 516 519 520 521 522
18 Graphene and Carbon Nanotubes . . . . . . . . . . . 18.1 Graphene . . . . . . . . . . . . . . . . . . . . . . . . 18.1.1 Structure . . . . . . . . . . . . . . . . . 18.1.2 Band Structure . . . . . . . . . . . . . 18.1.3 Electrical Properties . . . . . . . . . . 18.1.4 Other TwoDimensional Crystals . 18.2 Carbon Nanotubes. . . . . . . . . . . . . . . . . . 18.2.1 Structure . . . . . . . . . . . . . . . . . 18.2.2 Band Structure . . . . . . . . . . . . . 18.2.3 Optical Properties . . . . . . . . . . . 18.2.4 Other Anorganic Nanotubes . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
529 529 529 529 531 536 536 536 538 541 541
19 Dielectric Structures . . . . . . . . . . . . . . . . . . . 19.1 Photonic Band Gap Materials . . . . . . . . 19.1.1 Introduction . . . . . . . . . . . . . 19.1.2 General 1D Scattering Theory .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
545 545 545 546
. . . .
. . . . . . .
. . . . . . . . . . .
. . . . . . .
. . . .
. . . . . . .
. . . . . . . . . . .
xx
Contents
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
. . . . . . . . . . .
548 550 552 558 558 562 565 565 567 568 571
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
575 575 575 577
21 Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2 Metal–Semiconductor Contacts . . . . . . . . . . . . . . . . 21.2.1 Band Diagram in Equilibrium . . . . . . . . . . 21.2.2 SpaceCharge Region. . . . . . . . . . . . . . . . 21.2.3 Schottky Effect . . . . . . . . . . . . . . . . . . . . 21.2.4 Capacitance . . . . . . . . . . . . . . . . . . . . . . 21.2.5 Current–Voltage Characteristic . . . . . . . . . 21.2.6 Ohmic Contacts. . . . . . . . . . . . . . . . . . . . 21.2.7 Metal Contacts to Organic Semiconductors . 21.3 Metal–Insulator–Semiconductor Diodes . . . . . . . . . . 21.3.1 Band Diagram for Ideal MIS Diode . . . . . . 21.3.2 SpaceCharge Region. . . . . . . . . . . . . . . . 21.3.3 Capacitance . . . . . . . . . . . . . . . . . . . . . . 21.3.4 Nonideal MIS Diode . . . . . . . . . . . . . . . . 21.4 Bipolar Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.4.1 Band Diagram. . . . . . . . . . . . . . . . . . . . . 21.4.2 SpaceCharge Region. . . . . . . . . . . . . . . . 21.4.3 Capacitance . . . . . . . . . . . . . . . . . . . . . . 21.4.4 Current–Voltage Characteristics. . . . . . . . . 21.4.5 Breakdown . . . . . . . . . . . . . . . . . . . . . . . 21.4.6 Heterostructure Diodes . . . . . . . . . . . . . . . 21.4.7 Organic Semiconductor Diodes . . . . . . . . . 21.5 Applications and Special Diode Devices . . . . . . . . . 21.5.1 Rectification . . . . . . . . . . . . . . . . . . . . . . 21.5.2 Frequency Mixing . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
583 583 583 584 589 593 594 598 611 613 615 616 619 623 624 626 626 626 632 633 644 649 650 652 653 655
19.2
19.1.3 Transmission of an NPeriod Potential . 19.1.4 The QuarterWave Stack . . . . . . . . . . 19.1.5 Formation of a 3D Band Structure. . . . 19.1.6 Disorder . . . . . . . . . . . . . . . . . . . . . . 19.1.7 Defect Modes . . . . . . . . . . . . . . . . . . 19.1.8 Coupling to an Electronic Resonance . . Microscopic Resonators . . . . . . . . . . . . . . . . . . 19.2.1 Microdiscs . . . . . . . . . . . . . . . . . . . . 19.2.2 Purcell Effect . . . . . . . . . . . . . . . . . . 19.2.3 Deformed Resonators. . . . . . . . . . . . . 19.2.4 Hexagonal Cavities . . . . . . . . . . . . . .
20 Transparent Conductive 20.1 Introduction . . . . 20.2 Materials . . . . . . 20.3 Properties. . . . . . Part III
Oxide Semiconductors . .................. .................. ..................
. . . .
. . . .
. . . .
. . . .
Applications
Contents
xxi
21.5.3 21.5.4 21.5.5 21.5.6 21.5.7 21.5.8 21.5.9 21.5.10 21.5.11
Voltage Regulator . . . Zener Diodes . . . . . . Varactors . . . . . . . . . FastRecovery Diodes StepRecovery Diodes PinDiodes . . . . . . . . Tunneling Diodes . . . Backward Diodes . . . Gunn Diodes . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
656 658 658 660 661 662 663 666 667
22 LighttoElectricity Conversion . . . . . . . . . . . . . 22.1 Photocatalysis . . . . . . . . . . . . . . . . . . . . . 22.2 Photoconductors . . . . . . . . . . . . . . . . . . . 22.2.1 Introduction . . . . . . . . . . . . . . . 22.2.2 Photoconductivity Detectors . . . . 22.2.3 Electrophotography . . . . . . . . . . 22.2.4 QWIPs. . . . . . . . . . . . . . . . . . . 22.2.5 Blocked ImpurityBand Detectors 22.3 Photodiodes . . . . . . . . . . . . . . . . . . . . . . 22.3.1 Introduction . . . . . . . . . . . . . . . 22.3.2 pn Photodiodes . . . . . . . . . . . . . 22.3.3 Pin Photodiodes . . . . . . . . . . . . 22.3.4 PositionSensing Detector . . . . . . 22.3.5 MSM Photodiodes . . . . . . . . . . . 22.3.6 Avalanche Photodiodes . . . . . . . 22.3.7 TravelingWave Photodetectors . . 22.3.8 Charge Coupled Devices . . . . . . 22.3.9 Photodiode Arrays . . . . . . . . . . . 22.4 Solar Cells . . . . . . . . . . . . . . . . . . . . . . . 22.4.1 Solar Radiation . . . . . . . . . . . . . 22.4.2 Ideal Solar Cells . . . . . . . . . . . . 22.4.3 Real Solar Cells . . . . . . . . . . . . 22.4.4 Design Refinements . . . . . . . . . . 22.4.5 Modules . . . . . . . . . . . . . . . . . . 22.4.6 SolarCell Types . . . . . . . . . . . . 22.4.7 Commercial Issues. . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . .
669 669 670 670 671 674 675 678 680 680 681 684 686 686 692 695 698 705 707 708 709 714 715 716 718 721
23 ElectricitytoLight Conversion . . . . . . . . . . . 23.1 Radiometric and Photometric Quantities. 23.1.1 Radiometric Quantities . . . . . . 23.1.2 Photometric Quantities . . . . . . 23.2 Scintillators . . . . . . . . . . . . . . . . . . . . 23.2.1 CIE Chromaticity Diagram . . . 23.2.2 Display Applications . . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
725 725 725 725 727 727 730
. . . . . . .
. . . . . . .
xxii
Contents
23.3
23.4
23.5
23.2.3 Radiation Detection . . . . . . . . . . . . . . . 23.2.4 Luminescence Mechanisms . . . . . . . . . . LightEmitting Diodes . . . . . . . . . . . . . . . . . . . . 23.3.1 Introduction . . . . . . . . . . . . . . . . . . . . 23.3.2 Spectral Ranges. . . . . . . . . . . . . . . . . . 23.3.3 Efficiencies. . . . . . . . . . . . . . . . . . . . . 23.3.4 Device Design . . . . . . . . . . . . . . . . . . 23.3.5 White LEDs . . . . . . . . . . . . . . . . . . . . 23.3.6 Quantum Dot LEDs. . . . . . . . . . . . . . . 23.3.7 Organic LEDs. . . . . . . . . . . . . . . . . . . Lasers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 23.4.1 Introduction . . . . . . . . . . . . . . . . . . . . 23.4.2 Applications . . . . . . . . . . . . . . . . . . . . 23.4.3 Gain . . . . . . . . . . . . . . . . . . . . . . . . . 23.4.4 Optical Mode . . . . . . . . . . . . . . . . . . . 23.4.5 Loss Mechanisms . . . . . . . . . . . . . . . . 23.4.6 Threshold . . . . . . . . . . . . . . . . . . . . . . 23.4.7 Spontaneous Emission Factor . . . . . . . . 23.4.8 Output Power . . . . . . . . . . . . . . . . . . . 23.4.9 Temperature Dependence . . . . . . . . . . . 23.4.10 Mode Spectrum. . . . . . . . . . . . . . . . . . 23.4.11 Longitudinal SingleMode Lasers . . . . . 23.4.12 Tunability. . . . . . . . . . . . . . . . . . . . . . 23.4.13 Dynamics and Modulation . . . . . . . . . . 23.4.14 SurfaceEmitting Lasers . . . . . . . . . . . . 23.4.15 Optically Pumped Semiconductor Lasers 23.4.16 Quantum Cascade Lasers . . . . . . . . . . . 23.4.17 HotHole Lasers . . . . . . . . . . . . . . . . . Semiconductor Optical Amplifiers . . . . . . . . . . . .
24 Transistors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . 24.2 Bipolar Transistors . . . . . . . . . . . . . . . . . . 24.2.1 Carrier Density and Currents. . . . . 24.2.2 Current Amplification . . . . . . . . . 24.2.3 Ebers–Moll Model. . . . . . . . . . . . 24.2.4 Current–Voltage Characteristics. . . 24.2.5 Basic Circuits . . . . . . . . . . . . . . . 24.2.6 HighFrequency Properties . . . . . . 24.2.7 Heterojunction Bipolar Transistors . 24.2.8 LightEmitting Transistors . . . . . . 24.3 FieldEffect Transistors . . . . . . . . . . . . . . . 24.4 JFET and MESFET . . . . . . . . . . . . . . . . . . 24.4.1 General Principle. . . . . . . . . . . . . 24.4.2 Static Characteristics . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
731 732 733 733 734 735 736 743 746 747 749 749 750 752 755 762 763 765 766 768 769 770 771 774 778 782 783 784 785
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .
787 787 788 790 792 794 796 798 800 800 801 802 804 804 805
Contents
xxiii
. . . . . . . . . . . . . . . .
809 809 812 812 812 814 818 818 821 829 830 833 837 837 838 839
Appendix A: Tensors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
843
Appendix B: Point and Space Groups . . . . . . . . . . . . . . . . . . . . . . . .
847
Appendix C: Kramers–Kronig Relations. . . . . . . . . . . . . . . . . . . . . . .
851
Appendix D: Oscillator Strength . . . . . . . . . . . . . . . . . . . . . . . . . . . .
853
Appendix E: Quantum Statistics. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
859
Appendix F: Kronig–Penney Model . . . . . . . . . . . . . . . . . . . . . . . . . .
865
Appendix G: The k p Perturbation Theory . . . . . . . . . . . . . . . . . . . .
869
Appendix H: EffectiveMass Theory . . . . . . . . . . . . . . . . . . . . . . . . . .
873
Appendix I: Boltzmann Transport Theory . . . . . . . . . . . . . . . . . . . . .
875
Appendix J: Noise . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
881
References. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
891
Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
967
24.5
24.6
24.4.3 Normally on and Normally Off FETs. 24.4.4 FieldDependent Mobility . . . . . . . . . 24.4.5 HighFrequency Properties . . . . . . . . MOSFETs . . . . . . . . . . . . . . . . . . . . . . . . . . 24.5.1 Operation Principle . . . . . . . . . . . . . 24.5.2 Current–Voltage Characteristics. . . . . 24.5.3 MOSFET Types . . . . . . . . . . . . . . . 24.5.4 Complementary MOS . . . . . . . . . . . 24.5.5 LargeScale Integration . . . . . . . . . . 24.5.6 Tunneling FETs . . . . . . . . . . . . . . . 24.5.7 Nonvolatile Memories . . . . . . . . . . . 24.5.8 Heterojunction FETs . . . . . . . . . . . . ThinFilm Transistors . . . . . . . . . . . . . . . . . . 24.6.1 Annealing of Amorphous Silicon. . . . 24.6.2 TFT Devices. . . . . . . . . . . . . . . . . . 24.6.3 OFETs . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . .
Abbreviations
0D 1D 2D 2DEG 3D A AAAS AB ac ACS AFM AHE AIP AM APD APS AR ARPES ASE AVS bc bcc BC BD BEC BGR BIA BJT CAS CCD
Zerodimensional Onedimensional Twodimensional Twodimensional electron gas Threedimensional Atomic mass (A ¼ 12 for 12 C) American Association for the Advancement of Science Antibonding (position) Alternating current American Chemical Society Atomic force microscopy Anomalous Hall effect American Institute of Physics Air mass Antiphase domain, avalanche photodiode American Physical Society Antireflection Angleresolved photoemission spectroscopy Ampliﬁed spontaneous emission American Vacuum Society (The Science & Technology Society) Bodycentered Bodycentered cubic Bond center (position) BlurayTM disc Bose–Einstein condensation Band gap renormalization Bulk inversion asymmetry Bipolar junction transistor Calorimetric absorption spectroscopy Charge coupled device
xxv
xxvi
CD CEO CIE CIGS CIS CL CMOS CMY CNT COD CPU CRT CSL CVD cw CZ DAP DBR dc DF DFB DH(S) DLTS DMS DOS DPSS DRAM DVD EA EBL EEPROM EHL EIL EL ELA ELO EMA EML EPR EPROM ESF ESR ETL EXAFS F4 TCNQ
Abbreviations
Compact disc Cleavededge overgrowth Commission Internationale de l’Éclairage Cu(In,Ga)Se2 material CuInSe2 material Cathodoluminescence Complementary metal–oxide–semiconductor Cyan–magenta–yellow (color system) Carbon nanotube Catastrophical optical damage Central processing unit Cathode ray tube Coincident site lattice Chemical vapor deposition Continuous wave Czochralski (growth) Donor–acceptor pair Distributed Bragg reflector Direct current Dielectric function Distributed feedback Double heterostructure Deep level transient spectroscopy Diluted magnetic semiconductor Density of states Diodepumped solidstate (laser) Dynamic random access memory Digital versatile disc Electron afﬁnity Electron blocking layer Electrically erasable programmable readonly memory Electron–hole liquid Electron injection layer Electroluminescence Excimer laser annealing Epitaxial lateral overgrowth Effective mass approximation Emission layer Electron paramagnetic resonance Erasable programmable readonly memory Extrinsic stacking fault Electron spin resonance Electron transport layer Extended Xray absorption ﬁne structure 2,3,5,6tetrafluoro7,7,8,8tetracyanoquinodimethane
Abbreviations
fc fcc FeRAM FET FIB FIR FKO FLG FPA FQHE FWHM FZ Gb GIZO GLAD GRINSCH GSMBE GST HBL HBT Hcp HCSEL HEMT HIGFET HIL HJFET hh HOPG HOMO HR HRTEM HTL HWHM IBM IC IDB IE IEEE IF IPAP IQHE IR
1
xxvii
Facecentered Facecentered cubic Ferroelectric random access memory Fieldeffect transistor Focused ion beam Far infrared Franz–Keldysh oscillation Few layer graphene Focal plane array Fractional quantum Hall effect Full width at halfmaximum Floatzone (growth) Gigabit GaInZnO Glancingangle deposition Gradedindex separate conﬁnement heterostructure Gassource molecular beam epitaxy Ge2 Sb2 Te5 Hole blocking layer Heterobipolar transistor Hexagonally close packed Horizontal cavity surfaceemitting laser High electron mobility transistor Heterojunction insulating gate FET Hole injection layer Heterojunction FET Heavy hole Highly ordered pyrolitic graphite Highest occupied molecular orbital High reflection Highresolution transmission electron microscopy Hole transport layer Halfwidth at halfmaximum International Business Machines Corporation Integrated circuit Inversion domain boundary Ionization energy Institute of Electrical and Electronics Engineers1 Intermediate frequency Institute of Pure and Applied Physics, Tokyo Integral quantum Hall effect Infrared
Pronounced EyetripleE,
xxviii
ISF ITO JDOS JFET KKR KOH KTP LA LCD LDA LEC LED lh LO LPE LPCVD LPP LST LT LUMO LVM MBE MEMS MESFET MHEMT MIGS MILC MIOS MIR MIS MIT ML MLC MMIC MO MODFET MOMBE MOPA MOS MOSFET MOVPE MQW MRAM MRS MS
Abbreviations
Intrinsic stacking fault Indium tin oxide Joint density of states Junction ﬁeldeffect transistor Kramers–Kronig relation Potassium hydroxide KTiOPO4 material Longitudinal acoustic (phonon) Liquid crystal display Local density approximation Liquid encapsulated Czochralski (growth) Lightemitting diode Light hole Longitudinal optical (phonon), local oscillator Liquid phase epitaxy Lowpressure chemical vapor deposition Longitudinal phonon plasmon (mode) Lyddane–Sachs–Teller (relation) Low temperature Lowest unoccupied molecular orbital Local vibrational mode Molecular beam epitaxy Microelectromechanical system Metal–semiconductor ﬁeldeffect transistor Metamorphic HEMT Midgap (surface) states Metalinduced lateral crystallization Metal–insulator–oxide–semiconductor Midinfrared Metal–insulator–semiconductor Massachusetts Institute of Technology Monolayer Multilevel cell Millimeterwave integrated circuit Master oscillator Modulationdoped FET Metalorganic molecular beam epitaxy Master oscillator power ampliﬁer Metal–oxide–semiconductor Metal–oxide–semiconductor ﬁeldeffect transistor Metalorganic chemical vapor deposition Multiple quantum well Magnetic random access memory Materials Research Society Metal–semiconductor (diode)
Abbreviations
MSA MSM MTJ MWNT NDR NEP NIR NMOS NTSC OLED OMC ONO OPSL PA PBG pc PCM PFM PHEMT PL PLD PLE PMC PMMA PMOS PPC PPLN PV PWM PZT QCL QCSE QD QHE QW QWIP QWR RAM RAS RF RFID RGB RHEED RIE RKKY
xxix
Mobility spectral analysis Metal–semiconductor–metal (diode) Magnetotunneling junction Multiwalled (carbon) nanotube Negative differential resistance Noise equivalent power Near infrared Nchannel metal–oxide–semiconductor (transistor) National television standard colors Organic lightemitting diode Organic molecular crystals Oxide/nitride/oxide Optically pumped semiconductor laser Power ampliﬁer Photonic band gap Primitive cubic Phase change memory Piezoresponse force microscopy Pseudomorphic HEMT Photoluminescence Pulsed laser deposition Photoluminescence excitation (spectroscopy) Programmable metallization cell Polymethyl methacrylate Pchannel metal–oxide–semiconductor (transistor) Persistent photoconductivity Perodically poled lithium niobate Photovoltaic(s) Pulsewidth modulation PbTix Zr1x O3 material Quantum cascade laser Quantum conﬁned Stark effect Quantum dot Quantum Hall effect Quantum well Quantumwell intersubband photodetector Quantum wire Random access memory Reflection anisotropy spectroscopy Radio frequency Radio frequency identiﬁcation Red–green–blue (color system) Reflection highenergy electron diffraction Reactive ion etching Ruderman–Kittel–Kasuya–Yoshida (interaction)
xxx
rms ROM RRAM SAGB SAM sc SCH SdH SEL SEM SET SGDBR SHG si SIA SIA SIMS SL SLC SLG SNR so SOA SPD SPICE SPIE SPP SPS sRGB SRH SSR STEM STM SWNT TA TAS TCO TE TED TEGFET TEM TES TF TFET TFT
Abbreviations
Root mean square Readonly memory Resistance random access memory Smallangle grain boundary Separate absorption and ampliﬁcation (structure) Simple cubic Separate conﬁnement heterostructure Shubnikov–de Haas (oscillation) Surfaceemitting laser Scanning electron microscopy Singleelectron transistor, singleelectron tunneling Sampled grating distributed Bragg reflector Secondharmonic generation Semiinsulating Semiconductor Industry Association Structural inversion asymmetry Secondary ion mass spectrometry Superlattice Singlelevel cell Single layer graphene Signaltonoise ratio Spinorbit (or splitoff) Semiconductor optical ampliﬁer Spectral power distribution Simulation Program with Integrated Circuit Emphasis Society of Photographic Instrumentation Engineers Surface plasmon polariton Shortperiod superlattice Standard RGB Shockley–Read–Hall (kinetics) Sidemode suppression ratio Scanning transmission electron microscopy Scanning tunneling microscopy Singlewalled (carbon) nanotube Transverse acoustic (phonon) Thermal admittance spectroscopy Transparent conductive oxide Transverse electric (polarization) Transferred electron device Twodimensional electron gas FET Transmission electron microscopy Twoelectron satellite Thermionic ﬁeld emission Transparent FET, tunneling FET Thinﬁlm transistor
Abbreviations
TM TMAH TMR TO TOD TPA TSO UHV UV VCA VCO VCSEL VFF VGF VIS VLSI WGM WKB WS YSZ X XSTM XX Z ZnPc
xxxi
Transverse magnetic (polarization) Tetramethylammoniumhydroxide Tunnelmagnetoresistance Transverse optical (phonon) Turnon delay (time) Twophoton absorption Transparent semiconducting oxide Ultrahigh vacuum Ultraviolet Virtual crystal approximation Voltagecontrolled oscillator Verticalcavity surfaceemitting laser Valence force ﬁeld Vertical gradient freeze (growth) Visible Very large scale integration Whispering gallery mode Wentzel–Kramer–Brillouin (approximation or method) Wigner–Seitz (cell) Yttriastabilized zirconia (ZrO2 ) Exciton Crosssectional STM Biexciton Atomic number (Z ¼ 2 for helium) Zincphthalocyanine
Symbols
α αðωÞ αm αn αp αT β γ Γ γ1, γ 2, γ3 δij Δ0 ðωÞ 0 i r s S ij η ηd ηext ηint ηw θ ΘD ΘB κ λ
Madelung constant, disorder parameter, linewidth enhancement factor Absorption coefﬁcient Mirror loss Electron ionization coefﬁcient Hole ionization coefﬁcient Base transport factor Used as abbreviation for e=ðkB TÞ, spontaneous emission coefﬁcient, twophoton absorption coefﬁcient Broadening parameter, Grüneisen parameter, emitter efﬁciency Broadening parameter Luttinger parameters Kronecker symbol Spinorbit splitting Dielectric function Permittivity of vacuum Dielectric constant of insulator Relative dielectric function Dielectric function of semiconductor (¼ r 0 ) Gain compression coefﬁcient Components of strain tensor Quantum efﬁciency Differential quantum efﬁciency External quantum efﬁciency Internal quantum efﬁciency Wallplug efﬁciency Angle Debye temperature Typical phonon energy parameter Imaginary part of index of refraction, heat conductivity Wavelength
xxxiii
xxxiv
λp μ μ0 μh μH μn ν Π πij ρ ρij ρP σ Σn σ ij σn σp σP τ τn τnr τp τr ΘD φ Φ0 χ χex χsc χðrÞ ψ ΨðrÞ ω ωLO ωp ωTO Ω a a A A, A A a0 b
Symbols
Plasma wavelength Mobility Magnetic susceptibility of vacuum Hole mobility Hall mobility Electron mobility Frequency Peltier coefﬁcient Components of piezoresistivity tensor Mass density, charge density, resistivity Components of resistivity tensor Polarization charge density (per volume) Standard deviation, conductivity, stress, effective mass ratio Grain boundary type Components of stress tensor, conductivity tensor Electron capture cross section Hole capture cross section Polarization charge density (per area) Lifetime, time constant Electron (minority carrier) lifetime Nonradiative lifetime Hole (minority carrier) lifetime Radiative lifetime Debye temperature Phase Photon flux Electron afﬁnity, electric susceptibility Light extraction efﬁciency Electron afﬁnity (of semiconductor) Envelope wavefunction Angle Wavefunction Angular frequency Longitudinal optical phonon frequency Plasma frequency Transverse optical phonon frequency Interaction parameter Hydrostatic deformation potential, lattice constant Accelaration Area, bandimpurity recombination coefﬁcient Vector potential Richardson constant (Cubic) lattice constant Bowing parameter, deformation potential
Symbols
b B B, B c C Cn , C p Cij , Cijkl d di D D, D D De ðEÞ Dh ðEÞ Dn Dp e ei E E, E EA EAb EC Exc ED EDb EF EFn EFp Eg Ei Em EP EV Evac EX EXb EXX f F F, F FðMÞ FB fe
xxxv
Burger’s vector Bimolecular recombination coefﬁcient, bandwidth Magnetic induction ﬁeld Velocity of light in vacuum, lattice constant (along caxis) Capacitance, spring constant, Auger recombination coefﬁcient Auger recombination coefﬁcient Elastic constants Distance, shear deformation potential Insulator thickness Density of states, diffusion coefﬁcient Electric Displacement ﬁeld Detectivity Electron density of states Hole density of states Electron diffusion coefﬁcient Hole diffusion coefﬁcient Elementary charge Strain components (Voigt notation) Energy, electric ﬁeld Electric ﬁeld Energy of acceptor level Acceptor ionization energy Energy of conductionband edge Exchange interaction energy Energy of donor level, Dirac energy (in graphene) Donor ionization energy Fermi energy Electron quasiFermi energy Hole quasiFermi energy Band gap Intrinsic Fermi level Maximum electric ﬁeld Energy parameter Energy of valenceband edge Energy of vacuum level Exciton energy Exciton binding energy Biexciton energy Oscillator strength Free energy Force Excess noise factor Schottky barrier height Fermi–Dirac distribution function (for electrons)
xxxvi
fi fh Fn Fp FP g G G, G gm Gth h H H, H h i I ID Is Isc Ithr j js jthr k k kB kF l L L LD Lz m m0 m mij mc M M, M me mh mj ml mr
Symbols
Ionicity Fermi–Dirac distribution function for holes (¼ 1 fe ) Electron quasiFermi energy Hole quasiFermi energy Purcell factor Degeneracy, gfactor, gain Free enthalpy, generation rate Reciprocal lattice vector Transconductance Thermal generation rate Planck constant Enthalpy, Hamiltonian Magnetic ﬁeld h=ð2πÞ Imaginary number Current, light intensity Drain current Saturation current Short circuit current Threshold current Current density, orbital momentum Saturation current density Threshold current density Wavenumber, Boltzmann constant Wavevector Boltzmann constant Fermi wavevector Angular orbital momentum Length of line element Line vector (of dislocation) Diffusion length Quantumwell thickness Mass Free electron mass Effective mass Effective mass tensor Cyclotron mass Mass, multiplication factor Magnetization Effective electron mass Effective hole mass Magnetic quantum number Longitudinal mass Reduced mass
Symbols
mt n n NðEÞ n NA Nc NC ND ni nif nr ns Nt ntr nthr NV p p, p P P, P pcv pi q q, q Q r r R Rλ R rH RH s S Sij , Sijkl t tox T u U unk v, v
xxxvii
Transverse mass Electron concentration (in conduction band), ideality factor Normal vector Number of states Complex index of refraction (¼ nr þ iκ) Acceptor concentration Critical doping concentration Conductionband edge density of states Donor concentration Intrinsic electron concentration Ideality factor due to image force effect Index of refraction (real part) Sheet electron density Trap concentration Transparency electron concentration Threshold electron concentration Valenceband edge density of states Pressure, free hole density Momentum Power Electric polarization Momentum matrix element Intrinsic hole concentration Charge Heat flow Charge, quality factor, impuritybound exciton localization energy Radius Spatial coordinate Resistance, radius, recombination rate Responsivity Vector of direct lattice Hall factor Hall coefﬁcient spin Entropy, Seebeck coefﬁcient, total spin, surface index, surface recombination velocity Stiffness coefﬁcients Time (Gate) oxide thickness temperature Displacement, cellinternal parameter energy Bloch function Velocity
xxxviii
V VðλÞ Va VA Vbi vg VG Voc VP vs VSD vth w wB Wm X Y Z
Symbols
Volume, voltage, potential (Standardized) sensitivity of human eye Unitcell volume Early voltage Builtin voltage Group velocity Gate voltage Open circuit voltage Pinchoff voltage Velocity of sound, driftsaturation velocity Sourcedrain voltage Thermal velocity Depletionlayer width, width Base width (bipolar transistor) (Metal) work function Electronegativity Young’s modulus, CIE brightness parameter Partition sum, atomic order number
Physical Constants
Constant
Symbol
Numerical value
Unit
Speed of light in vacuum
c0
2:99792458 108
ms1
Permeability of vacuum
μ0
7
Elementary charge
0 ¼ e
Electron mass
me
Permittivity of vacuum
Planck constant
Boltzmann constant
NA2
4π 10 ðμ0 c20 Þ1
8:854187817 10
12
1:60217733 1019
Fm1 C
31
kg
34
9:1093897 10
h
6:6260755 10
Js
h ¼ h=ð2πÞ
1:05457266 1034
Js
h
6:582122 1016
eV s
1:380658 10
23
JK1
5
kB
vonKlitzing constant Rydberg constant Bohr radius
RH
8:617385 10 25812:8056 13.6056981
aB
5:29177249 1011
meVK1 Ω eV m
Avogadro constant
NA
6:0221418 1023
mol1
xxxix
Chapter 1
Introduction
The proper conduct of science lies in the pursuit of Nature’s puzzles, wherever they may lead. J.M. Bishop [2]
Abstract Important dates and events in the history of semiconductors are chronologically listed, from the early days (Volta, Seebeck and Faraday) to the latest achievements like the blue and white LED. Many known and not so well known scientists are mentioned. Also a list of semiconductor related Nobel prizes and their winners is given.
The historic development of semiconductor physics and technology began in the second half of the 19th century. Interesting discussions of the history of the physics and chemistry of semiconductors can be found in [3–5]. The development of crystal growth is covered in [6]. The history of semiconductor industry can be followed in [7, 8]. In 1947, the commercial realization of the transistor was the impetus to a fastpaced development that created the electronics and photonics industries. Products founded on the basis of semiconductor devices such as computers (CPUs, memories), opticalstorage media (lasers for CD, DVD), communication infrastructure (lasers and photodetectors for opticalfiber technology, high frequency electronics for mobile communication), displays (thin film transistors, LEDs), projection (laser diodes) and general lighting (LEDs) are commonplace. Thus, fundamental research on semiconductors and semiconductor physics and its offspring in the form of devices has contributed largely to the development of modern civilization and culture.
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_1
1
2
1 Introduction
1.1 Timetable and Key Achievements In this section early important milestones in semiconductor physics and technology are listed. 1782 A. Volta—coins the phrase ‘semicoibente’ (semiinsulating) which was translated then into English as ‘semiconducting’ [9]. 1821 T.J. Seebeck—discovery of thermopower (electrical phenomena upon temperature difference) in metals and PbS, FeS2 , CuFeS2 [10]. 1833 M. Faraday—discovery of the temperature dependence of the conductivity of Ag2 S (sulphuret of silver, negative dR/dT ) [11]. 1834 J. Peltier—discovery of the Peltier effect (cooling by current) [12]. 1873 W. Smith—discovery of photoconductivity in selenium [13]. Early work on photoconductivity in Se is reviewed in [14, 15]. 1874 F. Braun1 —discovery of rectification in metal–sulfide semiconductor contacts [17], e.g. for CuFeS2 and PbS. The current through a metal–semiconductor contact is nonlinear (as compared to that through a metal, Fig. 1.1), i.e. a deviation from Ohm’s law. Braun’s structure is similar to a MSM diode. 1876 W.G. Adams and R.E. Day—discovery of the photovoltaic effect in selenium [18]. W. Siemens—large response from selenium photoconductor [19], made by winding two thin platinum wires to the surface of a sheet of mica, and then covering the surface with a thin film of molten selenium. Resistance ratio between dark and illuminated by sunlight was larger than ten [19] and measured to 14.8 in [20]. 1879 E.H. Hall—measurement of the transverse potential difference in a thin gold leaf on glass [21, 22]. Experiments were continued by his mentor H.A. Rowland [23]. A detailed account of the discovery of the Hall efect is given in [24, 25]. 1883 Ch. Fritts—first solar cell, based on an gold/selenium rectifier [20]. The efficiency was below 1 %.
1 F.
Braun made his discoveries on metal–semiconductor contacts in Leipzig while a teacher at the Thomasschule zu Leipzig [16]. He conducted his famous work on vacuum tubes later as a professor in Strasbourg, France.
1.1 Timetable and Key Achievements
3
Fig. 1.1 Current through a silver–CuFeS2 –silver structure as a function of the current through the metal only, 1874. Data points are for different applied voltages. Experimental data from [17]
1901 J.C. Bose—point contact detector for electromagnetic waves based on galena (PbS) [26]. At the time, the term semiconductor was not introduced yet and Bose speaks about ‘substances of a certain class (...) presenting a decreasing resistance to the passage of the electric current with an increasing impressed electromotive force’. 1906 G.W. Pickard—rectifier based on point contact (cat’s whisker) diode on silicon [2729]. Erroneously, the rectifying effect was attributed to a thermal effect, however, the drawing of the ‘thermojunction’ (TJ in Fig. 1.2) developed into the circuit symbol for a diode (cmp. Fig. 21.61a). 1907 H.J. Round—discovery of electroluminescence investigating yellow and blue light emission from SiC [30].
Fig. 1.2 Circuit diagram for a radio receiver with a pointcontact diode (TJ). Adapted from [27]
4
1 Introduction
(001)
(111)
(110)
Fig. 1.3 Laue images of ‘regular’ (cubic) ZnS along three major crystallographic directions, directly visualizing their 4, 3 and 2fold symmetry. Adapted from [41]
K. Bädeker—preparation of metal (e.g. Cd, Cu) oxides and sulfides and also CuI from metal layers using a vapor phase transport method [31].2 CuI is reported transparent (∼200 nm thick films) with a specific resistivity of ρ = 4.5 × 10−2 cm, the first transparent conductor.3 Also CdO (films of thickness 100–200 nm) is reported to be highly conductive, ρ = 1.2 × 10−3 cm, and orangeyellow in color, the first reported TCO (transparent conductive oxide). 1909 K. Bädeker—discovery of doping. Controlled variation of the conductivity of CuI by dipping into iodine solutions (e.g. in chloroform) of different concentrations [34]. 1910 W.H. Eccles—negative differential resistance of contacts with galena (PbS), construction of crystal oscillators [38].4 1911 The term ‘Halbleiter’ (semiconductor) is introduced for the first time by J. Weiss [39] and J. Königsberger and J. Weiss [40]. Königsberger preferred the term ‘Variabler Leiter’ (variable conductor). 1912 M. von Laue—Xray diffraction of bulk crystals including ZnS (Fig. 1.3) [41, 42].
2 This
work was conducted as Habilitation in the Physics Institute of Universität Leipzig. Bädeker became subsequently professor in Jena and fell in WW I. His scientific contribution to semiconductor physics is discussed in [32, 33]. 3 CuI is actually a ptype transparent conductor; at that time the positive sign of the Hall effect [34, 35] could not be interpreted as hole conduction yet. 4 Historical remarks on Eccles’ contributions to radio technology can be found in [36, 37].
1.1 Timetable and Key Achievements
5
Fig. 1.4 Sketch of a fieldeffect transistor, 1926. From [46]
1925 J.E. Lilienfeld5 —proposal of the metalsemiconductor fieldeffect transistor (MESFET) [46], with suggested copper sulfide thin film channel and aluminum gate.6 (Fig. 1.4). Lilienfeld was also awarded patents for a depletion mode MOSFET [48] with proposed copper sulfide, copper oxide or lead oxide channel and current amplification with nppn and pnnptransistors [49]. Due to the lack of other publications of Lilienfeld on transistors, it is under discussion whether Lilienfeld just patented ideas or also build working devices with mounting evidence for the latter [44, 47, 50]. 1927 A. Schleede, H. Buggisch—synthesis of pure, stoichiometric PbS, influence of sulphur excess and impurities [51]. A. Schleede, E. Körner—activation of luminescence of ZnS [52, 53]. 1928 F. Bloch—quantum mechanics of electrons in a crystal lattice, ‘Bloch functions’ [54]. O.V. Losev—description of the light emitting diode7 (SiC) [58]; light emission was observed in forward direction and close to breakdown (Fig. 1.5a). Also current modulation of LED light output was reported (Fig. 1.5b) [58]. 1929 R. Peierls—explanation of positive (anomalous) Hall effect with unoccupied electron states [59, 60].
5 After
obtaining his PhD in 1905 from the FriedrichWilhelmsUniversität Berlin, Julius Edgar Lilienfeld joined the Physics Department of Universität Leipzig and worked on gas liquefaction and with Lord Zeppelin on hydrogenfilled blimps. In 1910 he became professor at the Universität Leipzig where he mainly researched on Xrays and vacuum tubes [43]. To the surprise of his colleagues he left in 1926 to join a US industrial laboratory [44, 45]. 6 In [44] it is suggested that the device works as a npn transistor, in [47] it is suggested to be a JFET. 7 The historic role of Losev regarding the invention of the LED and oscillators is discussed in [55–57].
6
1 Introduction
Fig. 1.5 (a) I –V characteristic of SiC/steel wire light emitting diode. The dotted curve is the flipped curve for negative voltage (3rd quadrant). (b) Recording of current modulated (at 500 Hz) LED on moving photographic plate. Adapted from [58] Fig. 1.6 First band structure calculation (ξ = k a). Adapted from [62]
1930 R. Peierls—first calculation of a band structure and band gap8 (Fig. 1.6) [62]. 1931 W. Heisenberg—theory of hole (‘Löcher’) states [63]. R. de L. Kronig and W.G. Penney—properties of periodic potentials in solids [64]. A.H. Wilson9 —development of bandstructure theory [67, 68]. 8 Peierls performed this work at suggestion of W. Pauli at ETH Zürich. The mathematical problem of Schrödinger’s equation with a sinusoidal potential had been already treated by M.J.O Strutt in 1928 [61]. 9 Wilson was theoretical physicist in Cambridge, who spent a sabbatical with Heisenberg in Leipzig and applied the brand new field of quantum mechanics to issues of electrical conduction,
1.1 Timetable and Key Achievements
7
1933 C. Wagner—excess (‘ElektronenüberschussLeitung’, ntype) and defect (‘ElektronenDefektleitung’, ptype) conduction [69]. Anion deficiency in ZnO causes conducting behavior [70]. 1934 C. Zener—Zener tunneling [71]. 1936 J. Frenkel—description of excitons [72]. 1938 B. Davydov—theoretical prediction of rectification at pnjunction [73] and in Cu2 O [74]. W. Schottky—theory of the boundary layer in metal–semiconductor contacts [75], being the basis for Schottky contacts and fieldeffect transistors. N.F. Mott—metal–semiconductor rectifier theory [76, 77]. R. Hilsch and R.W. Pohl—threeelectrode crystal (KBr) [78]. 1940 R.S. Ohl—Siliconbased photoeffect (solar cell, Fig. 1.7) [79] from a pnjunction formed within a slab of polycrystalline Si fabricated with directed solidification due to different distribution coefficients of p and ndopants (boron and phosphorus, cmp. Fig. 4.6b) (J. Scaff and H. Theurer) [80, 81]. 1941 R.S. Ohl—Silicon rectifier with point contact [82, 83] (Fig. 1.8), building on work from G.W. Pickard (1906) and using metallurgically refined and intentionally doped silicon (J. Scaff and H. Theurer) [80]. 1942 K. Clusius, E. Holz and H. Welker—rectification in germanium [84]. 1945 H. Welker—patents for JFET and MESFET [85]. 1947 W. Shockley, J. Bardeen and W. Brattain fabricate the first transistor in the AT&T
(Footnote 9 continued) first in metals and then in semiconductors. When he returned to Cambridge, Wilson urged that attention be paid to germanium but, as he expressed it long afterward,‘the silence was deafening’ in response. He was told that devoting attention to semiconductors, those messy entities, was likely to blight his career among physicists. He ignored these warnings and in 1939 brought out his famous book ‘Semiconductors and Metals’ [65] which explained semiconductor properties, including the muchdoubted phenomenon of intrinsic semiconductivity, in terms of electronic energy bands. His academic career seems indeed to have been blighted, because despite his great intellectual distinction, he was not promoted in Cambridge (he remained an assistant professor year after year) [66]. Compare the remark of W. Pauli (p. 205).
8
1 Introduction
(b)
ptype (Si:B)
ntype (Si:P)
(a)
1mm
Fig. 1.7 (a) Optical image of directionally solidified silicon. The lower part contains predominantly boron, the upper part contains predominantly phosphorous. First the growth is porous and subsequently columnar. Adapted from [80]. (b) Spectral response of silicon pnjunction photoelement, 1940. The inset depicts schematically a Si slab with builtin pnjunction formed during directed solidification as shown in panel (a). The arrow denotes the direction of solidification (cmp. Fig. 4.6). Adapted from [79] Fig. 1.8 Characteristics of a silicon rectifier, 1941. Adapted from [82]
Bell Laboratories, Holmdel, NJ in an effort to improve hearing aids [86].10 Strictly speaking the structure was a pointcontact transistor. A 50µm wide slit was cut with a razor blade into gold foil over a plastic (insulating) triangle and pressed with a spring on ntype germanium (Fig. 1.9a) [87]. The surface region of the germanium is ptype due to surface states and represents an inversion layer. The two gold con10 Subsequently, AT&T, under pressure from the US Justice Department’s antitrust division, licensed
the transistor for $25,000. This action initiated the rise of companies like Texas Instruments, Sony and Fairchild.
1.1 Timetable and Key Achievements
(a)
9
(b)
Fig. 1.9 (a) The first transistor, 1947 (length of side of wedge: 32 mm). (b) Cutaway model of a 1948 point contact transistor (‘Type A’) based on ntype bulk Ge (n = 5 × 1014 cm−3 ) and common base circuit diagram. The surface region (∼100 nm depth) of the Ge is ptype due to surface states and represents an inversion layer. The two wires are made from phosphor bronze. Adapted from [88]
tacts form emitter and collector, the largearea back contact of the germanium the base contact [88]. For the first time, amplification was observed [89]. Later models use two close point contacts made from wires with their tips cut into wedge shape (Fig. 1.9b) [88].11 More details about the history and development of the semiconductor transistor can be found in [90], written on the occasion of the 50th anniversary of its invention. 1948 W. Shockley—invention of the bipolar (junction) transistor [91]. 1952 H. Welker—fabrication of III–V compound semiconductors12 [94–97] W. Shockley—description of today’s version of the (J)FET [98].
11 The
setup of Fig. 1.9b represents a common base circuit. In a modern bipolar transistor, current amplification in this case is close to unity (Sect. 24.2.2). In the 1948 germanium transistor, the reversely biased collector contact is influenced by the emitter current such that current amplification ∂ IC /∂ IE for constant UC was up to 2–3. Due to the collector voltage being much larger than the emitter voltage, a power gain of ∼125 was reported [88]. 12 An early concept for III–V semiconductors was developed in [92, 93].
10
1 Introduction
Fig. 1.10 (a) The first integrated circuit, 1958 (germanium, 11 × 1.7 mm2 ). (b) The first planar integrated circuit, 1959 (silicon, diameter: 1.5 mm)
1953 G.C. Dacey and I.M. Ross—first realization of a JFET [99]. D.M. Chapin, C.S. Fuller and G.L. Pearson—invention of the silicon solar cell at Bell Laboratories [100]. A single 2 cm2 photovoltaic cell from Si, Si:As with an ultrathin layer of Si:B, with about 6 % efficiency generated 5 mW of electrical power.13 Previously existing solar cells based on selenium had very low efficiency ( u 0 . The diatomic planes have a stacking order of aAbBaAbB. . . along the [00.1]direction as visualized in Fig. 3.17b. In Fig. 3.20 the different local structural environment of the atoms in the zincblende and wurtzite structure is shown. Many important semiconductors with large band gap crystallize in the wurtzite structure, such as GaN, AlN, InN, [185] ZnO, [186] SiC, [187], CdS und CdSe.
Table 3.3 c/a ratio of various wurtzite semiconductors Material ξ (%) Material ξ(%) Material AlN GaN InN ZnS ZnSe
−2.02 −0.49 −1.35 0.25 0.06
CdS CdSe CdTe MgS MgSe
−0.61 −0.18 0.25 −0.80 −0.67
Listed is ξ = (c/a − ζ0 )/ζ0 . Data based on [184]
CuBr CuCl CuI AgI ZnTe
ξ (%)
Material
ξ (%)
0.43 0.55 0.74 0.12 0.74
BeO ZnO 6HSiC BN MgTe
−0.61 −1.9 0.49 0.74 −0.67
3.4 Important Crystal Structures
(a)
57
(b)
Fig. 3.19 (a) Top view (along the caxis) and (b) side view of the wurtzite structure with the tetragonal bonds indicated. The top (bottom) surface of the depicted structure is termed the Znface, ¯ (00.1) (Oface, (00.1))
Fig. 3.20 Comparison of the tetragonal bonds in the (a) zincblende and (b) wurtzite structure (i: inversion center, m: symmetry plane)
(a)
(b)
3.4.6 Chalcopyrite Structure The chalcopyrite [188] (ABC2 , named after ‘fool’s gold’ CuFeS2 , space group 122, ¯ I42d) structure is relevant for I–III–VI2 (with chalcogenide anions) and II–IV–V2 (with pnictide anions) semiconductors such as, e.g., (Cu,Ag)(Al,Ga,In)(S,Se,Te)2 and (Mg,Zn,Cd)(Si,Ge,Sn)(As,P,Sb)2 . A nonmetallic anion atom (‘C’) is tetrahedrally bonded to two different types of cation atoms (‘A’ and ‘B’) as shown in Fig. 3.21. The local surrounding of each anion is identical, two of both the A and B atoms. The structure is tetragonal. The aspect ratio η = c/(2a) deviates from its ideal value 1; typically η < 1 [189, 190]. If the C atom is in the tetrahedral center of the two A and two B atoms, the bond lengths RAC and RBC of the A–C and B–C bonds, respectively, are equal. Since the ideal A–C and B–C bond lengths dAC and dBC are typically unequal, this structure is strained. The common atom C is therefore displaced along [100] and [010] such
58
3 Crystals
Fig. 3.21 Chalcopyrite structure, red and yellow spheres denote the metal species. The bigger green spheres represent the nonmetal anion
that it is closer (if dAC < dBC ) to the pair of A atoms and further away from the B atoms. The displacement parameter is u=
R2 − R2 1 + AC 2 BC 4 a
(3.8)
and it deviates from the ideal value u 0 = 1/4 for the zincblende structure as listed in Table 3.4 for a number of chalcopyrite compounds. In the chalcopyrite structure RAC = a RBC = a
1 + η2 16 1 2 1 + η2 + . u− 2 16
u2 +
(3.9a) (3.9b)
The minimization of the microscopic strain yields (in first order) [191] 2 2 − dBC 1 3 dAC . u∼ = + 2 2 4 8 dAC + dBC
(3.10)
Compounds with u > u c , u c = 0.265 being a critical displacement parameter, (or u < 1/2 − u c = 0.235) are stable with regard to cation disorder [190]. In Fig. 3.22 the correlation of the calculated value for u according to (3.10) and the experimental values is shown.
3.4 Important Crystal Structures
59
Table 3.4 Lattice nonideality parameters η and u (from (3.10)) of various chalcopyrite compounds and their experimentally observed disorder stability (+/− indicates compound with/without order– disorder (D–O) transition, respectively) η u D–O η u D–O CuGaSe2 CuInSe2 AgGaSe2 AgInSe2 CuGaS2 CuInS2 AgGaS2 AgInS2
0.983 1.004 0.897 0.96 0.98 1.008 0.895 0.955
0.264 0.237 0.287 0.261 0.264 0.236 0.288 0.262
+ + − + + −
ZnSiAs2 ZnGeAs2 CdSiAs2 CdGeAs2 ZnSiP2 ZnGeP2 CdSiP2 CdGeP2
0.97 0.983 0.92 0.943 0.967 0.98 0.92 0.939
0.271 0.264 0.294 0.287 0.272 0.264 0.296 0.288
− + − − + − −
Data from [190]
Fig. 3.22 Experimental values u exp of the displacement parameter for various chalcopyrites versus the calculated value u calc according to (3.10). The dashed line indicates u exp = u calc . Adapted from [191]
3.4.7 Spinel Structure A large variety of ternary compounds of type AII BIII 2 CVI 4 crystallize in the cubic spinel structure (spinel, MgAl2 O4 , space group 227, Fd3m). Typical elements are A: Mg, Cr, Mn, Fe, Co, Ni, Cu, Zn, Cd, Sn, B: Al, Ga, In, Ti, V, Cr, Mn, Fe, Co, Rh, Ni, and C: O, S, Se, Te. As an example ZnGa2 O4 (zinc gallate) has received attention as interfacial layer in ZnO/GaAs epitaxy [192], luminescent material [193], and as ferromagnetic semiconductor [194]. Also the (unwanted) appearance of zinc gallate inclusions is in
60
3 Crystals
Fig. 3.23 Spinel AB2 C4 crystal structure, the cations are depicted as yellow (A atoms) and silver (B atoms) spheres, the anions (C atoms) as blue spheres
competition with the formation of highly doped wurtzite ZnO:Ga; in the (normal) spinel cubic structure of ZnGa2 O4 the Zn2+ ions still occupy tetrahedral sites, but the Ga3+ ions occupy octahedral sites instead of tetrahedral sites in doped wurtzite ZnO:Ga. (Sc,Al)MgO4 (SCAM) is available as substrate material. Also AVI BII 2 CVI 4 compounds exist, e.g., GeB2 O4 (with B = Mg, Fe, Co, Ni) The anion atoms (C2− ) sit on a fcc lattice. The A atoms fill 1/8 of all tetraeder spaces and the B atoms fill half of all octaeder places (Fig. 3.23). Often the cations are charged A2+ and B3+ , e.g., in ZnAl2 O4 , MgCr2 O4 or ZnCo2 O4 . Also A6+ and B1− exists, e.g., in WNa2 O4 . The cubic lattice constant is denoted as a. In real spinels, the anions deviate from the ideal fcc array which is accounted for by the parameter u, measuring the displacement of anions along the [111]direction [195]; if the Asite cation is at (0,0,0), an anion is at (u, u, u). The cationanion distances are given by [196] (3.11a) RAC = a 3 (u − 1/8), (3.11b) RBC = a 3 u 2 − 2 u − 3/8. The ideal value is u = 1/4; examples are u = 0.2624 for MgAl2 O4 , u = 0.2617 for ZnGa2 O4 and u = 0.2409 for SiFe2 O4 [196]. In the inverted spinel structure, for AII BIII 2 CVI 4 compounds, the cations are distributed like B(AB)C4 , i.e. the B cations occupy tetraeder and octaeder places, e.g., 2− 3+ 2+ 3+ in Mg2+ (Mg2+ Ti4+ )O2− 4 or Fe (Ni Fe )O4 . Examples are magnetite (Fe3 O4 ), a material with high spin polarization, or MgFe2 O4 . Also AVI BII 2 CVI 4 compounds exist in this structure, e.g., SnB2 O4 (with B = Mg, Mn, Co, Zn), TiB2 O4 (with B = Mg, Mn, Fe, Co, Zn), and VB2 O4 (with B = Mg, Co, Zn).
3.4 Important Crystal Structures
61
Fig. 3.24 Fluorite crystal structure, the cations are depicted as red spheres, the anions as blue spheres
3.4.8 Fluorite Structure Named after the minerale fluorite (CaF2 , space group 225, Fm3m), this structure for binary ionic compounds occurs when the cation valence is twice the anion valence, e.g., for (cubic) ZrO2 (zirconia) or HfO2 . The lattice is fcc with a triatomic base. At (0,0,0) is the cation (e.g., Zr4+ ), the anions (e.g., O2− ) are at (1/4, 1/4, 1/4) a (as in the zincblende structure) and (3/4, 3/4, 3/4) a (Fig. 3.24). The anion atom positions are on a simple cubic lattice with lattice constant a/2. Zirconia can crystallize in various phases [197], the most prominent being the monoclinic, tetragonal and cubic phases. The cubic phase can be extrinsically stabilized using yttrium [198, 199] (YSZ, yttriastabilized zirconia). Hafnium oxide has the remarkable property that the HfO2 /Si interface is stable and allows the fabrication of transistor gate oxides with high dielectric constant (see Sect. 24.5.5).
3.4.9 Delafossite Structure The I–III–O2 materials crystallize in the trigonal delafossite (CuFeO2 , space group ¯ 166, R3m) structure (Fig. 3.25). This structure is also called caswellsilverite (NaCrS2 ). In Table 3.5 the lattice parameters of some delafossite compounds are given. The (Cu, Ag) (Al, Ga, In)O2 materials are transparent conductive oxides (TCO). We note that Pt and Pd as groupI component create metallike compounds because of the d9 configuration as opposed to the d10 configuration of Cu and Ag.
3.4.10 Perovskite Structure The perovskite structure for ABO: 3 materials (calcium titanate, CaTiO3 , space group 62, Pnma) (Fig. 3.26) is relevant for ferroelectric semiconductors (cf. Sect. 15.3). It is cubic with the Ca (or Ba, Sr) ions (charge state 2+) on the corners of the
62
3 Crystals
Ga Cu O ES
c
DB ES 2uc
a
Fig. 3.25 Hexagonal unit cell of delafossite CuGaO2 . Oxygen atoms are bonded to the Cu in a dumbbell (‘DB’) configuration. In the edgesharing (‘ES’) layer the Ga atoms are octahedrally configured as GaO6 Table 3.5 Lattice parameters a, c, and u of some delafossite compounds a (nm) c (nm) u (nm) CuAlO2 CuGaO2 CuInO2
0.2858 0.2980 0.3292
1.6958 1.7100 1.7388
0.1099 0.1073∗ 0.1056∗
Theoretical values are shown with asterisk. Data from [200]
cube, the O ions (2−) on the face centers and the Ti (4+) in the body center. The lattice is simple cubic, the base is Ca at (0, 0, 0), O at (1/2, 1/2, 0), (1/2, 0, 1/2) and (0, 1/2, 1/2) and Ti at (1/2, 1/2, 1/2). The ferroelectric polarization is typically evoked by a shift of the negatively and positively charged ions relative to each other. LaAlO3 (lanthanium aluminate) is available as substrate material (space group 226, ¯ [201]). Perovskites are also important for high temperature superconductivity. Fm3c
3.4.11 NiAs Structure The NiAs structure (space group 194, P63 /mmc) (Fig. 3.27) is relevant for magnetic semiconductors, such as MnAs, and also occurs in the formation of Ni/GaAs Schottky contacts [202]. The structure is hexagonal. The arsenic atoms form a hcp structure and are trigonal prismatically configured with six nearest metal atoms. The metal atoms form hcp planes and fill all octahedral holes of the As lattice. For a cubic close
3.4 Important Crystal Structures
63
(a)
(b)
O
O 2
Ba Ti 4+ Ti
Ba2+
Fig. 3.26 Perovskite structure (BaTiO3 ), (a) A cell with 12fold (cuboctahedrally) configured Ba, (b) B cell with octahedrally configured Ti
Fig. 3.27 NiAs structure, metal atoms: dark grey, chalcogenide atoms: light grey
packed, i.e. fcc, structure this would correspond to the rocksalt crystal. The stacking is ABACABAC… (A: Ni, B,C: As).
3.4.12 Further Structures There are many other crystal structures that have relevance for semiconductor materials. Among them are the ¯ occurring, e.g., for sapphire • corundum structure (Al2 O3 , space group 167, R3c) substrates used in epitaxy or for gallium oxide αGa2 O3 (Ga2 O3 is a multiphase material [203]) ¯ (see Fig. 20.3) • bixbyite structure (In2 O3 , δGa2 O3 , space group 206, Ia3) • βGa2 O3 monoclinic structure (space group 12, C2/m) • quartz (SiO2 ) structures, αquartz (space group 154, P32 21) and βquartz (space group 180, P62 22)
64
3 Crystals
Space does not permit to discuss these and other structures in more detail here. The reader should refer to textbooks on crystallography, e.g., [204–206], and space groups [171, 207]. A good source for information and images of crystal structures on the web is [208].
3.5 Polytypism In polytype materials the stacking order is not only hcp or fcc but takes different sequences, such as, e.g., ACBCABAC as the smallest unit cell along the stacking direction. A typical example is SiC, for which in addition to hcp and fcc 45 other stacking sequences are known. The largest primitive unit cell of SiC [187] contains 594 layers. Some of the smaller polytypes are sketched in Fig. 3.28. In Fig. 3.29 cubic
C
(a)
A
C
B
B
A 2H wurtzite
A 3C zincblende
C
B
C
B
C
B
B
A
B
C
C
A
C
A
A
A
B
A
B
C
C
B
A
B
A
C
A
B
A
A
B
4H 6H
Zn S
B C A C B C
A
A
8H
B
10H
A
(b)
15R
Fig. 3.28 (a) Polytypes of the zincblende and wurtzite lattice (found in SiC), the letters A, B and C denote the three possible positions of the diatomic layers (see Fig. 3.12). (b) High resolution TEM image of 6HSiC. For the enlarged view on the left, the unit cell and the stacking sequence are indicated. Adapted from [209]
3.5 Polytypism
65
Fig. 3.29 Polytypes of diamond found in crystallites (metastable phases in silicon). (a) cubic type (3C) with stacking ABC, inset shows a diffractogram and the alignment of the C and Si lattice, (b) rhombohedral 9R crystallite with ABCBCACABA stacking, (c) 9R phase with interface to a hexagonal 2H (AB stacking) phase. Reprinted with permission from Nature [210], © 2001 Macmillan Magazines Limited
(a)
(b)
Fig. 3.30 (a) Hexagonality index α (3.12) of Zn1−x Cdx S for various ternary compositions. Dashed line is a guide to the eye. (b) Regions of different polytypes in ZnSex S1−x . Adapted from [211]
diamond crystallites and metastable hexagonal and orthorhombic phases (in silicon) are shown. For the ternary alloy (cf. Sect. 3.7) Zn1−x Cdx S the numbers n h of diatomic layers with hexagonal stacking (AB) and n c of layers with cubic stacking (ABC) have been investigated. CdS has wurtzite structure and ZnS mostly zincblende structure. The hexagonality index α as defined in (3.12) is shown in Fig. 3.30 for Zn1−x Cdx S α=
nh . nh + nc
(3.12)
66
3 Crystals
3.6 Reciprocal Lattice The reciprocal lattice is of utmost importance for the description and investigation of periodic structures, in particular for Xray diffraction [212], surface electron diffraction, phonons and the band structure. It is the quasiFourier transformation of the crystal lattice. The crystal lattice is also called the direct lattice, in order to distinguish it from the reciprocal lattice.
3.6.1 Reciprocal Lattice Vectors When R denotes the set of vectors of the direct lattice, the set G of the reciprocal lattice vectors is given by the condition5 exp (i G · R) = 1
(3.13)
for all R ∈ R and G ∈ G. Therefore, for all vectors r and a reciprocal lattice vector G exp (i G · (r + R)) = exp (i G · r) . (3.14) Each Bravais lattice has a certain reciprocal lattice. The reciprocal lattice is also a Bravais lattice, since when G1 and G2 are two reciprocal lattice vectors, then this is obviously true also for G1 + G2 . For the primitive translation vectors a1 , a2 and a3 of the direct lattice, the vectors b1 , b2 and b3 that span the reciprocal lattice can be given directly as 2π (a2 × a3 ) Va 2π b2 = (a3 × a1 ) Va 2π b3 = (a1 × a2 ), Va b1 =
(3.15a) (3.15b) (3.15c)
where Va = a1 · (a2 × a3 ) is the volume of the unit cell spanned by the vectors ai . The volume of the unit cell in the reciprocal space is Va∗ = (2π)3 /Va . The vectors bi fulfill the conditions ai · b j = 2π δi j .
(3.16)
Thus, it is clear that (3.13) is fulfilled. For an arbitrary reciprocal lattice vector G = k1 b1 + k2 b2 + k3 b3 and a vector R = n 1 a1 + n 2 a2 + n 3 a3 in direct space 5 The
dot product a · b of two vectors shall also be denoted as ab.
3.6 Reciprocal Lattice
67
we find G · R = 2π (n 1 k1 + n 2 k2 + n 3 k3 ) .
(3.17)
The number in brackets is an integer. Additionally, we note that the reciprocal lattice of the reciprocal lattice is again the direct lattice. The reciprocal lattice of the fcc is bcc and vice versa. The reciprocal lattice of hcp is hcp (rotated by 30◦ with respect to the direct lattice). For later, we note two important theorems. A (sufficiently well behaved) function f (r) that is periodic with the lattice, i.e. f (r) = f (r + R) can be expanded into a Fourier series with the reciprocal lattice vectors according to f (r) =
aG exp (i G · r),
(3.18)
where aG denotes the Fourier component of the reciprocal lattice vector G, aG =
f (r) exp (−i G · r) d3 r. If f (r) is lattice periodic, the integral given in (3.19) is V zero unless G is a reciprocal lattice vector.
f (r) exp (−i G · r) d3 r = V
aG . 0, G ∈ /G
(3.19)
3.6.2 Miller Indices A lattice plane is the set of all lattice points in a plane spanned by two independent lattice vectors R1 and R2 . The lattice points on that plane form a twodimensional Bravais lattice. The entire lattice can be generated by shifting the lattice plane along its normal n = (R1 × R2 )/R1 × R2 . The plane belongs to the reciprocal lattice vector Gn = 2πn/d , d being the distance between planes. This correspondence between reciprocal lattice vectors and sets of planes allows the orientation of planes to be described in a simple manner. The shortest reciprocal lattice vector perpendicular to the plane is used. The coordinates with respect to the primitive translation vectors of the reciprocal space bi form a triplet of integer numbers and are called Miller indices [213]. The plane described by Gn · r = A fulfills the condition for a suitable value of A. The plane intersects the axes ai at the points x1 a1 , x2 a2 and x3 a3 . Thus we find Gn xi ai = A for all i. From (3.17) follows Gn · a1 = 2π h, Gn · a2 = 2π k and Gn · a3 = 2π l, where h, k and l are integers. The triplet of integer numbers (hkl), the reciprocal values of the axis intersections in the direct lattice, are the Miller indices. An example is shown in Fig. 3.31. Planes are denoted as (hkl) with parentheses. The (outward) normal direction is denoted with [hkl] (square brackets). A set of equivalent planes is denoted with curly brackets as {hkl}. For example, in the simple cubic lattice (100), (010), (001),
68
3 Crystals
Fig. 3.31 The plane intersects the axes at 3, 2, and 2. The inverse of these numbers is 1/3, 1/2, and 1/2. The smallest integer numbers of this ratio form the Miller indices (233)
(−100), (0−10) are (00−1) equivalent and are denoted by {100}. (−100) can also ¯ be written as (100). A set of equivalent directions is denoted with hkl. In a cubic lattice the faces of the cubic unit cell are {001} and the planes perpendicular to the area (body) diagonals are {110} ({111}) (Fig. 3.32a). In the zincblende lattice the {111} planes consist of diatomic planes with Zn and S atoms. It depends on the direction whether the metal or the nonmetal is on top. These two cases are denoted by A and B. We follow the convention that the (111) plane is (111)A and the metal is on top (as in Fig. 3.16b). For each change of sign the type changes from ¯ A to B and vice versa, e.g., (111)A, (11¯ 1)B and (1¯ 1¯ 1)B. In Fig. 3.32b the inplane directions for the (001), (110) and (111) planes are visualized. In the wurtzite lattice the Miller indices are denoted as [hklm] (Fig. 3.33). Within the (0001) plane three indices hkl are used that are related to the three vectors a1 , a2 and a3 (see Fig. 3.33a) rotated with respect to each other by 120◦ . Of course, the four indices are not independent and l = −(h + k). The third (redundant) index can be denoted as a dot. The caxis [0001] is then denoted as [00.1]. Wurtzite (and trigonal, e.g., sapphire) substrates are available typically with a (11.0), r (01.2), m (01.0) and c ([00.1]) surface orientations (Fig. 3.33b). The distance of lattice planes d = 2π/G can be expressed via the Miller indices for cubic (3.20a), tetragonal (3.20b) and hexagonal (3.20c) crystals as c = √ dhkl t dhkl = h dhkl =
a h2 + k2 + l 2 a
h 2 + k 2 + l 2 (a/c)2 a 4 (h 2 + hk + k 2 )/3 + l 2 (a/c)2
(3.20a) (3.20b) (3.20c)
3.6 Reciprocal Lattice
69
(a)
(b)
(110)
(001)
[110] [010]
[110]
[111]
[001] [112] [111]
[100]
[100]
[110]
[110]
[110] [001]
[110]
[111]
[001]
[111]
(111) [112] [211]
[121] [110]
[110]
[211]
[112]
[121]
Fig. 3.32 (a) Miller indices of important planes for the simple cubic (and fcc, bcc) lattice. (b) Directions within three low index planes of cubic crystals
(a)
(b) [2110] [1010]
(00.1) [1100]
[1120]
[1210] [0110] [1120]
[0110] [1010] [1210] [1100] [2110]
(c)
a
r
m
c
Fig. 3.33 (a, b) Miller indices for the wurtzite (or hcp) structure. (c) Orientation of the a, r, m, and cplane in the wurtzite structure
70
3 Crystals
Table 3.6 High symmetry points and directions from Γ point in the Brillouin zone of the fcc lattice Point k Direction (0 ≤ λ ≤ 1) Γ X K L W U
(0,0,0) 2π a (0, 1, 0) 3π 2 a (1, 1, 0) π a (1, 1, 1) 2π a (1, 1/2, 0) 2π a (1, 1/4, 1/4)
2π a (0, λ, 0) 3π 2 a (λ, λ, 0) π a (λ, λ, λ)
Δ Σ Λ
Table 3.7 High symmetry points and directions from Γ point in the Brillouin zone of the hcp lattice Point k Direction (0 ≤ λ ≤ 1) Γ A L
(0,0,0) 2 π (0, 0, 21c ) 2 π (0, √1 , 21c )
Δ
π c
M
2 π (0,
Σ
√2 π 3a
T
2 π (− 3λa ,
H K
3a √1 , 0) 3a 2 π (− 31a , √1 , 21c ) 3a 2 π (− 31a , √1 , 0) 3a
(0, 0, λ) (0, λ, 0) √λ , 0) 3a
Useful formulas for the angle θ between a (hk.l)plane and the [00.1]direction in the cubic, tetragonal and wurtzite structures are: cos θc = √
l h2
(3.21a)
+ k2 + l2 l
cos θt = l2 + cos θh = l2 +
c2 (h 2 a2
l c2
4 3 a2
(3.21b)
+ k2)
(h 2 + hk + k 2 )
.
(3.21c)
3.6.3 Brillouin Zone The Wigner–Seitz cell in reciprocal space is called the (first) Brillouin zone. In Fig. 3.34, the Brillouin zones for the most important lattices are shown. Certain points in the Brillouin zone are labeled with dedicated letters. The Γ point always denotes k = 0 (zone center). Certain paths in the Brillouin zone are labeled with dedicated Greek symbols.
3.6 Reciprocal Lattice
71 kz
kz
(a)
X
X
(b)
W
R
L U
S T M
Z
X
ky
ky
K
kx
kx
H
(c)
kz
(d)
P
H
F D kx
ky
N
G
L R A
S
L
P K
H
M
S' H
U
P
T M
H
T'
A L kz
X
(e)
K
H
(f) Z
T
T
U Y
N
X
ky
S
kx Fig. 3.34 Brillouin zones and special k points for the (a) primitive cubic (pc), (b) fcc, (c) bcc, and (d) hcp lattice. (e) Brillouin zone for chalcopyrite structure with fcc Brillouin zone shown as dashed outline. (f) Brillouin zone for orthorhombic lattice with one quadrant shown with dashed lines.
72
3 Crystals
In the Brillouin zone of the fcc lattice (Si, Ge, GaAs, …) the X point denotes the point at the zone boundary in 001directions (at distance 2 π/a from Γ ), K for √ 2 a from Γ ) and L for the 111directions (at 110directions (at distance 3 π/ √ distance 3 π/a from Γ ) (see Table 3.6). The straight paths from Γ to X, K, and L are denoted as Δ, Σ, and Λ, respectively. High symmetry points and directions of the Brillouin zone of the hcp lattice are given in Table 3.7.
3.7 Alloys When different semiconductors are mixed various cases can occur: • The semiconductors are not miscible and have a socalled miscibility gap. They will tend to form clusters that build up the crystal. The formation of defects is probable. • They form an ordered (periodic) structure that is called a superlattice. • They form a random alloy.
3.7.1 Random Alloys Alloys for which the probability to find an atom at a given lattice site is given by the fraction of these atoms (i.e. the stoichiometry), independent of the surrounding, are called random alloys. Deviations from the random population of sites is termed clustering. For a Gex Si1−x alloy this means that any given atom site has the probability x to have a Ge atom and 1 − x to have a Si atom. The probability pn that a Si atom has n nextneighbor Ge atoms is 4 n x (1 − x)4−n , pn = n
(3.22)
and is depicted in Fig. 3.35 as a function of the alloy composition. The symmetry of the Si atom is listed in Table 3.8. If it is surrounded by four of the same atoms (either Ge or Si), the symmetry is Td . If one atom is different from the other three next neighbors, the symmetry is reduced to C3v since one bond is singled out. For two atoms each the symmetry is lowest (C2v ). In an alloy from binary compound semiconductors such as Alx Ga1−x As the mixing of the Al and Ga metal atoms occurs only on the metal (fcc) sublattice. Each As atom is bonded to four metal atoms. The probability that it is surrounded by n Al atoms is given by (3.22). The local symmetry of the As atom is also given by Table 3.8. For AlAsx P1−x the mixing occurs on the nonmetal (anion) sublattice. If the alloy ¯ surface contains three atom species it is called a ternary alloy. In Fig. 3.36 the (110)
3.7 Alloys
73
Fig. 3.35 Probability that a Si atom has n nextneighbor Ge atoms in a random Gex Si1−x alloy
Table 3.8 Probability pn (3.22) and symmetry of an A atom being surrounded by n B atoms in a tetrahedrally configured Bx A1−x random alloy
n
pn
Symmetry
0 1 2 3 4
x4
Td C3v C2v C3v Td
4 x 3 (1 − x) 6 x 2 (1 − x)2 4 x (1 − x)3 (1 − x)4
(UHV cleave) of an In0.05 Ga0.95 As alloy is shown. Indium atoms in the first layer show up as brighter round dots [214]. Along the [001]direction the positions are uncorrelated, along [110] an anticorrelation is found, corresponding to an effective repulsive pair interaction energy of 0.1 eV for the nearest neighbor In–In pairs along the [110]direction due to strain effects [215]. If the binary end components have different crystal structure, the alloy shows a transition (or compositional transition range) from one structure to the other at a particular concentration. An example is the alloy between wurtzite ZnO and rocksalt MgO. Mgx Zn1−x O alloy thin films exhibits wurtzite structure up to about x = 0.5 and rocksalt structure for x > 0.6 [216] (cmp. Fig. 3.39). If the alloy contains four atom species it is called quaternary. A quaternary zincblende alloy can have the mixing of three atom species on one sublattice, such as Alx Ga y In1−x−y As or GaAsx P y Sb1−x−y or the mixing of two atom species on both of the two sublattices, such as Inx Ga1−x As y N1−y . The random placement of different atoms on the (sub)lattice in an alloy represents a perturbation of the ideal lattice and causes additional scattering (alloy scattering). In the context of cluster formation, the probability of an atom having a direct neighbor of the same kind on its sublattice is important. Given a Ax B1−x C alloy, the probability pS to find a single A atom surrounded by B atoms is given by (3.23a). The probability
74
3 Crystals
(a)
(b)
(c)
¯ surface of an MBEgrown Fig. 3.36 (a) STM emptystate image (17.5 × 17.5 nm2 ) of the (110) In0.05 Ga0.95 As alloy on GaAs, (b) curvatureenhanced image. (c) Schematic atomic arrangement of the first and second atomic layer. Adapted from [215]
pD1 to find a cluster of two neighbored A atoms surrounded by B atoms is given by (3.23b). pS = (1 − x)12 pD1 = 12 x (1 − x)18 .
(3.23a) (3.23b)
These formulas are valid for fcc and hcp lattices. For larger clusters [217, 218], probabilities in fcc and hcp structures differ.
3.7.2 Phase Diagram The mixture Ax B1−x with average composition x between two materials A and B can result in a single phase (alloy), a twophase system (phase separation) or a metastable system. The molar free enthalpy ΔG of the mixed system is approximated by ΔG = Ω x (1 − x) + kT [x ln(x) + (1 − x) ln(1 − x)] .
(3.24)
The first term on the righthand side of (3.24) is the (regular solution) enthalpy of mixing with the interaction parameter Ω, which can depend on x. The second term is the ideal configurational entropy based on a random distribution of the atoms. The function is shown for various ratios of kT /Ω in Fig. 3.37a. In an equilibrium phase diagram (see Fig. 3.37b) the system is above the binodal curve in one phase (miscible). On the binodal line Tb (x) in the (x, T ) diagram the A and Brich disordered phases have equal chemical potentials, i.e. ∂G/∂x = 0. For Ω independent of x the temperature Tb is given by (3.25a). A critical point is at the maximum temperature
3.7 Alloys
75
(a)
(b)
Fig. 3.37 (a) Free enthalpy ΔG of mixed binary system (3.24) in units of Ω for Ω = const. and various values of kT /Ω as labeled. (b) Schematic phase diagram for binary mixture. The temperature is given in units of Ω/k. The solid (dashed) denotes the binodal (spinodal) line
(b) 350 AlxGa1xAs
90
Temperature (K)
Temperature (K)
(a)100 80 70
binodal
60 spinodal
50 40 GaAs
x=0.5
AlAs
GaPx As1x
300 250 200 150 100 GaAs
x=0.5
GaP
Fig. 3.38 Calculated phase diagrams for (a) Alx Ga1−x As and (b) GaPx As1−x . The binodal (spinodal) curve is shown as solid (dashed) line. Adapted from [219]
Tmg and concentration xmg of the miscibility gap. For Ω independent of x it is given by Tmg = Ω/2 and xmg = 1/2. In the region below the spinodal boundary, the system is immiscible and phases immediately segregate (by spinodal decomposition). On the spinodal line Tsp (x) the condition ∂ 2 G/∂x 2 = 0 is fulfilled. For Ω independent of x the temperature Tsp is given by (3.25b). The region between the binodal and spinodal curves is the metastable region, i.e. the system is stable to small fluctuations of concentration or temperature but not for larger ones. 2x − 1 ln(x) − ln(1 − x) kTsp (x) = 2Ω x (1 − x). kTb (x) = Ω
(3.25a) (3.25b)
In Fig. 3.38 calculated diagrams for GaAsAlAs and GaAsGaP [219] are shown. The arrows denote the critical point. These parameters and the interaction parameters for a number of ternary alloys are given in Table 3.9. For example, for Alx Ga1−x As
76
3 Crystals
Table 3.9 Calculated interaction parameter Ω(x) (at T = 800 K, 1 kcal/mol= 43.39 meV), miscibilitygap temperature Tmg and concentration xmg for various ternary alloys Alloy
Tmg (K)
xmg
Ω(0) (kcal/mol)
Ω(0.5) (kcal/mol)
Ω(1) (kcal/mol)
Alx Ga1−x As GaPx As1−x Gax In1−x P GaSbx As1−x Hgx Cd1−x Te Znx Hg1−x Te Znx Cd1−x As Inx Ga1−x N
64 277 961 1080 84 455 605 1505
0.51 0.603 0.676 0.405 0.40 0.56 0.623 0.50
0.30 0.53 2.92 4.51 0.45 2.13 2.24 6.32
0.30 0.86 3.07 3.96 0.80 1.88 2.29 5.98
0.30 1.07 4.60 3.78 0.31 2.15 2.87 5.63
Data for (In,Ga)N from [220], other data from [219]
complete miscibility is possible for typical growth temperatures (>700 K), but for Inx Ga1−x N the In solubility at a typical growth temperature of 1100 K is only 6 % [220]. The alloy system (Al,Ga,In)(As,P,Sb) always crystallizes in the zincblende structure and (Al,Ga,In)N always in the wurtzite structure. If the binary end components of a ternary alloy have a different crystal structure things become more complicated and the crystal phase has to be determined experimentally (and modelled) for each composition. As an example the energy of the wurtzite, hexagonal and rocksalt structure of Mgx Zn1−x O has been calculated [221] as depicted in Fig. 3.39 (cmp. Fig. 2.4 for silicon). The transition between wurtzite and rocksalt structure is predicted for x = 0.33. 1.0 0.6
0.9 0.8
0.5
0.7 0.4
0.6 0.5
0.3 0.4 0.3
0.2
0.2 0.1 0.1 0 18
20
24
22 3
Volume (Å )
26
0
Energy (eV)
Mgconcentration x
Fig. 3.39 Calculated energy versus volume of the formula unit for Mgx Zn1−x O in the wurtzite (WZ), hexagonal (HX) and rocksalt phase (RS). The separations between the three phase are denoted by straight bold lines. Adapted from [221]
3.7 Alloys
77
3.7.3 Virtual Crystal Approximation In the virtual crystal approximation (VCA) the disordered alloy ABx C1−x is replaced by an ordered binary compound AD with D being a ‘pseudoatom’ with properties that are configuration averaged over the properties of the B and C atoms, e.g., their masses or charges. Such an average is weighted with the ternary composition, e.g., the mass is MD = x MB + (1 − x)MC . For example, the A–D force constant would be taken as the weighted average over the A–B and A–C force constants.
3.7.4 Lattice Parameter In the VCA for an alloy a new sort of effective atom is assumed that has an averaged bond length that depends linearly on the composition. Typically, Vegard’s law (3.26), which predicts that the lattice constant of a ternary alloy Ax B1−x C depends linearly on the lattice constants of the binary alloys AC and BC, is indeed fulfilled a0 (Ax B1−x C) = a0 (BC) + x [a0 (AC) − a0 (BC)].
(3.26)
In reality, the bond length of the AC and BC bonds changes rather little (Fig. 3.40a) such that the atoms in the alloy suffer a displacement from their average position and the lattice is deformed on the nanoscopic scale. In a lattice of the type Inx Ga1−x As the anions suffer the largest displacement since their position adjusts to the local cation environment. For Inx Ga1−x As a bimodal distribution, according to the As– Ga–As and As–In–As configurations, is observed (Fig. 3.40b). The cation–cation secondneighbor distances are fairly close to the VCA. While the average lattice parameter in alloys changes linearly with composition, the cellinternal parameter u (for wurtzite structures, see Sect. 3.4.5) exhibits a nonlinear behavior as shown in Fig. 3.41. Therefore physical properties connected to u, such as the spontaneous polarization, will exhibit a bowing.
3.7.5 Ordering Some alloys have the tendency for the formation of a superstructure [225]. Growth kinetics at the surface can lead to specific adatom incorporation leading to ordering. For example, in In0.5 Ga0.5 P the In and Ga atoms can be ordered in subsequent (111) planes (CuPt structure) instead of being randomly mixed (Fig. 3.42). This impacts fundamental properties such as the phonon spectrum or the band gap. CuPt ordering ¯ ¯ planes CuPtB ordering. ¯ planes is called CuPtA , on (111) and (111) on (111) and (1¯ 11) In Fig. 3.43, a TEM image of a Cd0.68 Zn0.32 Te epilayer is shown with simultaneous
78
3 Crystals
√ Fig. 3.40 (a) Nearneighbor distance ( 3 a0 /4) of Inx Ga1−x As as measured by standard Xray diffraction (Bragg reflection, solid squares) and VCA approximation (dashdotted line). Nearneighbor Ga–As and In–As distances as determined by EXAFS (extended Xray absorption fine structure, solid squares). Dashed lines are guides to the eye. Data from [222]. (b) Secondneighbor distances for Inx Ga1−x As as determined from EXAFS, top: anion–anion distance (for As–As), bottom: cation–cation distance (for In–In, Ga–Ga, and Ga–In). Solid lines in both plots are the √ VCA (a0 / 2). Data from [223]
Fig. 3.41 Theoretical values (T = 0 K) for the cellinternal parameter u as a function of the composition for groupIII nitride alloys. The solid lines are quadratic curves (bowing parameter b is shown) through the points for x = 0, 0.5, and 1.0. Data from [224]
3.7 Alloys
79
Ga In P
C 3v
Td Disordered or “random” alloy
CuPt ordered
Fig. 3.42 CuPtordered ternary alloy In0.5 Ga0.5 P; the lattice symmetry is reduced from Td to C3v
Fig. 3.43 (a) Crosssectional transmission electron microscope image along the [110] zone axis of a Cd0.68 Zn0.32 Te epilayer on GaAs showing ordered domains having a doublet periodicity on the {111} and {001} lattice planes. Two different {111} variants are labeled ‘a’ and ‘b’. The doublet periodicity in the [001] is seen in the ‘c’ region. (b) Selectedarea diffraction pattern along the [110] zone. Strong peaks are fundamental peaks of the zincblende crystal, weak peaks are due to CuPt ordering, labeled A and B, and CuAuI ordering, labeled C and D. The latter are the weakest due to a small volume fraction of CuAuordered domains. Adapted from [226]
80
3 Crystals [001] [110]
(a)
Cd Zn Se
(b)
(c)
Fig. 3.44 Schematic diagrams of zincblende Cdx Zn1−x Te along [110] with (a) CuAuI type order¯ ing and (b,c) two types of the CuPtB type ordering. Doublet periodicity is along (a) [001] and [110], ¯ and (c) [111]. ¯ (b) [111] Adapted from [226]
¯ and 111 ¯ ) and in the ordering in the CuPt structure (doublet periodicity along 111 ¯ (Fig. 3.44). CuAuI structure6 (doublet periodicity along [001] and [110])
6 The
CuAuI structure has tetragonal symmetry. There exists also the CuAuII structure that is orthorhombic.
Chapter 4
Defects
Abstract No crystal is perfect. Various point defects and their thermodynamics, diffusion and distribution effects are discussed. Also dislocations and extended defects such as cracks, stacking faults, grain boundaries and antiphase domains are covered.
4.1 Introduction In an ideal lattice each atom is at its designated position. Deviations from the ideal structure are called defects. In the following, we will briefly discuss the most common defects. The electrical activity of defects will be discussed in Sects. 7.5 and 7.7. f At For the creation (formation) of a defect a certain free enthalpy GfD is necessary. thermodynamical equilibrium a (point) defect density ∝ exp −G D /kT will always be present (cf. Sect. 4.2.2). Point defects (Sect. 4.2) are deviations from the ideal structure involving essentially only one lattice point. The formation energy for line defects (Sect. 4.3) or area defects (Sect. 4.4) scales with N 1/3 and N 2/3 , respectively, N being the number of atoms in the crystal. Therefore, these defects are not expected in thermodynamic equilibrium. However, the path into thermodynamical equilibrium might be so slow that these defects are metastable and must be considered quasifrozen. There may also exist metastable point defects. By annealing the crystal, the thermodynamic equilibrium concentration might be reestablished. The unavoidable twodimensional defect of the bulk structure is the surface, discussed in Chap. 11.
4.2 Point Defects 4.2.1 Point Defect Types The simplest point defect is a vacancy V, a missing atom at a given atomic position. If an atom is at a position that does not belong to the crystal structure an interstitial I © Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_4
81
82
4 Defects
Fig. 4.1 Images of occupied (upper frames) and empty (lower frames) density of states of typical defects on Sidoped GaAs (110) surfaces. (a1, a2) show a Ga vacancy, (b1, b2) a SiGa donor, (c1, c2) a SiAs acceptor and (d1, d2) a SiGa –VGa complex. Adapted from [227]
(or Frenkel defect) is formed. Depending on the position of the interstitial different types are distinguished. An interstitial atom that has the same chemical species as the crystal is called ‘selfinterstitial’. If an atom site is populated with an atom of different order number Z , an impurity is present. An impurity can also sit on interstitial position. If the number of valence electrons is the same as for the original (or correct) atom, then it is an isovalent impurity and quasi fits into the bonding scheme. If the valence is different, the impurity adds extra (negative or positive) charge to the crystal bonds, which is compensated by the extra, locally fixed charge in the nucleus. This mechanism will be discussed in detail in the context of doping (Chap. 7). If in an AB compound an A atom sits on the B site, the defect is called an antisite defect A B . A Ga vacancy, a silicon impurity atom on Ga and Assite and a SiGa vacancy complex at the (110) surface of Si doped GaAs are shown in Fig. 4.1 as observed with STM [227, 228]. Also antisite defects in GaAs can be observed with STM [229, 230]. A point defect is typically accompanied by a relaxation of the surrounding host atoms. As an example, we discuss the vacancy in Si (Fig. 4.2a). The missing atom leads to a lattice relaxation with the next neighbors moving some way into the void (Fig. 4.2b). The bond lengths of the next and secondnext neighbor Si atoms around the neutral vacancy are shown in Fig. 4.2c. The lattice relaxation depends on the charge state of the point defect (Jahn–Teller effect) which is discussed in more detail in Sect. 7.7. In Fig. 4.2d the situation for the positively charged vacancy with one electron missing is shown. One of the two bonds is weakened since it lacks an electron. The distortion is therefore different from that for V 0 . Also the (self)interstitial is accompanied with a lattice relaxation as shown in Fig. 4.3 for a silicon interstitial at tetrahedral place. Selfinterstitials in silicon and germanium are reviewed and compared in [231] for their various charge states.
4.2 Point Defects
83
(a)
(b)
(c)
(d)
Fig. 4.2 (a) Schematic diamond lattice with vacancy, i.e. a missing Si atom without relaxation. (b) Si with neutral vacancy (V 0 ), lattice relaxation and formation of two new bonds. (c) Schematic diagram showing the (inward) relaxation of the neighbors around the neutral Si vacancy defect site (empty circle) calculated by an ab initio method. The distances of the outer shell of atoms (red circles) from the vacant site is labeled (in nm). The bond lengths of the two new bonds and the secondneighbor (blue circles) distance are also indicated. The bond length in bulk Si is 0.2352 nm, the secondneighbor distance 0.3840 nm. Adapted from [232]. (d) Si unit cell with positively charged vacancy (V + ). Parts (a, b, d) reprinted with permission from [233] Fig. 4.3 Silicon tetrahedral interstitial SiTi and its next atoms in ideal (white spheres) and relaxed (black spheres) position. Adapted from [155]
4.2.2 Thermodynamics For a given temperature, the free enthalpy G of a crystal (a closed system with regard to particle exchange) G = H − TS (4.1)
84
4 Defects
is minimum. H is the enthalpy and S the entropy. The enthalpy H = E + pV is the thermodynamic potential for a system whose only external parameter is the volume V . It is used when the independent variables of the system are the entropy S and pressure p. The free enthalpy is used when the independent parameters are T and p. G 0 (H0 ) is the free energy (enthalpy) of the perfect crystal. H f is the formation enthalpy of an isolated defect. This could be, e.g., the enthalpy of a vacancy, created by bringing an atom from the (later) vacancy site to the surface, or an interstitial, created by bringing an atom from the surface to the interstitial site. In the limit that the n defects do not interact with each other, i.e. their concentration is sufficiently small, they can be considered independent and the enthalpy is given by H = H0 + n H f .
(4.2)
The increase of entropy due to increased disorder is split into the configurational disorder over the possible sites, denoted as S d , and the formation entropy Sf due to localized vibrational modes. The total change ΔG of the free energy is ΔG = G − G 0 = n (H f − T S f ) − T S d = n G f − T S d ,
(4.3)
where G f = H f − T S f denotes the free enthalpy of formation of a single isolated defect. In Table 4.1 experimental values for the formation entropy and enthalpy are given for several defects. Surprisingly, despite their fundamental importance in semiconductor defect physics, these numbers are not very well known and disputed in the literature. The defect concentration is obtained by minimizing ΔG, i.e. ∂ Sd ∂ΔG = Gf − T = 0. ∂n ∂n
(4.4)
The entropy S d due to disorder is given as S d = kB ln W,
(4.5)
where W is the complexion number, usually the number of distinguishable ways to distribute n defects on N lattice sites Table 4.1 Formation enthalpy H f and entropy S f of the interstitial (I ) and vacancy (V ) in Si and the Ga vacancy in GaAs Material Defect H f (eV) S f (kB ) Si Si GaAs
I V VGa
Data for Si from [234, 235], for GaAs from [236]
3.2 2.8 3.2
4.1 ∼1 9.6
4.2 Point Defects
85
W =
N n
=
N! . n! (N − n)!
(4.6)
With Stirling’s formula ln x! ≈ x(ln x − 1) for large x we obtain ∂ Sd N N −n N = kB ln + ln . ∂n n N −n n
(4.7)
If n N , ∂ N /∂n = 0 and the right side of (4.7) reduces to kB ln(N /n). The condition (4.4) reads G f + kB T ln(n/N ), or Gf n = exp − . (4.8) N kT In the case of several different defects i with a degeneracy Z i , e.g. a spin degree of freedom or several equivalent configurations, (4.8) can be generalized to G if ni = exp − . (4.9) Zi N kT eq
In [237] the equilibrium concentration of interstitials C I in silicon has been given as 3.8 eV eq , C I = 1.0 × 1027 cm−3 exp − kT
(4.10)
about 1014 cm−3 at 1200 ◦ C. The vacancy concentration has been investigated in [238]. Around a temperature of 1200 ◦ C it is in the 1014 –1015 cm−3 range. Due to the reaction 0 I + V,
(4.11)
a mass action law holds for the concentrations of interstitials and vacancies eq
eq
C I CV = C I CV .
(4.12)
4.2.3 Diffusion The diffusion of point defects is technologically very important, in particular for silicon as host material. Typically a dopant profile should be stable under following technological processing steps and also during device performance. Also defect annihilation is crucial after implantation processes. Diffusion of an interstitial I and a
86
4 Defects
Fig. 4.4 The temperature dependent diffusion coefficient of Si interstitials I , vacancies V and various impurities in silicon. Also the selfdiffusion coefficient, labeled with ‘Si’ is shown. Based on data from [239]
vacancy V to the same site is prerequisite for recombination of defects (so called bulk process) according to the scheme I + V → 0. We note that the process 0 → I + V is called Frenkel pair process.1 Also the selfdiffusion of silicon has been studied, e.g. using radioactively marked isotopes [237]. The diffusion of point defects including dopants in silicon has been reviewed in [239, 240]. Usually Fick’s law is applied, stating how the flux J depends on the concentration gradient, for an interstitial it reads: (4.13) JI = −D I ∇C I , D I being the interstitial diffusion coefficient. For interstitials in Si it was found [237] that 1.2 eV (4.14) cm2 /s. D I = 0.2 exp − kT The diffusion of neutral vacancies occurs with [241]
0.45 eV DV = 0.0012 exp − kT
cm2 /s.
(4.15)
The temperature dependent diffusion coefficients of point defects and dopants in silicon are shown in Fig. 4.4. The selfdiffusion coefficient of silicon has been determined from the annealing of isotope superlattices (Sect. 12.5) of sequence 28 Sin /30 Sin , n = 20 to be [242]
1 At
higher temperatures a silicon atom can occasionally acquire sufficient energy from lattice vibrations to leave its lattice site and thus an interstitial and a vacancy are generated.
4.2 Point Defects
(a)
(d)
87
(c)
(b)
(e)
Fig. 4.5 Configurations of boron in Si: (a) Substitutional boron and Si selfinterstitial at ‘T’ site T (BS –SiTi ). Interstitial boron at (b) ‘H’ (BH i ) and (c) ‘T’ site (Bi ), each with the Si atoms on the Si lattice sites. The large bright ball represents the boron atom, large and small dark balls represent Si atoms. (d) Lowest energy barrier diffusion paths for positively charged and neutral B–Si states, total energy versus configuration. (e) Two diffusion pathways for positively charged B–Si, kickout (dashed line) and pair diffusion (solid line); the activation energy is labeled. Adapted from [245]
4.95 eV 3.6 eV SD DSi = 2175.4 exp − + 0.0023 exp − cm2 /s, kT kT
(4.16)
the first (second) term being due to interstitial (vacancy) mechanism, dominant for temperatures larger (smaller) than 900 ◦ C. The enthalpy in the exponent, e.g. HV = 3.6+0.3 −0.1 eV [242], consists of the formation and migration enthalpies, HV = HVf + HVm .
(4.17)
Using the experimental value HVf = 2.8 ± 0.3 eV [235] from Table 4.1, for the migration enthalpy a value around HVm ≈ 0.8 eV is obtained. As an example for a dopant diffusion process that has been understood microscopically, we discuss here boron in silicon. In Fig. 4.5a the lowestenergy configuration of a boronrelated defect in silicon is depicted, Bs –SiTi , i.e. boron on a substitutional site and a selfinterstitial Si on the ‘T’ place with highest symmetry2 (see Fig. 3.18). 2 The
positive charge state is stable, the neutral charge state is metastable since the defect is a negativeU center (see Sect. 7.7.5).
88
4 Defects
Due to its importance as an acceptor in Si, the configuration and diffusion of B in Si has found great interest [243–245]. The diffusion depends on the charge state of boron. The diffusion of positively charged boron has been suggested [245] to occur via the following route: The boron leaves its substitutional site and goes to the hexagonal site (‘H’) (Fig. 4.5b) with an activation energy of about 1 eV (Fig. 4.5d). It can then relax (∼0.1 eV) without barrier to the tetrahedral ‘T’ position (Fig. 4.5c). → BT+ has a higher activation energy of 1.12 eV The direct migration Bs –SiT+ i i and is thus unlikely. The boron atom can then diffuse through the crystal by going from ‘H’ to ‘T’ to ‘H’ and so on (Fig. 4.5e). However, longrange diffusion seems to be not possible in this way because the kickin mechanism will bring back the boron to its stable configuration. The pair diffusion mechanism for neutral boron T Bs –SiTi → BH i → Bs –Sii via the hexagonal site has an activation energy of about 0.5 eV (Fig. 4.5d) while the path via BTi has a larger 0.9 eV barrier. The concentration dependence of the diffusion mechanism has been discussed in [246]. Similarly, indium diffusion in silicon has been investigated suggesting a minimum energy Ins –SiTi → InTi → Ins –SiTi diffusion pathway via the tetrahedral site with 0.8 eV activation energy [247]. Microscopic modeling has been reported also for diffusion of phosphorus [248].
4.2.4 Dopant Distribution The introduction of impurities into a semiconductor (or other materials such as glasses) is termed doping. The unavoidable incorporation of impurities in the nominally pure (nominally undoped) material is called unintentional doping and leads to a residual or background impurity concentration. Several methods are used for doping and the creation of particular doping profiles (in depth or lateral). All doping profiles underly subsequent diffusion of dopants (Sect. 4.2.3). Various methods of doping are used. A straightforward method of doping is the incorporation during crystal growth or epitaxy. For semiconductor wafers a homogeneous doping concentration is targeted, both laterally and along the rod from which the wafer is cut (Sect. 12.2.2). When a crystal is grown from melt, containing a concentration c0 of the impurity, the concentration in the solid is given by (‘normal freezing’ case [249–251])3 c(x) = c0 k (1 − x)k−1 ,
(4.18)
where c(x) is the impurity concentration in the crystal at the freezing interface, x is the frozen melt fraction (ratio of solid mass to total mass, 0 ≤ x ≤ 1). k is the distribution x preservation of the impurities can be written at any time cm (1 − x) + 0 c(x ) dx = c0 , where cm is the (remaining) concentration in the melt. At the beginning cm (0) = c0 . At the interface c(x) = k cm (x). Putting this into the mass preservation, building c (x) and solving the resulting differential equation c = c(1 − k)/(1 − x) with c(0) = k c0 leads to (4.18).
3 Mass
4.2 Point Defects
(a)
89
(b)
Fig. 4.6 (a) Relative concentration of indium along a CZgrown germanium crystal. Absolute concentration is in the 1016 cm−3 range. Solid line follows (4.19) with k = 1.2 × 10−3 . Symbols are experimental data from [254]. (b) Impurity distribution (relative concentration c(x)/c0 ) for CZ (4.18) (solid lines) and FZ (4.20) (dashed lines, z = 0.01) silicon crystals for B (blue), P (red), and Al (green). Distribution coefficients have been taken from Table 4.2. Note crossing of B and P lines and possibly associated change from ptype to ntype (cmp. Fig. 1.7)
coefficient (or segregation coefficient) which is the fraction of impurities that is built into the crystal at the liquid–solid interface. Since the melt volume reduces during the solidification, the impurity concentration rises over time. For small distribution coefficients (4.18) can be approximated to c(x) ≈ c0
k , 1−x
(4.19)
An experimental example for Ge:In is shown in Fig. 4.6a. In Table 4.2 the distribution coefficients for various impurities in Si, Ge and GaAs is given. The modification of distribution coefficients in SiGe alloys is discussed in [252]. Equilibrium values (keq ) are obtained for ‘slow’ crystal growth. For finite growth rates, k becomes a function of the growth rate and is then called the effective distribution coefficient. For k < 1, keff > keq . keff approaches 1 for high growth rates, i.e. all impurities at the rapidly moving interface are incorporated. Equation (4.18) applies to Czrochalski growth where the crystal is pulled out of the melt [257]. In floatzone (FZ) growth [257] a polycrystalline rod is transformed into a crystalline one while a RFheated and liquid ‘float’ zone is moved through the crystal. In this case the impurity distribution is given by4
m = cm z in the liquid is m m = c0 −kcm . The first term stems from the melting of the polycrystalline part, the second
= (c − kc )/z from the solidification of the crystal. Solving the resulting differential equation cm 0 m with cm (0) = c0 and using c(x) = kcm (x) yields (4.20). 4 When the float zone moves through the crystal, the change of mass of impurities m
90
4 Defects
Table 4.2 Equilibrium distribution coefficients (at melting point) of various impurities in silicon, germanium and GaAs Impurity Si Ge GaAs C Si Ge N O B Al Ga In P As Sb S Fe Ni Cu Ag Au Zn
>1.85 5.5
0.07 0.33 7 × 10−4 ≈1 0.8 2.8 × 10−3 8 × 10−3 4 × 10−4 0.35 0.3 0.023 10−5 6.4 × 10−6 ≈ 3 × 10−5 8 × 10−4 ≈ 1 × 10−6 2.5 × 10−5 2.5 × 10−5
0.8 0.1 0.03 0.3
12.2 0.1 0.087 1.2 × 10−3 0.12 0.04 3.3 × 10−3 > 5 × 10−5 3 × 10−5 2.3 × 10−6 1.3 × 10−5 10−4 1.5 × 10−5 6 × 10−4
3 0.1 2 1019 cm−3 ) must be considered a lowconcentration alloy. The lattice constant is thus slightly changed, which can cause problems in the subsequent (latticemismatched) epitaxy of pure layers.
4.4 Extended Defects
103
4.4 Extended Defects 4.4.1 Microcracks If the stress in a material becomes too big to be accommodated by dislocations, cracks may form to release strain energy.8 In Fig. 4.25 an example is shown. In this case, microcracks have formed in a bulk mercury indium telluride crystal upon incorporation of residual stress and thermal stress during cooling of the material from growth temperature (about 1000 K) to room temperature. See also Fig. 12.19 for microcracks in an epitaxial layer.
4.4.2 Stacking Faults The ideal stacking of (111) planes in the zincblende structure, ABCABC. . ., can be disturbed in various ways and creates area defects. If one plane is missing, i.e. the stacking is ABCACABC, an intrinsic stacking fault is present. If an additional plane is present, the defect is called an extrinsic stacking fault, i.e. ABCABACABC. An extended stacking fault in which the order of stacking is reversed is called a twin lamella, e.g. ABCABCB AC BABCABC. If two regions have inverted stacking order they are called twins and their joint interface is called a twin boundary, e.g. . . .ABCABCABCBACBACBA. . . (Fig. 4.28). The various types of stacking faults are shown in Fig. 4.26. In Fig. 4.27 a crosssectional image of stacking faults in GaAs on Si is shown. They block each other and thus partially annihilate with increasing thickness.
Fig. 4.25 Microcracks in a mercury indium telluride crystal. Adapted from [306]
8 We
note that in elasticity theory a continuous deformation is assumed. Obviously the separation (fracture) into two unstrained blocks is the lowest strain energy state of a stressed piece of material.
104
4 Defects
Fig. 4.26 HRTEM images of (a) thinfilm silicon with intrinsic (labeled ‘ISF’) and extrinsic (‘ESF’) stacking faults and twin boundary (‘Twin’). (b) Six monolayer thick hexagonal (wurtzite) CdTe layer in cubic (zincblende) CdTe. Stacking order (from bottom to top) is: ABCABABABABC. . . Reprinted with permission from [307]
Fig. 4.27 Crosssectional TEM image showing stacking faults in heteroepitaxial GaAs on Si. Adapted from [308]
Fig. 4.28 High resolution TEM image of ZnS nanowire exhibiting periodical twin structures. Adapted from [309]
4.4 Extended Defects
105
Fig. 4.29 Reduced stacking fault energy (stacking fault energy per bond) γ for various compound semiconductors plotted as a function of the sparameter. Dashed line is guide to the eye. Data from [164]
A stacking fault is bounded by two partial dislocations (Sect. 4.3.1) formed by the dissociation of a perfect dislocation. A full (or perfect) dislocation with Burger’s vector a/2[110] in a III–V compound is dissociated into two Shockley partials according to (4.22) [310]. Since the dislocation energy is proportional to b2 , the dissociation is energetically favored (see Sect. 4.3.1). The stackingfault energy in pure silicon is γ = 47 mJ m−2 [311]. A similar value is found for Ge, γ = 60 mJ m−2 [312] and undoped GaAs, γ = 45 mJ m−2 [313]. In diamond a much larger value is found, γ = 285 mJ m−2 [314]. Impurity incorporation typically reduces the stacking fault energy. The systematics of stacking fault energy for various III–V and II–VI compounds has been discussed [164, 315, 316]. It can be correlated with the sparameter (2.11) as depicted in Fig. 4.29.
4.4.3 Grain Boundaries The boundaries of crystal grains are called grain boundaries. They are defined by five parameters, three rotation angles (e.g. Euler angles) to describe how the orientation of grain II results from grain I and two parameters to define the boundary plane of the two grains in the coordinate system of reference grain I. Such defects can have a large impact on the electric properties. They can collect point defects and impurities, act as barriers for transport (Sect. 8.3.8) or as carrier sinks due to (nonradiative) recombination. Details of their structure and properties can be found in [317, 318]. The two crystal grains meet each other with a relative tilt and/or twist. The situation is shown schematically in Fig. 4.30a for a small angle between the two crystals. A periodic pattern of dislocations forms at the interface that is called a smallangle grain boundary (SAGB) (Fig. 4.30b). In
106
4 Defects
(a)
(b)
(c)
(d)
(e)
(f)
Fig. 4.30 Schemes of (a, b, c) pure tilt and (d, e, f) pure twist boundary, dislocation formation in (c) pure tilt and (f) twist boundaries
Fig. 4.31, experimental results for pure tilt SAGB are shown. The dislocation spacing is inversely proportional to the tilt angle θ. An image of a twist SAGB is shown in Fig. 4.32. Special large angle boundaries possess (for a certain angle) a coincident site lattice (CSL). Some of these grain boundaries have a low energy and are thus commonly observed. The ratio of lattice points of the CSL and the lattice unit cell is an odd integer number n; the corresponding grain boundary is then labeled Σn. SAGB are also termed Σ1. Σ3 grain boundaries are always twin boundaries. An example with (111) grain boundary is schematically shown in an example in Fig. 4.33a. A Σ3 (twin) boundary in silicon with {112} grain boundary [319, 320] is depicted in Fig. 4.34 together with the atomic arrangement of the grain boundary itself. A Σ5 (001) grain boundary is schematically shown in Fig. 4.33b; the special angle is θ = arctan 3/4 ≈ 36.87◦ . Real grain boundaries may not be flat, contain impurities or precipitates and even consist of a thin amorphous layer.
4.4.4 Antiphase and Inversion Domains Antiphase domains occur when one part of the crystal is shifted with respect to another by an antiphase vector p. This does not form a twin. If the polar direction changes between two domains they are called inversion domains. ¯ In the zincblende structure the [110] and [110] directions are not equivalent. In one case there is a ZnS lattice and in the other a SZn lattice. Both lattices vary by a 90◦ rotation or an inversion operation (which is not a symmetry operation of the zincblende crystal). If, e.g., a zincblende crystal is grown on a Si surface with monoatomic steps (Fig. 4.35, cmp. Fig. 11.6), adjoint regions have a different phase;
4.4 Extended Defects
107
(a)
(c)
6
5
(b)
4
3
2
1
0
0
1
2
3
4
5
4
(d)
(e)
Fig. 4.31 (a) Scheme of a smallangle (pure tilt) grain boundary. (b) Model of edge dislocations in a {110} plane in Ge. (c) Relation of dislocation distance d and tilt angle θ for various smallangle grain boundaries in Ge. Solid line is relation d = 4.0 × 10−8 /θ. (d) Optical image of an etched (CP–4 etch) Ge sample with a smallangle grain boundary. Adapted from [321]. (e) HRTEM image of a smallangle grain boundary in Si with dislocations highlighted. From [322]
they are called antiphase domains (APD). The antiphase vector is (0, 0, 1) a0 /4. At the boundaries a twodimensional defect, an antiphase domain boundary, develops. The APD boundary contains bonds between identical atom species. In Fig. 4.36, intertwining APD boundaries are shown on the surface of InP layers on Si. The antiphase domains can be visualized with an anisotropic etch. In Fig. 4.37a, inversion domains in irondoped ZnO are shown. Between domains the direction of the caxis is reversed. The iron is found preferentially in the inversion domain boundary (IDB) (Fig. 4.37b) and plays an important role in its formation [326, 327].
108
4 Defects
100 nm
Fig. 4.32 Brightfield TEM image of pure twist boundary with network of pure twist dislocations fabricated by wafer bonding of two Si (001) surfaces with a relative twist. Adapted from [323]
(a)
(b)
Fig. 4.33 (a) Schematic of Σ3 (111) twin boundary in a diamond or zincblende structure (cmp. Fig. 4.28). The grain boundary is marked by a dashed line shown in sideview. The hexagonal and rectangular grey boxes have the same area. The lattice points of the coincident site lattice (CSL) are shown with black circles in the lower part of the figure. The unit cell of the CSL has three times the volume of the unit cell of the fcc lattice. (b) Schematic of a Σ5 (001) grain boundary in a (simple) cubic crystal shown in planeview. The blue and the red lattice are rotated by 36.86◦ , the lattice points of the CSL are shown in black. The unit cell of the CSL lattice (dark grey) has five times the volume of the cubic unit cell (light grey)
4.4 Extended Defects
109
Fig. 4.34 TEM images in two magnifications of a Σ3 {112} boundary in silicon together with a schematic of the atomic arrangement. Adapted from [320]
Fig. 4.35 Monoatomic step on the Si (001) surface and subsequent formation of an antiphase boundary in InP (zincblende)
Fig. 4.36 Antiphase domains in InP on Si. HCl etchs InP anisotropically and prepares (111)A planes. The etch patterns of layers with (without) APDs are crosshatched (linear). Adapted from [324]
110
4 Defects
(a)
(b)
(21 15
)
(0001)
Fe Fig. 4.37 Transmission electron microscopy of inversion domains in ZnO:Fe. (a) Inversion domains in irondoped ZnO (ZnO:Fe2 O3 = 100:1). Arrows denote the orientation of the caxis in the respective domains. (b) Top: bright field TEM, bottom Fe distribution from energyfiltered image. Adapted from [325]
4.5 Disorder Disorder is a general term for deviations from the ideal structure on a microscopic scale. Apart from the various structural defects discussed in the previous chapters, further examples of disorder are • The presence of various isotopes of an element. This introduces disorder with regard to the mass of the atoms and impacts mostly phonon properties (see Fig. 8.24). • The occupation of lattice sites in alloys (Sect. 3.7) ranging from a random alloy, clustering to (partially) ordered phases. • The thermal and zeropoint motion of atoms around their equilibrium position.
Chapter 5
Mechanical Properties
Abstract Lattice vibrations and phonons are treated with onedimensional models and examples for real phonon dispersions for several semiconductors including phonons in alloys and disordered materials are given. Then the theory of linear elasticity and its application to semiconductors with regard to epitaxial strain, substrate bending and sheetscrolling is given. Finally plastic relaxation effects such as critical thickness and wafer breakage are discussed.
5.1 Introduction The atoms making up the solid have an average position from which they can deviate since they are elastically bonded. The typical atomic interaction potential looks like the one shown in Fig. 2.1. The atoms thus perform a vibrational motion (including zero point fluctuations) and the solid is elastic. The potential is essentially asymmetric, being steeper for small distances due to quantummechanical overlap of orbitals. However, for small amplitudes around the minimum a harmonic oscillator can be assumed (harmonic approximation). Beyond the elastic regime, plastic deformation occurs such as generation of defects, e.g. dislocations. Eventually also the crystal can break.
5.2 Lattice Vibrations In the following we will discuss the dispersion relations for lattice vibrations, i.e. the connection between the frequency ν (or energy hν = ω) of the wave and its wavelength λ (or kvector k = 2π/λ). Acoustic and optical vibrations are introduced in onedimensional models. A detailed treatment of the physics of lattice vibrations is given in [328].
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_5
111
112
5 Mechanical Properties
5.2.1 Monoatomic Linear Chain The essential physics of lattice vibrations can best be seen from a onedimensional model that is called the linear chain. The mechanical vibrations will also be called phonons, although technically this term is reserved for the quantized lattice vibrations resulting from the quantummechanical treatment. In the monoatomic linear chain the atoms of mass M are positioned along a line (xaxis) with a period (lattice constant) a at the positions xn 0 = na. This represents a onedimensional Bravais lattice. The Brillouin zone of this system is [−π/a, π/a]. The atoms will interact with a harmonic potential, i.e. the energy is proportional to the displacement u n = xn − xn 0 to the second power. The total (mechanical) energy of the system is then: 1 (u n − u n+1 )2 . (5.1) U= C 2 n The model assumes that the mass points are connected via massless, ideal springs with a spring constant C. If φ(x) is the interaction energy between two atoms, C is given by C = φ (a). Again, the harmonic approximation is only valid for small displacements, i.e. u n a. The displacement of the atoms can be along the chain (longitudinal wave) or perpendicular to the chain (transverse wave), see Fig. 5.1. We note that for these two types of waves the elastic constant C must not be the same. When the sum in (5.1) has a finite number of terms (n = 0,. . . ,N − 1), the boundary conditions have to be considered. There are typically two possibilities: The boundary atoms are fixed, i.e. u 0 = u N −1 = 0, the boundary conditions are periodic (Born–von Karman), i.e. u i = u N +i . If N 1, the boundary conditions play no significant role anyway, thus those with the greatest ease for subsequent math are chosen. In solidstate physics typically periodic boundary conditions are Fig. 5.1 Visualization of transverse (‘T’) and longitudinal (‘L’) waves in a linear monoatomic chain at different wavevectors
a k=1/4 /a
T L k=1/2 /a
T L k= /a
T L
5.2 Lattice Vibrations
113
used. Boundary phenomena, such as at surfaces, are then treated separately (see Sect. 11.6.1). The equations of motion derived from (5.1) are M u¨ n = Fn = −
∂U = −C (2u n − u n−1 − u n+1 ). ∂u n
(5.2)
We solve for solutions that are periodic in time (harmonic waves), i.e. u n (x, t) = u n exp(−iωt). Then the time derivative can be executed immediately as u¨ n = −ω 2 u n and we obtain: (5.3) Mω 2 u n = C (2u n − u n−1 − u n+1 ). If, also, the solution is periodic in space, i.e. is a (onedimensional) plane wave, i.e. u n (x, t) = v0 exp(i(kx − ωt)) with x = na, we find from the periodic boundary condition exp(ik N a) = 1 and thus k=
2π n , n ∈ N. a N
(5.4)
It is important that, when k is altered by a reciprocal space vector, i.e. k = k + 2πn/a, the displacements u n are unaffected. This property means that there are only N values for k that generate independent solutions. These can be chosen as k = −π/a, . . . , π/a, so that k lies in the Brillouin zone of the lattice. In the Brillouin zone there is a total number of N kvalues, i.e. one for each lattice point. The distance between adjacent kvalues is 2π 2π = , (5.5) Na L L being the lateral extension of the system. The displacements at the lattice points n and n + m are now related to each other via u n+m = v0 exp(ik(n + m)a) = v0 exp(ikna) exp(ikma) = exp(ikma) u n .
(5.6)
Thus, the equation of motion (5.3) reads Mω 2 u n = C 2 − exp(−ika) − exp(ika) u n .
(5.7)
Using the identity exp(ika) + exp(−ika) = 2 cos(ka), we find the dispersion relation of the monoatomic linear chain (Fig. 5.2): ω 2 (k) =
4C 1 − cos(ka) 4C = sin2 M 2 M
ka 2
.
(5.8)
114
5 Mechanical Properties
Fig. 5.2 Dispersion relation for a monoatomic linear chain
The solutions describe plane waves that propagate in the crystal with a phase velocity c = ω/k and a group velocity vg = dω/dk vg =
4C a ka cos . M 2 2
(5.9)
In the vicinity of the Γ point, i.e. k π/a the dispersion relation is linear in k ω(k) = a
C k. M
(5.10)
We are used to such linear relations for sound (and also light) waves. The phase and group velocity are the same and do not depend on k. Thus, such√solutions are called acoustic. The sound velocity of the medium is given by vs = a C/M. It is characteristic of the nonhomogeneous medium that, when k approaches the boundary of the Brillouin zone, the behavior of the wave is altered. For k = π/a the wavelength is just λ = 2π/k = 2a, and thus samples the granularity of the medium. The maximum phonon frequency ωm is ωm =
4C . M
(5.11)
The group velocity is zero at the zone boundary, thus a standing wave is present. Since the force constants of the longitudinal and transverse waves can be different, the dispersion relations are different. The transverse branch of the dispersion relation is 2fold degenerate, unless the two directions that are perpendicular to x are not equivalent.
5.2 Lattice Vibrations
115
5.2.2 Diatomic Linear Chain Now we consider the case that the system is made up from two different kinds of atoms (Fig. 5.3). This will be a model for semiconductors with a diatomic base, such as zincblende. We note that the diamond structure also needs to be modeled in this way, although both atoms in the base are the same. The lattice will be the same and the lattice constant will be a. Alternating atoms of sort 1 and 2 with a relative distance of a/2 are on the chain. The displacements of the two atoms are labeled u 1n and u 2n , both belonging to the lattice point n. The atoms have the masses M1 and M2 . The force constants are C1 (for the 1–2 bond within the base) and C2 (for the 2–1 bond between different bases). The total energy of the system is then given as U=
2 1 2 1 u 1n − u 2n + C2 u 2n − u 1n+1 . C1 2 2 n n
(5.12)
The equations of motion are M1 u¨ 1n = −C1 u 1n − u 2n − C2 u 1n − u 2n−1 M2 u¨ 2n = −C1 u 2n − u 1n − C2 u 2n − u 1n+1 .
(5.13a) (5.13b)
With the planewave ansatz u 1n (x, t) = v1 exp (i(kna − ωt)) and u 2n (x, t) = v2 exp (i(kna − ωt)) and periodic boundary conditions we find 0 = −M1 ω 2 v1 + C1 (v1 − v2 ) + C2 [v1 − v2 exp(−ika)] 0 = −M2 ω 2 v2 + C1 (v2 − v1 ) + C2 [v2 − v1 exp(ika)].
Fig. 5.3 Visualization of acoustic and optical waves in a diatomic linear chain
(5.14a) (5.14b)
116
5 Mechanical Properties
These equations for v1 and v2 can only be solved nontrivially if the determinant vanishes, i.e.
M ω 2 − (C1 + C2 ) C1 + e−ika C2
(5.15) 0 =
1 C1 + eika C2 M2 ω 2 − (C1 + C2 )
= M1 M2 ω 4 − (M1 + M2 )(C1 + C2 ) ω 2 + 2C1 C2 [1 − cos(ka)]. √ Using the substitutions C+ = (C1 + C2 )/2, C× = C1 C2 , the arithmetic and geometrical averages, and accordingly for M+ and M× , the solution is 1 − cos(ka) 2C× 2 , 1± 1−γ ω (k) = γ M× 2 2
with γ=
C × M× ≤ 1. C + M+
(5.16)
(5.17)
The dispersion relation, as shown in Fig. 5.4, now has (for each longitudinal and transverse mode) two branches. The lower branch (‘−’ sign in (5.16)) is related to the acoustic mode; neighboring atoms have similar phase (Fig. 5.3). For the acoustic mode ω = 0 at the Γ point and the frequency increases towards the zone boundary. The maximum phonon frequency ωm is in the upper branch (‘+’ sign in (5.16)) at the zone center
4C× C + M+ =2 . (5.18) ωm = γ M× M×2 The upper branch is called the optical mode (since it can interact strongly with light, see Sect. 9.9) and neighboring atoms have opposite phase. In the vicinity of the Γ point the dispersion of optical phonons is parabolic with negative curvature:
Fig. 5.4 Dispersion relation for a diatomic linear chain with acoustic (blue) and optical (green) branch
5.2 Lattice Vibrations
117
1 γ a 2 2 k . ω(k) ∼ = ωm 1 − 2 4
(5.19)
Thus, four different vibrations exist that are labeled TA, LA, TO, and LO. Both the TA and TO branches are degenerate. At the zone boundary (X point) a frequency gap exists. The gap center is at ωm ωX = √ , 2
(5.20)
C + M+ − C × M× . Δω X = ωm 1 − γ = 2 M×2
(5.21)
and the total width of the gap is
The group velocity is zero for optical and acoustic phonons at k = π/a and for optical phonons at the Γ point. Usually two cases are treated explicitly: (i) atoms with equal mass (M = M1 = M2 ) and different force constants or (ii) atoms with unequal mass and identical force constants C = C1 = C2 . For the case C1 = C2 and M1 = M2 , γ = 1 and thus Δω X = 0. Then the dispersion relation is the same as for the monoatomic chain, except that the k space has been folded since the actual lattice constant is now a/2. M1 = M2 In this case, M+ = M× = M and the dispersion relation is
2 1 − cos(ka) 2C C + × ω2 = 1± 1− 2 . M 2 C+
(5.22)
At the√zone boundary the frequencies for √ the acoustic and the optical branch are ω X,1 = 2C1 /M with v1 = v2 and ω X,2 = 2C2 /M with v1 = −v2 , respectively (assuming C2 > C1 ). The motion for k = π/a is phase shifted by 180 ◦ for adjacent bases. Additionally, for the acoustic branch the atoms of the base are in phase, while for the optical branch the atoms of the base are 180 ◦ out of phase. The vibration looks as if only one of the springs is strained. C1 = C2 In this case, C+ = C× = C and the dispersion relation is
2C M+ M×2 1 − cos(ka) 2 ω = . 1± 1− 2 2 M×2 M+
(5.23)
At the√zone boundary the frequencies for the √ acoustic and the optical branch are ω X,1 = 2C/M1 with v2 = 0 and ω X,2 = 2C/M2 with v1 = 0, respectively
118
5 Mechanical Properties
(assuming M2 < M1 ). In the vibration for k = π/a thus only one atom species oscillates, the other does not move. Close to the Γ point the atoms are in phase in the acoustic branch, √ i.e. v1 = v2 . For the optical branch, the frequency at the Γ point is given by ω = 2C/Mr (with the reduced mass Mr−1 = M1−1 + M2−1 = 2M+ /M×2 ) and the amplitude ratio is given by the mass ratio: v2 = −(M1 /M2 ) v1 , i.e. the heavier atom has the smaller amplitude.
5.2.3 Lattice Vibrations of a ThreeDimensional Crystal When calculations are executed for a threedimensional crystal with a monoatomic base, there are 3N equations of motion. These are transformed to normal coordinates and represent 3 acoustic branches (1 LA phonon mode and 2 TA phonon modes) of the dispersion relation. In a crystal with a base with p atoms, there are also 3 acoustic branches and 3( p − 1) optical branches. For a diatomic base (as in the zincblende structure) there are 3 optical phonon branches (1 LO phonon mode and 2 TO phonon modes). The total number of modes is 3 p. The dispersion ω(k) now has to be calculated for all directions of k. In Figs. 5.5 and 5.6, the phonon dispersion in silicon, GaAs and GaP is shown along particular lines in the Brillouin zone (cf. Fig. 3.34b). The degeneracy of the LO and TO energies at the Γ point for the covalent groupIV semiconductor is lifted for the III–V semiconductors due to the ionic character of the bond and the macroscopic electric field connected with the longwavelength LO phonon (see Sect. 5.2.9). Comparing GaAs [329] and GaP [330], the quite different mass of Ga and Patoms (M× /M+ ≈ 0.92) leads to the formation of a clear gap between the acoustic and optical branches, while for GaAs M× /M+ ≈ 0.9994 is close to 1 and no gap forms. We note that the degeneracy of the TA phonon is lifted for propagation along the ¯ are not 110 directions (Σ) because the two transverse directions 001 and 110 equivalent.
Fig. 5.5 Phonon dispersion in Si, experimental data and theory (solid lines: bond charge model, dashed lines: valence force field model). Adapted from [146]
5.2 Lattice Vibrations X
8
LO
6
TO
K
L
GaP 30
20 4
LA
Energy (meV)
Frequency (THz)
(a)
10
2
TA 0
0
LO
8
TO 6
30
[0,0, ]
[ , ,0]
L T
[ , , ]
I II T
L T
20
4
LA
Energy (meV)
(b) Frequency (THz)
Fig. 5.6 Phonon dispersion in (a) GaP and (b) GaAs. Experimental data (symbols) and theory (solid lines, 14parameter shell model). ‘L’ and ‘T’ refer to longitudinal and transverse modes, respectively. ‘I’ and ‘II’ (along [ζ, ζ, 0]) are modes whose polarization is ¯ 0) plane. The in the (1, 1, grey area in (a) denotes the gap between acoustical and optical states. (a) Adapted from [331], (b) adapted from [329]
119
10
2
TA
GaAs
0 0 0.2 0.4 0.6 0.8 1.0
0 0.8 0.6 0.4 0.2
0
0.2
0.4
Reduced wavevector
In boron nitride the masses of the two constituents are so similar that no gap exists between acoustical and optical branches (Fig. 5.7). Also the density of states (averaged over the entire Brillouin zone) is depicted (see next Sect.). The displacement of atoms is shown in Fig. 5.8 for the different phonon modes present in zincblende crystals and in Fig. 5.9 for wurtzite crystals. The modes are labeled with their symmetry (in molecular notation) according to group theory (see remark in Sect. 6.2.5).
Fig. 5.7 Phonon dispersion in BN (left panel), experimental data (symbols) and theory (solid lines, first principles pseudopotential model). In the right panel the density of states is depicted. Adapted from [332]
120
5 Mechanical Properties
A1
E
T2(1)
T2
T2
T2(2)
T2(2)
T2(2)
(1)
E
(1)
Fig. 5.8 Displacement of atoms for various phonon modes in zincblende crystals. Adapted from [333]
Fig. 5.9 Displacement of atoms for various phonon modes in wurtzite crystals. Adapted from [334]
√ The dependence of the phonon frequency on the mass of the atoms (∝ 1/ M) can be demonstrated with the isotope effect, visualized for GaAs in Fig. 5.10. The dependence of the phonon frequencies on the stiffness of the spring can be seen from Fig. 5.11; the smaller lattice constant provides the stiffer spring.
5.2 Lattice Vibrations
121
Fig. 5.10 (a) Raman spectra of GaAs with different isotope content as labeled. (b) Energy of optical phonons in GaAs with different isotope content [using the Raman spectra shown in (a)]. Reprinted with permission from [335], © 1999 APS
Fig. 5.11 Optical phonon frequencies (TO: filled squares, LO: empty squares) for a number of III–V compounds with different lattice constant a0 . 1 meV corresponds to 8.065 wave numbers (or cm−1 ). Adapted from [336]
5.2.4 Density of States The density of states (DOS) tells how many of the total 3 pN modes are in a given energy interval. The states are spaced equally in kspace but not on the energy scale (see also Sect. 6.11).
122
5 Mechanical Properties
(b)
(a)
Fig. 5.12 (a) Phonon dispersion for the diatomic linear chain model for γ = 1 (black line) and γ = 0.9 (blue lines). (b) Corresponding density of states (in units of N /E m )
For the monoatomic linear chain model, the number of states N (E ) from E = 0 up to E = ω = E (k ) for the dispersion of the acoustic phonons (5.8) is given as N (E ) = k
N L = k. π/a π
(5.24)
Using (5.8), we find for one polarization (E m = ωm ) N (E) =
2N arcsin π
E Em
.
(5.25)
The DOS D(E) is given by D(E) =
1 dN (E) 2N . = dE π E m 1 − (E/E m )2
(5.26)
Often the density of states is scaled by the (irrelevant) system size and given per atom (D/N ) or per volume (D/L 3 ), per area (D/L 2 ) or per length (D/L) for three, two or onedimensional systems, respectively. In the diatomic linear chain model, additionally the optical phonons contribute to the density of states. In Fig. 5.12 the phonon density of states is shown for γ = 0.9 and for comparison for γ = 1 (gapless phonon dispersion). For small wavevector, the density of states is 4N /(π E m ).1 Within the gap the density of states vanishes. At the edges of the band gap the density of states is enhanced. The total number of states for both dispersions is the same.
1 The factor 2 compared to (5.26) stems from the folded Brillouin zone compared to the monoatomic
chain model.
5.2 Lattice Vibrations
123
In a threedimensional solid, (5.24) is modified to (for three degenerate polarizations) 4π 3 k 3 , (5.27) N (E ) = 3 (2π/L)3 taking into account all states within a sphere in kspace of radius k . Assuming a linear dispersion ω = vs k, we obtain N (E) =
V E3 . 2π 2 3 vs3
(5.28)
Thus the density of states is proportional to E 2 , D(E) =
3 V E2 . 2π 2 3 vs3
(5.29)
This dependence is the base for Debye’s law for the T 3 temperature dependence of the heat capacity. As realistic example the phonon density of states for BN is depicted next to the dispersion in Fig. 5.7.
5.2.5 Phonons Phonons are the quantized quasiparticles of the lattice vibrations (normal modes). The energy of a phonon can take the discrete values of a harmonic oscillator
E ph
1 = n+ ω, 2
(5.30)
where n denotes the quantum number of the state, which corresponds to the number of energy quanta ω in the vibration. The amplitude of the vibration can be connected to n via the following discussion. For the classical oscillation u = u 0 exp i(kx − ωt) the space and time average for the kinetic energy yields E kin =
1 ρV 2
∂u ∂t
2 =
1 ρ V ω 2 u 20 , 8
(5.31)
where ρ is the density and V the volume of the (homogeneous) solid. The energy of the oscillation is split in half between kinetic and potential energy. From 2E kin = E ph we find 1 4 u 20 = n + . (5.32) 2 ρV ω
124
5 Mechanical Properties
The number of phonons with which a vibrational mode is populated is thus directly related to the classical amplitude square. Phonons act with a momentum k, the socalled crystal momentum. When phonons are created, destroyed or scattered the crystal momentum is conserved, except for an arbitrary reciprocalspace vector G. Scattering with G = 0 is called a normal process, otherwise (for G = 0) it is called an umklapp process.
5.2.6 Localized Vibrational Modes A defect in the crystal can induce localized vibrational modes (LVM). The defect can be a mass defect, i.e. one of the masses M is replaced by Md , or the force constants in the neighborhood are modified to Cd . A detailed treatment can be found in [337]. LVM are discussed, e.g., in [338–340]. First we consider the LVM for the onedimensional, monoatomic chain. If the mass at lattice point i = 0 is replaced by Md = M + ΔM (M = ΔM/M), the displacements are given by u i = AK i , A being an amplitude, with K =−
1 + M , 1 − M
(5.33)
and the defect phonon frequency ωd is
ω d = ωm
1 . 1 − 2M
(5.34)
A real frequency is obtained for√M  < 1. ωd is then higher than the highest frequency of the bulk modes ωm = 4C/M (5.11). For M < 0, i.e. the mass of the defect is smaller than the mass of the host atoms, K is negative and K  < 1. Thus, the displacement can be written as u i ∝ (−K )i = (−1)i exp (+ i log K ) .
(5.35)
The numerical value of the exponent is negative, thus the amplitude decreases exponentially from the defect and indeed makes a localized √ vibrational mode. For small mass Md M (5.34) yields approximately ωd = 2C/Md . This approximation is the socalled oneoscillator model. Since typically the extension of the localized mode is only a few lattice constants, the picture of LVM remains correct for impurity concentrations up to ∼1018 − 1020 cm−3 . For higher concentrations the concept of alloy modes has to be invoked (cf. Sect. 5.2.7). For the case of groupIII or V substitutional impurities in groupIV semiconductors the change in force constants (treated below) can be neglected to some extent. For silicon (M = 28) and germanium (M = 73) the effect of various substitutions is shown in Fig. 5.13.
5.2 Lattice Vibrations
125
Fig. 5.13 Energy of local vibrational modes in Si and Ge. Experimental values at T = 300 K (B in Ge: T = 80 K) taken from [337] and references therein and from [341] (C in Ge). The dashed lines are the mass dependence according to (5.34) scaled to the experimental frequency of the 10 B LVM
Now, additionally the force constants left and right of the defect are replaced by Cd = C + ΔC (C = ΔC/C). The displacements are still given by u i = AK i , now with (1 + M ) (1 + C ) . (5.36) K =− 1 − M − 2C An exponential decrease of the LVM amplitude occurs for negative K that is ensured for M + 2C < 0 (and M > −1 and C > −1). The defect frequency is given by
(1 + C ) (2 + C (3 + M )) . (5.37) ω d = ωm 2(1 + M ) (2C + 1 − M ) We note that for C = 0 (5.33) and (5.34) are recovered. For a given mass defect, the change of frequency with ΔC is (in linear order, i.e. for C 1) ∂ωd (M , C ) 1 − 4 M − 2M = C . ∂C 4 (1 − M ) 1 − 2M
(5.38)
The linear coefficient diverges for M → −1. For M between −0.968 and 0 the linear coefficient varies between 2 and 1/4. Therefore, a larger force constant (C > 0) increases the LVM frequency of the defect, as expected for a stiffer spring. In a binary compound the situation is more complicated. We assume here that the force constants remain the same and only the mass of the substitution atom Md is different from the host. The host has the atom masses M1 and M2 with M1 < M2 . Substitution of the heavy atom with a lighter one creates a LVM above the optical branch for Md < M2 . Additionally, a level in the gap between the optical and acoustic
126
(a)
5 Mechanical Properties
(b) 0 27
11
AlGa
20
28
BP
SiGa
12
40
CGa
10
BP
60 14
NP
80 100 400
GaP 450
500
550
600
1
Fig. 5.14 (a) Numerical simulation of a linear chain model for GaP (M1 = 31, M2 = 70). Energy of local vibrational modes (dashed (solid) line): substitution on P (Ga) site in units of the optical phonon frequency at Γ (ωm = 45.4 meV). The grey areas indicate the acoustic and optical phonon bands. Solid squares are experimental data (from [337]), scaled to the theoretical curve for the 27 Al Ga LVM frequency. (b) Differential transmission spectrum of GaP structure (nitrogendoped layer on zincdoped compensated substrate) against pure crystal (T = 77 K). Data from [342]
branch is induced. Such LVM is called a gap mode. Substitution of the lighter atom of the binary compound induces a LVM above the optical branch for Md < M1 . A gap mode is induced for Md > M1 . The situation for GaP is depicted in Fig. 5.14. LVM in GaAs have been reviewed in [338]. The energy position of a local vibrational mode is sensitive to the isotope mass of the surrounding atoms. In Fig. 5.15, a highresolution (0.03 cm−1 ) spectrum of the 12 CAs LVM in GaAs is shown together with a theoretical simulation. The various theoretical peak positions are given as vertical bars, their height indicating the oscillator
Fig. 5.15 Experimental (Exp., T = 4.2 K, resolution 0.03 cm−1 ) and theoretical (Th., artificial Lorentzian broadening) infrared spectra of LVM of 12 CAs in GaAs. The positions and oscillator strengths of the theoretical transitions involving different configurations with 69 Ga and 71 Ga isotopes are shown as vertical bars. Data from [338]
GaAs 12
CAs
Exp. Th. 1
5.2 Lattice Vibrations
127
strength. Five experimental peaks are obvious that are due to a total of nine different transitions. The C atom can experience five different surroundings (see Table 3.8) with the four neighbors being 69 Ga or 71 Ga. The natural isotope mix is an ‘alloy’ 69 Gax 71 Ga1−x As with x = 0.605. The configurations with Td symmetry contribute one peak each, the lowest (71 Ga surrounding) and highest (69 Ga surrounding) energy transitions. The configurations with C3v and C2v symmetry contribute each with 2 and 3 nondegenerate modes, respectively. The vibrations of impurity complexes have been discussed in [343].
5.2.7 Phonons in Alloys In an alloy of the type AB1−x Cx the phonon frequencies will depend on the ternary composition. For the binary end materials AB and AC clearly TO and LO frequencies exist. The simplest behavior of the alloy is the onemode behavior (Fig. 5.16d) where the mode frequencies vary continuously (and approximately linearly) with the composition. The oscillator strength (LO–TO splitting, (9.74)) remains approximately constant. In many cases, the twomode behavior is observed where the LO–TO gap closes (accompanied by decreasing oscillator strength) and a localized vibrational mode and a gap mode occur for the binary end materials (Fig. 5.16a). Also, a mixedmode behavior (Fig. 5.16b, c) can occur. The masses of the three constituent atoms will be MA , MB , and MC . Without limiting the generality of our treatment, we assume MB < MC . From the considerations in Sect. 5.2.6 on LVM and gap modes, the condition
localized mode
LO1
(d)
(c)
(b)
(a)
localized mode
LO1
LO1
Frequency
LO TO1
TO1
LO2
TO1
LO2
LO2 TO
TO2
gap mode
0
0.5
Composition
TO2
1
0
0.5
Composition
TO2
gap mode
1
0
0.5
Composition
1
0
0.5
1
Composition
Fig. 5.16 Schematic behavior of phonon modes in an alloy. (a) Twomode behavior with gap mode and localized mode, (b, c) mixedmode behavior, (b) only localized mode allowed, (c) only gap mode allowed, (d) onemode behavior with neither localized mode nor gap mode allowed
128
5 Mechanical Properties
Table 5.1 Atomic masses of the constituents of various ternary compounds, reduced mass μAC (5.40), fulfillment of the relation from (5.40) (‘+’: fulfilled, ‘−’: not fulfilled) and experimental mode behavior (‘2’: twomode, ‘1’: onemode) Alloy A B C MA MB MC μAC Rel. Modes GaP1−x Asx GaAs1−x Sbx CdS1−x Sex Cdx Zn1−x S Mgx Zn1−x O
Ga Ga Cd S O
P As S Zn Mg
As Sb Se Cd Zn
69.7 69.7 112.4 32.1 16.0
31.0 74.9 32.1 65.4 24.3
74.9 121.8 79.0 112.4 65.4
36.1 44.3 46.4 25.0 12.9
MB < MA , MC
+ − + − −
2 1 2 1 1
(5.39)
for twomode behavior can be deduced. This ensures a LVM of atom B in the compound AC and a gap mode of atom C in the compound AB. However, it turns out that this condition is not sufficient, e.g. Na1−x Kx Cl fulfills (5.39) but exhibits onemode behavior. From a modified REI2 model (for k ∼ 0 modes) it has been deduced that MB < μAC =
MA MC < MA , MC MA + MC
(5.40)
is a necessary and sufficient condition (unless the force constants between A–B and A–C are significantly different) for twomode behavior [344]. A detailed discussion is given in [345]. Equation (5.40) is a stronger condition than the previous one (5.39). If (5.40) is not fulfilled the compound exhibits onemode behavior. As an example, we show the mass relations for CdS1−x Sex and Cdx Zn1−x S in Table 5.1 and the experimental phonon energies in Fig. 5.17. Also in Table 5.1 the masses for GaP1−x Asx (GaAs1−x Sbx ) exhibiting two (one) mode behavior are shown. If the binary end components of a ternary alloy have different crystal structure, a transition between the two occurs which is reflected in the phonon structure (energies and mode symmetries). As an example, the optical phonon energies of Mgx Zn1−x O are depicted in Fig. 5.18 (cmp. Fig. 3.39).
5.2.8 Disorder An example of ‘small’ disorder are the localized vibrational modes due to a single defect. Here we consider in our onedimensional model random fluctuations of the model parameters. To that avail we set up a numerical implementation of an onedimensional chain with masses M1 = M2 and spring constants C1 = C2 , here C2 = 2 C1 . Now each spring constant varies randomly by ±ξ percent. The density 2 Random
element isodisplacement.
5.2 Lattice Vibrations
129 320
360 Cd x Zn 1x S
1
1
CdS1x Sex
300
340 320
280 260
300
240 280
220
260
200
240
180
220
160
ZnS
x
CdS
x
CdS
CdSe
700
Mg x Zn1xO F1u
1
Fig. 5.18 LO (solid lines) and TO (dashed lines) phonon energies of Mgx Zn1−x O in the wurtzite structure (A1 symmetry: blue lines, E1 symmetry: red lines) and in the rocksalt phase (F1u symmetry: black lines). Experimental data are shown as symbols. Adapted from data of [346]
Phonon energy (cm )
Fig. 5.17 Phonon energies of Cdx Zn1−x S and CdS1−x Sex as a function of the ternary composition. Experimental data (solid circles) are from [344], dashed lines are guides to the eye
A1
600
E1 500
400 0.0
0.2
0.4
0.6
0.8
1.0
Mgconcentration x
of states is displayed for ξ = 10, 20, 40 and 60 %. The effects as shown in Fig. 5.19 are broadening of peaks in the DOS, broadening of the band edges, the development of band tails into the gap and eventually a closing of the gap. This is a typical behavior that also exists for electronic states (cmp. Fig. 6.46).
5.2.9 Electric Field Created by Optical Phonons Adjacent atoms oscillate with opposite phase in an optical phonon. If the bond has (partial) ionic character, this leads to a timedependent polarization and subsequently to a macroscopic electric field. This additional field will influence the phonon frequencies obtained from a purely mechanical approach. We consider in the following the case k ≈ 0. The phonon frequency for TO and LO vibrations is given by
5 Mechanical Properties
Density of States (arb. units)
130
0.0
10% 20% 40% 60%
0.5
1.0
Energy (Em)
Fig. 5.19 Density of states versus energy (in units of maximum phonon energy E m = ωm ) for diatomic linear chain model (M1 = M2 , C2 = 2 C1 , 29 atoms, average over 27 configurations) for various levels of random relative variations of the spring constants (solid lines). As dashed lines the density of states of the perfect chain is depicted (cmp. Fig. 5.12b) with the forbidden energy ranges shown in light grey
ω0 =
2C , Mr
(5.41)
where Mr is the reduced mass of the two different atoms (cf. Sect. 5.2.2). u is the relative displacement u1 − u2 of the two atoms in a diatomic base. When the interaction with the electric field E (which will be calculated selfconsistently in the following) is considered, the Hamiltonian for the longwavelength limit is given by [347]: 1 1 2 p + b11 u2 + 2b12 u · E + b22 E2 . Hˆ (p, u) = (5.42) 2 Mr The first term is the kinetic energy (p stands for the momentum of the relative ˙ the second the potential energy, motion of the atoms 1 and 2 in the base, p = Mr u), the third the dipole interaction and the fourth the electricfield energy. The equation of motion for a plane wave u = u0 exp [−i(ωt − k · r)] (u¨ = −ω 2 u) yields Mr ω 2 u = b11 u + b12 E. Thus, the electric field is 2 ) E = (ω 2 − ωTO
Mr u. b12
(5.43)
(5.44)
2 = b11 /Mr was introduced that is consistent with (5.41) Here, the substitution ωTO and b11 = 2C. ωTO represents the mechanical oscillation frequency of the atoms
5.2 Lattice Vibrations
131
undisturbed by any electromagnetic effects. Already now the important point is visible. If ω approaches ωTO , the system plus electric field oscillates with the frequency it has without an electric field. Therefore the electric field must be zero. Since the polarization P = ( − 1)0 E is finite, the dielectric constant thus diverges. The polarization is P = −∇E Hˆ = − (b12 u + b22 E) .
(5.45)
The displacement field is 2 /Mr b12 D = 0 E + P = 0 E − b22 − 2 E = 0 (ω) E. ωTO − ω 2
(5.46)
Therefore, the dielectric function is (ω) = (∞) +
(0) − (∞) . 1 − (ω/ωTO )2
(5.47)
Here, (∞) = 1 − b22 /0 is the highfrequency dielectric constant and (0) = 2 /(b11 0 ) the static dielectric constant. The relation (5.47) is shown in (∞) + b12 Fig. 5.20. From the Maxwell equation ∇ · D = 0 for zero free charge we obtain the relation 0 (ω) ∇ · E = 0.
(5.48)
Thus, either (ω) = 0 or ∇ · E = 0, i.e. u is perpendicular to k. In the latter case we have a TO phonon and, neglecting retardation effects, using ∇ × E = 0 we find
Fig. 5.20 Dielectric function according to (5.47) with (0) = 3 and (∞) = 2 (without damping). Grey area denotes the region of negative
4
(0)
3
( )
2 1 0
1 2 3 0
1
Frequency (
2 T
)
132
5 Mechanical Properties
E = 0 and therefore ω = ωTO , justifying our notation. In the case of (ω) = 0, we call the related frequency ωLO and find the socalled Lyddane–Sachs–Teller (LST) relation 2 ωLO (0) = . (5.49) 2 (∞) ωTO This relation holds reasonably well for optically isotropic, heteropolar materials with two atoms in the basis, such as NaI and also GaAs. Since at high frequencies, i.e. ω ωTO , only the individual atoms can be polarized, while for low frequencies the atoms can also be polarized against each other, (0) > (∞) and therefore also ωLO > ωTO . For GaAs, the quotient of the two phonon energies is 1.07. Using the LST relation (5.49), we can write for the dielectric function (ω) = (∞)
2 − ω2 ωLO 2 ωTO − ω2
.
(5.50)
The (longwavelength) TOphonon does not create a longrange electric field. Using ∇ · D = 0 and (5.46) and looking at the longitudinal fields, we have 0 E = b12 u + b22 E.
(5.51)
This can be rewritten as
E = − ωLO
Mr 0
1 1 − u ∝ −u. (∞) (0)
(5.52)
The (longwavelength) LOphonon thus creates a longrange electric field acting against the ion displacement and represents an additional restoring force; this is consistent with the fact that ωLO > ωTO .
5.3 Elasticity The elastic properties of the semiconductor are important if the semiconductor is subjected to external forces (pressure, temperature) or to lattice mismatch during heteroepitaxy.
5.3.1 Thermal Expansion The lattice constant depends on temperature. The (linear) thermal expansion coefficient is defined as
∂a0 (T )
(5.53) α(T0 ) = ∂T T =T0
5.3 Elasticity
133
Fig. 5.21 Linear thermal expansion coefficient of silicon (solid circles) and germanium (open circles). Adapted from [348] based on experimental data from various sources. Dashed lines are guide to the eyes
and is temperature dependent. The temperature dependence of α for silicon and germanium is shown in Fig. 5.21. α is approximately proportional to the heat capacity (CV ) except at low temperatures. The negative values are due to negative Grüneisen parameters [348]. These anharmonicity effects are discussed in detail in [328].
5.3.2 Stress–Strain Relation In this section, we recall the classical theory of elasticity [349]. The solid is treated as a continuous medium (piecewise homogeneous) and the displacement vector is thus a continuous function u(r) of the spatial coordinates. When the spatial variation ∇u of u is small, the elastic energy can be written as 1 U= 2
∂u n 3 ∂u l Cklmn d r, ∂xk ∂xm
(5.54)
where C is the (macroscopic) tensor of the elastic coefficients. 21 components of this tensor can be independent. For crystals with cubic symmetry the number of independent constants is reduced to 3. An exchange k ↔ l and m ↔ n does not matter, only six indices have to be considered (x x, yy, zz, yz, x z, and x y). The strain components i j are symmetrized according to i j =
1 2
∂u j ∂u i + ∂xi ∂x j
.
(5.55)
134
(a)
5 Mechanical Properties
(b)
(c)
(d)
Fig. 5.22 Deformation of a square (a). (b) Pure hydrostatic deformation (x x = yy = 0.2, x y = 0), (c) pure shear deformation (x x = yy = 0, x y = 0.2), and (d) mixed deformation (x x = yy = 0.1, x y = 0.1)
The strains x x are along the main axes of the crystal as visualized in Fig. 5.22. The stresses3 σkl are then given by σkl = Cklmn mn .
(5.56)
The inverse relation is mediated by the stiffness tensor S. kl = Sklmn σmn .
(5.57)
Typically, the strain components ei j or ei are used with the convention x x → 1, yy → 2, zz → 3, yz → 4, x z → 5, and x y → 6 (Voigt notation): ei j = i j (2 − δi j ).
(5.58)
Then, σm = Cmn en with the Ci j being the elastic constants. The x, y, and z directions are the main axes of the cubic solid, i.e. the 100 directions. For zincblende material, the stress–strain relation reads4 ⎛ ⎞ ⎛ ⎞⎛ ⎞ σ1 C11 C12 C12 0 0 0 e1 ⎜ σ2 ⎟ ⎜ C12 C11 C12 0 0 0 ⎟ ⎜ e2 ⎟ ⎜ ⎟ ⎜ ⎟⎜ ⎟ ⎜ σ3 ⎟ ⎜ C12 C12 C11 0 0 0 ⎟ ⎜ e3 ⎟ ⎜ ⎟=⎜ ⎟⎜ ⎟ (5.59) ⎜ σ4 ⎟ ⎜ 0 0 0 C44 0 0 ⎟ ⎜ e4 ⎟ . ⎜ ⎟ ⎜ ⎟⎜ ⎟ ⎝ σ5 ⎠ ⎝ 0 0 0 0 C44 0 ⎠ ⎝ e5 ⎠ σ6 e6 0 0 0 0 0 C44 Values of the compliances for several semiconductors are given in Table. 5.2. The inverse relation is given by the matrix
3 The 4C
11
stress is a force per unit area and has the dimensions of a pressure. = C1111 , C12 = C1122 and C44 = C1212 = C1221 = C2121 = C2112 .
5.3 Elasticity
135
Table 5.2 Elastic constants (in GPa) of some cubic semiconductors at room temperature. IK refers to the Keating criterion (5.63)
⎛
Material
C11
C12
C44
IK
C Si Ge BN GaAs InAs AlAs ZnS MgO
1076.4 165.8 128.5 820 119 83.3 120.5 104.6 297
125.2 63.9 48.3 190 53.4 45.3 46.86 65.3 156
577.4 79.6 66.8 480 59.6 39.6 59.4 46.3 95.3
1.005 1.004 1.08 1.11 1.12 1.22 1.03 1.33 0.80
S11 ⎜ S12 ⎜ ⎜ S12 ⎜ ⎜ 0 ⎜ ⎝ 0 0
S12 S11 S12 0 0 0
S12 S12 S11 0 0 0
0 0 0 S44 0 0
0 0 0 0 S44 0
⎞ 0 0 ⎟ ⎟ 0 ⎟ ⎟, 0 ⎟ ⎟ 0 ⎠ S44
(5.60)
with the stiffness coefficients in this notation given by C11 + C12 (C11 − C12 ) (C11 + 2C12 ) C12 = 2 2 −C11 − C11 C12 + 2C12 1 = . C44
S11 =
(5.61a)
S12
(5.61b)
S44
(5.61c)
We emphasize that in this convention (also called the engineering convention), e.g. e1 = x x and e4 = 2 yz . There is also another convention (the physical convention) without this factor of two; in this case the matrix in (5.59) contains the elements 2C44 . We introduce (5.62) C0 = 2 C44 + C12 − C11 , and note that C0 = 0 for an isotropic material. The relation IK =
2 C44 (C11 + C12 ) =1 (C11 − C12 ) (C11 + 3C12 )
(5.63)
known as the Keating criterion [350, 351], stems from the consideration of bending and stretching of the tetrahedral bonds in the valence force field (VFF) model. It is closely fulfilled (Table 5.2) for many tetrahedrally bonded semiconductors, in particular for the covalent ones. For MgO, the Keating criterion is not fulfilled because it has (sixfold coordinated) rocksalt structure and is thus not tetrahedrally bonded.
136
5 Mechanical Properties
The Young’s modulus Y , σnn = Y (n) nn ,
(5.64)
generally depends on the normal direction n of a strain. It is equivalent to 1/S11 of (5.61a). For isotropic material Y and the Poisson ratio ν are related to the elastic constants of cubic material by Y = C11 − ν=
2 2 C12 C11 + C12
C12 . C11 + C12
(5.65a) (5.65b)
For isotropic materials also Lamé’s constants λ and μ are used. They are given by5 C11 = λ + 2μ, C12 = λ and C44 = μ (note that C0 according to (5.62) is zero). The bulk modulus B (inverse of the compressibility), 1 ∂V 1 =− , B V ∂p
(5.66)
for the zincblende crystal is given as B=
C11 + 2 C12 . 3
(5.67)
We note that Y , ν and Ci j of typical materials are both positive. Materials with negative Poisson ratio are called auxetic [352–354]. Also materials with negative compressibility are possible [355]. Beyond the dependence of the elastic constants on the bond length (as materialized in the phonon frequencies in Fig. 5.11), they depend on the ionicity. In Fig. 5.23, the elastic constants of various zincblende semiconductors are shown as a function of the ionicity f i . The values for the elastic constants are normalized by e2 /a 4 , a being the average nearestneighbor distance. For wurtzite crystals, five elastic constant are necessary for the stress–strain relation that reads6 ⎞ ⎛ 0 C11 C12 C13 0 0 ⎟ ⎜ C12 C11 C13 0 0 0 ⎟ ⎜ ⎟ ⎜ C13 C13 C33 0 0 0 ⎟. ⎜ Ci j = ⎜ (5.68) ⎟ 0 0 0 0 0 C 44 ⎟ ⎜ ⎠ ⎝ 0 0 0 0 C44 0 0 0 0 0 0 21 (C11 − C12 ) 5 For 6 (C
an isotropic material, Ci jkl = λ δi j δkl + μ (δik δ jl + δil δ jk ). − C12 )/2 = C1212 , C44 = C1313 = C2323 .
11
5.3 Elasticity
137
(c)
(b)
(a)
Fig. 5.23 Elastic constants as a function of ionicity for various semiconductors with diamond or zincblende (circles) and wurtzite (squares) structure. Constants are normalized by the modulus C0 = e2 /d 4 , d being the average nearestneighbor distance. (a) Bulk modulus, ∗ = C /C . B ∗ = (C11 + 2C12 )/(3C0 ), (b, c) shear moduli, (b) CS∗ = (C11 − C12 )/C0 , (c) C44 44 0 Solid lines are a simple model as discussed in [356]. Adapted from [357] Table 5.3 Elastic constants (in GPa) of some wurtzite semiconductors
Material
C11
C12
C13
C33
C44 Reference
GaN AlN ZnS ZnO
391 410 124 206
143 149 60.2 118
108 99 45.5 118
399 389 140 211
103 125 28.6 44
[359] [360] [361] [362]
Experimental values for wurtzite materials are given in Table 5.3. The relation of the elastic tensor of wurtzite and zincblende materials, in particular viewed along the 111 direction has been discussed in [357, 358]. The bulk modulus of the wurtzite crystal is given by B=
2 (C11 + C12 ) C33 − 2 C13 . C11 + C12 + 2 C33 − 4 C13
(5.69)
5.3.3 Biaxial Strain In heteroepitaxy (cf. Sect. 12.2.6), a biaxial strain situation arises, i.e. layered material is compressed (or expanded in the case of tensile strain) in the interface plane and is expanded (compressed) in the perpendicular direction. Here, we assume that the substrate is infinitely thick, i.e. that the interface remains planar. Substrate bending is discussed in Sect. 5.3.5. The simplest case is epitaxy on the (001) surface, i.e. e1 = e2 = . The component e3 is found from the condition σ3 = 0 (no forces in the z direction). All shear strains are zero. For zincblende material it follows
138
5 Mechanical Properties
(b)
(a)
Fig. 5.24 Ratio −⊥ / for GaAs under symmetric biaxial strain. The angle θ denotes the surface normal in the 110 azimuth (θ = 0: [001], θ = 90◦ : [110], the maximum of ⊥ / is for [111]). (b) Is a threedimensional visualization
100 ⊥ = e3 = −
C12 2 C12 (e1 + e2 ) = − . C11 C11
(5.70)
In Fig. 5.24 the ratio ⊥ / is depicted for GaAs and various crystal orientations; the formulas for other orientations are more involved [363]: 2C12 − C0 /2 C11 + C0 /2 2C12 − 2C0 /3 =− . C11 + 2C0 /3
110 ⊥ =−
(5.71)
111 ⊥
(5.72)
For wurtzite crystals and pseudomorphic growth along [00.1] the strain along the epitaxial direction (caxis) is given by ⊥ = −
C13 2C13 (e1 + e2 ) = − a , C33 C33
(5.73)
where ⊥ = c = (c − c0 )/c0 and a = (a − a0 )/a0 . For symmetric biaxial inplane strain, the ratio ⊥ / is shown in Fig. 5.25 for GaN and varying angle θ of the caxis against the epitaxy direction. For the growth of wurtzite on wurtzite for θ = 0, the epitaxial strain is actually asymmetric in the interface plane. For θ = 90◦ , e.g. the epitaxy on mplane substrate (cmp. Fig. 3.33) (caxis lies inplane), the inplane strains are e1 = a and e2 = c . For θ = 90◦ , we find ⊥ = −
C12 a + C13 c . C11
(5.74)
5.3 Elasticity
(a)
139
(b)
Fig. 5.25 Ratio −⊥ / for GaN under symmetric biaxial strain. In (a) θ denotes the angle of the caxis with respect to the surface normal, (b) is a threedimensional visualization, showing the inplane isotropy Fig. 5.26 Strains c (dashed lines) and ⊥ (solid lines) for Al0.17 Ga0.83 N/GaN (blue) and Mg0.3 Ga0.7 O/ZnO (red) as a function of the interface tilt angle θ with respect to [00.1]
The situation for pseudomorphic growth in the (Al,Ga,In)N system has been discussed for various interface orientations in [364] (cmp. also Fig.15.14). The strains ⊥ along the epitaxy direction and c along the cdirection are depicted for Al0.17 Ga0.83 N/GaN and Mg0.3 Ga0.7 O/ZnO in Fig. 5.26. The different behavior of the nitride and the oxide system, e.g. regarding the sign change of c , is due to the fact that a is negative (positive) for Alx Ga1−x N/GaN (Mgx Ga1−x O/ZnO) (c < 0 for both cases) [365].
5.3.4 ThreeDimensional Strain The strain distribution in twodimensional or threedimensional objects such as quantum wires and dots (see also Sect. 14) is more complicated.
140
5 Mechanical Properties
A simple analytical solution for the problem of a strained inclusion is only possible for isotropic material parameters [366]. The solution for a sphere can be extended to yield the strain distribution of an inclusion of arbitrary shape. This scheme applies only for isotropic materials and identical elastic properties of the inclusion and the surrounding matrix. The solution will be given in terms of a surface integral of the boundary of the inclusion, which is fairly easy to handle. Several disconnected inclusions can be treated by a sequence of surface integrals. The strain distribution for the inner and outer parts of a sphere with radius ρ0 is given (in spherical coordinates) by 2 0 3 2 = 0 3
in ρρ = out ρρ
1 − 2ν in = in θθ = φφ 1−ν 1 + ν ρ0 3 out = −2out θθ = −2φφ , 1−ν ρ
(5.75) (5.76)
where ρ denotes the radius, ν the Poisson ratio, and 0 the relative lattice mismatch of the inclusion and the matrix. The radial displacements are 2 0 3 2 = 0 3
u in ρ = u out ρ
1 − 2ν ρ 1−ν 1 − 2ν 3 1 . ρ 1 − ν 0 ρ2
(5.77) (5.78)
Dividing the displacement by the sphere’s volume, we obtain the displacement per unit volume of the inclusion. From the displacement we can derive the stress σi0j per unit volume. 1 Y 0 2xi2 − x j − xk 4π 1 − ν ρ5 3 1 Y 0 xi x j , σi0j = 2 4π 1 − ν ρ5 σii0 =
(5.79) (5.80)
where i, j and k are pairwise unequal indices. Due to the linear superposition of stresses, the stress distribution σiVj for the arbitrary inclusion of volume V can be obtained by integrating over V σiVj
= V
σi0j (r − r0 ) d3 r.
(5.81)
The strains can be calculated from the stresses. When 0 is constant within V , the volume integral can be readily transformed into an integral over the surface ∂V of V using Gauss’ theorem. With the ‘vector potentials’ Ai j we fulfill divAi j = σi j .
5.3 Elasticity
141
Fig. 5.27 Strain components in an InAs pyramid (quantum dot with {101} faces), embedded in GaAs. The cross section is through the center of the pyramid. The lattice mismatch between InAs and GaAs amounts to ≈ −7 %. Reprinted with permission from [367], © 1995 APS
1 Y 0 xi ei 4π 1 − ν ρ3 1 1 Y 0 xi e j + x j ei . Ai j = − 2 4π 1 − ν ρ3 Aii = −
(5.82) (5.83)
Equation (5.83) is valid for the case i = j. ei is the unit vector in the ith direction. However, special care must be taken at the singularity r = r0 if r0 lies within V because the stress within the ‘δinclusion’ is not singular (in contrast to the electrostatic analog of a δcharge). Thus, we find σiVj (r0 ) =
∂V
Ai j dS + δi j
Y 0 1−ν
δ(r − r0 ) d3 r.
(5.84)
V
As an example, we show in Fig. 5.27 the numerically calculated strain components [367] (taking into account the different elastic properties of the dot and matrix materials) in the cross section of a pyramidal InAs quantum dot in a GaAs matrix on top of a twodimensional InAs layer. The strain component zz is positive in the 2D layer, as expected from (5.70). However, in the pyramid zz exhibits a complicated dependence and even takes negative values at the apex.
5.3.5 Substrate Bending If a latticemismatched layer is pseudomorphically grown on top of a substrate it suffers biaxial strain. For finite substrate thickness part of the strain will relax via substrate bending. If the substrate is circular, a spherical cap is formed. If the lattice constant of the film is larger (smaller) than that of the substrate, the film is under compressive (tensile) strain and the curvature is convex (concave) with respect to
142
5 Mechanical Properties
(b) au (a)
compressive
tensile
d ai R
Fig. 5.28 (a) Schematic bending of a film/substrate system for compressive (left) and tensile (right) film strain. (b) Schematic deformation of curved film of thickness d. The lattice constants at the inner and outer surface are ai and au , respectively
the outward normal given by the growth direction (Fig. 5.28a). Substrate bending f and can also be induced by a mismatch of the thermal expansion coefficients αth s αth of the film and substrate, respectively. If a film/substrate system is flat at a given temperature, e.g. growth temperature, a decrease of temperature, e.g. during cooling, f s is smaller (larger) than αth . will lead to compressive (tensile) strain if αth In a curved structure, the lattice constant in the tangential direction increases from ait at the inner surface (r = R = κ−1 ) to aut at the outer surface (r = R + d). Thus, the tangential lattice constant varies with the radial position a t (r ) = ait (1 + r κ) ,
(5.85)
where d is the layer thickness (Fig. 5.28b). Therefore au = ai (1 + d/R). We note that (5.85) holds in all layers of a heterostructure, i.e. the film and the substrate. The lattice constant in the radial direction a r , however, depends on the lattice constant a0 of the local material and is calculated from the biaxial strain condition, such as (5.70). The inplane strain is = (a t − a0 )/a0 (we assume a spherical cap with = θθ = φφ ). For an isotropic material we find a r = a0 (1 + ⊥ ) with ⊥ = −2ν /(1 − ν). The local strain energy density U is given by U=
Y 2 . 1−ν
(5.86)
The total strain energy per unit area U of a system of two layers with lattice constants a1 , a2 , Young’s moduli Y1 , Y2 and thickness d1 , d2 (we assume the same Poisson constant ν in both layers) is
U = 0
d1
U1 dr +
d2
U2 dr.
(5.87)
d1
The total strain energy needs to be minimized with respect to ai and R in order to find the equilibrium curvature κ. We find
5.3 Elasticity epitaxy
1100
cooling 0.05
0.05
1070
0.1
1060 1050
0.0
1
6K
1080
Curvature (m )
1090 Temperature (°C)
Fig. 5.29 Curvature of the middle of a Si wafer during GaN growth on an AlN interlayer grown at low temperatures on GaN and subsequent cooling. During growth the decrease in curvature indicates convex bowing due to compressive stress; during cooling the wafer flattens and becomes concave due to thermally induced tensile stress. Adapted from [372]
143
0
200 400 600 800 1000 1200 1400 Time (s)
6a1 a2 (a2 − a1 ) d1 d2 (d1 + d2 ) Y1 Y2 a23 d14 Y12 + α Y1 Y2 + a13 d24 Y24 α = a1 a2 d1 d2 −a2 d1 (2d1 + 3d2 ) + a1 (6d12 + 9d1 d2 + 4d22 ) . κ=
0.15
(5.88)
For a2 = a1 (1 + ) we develop κ to first order of and find (χ = Y2 /Y1 ) [368, 369] 6χ d1 d2 (d1 + d2 ) . (5.89) κ= 4 d1 + 4χ d13 d2 + 6χ d12 d22 + 4χ d1 d23 + χ2 d24 In the case of a substrate (ds ) with a thin epitaxial layer (df ds ), the radius of curvature is approximately (Stoney’s formula [370]) κ = 6
df Yf . ds2 Ys
(5.90)
Conversely, if the radius of curvature is measured [371], e.g. optically, the film curvature (and through models also the film strain) can be determined during epitaxy as depicted in Fig. 5.29.
5.3.6 Scrolling In some cases cylindrically scrolled structures are important, e.g. for thinfilm flexible electronics, nanotubes, nanoscrolls or nanohelixes. The scrolling of thin layers must be avoided by suitable strain management for thin layers that are lifted off from their substrate for transfer to another flat substrate. If the film remains attached to its substrate, a scroll can be fabricated as schematically shown in Fig. 5.30. Such structures were first reported in [373], a review can be found in [374]. The shape of such scroll is investigated in [375] without a priori assumptions on its shape.
144
5 Mechanical Properties
(c)
(b)
(a)
Fig. 5.30 Schematic representation of nanoscroll formation. (a) Strained heterostructure (blue/green) that is planar due to large substrate thickness, (b) starting removal of sacrificial layer (black), (c) release of thin film into nanoscroll geometry
If bending strain occurs only in one of the tangential directions, the energy density is given by Y U= (5.91) (2 + 2y + 2ν t y ), 2 (1 − ν 2 ) t where y is the strain in the unbent direction (cylinder axis) as shown in Fig. 5.31a. For a strained heterostructure made up from two layers the curvature is given by (calculated analogous to (5.89), χ = Y2 /Y1 [369]) κ=
6(1 + ν) χ d1 d2 (d1 + d2 ) , d14 + 4χ d13 d2 + 6χ d12 d22 + 4χ d1 d23 + χ2 d24
(5.92)
which differs from (5.89) only by the factor 1 + ν in the nominator. For cubic material and a (001) surface the energy is given as U100 =
C11 − C12 C11 (2t + 2y + C12 (t + y )2 ) 2C11
(b)
(a)
(5.93)
(a)
y t r
(b)
(c)
Fig. 5.31 (a) Schematic representation of a cylindrically rolled sheet with radial direction r , tangential direction t and direction along the cylinder axis y. (b) SEM images of multiwall InGaAs/GaAs nanoscroll rolled up over about 50 µm. Part (b) from [376]
5.3 Elasticity
145
(b)
(a)
=14° [010]
[100]
Fig. 5.32 (a) Strain energy (in units of the strain energy of the flat pseudomorphic layers) of a scroll of a 4layer SiGe structure (Si0.3 Ge0.7 , Si0.6 Ge0.4 and Si0.8 Ge0.2 , each 3 nm thick and a 1nm Si cap) as a function of radius for winding directions along 100 and 110 . Top (bottom) curves without (with complete) strain relaxation along the cylinder axis. Vertical lines indicate the positions of the respective energy minima [369]. (b) SEM image of curled InGaAs/GaAs nanoscroll rolled φ = 14◦ off 100 . The stripe from which the film was rolled off is indicated by white dashed lines. Part (b) from [379]
for a scrolling direction along 100 . When the (001)oriented film winds up along a direction hk0 having an angle φ with the [100] direction (φ = 45◦ for 110 ), the strain energy is given by (C0 is given by (5.62)) Uφ = U100 + C0
t − y 2
2 sin2 (2φ).
(5.94)
The strain energy versus bending radius (= κ−1 ) is shown for a SiGe nanoscroll in Fig. 5.32. First, the relaxation along the cylinder axis plays a minor role. The smallest strain energy is reached for scrolling along 100 , also yielding the smaller bending radius (larger curvature). Therefore, the film preferentially scrolls along 100 . This explains the observed ‘curl’ behavior of scrolls winding up for φ = 0 [373, 377] (Fig. 5.32b). The effect of surface strain needs to be included to yield improved quantitative agreement with experimental values of κ(, d) [378].
5.4 Plasticity 5.4.1 Critical Thickness Strained epitaxial films are called pseudomorphic when they do not contain defects and the strain relaxes elastically, e.g. by tetragonal distortion. When the layer thick
146
(a)
5 Mechanical Properties
(b)
g 002
Fig. 5.33 (a) Series of crosssectional TEM images of 100nm thick Gex Si1−x layers on Si(001) with different ternary compositions x = 0.1, 0.2, 0.5, and 1.0. The growth temperature was 550◦ C. The transition from commensurate to incommensurate growth is obvious. Adapted from [380]. (b) Plan view 022 TEM bright field image of a 250nm Ge0.15 Si0.85 layer on Si (001), annealed at about 700◦ C. The arrow denotes the position of a dislocation loop. Reprinted with permission from [381], © 1989 AVS
ness increases, however, strain energy is accumulated that will lead at some point to plastic relaxation via the formation of defects. In many cases, a grid of misfit dislocations forms at the interface (Figs. 4.18 and 5.33). In Fig. 5.34 the strain around misfit dislocations at a GaAs/CdTe heterointerface, as calculated from a TEM image (Fig. 4.14), is shown.
xz of the strain tensor (with respect to the GaAs lattice constant) of Fig. 5.34 Components xzxx zz the dislocation array shown in Fig. 4.14, red/blue: positive/negative value, white: zero. From [286]
5.4 Plasticity
147
(a)
(b)
c
h3
b
h2 h1
a c
b
a
Fig. 5.35 Schematic formation of misfit dislocations by (a) elongation of a grownin threading dislocation and (b) by the nucleation and growth of dislocation halfloops. (a) depicts a threading dislocation. Initially, for thickness h 1 the interface is coherent ‘a’, for larger thickness h 2 the interface is critical and the force of the interface on the dislocation is equal to the tension in the dislocation line, ‘b’. For larger thickness, e.g. h 3 , the dislocation line is elongated in the plane of the interface, ‘c’. In (b) ‘a’ denotes a subcritical dislocation halfloop, ‘b’ depicts a halfloop being stable under the misfit stress and for ‘c’ the loop has grown under the misfit stress into a misfit dislocation line along the interface
The average distance p of the dislocations is related to the misfit f = (a1 −a2 )/a √ 2 and the edge component b⊥ of the Burger’s vector (for a 60◦ dislocation b⊥ = a0 / 8) p=
b⊥ . f
(5.95)
Two mechanisms have been proposed for the formation of misfit dislocations (Fig. 5.35), the elongation of a grownin threading dislocation [382] and the nucleation and growth of dislocation halfloops [383]. For the modeling of such systems a mechanical approach based on the forces on dislocations [382] or an energy consideration based on the minimum strain energy necessary for defect formation [383–386] can be followed. Both approaches have been shown to be equivalent [387] (if a periodic array of dislocations is considered). In [388] it was pointed out that the finite speed of plastic flow also has to be considered to explain experimental data. Temperature affects the observed critical thickness and a kinetic model is needed. Another way of introducing dislocations is the plastic relaxation at the edge of coherent strained islands (cmp. Fig. 14.26). In the following, isotropic materials and identical elastic constants of substrate and thin film are assumed, following [387]. The interface plane is the (x,y)plane, the growth direction is z. The energy E d of a periodic dislocation array with period p and Burgers vector b = (b1 , b2 , b3 ) is Ed = β = 2
Y β2 8π (1 − ν 2 )
b12
+ (1 −
ν) b22
+
b32
ln
p 1 − exp(−4πh/ p) 2π q
148
5 Mechanical Properties
4πh exp(−4πh/ p) + b12 − b32 p 1 − exp(−4πh/ p) 4πh 2 1 2 exp(−4πh/ p) 2 − b1 + b3 2 2 p 1 − exp(−4πh/ p) 2πh exp(−2πh/ p) + b32 , p 1 − exp(−2πh/ p)
(5.96)
where h is the film thickness and q denotes the cutoff length for the dislocation core, taken as q = b. The misfit strain including the relaxation due to dislocations with ˆ We Burger’s vectors b and bˆ in the two orthogonal interface 110 directions n and n. chose the coordinate system such that n = (1, 0, 0) and nˆ = (0,1, 0) (the z direction √ remains). With respect to these axes the Burger’s vectors are ± 21 , 21 , √12 a0 / 2. The misfit strain imj is reduced due to the dislocation formation to the ‘relaxed’ misfit strain ir j with bi n j + b j n i bˆi nˆ j + bˆ j nˆ i ir j = imj + + , (5.97) 2p 2p with an associated stress σi j . The strain energy E s of the layer due to the relaxed misfit is then 1 h σi j ir j 2 Y (1 + ν) 2 f . lim E s = 2h p→∞ 1−ν Es =
(5.98) (5.99)
The total strain energy E is given by pE = 2E d + 2E c + p E s E ∞ = lim E, p→∞
(5.100) (5.101)
with the core energy E c of the dislocation that needs to be calculated with an atomistic model (not considered further here). This energy is shown in Fig. 5.36a for the material parameters of Ge0.1 Si0.9 /Si(001) (misfit −0.4%) for various layer thicknesses as a function of 1/ p. This plot looks similar to that for a firstorder phase transition (with 1/ p as the order parameter). For a certain critical thickness h c1 the energy of the layer without any dislocation and the layer with a particular dislocation density p1 are identical (E − E ∞ = 0) and additionally ∂ E/∂ p p= p1 = 0. However, between p → ∞ and p = p0 there is an energy barrier. The critical thickness h c2 is reached when (5.102) ∂ E/∂ p  p→∞ = 0,
5.4 Plasticity
149
(b)
(a)
Fig. 5.36 (a) Theoretical calculation for the strain energy versus inverse dislocation density for various thicknesses of Ge0.1 Si0.9 layers on Si (001). The ordinate is b/2 p, b/2 being the edge component of the Burgers vector and p being the dislocation spacing. The abscissa is the strain energy E scaled with E ∞ (5.101). (b) Critical thickness for Gex Si1−x layers on Si (001). The solid line is theory (h c2 ) according to (5.103). Data points are from [389] (squares, growth temperature of 750 ◦ C) and from [380] (triangles for growth temperature of 550 ◦ C)
i.e. the energy decreases monotonically for increasing dislocation density up to the global energy minimum at a certain equilibrium dislocation spacing p2 . Equation (5.102) leads to the following implicit equation for the determination of h c2 : h c2
b −16 + 3b2 + 8 (−4 + ν) ln (2h c2 /q) = , 128 f π (1 + ν)
(5.103)
√ with the length of the Burgers vector b = a0 / 2. The theoretical dependence of h c2 for Gex Si1−x /Si(001) with varying composition is shown in Fig. 5.36b together with experimental data. The critical thickness for a fairly high growth temperature is much closer to the energetic equilibrium than that deposited at lower temperature. This shows that there are kinetic limitations for the system to reach the mechanical equilibrium state. Also, the experimental determination of the critical thickness is affected by finite resolution for large dislocation spacing, leading generally to an overestimate of h c . In zincblende materials two types of dislocations are possible, α and β, with ¯ Ga and Asbased cores, respectively. They have [110] and [110] line directions for a compressively strained interface. The α dislocation has the larger glide velocity. Therefore, strain relaxation can be anisotropic with regard to the 110 directions for zincblende material, e.g. InGaAs/GaAs [390, 391].
150
5 Mechanical Properties
5.4.2 Cleaving The cleavage planes of the diamond structure are {111} planes (Fig. 5.37a). It is easiest to break the bonds connecting the double layers in the 111 directions. The cleavage planes of the zincblende structure are {110} planes (Fig. 5.37b). Due to the ionic character, breaking the bonds connecting the double layers in the 111 directions would leave charged surfaces, which is energetically unfavorable. The {100} planes contain only one sort of atom and would also leave highly charged surfaces. The {110} planes contain equal amounts of A and B atoms and are neutral. Ideally, the cleaving plane is atomically flat (Fig. 5.38a) or exhibits large monoatomically flat terraces. However, certain dopants in high concentrations, e.g. GaAs:Te, can induce a rough surface due to lattice distortion [392]. ¯ (mtype) planes [393]. The natural cleavage planes of wurtzite (GaN) are {11.0}
(b)
(a)
Fig. 5.37 Cleaving planes of the (a) diamond and (b) zincblende lattice
(b)
(a)
10 nm Fig. 5.38 Scanning tunneling microscopy images of a cleaved GaAs (110) surface with (a) good cleave and (b) bad cleave with defects dominating. Adapted from [394]
5.4 Plasticity
151
5.4.3 Wafer Breakage The thickness and thus strength of wafers for semiconductor production (cmp. Sect. 12.2.2) is an important issue. The wafer should be as thin as possible for saving expensive materials but thick enough to avoid loss due to stress during handling, in particular during the later steps in a process since the value of a wafer increases with number of process steps it has undergone. Reasons for wafer breakage is the mechanical handling (pick, place, transport) [395], stress loads due to processing (dielectrics, metals, asymmetric structures) and stress during processing for example due to thermal loads in annealing or deposition steps and cutting/dicing. The problem is less important in microelectronics but especially severe in photovoltaics (PV) industry, handling large total areas; on the other hand the profit loss per broken wafer is much higher in microelectronics industry. An additional problem poses the grain structure of multicrystalline silicon wafers used for PV [396] and the effect of surface cracks and irregularities at wafer edges and corners. Just going from a wafer thickness of 270 to 250 µm can more than double the breakage rate at certain process steps [397]. The minimum strength of a wafer with surface cracks is about 100 MPa, while the strength of wafers with cracks at the edge can reach rather low values around 20 MPa. Also the careful shaping of the wafer edge is important to avoid breakage [398].
Chapter 6
Band Structure
Silicon is a metal. A.H. Wilson, 1931 [67]
Abstract A treatment of electron states in onedimensional potentials introduces into the concepts of band gap and effective mass. The band structures of various semiconductors are reviewed. The systematics of band gaps, symmetry considerations, band gaps in alloys, amorphous semiconductors and the effect of strain and temperature are discussed. Electron and hole dispersions are treated and the density of states in various dimensions is derived.
6.1 Introduction Valence electrons that move in the crystals feel a periodic potential U (r) = U (r + R)
(6.1)
for all vectors R of the direct lattice. The potential1 is due to the effect of the ion cores and all other electrons. Thus a serious manybody problem is present. In principle, the band structure can be calculated from the periodic arrangements of the atoms and their atomic order number. We note that for some problems, e.g. the design of optimal solar cells, a certain band structure is known to be ideal and a periodic atomic arrangement, i.e. a material, needs to be found that generates the optimal band structure. This problem is called the inverse band structure problem.
1 In
this book the form of the potential will never be explicitly given.
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_6
153
154
6 Band Structure
6.2 Electrons in a Periodic Potential 6.2.1 Bloch’s Theorem First, we will deduce some general conclusions about the structure of the solution as a consequence of the periodicity of the potential. We first investigate the solution of a Schrödinger equation of the type 2 2 ∇ + U (r) Ψ (r) = E Ψ (r) H Ψ (r) = − 2m
(6.2)
for an electron. U will be periodic with the lattice, i.e. it will obey (6.1). Bloch’s theorem says that the eigenstates Ψ of a oneparticle Hamiltonian as in (6.2) can be written as the product of plane waves and a latticeperiodic function, i.e. Ψnk (r) = A exp(i k r) u nk (r).
(6.3)
The normalization constant A is often omitted. If u nk (r) is normalized, A = √ 1/ V , where V is the integration volume. The wavefunction is indexed with a quantum number n and the wavevector k. The key is that the function u nk (r), the socalled Bloch function, is periodic with the lattice, i.e. u nk (r) = u nk (r + R)
(6.4)
for all vectors R of the direct lattice. The proof is simple in one dimension and more involved in three dimensions with possibly degenerate wavefunctions, see [399]. If E nk is an energy eigenvalue, then E nk+G is also an eigenvalue for all vectors G of the reciprocal lattice, i.e. E n (k) = E n (k + G).
(6.5)
Thus the energy values are periodic in reciprocal space. The proof is simple, since the wavefunction (for k + G) exp (i(k + G)r) u n(k+G) (r) is for u n(k+G) (r) = exp (−iGr) u nk (r) obviously an eigenfunction to k. A band structure along one kdirection can be displayed in various zone schemes as depicted in Fig. 6.1. The most frequently used scheme is the reduced zone scheme. In three dimensions, the band structure is typically shown along particular paths in the Brillouin zone, as depicted, e.g., in Fig. 6.2c.
6.2 Electrons in a Periodic Potential
155
(b)
(a)
(c)
Fig. 6.1 Zone schemes for a band structure: (a) extended, (b) reduced and (c) repetitive zone scheme
(a)
(b)
(c)
X
4 3 2 1 0 X
W
L
K X
Fig. 6.2 Dispersion of free electrons (empty lattice calculation, U = 0, shown in the first Brillouin zone) in (a) a onedimensional lattice (G = n 2π/a), (b) a simple cubic lattice (G = (h, k, l) 2π/a) and (c) in a fcc lattice. The energy is measured in units of the energy at the Xpoint, E X = (2 /2m)(2π/a)2 . The shaded circle in (c) represents the region where the band gap develops for finite periodic potential U = 0
6.2.2 FreeElectron Dispersion If the entire wavefunction (from (6.3)) obeys the Schrödinger equation (6.2), the Bloch function u nk fulfills the equation 1 (6.6) (p + k)2 + U (r) u nk (r) = E nk u nk (r), 2m which is easy to see from p = −i∇. First, we discuss the simplest case of a periodic potential, U ≡ 0. This calculation is also called the empty lattice calculation. The solution of (6.6) is then just constant,
156
6 Band Structure
i.e. u k = c and Ψk (r) = c exp (ikr). The dispersion of the free electron is then given by 2 2 (6.7) k , E(k) = 2m where k is an arbitrary vector in the reciprocal space. k is a vector from the Brillouin zone such that k = k + G with a suitable reciprocal lattice vector G. Because of (6.5) the dispersion relation can be written also as E(k) =
2 (k + G)2 , 2m
(6.8)
where k denotes a vector from the Brillouin zone. Thus, many branches of the dispersion relation arise from using various reciprocal lattice vectors in (6.8). The resulting dispersion relation for the free electron is shown in Fig. 6.2a for a onedimensional system (k and G are parallel) and in Fig. 6.2b for the simple cubic lattice (in the socalled reduced zone scheme). In Fig. 6.2c, the (same) dispersion of the free electron is shown for the fcc lattice.
6.2.3 NonVanishing Potential Now the effect of a nonvanishing periodic potential on electron motion will be discussed. A simple, analytically solvable model that visualizes the effect of a periodic potential on the dispersion relation of the electrons and the formation of a (onedimensional) band structure with gaps is the Kronig–Penney model [64] which is discussed in the Appendix F. General Wave Equation In this section, we will discuss the solution of a general wave equation for electrons in a periodic potential. The solution is investigated particularly at the zone boundary. The potential U is periodic with the lattice (6.1). It can be represented as a Fourier series with the reciprocal lattice vectors (lattice vector expansion, cf. (3.18)): U (r) =
UG exp (i G r) .
(6.9)
G
Since U is a real function, U−G = UG∗ . The deeper reason for the success of such an approach is that for typical crystal potentials, the Fourier coefficients decrease rapidly with increasing G, e.g. for the unscreened Coulomb potential UG ∝ 1/G 2 . The wavefunction is expressed as a Fourier series (or integral) over all allowed (Bloch) wavevectors K,
6.2 Electrons in a Periodic Potential
157
Ψ (r) =
CK exp (i K r) .
(6.10)
K
The kinetic and potential energy terms in the Schrödinger equation (6.6) are ∇ 2Ψ = −
K2 CK exp (i K r)
(6.11a)
K
UΨ =
G
UG CK exp (i (G + K) r) .
(6.11b)
K
With K = K + G, (6.11b) can be rewritten as UΨ =
G
UG CK −G exp i K r .
(6.12)
K
Now, the Schrödinger equation can be written as an (infinite) system of algebraic equations: UG CK−G = 0, (6.13) (λK − E) CK + G
with λK = 2 K2 /(2m). Solution for One Fourier Coefficient The simplest (nontrivial) potential energy has only one important Fourier coefficient U for the shortest reciprocal lattice vector G. Also, we have U−G = UG . Thus, the (onedimensional) potential has the form U (x) = 2 U cos(Gx). Then the equation system (6.13) has only two equations for CK and CK−G , leading to the condition λK − E U = 0. U λK−G − E
(6.14)
We find two solutions λK + λK−G ± E± = 2
λK − λK−G 2
2 + U 2.
(6.15)
Solution at the Zone Boundary We consider the solution at the zone boundary, i.e. at K = G/2. The kinetic energy is then the same for K = ±G/2, i.e. λK = λK−G = (2 /2m) (G 2 /4) = λ. The determinant (6.14) reads then (λ − E)2 − U 2 = 0.
(6.16)
158
6 Band Structure
Fig. 6.3 Periodic potential U (onedimensional cosine, black) and the squares of the wavefunctions Ψ− (red) and Ψ+ (blue) for the wavevector at the zone boundary, K = G/2 = π/a
Thus the energy values at the zone boundary are E± = λ ± U =
2 G 2 ± U. 2m 4
(6.17)
At the zone boundary, a splitting of the size E + − E − = 2U occurs. The center of the energy gap is given by the energy λK of the freeelectron dispersion. The ratio of the coefficients is CG/2 /C−G/2 = ∓1. The ‘−’ solution of (6.17) (lower energy) is a standing cosine wave (Ψ− ), the ‘+’ solution (Ψ+ ) is a standing sine wave as visualized in Fig. 6.3. For the lowerenergy (binding) state the electrons are localized at the potential minima, i.e. at the atoms, for the upper state (antibinding) the electrons are localized between the atoms. Both wavefunctions have the same periodicity since they belong to the same wavevector K = G/2. We note that the periodicity of Ψ is 2a, while the periodicity of Ψ 2 is equal to the lattice constant a. Gap States For energies within the gap, solutions with a complex wavevector K = G/2 + i q exist. Solving (6.16) results (in terms of q 2 = (2 /2m) q 2 ) to E± = λ − q ± 2
−4 λ q 2 + U 2 .
(6.18)
For energies E = λ + with −U ≤ ≤ U , the complex part of the wavevector is given by (6.19) q 2 = −( + 2λ) + 4λ ( + λ) + U 2 . The maximum value of q is in the center of the band gap ( = 0); for U  2 λ, it is q 2max ≈ U 2 /(4λ). At the band edges ( = ±U ), q = 0. q is the characteristic length of an exponentially decaying wave function. Such solutions occur at surfaces or interfaces. For larger band gaps, the localization length is smaller (larger q) (Fig. 6.4).
6.2 Electrons in a Periodic Potential Fig. 6.4 Complex band structure q () according to (6.19) for two different values of λ/U
159
Complex wavevector q'
0.25 =5U
0.2
0.15
=10U
0.1
0.05
0
1
0.5
0
0.5
1
/U
Solution in the Vicinity of the Zone Boundary For K in the vicinity of the zone boundary the solutions (6.15) can be developed.
= K − G/2. With Therefore, we use the (small) distance from the zone boundary K 2 2 λ = ( /2m) (G /4) we rewrite still exactly (6.15): 2
= E± K 2m
with For small K
2 GK 2m
1/2
2 1 2 2 2 K 2 . G + K ± 4λ +U 4 2m
(6.20)
U , the energy is then approximately given by
2 2 K
∼ E± K = λ±U + 2m
1±
2λ . U
(6.21)
Thus the energy dispersion in the vicinity of the zone boundary is parabolic. The lower state has a negative curvature, the upper state a positive curvature. The curvature is 1 U ≈ ±m , (6.22) m∗ = m 1 ± 2λ/U 2λ and will be later related to the effective mass. The approximation in (6.22) is valid for U  2λ. We note that in our simple model m ∗ increases linearly with increasing band gap 2U (see Fig. 6.28 for experimental data).
6.2.4 Kramer’s Degeneracy E n (k) is the dispersion in a band. The timereversal symmetry (Kramer’s degeneracy) implies
160
6 Band Structure
Fig. 6.5 Theoretical calculation of the spin splitting of (a) the three lowest conduction bands (CB1, CB2, and CB3) and (b) the top three valence bands (VB1, VB2, and VB3) of GaAs. Adapted from [401]
(a)
120
GaAs
100 80
Spin splitting (meV)
60 40 20 0
(b)
120 100 80 60 40 20 0 X
U,K
E n↑ (k) = E n↓ (−k),
W
(6.23)
where the arrow refers to the direction of the electron spin. If the crystal is symmetric under inversion, we have additionally E n↑ (k) = E n↑ (−k).
(6.24)
With both time reversal and inversion symmetry the band structure fulfills E n↑ (k) = E n↓ (k).
(6.25)
The inversion symmetry is particularly important for the spinorbit interaction. In the absence of inversion symmetry, e.g. in (noncentrosymmetric) zincblende crystals (Fig. 3.16b) or in heterostructures (Fig. 12.34b), a spin splitting, e.g. E n↑ (k) = E n↓ (k), is present. It can be thought of as provoked by an effective magnetic field. Bulk inversion asymmetry (BIA) leads to the Dresselhaus spin splitting [400, 401] that is shown in Fig. 6.5 for GaAs (cmp. Fig. 6.7a). The spin splitting due to structural inversion asymmetry (SIA) is described by the BychkovRashba Hamiltonian [402, 403]. A review on these topics can be found in [404].
6.2.5 Symmetry Considerations In general the symmetry of the lattice is a symmetry of the system’s Hamiltonian and thus transfers into the electronic (and other) properties of the semiconductor.
6.2 Electrons in a Periodic Potential
161
The means to formulate this mathematically is group theory. At a given reciprocal lattice point, the wave function must fulfill the given spatial symmetry. Additional symmetry due to spin and spinorbit interaction enters via the doublegroup scheme. This problem has been treated for the 32 point groups (cmp. Table B.2) in [405] and in [406] particularly for the pc, fcc, bcc and hcp lattices. A detailed treatment for the zincblende structure has been given in [407]. The symmetry at particular lattice points is denoted by the irreducible representations of the symmetry group, e.g. by the Γi symbols used in Figs. 6.6, 6.7 or also Fig. 6.38. As an example base functions with the symmetry of the irreducible representations of tetraeder group
(b)
(a) 6
Ge
4 2
Si
4 0
Energy (eV)
Energy (eV)
2 0 2 4
2 4 6
6
8
8 10
10
12
12
L
L
X U,K
X U,K
Fig. 6.6 Band structure of (a) silicon (indirect) and (b) germanium (indirect). In Si, the minima of the conduction band are in the 100 direction, for germanium in the 111 direction. Adapted from [146], based on [409]
(a)
6
GaAs
(b)
4
4
2
2
0
Energy (eV)
Energy (eV)
GaP
6
2 4 6 8
0 2 4 6 8
10
10
12
12
L
X U,K
L
X U,K
Fig. 6.7 Band structure of (a) GaAs (direct) and (b) GaP (indirect). For GaAs the minimum of the conduction band is at Γ , for GaP in the 100 direction. Adapted from [146], based on [409]
162
6 Band Structure X 15
W
15
GaN
10
10
5
5
0
0
5
5
w
zb 10
Fig. 6.8 Band structure of GaN (direct) in zincblende (zb) modification (left) and wurtzite (w) modification (right), both displayed in the wurtzite Brillouin zone to facilitate comparison Table 6.1 Representations of the tetraeder group (zincblende structure) in molecular, BSW [408] and Koster [405] notation and corresponding base functions (c.p.: cyclic permutations) Molecular BSW Koster Base functions A1 A2 E T2 T1
Γ1 Γ2 Γ12 Γ15 Γ25
Γ1 Γ2 Γ3 Γ4 Γ5
x yz x 4 (y 2 − z 2 ) + c.p. 2 z 2 − (x 2 + y 2 ), (x 2 − y 2 ) x, y, z z (x 2 − y 2 ) and c.p.
are listed in Table 6.1. With the knowledge of the wave functions at the points of high symmetry, it is possible to deduce the general nature of the energy bands in the vicinity of such symmetry points.
6.3 Band Structures of Selected Semiconductors In the following, the band structures of various important and prototype semiconductors are discussed. The band below the energy gap is called the valence band; the band above the gap is the conduction band. The band gap ΔE cv , mostly denoted as E g , is the energy separation between the highest valenceband state and the lowest conductionband state. The maximum of the valence band is for most semiconductors at the Γ point.
6.3 Band Structures of Selected Semiconductors
163
6.3.1 Silicon For silicon, an elemental semiconductor, (Fig. 6.6a) the minimum of the conduction band is located close to the X point at 0.85π/a in the 100 direction. Thus, it is not at the same point in k space as the top of the valence band. Such a band structure is called indirect. Since there are six equivalent 100 directions, there are six equivalent minima of the conduction band.
6.3.2 Germanium Germanium, another elemental semiconductor, (Fig. 6.6b) also has an indirect band structure. The conduction minima are at the L point in the 111 direction. Due to symmetry there are eight equivalent conductionband minima.
6.3.3 GaAs GaAs (Fig. 6.7a) is a compound semiconductor with a direct band gap since the top of the valence band and the bottom of the conduction band are at the same position in k space (at the Γ point). The next highest (local) minimum in the conduction band is close to the L point.
6.3.4 GaP GaP (Fig. 6.7b) is an indirect compound semiconductor. The conductionband minima are along the 100 directions.
6.3.5 GaN GaN (Fig. 6.8) is a direct semiconductor that has wurtzite structure but can also occur in the metastable cubic (zincblende) phase.
6.3.6 Lead Salts The band gap of PbS (Fig. 6.9), PbSe and PbTe is direct and located at the L point. The lead chalcogenide system shows the anomaly that with increasing atomic weight
164
6 Band Structure
Fig. 6.9 Calculated band structure of PbS (direct). The energy gap is at the L point. The forbidden band is shown in grey. Adapted from [410]
the band gap does not decrease monotonically. At 300 K, the band gaps are 0.41, 0.27 and 0.31 eV for PbS, PbSe and PbTe, respectively.
6.3.7 MgO, ZnO, CdO Cadmium oxide is a cubic semiconductor in the rocksalt structure. Due to symmetry considerations, coupling (repulsion) of oxygen 2p and cadmium 3dorbitals does not occur at the zone center in the rocksalt structure. Repulsion occurs though away from the Γ point and therefore the valence band maximum is not located at the zone center (Fig. 6.10). Thus CdO is an indirect semiconductor. A similar effect would occur in rsZnO due to zinc 3d orbitals; however, ZnO has wurtzite structure for
Fig. 6.10 Calculated indirect band structure of CdO. The top of the valence band is at E = 0. Adapted from [412]
12 10
CdO
8 6 4 2 0 2 4 6
X
K
L
6.3 Band Structures of Selected Semiconductors
165
which p–d coupling at the Γ point is allowed; thus ZnO is direct. In MgO, Mg of course only possesses populated s and porbitals and no such repulsion is present; thus MgO even with its rocksalt structure is also direct [411].
6.3.8 Chalcopyrites The experimental band gaps of a number of chalcopyrite semiconductors are listed in Table 6.2. The band structures of CuAlS2 , CuAlSe2 , and CuGaSe2 are compared in Fig. 6.11.
Table 6.2 Band gaps of various chalcopyrite semiconductors Material E g (eV) E g (eV) CuAlS2 CuAlSe2 CuAlTe2 AgAlS2 AgAlSe2 AgAlTe2 ZnSiP2 ZnSiAs2 CdSiP2 CdSiAs2
3.5 2.71 2.06 3.13 2.55 2.2 2.96 2.12 2.45 1.55
CuGaS2 CuGaSe2 CuGaTe2 AgGaS2 AgGaSe2 AgGaTe2 ZnGeP2 ZnGeAs2 CdGeP2 CdGeAs2
CuAlS 2
T
2.5 1.7 1.23 2.55 1.83 1.1–1.3 2.34 1.15 1.72 0.57
E g (eV) CuInS2 CuInSe2 CuInTe2 AgInS2 AgInSe2 AgInTe2 ZnSnP2 ZnSnAs2 CdSnP2 CdSnAs2
CuGaSe 2
CuAlSe 2
N
T
1.53 1.0 1.0–1.15 1.87 1.24 1.0 1.66 0.73 1.17 0.26
N
T
N
Fig. 6.11 Calculated band structures of CuAlS2 , CuAlSe2 , and CuGaSe2 . The absolute values of the gap energies are incorrect due to LDA calculation. Adapted from [413]
166
6 Band Structure ZnGeN 2
GaN
15 10 5 0 5 10 15
X
Z
U
R
S
Y
X
Z
U
R
S
Y
Fig. 6.12 Calculated (within LDA) band structures of ZnGeN2 and its related III–V compound GaN, both displayed in the chalcopyrite (orthorhombic) Brillouin zone to facilitate comparison. Adapted from [414]
In Fig. 6.12, the theoretical band structure of GaN and its closest related chalcopyrite ZnGeN2 are compared, both shown in the chalcopyrite (orthorhombic) Brillouin zone. The band gap of ZnGeN2 is smaller than that of GaN and the difference of 0.4 eV is fairly well reproduced by the calculation2 (giving 0.5 eV).
6.3.9 Spinels The band structure of spinels (in particular CdIn2 S4 ) has been discussed in [415], the band structure of ZnM2 O4 has been calculated in [412] for (M = Co, Rh, Ir) (Fig. 6.13) and in [416] for (M = Al, Ga, In).
6.3.10 Delafossites In Fig. 6.14, the theoretical band structures of the delafossites CuAlO2 , CuGaO2 , and CuInO2 are shown. The maximum of the valence band is not at Γ but near the F point. The direct band gap at Γ decreases for the sequence Al → Ga → In, similar to the trend for AlAs, GaAs and InAs. The direct band gap at F and L, causing the optical absorption edge, increases, however (experimental values are 3.5, 3.6, and 3.9 eV). 2 Due
to the local density approximation (LDA) the absolute values of the band gaps are too small by about 1 eV.
6.3 Band Structures of Selected Semiconductors
167
ZnCo2O4
8
ZnIr2O4
6 4 2 0 2 4 6 8
X
W
L
X
W
L
Fig. 6.13 Calculated band structures of ZnCo2 O4 and ZnIr2 O4 . Adapted from [412] CuAlO 2
CuGaO 2
CuInO 2
6
4
2
0
2
Fig. 6.14 Band structures of CuAlO2 , CuGaO2 , and CuInO2 , calculated with LDA (underestimating the absolute value of the band gaps). The arrows denote the maximum of the valence band that has been set to zero energy for each material. Adapted from [200]
6.3.11 Perovskites The calculated band structure of BaTiO3 in the tetragonal phase is shown in Fig. 6.15. The minimum of the conduction band is at the Γ point. The maximum of the valence band is not at the Γ point but at the M point. The band gap of the LDA3 calculation is too small (2.2 eV) compared to the experimental value ∼3.2 eV. 3 local
density approximation.
168
6 Band Structure
Fig. 6.15 Calculated energy band structure of BaTiO3 along the major symmetry directions. The Fermi level (E F ) is set at zero energy. Adapted from [417]
6.4 Systematics of Semiconductor Band Gaps The trends with regard to the size of the band gap for elemental, III–V and II–VI semiconductors can essentially be understood in terms of the bond strength and ionicity. In Fig. 6.16, the band gaps of many important semiconductors are shown as a function of the lattice constant. For elemental semiconductors, the band gap decreases with reduced bond strength, i.e. lattice constant (C→Si→Ge). A similar trend exists both for the III–V and the II–VI semiconductors.
Fig. 6.16 Band gaps as a function of the lattice constant for various elemental, III–V and II–VI semiconductors. The lattice constant of wurtzite semiconductors has been recalculated for a cubic cell
6.4 Systematics of Semiconductor Band Gaps
169
For the same lattice constant, the band gap increases with increasing ionicity, i.e. IV–IV→III–V→II–VI→I–VII. A typical example is the sequence Ge→ GaAs→ ZnSe→CuBr, for which all materials have almost the same lattice constant, and the band gaps increase 0.66 eV→1.42 eV→2.7 eV→2.91 eV. This behavior can be understood within the framework of a modified Kronig– Penney model [418] (Appendix F). Double potential wells (b/a = 3) are chosen to mimic the diatomic planes along the 111 direction in the zincblende structure (Fig. 6.17a). Symmetric wells (depth P0 ) are chosen to model covalent semiconductors and asymmetric wells with depths P0 ± ΔP to model partially ionic semiconductors. Results are shown in Fig. 6.17a for P0 = −3. With increasing asymmetry, i.e. ionicity, the band gap increases, mostly due to a downward shift of the valence band. The case of III–V (II–VI) semiconductors is reached for ΔP ≈ 2 (4).
(a)
(b)
(c)
60 50 40 30
2
20
2
2md E/h
Fig. 6.17 Kronig–Penney model (along 111, b/a = 3) for a (a) IV–IV semiconductor and (b) for a III–V (or II–VI) semiconductor, (c) resulting band structure (P0 = −3). d is the lattice constant (b + a). Adapted from [418]
10 0 10
Eg
20 30 40 50 0
0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 4.5
P
170
6 Band Structure
Fig. 6.18 Optical image of two inch wafers of GaAs (left), GaP (center) and ZnO (right). A GaN wafer would look like the ZnO wafer Table 6.3 Comparison of band gap, lattice constant and ionicity of gallium–group V semiconductors for various anions Anion E g (eV) a0 (nm) fi N P As Sb
3.4 2.26 1.42 0.72
0.45 0.545 0.565 0.61
0.50 0.33 0.31 0.26
Lattice constant for GaN has been recalculated for a cubic cell
In Fig. 6.18, the visual impression of 2” wafers of GaAs, GaP and GaN on white paper is shown. GaAs (and GaSb) is opaque since the band gap is below the visible spectral range. GaP has a band gap in the green and appears red, GaN has a band gap in the ultraviolet and thus appears transparent. As can be seen from Table 6.3, the anion sequence Sb, As, P, and N leads to smaller lattice constant and higher ionicity. A notable deviation from this rule is InN whose band gap (0.7 eV) is much smaller than that of InP [419].
6.5 Alloy Semiconductors In alloy semiconductors, the size of the band gap and the character of the band gap will depend on the composition. The dependence of the band gap on the ternary composition is mostly nonlinear and can usually be expressed with a bowing parameter b that is mostly positive. For a compound Ax B1−x C the band gap is written as E g (Ax B1−x C) = E g (BC) + x E g (AC) − E g (BC) − b x (1 − x).
(6.26)
Even on the virtual crystal approximation (VCA) level (Sect. 3.7.3) a nonzero bowing parameter b is predicted. However, a more thorough analysis shows that the bowing cannot be treated adequately within VCA and is due to the combined effects of volume deformation of the band structure with the alloy lattice constant, charge exchange in
6.5 Alloy Semiconductors
171
the alloy with respect to the binary end components, a structural contribution due to the relaxation of the cation–anion bond lengths in the alloy and a small contribution due to disorder [420]. The discussion of Sect. 6.11.3 is related. The Six Ge1−x alloy has diamond structure for all concentrations and the position of the conductionband minimum in kspace switches from L to X at about x = 0.15 (Fig. 6.19a). However, for all concentrations the band structure is indirect. The
(b) 1.5
(a)
InxGa1xAs 1.3
Eg (eV)
1.1 0.9 0.7 0.5 0.3 0.0
(c)
0.2
0.4
0.6
0.8
1.0
x
(d)
2.6 AlxGa1xAs 1
2.4
L1
Eg (eV)
2.2 2.0
X1 Edd
1.8 1.6 1.4 0.0
0.2
0.4
0.6
0.8
1.0
x
Fig. 6.19 (a) Band gap of Six Ge1−x alloy (T = 296 K) with a change from the conductionband minimum at L (Gerich) to X. The inset depicts the transition energy of the indirect (Γ –L) and direct (Γ –Γ ) absorption edge for low Si content. Adapted from [424]. (b) Band gap (at room temperature) of Inx Ga1−x As. The solid line is an interpolation with bowing (b = 0.6 eV) and the dashed line is the linear interpolation. Data from [421]. (c) Band gap (at room temperature) in the ternary system Alx Ga1−x As. For x < 0.4 the alloy is a direct, for x > 0.4 an indirect, semiconductor. E dd denotes the energy position of a deep donor (cf. Sect. 7.7.6). Adapted from [425]. (d) Band gap (at room temperature) in the ternary system Mgx Zn1−x O. Data (from spectroscopic ellipsometry [426, 427]) are for hexagonal wurtzite phase (circles), and Mgrich cubic rocksalt phase (squares). Dashed lines are fits to data with a different bowing parameter for each phase
172
6 Band Structure
Inx Ga1−x As alloy has zincblende structure for all compositions. The band gap is direct and decreases with a bowing parameter of b = 0.6 eV [421] (Fig. 6.19b). This means that for x = 0.5 the band gap is 0.15 eV smaller than expected from a linear interpolation between GaAs and InAs, as reported by various authors [422]. If one binary end component has a direct band structure and the other is indirect, a transition occurs from direct to indirect at a certain composition. An example is Alx Ga1−x As where GaAs is direct and AlAs is indirect. For all concentrations the crystal has zincblende structure. In Fig. 6.19c, the Γ , L and X conductionband minima for ternary Alx Ga1−x As are shown. Up to an aluminum concentration of x = 0.4 the band structure is direct. Above this value the band structure is indirect with the conductionband minimum being at the X point. The particularity of Alx Ga1−x As is that the lattice constant is almost independent of x. For other alloys lattice match to GaAs or InP substrates is only obtained for specific compositions, as shown in Fig. 6.20. Bowing in the groupIII–nitride system has been discussed in [423]. If the two binary end components have different crystal structure, a phase transition occurs at a certain composition (range). An example is Mgx Zn1−x O, where ZnO has wurtzite structure and MgO has rocksalt structure. The band gap is shown in Fig. 6.19d. In this case, each phase has its own bowing parameter. All alloys of Fig. 6.19b–d have mixed cations. The band gap also varies upon anion substitution in a similar way as shown in Fig. 6.21 for ternary alloys with the cation Zn and the chalcogenides S, Se, Te and O. Fig. 6.20 Band gap versus lattice constant for Gax In1−x P and Alx In1−x P (lattice matched to GaAs) as well as for Inx Al1−x As and Inx Ga1−x As alloys (lattice matched to InP)
6.6 Amorphous Semiconductors
173
Fig. 6.21 Band gap of various Znbased alloys. The lines are fits with (6.26), the bowing parameter b is labeled. Data for Zn(S,Se,Te) from [428], for Zn(O,Se/Te) from [429]
6.6 Amorphous Semiconductors Since the crystal lattice in an amorphous semiconductor is not periodic, the concept of kspace and the related concepts such as band structure E(k) break down at least partially. The density of states, however, remains a meaningful and useful quantity (Sect. 6.12.2).
Fig. 6.22 (a) Calculated band structure of crystalline silicon. (b) Calculated band structure of amorphous silicon with α = 0.05 (cf. (3.7)). The solid lines denote the real part of the energy, the shaded areas denote the regions with a width of twice the imaginary part of the energies centered around the real part. Adapted from [431]
174
6 Band Structure
In a perfectly crystalline semiconductor the eigenenergies of the states in the bands are real. An amorphous semiconductor can be modeled using a spectrum of complex energies [430]. In Fig. 6.22 the band structure of crystalline silicon is shown next to that calculated for amorphous silicon with α = 0.05.
6.7 Temperature Dependence of the Band Gap The band gap typically decreases with increasing temperature (see Fig. 6.23 for Si and GaAs). The reasons for this are the change of electron–phonon interaction and the expansion of the lattice. The temperature coefficient may be written as
∂ Eg ∂T
= p
∂ Eg ∂T
− V
α β
∂ Eg ∂p
,
(6.27)
T
where α is the volume coefficient of thermal expansion and β is the volume compressibility. A recommendable discussion of the thermodynamic role of the band gap as chemical potential for the mass action law (7.12), entropy contributions and its temperature dependence can be found in [432]. An anomaly is present for the lead salts (PbS, PbSe, PbTe) for which the temperature coefficient is positive (Fig. 6.24a). Theoretical calculations [434] show that both − terms in (6.27) are positive for the lead salts. The L+ 6 and L6 levels (see Fig. 6.9) shift as a function of temperature in such a way that their separation increases (Fig. 6.24b). Also in copper and silver halides [435, 436] (Fig. 6.25a) and chalcopyrites [437] (Fig. 6.25b) the increase of band gap with increasing temperature has been found, sometimes only for a certain temperature range. This effect is attributed to the pd
(a)
0
Si
(b)
Eg (meV)
Eg (meV)
50
100
150
200 0
100 200 300 400 500 600 700 800
Fig. 6.23 Temperature dependence of the band gap of (a) Si (data from [433]) and (b) ZnO (experimental data from photoluminescence (triangles) and ellipsometry (circles)). The solid lines are fits with (6.30) and the parameters given in Table 6.4
6.7 Temperature Dependence of the Band Gap
(a)
175
(b)
0.35 0.34
PbTe 7.5
0.33
E g (eV)
8.0
PbS
L6
0.32 7.0 0.31
L6
0.30
6.5
0.29 0.28
0
50
100
6.0
150
0
100
200
300
− Fig. 6.24 (a) Band gap versus temperature for PbS. (b) Theoretical position of L+ 6 and L6 as a function of temperature for PbTe. Adapted from [410]
(a)
CuI1xBrx
(b)
1.82
AgGaSe2
x=0
3.05
x=1
3.00
1.81
x=0.1 x=0.8
2.95
1.80
x=0.2 x=0.64
2.90 x=0.42
0
100
200
300
1.79
0
100
200
300
Fig. 6.25 (a) Band gap versus temperature for zincblende CuI1−x Brx alloys with various compositions x (including binary CuI and CuBr) as labeled. Dashed lines are guide to the eyes. Adapted from [435]. (b) Band gap versus temperature for chalcopyrite AgGaSe2 . Solid line is fit with twooscillator BoseEinstein model. Adapted from [437]
electron hybridization in the valence band with Cu 3d electrons and to even stronger effect with Ag 4d electrons. For many semiconductors the temperature dependence can be described with the empirical, threeparameter Varshni formula [438], E g (T ) = E g (0) −
αT2 , T +β
(6.28)
176
6 Band Structure
Table 6.4 Parameters for the temperature dependence of the band gap (6.29) and (6.30) for various semiconductors α (10−4 eV/K) Θ (K) Δ αB (10−4 eV/K) ΘB (K) Si Ge GaAs InP InAs ZnSe ZnO
3.23 4.13 4.77 3.96 2.82 5.00 3.8
446 253 252 274 147 218 659
0.51 0.49 0.43 0.48 0.68 0.36 0.54
2.82
351
5.12
313
where E g (0) is the band gap at zero temperature. A more precise and physically motivated formula (based on a Bose–Einstein phonon model) has been given in [439]
ΘB −1 , E g (T ) = E g (0) − 2 αB ΘB coth 2T
(6.29)
where α B is a coupling constant and kΘB is a typical phonon energy; typical values are given in Table 6.4. This model reaches a better description of the fairly flat dependence at low temperatures. The more elaborate model of [440] takes into account a more variable phonon dispersion, including optical phonons, and proposes the fourparameter formula
1 − 3 Δ2 3 Δ2 6 1+β−1 + exp (2/γ) − 1 2 2 2 π 3Δ − 1 3 8 4 β= γ2 + γ + γ + γ6 3 (1 + Δ2 ) 4 3 γ = 2 T /Θ,
E g (T ) = E g (0) − α Θ
(6.30)
where α is the hightemperature limiting magnitude of the slope (of the order of several 10−4 eV/K), Θ is an effective average phonon temperature and Δ is related to the phonon dispersion. Δ takes typically values between zero (Bose–Einstein model) and 3/4 [440].
6.8 Isotope Dependence of the Band Gap The band edge slightly depends on the isotope composition of semiconductor, as shown for GaAs in Fig. 6.26. The effect is discussed in detail in [441].
6.9 Electron Dispersion
177
Fig. 6.26 Band gap of GaAs (at T = 10 K) as a function of the Ga isotope content. Dashed line is linear fit. Adapted from [441]
6.9 Electron Dispersion 6.9.1 Equation of Electron Motion The equation of motion for the electron in the band structure is no longer given by Netwon’s law F = d(mv)/dt as in vacuum. Instead, the propagation of quantummechanical electron wave packets has to be considered. Their group velocity is given by (vg = ∂ω/∂k) 1 v = ∇k E(k), (6.31) where ∇k is the gradient with respect to k. Through the dispersion relation the influence of the crystal and its periodic potential on the motion enters the equation. An electric field E acts on an electron during the time δt the work δ E = −eEvg δt. This change in energy is related to a change in k via δ E = dE/dk δk = vg δk. Thus, we arrive at dk/dt = −eE. For an external force we thus have
dk = −e E = F. dt
(6.32)
Thus, the crystal momentum p = k takes the role of the momentum. A more rigorous derivation can be found in [399]. In the presence of a magnetic field B the equation of motion is:
e dk = −e v × B = − (∇k E) × B. dt
(6.33)
The motion in a magnetic field is thus perpendicular to the gradient of the energy, i.e. the energy of the electron does not change. It oscillates therefore on a surface of constant energy perpendicular to B.
178
6 Band Structure
6.9.2 Effective Mass of Electrons From the freeelectron dispersion E = 2 k 2 /(2m) the mass of the particle is inversely proportional to the curvature of the dispersion relation, i.e. m = 2 /(d2 E/dk 2 ). This relation will now be generalized for arbitrary dispersion relations. The tensor of the effective mass is defined as (m ∗−1 )i j =
1 ∂2 E . 2 ∂ki ∂k j
(6.34)
The equation F = m ∗ v˙ must be understood as a tensor equation, i.e. for the components of the force Fi = m i∗j a j . Force and acceleration must no longer be collinear. In order to find the acceleration from the force, the inverse of the effectivemass tensor must be used, a = (m∗ )−1 F. In Fig. 6.27 the energy dispersion of the (lowest) conduction band in a typical semiconductor, the related electron velocity and the effective mass are shown schematically. In (6.22) the ratio of the effective mass and the freeelectron mass is of the order of m ∗ /m ≈ U/λ, the ratio of the free particle energy and the band gap. For typical semiconductors, the width of the (valence) band is of the order of 20 eV, and the gap is about 0.2–2 eV. Thus, the effective mass is expected to be 10–100 times smaller than the freeelectron mass. Additionally, the relation m ∗ ∝ E g is roughly fulfilled (Fig. 6.28).
Fig. 6.27 Schematic diagram of the electron dispersion E(k) in a typical semiconductor (blue) and corresponding carrier velocity (∝ ∂ E/∂k) (red) and effective mass (∝ 1/(∂ 2 E/∂k 2 )) (green)
6.9 Electron Dispersion
179
Fig. 6.28 Effective electron mass (in units of the freeelectron mass m 0 ) as a function of the (lowtemperature) band gap for several (direct band gap) semiconductors. The dashed line fulfills m ∗/m 0 = E g /20 eV
From socalled k · p theory [442] (see Appendix G) the effective electron mass is predicted to be related to the momentum matrix element pcv pcv = cpv =
Ω0
u ∗c,k (r) p u c, k (r) d3 r,
(6.35)
with Ω0 being the unit cell volume and the Bloch functions c and v of the conduction and valence band, respectively, given as c = u c,kc (r) exp (i kc r) v = u v,kv (r) exp (i kv r) .
(6.36a) (6.36b)
Typically, the kdependence of the matrix element is small and neglected. The momentum matrix element will also be important for optical transitions between the valence and conduction bands (Sect. 9.5). Other related quantities that are often used are the energy parameter E P 2 pcv 2 EP = , (6.37) m0 and the bulk momentum matrix element Mb2 that is given by Mb2 =
1 m0 pcv 2 = EP . 3 6
(6.38)
180
6 Band Structure
(a)
(b)
(c)
(d)
Fig. 6.29 Energy isosurfaces in kspace in the vicinity of the conductionband minima for (a) GaAs with isotropic (spehrical) minimum at Γ point, (b) ZnO with anisotropic (ellipsoidal) minimum at Γ point (anisotropy exaggerated), (c) silicon with six equivalent anisotropic minima (m l /m t = 5 not to scale) along 100 and (d) germanium with eight equivalent anisotropic minima along 111. The cube indicates the 100 directions for the cubic materials. For the wurtzite material (part b) the vertical direction is along [00.1]
The electron mass is given by4
1 2 + Eg E g + Δ0 E g + 2Δ0 /3 EP EP ≈1+ . ≈ = 1 + EP E g + Δ0 /3 Eg E g E g + Δ0
m0 EP = 1+ ∗ me 3
(6.39)
Comparison with the fit from Fig. 6.28 yields that E P is similar for all semiconductors [443] and of the order of 20 eV (InAs: 22.2 eV, GaAs: 25.7 eV, InP: 20.4 eV, ZnSe: 23 eV, CdS: 21 eV). In silicon there are six conductionband minima. The surfaces of equal energy are schematically shown in Fig. 6.29c. The ellipsoids are extended along the 100 4Δ 0
is the spinorbit splitting discussed in Sect. 6.10.2.
6.9 Electron Dispersion
181
Table 6.5 Longitudinal direction of effective mass ellipsoid, longitudinal and transverse effective electron mass in several semiconductors Long. dir. ml mt m l /m t m d,e References C Si Ge ZnO CdS
100 100 111 [00.1] [00.1]
1.4 0.98 1.59 0.21 0.15
0.36 0.19 0.082 0.25 0.17
3.9 5.16 19.4 0.88 0.9
1.9 1.08 0.88
[446] [447] [447] [448] [449]
Mass values in units of the free electron mass m 0 . For the density of states mass m d,e see (6.68)
direction because the longitudinal mass (along the Δ path) is larger than the transverse mass in the two perpendicular directions (Table 6.5). For example, the dispersion relation around the [100] minimum is then given as (k x0 denotes the position of the conductionband minimum) E(k) =
2
k 2y + k z2 (k x − k x0 )2 + 2 ml 2 mt
.
(6.40)
For germanium surfaces of constant energy around the eight conductionband minima in the 111 directions are depicted in Fig. 6.29d. The longitudinal and the transverse masses are again different. For GaAs, the conductionband dispersion around the Γ point is isotropic, thus the surface of constant energy is simply a sphere (Fig. 6.29a). In wurtzite semiconductors the conductionband minimum is at the Γ point. The mass along the caxis is typically smaller than the mass within the (00.1) plane [444] (m l /m t ≈ 0.8 for ZnO [445]), see Fig. 6.29b. In [444] also an anisotropy within the (00.1) plane is predicted. The directional dependence of the mass can be measured with cyclotron resonance experiments with varying direction of the magnetic field. In Fig. 6.30, the field B is in the (110) plane with different azimuthal directions. When the (static) magnetic field makes an angle θ with the longitudinal axis of the energy surface, the effective mass is given as [450] cos2 θ sin2 θ 1 = + . (6.41) ∗ m mt ml m 2t
6.9.3 Nonparabolicity of Electron Mass The dispersion around the conductionband minimum is only parabolic for small k. The further away the wavevector is from the extremum, the more the actual dispersion deviates from the ideal parabola (see, e.g., Fig. 6.7). This effect is termed
182
6 Band Structure
(a)
(b)
Fig. 6.30 Effective electron mass from cyclotron resonance experiments (at T = 4 K) on (a) Si and (b) Ge for the magnetic field in the (110) plane and various azimuthal directions θ. Experimental data and fits (solid lines) using (6.41) with (a) m l = 0.98, m t = 0.19 and (b) m l = 1.58, m t = 0.082. Data from [447]
nonparabolicity. Typically, the energy increases less quickly with k than in the parabolic model. This can be described in a socalled twolevel model with the dispersion relation
E 2 k 2 = E 1+ ∗ , (6.42) 2m ∗0 E0 where E 0∗ > 0 parameterizes the amount of nonparabolicity (a parabolic band corresponds to E 0∗ = ∞). The nonparabolic dispersion for GaAs is shown in Fig. 6.31a. The curvature is reduced for larger k and thus the effective mass is energy dependent and increases with the energy. Equation (6.42) leads to the energydependent effective mass
2E (6.43) m ∗ (E) = m ∗0 1 + ∗ , E0 where m ∗0 denotes here the effective mass at k = 0. Theory and experimental data for the effective electron mass of GaAs are shown in Fig. 6.31b.
6.10 Holes
183 18
(a)
3
E F (meV)
(b) 0.14 [001] [111]
GaAs 0.3
GaAs
m*/m0
0.12
0.2
0.1
0.10
0.08
0
0.06 16 10 2
13
17
18
10
k (10 cm )
19
10 3
2
10
)
Fig. 6.31 (a) Dispersion relations for the conduction band of GaAs. The solid line is parabolic dispersion (constant effective mass). The dashed (dashdotted) line denotes the dispersion for k along [001] ([111]) from a fivelevel k · p model (5LM). (b) Cyclotron resonance effective mass of electrons in GaAs as a function of the Fermi level (upper abscissa) and the corresponding electron concentration (lower abscissa). The dashed line is from a 2LM according to (6.43) with E 0∗ = 1.52 eV. The solid lines are for a 5LM for the three principal directions of the magnetic field. The symbols represent experimental data from different sources. Data from [451]
6.10 Holes 6.10.1 Hole Concept Holes are missing electrons in an otherwise filled band. A Schrödingertype waveequation for holes (unoccupied electron states) was derived by Heisenberg [63] to interpret Hall effect data. The hole concept is useful to describe the properties of charge carriers at the top of the valence band. The hole is a new quasiparticle whose dispersion relation is schematically shown in Fig. 6.32 in relation to the dispersion of electrons in the valence band. Fig. 6.32 Hole dispersion (dashed line) in relation to the electron dispersion in the valence band (solid line)
E
ke kh
k
184
6 Band Structure
The wavevector of the hole (filled circle in Fig. 6.32) is related to that of the ‘missing’ electron (empty circle in Fig. 6.32) by kh = −ke . The energy is E h (kh ) = −E e (ke ), assuming that E V = 0, otherwise E h (kh ) = −E e (ke ) + 2E V . The hole energy is larger for holes that are further away from the top of the valence band, i.e. the lower the energy state of the missing electron. The velocity of the hole, vh = −1 dE h /dkh , is the same, vh = ve , and the charge is positive, +e. The effective mass of the hole is positive at the top of the valence band, m ∗h = −m ∗e . Therefore, the drift velocities of an electron and hole are opposite to each other. The resulting current, however, is the same.
6.10.2 Hole Dispersion Relation The valence band at the Γ point is 3fold degenerate. The band developed from the atomic (bonding) p states; the coupling of the spin s = 1/2 electrons with the orbital angular momentum l = 1 leads to a total angular momentum j = 1/2 and j = 3/2. The latter states are degenerate at Γ in zincblende bulk material and are called heavy holes (hh) for m j = ±3/2 and light holes (lh) for m j = ±1/2 due to their different dispersion (Fig. 6.33a). The two (m j = ±/ 2) states of the j = 1/2 state are splitoff from these states by an energy Δ0 due to spinorbit interaction and are called splitoff (so) holes. The spinorbit interaction increases with increasing atomic order number Z of the anion since the electrons are located preferentially there (Fig. 6.34).
(a) (b)
Fig. 6.33 (a) Simplified band structure with conduction band and three valence bands and (b) threedimensional visualization (E vs. (kx , ky )) of the valence bands of Ge (including warping). Part (b) from [453]
6.10 Holes
185
Fig. 6.34 Spinorbit splitting Δ0 for elemental (diamonds) and various III–V and II–VI (circles) semiconductors. The data are plotted as empty (filled) circles as a function of the cation (anion) order number. Obviously, Δ0 correlates with the anion Z . The dashed line is proportional to Z 2
A detailed discussion of the spinorbit splitting in zincblende semiconductors is given in [452]. All three holes have different mass. In the vicinity of the Γ point the dispersion for heavy and light holes can be described with (+:hh, −:lh) E(k) = A k ± 2
B 2 k 4 + C 2 kx2 ky2 + ky2 kz2 + kx2 kz2 .
(6.44)
For heavy and light holes there is a dependence of the dispersion, i.e. the mass, in the (001) plane. This effect, sketched in Fig. 6.33b, is called warping. The warping at the GaAs valenceband edge is shown in Fig. 6.35. Equation (6.44) can also be expressed in terms of angular coordinates [454]. The so holes have the dispersion E(k) = −Δ0 + A k 2 .
(6.45)
Values for A, B, C 2 and Δ0 for a number of semiconductors are given in Table 6.6. The valenceband structure is often described with the Luttinger parameters γ1 , γ2 , and γ3 that can be represented through A, B, and C via 2 γ1 = −A 2m 0 B 2 γ2 = − 2m 0 2 2 B 2 + C 2 /3 γ3 = . 2m 0 2
(6.46a) (6.46b) (6.46c)
The mass of holes in various directions can be derived from (6.44). The mass along the [001] direction, i.e. 2 / ∂ 2 E(k)/∂k x2 for k y = 0 and k z = 0, is
186
6 Band Structure
(b) 4
(a)
2
0
2
4
(c)
4
2
0
2
4
4
2
0
2
4
(d) 4 2
0
2
4
Fig. 6.35 Dispersion at the valence band edge of GaAs for (a, b) heavy holes and (c, d) light holes. (a, c) Constant energy surfaces and (b, d) isolines in the (k x , k y )plane ((b) and (d) have different energy scales)
Table 6.6 Valenceband parameters (for (6.44)) A and B in units of (2 /2m 0 ), C 2 in units of (2 /2m 0 )2 , and Δ0 in eV Material A B C2 Δ0 C Si Ge GaAs InP InAs ZnSe
−4.24 −4.28 −13.38 −6.9 −5.15 −20.4 −2.75
From [146, 455, 456]
−1.64 −0.68 −8.5 −4.4 −1.9 −16.6 −1.0
9.5 24 173 43 21 167 7.5
0.006 0.044 0.295 0.341 0.11 0.38 0.43
6.10 Holes
187
(a)
(b)
Fig. 6.36 Effective hole masses from cyclotron resonance experiments (T = 4 K) for heavy and light holes in (a) Si and (b) Ge for the magnetic field in the (110) plane and various azimuthal directions θ. Experimental data (symbols) and fits (solid lines) using (6.48). Adapted from [447]
1 2 = 2 (A + B) 100 m hh 1 2 = 2 (A − B). 100 m lh
(6.47a) (6.47b)
The anisotropy of hole masses has been investigated with cyclotron resonance experiments (Fig. 6.36). For θ being the angle between the magnetic field and the [001] direction, the effective heavy hole (upper sign) and light hole (lower sign) mass in cubic semiconductors is given by [447] m∗ =
2 1 2 A ± B 2 + C 2 /4 ⎧ ⎫ ⎨ ⎬ C 2 (1 − 3 cos2 θ)2 + ... . × ⎩ 64 B 2 + C 2 /4 A ± B 2 + C 2 /4 ⎭
(6.48)
For C 2 = 0 the hole bands are isotropic, as is obvious from (6.44). In this case γ2 = γ3 , the socalled spherical approximation. The average of the hole masses over all directions is
188
6 Band Structure
(a)
(b)
Fig. 6.37 Luttinger parameters for various IIIV semiconductors versus their band gap. (a) Inverse values of γ1 (squares) and γ2 (diamonds). Dashed lines are guides to the eyes. (b) γ3 − γ2 versus band gap
2 C2 A+ B 1+ 15 B 2
2 1 2 C2 = A − B 1 + . m av 2 15 B 2 lh
1 2 av = 2 m hh
(6.49a) (6.49b)
Similar to the correlation of the electron mass with the band gap (Fig. 6.28), the Luttinger parameters are correlated with the band gap as shown in Fig. 6.37. The parameters 1/γ1 and 1/γ2 increase about linearly with E g . The parameter γ3 − γ2 , which is responsible for the valence band warping, decreases with increasing band gap.
6.10.3 ValenceBand Fine Structure In Fig. 6.38, the schematic structure of the band edges for zincblende structure semiconductors is shown. The so holes in the zincblende structure are splitoff due to the spinorbit interaction Δso , the Γ8 band is degenerate (heavy and light holes). Degeneracies for the holes are removed in the wurtzite and chalcopyrite structures by the additional crystal field splitting Δcf due to the anisotropy between the a and caxes. Typically, e.g. for CdS, the topmost valence band in the wurtzite structure has Γ9 symmetry (allowed optical transitions only for E ⊥ c); an exception is ZnO for which the two upper bands are believed to be reversed. In the chalcopyrite structure optical transitions involving the Γ6 band are only allowed for E ⊥ c. The three hole bands are usually labeled A, B, and C from the top of the valence band. The energy positions of the three bands (with respect to the position of the Γ15 band) in the presence of spinorbit interaction and crystal field splitting are given
6.10 Holes
189
Fig. 6.38 Schematic band structure of zincblende and the valenceband splitting due to spinorbit interaction Δso and crystal field splitting Δcf for chalcopyrites (typically Δcf < 0, see Fig. 6.39) and wurtzites. For the wurtzites the situation is schematically shown for CdS (Δso = 67 meV, Δcf = 27 meV) (or GaN) and ZnO (Δso = −8.7 meV, Δcf = 41 meV)
within the quasicubic approximation [457] by Δso + Δcf 2
Δso + Δcf 2 2 =± − Δso Δcf . 2 3
E1 = E 2,3
(6.50a) (6.50b)
In chalcopyrites the crystal field splitting is typically negative (Fig. 6.39). It is approximately linearly related to 1 − η (for η = c/2a see Sect. 3.4.6).
6.10.4 Band Inversion In certain compounds the band gap can shrink to zero (zerogap semiconductor, cf. Sect. 18.1.2) and even become negative in the sense that the sorbital type Γ6 symmetry (conduction) band is inverted below the valenceband edge. HgTe is a classical example for such material as shown in Fig. 6.40, but similar effects are also present in other semiconductors, for example various chalcopyrites [459]. For the zerogap case, the dispersion of some bands is linear (cmp. Sect. 18.1.2); this corresponds to a very strong nonparabolicity. The dielectric function of zerogap semiconductors is discussed in [460].
190
6 Band Structure
Fig. 6.39 Crystal field splitting Δcf for various chalcopyrite compounds versus the tetragonal distortion 2 − c/a = 2 (1 − η). Dashdotted line represents Δcf = 1.5 b (2 − c/a) for b = 1 eV. Data from [458]
0.3 AgGaS2 AgGaSe2
0.2
cf
(eV)
AgInS2 CuAlS2 CuGaS2 CuGaSe2
0.1
AgGaTe2 AgAlTe2
AgInSe2
AgInS2(w)
CuInS2
0
CuInSe2
0.1
0.0
0.2
2 c/a
Fig. 6.40 Schematic band structure of zincblende with vanishing energy gap for the ternary compounds Mnx Hg1−x Te. Note the linear dispersion for the zerogap case at x ≈ 0.07
zerogap
6
0
6
8 0
>0
8
0 is the valenceband hydrostatic deformation potential. Therefore the band gap increases by ΔE g = a Tr() = a xx + yy + zz ,
(6.53)
with a = aC −aV . Such linear behavior upon hydrostatic pressure has been found for many semiconductors and is shown in Fig. 6.41a for Ga0.92 In0.08 As. The anomaly for Ndoping is discussed below in Sect. 6.11.3. In Fig. 6.42 the dependence of the direct and indirect gaps of GaAs is shown. The dependence of the direct gap on pressure is nonlinear, that on the density is linear [465].
(a)
(b)
Fig. 6.41 (a) Dependence of the band gap of Ga0.92 In0.08 As alloy (squares) and nitrogendoped (Ga,In)As on (compressive) hydrostatic pressure, determined by photomodulated transmission at T = 295 K. (b) Pressure dependence of band gap for two (Ga,In)(As,N) samples together with model calculation (6.58). The coupling parameter is V = 0.12 eV (0.4 eV) for a nitrogen content of 0.9 % (2.3 %). Adapted from [466]
192
6 Band Structure
V –Γ C and indirect Γ V –X C band gap of GaAs (T = 300 K) Fig. 6.42 Dependence of the direct Γ15 1 1 15 on pressure. Solid lines are interpolations of experimental data, dashed line is extrapolation to p = 0. The crossing of the direct and indirect band gap occurs at 4.2 GPa. The arrow denotes the pressure of the phase transition from zincblende to an orthorhomic structure around 17 GPa. Adapted from [465]
Biaxial and shear strains affect the valence bands and lead to shifts and splitting of the heavy and light holes at the Γ point: E v,hh/lh = E v0 ± E 2 = b2 /2 E
xx − yy
2
(6.54a)
2 + yy − zz + (xx − zz )2 + d 2 2xy + 2yz + 2xz ,
where E v0 denotes the bulk valenceband edge. b and d are the optical deformation potentials. For compressive strain the heavyhole band is above the lighthole band. For tensile strain there is strong mixing of the bands (Fig. 6.43). In Table 6.7 the deformation potentials for some III–V semiconductors are listed. Typical values are in the eV regime. In a wurtzite crystal, seven (or eight) deformation potentials are needed that are termed a (for the change of band gap with hydrostatic strain, again a = aC − aV ) and D1 –D6 (for the valence band structure) [467, 468]. In Si and Ge, three deformation potentials, termed a, b, d, are needed for the valence band and two for each conduction band minimum, u and d [469]. The energy position of the ith conductionband edge (with unit vector ai pointing to the valley) is 0 + d Tr() + u ai ai , (6.55) E C,i = E C,i 0 where E C,i denotes the energy of the unstrained conductionband edge. The deformation potentials for Si and Ge are given in Table 6.8.
6.11 Strain Effects on the Band Structure E
193 E
E
electrons
k
k
k
m j=3/2 m j=1/2
m j=1/2 mj=3/2
m j =3/2 m j=1/2
compressive
unstrained
tensile
Fig. 6.43 Schematic band structure of GaAs in unstrained state (center) and under compressive and tensile biaxial strain as labeled. Dashed lines indicate shift of band edges due to hydrostatic part of strain Table 6.7 Deformation potentials for some III–V semiconductors Material a b −9.8 −6.0
GaAs InAs
−1.7 −1.8
d −4.6 −3.6
All values in eV Table 6.8 Deformation potentials for silicon and germanium (Δ) (Δ) (L) (L) Material d u d u a Si Ge
1.1 4.5
10.5 9.75
−7.0 −4.43
18.0 16.8
2.1 2.0
b
d
−2.33 −2.16
−4.75 −6.06
All values in eV from [470]
6.11.2 Strain Effect on Effective Masses In the presence of strain the band edges are shifted (cf. Sect. 6.11). Since the electron mass is related to the band gap, it is expected that the mass will also be effected. In the presence of hydrostatic strain H the electron mass is [471] (cf. to (6.39) for H → 0)
m0 EP 3a = 1 + 1 − , (6.56) 2 + H m ∗e E g + Δ0 /3 E g + Δ0 /3 with a being the hydrostatic deformation potential and H = Tr(). In [471], formulas are also given for biaxial and shear strain and also for hole masses. Since the effective
194
6 Band Structure
mass enters the mobility, the electrical conductivity depends on the stress state of the semiconductor (piezoresistivity, see Sect. 8.3.11).
6.11.3 Interaction with a Localized Level The normal dependence of the band gap on hydrostatic pressure is linear and given by (6.53). (Ga,In)As containing nitrogen exhibits a remarkable deviation from this behavior as shown in Fig. 6.41a. This is due to the interaction of the continuum states of the conduction band with the electron level of the isoelectronic nitrogen impurity (Sect. 7.7.9) E N , being within the conduction band. For GaAs it is 0.2 eV above the conduction band edge E C . This phenomenon has been investigated theoretically within microscopic detail [472]. Within a simple ‘band anticrossing’ twolevel model, the coupling of the pressuredependent conduction band edge E C and the nitrogen level can be obtained from the Eigenwert equation E − EC V = 0, V E − EN
(6.57)
V being the coupling constant. The determinant vanishes for E± =
1 E C + E N ± (E C − E N )2 + 4V 2 . 2
(6.58)
Here the weak pressure dependence of E N is neglected for simplicity. This model can explain the pressure dependence of the band gap of (Ga,In)As:N fairly well [466] (Fig. 6.41b). The coupling parameter V is in the order of a few 0.1 eV for small
1.5
GaAs1xNx 1.4
Energy (eV)
Fig. 6.44 Bandgap of GaAs1−x Nx , experimental data from various sources (symbols) and model (curve) according √to (6.58) with V = V0 x for V0 = 2.7 eV. Adapted from [473]
1.3
1.2
1.1
1.0
0.9 0
1
2
3
Nitrogen concentration x (%)
4
5
6.11 Strain Effects on the Band Structure
195
nitrogen content. In photomodulated reflection also the E + levels can be observed [473]. The anticrossing model can also model the dependence of the GaAs1−x Nx bandgap on the nitrogen concentration [473] (Fig. 6.44).
6.12 Density of States 6.12.1 General Band Structure The dispersion relation yields how the energy of a (quasi) particle depends on the k vector. Now we want to know how many states are at a given energy. This quantity is called the density of states (DOS) and is written as D(E). It is defined in an infinitesimal sense such that the number of states between E and E + δ E is D(E)δ E. In the vicinity of the extrema of the band structure many states are at the same energy such that the density of states is high. The dispersion relation of a band will be given as E = E(k). If several bands overlap, the densities of state of all bands need to be summed up. The density of states at the energy E˜ for the given band is ˜ dE = 2 D( E)
d3 k δ( E˜ − E(k)), (2π/L)3
(6.59)
where, according to (5.5), (2π/L)3 is the kspace volume for one state. The factor 2 is for spin degeneracy. The integral runs over the entire kspace and selects only ˜ The volume integral can be converted to a surface integral those states that are at E. ˜ with E(k) = E. ˜ The volume element d3 k is written over the isoenergy surface S( E) 2 ˜ and proportional to ∇k E(k), as d S dk⊥ . The vector dk⊥ is perpendicular to S( E) i.e. dE = ∇k E(k) dk⊥ . ˜ =2 D( E)
˜ S( E)
d2 S 1 . 3 (2π/L) ∇k E(k)
(6.60)
In this equation, the dispersion relation is explicitly contained. At band extrema the gradient diverges, however, in three dimensions the singularities are integrable and the density of states takes a finite value. The corresponding peak is named a vanHove singularity. The concept of the density of states is valid for all possible dispersion relations, e.g. for electrons, phonons or photons. The density of states for the silicon band structure (see Fig. 6.6a) is shown in Fig. 6.45.
196
6 Band Structure
Fig. 6.45 Density of states in the silicon valence (blue) and conductionband (red) as obtained from theoretical calculation using empirical pseudopotentials. Grey regions denotes the band gap. Critical points (cf. Fig. 6.6a) are labeled. In the lower three graphs, the DOS is decomposed into contributions from different angular momentum states (s (green), p (orange) and d (purple)). Top part adapted from [474], bottom part adapted from [155]
6.12.2 Amorphous Semiconductors If disorder is introduced, the density of states is modified as shown in Fig. 6.46 for amorphous germanium using a calculation with complex eigenenergies. The defects, as compared to the perfect lattice, introduced states in the band gap and generally wash out the sharp features from the crystalline DOS. Several models exist for the defect level distributions within the band gap. The first model was the Mott model which has band tails at the valence and conduction band edges [475]. In the CohenFritzscheOvshinsky (CFO) model [476], the band tails are more severe and overlap; the Fermi energy lies at the minimum of the density of states. In the Davis–Mott model [477] deep states were added in the gap and eventually the MarshallOwen model [478] assumes band tails and donor and acceptorlike deep states. The four models are schematically shown in Fig. 6.47. These model densities of states allow also the interpretation of carrier transport in amorphous semiconductors, taking into account localized and delocalized states (see Sect. 8.8). The density of states for an amorphous semiconductor is best calculated from atomistic models, possibly averaging over many configurations. The typical features,
6.12 Density of States
197
Fig. 6.46 Theoretical calculation for the density of states of amorphous Ge models as obtained for various degrees of disorder α (3.7). α = 0.09 corresponds to a mean shortrange order distance of about 2.4 lattice constants (cmp. Fig. 3.14b). Adapted from [177]
(a) DOS (arb. units)
(b)
EC
EV
(c)
EV
EC
DOS (arb. units)
(d)
EV
EC Energy
EV
EC Energy
Fig. 6.47 Model density of states in amorphous semiconductors (solid lines) according to Mott [475], CohenFritzscheOvshinsky [476], Davis–Mott [477] and Marshall–Owen [478]. Dashed lines represent the DOS of the same material without disorder
compared to the clear band gap of a similar ordered material, are band tails due to disorder (cmp. Sect. 5.2.8) and deep levels within the gap due to specific atomic arrangements not present in ordered bulk. The most investigated system is amorphous silicon; in Fig. 6.48 a numerical calculation of the density of states is shown together with charge distribution of four states at selected energies [479]. The further the states are in the band tail, the stronger their localization is. The two most right states shown in Fig. 6.48 are not conducting.
198
6 Band Structure Energy (eV)
DOS (1022 eV1 cm3 )
0.5 1.0
0.0
0.5
1.0
1.5
aSi
0.5
0
Fig. 6.48 Theoretical calculation of the density of electronic states of amorphous silicon. The charge distribution in four selected states at the indicated energies is shown, from right to left with decreasing localization. Adapted from [479]
As another example, simulations of ZnSnO3 are shown in Fig. 6.49. The band tail between 0 and 0.5 eV is due to disorder of oxygen 2p orbitals [480]. At 0.9 eV a level due to undercoordinated oxygen appears. Deep levels are due to metalmetal bonds. Band tails due to chemically disordered oxygen have been experimentally observed for amorphous GIZO [481].
ZnSnO 3
60
Density of states (eV 1)
Fig. 6.49 Theoretical calculation for the density of states of crystalline (dashed lines, conduction and valence bands indicated by greay areas) and amorphous ZnSnO3 with different configurations (solid lines). States due to undercoordinated oxygen (Ouc ) and metalmetal binds are labelled. Adapted from [480]
40
20
Ouc SnSn
0
1
0
1
SnZn 2Sn 1Sn
2
Energy (eV)
3
4
5
6.12 Density of States
199
6.12.3 FreeElectron Gas In M dimensions, the energy states of a freeelectron gas are given as M 2 2 k . E(k) = 2 m ∗ i=1 i
(6.61)
The ki can take the values ±πn/L (in the first Brillouin zone) with n ≤ N , N being the number of unit cells in one dimension. These values are equidistant in kspace. Each Mdimensional kpoint takes a volume of (2π/L) M . The number of 2 2 states N (E F ) up to the energy E F = 2m kF (later used as Fermi energy E F and Fermi vector kF ) is k=kF 2 d M k. (6.62) N (E F ) = (2π/L) M k=0 The factor 2 is for spin degeneracy, the integration runs over M dimensions. The density of states is the derivative D(E) =
dN . dE
(6.63)
In the following, the density of states for M = 3, 2, 1 and zero dimensions is derived. A visualization is given in Fig. 14.1. M=3 This case relates to bulk material in which electrons are free to move in all three dimensions. Performing the integral (6.62) for M = 3 yields for an isotropic mass, N 3D =
V 3 V k = 3π 2 F 3π 2
2 m EF 2
3/2 .
(6.64)
Therefore, kF and E F are given by
1/3 3π 2 N kF = V 2 2/3 2 3π N , EF = 2 m∗ V
(6.65) (6.66)
and the density of states in three dimensions is D 3D (E) =
V 2π 2
2 m∗ 2
3/2
√
E.
(6.67)
200
6 Band Structure
Mostly the density of states is used as density of states per volume, then the factor V in (6.67) is omitted. If a conductionband minimum is degenerate, a factor gv (valley degeneracy) must be included in the density of states, i.e. gv = 6 for Si and gv = 8 for Ge (gv = 1 for GaAs). This factor is typically included in the mass used in (6.67) that then becomes the density of states mass m d,e . If the conductionband minimum has cylindrical symmetry in kspace, such as for Si and Ge, the mass that has to be used is 1/3 . m d,e = gv2/3 m 2t m l
(6.68)
In the case of a degeneracy of the valence band, the states of several bands need to be summed. In bulk material, typically the heavy and light hole bands are degenerate at the Γ point. If the splitoff band is not populated because of insufficient temperature, the valenceband edge density of states is expressed by the density of states hole mass 2/3 3/2 3/2 . m d,h = m hh + m lh
(6.69)
The density of states (per volume) at the conduction and valence band edges are thus given by De3D (E) =
1 2π 2
Dh3D (E) =
1 2π 2
2 m d,e 2 2 m d,h 2
3/2
3/2
E − EC, E > EC
(6.70)
E V − E, E < E V .
(6.71)
M=2 This case is important for thin layers in which the electron motion is confined in one direction and free in a plane. Such structures are called quantum wells (see Sect. 12.3.2). We find for the 2D density of states (for each subband over which it is not summed here, including spin degeneracy) N 2D =
A 2 A m∗ E, kF = 2π π 2
(6.72)
where A is the area of the layer. The density of states is thus constant and given by D 2D (E) =
A m∗ . π 2
(6.73)
M=1 The case M = 1 describes a quantum wire in which the electron motion is confined in two dimensions and free in only one dimension. For this case, we find for a wire
6.12 Density of States
201
of length L N 1D =
2L 2L kF = π π
2m ∗ E 2
1/2 .
(6.74)
The density of states becomes singular at E = 0 and is given by (for one subband) D 1D (E) =
L π
2m ∗ 2
1/2
1 √ . E
(6.75)
M=0 In this case electrons have no degrees of freedom, as, e.g., in a quantum dot (Sect. 14.3), and each state has a δlike density of states at each of the quantized levels.
Chapter 7
Electronic Defect States
Über Halbleiter sollte man nicht arbeiten, das ist eine Schweinerei, wer weiß ob es überhaupt Halbleiter gibt. One should not work on semiconductors. They are a mess. Who knows whether semiconductors exist at all. W. Pauli, 1931 [482]
Abstract After the carrier statistics for intrinsic conduction and general doping principles, donors and acceptors, compensation and high doping effects are treated in detail. The concept of quasiFermi levels is introduced. Finally for deep levels and their thermodynamics general remarks and several examples are given.
7.1 Introduction One centimeter cube of a semiconductor contains about 5 × 1022 atoms. It is practically impossible to achieve perfect purity. Typical low concentrations of impurity atoms are in the 1012 –1013 cm−3 regime. Such a concentration corresponds to a purity of 10−10 , corresponding to about one alien in the world’s human population. In the beginning of semiconductor research the semiconductors were so impure that the actual semiconducting properties could only be used inefficiently. Nowadays, thanks to large improvements in highpurity chemistry, the most common semiconductors, in particular silicon, can be made so pure that the residual impurity concentration plays no role in the physical properties. However, the most important technological step for semiconductors is doping, the controlled incorporation of impurities, in order to manage the semiconductor’s conductivity. Typical impurity concentrations used in doping are 1015 –1020 cm−3 . A milestone in the understanding of doping and the spreading of semiconductor technology was the 1950 textbook by Shockley [483].
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_7
203
204
7 Electronic Defect States
7.2 Carrier Concentration Generally, the density of electrons in the conduction band is given by n=
∞
De (E) f e (E) dE,
(7.1)
EC
and accordingly the density of holes in the valence band is p=
EV
Dh (E) f h (E) dE.
−∞
(7.2)
The energy of the top of the valence band is denoted by E V , the bottom of the conduction band as E C . The distribution function for holes is f h = 1 − f e . Thus, f h (E) = 1 −
exp
1 E−EF kT
+1
=
exp
1
F − E−E kT
+1
.
(7.3)
If several hole bands (hh, lh, so) are considered, the same distribution is valid for all hole bands in thermal equilibrium. We assume parabolic band edges, i.e. effective masses m e and m h for electrons and holes, respectively. The density of states (per volume) in the conduction and valence bands is given by (6.70) and (6.71). In thermodynamic equilibrium, the distribution function f e (E) for electrons is given by the Fermi–Dirac distribution (Fermi function) f e (E) (E.22) f e (E) =
exp
1 E−EF kT
+1
,
(7.4)
If the Boltzmann distribution (E.23) is a good approximation, the carrier distribution is called nondegenerate. If the Fermi distribution needs to be invoked, the carrier ensemble is called degenerate. If the Fermi level is within the band, the ensemble is highly degenerate. If the Boltzmann approximation (E.23) cannot be applied, i.e. at high temperatures or for very small band gaps, the integral over D f cannot be analytically evaluated. In this case the Fermi integral is needed that is defined1 as 2 Fn (x) = √ π
∞ 0
yn dy. 1 + exp(y − x)
(7.5)
∞ 1 is restricted to n > −1. A form without restriction is Fn (x) = Γ (n+1) 0 √ yn dy. The factor 2/ π is often omitted but must be then added explicitly in, e.g. (7.6). 1+exp(y−x)
1 Equation (7.5)
7.2 Carrier Concentration
205
(b)
(a)
√ Fig. 7.1 Fermi integral Fˆ1/2 = ( π/2)F1/2 with approximations in three regions of the argu√ √ ment: A1 (x) = ( π/2) exp(x) for x < 2, A2 (x) = ( π/2)(1/4 + exp(−x))−1 for −2 < x < 2, A3 (x) = 2/3x 3/2 for x > 2. (a) linear, (b) semilogarithmic plot
In the present case of bulk materials n = 1/2. For large negative argument, i.e. x < 0 and x 1, F1/2 (x) ≈ exp(x), which is the Boltzmann approximation. √ F1/2 (0) = 0.765 . . . ≈ 3/4. For large argument, i.e. x 1, F1/2 (x) ≈ (2/ π)(2/3) x 3/2 . Such fairly simple approximations are plotted in Fig. 7.1 in comparison with the Fermi integral. For computations, analytical [484–486] or numerical approximations [487, 488] are used. The derivative of the Fermi integral is given by Fn (x) = n Fn−1 (x), n > 0. For n =√0, i.e. a twodimensional system, the integral can be executed explicitly, F0 (x) = (2/ π) ln 1 + exp(x) . With the Fermi integral F1/2 (7.10) and (7.11) the freecarrier densities can be written as EF − EC (7.6) n = NC F1/2 kT EF − EV , (7.7) p = NV F1/2 − kT with
m e kT 3/2 NC = 2 2π 2 m h kT 3/2 , NV = 2 2π 2
(7.8) (7.9)
where NC (NV ) is called the conductionband (valenceband) edge density of states. The masses in (7.8) and (7.9) are the density of states masses given in (6.68) and (6.69). Values of NC,V for Si, Ge and GaAs are given in Table 7.1. Now, we assume that the Boltzmann approximation (Appendix E) can be used, i.e. the probability that a band state is populated is 1. Then, the integral (7.1) can
206
7 Electronic Defect States
Table 7.1 Band gap, intrinsic carrier concentration, conduction band and valenceband edge density of states at T = 300 K for various semiconductors
InSb InAs Ge Si GaAs GaP GaN
E g (eV)
n i (cm−3 )
0.18 0.36 0.67 1.124 1.43 2.26 3.3
1.6 × 1016 8.6 × 1014 2.4 × 1013 1.0 × 1010 1.8 × 106 2.7 × 100 1
NC (cm−3 )
NV (cm−3 )
1.04 × 1019 7.28 × 1019 4.35 × 1017
6.0 × 1018 1.05 × 1019 5.33 × 1018
be executed analytically and the concentration n of electrons in the conduction band is given as n=2
m e kT 2π2
3/2 exp
EF − EC kT
= NC exp
EF − EC kT
.
(7.10)
For the Boltzmann approximation and a parabolic valence band, the density of holes is given by p=2
m h kT 2π2
3/2
EF − EV EF − EV exp − = NV exp − . kT kT
(7.11)
The product of the electron and hole density is Eg EC − EV = NV NC exp − n p = NV NC exp − kT kT 3 Eg kT (m d,e m d,h )3/2 exp − . =4 2π2 kT
(7.12)
Thus, the product np is independent of the position of the Fermi level, as long as the Boltzmann approximation is fulfilled, i.e. the Fermi level is not in the vicinity of one of the band edges within several kT : E V + 4kT < E F < E C − 4kT.
(7.13)
The relation (7.12) is called the massaction law. In Fig. 7.2, the product np is shown for silicon over a wide range of Fermi energies. If E F is within the band gap, np is essentially constant. If the Fermi level is in the valence or conduction band, np decreases exponentially.
7.3 Intrinsic Conduction
207
(b)
(a)
Fig. 7.2 (a) np for silicon at T = 300 K as a function of the position of the Fermi level. The valenceband edge E V is chosen as E = 0. np is constant for the range of Fermi energies given by √ (7.13) (4kT ≈ 0.1 eV). (b) n, p and np as a function of the Fermi level
7.3 Intrinsic Conduction First, we consider the conductivity of the intrinsic, i.e. an ideally pure, semiconductor. At T = 0 all electrons are in the valence band, the conduction band is empty and thus the conductivity is zero (a completely filled band cannot conduct current). Only at finite temperatures the electrons have a finite probability to be in a conductionband state and to contribute to the conductivity. Due to neutrality, the electron and hole concentrations in the intrinsic semiconductors are the same, i.e. each electron in the conduction band comes from the valence band, − n + p = 0,
(7.14)
or n i = pi . Therefore
Eg n i = pi = NV NC exp − 2kT 3/2 Eg kT 3/4 (m m ) exp − . =2 e h 2π2 2kT
(7.15)
The massaction law np = n i pi = n 2i = pi2
(7.16)
will be essential also for light and moderately doped semiconductors. The intrinsic carrier concentration is exponentially dependent on the band gap. Thus, in thermodynamic equilibrium intrinsic widegap semiconductors have much smaller electron concentrations than intrinsic smallgap semiconductors (see Table 7.1). The intrinsic carrier concentration of Si (in cm−3 ) has been determined to be (within 1 %, T in K)
208
7 Electronic Defect States
(b)
(a)
Fig. 7.3 (a) Band gap of silicon versus temperature. (b) Intrinsic carrier concentration of silicon versus temperature. Solid line is (7.17) using E g = 1.204 eV − (2.73 × 10−4 eV/K) T [491], symbols are experimental data from [492]
E g (T ) 15 1.706 n Si = 1.640 × 10 T exp − i 2kT
(7.17)
for temperatures between 77 and 400 K [489, 490] (Fig. 7.3). As we will see later in Part II, many semiconductor devices rely on regions of low conductivity (depletion layers) in which the carrier concentration is small. Since the carrier concentration cannot be smaller than the intrinsic concentration (n + p ≥ 2n i ), an increase of temperature leads to increasing ohmic conduction in the depletion layers and thus to a reduction or failure of device performance. The small band gap of Ge leads to degradation of bipolar device performance already shortly above room temperature. For silicon, intrinsic conduction limits operation typically to temperatures below about 300 ◦ C. For higher temperatures, as required for devices in harsh environments, such as close to motors or turbines, other semiconductors with wider band gaps need to be used, such as GaN, SiC or even diamond. From the neutrality condition for the intrinsic semiconductor (7.14), (7.10) and (7.11), the Fermi level of the intrinsic semiconductor can be determined as EV + EC kT + ln EF = Ei = 2 2
NV NC
3 mh EV + EC + kT ln = . (7.18) 2 4 me
Since the hole mass is perhaps a factor of ten larger than the electron mass, the second term has the order of kT . Thus, for typical semiconductors where E g kT , the intrinsic Fermi level, denoted by E i , is close to the middle of the band gap, i.e. E i ≈ (E C + E V )/2. The situation for an intrinsic semiconductor is schematically shown in Fig. 7.4b.
7.4 Doping Fig. 7.4 Density of states (left column), Fermi distribution (center column) and carrier concentration (right column) for (a) ntype, (b) intrinsic and (c) ptype semiconductors in thermal equilibrium
209
(a)
E
E
EC ED
EF
E
EV
EV
D(E)
(b)
n
EC
f(E) E
E
p
n,p E
EC
EC
n
EV
p
EF EV
D(E)
(c)
f(E) E
E
n,p E
EC
EC
n
EF
EA EV
EV
D(E)
f(E)
p
n,p
7.4 Doping 7.4.1 Concept The modification of the conductivity of a semiconductor using point defects is termed doping. In 1930 electrical conduction of semiconductors was attributed solely to impurities [493]. However ‘chemically pure’ substances become conductive upon deviation from stoichiometry, e.g. historically found for changes in the anion concentration and conductivity in CuI [31] (ptype) and ZnO [70] (ntype). The modification of CuI by exposure to different partial pressure of iodine in organic solutions
210
7 Electronic Defect States
with different iodine concentration [34] and subsequently various concentrations of copper vacancies [494] can be considered the first doping of a semiconductor (1909). The electronic levels of a defect or an impurity can exist within the forbidden gap of the bulk host material. These levels can lie close to the band edges or in the vicinity of the middle of the band gap. In a simplified approach, the first stem from shallow defects (Sect. 7.5), the latter from deep defects (Sect. 7.7).
7.4.2 Doping Principles In [495] various doping principles are formulated. Essentially, the amount of impurities that lead to electrically active dopants is limited by the increasingly probable formation of compensating defects. In the case of donors, these are electron killers, e.g. ntype doping of Si:As is limited by the formation of VSi [496]. In the case of acceptors, the compensating defects are hole killers. The socalled ntype pinning n,pin is the Fermi level at which such killer defect (e.g. a cation vacancy) energy E F forms. When the Fermi level reaches the pinning energy, no further progress in ntype doping can be made, since the spontaneously generated electron killers will negate the introduced (impurity) donors. As a tendency, materials with low lying conduction band, i.e. large electron affinity (difference between vacuum level and conduction band) can be doped ntype. Similarly, ptype doping by acceptors, shifting the Fermi p,pin level towards the valence band, will meet at some point E F , called ptype pinning energy, when native hole killers, such as anion vacancies or cation interstitials form spontaneously. At this point, further ptype doping is no longer possible. ptype doping is facilitated by materials whose valance band maximum is close to the vacuum level [495]. A comparison of the wide gap materials ZnO, NiO and MgO is depicted in Fig. 7.5. The position of the pinning levels is marked on a common energy scale. From the n,pin position of E F it can be understood, that ZnO can be highly ndoped while NiO
NiO
MgO
EE V
ZnO
Fig. 7.5 Comparison of ZnO, NiO and MgO on a common energy scale, comparing conduction band and valence band edges and ntype (red) and ptype (blue) pinning energies (determined for metalrich and oxygenrich conditions, respectively). Adapted from [497]
7.4 Doping
211 p,pin
and MgO cannot [497]. From E F , NiO can be doped ptype, while MgO cannot be doped at all. For dopability, generally, it is also important that the ionized charges from impurities are free and thus contribute to the free charge carrier density and do not form localized states, e.g. due to polaronic effects (Sect. 8.6).
7.5 Shallow Defects In Fig. 7.6, the positions of the energy levels of a variety of impurities are shown for Ge, Si and GaAs. An impurity for which the longrange Coulomb part of the ioncore potential determines the energetic level is termed a shallow impurity. The extension of the wavefunction is given by the Bohr radius. This situation is in contrast to a deep level where the shortrange part of the potential determines the energy level. The extension of the wavefunction is then of the order of the lattice constant. A view on the history of the science of shallow impurity states is given in [498, 499]. We will consider first a groupIV semiconductor, Si, and (impurities) dopants from the groups III and V of the periodic system. When these are incorporated on a lattice site (with tetrahedral bonds), there is one electron too few (group III, e.g. B) or one electron too many (group V, e.g. As). The first case is called an acceptor, the latter a donor. The doping of III–V semiconductors is detailed in [501].
7.5.1 Donors Silicon doped with arsenic is denoted as Si:As. The situation is schematically shown in Fig. 7.7. The arsenic atom has, after satisfying the tetrahedral bonds, an extra electron. This electron is bound to the arsenic atom via the Coulomb interaction since the ion core is positively charged compared to the silicon cores. If the electron is ionized, a fixed positive charge remains at the As site. Without being in the silicon matrix, an arsenic atom has an ionization energy of 9.81 eV. However, in the solid the Coulomb interaction is screened by the dielectric constant of the material, typically r is of the order of 10 for typical semiconductors. Additionally, the mass is renormalized (effective mass) by the periodic potential to a value that is smaller than the free electron mass. Within effectivemass theory (Appendix H) Bohr’s theory of the hydrogen problem is scaled with the (isotropic) effective mass m ∗e and the dielectric constant r , the binding energy (ionization energy) E Db of the electron to the shallow donor is (relative to the continuum given by the conductionband edge E C ) E Db =
m 0 e4 m ∗e 1 . 2 m 0 r 2 (4π0 )2
(7.19)
212
7 Electronic Defect States
(a)
(b)
(c)
Fig. 7.6 Energetic position (ionization energy labeled in meV) of various impurities (A: acceptor, D: donor) in (a) Ge, (b) Si and (c) GaAs. Based on [500] Fig. 7.7 Arsenic impurity in silicon. Arsenic donates one electron, and a fixed positive charge remains
Si
Si
As
Si
Si
Si
Si
Si
7.5 Shallow Defects
213
The absolute energy position of the level is E D = E C − E Db . The first factor in the right side of (7.19) is the ratio of effective and freeelectron mass, typically 1/10, the second factor is typically 1/100. The third factor is the ionization energy of the hydrogen atom, i.e. the Rydberg energy of 13.6 eV. Thus, the binding energy in the solid is drastically reduced by a factor of about 10−3 to the 10 meV regime. The excited states of the hydrogenlike spectrum can also be investigated experimentally (Sect. 9.7). The extension of the wavefunction of the electron bound to the fixed ion is given by the Bohr radius m0 (7.20) aD = ∗ r aB , me where aB = 0.053 nm denotes the hydrogen Bohr radius. For GaAs aD = 10.3 nm. A similar value has been determined for InP [502]. For semiconductors with a nonisotropic band minimum, such as Si, Ge or GaP, an ‘elliptically deformed’ hydrogen problem with the masses m l and m t has to be treated [503]. An impurity that fulfills (7.19) is called an effectivemass impurity. For GaAs, the effectivemass donor has a binding energy of 5.715 meV, which is closely fulfilled for several chemical species (Table 7.3). In GaP, experimental values deviate considerably from the effectivemass donor (59 meV). For silicon, considering the anisotropic tensor of the effective masses, the result for the effectivemass donor binding energy is 29 meV [503]. Some experimentally observed values are summarized in Table 7.2.
Table 7.2 Binding energies E Db of Li and groupV donors in elemental semiconductors Li C Si Ge
N
P
As
Sb
1700
≈500 45 12.0
49 12.7
39 9.6
33 9.3
Data for carbon from [505]. All values in meV Table 7.3 Binding energies E Db of donors in GaAs (data from [506]), GaP (data from [507]) and GaN (low concentration limits, data from [508, 509]) V site III site GaAs
GaP
GaN All values in meV
S Se Te O S Se Te O
5.854 5.816 5.786 897 107 105 93 39
C Si Ge Si Ge Sn
5.913 5.801 5.937 85 204 72
Si Ge
22 19
214
7 Electronic Defect States
Fig. 7.8 Electron spin resonance signal from As and P in Ge with the magnetic field H parallel to [100], T ≈ 1.3 K. Adapted from [504]
Deviations from the effectivemass theory are due to modification of the potential in the immediate vicinity of the impurity atom and breakdown of the effectivemass formalism. Different impurities can have quite similar binding energies. They can be distinguished, e.g. by electron spin resonance (ESR). At low temperatures the electron is localized on the impurity and the hyperfine interaction with the nucleus can be resolved in ESR. In Fig. 7.8 data are shown for As and P in germanium. The multiplets distinguish the nuclear spins I = 3/2 for arsenic (75 As) and I = 1/2 for phosphorus (31 P) [504]. The donors are typically distributed statistically (randomly) in the solid. Otherwise their distribution is called clustered. The concentration of donors is labeled ND and usually given in cm−3 . The concentration of donors populated with an electron (neutral donors) is denoted by ND0 , the concentration of ionized donors (positively charged) is ND+ . Other conventions in the literature label the concentrations N1 and N0 , respectively: N1 = ND0 = ND f e (E D )
N0 = ND+ = ND (1 − f e (E D )),
(7.21a) (7.21b)
−1 with f e (E D ) = 1 + exp(E D − E F ) . For the sum of these quantities the condition ND = ND+ + ND0
(7.22)
holds. The ratio of the two concentrations is first given as (caveat: this formula will be modified below) ND0 N1 f EF − ED = = = exp . (7.23) N0 1− f kT ND+ Now, the degeneracy of the states has to be considered. The donor charged with one electron has a 2fold degeneracy g1 = 2 since the electron can take the spin up and
7.5 Shallow Defects
215
down states. The degeneracy of the ionized (empty) donor is g0 = 1. Additionally, we assume here that the donor cannot be charged with a second electron (cmp. Sect. 7.7.2). Due to Coulomb interaction, the energy level of the possible ND− state is in the conduction band. Otherwise, a multiply charged center would be present. We also do not consider excited states of ND0 that might be in the band gap as well. In the following, we will continue with gˆD = g1 /g0 = 2 as suggested in [510].2 We note that the definition of the degeneracy factor for donors (and acceptors, see (7.39)) is not consistent in the literature as summarized in [511]. Considering now the degeneracy, (7.23) is modified to N1 ND0 = = gˆD exp N0 ND+
EF − ED kT
.
(7.24)
This can be understood from thermodynamics (cf. Sect. 4.2.2), a rate analysis or simply the limit T → ∞. The probabilities f 1 and f 0 for a populated or empty donor, respectively, are N1 1 = −1 ED −EF ND +1 gˆD exp kT N0 1 = . ED −EF f0 = ND +1 gˆD exp − kT f1 =
(7.25a) (7.25b)
First, we assume that no carriers in the conduction band stem from the valence band (no intrinsic conduction). This will be the case at sufficiently low temperatures when ND n i . Then the number of electrons in the conduction band is equal to the number of ionized donors, i.e. n = f 0 ND = N0 =
ND 1 + gˆD exp
EF −ED = kT
1 ND , 1 + n/n 1
with n 1 = (NC /gˆD ) exp −E Db /kT . The neutrality condition (its general from is given in (7.41)) is (7.26) − n + ND+ = −n + N0 = 0, leading to the equation (n is given by (7.10)) NC exp
EF − EC kT
−
ND −ED = 0. 1 + gˆ exp EFkT
(7.27)
2 We do not agree with the treatment of the conduction band valley degeneracy in [510] for the donor
degeneracy factor for Ge and Si.
216
7 Electronic Defect States
(b)
(a)
Fig. 7.9 (a) Position of the Fermi level in Si:P (ND = 1015 cm−3 , E Db = 45 meV, no acceptors) as a function of temperature without consideration of intrinsic carriers. Zero energy refers to the (temperaturedependent, Table 6.4) conductionband edge E C with approximative solutions for low (dashed line, (7.29)) and high (dashdotted line, (7.30)) temperatures. (b) Corresponding density of conductionband electrons as a function of temperature
Solving this equation will yield the Fermi level (as a function of temperature T , doping level E D and doping concentration ND ).3 The solution is ⎛ ⎜ E F = E C − E Db + kT ln ⎝
1 + 4gˆD
ND NC
exp
E Db kT
1/2
2 gˆD
−1
⎞ ⎟ ⎠.
(7.28)
For T → 0 the Fermi level is, as expected, in the center between the populated and unpopulated states, i.e. at E F = E C − E Db /2. In Fig. 7.9a the position of the Fermi is shown for a donor with 45 meV binding energy in Si. For low temperatures the solution can be approximated as (dashed curve in Fig. 7.9b) 1 1 ND . EF ∼ = E C − E Db + kT ln 2 2 gˆD NC
(7.29)
The freezeout of carriers in ntype silicon has been discussed in detail in [512], taking into account the effects of the fine structure of the donor states. We note that the fairly high donor binding energy in silicon leads to freezeout of carriers at about 40 K and is thus limiting for the lowtemperature performance of devices. Ge has smaller donor ionization energies and subsequently a lower freezeout temperature of 20 K. For ntype GaAs, conductivity is preserved down to even lower temperatures.
3 As
usual, the Fermi level is determined by the global charge neutrality, see also Sect. 4.2.2.
7.5 Shallow Defects
217
We note that the freezeout of carriers involves the recombination of free electrons with the ionized donors. This aspect is considered in Sect. 10.9. Microscopically this process is equal to the emission of a (far infrared) photon [513, 514]. Similarly the release of an electron from the donor is due to the absorption of a photon. For higher temperatures, when the electron density saturates towards ND , the approximate solution is (dashdotted curve in Fig. 7.9a)
EF ∼ = E C + kT ln
ND NC
.
(7.30)
The electron density n is given (still in the Boltzmann approximation) by n = NC exp − =
E Db
1 + 4 gˆD
ND NC
exp
E Db kT
1/2
−1
2 gˆD
kT 2 ND
1 + 1 + 4 gˆD
ND NC
exp
E Db kT
1/2 .
(7.31)
The theoretical electron density as a function of temperature is shown in Fig. 7.9b. It fits very well to experimental data for arsenic doped germanium [515] as shown in Fig. 7.10 (Arrhenius plot, ln n vs. 1/T ). For low temperatures, the solution (7.31) is close to n∼ =
Fig. 7.10 Electron concentration as a function of temperature for a Ge:As sample with ND ≈ 1013 cm−3 . Solid line is fit to the data with a donor binding energy of 12.7 meV. Adapted from [515]
ND NC Eb exp − D = n 1 ND . gˆD 2kT
300 78
33.3
14
(7.32)
20.4
14.3
10
10
Ge:As
3
1013
1012 ni 1011 0
20
40
60
1000/T (1/K)
80
100
218
7 Electronic Defect States
∼ ND . This regime is called exhaustion or saturation For high temperatures, n = since all possible electrons have been ionized from their donors. We note that even in this case np = n i pi holds, however, n p. While the characteristic energy for the ionization of electrons from donors is E Db , at high enough temperatures electrons are transferred also from the valence band into the conduction band. Thus, in order to make the above consideration valid for all temperatures, the intrinsic conduction also has to be considered. The neutrality condition (still in the absence of any acceptors) is − n + p + ND+ = 0.
(7.33)
Using (7.10) and p = n 2i /n, the equation reads: NC exp
EF − EC kT
−
ND n 2i EF −EC − −ED = 0. NC exp kT 1 + gˆD exp EFkT
(7.34)
The solution is
EF = EC −
E Db
β/γ + γ/NC2 − 1 + kT ln , 3 gˆD
(7.35)
with ⎛ γ=⎝
−NC4 α +
(NC4 α)2 − 4(NC2 β)3 2
⎞1/3 ⎠
ED 2E D 2 2 β= + 3gˆD NC ND exp + 3gˆD n i exp kT kT ED 2E D 2 2 2 − 18gˆD n i exp . α = 2NC + 9gˆD NC ND exp kT kT
(7.36a)
NC2
(7.36b) (7.36c)
The temperaturedependent position of the Fermi level is shown in Fig. 7.11. The carrier concentration is given by
Eb n = NC exp − D kT
β/γ + γ/NC2 − 1 . 3 gˆD
(7.37)
The three important regimes are the intrinsic conduction at high temperatures when n i ND , the exhaustion at intermediate temperatures when n i ND and kT > E D , and finally the freezeout regime for kT E D at low temperatures when the electrons condense back into the donors. The three regimes can be seen in the experimental data of Fig. 7.10 for donors (nGe) and Fig. 7.15 for acceptors (pGe).
7.5 Shallow Defects
(a)
219
(b)
Fig. 7.11 (a) Position of the Fermi level in Si:P (ND = 1015 cm−3 , E Db = 45 meV, no acceptors) as a function of temperature. The temperature dependence of the band gap (as given in Table 6.4) has been taken into account. Zero energy refers to the conductionband edge for all temperatures. The dotted curve shows E g /2. The dashed (dashdotted) line shows the low (high) temperature limit according to (7.29) and (7.18), respectively. (b) Corresponding electron concentration as a function of temperature. The dashed line shows the intrinsic carrier density Fig. 7.12 Fermi level in silicon as a function of temperature for various doping levels (ntype (blue lines) and ptype (red lines)) of 1012 , 1013 , . . . , 1018 cm−3 . The intrinsic Fermi level is chosen as zero energy for all temperatures. The (temperaturedependent) conduction and valence band edges are shown as dashed lines
A similar plot as in Fig. 7.11a is shown in Fig. 7.12. With increasing temperature the Fermi level shifts from close to the band edge towards the band center. At higher doping the shift begins at higher temperatures. The electronic states of individual donors can be directly visualized by scanning tunneling microscopy (STM) as shown in Fig. 7.13 for Si:P. For small negative bias, tunneling occurs through the charged dopant that is located within the first three monolayers. At high negative bias the large contribution from the filled valence band masks the effect of the donor. This image, however, shows that the contrast attributed to the dopant atom is not due to surface defects or absorbates.
220
7 Electronic Defect States
(b)
(a)
Si EF
tip
D EF
Fig. 7.13 Filledstate image of a phosphorus atom underneath a Si (001) surface at a tunneling current of 110 pA. The doping level is 5 × 1017 cm−3 . (a) Sample bias −0.6 V, (b) sample bias −1.5 V between Si:P and tip. Image sizes are 22 × 22 nm2 . Reprinted with permission from [516], c 2004 APS. Lower row Schematic band diagrams for the two bias situations
7.5.2 Acceptors A groupIII atom in Si has one electron too few for the tetrahedral bond. Thus, it ‘borrows’ an electron from the electron gas (in the valence band) and thus leaves a missing electron (termed hole) in the valence band (Fig. 7.14). The energy level of the impurity is in the gap close to the valenceband edge. The latter consideration is made in the electron picture. In the hole picture, the acceptor ion has a hole and the hole ionizes (at sufficient temperature) into the valence band. After ionization the acceptor is charged negatively. Also, for this system a Bohrlike situation arises that is, however, more complicated than for donors because of the degeneracy of the valence bands and their warping. In Table 7.4 the acceptor binding energies E Ab for groupIII atoms in C, Ge and Si are listed. The absolute acceptor energy is given as E A = E V + E Ab . In Table 7.5 acceptor binding energies are listed for GaAs, GaP and GaN. While in GaAs some
7.5 Shallow Defects
221
Fig. 7.14 Boron impurity in silicon. Boron accepts one electron and a fixed negative charge remains
Si
Si
Si
Si
Si
B
Si
Si
Table 7.4 Binding energies E Ab of groupIII acceptors in elemental semiconductors C Si Ge
B
Al
Ga
In
369 45 10.4
57 10.2
65 10.8
16 11.2
Data for diamond from [517, 518]. All values in meV Table 7.5 Binding energies E Ab of acceptors in GaAs, GaP and GaN (low concentration values, data from [519, 520]) V site III site GaAs
GaP
GaN
C Si Ge Sn C Si Ge
27 34.8 40.4 167 54 210 265
C Si
230 224
Be Mg Zn Cd Be Mg Zn Cd Mg Zn Cd
28 28.8 30.7 34.7 57 60 70 102 220 340 550
All values in meV
acceptors are close to the effective mass value of 27 meV, in GaP the deviation from the effectivemass value ≈50 meV is large. When the conductivity is determined by holes or electrons, the material is called ptype or ntype, respectively. We note that some metals also show hole conduction (e.g. Al). However, for metals the conductivity type is fixed, while the same semiconductor can be made n or ptype with the appropriate doping. The acceptor concentration is denoted by NA . The concentration of neutral acceptors is NA0 , the concentration of charged acceptors is NA− . Of course NA = NA0 + NA− .
(7.38)
222
7 Electronic Defect States
The ratio of the degeneracy of the (singly) filled and empty acceptor level is gˆA . In Ge gˆA = 4 since the localized hole wave function may be formed in EMA with four Bloch wave functions (heavy and light holes) [521]. For Si with its small splitoff energy (Table 6.6) gˆA = 6 according to [522]. For doubly ionized acceptors, e.g. Zn in Si and Ge (see Sect. 7.7.3), the more shallow level (Zn− → Zn0 ) has gˆA = 6/4 = 1.5 in Ge [522]. A more general discussion of the degeneracy factor for multiply charged acceptors can be found in [510, 523]. Similar to the considerations for electrons and donors we have EF − EA NA0 = g ˆ exp − . (7.39) A kT NA− The population of the acceptor levels is given by NA− =
NA . −E A 1 + gˆA exp − EFkT
(7.40)
The formulas for the position of the Fermi level and the hole density are analogous to those obtained for electrons and donors and will not be explicitly given here. The analogue to Fig. 7.11b is shown for data on pdoped Ge [524, 525] in Fig. 7.15. The acceptor activation energy is 11 meV which could be due to various impurities (cf. Table 7.4). The different impurities (B, Al, Ga) can be distinguished by photothermal ionization spectroscopy [525] (cmp. Sect. 9.7). In Fig. 7.12, the temperature dependence of the Fermi level is included for ptype Si. With increasing temperature the Fermi level shifts from the valenceband edge (For T = 0, E F = E V + E Ab /2) towards the middle of the band gap (intrinsic Fermi level). Also, the wavefunction at acceptors can be imaged using scanning tunneling microscopy [526]. In [527] images of ionized and neutral Mn in GaAs have been
Fig. 7.15 Carrier concentration as a function of temperature for ptype Ge. The net shallow level concentration is 2 × 1010 cm−3 . Solid line is fit to the data, the dashed line indicates the intrinsic hole concentration pi . Adapted from [525]
7.5 Shallow Defects
223
(c)
(b) (a) GaAs:Mn 40 Mn A0 channel 20
GaAs
UFB
0.8
EF
MnGa
0
A
GaAs
0.4
0.0
0.4
0.8
1.2
tip
A
EF
1.6 negative bias
Fig. 7.16 (a) Tunneling I –V characteristic of GaAs:Mn sample. Solid (dashed) line is for pure GaAs (subsurface Mn on Ga site). UFB denotes the simulated flatband voltage. Adapted from [527]. (b, c) STM images of a Mn atom underneath a GaAs (110) surface. The doping level is 3 × 1018 cm−3 . (b) Sample bias −0.7 V, (c) sample bias +0.6 V. Below the images are schematic band diagrams of GaAs:Mn and tip. Image sizes are (b) 8 × 8 nm2 and (c) 5.6 × 5 nm2 . Reprinted with c permission from [527], 2004 APS. Lower row under parts (a, b): Schematic band diagrams for the two bias situations
reported (Fig. 7.16b). The tunneling I –V characteristics are shown in Fig. 7.16a. At negative bias, the acceptor is ionized and appears spherically symmetric due to the effect of the A− ion Coulomb potential on the valenceband states. At intermediate positive voltages, tunneling is through the neutral state. The wavefunction of A0 looks like a bowtie due to the admixture of dwavefunctions [528]. The Mn atom is presumably in the third subsurface atomic layer. At even higher positive bias the contrast due to the dopant is lost because the image is dominated by a large tunneling current from the tip to the empty conduction band.
7.5.3 Compensation When donors and acceptors are simultaneously present, some of the impurities will compensate each other. Electrons from donors will recombine with holes on the acceptors. Depending on the quantitative situation the semiconductor can be n or ptype. This situation can be invoked by intentional doping with donors or acceptors or by the unintentional background of donors (acceptors) in pdoped (ndoped) material. Also the formation of pairs, exhibiting a new defect level different from the single donor or single acceptor, has been described, e.g. for Se and B in silicon [273].
224
7 Electronic Defect States
The chargeneutrality condition (now finally in its most general form) reads − n + p − NA− + ND+ = 0.
(7.41)
We will now discuss the case of the presence of donors and acceptors, but limit ourselves to sufficiently low temperatures (or wide band gaps) such that the intrinsic carrier density can be neglected. We assume Boltzmann statistics and assume here ND > NA . Then it is a very good approximation to use NA− = NA since there are enough electrons from the donors to recombine with (and thus compensate) all acceptors. Under the given assumptions regarding the temperature p = 0 and the material is ntype. Thus, in order to determine the position of the Fermi level, the chargeneutrality condition (7.42) n + NA − ND+ = 0 must be solved (compare to (7.27)) NC exp
EF − EC kT
+ NA −
ND −E D 1 + gˆ exp( EFkT )
= 0.
We rewrite (7.42) and find ND − NA − n = ND0 = ND+ gˆD exp (7.24). Using again (7.42) and also (7.10), (7.43) can be written as
(7.43)
EF −ED kT
Eb NC n (n + NA ) exp − D , = ND − NA − n gˆD kT
using
(7.44)
a form given in [529]. Analogously for compensated ptype material p ( p + ND ) Eb NV exp − A = NA − ND − p gˆA kT
(7.45)
holds. The solution of (7.43) is ⎛ ⎞ b 1/2 ED ND −NA 2 −α α + 4gˆD NC exp kT ⎜ ⎟ E F = E C − E Db + kT ln ⎝ ⎠, 2 gˆD
(7.46)
with b NA ED NA α = 1 + gˆD exp =1+ NC kT β
(7.47a)
7.5 Shallow Defects
225
NC E Db β= exp − . gˆD kT
(7.47b)
The carrier density is best obtained from (7.44), n=
NA + β (NA − β)2 + 4 ND β − . 2
(7.48)
For NA = 0 we have α = 1 and (7.28) is reproduced, as expected. For T = 0 (and NA = 0) the Fermi energy lies at E F = E D since the donor level is partially filled (ND0 = ND − NA ). For low temperatures the Fermi level is approximated by EF ∼ = E C − E Db + kT ln
ND /NA − 1 . gˆD
(7.49)
The corresponding carrier density at low temperatures is n=
Eb ND NC exp − D −1 . gˆD kT NA
(7.50)
For higher temperatures (7.32) holds approximately for n > NA ; the slope is now given by E Db /2 as in the uncompensated case (Fig. 7.17b). For sufficiently high
(a)
(b)
Fig. 7.17 (a) Position of Fermi level in partially compensated Si:P,B (ND = 1015 cm−3 , E Db = 45 meV, E Ab = 45 meV, solid line NA = 1013 cm−3 , dashed line NA = 0, dashdotted line NA = 1012 cm−3 , shortdashed line NA = 1014 cm−3 , dashdouble dotted line NA = 5 × 1014 cm−3 ) as a function of temperature. (b) Corresponding electron concentration for NA = 1013 cm−3 as a function of temperature (neglecting intrinsic carriers), dashed line for NA = 0 according to (7.31), dashdotted line approximation for n NA as in (7.50)
226
7 Electronic Defect States
Fig. 7.18 Hole density in ptype silicon (NA = 7.4 × 1014 cm−3 , E Ab = 46 meV (probably boron) and partial compensation with ND = 1.0 × 1011 cm−3 ). Adapted from [530]
1015
NA
14
3
10
slope =^
1013 1012 1011
ND slope =^
1010 109 10
Si
8
0
0.01
0.02
0.03
0.04
0.05
0.06
1/T (1/K)
temperatures in the exhaustion regime (but still n i < n) the electron density is given by n∼ = ND − NA .
(7.51)
At even higher temperatures the electron density will be determined by the intrinsic carrier concentration. Only in this case p = 0! An experimental example is shown in Fig. 7.18 for partially compensated pSi (with ND NA ). The change of slope around p ≈ ND is obvious. If donors are added to a ptype semiconductor, first the semiconductor remains pconducting as long as ND NA . If the donor concentration becomes larger than the acceptor concentration, the conductivity type switches from p to nconduction. If the impurities are exhausted at room temperature, the lowest carrier concentration is reached for ND = NA . Such a scenario is shown for ptype Inx Ga1−x As1−y N y doped with various concentrations of Si in Fig. 7.19. At high Si incorporation, the number of charge carriers saturates due to autocompensation (see Sect. 7.5.5) and the formation of Si precipitates. Since the ionization energies of donors and acceptors are typically different, the situation for ND ≈ NA needs, in general, to be investigated carefully and will depend on the temperature.
7.5.4 Multiple Impurities If more than one donor species is present, (7.43) can be generalized, e.g. for the case of two donors D1 and D2 in the presence of compensating acceptors, n + NA −
ND1 1+
D1 gˆ1 exp( EF −E ) kT
−
ND2 D2 1 + gˆ2 exp( EF −E ) kT
= 0.
(7.52)
7.5 Shallow Defects
227
Fig. 7.19 Carrier concentration and conductivity type (red circles p, blue squares n) for MOVPEgrown Inx Ga1−x As1−y N y layers on GaAs (001) (layer thickness ≈ 1 µm, x ≈ 5%, y ≈ 1.6%) doped with different amounts of silicon. The ordinate is the ratio of the partial pressures of disilane and the groupIII precursors (TMIn and TMGa) in the gas phase entering the MOVPE reactor. Lines are guides to the eye. Experimental data from [531]
(a)
(b)
Fig. 7.20 (a) Electron concentration versus temperature as determined from Hall effect for a CdTe sample doped with indium. (b) −kT dn/dE F , as determined from the experimental Hall data (symbols). The solid line is theory for three donor levels (E D1 = E C − 0.37 eV, ND1 = 2.5 × 1012 cm−3 ; E D2 = E C − 0.24 eV, ND2 = 7.0 × 1011 cm−3 ; E D3 = E C − 0.18 eV, ND3 = 2.5 × 1011 cm−3 ) whose energy positions are indicated by dashed lines. Adapted from [533]
This case is treated in [532]. Simple high and low temperature approximations can be found where the trap with the larger and smaller activation energy, respectively, dominates. The case for multiple acceptors (and compensating donors) is treated analogously. As detailed in [533], the function dn/dE F has a maximum at the donor level position; this can be used to visualize the contribution of several donors (with sufficiently different binding energies) from n(T ) as measured by Hall effect (Fig. 7.20).
228
7 Electronic Defect States
7.5.5 Amphoteric Impurities If an impurity atom can act as a donor and acceptor it is called amphoteric. This can occur if the impurity has several levels in the band gap (such as Au in Ge or Si). In this case, the nature of the impurity depends on the position of the Fermi level. Another possibility is the incorporation on different lattice sites. For example, carbon in GaAs is a donor if incorporated on the Gasite. On the Assite carbon acts as an acceptor. Thus, e.g. crystal growth kinetics can determine the conductivity type. In Fig. 7.21 the conductivity due to carbon background is shown for GaAs grown using MOVPE under various growth conditions. At high (low) arsine partial pressure incorporation of carbon on Assites is less (more) probable, thus the conductivity is ntype (ptype). Also, growth on different surfaces can evoke different impurity incorporation, e.g. ntype on (001) GaAs and ptype on (311)A GaAs, since the latter is Gastabilized. The charge density at an impurity nucleus can be investigated via the isomer shift as determined by Mössbauer spectroscopy [535, 536]. The incorporation of the isotope 119 Sn can be controlled in IIIV compounds to be on cation or anion site as donor or acceptor, respectively. This is accomplished by introducing 119 In or 119 Sb on groupIII and groupV site, respectively, both decaying into 119 Sn without leaving their lattice site. The isomer shifts of 119 Sn in various IIIV compounds are shown in Fig. 7.22. In [536] it is concluded from these data that the tin donor is formed by a positive tin ion and the electron charge transfer to its neighboring (groupV) atoms is rather small. For tin as an acceptor, for the present conditions an ionized, i.e. negatively charged acceptor, the isomer shift follows closely the trend from substitution in groupIV semiconductors. Therefore four electrons form the tetrahedral bond, while the extra electron is located rather at the (positively charged) groupIII next neighbors and not in the impurity cell. The difference to the point charge Coulomb distribution is called centralcell correction.
Fig. 7.21 Background doping of GaAs due to carbon in MOVPE for different ratios of the partial pressures of AsH3 and TMG (trimethylgallium). The conductivity type (blue squares ntype, red circles ptype) depends on the incorporation of C from CH3 radicals on Ga or Assite. Lines are guides to the eye. Experimental data from [534]
7.5 Shallow Defects
229
Fig. 7.22 Isomer shift (relative to CaSnO3 ) of 119 Sn in various groupIV and IIIV compound semiconductors as labeled. Dashed line is trend from isoelectronic substitution. Experimental data from [536]
Fig. 7.23 Carrier concentration and conductivity type (blue squares ntype, red circles ptype) as a function of stoichiometry for CuInSe2 thin films. Lines are guides to the eye. Experimental data from [537]
Deviation from the ideal stoichiometry introduces point defects that can be electrically active and change conductivity type and carrier concentration. In the case of CuInSe2 , excess Cu could go on interstitial positions or promote selenium vacancies, both leading to ntype behavior. This material is particularly sensitive to deviations from ideal stoichiometry for both Cu/In ratio (Fig. 7.23) and Se deficiency [537].
7.5.6 Autodoping If intrinsic defects such as vacancies or interstitials, possibly as a result of nonstoichiometry, or antisite defects cause electronic levels relevant for conductivity one speaks of autodoping. An example is the role of AB antisites in AB2 O4 spinels
230 Fig. 7.24 Schematic position of electronic levels of AB (blue, 0/− transition level) and BA (red, +/0 transition level) defects in AB2 O4 spinels and resulting material properties (compensated, n or ptype or semiinsulating). After [538]
7 Electronic Defect States
comp.
ptype
ntype
s.i.
CB
B Td
EF
A oh
VB
(Sect. 3.4.7). In the perfect crystal the A (B) atoms occupy tetraeder (octaeder) places. Typical charges are A2+ and B3+ . Thus (without charge transfer) the A atom on octaeder site (AOh ) acts like a donor and the B atom on a tetraeder site (BTd ) as an acceptor. Such defects have been classified in [538] as being able to create compensated, semiinsulating, ntype or ptype material depending on the defect formation energies and the position of the electronic levels of the AB and BA defects in the band gap (Fig. 7.24). An example for a ptype spinel oxide is ZnCo2 O4 [539].
7.5.7 High Doping For low doping concentrations, the impurity atoms can be considered to be decoupled. At low temperature, only hopping from one impurity to the next is possible due to thermal emission or tunneling and the semiconductor becomes an insulator. With increasing concentration, the distance between impurities decreases and their wavefunctions can overlap. Then, an impurity band develops (Fig. 7.25). A periodic arrangement of impurity atoms would result in welldefined band edges as found in the Kronig–Penney model. Since the impurity atoms are randomly distributed, the band edges exhibit tails. For high doping, the impurity band overlaps with the conduction band. In the case of compensation, the impurity band is not completely filled and contains (a new type of) holes. In this case, conduction can take place within the impurity band even at low temperature, making the semiconductor a metal. This metal–insulator transition has been discussed by Mott [540]. Examples for highly doped semiconductors are transparent conductive oxides (Chap. 20), the contact layer for an ohmic contact (Sect. 21.2.6) or the active
7.5 Shallow Defects
231
Fig. 7.25 Principle of the formation of a (donor) impurity band. (a) Small doping concentration and sharply defined impurity state at E D , (b) increasing doping and development of an impurity band that (c) widens further and eventually overlaps with the conduction band for high impurity concentration. The shaded areas indicate populated states at T = 0 K
(a)
(b)
(c)
E
E
E
EC ED
EC
EV
EV
D(E)
EV
D(E)
D(E)
layers in a tunneling diode (Sect. 21.5.9). The physics, properties and preparation of highly doped semiconductors are treated in detail in [541]. The formation of the impurity band leads to a reduction of the impurity ionization energy as known from (7.19). Typical results are shown in Fig. 7.26a for ntype Ge [515] and Fig. 7.26b for ptype ZnTe [542]. At the critical doping concentration of Nc = 1.5 × 1017 , the activation energy for the carrier concentration disappears. Similar effects have been observed for Si [543] and GaAs [544]. The freezeout of the carrier concentration (see Fig. 7.9) disappears as shown in Fig. 7.27. Critical doping concentrations are listed in Table 7.6. The decrease of the ionization energy E b (donor or acceptor) follows the dependence [515, 543]
(a)
(b)
15
Ge:As
b
ED
10
5
0 1012 1013
1014
1015
1016
1017
1018
3
NDNA (cm )
Fig. 7.26 (a) Donor ionization energy in ntype Ge for various doping concentrations. Dashed line is a guide to the eye. The arrow labeled E Db denotes the lowconcentration limit (cf. Table 7.2). Experimental data from [515]. (b) Acceptor ionization energy for ZnTe:Li and ZnTe:P as a function of the third root of the ionized acceptor concentration. Data from [542]
232
7 Electronic Defect States 10
20
10
19
10
18
10
17
10
16
3
Fig. 7.27 Electron concentration versus inverse temperature for Si:P for three different doping concentrations ((i): 1.2 × 1017 cm−3 , (ii): 1.25 × 1018 cm−3 , (iii): 1.8 × 1019 cm−3 ). Experimental data from [543]
(iii)
(ii)
(i) Si:P
10
15
0
2
4
6
8
10
12
14
1/T (1000/K) Table 7.6 Critical doping concentration for various semiconductors (at room temperature)
Material
Type
Nc (cm−3 )
Ref.
C:B Ge:As Si:P Si:B GaAs GaP:Si GaP:Zn GaN:Si GaN:Mg Al0.23 Ga0.77 N:Si ZnTe:Li ZnTe:P ZnO:Al
p n n p n n p n p n p p n
2 × 1020 1.5 × 1017 1.3 × 1018 6.2 × 1018 1.0 × 1016 6 × 1019 2 × 1019 2 × 1018 4 × 1020 3.5 × 1018 4 × 1018 6 × 1018 8 × 1018
[518] [515] [543] [543] [544] [546] [547] [548] [519] [549] [542] [542] [550]
E = b
E 0b
−α
1/3 Ni
=
E 0b
1−
Ni Nc
1/3 ,
(7.53)
where Ni is the concentration of ionized dopants. A refined theory, considering screening, shift and tails of the conduction band and most importantly broadening of the donor level has been presented in [545]. The critical density can be estimated from the Mott criterion when the distance of the impurities becomes comparable to their Bohr radius (7.20) 2aD =
3 1/3 N . 2π c
(7.54)
7.5 Shallow Defects Table 7.7 Maximum electrically active doping concentration for GaAs
233 Material
Type
Nc (cm−3 )
Ref.
GaAs:Te GaAs:Si GaAs:C GaAs:Be
n n p p
2.6 × 1019 1.8 × 1019 1.5 × 1021 2 × 1020
[554] [555] [556] [557]
The prefactor 3/(2π) stems from the random distribution of impurities and disappears for a periodic arrangement. The Mott criterion is (rewriting (7.54)) aD Nc1/3 ≈ 0.24.
(7.55)
For GaAs with aD = 10.3 nm, the criterion yields Nc = 1.2 × 1016 cm−3 , in agreement with experiment. The achievable maximum concentration of electrically active dopants is limited by the concentration dependence of the diffusion coefficient, Coulomb repulsion, autocompensation and the solubility limit [501]. In Table 7.7 the maximum carrier concentrations for GaAs with various dopants are listed. As an example we show the Gadoping of epitaxial ZnO layers on sapphire in Fig. 7.28. Under slightly Znrich (Opolar) conditions the growth mode is twodimensional and the carrier concentration increases linearly with the Ga concentration, n ≈ cGa , up to high values in the 1020 cm−3 range [551]. For Orich (Znpolar) conditions the growth mode changes to threedimensional growth and the activation ratio of Ga donors becomes low [552]. Above a gallium content of 2 %, the octahedral coordination of gallium and thus the partial segregation into a parasitic ZnGa2 O4 spinel phase is observed for [Ga] = 4 % [553]. The random distribution of dopants essentially makes a doped semiconductor a disordered system. The physics of electronic states in disordered systems has been reviewed in [558]. A metal–insulator transition is observed at a certain value of
Fig. 7.28 Electron concentration as a function of gallium concentration in MBE grown ZnO:Ga on sapphire for the two different polarities. Adapted from [551, 552]
234
7 Electronic Defect States 10
3
Si:P 102
(T=0) (S/cm)
Fig. 7.29 Zero temperature conductivity of Si:P for various (donor) doping concentrations. Experimental data (symbols) and guide to the eye (dashed line). Adapted from [559]
101 100 101 10
insulator
metal
2
0
2
4
6
8
ND (1018 cm3)
doping (NP = 3.8 × 1018 cm−3 ), as shown in Fig. 7.29 for Si:P [559]. For a certain value of disorder all states become localized (Anderson localization [560], cmp. Sect. 8.8).
7.6 QuasiFermi Levels The carrier concentrations were given by (7.6) and (7.7). So far, we have only considered semiconductors in thermodynamic equilibrium for which np = n 2i . In a nonequilibrium situation, e.g. for external excitation or carrier injection in a diode, the electron and hole densities can each take arbitrary values, in principle. In particular, np will no longer be equal to n 2i and there is no Fermi level constant throughout the structure. In this case, however, quasiFermi levels Fn and Fp for electrons and holes, respectively, are defined via Fn (r) − E C n(r) = NC F1/2 kT Fp (r) − E V . p(r) = NV F1/2 − kT
(7.56a) (7.56b)
A quasiFermi level is sometimes called imref4 and can also be denoted as E Fn or E Fp . We emphasize that the quasiFermi levels are only a means to describe the local carrier density in a logarithmical way. The quasiFermi levels can be obtained from the density via
4 W.
Shockley had asked E. Fermi for permission to use his name reversed. Fermi was not too enthusiastic but granted permission.
7.6 QuasiFermi Levels
235
n NC p . Fp = E V − kT ln NV
Fn = E C + kT ln
(7.57a) (7.57b)
The quasiFermi levels do not imply that the carrier distribution is actually a Fermi distribution. This is generally no longer the case in thermodynamical nonequilibrium. However, in ‘wellbehaved’ cases the carrier distribution in nonequilibrium can be approximated locally as a Fermi distribution using a local quasiFermi level and a local temperature, i.e. 1 . (7.58) f e (r, E) ∼ = E−Fn (r) exp kT (r) + 1 Using the quasiFermi levels, np is given by n(r) p(r) = n 2i exp
Fn (r) − Fp (r) . kT
(7.59)
We note that for an inhomogeneous semiconductor or a heterostructure (cf. Chap. 12), n i may also depend on the spatial position. In the case of thermodynamic equilibrium the difference of the quasiFermi levels is zero, i.e. Fn − Fp = 0 and Fn = Fp = E F .
7.7 Deep Levels For deep levels the shortrange part of the potential determines the energy level. The longrange Coulomb part will only lead to a correction. The term ‘deep level’ implies that the level is within the band gap and far from the band edges. However, some deep levels (in the sense of the potential being determined by the ion core) have energy levels close to the band edges or even within a band. Details can be found in [233, 561–564]. The wavefunction is strongly localized. Thus, it cannot be composed of Bloch functions, as has been done for the shallow levels for the effectivemass impurity. The localization in r space leads to a delocalization in k space. Examples are Si:S, Si:Cu or InP:Fe, GaP:N, ZnTe:O. Deep levels can also be due to intrinsic defects such as vacancies or antisite defects. Due to the larger distance to the band edges, deep levels are not efficient at providing free electrons or holes. Quite the opposite, they rather capture free carriers and thus lead to a reduction of conductivity. Centers that can capture electrons and holes lead to nonradiative recombination of electrons through the deep level into the valence band (see also Chap. 10). This can be useful for the fabrication of semiinsulating
236
7 Electronic Defect States
layers with low carrier concentration and fast time response of, e.g. switches and photodetectors. While the electronic properties of deep levels can be readily characterized, the microscopic origin is not immediately apparent. Next to theoretical modeling of defects and correlation with experimental results, paramagnetic hyperfine interactions have proven useful to identify the microscopic nature of various defects [565].
7.7.1 Charge States The deep level can have different charge states depending on the occupancy with electrons. The energy position within the gap varies with the charge state due to the Coulomb interaction. Also, the lattice relaxation around the defect depends on the charge state and modifies the energy level. The localized charge qd at the defect is the integral over the change Δρ of the charge density compared to the perfect crystal over a sufficiently large volume V∞ around the defect ne Δρ(r) d3 r = . (7.60) qd = r V∞ In semiconductors, the charge qd r is an integer multiple of the elementary charge. The defect is said to be in the nth charge state. Each charge state has a certain stable atomic configuration Rn . Each charge state has a ground state and excited states that can each have different stable atomic configurations. Now, we discuss how the concentration of the various charge states depends on the position of the Fermi level. The overall constraint of global charge neutrality determines the chemical potential of the electron, i.e. the Fermi level in Fermi–Dirac statistics. We use the approximation that the concentration of defects is so small that the mutual interaction of defects becomes negligible. As an example, we treat the possible reaction V 0 V + + e− , where V 0 denotes a neutral vacancy and V + is a positively charged vacancy, created by the ionization of an electron from the vacancy into the conduction band. The free energy G depends on the numbers n 0 of neutral and n + of positively charged vacancies. The minimum condition is met by ∂G ∂G dn 0 + dn + = 0. (7.61) dG = ∂n 0 ∂n + The neutrality constraint is dn 0 + dn + = 0 and therefore the minimum condition reads ∂G ∂G = . (7.62) ∂n 0 ∂n +
7.7 Deep Levels
237
For noninteracting defects and using (4.9) we write n0 ∂G f 0 = G (V ) + kT ln ∂n 0 N0 ∂G ∂G(V + ) ∂G(e− ) n+ f = + = G V + + kT ln + μe− , ∂n + ∂n + ∂n + N+
(7.63a) (7.63b)
where N0 = N Z 0 and N+ = N Z + are the number of available sites, given by the number N of atomic sites and including possible internal degeneracies Z 0 and Z + , respectively. Degeneracy factors of deep levels are not a simple subject [522] and, e.g. the degeneracy factors of Au donor and acceptor levels in Si are under discussion [566–568]. G f denotes the free enthalpy of formation of the respective defect, as in (4.3). We have written the free enthalpy of the separated pair V + and e− as the sum G(V + ) + G(e− ). μe− = ∂G(e− )/∂n + is (by definition) the chemical potential of the electron, i.e. the Fermi energy E F of Fermi–Dirac statistics.5 From (7.63a, b) we find for the ratio of the concentrations of defects c0 = n 0 /N and c+ = n + /N G fV + − G fV 0 + E F Z+ E t (V 0 ) − E F Z+ c0 = exp − exp = , c+ Z0 kT Z0 kT
(7.64)
where the trap level energy (for the particular charge transition), E t (V 0 ) = G fV 0 − G fV + , is the free enthalpy of ionization of V 0 . We note that c0 can be obtained from (4.9) and E F is determined by the chargeneutrality condition. As example experimental data on the charge transition Fe0 Fe+ + e− of interstitial iron (in tetrahedral position, Fig. 7.30a, cmp. Fig. 3.18) in silicon is shown. The concentration of Fe0 is tracked via the EPR signal from the neutral S = 1 state6 with gfactor g = 2.07 [569]. For ntype samples the iron is in neutral state and the maximum EPR signal is found. For strongly ptype samples, the Fermi energy is below the trap level and all iron is in Fe+ state, yielding no EPR signal at the given gfactor. From the investigation of various silicon samples with different doping levels and consequently different position of the Fermi level, the trap (deep donor) energy is found to be E V + 0.375 eV as indicated in Fig. 7.30b.
chemical potential in a onecomponent system is μ = ∂G/∂n = G/n. In a multicomponent system it is, for the ith component, μi = ∂G/∂n i = G/n i . 6 The electron configuration is 3d8 with two paramagnetic electrons. Under uniaxial stress along [100] the EPR line splits into a doublet. [569] Further details can be found in [570]. 5 The
238
7 Electronic Defect States
(b)
(a)
Fig. 7.30 (a) Silicon cubic unit cell with an interstitial iron atom (red) at tetrahedral site. (b) EPR intensity (at T = 95 K from interstitial iron in neutral state, Fe0 with S = 1) versus Fermi level position for irondoped silicon with varying Fermi level due to different amounts of shallow impurity levels from to Al, B and P as labeled. The shaded areas indicate the valence and conduction band. The dashed line at E t = E V + 0.375 eV indicates the trap level. The inset shows a typical EPR spectrum of Fe0 . Adapted from [571], inset adapted from [572]
7.7.2 Double Donors An impurity that has two extra electrons available after bonding in the matrix may give rise to a double donor. Typical examples are substitutional chalcogenide atoms (S, Se or Te) in silicon [573] and germanium [574], interstitial impurities such as Mgi in Si [575], or groupV atoms on a groupIII site in a III–V compound (antisite defect), such as PGa in GaP [576] or AsGa in GaAs [577]. The double donor is electronically similar to a helium atom. Due to the repulsive Coulomb interaction of the two electrons on the neutral double donor, the (single) ionization energy E 1 (also often labeled E(0, 1) or E(0, +)) of D0 is smaller than that of D+ (E 2 , also labeled E(1, 2) or E(+, ++)). For He and He+ the ratio of ionization energies is 0.45; for chalcogenides in Si and Ge similar ratios have mostly been found (Table 7.8). The carrier statistics and the degeneracy factors for a double donor have been discussed in [510, 578]. Typically, the degeneracy factor for the ionization of the double donor D0 → D+ is gˆD = g2 /g1 = 1/2 and for the ionization D+ → D++ is gˆD = g1 /g0 = 2/1 = 2. For the probabilities to find a neutral, single and double ionized donor we find following the treatment in [578]
7.7 Deep Levels
239
Table 7.8 Binding energies (to conduction band) of double donor chalcogenide impurities in Si and Ge Host State S Se Te Si Ge
D0 D+ D0 D+
318 612 280 590
307 589 268 512
199 411 93 330
All energies in meV, data from [573, 574]
d0 =
ND0 = ND exp
d+ =
ND+ = ND exp
d ++ =
ND++ = ND
E 1 +E 2 kT
exp 2kTEF + exp 2kTEF + 2 exp
E 1 +E F kT
E 1 +E 2 kT E 1 +E 2 2 EF +E F + exp + 2 exp E1kT kT kT +E F 2 exp E1kT +E 2 +E F exp E1kT + exp 2kTEF + 2 exp E1kT
exp
(7.65a) (7.65b) (7.65c)
The probabilities are depicted in Fig. 7.31a. The maximum of d + is at the energy (E 1 + E 2 )/2. Its value is d
(a)
+
E1 + E2 2
=
1 E1 −E2 1 + exp − 2kT
(7.66)
(b)
Fig. 7.31 (a) Population of states of a double donor (neutral: black, single ionized: red, double ionized: blue) according to (7.65a–c) as a function of the Fermi level. The ionization energies have been chosen as E 1 = −0.2 eV and E 2 = −0.4 eV and are indicated by dashed lines (kT = 25 meV); these energies are similar to Si:Te (cmp. Table 7.8). The conduction band edge is taken as zero energy. (b) depicts the according number of electrons n˜ ionized from the donor.
240
7 Electronic Defect States
(a)
1000 500
1018
300
(b)
200
2 1017
900
700 600
500
400 Si:Te
3
Si:Te
17
10
1017 8 1016 6 1016
1016
4 1016 1015
0
1
2
3
4
1000/T (1000/K)
5
6
1.0
1.5
2.0
2.5
3.0
1000/T (1000/K)
Fig. 7.32 Temperature dependent electron concentration (from Hall data) for Si:Te. (a) Experimental data and fit with double donor model using NTe = 5 × 1016 cm−3 , E 1 = 200 meV and E 2 = 440 meV (solid line). Single donor models would fail (NTe = 5 × 1016 cm−3 and NTe = 2 × 1017 cm−3 , dashed lines). (b) Second ionization step in more detail with fits using different values for E 2 ; the solid line is for E 2 = 440 meV, the other dashed lines for E 2 = 420 and 460 meV. Adapted from [579]
and reaches a value close to one for (E 1 − E 2 )/kT 1. In Fig. 7.31b the number of electrons per donor n˜ = (ND+ + 2 ND++ )/ND is shown as a function of the Fermi level; at (E 1 + E 2 )/2, exactly n˜ = 1. In Fig. 7.32 the temperature dependent electron concentration in Si:Te is depicted. Up to 570 K the single ionization is visible (other shallow impurities present in the sample in lower concentrations < 1014 cm−3 play no role). From the fit E 1 = 200 ± 2.7 meV is determined [579]. Single donor models would fail. The second ionization step is somewhat masked by the onset of intrinsic conduction. According to (7.15), the slope of n i is E g /2 ≈ 500 meV which is similar to E 2 ≈ 440 meV.
7.7.3 Double Acceptors In analogy to double donor defects, double acceptors can introduce up to two holes into the valence band. A typical example is Zn in silicon [580], exhibiting its ‘normal’ acceptor level (Zn0 /Zn− ) at E V + 0.31 eV. In moderately ndoped silicon another level (Zn− /Zn2− ) is observed at E C − 0.55 eV, when the ndoping is sufficient to partially compensate the Zn and supply one electron for each Zn atom but not two (2NZn > ND > NZn ). A similar situation has been observed for Zn in germanium, exhibiting the levels E V + 0.03 eV and E V + 0.09 eV [581]. In Fig. 7.33 three
7.7 Deep Levels
241
Fig. 7.33 Inverse (absolute) Hall coefficient (cmp. −1 , i.e. charge Sect. 13.2.1) RH concentration, for three Ge:Zn samples with different degree of compensation with Sb donors as labeled. The dashdotted lines indicate typical slopes. The dashed lines sketch the Zn0 → Zn− and the Zn− → Zn−− processes. Adapted from [581]
different Ge:Zn samples are compared. If the additional Sb donor concentration (ND ≈ 3.4 × 1016 cm−3 ) is larger than 2NZn (NZn ≈ 1.2 × 1016 cm−3 ), the sample is ntype (upper curve). The slope is similar to the Ge:Sb donor binding energy (Table 7.2). If compensation with donors is weak (NZn > ND , middle curve) first the shallow donor level with 0.03 eV activation energy is activated and subsequently the deeper one with 0.09 eV activation energy, creating pconduction with a saturated hole density of p ≈ 2NA − ND > NZn (negative Hall coefficient). The two individual activation processes are sketched as dashed lines in Fig. 7.33. If the Sb concentration is larger than NZn but smaller than 2NZn , the shallow acceptor level is filled with electrons, leaving still the only partially filled deeper acceptor level available for ionization (lower curve). In this case the sample is still ptype, but the saturation hole density is p ≈ 2NA − ND < NZn . The degeneracy factors for Zn in Si and Ge have been discussed in [522].
7.7.4 Jahn–Teller Effect The lattice relaxation can reduce the symmetry of the defect. Many defects, such as a vacancy, a tetrahedral interstitial or an impurity, occupy initially tetrahedral sites in the zincblende structure. The lattice relaxation reduces the symmetry, e.g. to tetragonal or trigonal, and therefore causes initially degenerate levels to split. Such splitting is called the static Jahn–Teller effect [561, 582]. The energy change in terms of the atomic displacement Q can be denoted (using perturbation theory for the simplest, nondegenerate case) as −I Q (I > 0). Including the elastic contribution
242
7 Electronic Defect States
with a force constant C, the energy of a configuration Q is E = −I Q +
1 C Q2. 2
(7.67)
The stable configuration Q min , for which the energy is minimal (E min ), is therefore given by I (7.68a) Q min = C I2 E min = − . (7.68b) 2C Several equivalent lattice relaxations may exist, e.g. a 3fold minimum for remaining C3v symmetry. The energy barrier between them has a finite height. Therefore, e.g. at sufficient temperature, the defect can switch between different configurations and eventually again becomes isotropic (dynamic Jahn–Teller effect). The experimental observation depends on the relation between the characteristic time of the experiment and the reorientation time constant of the defect.
7.7.5 NegativeU Center We explain the principle of a socalled negativeU center [583] for the Si vacancy [584] (cf. Fig. 4.2). It was first proposed by Anderson to explain the properties of amorphous chalcogenide glasses [585]. Many defects in semiconductors exhibit negativeU behavior, e.g. also the boron interstitial in Si [584, 586]. Coulomb energy and the Jahn–Teller effect compete for the position of the occupancy level for different charge states. U refers to the additional energy upon charging of the defect with an additional electron. The Coulomb repulsion of electrons leads to an increase of the energy, i.e. positive U , which has been calculated to be 0.25 eV for the Si vacancy [587] for all charge states. The occupation level (cf. Sect. 4.2.2) E 0 (1, 2) (the index 0 indicates effects only due to manyelectron Coulomb interaction), separating the domination of V ++ and V + (Fig. 7.34) is 0.32 eV above the valanceband edge. Therefore, the occupation level E 0 (0, 1) is expected to lie at about 0.57 eV about E V . The Jahn–Teller effect may lead to a splitting of the otherwise 4fold degenerate states of the vacancy. A detailed experimental study using hyperfine interactions can be found in [588]. The schematic level diagram for the Jahn–Teller splitting is shown in Fig. 7.35. The V ++ state (A1 is always populated with two electrons) is resonant with the valence band. The T2 state lies in the band gap. When the Jahn–Teller effect (now on the T2 state) is included, the energies of the different charge states depend on the configuration coordinate (a mostly tetragonal distortion in the case of the Si vacancy).
7.7 Deep Levels
243
V0 E0(0,1) E0(1,2)
V E(1,2) V 0 E(0,2) E(0,1) V
V
Fig. 7.34 Charge states of the vacancy in silicon. Left level scheme without lattice relaxation, right level scheme including the Jahn–Teller effect. For a Fermi level below (above) E(0, 2) the charge state V ++ (V 0 ) is dominant
T2
A1 V
V
V0
V
Fig. 7.35 Jahn–Teller splitting for different charge states of the vacancy. A1 and T2 refer to irreducible representations of the Td point symmetry group. A1 is nondegenerate and therefore does not exhibit a Jahn–Teller effect. T2 is triply degenerate. The arrows represent electrons and their spin orientation
1 E V 0 = E(0, Q) = E(0, Q = 0) − 2I Q + C Q 2 2 1 E V + = E(1, Q) = E(1, Q = 0) − I Q + C Q 2 2 1 2 E V ++ = E(2, Q) = E(2, Q = 0) + C Q . 2
(7.69a) (7.69b) (7.69c)
For the n = 2 state the T2 gap state is empty and thus no degeneracy and Jahn– Teller term arises. For n = 1 there is a linear Jahn–Teller term. The occupation with two electrons (V 0 ) causes an approximately twice as large Jahn–Teller splitting for the n = 0 state. The force constant is assumed to be independent of the charge state. The energies for the minimum configurations Q nmin are therefore E(0, Q 0min ) = E(0, Q = 0) − 4 E(1, Q 1min ) = E(1, Q = 0) − E(2, Q 2min ) = E(2, Q = 0).
I2 2C
I2 2C
(7.70a) (7.70b) (7.70c)
244
7 Electronic Defect States
The Jahn–Teller energy E JT = I 2 /2C lowers the position of the occupancy levels E 0 calculated with Coulomb terms only. The occupancy levels including the Jahn– Teller contribution are therefore given as E(1, 2) = E 0 (1, 2) − E JT E(0, 1) = E 0 (0, 1) − 3 E JT .
(7.71a) (7.71b)
For the vacancy in silicon the Jahn–Teller energy E JT is about 0.19 eV. Thus the E(1, 2) level is lowered from 0.32 to 0.13 eV. The E(0,1) occupancy level, however, is reduced from 0.57 to 0.05 eV [584, 589] (see Fig. 7.34). The occupancy level E(0, 2) is in the middle between E(0, 1) and E(1, 2) (E(0, 2) = (E(0, 1) + E(1, 2))/2) and indicated in Fig. 7.36a. At this energy, c(V 0 ) = c(V ++ ) and the value of c(V + ) is 1 −E 2 ) since E(0, 1) < E(1, 2) (cmp. (7.66)). small (≈ exp E2kT The relative concentrations of the three charge states are determined by (7.64) (degeneracy and entropy terms have been neglected) E(1, 2) − E F c(V ++ ) = exp c(V + ) kT + c(V ) E(0, 1) − E F = exp . c(V 0 ) kT
(7.72a) (7.72b)
They are depicted in Fig. 7.36a in a plot related to Fig. 7.31a. Therefore, V ++ dominates if E F < E(0, 1) and V 0 dominates for E F > E(1, 2). In the intermediate range E(0, 1) < E F < E(1, 2) we know from (7.72a, b) that V + is dominated by V 0 and V ++ . However, at this point it is not clear whether V ++ or V 0 dominates
(a)
(b)
Fig. 7.36 (a) Population of states of a negativeU defect (neutral: black, single ionized: red, double ionized: blue) according to (7.65a–c) as a function of the Fermi level. The ionization energies have been chosen as E 1 = −0.4 eV and E 2 = −0.2 eV (cmp. Fig. 7.31) and are indicated by dashed lines (kT = 25 meV). The occupancy level E(0, 2) is indicated with a dashdotted line. The conduction band edge is taken as zero energy. (b) depicts the according number of electrons ionized from the defect.
7.7 Deep Levels
245
overall. The ratio of the concentrations of V ++ and V 0 is given by c(V ++ ) = exp c(V 0 )
E(1, 2) + E(0, 1) − 2E F kT
= e exp 2
E(0, 2) − E F kT
. (7.73)
The occupancy level E(0, 2) is thus again given as E(0, 2) =
E(0, 1) + E(1, 2) , 2
(7.74)
and is shown in Fig. 7.34. V ++ dominates if E F < E(0, 2) and V 0 dominates for E F > E(0, 2). V + is, for no position of the Fermi level, the dominating charge state of the Si vacancy. We note that for ndoped Si the V − and V −− can also be populated. The population of the V 0 state with an extra electron introduces another Jahn–Teller splitting (Fig. 7.35) that has trigonal symmetry. Generally, the Jahn–Teller effect can make the addition of an electron cause an effectively negative charging energy; in this case the center is termed a negativeU center. We note that the single vacancy in germanium is not a negativeU center due to smaller Jahn–Teller distortion and smaller electronlattice coupling [590].
7.7.6 DX Center The DX center is a deep level that was first investigated for ndoped (e.g. Sidoped) Alx Ga1−x As. It dominates the transport properties of the alloy for x > 0.22. For smaller Al concentrations and GaAs the DX level lies in the conduction band. DXtype deep levels have also been found for other alloys and dopants, e.g. GaAsP:S. It is experimentally found that the capture process of electrons into the DX center is thermally activated. The capture energy E c depends on the AlAs mole fraction (Fig. 7.37). The (average) barrier for electron capture has a minimum of 0.21 eV for x ≈ 0.35, near the crossover point between direct and indirect band gap
Fig. 7.37 Energy barrier for electron capture E c at the SiDX center in Alx Ga1−x As for various compositions. Experimental data from [591]
0.5
Al xGa1x As:Si 0.4
0.3
0.2
0.1
0.3
0.4
0.5
0.6
0.7
246
7 Electronic Defect States
(cf. Fig. 6.19). For lower Al concentrations, the capture barrier increases to 0.4 eV for x = 0.27; for x > 0.35 the capture barrier increases to about 0.3 eV for x around 0.7 [591]. The barrier for thermally releasing carriers from the DX center has been determined to be about 0.43 eV, independent of the Al mole fraction [591]. Carriers can be removed from the DX center by optical absorption of photons with energy larger than about 1.2 eV. If carriers are removed by optical excitation at low temperatures the (re)capture is so slow (σ < 10−30 cm2 ) that the carriers remain in the conduction band and cause persistent photoconductivity (PPC). The PPC is only reduced upon increasing the sample temperature. The concentration of the DX center is about the same as the net doping concentration. The properties of the DX center are reviewed in [592, 593]. So far, no definite microscopic model of the DX center has been agreed on. Lang [594] proposed that the DX center involves a donor and an unknown defect (probably a vacancy). It probably involves large lattice relaxation as in the configuration coordinates model of Fig. 7.38 where the donor binding energy E Db with respect to the conductionband minimum, the barrier for electron capture E c , the barrier for electron emission E e and the optical ionization energy E o are labeled. The donor binding energy is measured with Hall effect (cf. Sect. 13.2.1) at temperatures sufficient to overcome the capture and emission barriers, the emission barrier is measured with deep level transient spectroscopy (DLTS). The capture barrier manifests itself in PPC experiments. We note that the DX center is related to the Lconduction band. For small Al mole fraction, the DX level is degenerate with the Γ related conduction band (see Fig. 7.38b). Theoretical models and experimental evidence hint at a vacancyinterstitial model for the SiDX center [595]. The donor (Si) is displaced along the 111 direction from the Ga substitution site. The displacement is predicted to be 0.117 nm and the
(b)
(a) E
E
Eopt EC EDX
Ec EbD
EL EDX EC
Ee
q0
qt
q
L
DX
Ec
Ee
q0
qt
q
Fig. 7.38 (a) Schematic configuration coordinate diagram for the DX level with large lattice relaxation. q0 is the configuration of the empty defect, qt is the configuration of the filled defect. The donor binding energy E Db , the barrier for electron capture E c , the barrier for electron emission E e and the optical ionization energy E o are labeled. E C denotes the conductionband edge. We note that in AlGaAs the DX level is associated with the L conduction band (see Fig. 6.19). (b) Schematic configuration coordinate diagram for the DX level in Al0.14 Ga0.86 As with the DX level being degenerate with the (Γ related) conduction band
7.7 Deep Levels 4
GaAs
1
Fig. 7.39 Absorption spectrum of GaAs at low temperatures (T = 10 K) when cooled in the dark (solid line). The dashed (dashdotted) line is the absorption after illuminating the sample for 1 min (10 min) with white light, leading to quenching of the EL2related absorption. Adapted from [597]
247
3
2
1
0 0.8
1.0
1.2
1.4
distorted geometry can be viewed as a Ga vacancy and a Si interstitial. The charge state of the (filled) DX center is proposed to be a twoelectron negativeU state.
7.7.7 EL2 Defect The EL2 defect is a deep donor in GaAs. It is not related to impurities but occurs for intrinsic material, in particular grown under Asrich conditions. It has physical properties similar to the DX center. The bleaching of absorption due to EL2, i.e. the optical removal of electrons from the defect at low temperatures, is shown in Fig. 7.39. The microscopic model [596] describes the EL2 defect as an arsenic antisite defect, i.e. an arsenic atom on a Ga site, AsGa . In the charged state the arsenic atom is displaced from the lattice position and a complex of a Ga vacancy (symmetry T3d ) and an interstitial As (symmetry C3v ) with 0.14 nm displacement along 111 forms (VGa Asi ). The charged state is filled with two electrons.
7.7.8 Semiinsulating Semiconductors Semiconductors with high resistivity (107 –109 cm) are called semiinsulating (‘s.i.’ or ‘si’). Semiinsulating substrates are needed for highspeed devices. The high resistivity should stem from a small freecarrier density at finite temperature and not from a small mobility due to poor crystal quality. For sufficiently wide band gap, the intrinsic carrier concentration is small and such pure material is semiinsulating, e.g. GaAs with n i = 1.47 × 106 cm−3 and 5.05 × 108 cm [598]. Since shallow impurities are hard to avoid, another route is used technologically. Impurities that form deep levels are incorporated in the semiconductor in order to compensate free carriers. For
248
7 Electronic Defect States
(b) EC 5
InP:Fe
T2
1.14
5
0.78
E
InP:Sn
3
(a) 1.34
InP:Sn,Fe
InP:Sn
1017 n
0.25 0
Fe3+
Fe2+
EV
1016 0
0.2
0.4
0.6
0.8
1.0
Fig. 7.40 (a) Schematic band diagram of InP with levels of Fe impurities in the 3+ and 2+ charge states at low temperature. All energies are given in eV. The arrow denotes capture of an electron (from the conduction band or a shallow donor) on the deep acceptor. Compare this figure also with Figs. 9.33 and 10.25. (b) Depth profile of electron concentration in an InP:Sn/InP:Sn,Fe/InP:Sn structure. The change Δn ≈ 4.5 × 1016 cm−3 of electron concentration is due to the compensation by Fe and corresponds to the chemical iron concentration determined by SIMS, [Fe] = 4.9 × 1019 cm−3 . Part (b) adapted from [610]
example, a deep acceptor compensates all electrons if NA > ND . Since the acceptor is deep (E Ab kT ), it does not release holes for reasonable temperatures. Examples of suitable impurities for compensation of electrons are Si:Au [599], GaAs:Cr [600] and InP:Fe [601]. A deep donor, e.g. InP:Cr [602], is necessary to compensate ptype conductivity. Figure 7.40a shows the terms of Fe in InP [603, 604]. An overview of transition metals in III–V semiconductors can be found in [605]. The electron configuration of neutral Fe atoms is 3d6 4s2 (cf. Table 16.2). The Fe is incorporated on the In site and thus has a Fe3+ state as a neutral acceptor (A0 ). The Fe3+ state has the electron configuration 3d5 . The arrow in Fig. 7.40a represents the capture of an electron from the conduction band or from a shallow donor. The charge state of the Fe becomes Fe2+ (charged acceptor, A− ) with the electron configuration 3d6 . The cubic crystal field (Td symmetry) splits this 5 D Fe state7 into two terms [606] that exhibit further fine structure [604]. The large thermal activation energy of 0.64 eV found in the Hall effect on semiinsulating InP:Fe [601] corresponds to the energy separation of the 5 E level and the conduction band. The maximum electron concentration that can be compensated in this way is limited by the solubility of Fe in InP [607], about 1 × 1017 cm3 . Higher Fe incorporation leads to the formation of Fe (or FeP) precipitates and degrades the crystal quality. Only a fraction of the incorporated Fe may then be electrically active and contribute to the compensation. The maximum electrically active Fe concentration is found
7 The
notation is momentum.
2S+1 J
(multiplicity), with S being the total spin and J being the total angular
7.7 Deep Levels
249
to be 5–6×1016 cm−3 [608]. The compensation can be directly visualized via the depth profile of the electron concentration in a nsin structure (Fig. 7.40b). The poor thermal stability of Fe, i.e. high diffusion coefficient, has evoked proposals for more stable dopants such as InP:Ru [609].
7.7.9 Isoelectronic Impurities Isoelectronic impurities, generally represent a deep level with a short range potential. The isoelectronic trap introduces a bound state for an electron or a hole. Once a carrier has been captured, the defect becomes charged. The other carrier type is then easily trapped, forming a bound exciton (Sect. 10.3.2). The theory of isoelectronic impurities is outlined in [611]. A detailed theoretical treatment of N in GaAs and GaP is given in [472]. In GaP:N, an electron is spatially localized on the N impurity. Most of the wave function is at the Xpoint. The nitrogenbound electron level in GaP (A1 symmetry) is close to the conduction band edge and within the band gap. Important for the energy position is the lattice relaxation, leading to an inward relaxation of the surrounding Ga atoms (Fig. 7.42). Due to the spatial localization of the wave function it is delocalized in kspace (Fig. 7.41a) and obtains a sizeable component at the Γ point, facilitating zerophonon absorption from the valence band. This effect is present only when the lattice relaxation around the impurity is considered; without relaxation the Γ component is zero, with relaxation about 1 % [472]. The Γ component of the wavefunction is larger for localization at an isoelectronic impurity than at a shallow donor such as sulfur [612]. This way a large oscillator strength for optical transitions occurs
(a)
(b)
Fig. 7.41 (a) Model calculation of the wavevector dependence of the probability density of an electron bound to a 10 meV deep isoelectronic trap (N) and to a 100 meV deep shallow donor (S) in GaP. Adapted from [612]. (b) Wavefunction (isosurface at 20 % of maximum) of isolated nitrogen (N) and neighboring N–N pair (NN1 ) in GaP. Adapted from [472]
250
7 Electronic Defect States
(a) (b) (c)
(d)
(a) (b) (c)
(d)
Fig. 7.42 Energy levels of nitrogen impurity states in GaP (left) and GaAs (right). The energy scale is relative to the bulk GaP valence band maximum, the conduction band minima (CBM) are thus shown relative to the vacuum level. The conduction band is shown in grey. For both materials, (a) denotes the isolated N impurity level calculated without lattice relaxation (dashed line), and (b) with lattice relaxation. (c) denotes the position of N–N pair levels, m denoting the neighbor. (d) shows selected experimental data. NN1 denotes the direct neighbor NNpair. The other NNn follow the usual nomenclature as in [616]. Data taken from [472] (color figure online)
Fig. 7.43 Pressure dependence of the energy of excitons bound to isolated nitrogen impurities in GaAs (circles), measured from the top of the GaAs valence band. The dashed lines are the pressure dependent GaAs bulk band gaps (cmp. Fig. 6.42). The solid (dashdotted) line is a theoretical model for the nitrogenbound exciton (electron) level. Adapted from [615]
(Sects. 9.6.9 and 10.3.2). The wavefunction of an isolated single N impurity and a neighboring N–N pair (NN1 ) in GaP are shown in Fig. 7.41b. Isolated nitrogen impurities in (unstrained) GaAs introduce states only within the conduction band (Fig. 7.42). The reason is that the GaAs conduction band edge is further from the vacuum level than that of GaP (see Fig. 12.21). Only the NN1 and NN4 pair levels are theoretically expected to be within the GaAs band gap. The index denotes the nth neighbor position. The NN1 level has been experimentally observed [613, 614]. The isolated nitrogen impurity level is forced into the GaAs band gap upon hydrostatic pressure [614, 615] (Fig. 7.43). Further levels deeper within the band gap are due to clusters containing more than two nitrogen atoms.
7.7 Deep Levels (b)
251 4.26 (d)
4.24
4.22
(a) 2 (c) 1 0 0
z=1.56nm 100
200
300
400
Fig. 7.44 Image of (a) topography (Δz = 2.8 nm) and (b) work function (Δφ = 4.21–4.26 eV) of a surface step along [111] on a nGaP(110) surface cleaved in UHV. Adapted from [618]. (c) and (d) show the corresponding linescans. Adapted from [618]
7.7.10 Surface States The investigation of (semiconductor) surfaces is a large field with sophisticated methods that allow realspace imaging with atomic resolution by scanning probe microscopy and highly depth resolved electronic studies. The surface represents first of all a break in the periodic crystal potential and thus a defect of the bulk crystal. The unsatisfied bonds partly rearrange, e.g. by building dimers, forming a surface reconstruction or remain as dangling bonds. The surface exhibits a surface density of states. Such states can lie in the band gap and capture electrons, leading to recombination and a depletion layer. For a brief introduction on semiconductor surface physics see Chap. 11; for more details we refer to [617]. As an example of the formation of electronic states at surface defects we show in Fig. 7.44 the comparison of topography and work function (measured by Kelvin probe force microscopy [618]) at a surface step on a GaP(110) surface that has been prepared by cleaving insitu in ultrahigh vacuum (UHV). The depletiontype band bending of the surface is about 0.4 eV. The further increase of the position of the vacuum level at the step edge shows the presence of trap states in the band gap causing the conduction band to bend upwards (cf. Sect. 21.2.1). Modeling of the effect shows that the charge density at the surface is 6 × 1011 cm−2 and at the step edge 1.2 × 106 cm−1 .
7.8 Hydrogen in Semiconductors The role of hydrogen in semiconductors was first recognized in studies of ZnO [619]. It is now clear that hydrogen plays an important role in the passivation of defects. As a ‘small’ atom, it can attach easily to dangling bonds and form an electronpair
252
7 Electronic Defect States
bond. Thus, surfaces, grain boundaries, dislocations and shallow (donor and acceptor) and deep impurity levels become passivated. A good overview and many details of the physics and technological use of hydrogen in semiconductors can be found in [620, 621]. The hydrogen must be typically introduced as atomic species into semiconductors, e.g. from a plasma in the vicinity of the surface or by ion irradiation. With regard to silicon it is important to note that the Si–H bond is stronger than the Si–Si bond. Thus a silicon surface under atomic hydrogen exhibits Si–H termination rather than Si–Si dimers [622]. Due to the stronger bond, the hydrogenation leads to an increase of the silicon band gap, which can be used for surface passivation [623], leading to reduced reverse diode current. The hydrogen concentration in amorphous Si (aSi) can be as high as 50 % [624]. Electronic grade aSi contains typically 10–30 atomic % hydrogen and is thus rather a silicon–hydrogen alloy. Hydrogen in crystalline silicon occupies the bondcenter interstitial position (see Fig. 3.18b) as shown in Fig. 7.45a. The complexes formed by hydrogen with shallow acceptors and donors have been studied in detail. It is now generally accepted that for acceptors (e.g. boron) in silicon the hydrogen is located close to the bondcenter position of the Si–B pair (BM, bond minimum) as sketched in Fig. 7.46a. The boron atom forms an electronpair bond with three silicon atoms of the tetrahedra, the fourth silicon bonds to the hydrogen atom. The complex therefore no longer acts as an acceptor. The silicon atoms and the acceptor relax their positions. The adiabatic potential energy surface of hydrogen in Si:B is shown in Fig. 7.45b. The hydrogen can sit on four equivalent sites (BM) along the 111 directions of the initial B–Si4 tetrahedron. This reduces the symmetry, e.g. of H–B vibrations [626].
(a)
Si
(b)
Si/B
0.5
Td
Td 0.0 0.5 1.0
AB
1.5 2.0 0.5
+
H0
BM 0.25
0.0
0.25
Fig. 7.45 (a) Energy for positions u of the hydrogen atom along the 111 direction for H+ in pure Si √ (Si atom at u = −0.25) and neutral hydrogen (B atom at u = −0.25). u is measured in units of 3a0 . For all positions of the hydrogen atom the positions of the other atoms have been relaxed in the calculation. Data from [625]. (b) Adiabatic potential energy in the (110) plane for hydrogen in Si:B. ‘BM’ denotes the bond minimum site (high valence electron density), C and C’ are equivalent c for pure Si. Reprinted with permission from [625], 1989 APS
7.8 Hydrogen in Semiconductors
253
(b)
(a)
Fig. 7.46 Schematic model for hydrogen in silicon forming a complex with (a) a shallow acceptor (boron, empty orbital) and (b) a shallow donor (phosphorus, doublefilled orbital)
(b)
(a)
[001]
[110]
[110]
Fig. 7.47 (a) Structure of the V–O complex (A center) in silicon. The black sphere represents the c oxygen atom. Reprinted with permission from [628], 2004 APS. (b) Calculated groundstate structure for the V–O–H2 center in silicon. Oxygen is over the C2 axis, and the two white spheres c represent hydrogen. Reprinted with permission from [629], 2000 APS
The energetic barrier for the hydrogen orientation has been determined to be 0.2 eV theoretically [625] for a hydrogen motion along the path BM–C–BM in Fig. 7.45b. Stress (along [100] and [112]) reduces the symmetry and leads to splitting of the local vibrational modes, now showing axial symmetry [627]. However, this preferential orientation disappears with an activation energy of 0.19 eV, close to the theoretical value. Hydrogen has experimentally been found to also passivate shallow donors. The microscopic configuration is sketched in Fig. 7.46b. The hydrogen atom sits on the Si– AB (antibonding) position and forms an electronpair bond with the silicon atom. The donor, e.g. phosphorus, is left with a doublefilled porbital (lone pair) whose level is in the valence band and thus no longer contributes to conductivity. Molecular hydrogen can passivate the socalled A center in Si, an oxygen–vacancy complex [629]. The atomistic configuration of the V–O–H2 complex is shown in Fig. 7.47. The deep double donor S in Si with a level at 0.3 eV below the conductionband edge can also be passivated by two hydrogen atoms [630].
Chapter 8
Transport
Abstract The physics of transport in semiconductors is treated foremost for charge transport. Band transport and scattering, mobility, low field and high field effects as well as polarons and hopping transport are covered. A short section mentions ionic transport before heat conduction and coupled heat and charge transport including thermopower and Peltier effect are discussed.
8.1 Introduction Charge and heat energy can be transported through the semiconductor in the presence of appropriate (generalized) forces. Such a force can be an electric field or a temperature gradient. Both transport phenomena are coupled since electrons transport energy and charge simultaneously through the crystal. First, we will treat the charge transport as a consequence of a gradient in the Fermi level, then the heat transport upon a temperature gradient and finally the coupled system, i.e. the Peltier and Seebeck effects. Detailed treatments of carrier transport can be found in [631, 632]. Practically all important semiconductor devices are based on the transport of charge, such as diode, transistor, photodetector, solar cell and laser. Carriers move in the semiconductor driven by a gradient in the Fermi energy. We distinguish • drift, as a consequence of an electric field E, • diffusion, as a consequence of a concentration gradient ∇n or ∇ p. In inhomogeneous semiconductors for which the position of the band edges is a function of position, another force occurs. This will not be treated here, since later (cf. Chap. 12) it will be included as an additional, internal electric field. In Sects. 8.2–8.5 we treat band conductivity, i.e. the transport of charge carriers in extended states, the conduction and valence bands characterized by an effective mass. Conductivity is then determined by the carrier concentration (free electrons and holes) and scattering mechanisms (mobility). In disordered semiconductors such as amorphous material, the charge transport due to hopping between localized states close to the Fermi level dominates the conductivity which is discussed in Sect. 8.7. © Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_8
255
256
8 Transport
Many semiconductor properties, such as the carrier concentration and the band gap, depend on the temperature. Thus, device properties will also depend on temperature. During operation of a device typically heat is generated, e.g. by Joule heating due to finite resistivity. This heat leads to an increase of the device temperature that subsequently alters the device performance, mostly for the worse. Ultimately, the device can be destroyed. Thus cooling of the device, in particular of the active area of the device, is essential. Mostly the thermal management of device heating limits the achievable performance (and lifetime) of the device. In highpower devices quite high energy densities can occur, e.g. the facet of a highpower semiconductor laser has to withstand an energy density beyond 10 MW cm−2 .
8.2 Conductivity Under the influence of an electric field the electrons accelerate according to (cf. (6.32)) dv dk = = q E = −e E. (8.1) F = m∗ dt dt In the following, q denotes a general charge, while e is the (positive) elementary charge. We also consider an isotropic effective mass m ∗ at first. After the time δt the k vector of all conduction electrons (and the center of the Fermi sphere) has been shifted by δk eE δt. (8.2) δk = − In the absence of scattering processes this goes on further (similar to an electron in vacuum). This regime is called ballistic transport. In a (periodic) band structure, the electron will perform a closed cycle as indicated in Fig. 8.1. Such motion is called a Bloch oscillation. However, in a bulk crystal the period T of such an oscillation eE T / = 2π/a0 is of the order of 10−10 s for E = 104 V/cm. This time is much longer than a typical scattering time of 10−14 s. Thus, in bulk material the Bloch electron cannot reach the zone boundary. However, in artificial superlattices (cf. Chap. 12) with larger periodicity (≈10 nm), high electric fields (≈106 V/cm) and high quality (reduced collision time) such motion is possible. We note that in the absence of scattering, electrons also perform a periodic oscillation in a magnetic field (cyclotron motion). In a real semiconductor, at finite temperatures, impurities, phonons and defects (finally also the surface) will contribute to scattering. In the relaxationtime approximation it is assumed that the probability for a scattering event, similar to friction, is proportional to the (average) carrier velocity. The average relaxation time τ is introduced via an additional term v˙ = −v/τ that sums up all scattering events.1 1 Going
beyond the relaxation time approximation is discussed in Sect. I.
8.2 Conductivity
257
Fig. 8.1 Schematic representation of a Bloch oscillation
/a
/a
Thus, the maximum velocity that can be reached in a static electric field is given by (steadystate velocity) eEτ (8.3) v=− ∗ . m The current density per unit area is then linear in the field, i.e. fulfills Ohm’s law j = nqv =
n e2 E τ = σ E. m∗
(8.4)
The conductivity σ in the relaxationtime approximation is given by σ=
n e2 τ 1 . = ρ m∗
(8.5)
In the case of a cylindrically symmetric mass such as for electrons in silicon or germanium, for the effective mass in (8.5) the effective conductivity mass must be used, 1 1 2 1 = + . (8.6) m ∗σ 3 mt ml The specific resistivity is the inverse of the conductivity. Metals have a high conductivity (see Table 8.1), e.g. for Cu at room temperature σ = 5.8 × 105 −1 cm−1 . At low temperatures (4 K) the conductivity is even a factor of 105 higher. The mean free path d = τ vF is σ m ∗ vF d= , (8.7) n e2 vF being the Fermi velocity (E F = m ∗ vF2 /2). For copper, d = 3 mm at low temperature (and thus susceptible to the sample geometry) while at room temperature the mean free path is only about 40 nm. However, this becomes an issue when the metal line width and height of interconnects in integrated circuits approaches this length scale [633] (see Sect. 24.5.5). In semiconductors, the carrier concentration depends strongly on the temperature. At zero temperature the conductivity is zero. Also, the scattering processes and thus the relaxation time constant exhibit a temperature dependence. The conductivity spans a large range from insulating to almost metallic conduction (see Table 8.1).
258 Table 8.1 Conductivity at room temperature for various metals, semiconductors, insulators and liquids
8 Transport Material
σ (−1 cm−1 )
Ag Al Au Cu Fe Pt Ge pure (ND ∼ 1013 cm−3 ) Ge (ND ∼ 1015 cm−3 ) Ge (ND ∼ 1017 cm−3 ) Ge (ND ∼ 1018 cm−3 ) Si pure Si:As (ND ∼ 3 × 1019 cm−3 ) Si:B (NA ∼ 1.5 × 1019 cm−3 ) GaAs pure ZnO:Al (highly doped) Pentacene SiO2 Al2 O3 H2 O pure Hexane
6.25 × 105 3.6 × 105 4.35 × 105 5.62 × 105 1.1 × 105 1.02 × 105 10−2 1 2 × 101 2 × 102 4.5 × 10−6 4 × 102 1.2 × 102 1.4 × 10−7 ≈1 × 104 10−8 –10−4 ≈10−15 ≈10−16 4 × 10−8 ≈10−18
8.3 LowField Transport First we consider only small electric fields. The real meaning of this will only become clear in Sect. 8.4 on highfield transport. In the lowfield regime the velocity is proportional to the electric field.
8.3.1 Mobility The mobility is defined (scalar terms) as μ=
v . E
(8.8)
By definition, it is a negative number for electrons and positive for holes. However, the numerical value is usually given as a positive number for both carrier types. In an intrinsic semiconductor the mobility is determined by scattering with phonons.
8.3 LowField Transport Table 8.2 Mobilities of electrons and holes at room temperature for various semiconductors
259 Material
−μn (cm2 /Vs)
μp (cm2 /Vs)
Si Ge GaAs GaN InSb InAs InP ZnO
1300 4500 8800 300 77 000 33 000 4600 230
500 3500 400 180 750 460 150 8
Further scattering is introduced by impurities, defects or alloy disorder. The conductivity is (8.4) σ =qnμ (8.9) for each carrier type. Using (8.5) the mobility in the relaxation time approximation is qτ (8.10) μ= ∗. m In the presence of both electrons and holes, σ = σe + σh = −e n μn + e p μp ,
(8.11)
where μn and μp are the mobilities for electrons and holes, respectively. These are given by μn = −e τn /m ∗e and μp = e τp /m ∗p . As the unit for mobility, usually cm2 /Vs is used. While Cu at room temperature has a mobility of 35 cm2 /Vs, semiconductors can have much higher values. In twodimensional electron gases (cf. Chap. 12), the mobility can reach several 107 cm2 /Vs at low temperature (Fig. 12.36). In bulk semiconductors with small band gap, a high electron mobility is caused by its small effective mass. Some typical values are given in Table 8.2.
8.3.2 Microscopic Scattering Processes The relaxation time constant summarizes all scattering mechanisms. If the relaxation times τi of various processes are independent, the Matthiesen rule can be used to obtain the mobility (μi = q τi /m ∗ ) 1 1 . = μ μi i
(8.12)
260
8 Transport
The various scattering mechanisms have quite different temperature dependences such that the mobility is a rather complicated function of temperature. In [634] the mechanisms determining the low and highfield transport properties of (cubic) semiconductors are reviewed.
8.3.3 Ionized Impurity Scattering Theoretically, this problem is treated similar to Rutherford scattering. A screened Coulomb potential is assumed, as the scattering potential V (r ) = −
r Ze 1 exp − , 4π0 r r lD
(8.13)
where lD is the screening length. The problem has been treated classically by Conwell and Weisskopf [635] and quantum mechanically by Brooks [636] and Herring. An expression for the mobility that encompasses the Conwell–Weisskopf and Brooks– Herring results is derived in [637]. Further details are given in [638, 639]. For the mobility it is found that μion.imp. =
1 27/2 (4π0 r )2 (kT )3/2 , √ π 3/2 Z 2 e3 m ∗ Nion ln(1 + b) − 1/(1 + 1/b)
(8.14)
with b = 4 (k/lD )2 = 8 m ∗ E (lD /)2 . In the Thomas Fermi screening model lD2
e2 = 4π N (E F ) = 0 r
1/3 4 m ∗ e2 1/3 3 n . π 0 r 2
(8.15)
The formula (8.14) is valid only for b 1, i.e. small carrier densities. A similar formula from [638] is μion.imp.
√ −1 128 2π (0 r )2 (kT )3/2 24 m ∗ 0 r (kT )2 = . ln m ∗1/2 Z 2 Nion e3 n e 2 2
(8.16)
For large ionized impurity (and carrier) density (b 1), the mobility is given by [483] 4e (8.17) μion.imp. = 1/3 2/3 n −2/3 , 3 π h the value of the prefactor being about 3 × 1014 (Vs)−1 . The scattering time depends like τ ∝ (E/kT )s on the kinetic energy; for moderate or weak scattering s = 3/2, for very strong scattering, s = −1/2 [632]. For typical substitutional impurities, the charge of the scattering center is Z  = 1; in oxides, oxygen vacancies may have Z = 2. At high impurity densities, impurity
8.3 LowField Transport
261
(a)
(a) Impurity custering Z
Si
2
Electron mobilty (cm /Vs)
300
200
100
6 5 4
nSi
3 2
1 0 18 10
19
10
20
10
21
10
22
10
Donor concentration (cm3)
10 20
10 21
Donor concentration (cm3)
Fig. 8.2 (a) Electron mobility in highly doped silicon. Experimental data (symbols) from various sources and modeling with ionized impurity scattering with (solid line) and without (dashed line) considering impurity clustering. (b) Effective impurity cluster charge Z D . Adapted from [640]
clusters may form with Z  > 1; this will have a strong influence on the scattering rate since it proportional to Z 2 . The decrease of mobility for ND > 1020 cm−3 (Fig. 8.2a) is attributed to such effect which can be described with an effective impurity clustering charge Z D (Fig. 8.2b) [640, 641].
8.3.4 Deformation Potential Scattering Acoustic phonons with small wavevector, i.e. a wavelength large compared to the unit cell, can have TA or LA character. The TA phonons represent a shear wave (with zero divergence), the LA phonons are a compression wave (with zero rotation). The LA is a plane wave of displacement δR parallel to the kvector q, δR = A sin (q · R − ωt) .
(8.18)
The strain tensor is given by i j =
1 qi A j + q j Ai cos (q R − ωt) . 2
(8.19)
It has a diagonal form i j = qi A j for q and ω → 0. Therefore, the LA phonon creates an oscillatory volume dilatation (and compression) with amplitude q · A. This volume modulation affects the position of the band edges. For the conductionband edge the energy change is related to the volume change by the hydrostatic deformation potential E ac.def. = V ∂ E C /∂V . Since the modulation is small compared to the energy of the charge carriers, it is mostly an elastic scattering process. The Hamilton operator for the LA scattering is
262
8 Transport
Hˆ = E ac.def. (q · A).
(8.20)
The size of the LA amplitude is given by the number of phonons in the mode that −1 . The mobility is given by the Bose–Einstein distribution, Nph (ω) = exp ω kT due to acoustic deformation potential scattering is found to be μac.def. =
√ 2 2π e 4 cl (kT )−3/2 , 2 3 m ∗ 5/2 E ac.def.
(8.21)
where cl = ρcsLA , ρ being the density and cs being the sound velocity. The scattering time increases like τ ∝ E −1/2 with the kinetic energy [632]. The acoustical deformation potential scattering is important at high temperatures. It is dominating in nonpolar semiconductors (Ge, Si) at high temperatures (typically at and above room temperature).
8.3.5 Piezoelectric Potential Scattering In piezoelectric crystals (see Sect. 15.4), i.e. crystals that show an electric polarization upon strain, certain acoustic phonons lead to piezoelectric fields. In GaAs, with 111 being the piezoelectric directions, this is the case for shear waves. In strongly ionic crystals, e.g. II–VI semiconductors, the piezoelectric scattering can be stronger than the deformation potential scattering. The mobility due to piezoelectric potential scattering is √ 16 2π 0 r (kT )−1/2 , (8.22) μpz.el. = 3 m ∗ 3/2 e K 2 with K =
ep2 /cl , ep 0 r +ep2 /cl
being the piezoelectric coefficient.
8.3.6 Polar Optical Scattering LO phonons are connected with an electric field antiparallel to the displacement (5.52). In the scattering mechanism the absorbed or emitted phonon energy ω0 is comparable to the thermal energy of the carriers. Therefore, the scattering is inelastic and the relaxationtime approximation does not work. The general transport theory is complicated. If the temperature is low compared to the Debye temperature, T ΘD μpol.opt.
e ΘD = exp , 2 m ∗ α ω0 T
(8.23)
8.3 LowField Transport
where α =
1 137
m ∗ c2 2 k ΘD
263
1 (∞)
−
1 (0)
is the dimensionless polar constant.
8.3.7 Dislocation Scattering Dislocations can contain charge centers and thus act as scattering centers [642]. This has been first demonstrated for nGe crystals that have been deformed [643, 644]. The deformation has introduced acceptortype defects reducing the mobility in particular at low temperatures (similar to ionized impurity scattering). The mobility due to dislocation scattering in an ntype semiconductor is given by [645, 646] μdisl.
√
√ 2π 2 d 2 (kT )3/2 n = ∝ T, √ 3 2 ∗ Ndisl Ndisl e f L D m 30
(8.24)
d being the average distance of acceptor centers along the dislocation line, f their and L D = (kT /(e2 n))1/2 the occupation rate, Ndisl the area density of dislocations √ Debye screening length. The relation μ ∝ n/Ndisl has been confirmed for various ntype GaN samples [647].
8.3.8 Grain Boundary Scattering The lowering of mobility due to transport across grain boundaries is an important effect in polycrystalline materials, such as polysilicon for solar cells or thin film transistors [648–651]. Grain boundaries contain electronic traps whose filling depends on the doping of the bulk of the grains. Charges will be trapped in the grain boundaries and a depletion layer will be created.2 At low doping the grains are fully depleted and all free carriers are trapped in the grain boundaries. This means low conductivity, however, no electronic barrier to transport exists. At intermediate doping, traps are partially filled and the partial depletion of the grain leads to the creation of an electronic barrier ΔE b (Fig. 8.3a) hindering transport since it must be overcome via thermionic emission. At high doping the traps are completely filled and the barrier vanishes again. Accordingly the mobility goes through a minimum as a function of the doping concentration (Fig. 8.3b) [648]. In [652] these data have been modeled with a 20 nm grain size, the value found in [648] from TEM analysis.
2 The
following arguments may only be followed once the concept of depletion layers and band bending is understood, see Sect. 21.2.1.
264
8 Transport
(b)
(a)
Fig. 8.3 (a) Electronic barrier (ΔE b ) for (hole) transport at a grain boundary (GB). (b) Average hole mobility in polysilicon, experimental data (symbols) and theoretical model (solid line). The dependence for monocrystalline silicon is shown for comparison as dashed line. Adapted from [648]
The expression for the limitation of the mobility due to scattering at grain boundaries is given by [651, 653] e LG
T μGB = √ 8m ∗ πk
−1/2
ΔE b exp − kT
,
(8.25)
where L G is the grain size.
8.3.9 Temperature Dependence The sum of all scattering processes leads to a fairly complicated temperature dependence of the mobility μ(T ). In covalent semiconductors (Si, Ge) the most important processes are the ionized impurity scattering (μ ∝ T 3/2 ) at low temperatures and the deformation potential scattering (μ ∝ T −3/2 ) at high temperatures (Fig. 8.4a). In polar crystals (e.g. GaAs) at high temperatures the polar optical scattering is dominant (Fig. 8.4b). In Fig. 8.5 the electron mobility of bulk and thinfilm ZnO is compared. Since ZnO is polar the mobility at room temperature is limited by polar optical phonon scattering. In the thin film, grainboundary scattering (Sect. 8.3.8) additionally occurs and limits the mobility. Since the carrier concentration increases with increasing temperature and the mobility decreases, the conductivity has a maximum, typically around 70 K
8.3 LowField Transport
(a)
265
(b)
Fig. 8.4 (a) Temperature dependence of the electron mobility in ndoped Ge (for various doping levels from ND ≈ 1018 for sample A to 1013 cm−3 for sample F in steps of a factor of ten). Dashed line indicates T −3/2 dependence of deformation potential scattering, solid lines are guides to the eye. Adapted from [515]. (b) μn (T ) for ntype GaAs (ND ≈ 5 × 1013 cm−3 , NA ≈ 2 × 1013 cm−3 ). Solid lines are theoretical mobilities for various scattering mechanisms and combined mobility according to (8.12). Adapted from [654]
(a)
(b)
Fig. 8.5 Temperature dependence of the electron mobility in ntype (a) bulk ZnO and (b) a PLDgrown ZnO thin film on sapphire. In the latter, grainboundary scattering is limiting the mobility. Squares are experimental data, solid lines are theoretical mobilities for various scattering mechanisms and combined mobility according to (8.12). Experimental data from [655]
(see Fig. 8.6). At very high temperature, when intrinsic conduction starts, σ shows a strong increase due to the increase in n. At low temperature, the disorder due to doping (random positions of the impurity atoms) leads to a temperature driven metal–insulator transition as depicted in Fig. 7.29.
266
8 Transport
(a)
(b)
Fig. 8.6 (a) Carrier concentration and (b) conductivity of ntype Ge as a function of temperature. The doping level varies from ND ≈ 1013 –1018 (samples A–F as in Fig. 8.4a where the mobility of the same samples is shown). The dashed lines are for intrinsic Ge. The solid lines are guides to the eye. Adapted from [515]
8.3.10 Doping Dependence The mobility decreases with increasing dopant concentration as already shown in Figs. 8.2 and 8.4a. In Fig. 8.7a the low doping limit is due to deformation potential scattering; the decrease with doping is due to ionized impurity scattering. At high doping level, it becomes more important at room temperature than (acoustical or optical) phonon scattering [656]. The mobility of carriers in n and ptype silicon with very high carrier concentrations is depicted in Fig. 8.7b. Thus, for bulk material high carrier density and high mobility are contrary targets and cannot be achieved simultaneously. A solution will be provided with the concept of modulation doping where the dopants and the (twodimensional) carrier gas will be spatially separated in a heterostructure (cf. Sect. 12.3.4). At high doping, the substitutional character of the impurities may be lost and secondary phases can arise, e.g. as observed for highly doped ZnO:Ga, exhibiting octahedral coordination of gallium in a parasitic ZnGa2 O4 spinel phase for [Ga]=4 % [553]. The onset of such segregation phenomena is accompanied with the decrease of mobility and conductivity.
8.3 LowField Transport
(a)
267
(b)
Fig. 8.7 (a) Electron mobility in Si:P at room temperature over a wide range of carrier concentrations. (b) Electron mobility in Si:P and hole mobility in Si:B for various high carrier concentrations. Adapted from [657]
8.3.11 Piezoresistivity The dependence of resistivity on stress or strain is known as piezoresistive effect, first described in [658]. It is a consequence of the modification of the band structure upon stress and the change of effective masses (Sect. 6.10.2). In a cubic material, the resistivity ρi for transport in cartesian direction i changes compared to the unstrained state in a phenomenological description according to Δρi = πi j σ j , ρi
(8.26)
where π is the piezoresistivity tensor (8.27) and the σ j form the sixcomponent stress tensor (5.59), ⎞ ⎛ π11 π12 π12 0 0 0 ⎜ π12 π11 π12 0 0 0 ⎟ ⎟ ⎜ ⎜ π12 π12 π11 0 0 0 ⎟ ⎟. ⎜ π=⎜ (8.27) ⎟ ⎜ 0 0 0 π44 0 0 ⎟ ⎝ 0 0 0 0 π44 0 ⎠ 0 0 0 0 0 π44 Values for the piezoelectric coefficients are given in Table 8.3 for Si, Ge and GaAs. The piezoelectric effect has been discussed in detail [659] and modeled for ptype Si [660]. We shall only give a simple example which is particularly relevant for advanced CMOS design (Sect. 24.5.5); the directional dependence of the piezoresistive coefficient of silicon is shown for uniaxial stress within in the (001) plane in Fig. 8.8. Uniaxial tensile stress increases hole resistivity along 110 stress directions, compressive stress thus increases hole conductivity.
268
8 Transport
Table 8.3 Piezoresistivity coefficients (in 10−11 Pa−1 ) for Si, Ge and GaAs at room temperature Material ρ ( cm) π11 π12 π44 Reference pSi nSi pGe (Ge:Ga) nGe (Ge:As) pGaAs nGaAs
7.8 11.7 15.0 9.9 ∼10−3 ∼10−3
6.6 −102.2 −10.6 −4.7 −12.0 −3.2
(a)
−1.1 53.4 5.0 −5.0 −0.6 −5.4
138.1 −13.6 98.6 −137.9 46 −2.5
[658] [658] [658] [658] [662] [662, 663]
(b)
Fig. 8.8 Piezoresistive coefficient for current parallel (perpendicular) to the stress πl as blue lines (πt , red lines) for uniaxially stressed Si (001) at room temperature, (a) for ptype Si, (b) for ntype Si. The upper (lower) halves of the graphs show positive (negative) values of the piezoresistive coefficient, i.e. resistivity increases (decreases) with tensile stress. The solid circle indicates the value of π = 10−9 Pa−1 , the dashed circle half that value. Adapted from [661]
8.4 HighField Transport In the case of small electric fields the scattering events are elastic. The drift velocity is linearly proportional to the electric field. The average thermal energy is close to its thermal value 3kT /2 and the carriers are close to their band edges (Fig. 8.9a). The scattering efficiency, however, is reduced already at moderate fields. Then, the electron temperature [664] becomes larger than the lattice temperature. With increasing electrical field the carriers can gain more and more energy and will on average populate higher states, assuming a nonBoltzmann (and nonFermi) statistical distribution [665]. The electron distribution in kspace is depicted for silicon for three different electric fields in Fig. 8.9b,c. Hot carriers suffer additional scattering processes that are discussed in the following, namely optical phonon emission, intervalley scattering and impact ionization.
8.4 HighField Transport
269
Fig. 8.9 Distribution of electrons in silicon in momentum space (cmp. Fig. 6.29c) for electric fields of (a) 10 kV/cm, (b) 102 kV/cm and (c) 103 kV/cm. Adapted from [665]
8.4.1 DriftSaturation Velocity If the carrier energy is large enough it can transfer energy to the lattice by the emission of an optical phonon. This mechanism is very efficient and limits the maximum drift velocity. Such behavior is nonohmic. The limiting value for the drift velocity is termed the driftsaturation velocity. It is given by [666] vs =
8 3π
ωLO . m∗
(8.28)
This relation can be obtained from an energybalance consideration. The energy gain per unit time in the electric field is equal to the energy loss by the emission of an optical phonon. ωLO , (8.29) qv·E= τ where τ is the typical relaxation time constant for LO phonon emission. Together with (8.3) we find (8.29) except for the prefactor, which is close to 1. The exact prefactor results from a more exact quantummechanical treatment. For Ge the driftsaturation velocity at room temperature is 6 × 106 cm/s, for Si it is 1 × 107 cm/s (Fig. 8.10a). The carrier velocity also depends on the crystallographic direction [667].
8.4.2 Negative Differential Resistivity In GaAs there is a maximum drift velocity of about 2 × 107 cm/s and following a reduction in velocity with increasing field (1.2 × 107 cm/s at 10 kV/cm, 0.6 × 107 cm/s at 200 kV/cm) as shown in Fig. 8.10a. This regime, above the threshold field of E thr = 3.2 kV/cm in GaAs, is called negative differential resistivity (NDR) and was predicted in [673]. This phenomenon can be used in microwave oscillators, e.g. the Gunn element (Sect. 21.5.11).
270
8 Transport
(b)
(a) 108
ZnO
3.0
10
7
GaAs 7
GaN InP
2.0 Ge
106
InGaAs GaAs
1.0 electrons holes
Si
105 102
103
104
105
Si
106
0
0
100
200
300
Fig. 8.10 Drift velocity at room temperature as a function of applied electric field for (a) highpurity Si, Ge, and GaAs on a doublelogarithmic plot and (b) on linear plots for Si [668], Ge [669], GaAs [598], InP [670], InGaAs [671], GaN and ZnO [672] Table 8.4 Material parameters for multivalley bandstructure of GaAs and InP vP Material E g (eV) ΔE (eV) E thr Lower valley (Γ ) Upper valley (L) (kV/cm) (107 cm/s) m ∗ (m 0 ) μn m ∗ (m 0 ) μn 2 (cm /Vs) (cm2 /Vs) GaAs InP
1.42 1.35
0.36 0.53
3.2 10.5
2.2 2.5
0.068 0.08
≈8000 ≈5000
1.2 0.9
≈180 ≈100
ΔE denotes the energetic separation of the two lowest valleys of the conduction band, E thr the threshold field for NDR and vP the peak velocity (at E thr ). Most values from [675]
The effect occurs in a multivalley band structure (see Fig. 8.11, for values cf. Table 8.4), e.g. in GaAs or InP, when the carrier energy is high enough to scatter (Fig. 8.11c, d) from the Γ minimum (small mass and high mobility) into the L valley (large mass and low mobility) [674]. The temperature dependence of the saturation velocity is shown in Fig. 8.12. With increasing temperature the saturation velocity decreases since the coupling with the lattice becomes stronger.
8.4.3 Velocity Overshoot When the electric field is switched on, the carriers are at first in the Γ minimum (Fig. 8.11a). Only after a few scattering processes are they scattered into the L minimum. This means that in the first moments transport occurs with the higher mobility of the lowest minimum (Fig. 8.11e). The velocity is then larger than the (steadystate) saturation velocity in a dc field. This phenomenon is called velocity overshoot and is
8.4 HighField Transport
271
(a)
(b)
(c)
(d)
(e)
Fig. 8.11 Chargecarrier distribution in a multivalley band structure (e.g. GaAs, InP) for (a) zero, (b) small (E < E a ), (c) intermediate and (d) large (E > E b ) field strength. The situation shown in (e) is reached temporarily during velocity overshoot (see also Fig. 8.13) Fig. 8.12 Temperature dependence of the saturation velocity for Si (following vs = vs0 (1 + 0.8 exp(T /600 K))−1 with vs0 = 2.4 × 107 cm/s from [668]) and GaAs [598, 676, 677]
a purely dynamic effect (Fig. 8.13). Velocity overshoot in GaN is discussed in [678]. It is an important effect in small transistors.
8.4.4 Impact Ionization If the energy gain in the field is large enough to generate an electron–hole pair, the phenomenon of impact ionization occurs. The kinetic energy is ∝ v 2 . Momentum and energy conservation apply. Thus, at small energies (close to the threshold for impact ionization) the vectors are short and collinear to fulfill momentum conservation. At
272
8 Transport
Fig. 8.13 Time dependence of the electron velocity at room temperature upon a steplike electric field (40 kV/cm) for GaAs (dashdotted line), InP (dashed line) and In0.53 Ga0.47 As (solid line)
In0.53Ga0.47As
7
8
6
4
InP
2
GaAs 0
0.2
0
0.4
0.6
0.8
higher energy, larger angles between the velocity vectors of the impact partners can also occur. If the process is started by an electron (Fig. 8.14a) the threshold energy is given by [679] me thr (8.30) Eg. Ee = 1 + m e + m hh If the process starts with a heavy hole, the threshold [679], thr = 1+ E hh
m hh m e + m hh
Eg,
(8.31)
is larger because of the larger hole mass. The threshold for impact ionization triggered by a splitoff hole (shown schematically in Fig. 8.14b) is [680] m so (1 − Δ0 /E g ) Eg. E hthr = 1 + 2 m hh + m e − m so
(8.32)
Thus soholes have typically the smaller threshold.3 At energies where impact ionization occurs, nonparabolicities are typically important, thus (8.30)–(8.32) are only indicative. The threshold behavior and the dependence of the scattering rate as a function of the primary carrier energy in Si, calculated considering the detailed band structure, is shown in Fig. 8.15.
3 Assuming
thr /E thr ≈ 1 − (m /m )(1 + Δ/E )/2 < 1. m so = m e , m e m hh and Δ0 E g , E so e hh g e
8.4 HighField Transport Fig. 8.14 Electron and hole transitions for impact ionization close to the threshold energy. Ionization is triggered by (a) an electron and (b) a splitoff hole of velocity vi
273
(a) e
(b)
E
E
vi e
Eg Eg
hh
lh
hh
lh
vi so
so
k 15
10
Si
14
10
Ionization rate (s1)
Fig. 8.15 Impact ionization rate as a function of primary carrier energy for electrons (solid line) and holes (dashed line) in silicon at room temperature. The curves are fit to results from a MonteCarlo simulation. Adapted from [681, 682]
k
h
13
e
10
12
10
11
10
10
10
9
10
8
10
7
10
0
1
2
3
4
5
Primary energy (eV)
The generation rate G of electron–hole pairs during impact ionization is given by G = αn n vn + αp p vp ,
(8.33)
where αn is the electron ionization coefficient. It describes the generation of electron– hole pairs per incoming electron per unit length. αp denotes the hole ionization coefficient. The coefficients depend strongly on the applied electric field. They are shown in Fig. 8.16. They also depend on the crystallographic direction. The impact ionization initiated by electrons and holes in silicon has been calculated considering the full band structure using a Monte Carlo technique in [681] and [682], respectively. In both cases the impact ionization rate is anisotropic for excess energies smaller than 3 eV and become isotropic above. The average energies
274
8 Transport
Fig. 8.16 Impact ionization rates for electrons and holes as a function of the inverse electric field for Si, Ge and other compound semiconductors at 300 K. Adapted from [500]
Fig. 8.17 Averaged rates for electron initiated impact ionization in GaAs (circles) and GaN (squares). Adapted from [683]
at the moment of generation of secondary generated carriers depends linearly on the primary electron or hole energy. The energy dependence of the electron initiated impact ionization rate has been calculated for GaAs, GaN and ZnS considering details and anisotropy of the band structure in [683]. The rates averaged over the Brillouin zone are compared in Fig. 8.17. Because of the large band gap of GaN, impact ionization can only be generated by electrons in higher conduction bands. The sharp increase of ionization rate for GaN around 5.75 eV correlates with a large valence band DOS from hole states at the zone boundary.
8.5 HighFrequency Transport
275
8.5 HighFrequency Transport The above consideration pertained to dc (or slowly varying) fields. Now, we consider an ac field. It accelerates the carriers but at the same time the dissipative force in the relaxationtime approximation is present, i.e. (for electrons) m ∗ v˙ = −e E − m ∗
v . τ
(8.34)
For a harmonic field E ∝ exp(−iωt) the complex conductivity (j = σE = nqv) is σ=
1 i n e2 n e2 τ = , ∗ ∗ m 1 − i ωτ m ω + iγ
(8.35)
with γ = 1/τ being the damping constant. Splitting into real and imaginary parts yields ωτ 1 n e2 τ +i . (8.36) σ= m∗ 1 + ω2 τ 2 1 + ω2 τ 2 For small frequencies (ω → 0) the dc conductivity from (8.5) is recovered, i.e. σ = ne2 τ /m ∗ . For high frequencies (ωτ 1) n e2 τ σ= m∗
1 1 +i ω2 τ 2 ωτ
.
(8.37)
8.6 Polarons In an ionic lattice, the electron polarizes the ions and causes a change of their equilibrium position. Depending of the severity of this effect, the lattice polarization leads to a modification of carrier (electron or hole) mass during band transport (Sect. 8.6.1) (large polarons) or the lattice deformation is so strong that it leads to carrier localization on the length scale of the lattice constant. Such selftrapped carriers are termed small polarons and discussed in Sect. 8.6.1. Reviews are given in [684, 685].
8.6.1 Large Polarons When the electron moves through the ionic crystal and must drag an ion displacement with it, the effective electron mass changes to the ‘polaron mass’ m p ,4 4 For the calculation, manyparticle theory and techniques are needed; the best solution is still given
by Feynman’s path integral calculation [686–688].
276
8 Transport
Table 8.5 Fröhlich coupling constant α for various semiconductors GaSb GaAs GaP GaN InSb InAs 0.025 0.068 0.201 0.48 0.022 0.045 3CSiC ZnO ZnS ZnSe ZnTe CdS 0.26 1.19 0.63 0.43 0.33 0.51
InP 0.15 CdSe 0.46
InN 0.24 CdTe 0.35
Data from [691]
α m p = m ∗ 1 + + 0.025 α2 + · · · , 6
(8.38)
for α ≤ 1, with m ∗ being the band mass as defined in Sect. 6.8.2 and α the Fröhlich coupling constant5 1 e2 2 m ∗ 1 1 α= − . (8.39) 2 ωLO ∞ 0 This process it called the polaronic effect and requires additional energy [686, 689]. Often, the polaron mass is given as m p = m ∗ /(1 − α/6) which is the result of perturbation theory [689] and an approximation to (8.38) for small α. For large coupling parameter, α 1, the polaron mass is given by [687] mp = m∗
16 α4 . 81 π 4
(8.40)
The energy of the electron is lowered due to the interaction with the lattice. The energy E 0 for k = 0 is given, relative to the uncoupled case, by E 0 = − α + 0.0098 α2 + · · · ω0 , α ≤ 1 E 0 = − 2.83 + 0.106 α2 ω0 , α 1
(8.41a) (8.41b)
Numerical results are reported in [690]. Polarons in semiconductors are typically ‘large’ or Fröhlichtype polarons, i.e. the coupling constant is small (Table 8.5). The dressing with phonons (as the ion displacement is called in a quantummechanical picture) is then only a perturbative effect and the number of phonons per electron (≈α/2) is small. If α becomes large (α > 1, α ∼ 6), as is the case for strongly ionic crystals such as alkali halides, the polaron becomes localized by the electron–phonon interaction6 and hopping occurs infrequently from site to site.
5 This constant is part of the matrix element in the Hamiltonian of the electron–phonon interaction and is related to the electric field created by LO phonons, as given in (5.52). 6 One can think about it in the way that the electron strongly polarizes the lattice and digs itself a potential hole out of which it can no longer move.
8.6 Polarons
277
Fig. 8.18 Hole from Nb acceptor localized on Ti site (small polaron) in rutile TiO2 . Adapted from [694]
simulation
experiment
(101) Fig. 8.19 Simulated and experimental TEM images of βGa2 O3 in (101) projection. The arrow denotes the position of a polaron. Adapted from [693]
8.6.2 Small Polarons In a polaron, the charge carrier (electron or hole) sits in a potential well resulting from the ionic displacements it created. In some materials, the shape and strength of this potential well is such that the charge is confined to a volume of approximately one unit cell or less. In this case, the polaron is called a small polaron. An example of a hole polaron in rutile TiO2 :Nb is depicted in Fig. 8.18. In oxides often the hole from an acceptor is bound to oxygen, e.g. in BaTiO3 :Na, as reviewed in [692]. In Fig. 8.19 the lattice relaxation due to a hole bound to oxygen in the monoclinc unit cell of βGa2 O3 is depicted directly using aberration corrected TEM. The bonding of the hole to the oxygen atom breaks the bond to a Ga atom which moves by 0.1 nm from its equilibrium position [693]. A proper theoretical analysis of a small polaron requires ab initio techniques that account for the motion of each atom in the few unit cells nearest the electron.7 The transport of small polarons occurs generally via thermallyactivated hopping (cmp. Sect. 8.7). Under certain conditions the following mobilities for drift and Hall 7 This
paragraph has been taken from the concise tutorial by S.J.F. Byrnes [695].
278
8 Transport
effect have been given [684]: μd ∝ T −1 exp(−W/(2kT )), μH ∝ T −1/2 exp(−W/(6kT )),
(8.42) (8.43)
W being the polaron binding energy. Generally, materials with small polar on transport exhibit high carrier density, often due to structural defects, and low mobility.
8.7 Hopping Transport Disordered solids such as amorphous semiconductors, films containing quantum dots or material with many defects are characterized by a large density of localized states which can form band tails or a large density of states within the band gap. Hopping conduction is the tunneling between localized states and has been treated with various models [696–698]. A commonly observed phenomenon is the variable range hopping with a conductivity given by (8.44) σ = σ0 exp −(T0 /T )s with s = 1/4. Such law is fulfilled for amorphous silicon (Fig. 8.20). Mott has derived [700] and the exponent s = 1/4 using the following argument: The probability p to
Fig. 8.20 Temperature dependence of the planar resistance for Si films deposited at room temperature. Solid line is linear fit with T0 = 8 × 107 K according to (8.44) (s = 1/4). Adapted from [699]
T 300
200
100
aSi 12
10
11
10
10
10
9
10
8
10
7
10
6
10
0.25
0.27
0.29
0.31
T1/4 (K1/4)
0.33
0.35
8.7 Hopping Transport
279
hop from one localized site to another is proportional to p ∝ exp(−2αR − W/kT ).
(8.45)
The first term stems from the probability to find the electron within radius R from its initial site, α being the decay constant of its wave function, Ψ (r ) ∝ exp(−α r ). The second term is the Boltzmann factor for bridging the energy mismatch W between localized states with a phononassisted process, assuming a low temperature limit (kT W ). There is a tradeoff between hopping to levels closer in energy but spatially further away (on average), preferred at low temperature and the hopping to energy levels with larger W but spatially closer at higher temperatures. Thus the hopping range changes with temperature, giving the mechanism its name. D(E F ) shall be the (constant) density of localized states around the Fermi level. Within a radius R, there is on average one state of energy between 0 and W (R) when (for threedimensional bulk material) W (R) =
1 . D(E F ) (4π/3) R 3
(8.46)
Substituting (8.46) in (8.44) and searching for the maximum yields the most probable hopping distance (8.47) R ≈ (α kT D(E F ))−1/4 , showing again, the varying range of hopping with temperature. Thus we find for T0 in (8.44), α3 . (8.48) T0 ≈ k D(E F ) Other types of hopping mechanisms are the Efros–Shklovskii variable range hopping (s = 1/2), emerging for an energy dependent density of states D(E) ∝ (E − E F )2 due to Coulomb interaction between hopping sites [701], or the next neighbor hopping (s = 1). From (8.44) one can rewrite for ξ = d(ln σ(T ))/d ln T , ln ξ = ln s + s ln T0 − s ln T.
(8.49)
Thus in a plot of ln ξ versus ln T , the exponent s can be determined from the slope. As can be seen in Fig. 8.21, for the conductivity of a hydrogenated amorphous silicon thin film the transition of hopping mechanism from Efros–Shklovskii variable range hopping (s ≈ 1/2) to next neighbor hopping (s ≈ 1) takes place around T = 220 K, as discussed in detail in [702].
280
8 Transport
Fig. 8.21 Temperature dependence of conductivity of a hydrogenated amorphous Si thin film, plotted as ln ξ versus ln T (8.49). Solid lines are linear fits for constant s according to (8.49) as labelled. Adapted from [702]
T 100
150
200
250
300
0.0
aSi:H 0.2
s=0.54±0.05
0.4
ln
0.6 0.8 1.0
s=1.08±0.14 1.2 1.4
4.8
5.0
5.2
5.4
5.6
5.8
ln (T
8.8 Transport in Amorphous Semiconductors Many models have been presented for the carrier transport in amorphous semiconductors [178]. The most important concept is that of a mobility edge, an energy separating localized from delocalized states [475, 476, 703]. This is schematically depicted in Fig. 8.22. The carrier transport between localized states is mediated via tunneling (hopping) which has been described in the previous section (Sect. 8.7). The localization of carriers in random lattices has been treated by Anderson [560] and reviewed in [558]. If the degree of disorder surpasses a certain value, diffusion is suppressed (at T = 0) and conductivity vanishes altogether (Anderson metal–insulator transition).
delocalized
localized
delocalized
DOS (arb. units)
Fig. 8.22 Schematic density of states of amorphous semiconductor with band tails and deep levels. The localized (delocalized) states are shown in dark (light) grey. The mobility edges for electrons and holes are indicated by dashed lines
EV
EF Energy
EC
8.8 Transport in Amorphous Semiconductors
281
The transport in delocalized states is similar to band transport. The conductivity (for electrons) is given as σ = −e
∞
De (E) μe (E) f e (E) dE.
(8.50)
EC
If the Fermi energy is close to the middle of the gap, pinned to deep states, the FermiDirac distribution can be replaced by the Boltzmann factor. Assuming a constant density of states and mobility for the delocalized states, σ = −e De (E C ) μe (E C ) kT exp
EC − EF kT
.
(8.51)
Charge carriers from localized states in the tails can be thermally excited into delocalized states and contribute to conductivity (thermally activated hopping). The mobility then contains an exponential thermal activation term [178].
8.9 Ionic Transport Ionic transport is the movement of ions upon application of a voltage. Here, we discuss only solid electrolytes. The transport can include the motion of one or several of the constituents of the lattice and the transport of other ions (e.g. hydrogen ions (protons), oxygen ions) through the crystal. Related to this is the diffusive ionic movement of impurities or defects through the crystal (cmp. Sect. 4.2.3). Ionic conduction of the lattice constituents under dc voltage will eventually destroy the crystal. In typical semiconductors like silicon or gallium arsenide, the conductivity is entirely due to electronic conduction. A typical solid electrolyte is zirconia (ZrO2 ) doped with yttria, socalled yttriastabilized zirconia (YSZ) that takes on a cubic fluorite lattice (see Sect. 3.4.8). It can conduct oxygen ions via the mobility of oxygen vacancies for use in solidoxide fuel cells (SOFC) [704]. The conductivity is about 0.01 S/cm at a temperature around 1000 K, almost entirely due to ionic transport. Doping with calcium oxide results in an oxygen conductor that is used in oxygen sensors in automobiles (lambda sensor). The ionic conductivity can be significantly increased, compared to bulk material, along interfaces [705, 706]. Other typical solid electrolytes are cuprous iodide (CuI) [494] and also AgI. In the high temperature cubic phase (αpolymorph), the iodide ions form a fairly rigid cubic framework and the metal ions are mobile; the copper diffusion pathways have been discussed [707, 708]. The temperature dependence of conductivity of CuI is shown in Fig. 8.23.
282 Fig. 8.23 Total (circles) and electronic (squares) conductivity of CuI coexisting with copper. Filled (empty) symbols refer to polycrystalline (single crystal) samples. The different structural phases (α (cubic), β (wurtzite), γ (zincblende)) are indicated by shaded areas as labeled. Dashed lines are guides to the eyes. Adapted from [709]
8 Transport
405
369 350
300
275
CuI 1
10
0
10
10
1
10
2
1.3
1.4
1.5
1.6
1.7
1.8
1.9
1000/T (1000/K)
8.10 Diffusion A gradient of a particle concentration n leads to a particle current proportional to −∇n. This diffusion law (Fick’s law) corresponds microscopically to a random walk. The gradients of the semiconductor carrier densities ∇n or ∇ p thus lead to electron and hole currents, respectively: jn = eDn ∇n jp = −eDp ∇ p.
(8.52a) (8.52b)
The coefficients Dn and Dp are called the electron and hole diffusion coefficient, respectively. Thus the total electron and hole currents in the presence of an electric field E and diffusion are jn = −eμn n E + eDn ∇n jp = eμp p E − eDp ∇ p.
(8.53a) (8.53b)
This relation can also be deduced more generally from the gradient of the Fermi level as jn = −eμn n E − nμn ∇ E F jp = eμp p E − pμp ∇ E F .
(8.54a) (8.54b)
8.10 Diffusion
283
Using (7.6) and (7.7) for the concentrations (valid also in the case of degeneracy) and using dF j (x)/dx = F j−1 (x) we obtain F1/2 (η) ∇n F−1/2 (η) F1/2 (ζ) ∇ p, jp = eμp p E − kT μp F−1/2 (ζ)
jn = −eμn n E − kT μn
(8.55a) (8.55b)
with η = (E F − E C )/kT and ζ = −(E F − E V )/kT . If the prefactor of the density gradient is identified as the diffusion coefficient we find the (generalized) socalled ‘Einstein relations’ (β = e/(kT )) [529, 710]: F1/2 (η) F−1/2 (η) F 1/2 (ζ) . Dp = β −1 μp F−1/2 (ζ)
Dn = −β −1 μn
(8.56a) (8.56b)
Useful analytical approximations have been discussed in [711]. We note that, e.g., (8.56a) can also be written as [712, 713] Dn = −β −1 μn n
∂η . ∂n
(8.57)
In the case of nondegeneracy, i.e. when the Fermi level is within the band gap and not closer than about 4kT to the band edges, η = ln(n/NC ). Then ∂η/∂n = 1/n, and the equation simplifies to D = (kT /q) μ, i.e. the ‘regular’ Einsteinrelations, Dn = −β −1 μn Dp = β −1 μp .
(8.58b)
jn = −eμn n E − kT μn ∇n jp = eμp p E − kT μ p ∇ p.
(8.59a) (8.59b)
(8.58a)
In this case, (8.53a,b) read
We recall that both diffusion coefficients are positive numbers, since μn is negative. Generally, the diffusion coefficient depends on the density. A Taylor series of the Fermi integral yields −1
Dn = −β μn 1 + 0.35355
n NC
− 9.9 × 10
−3
n NC
2
+ ··· .
(8.60)
284
8 Transport
8.11 Continuity Equation The balance equation for the charge is called the continuity equation. The temporal change of the charge in a volume element is given by the divergence of the current and any source (generation rate G), e.g. an external excitation, or drain (recombination rate U ). Details about recombination mechanisms are discussed in Chap. 10. Thus, we have ∂n = G n − Un − ∂t ∂p = G p − Up − ∂t
1 1 ∇ · jn = G n − U n + ∇ · jn q e 1 ∇ · jp . e
(8.61a) (8.61b)
In the case of nondegeneracy we find, using (8.53a,b) ∂n = G n − Un − μn n ∇ · E − μn E ∇n + Dn Δn ∂t ∂p = G p − Up − μp p ∇ · E − μp E ∇ p + Dp Δp. ∂t
(8.62a) (8.62b)
In the case of zero electric field these read ∂n = G n − Un + Dn Δn ∂t ∂p = G p − Up + Dp Δp, ∂t
(8.63a) (8.63b)
and if the stationary case also applies: Dn Δn = −G n + Un Dp Δp = −G p + Up .
(8.64a) (8.64b)
8.12 Heat Conduction We consider here the heat transport [714] due to a temperature gradient. The heat ˆ is proportional to the local flow q, i.e. energy per unit area per time in the direction q, gradient of temperature. The proportionality constant κ is called, heat conductivity, q = −κ ∇T.
(8.65)
In crystals, the heat conductivity can depend on the direction and thus κ is generally a tensor of rank 2. In the following, κ will be considered as a scalar quantity. The quite generally valid Wiedemann–Franz law connects the thermal and electrical
8.12 Heat Conduction
285
conductivities
π2 κ= 3
2 k T σ. e
(8.66)
The balance (continuity) equation for the heat energy Q is ∇· q = −
∂T ∂Q = −ρC + A, ∂t ∂t
(8.67)
where ρ denotes the density of the solid and C the heat capacity. A denotes a source or drain of heat, e.g. an external excitation. Combining (8.65) and (8.67), we obtain the equation for heat conductivity ΔT =
A ρ C ∂T − , κ ∂t κ
(8.68)
which simply reads ΔT = 0 for a stationary situation without sources. The random mixture of various atoms in natural elements represents a perturbation of the perfectly periodic lattice. Since the mass of the nuclei varies, in particular lattice vibrations will be perturbed. Thus we expect an effect on the heat conductivity. In Fig. 8.24, the thermal conductivity of crystals from natural Ge and enriched 74 Ge are compared [715], the latter having, as expected, the higher heat conductivity, i.e. less scattering. The thermal conductivity of isotopically pure 28 Si thin films has been measured to be 60 % greater than natural silicon at room temperature and at least 40 % greater at 100 ◦ C, a typical chip operating temperature [716, 717]. 100
T3
50
enriched 74Ge
1
20 10
1
Fig. 8.24 Thermal conductivity of Ge versus temperature. The enriched Ge consists of 96 % 74 Ge while the natural isotope mix is 20 % 70 Ge, 27 % 72 Ge, 8 % 73 Ge, 27 % 74 Ge and 8 % 76 Ge. The dashed line shows the κ ∝ T 3 dependence at low temperatures (Debye’s law). Adapted from [715]
5 2 1 0.5 0.2
1
2
5
10
20
50
100 200
500
286
8 Transport
8.13 Coupled Heat and Charge Transport The standard effect of coupled charge and heat transport is that a current heats its conductor via Joule heating. However, more intricate use of thermoelectric effects can also be employed to cool certain areas of a device. For further details see [718, 719]. For the analysis of coupled charge and heat transport we first sum the electric field and the concentration gradient to a new field Eˆ = E + ∇ E F /e. Then, the heat flow and charge current are j = σ Eˆ + L ∇T q = M Eˆ + N ∇T,
(8.69) (8.70)
where Eˆ and ∇T are the stimulators for the currents. From the experimental point of view there is interest to express the equations in j and ∇T since these quantities are measurable. With new coefficients they read Eˆ = ρ j + S ∇T q = j − κ ∇T,
(8.71) (8.72)
where ρ, S and Π are the specific resistance, thermoelectric power and Peltier coefficient (transported energy per unit charge), respectively. The relations with the coefficients σ, L, M, and N are given by ρ=
1 σ
L σ M Π= σ ML κ= − N. σ S=−
(8.73a) (8.73b) (8.73c) (8.73d)
8.13.1 Thermopower and Seebeck Effect A semiconductor shall have two ends at different temperatures T2 and T1 and a temperature gradient in between in an open circuit, i.e. j = 0. Then a field Eˆ = S ∇T and a voltage U = S/(T2 − T1 ) will arise. This effect is called the thermoelectric or Seebeck effect. S is termed the Seebeck coefficient or the thermoelectric power, often also denoted as Q in the literature. The voltage can be measured and used to determine the temperature at one end if the temperature at the other end is known, forming a thermometer. The Seebeck coefficient is positive if the electric field is in the same direction as the temperature gradient.
8.13 Coupled Heat and Charge Transport
287
A famous relation from irreversible thermodynamics connects it to the Peltier coefficient via Π (8.74) S= . T The Seebeck coefficient is related to the energy transport by charge carriers. The heat (energy) flow is obviously from the hot to the cold end (assuming here T2 > T1 ), so is the flow of charge carriers. In a simple picture, if the energy is carried by (hot) holes, the current (by definition the direction of positive charge carriers) is from the hot to the cold end (2 → 1); if the energy flow is carried by electrons, the current flows from the cold to the hot end (1 → 2). Accordingly, energy transport by electrons and holes gives rise to different signs of the thermoelectric coefficient (Fig. 8.25). If the cold (unheated) substrate is grounded, the sign of the voltage at a hot solder tip pressed (carefully) on the surface of the semiconductor yields the conductivity type, ntype (ptype) for a negative (positive) voltage. However, the semiconductor should not be heated so strongly that intrinsic conduction arises. In this case the conductivity and the thermoelectric power is determined by the carrier type with the higher mobility; typically, and for the case of silicon shown in Fig. 8.25, these are the electrons thus yielding a negative Seebeck coefficient in the intrinsic regime. For band conduction the thermopower (I.29) is given for electrons (Sn ) and holes (Sp ) by [722] (for a derivation see Sect. I.4)
(a)
(b) 0.6
Ge 0.6 0.3 0 0.3 0.6 0.9
100 200 300 400 500 600 700 800 900 1000
Temperature (K)
Thermoelectric force S T (V)
Thermoelectric force S (mV/K)
0.9
Si
0.4 0.2 ptype
0 ntype
0.2 intrinsic
0.4 0.6 0.8
200
300
400
500
600
700
800
900 1000
Temperature (K)
Fig. 8.25 (a) Seebeck coefficient S for n and pdoped germanium. Experimental data (symbols) and theory (lines). NA − ND is 5.7 × 1015 cm−3 (white circles), 1.7 × 1017 cm−3 (grey) and 7.2 × 1018 cm−3 (black); ND − NA is 3.3 × 1015 cm−3 (white squares), 1.1 × 1017 cm−3 (grey) and 6.2 × 1017 cm−3 (black) Adapted from [720]. (b) Thermoelectric force of lowly doped n and psilicon as a function of temperature. Solid line is from simple model calculation and symbols represent data from silicon samples with the approximate doping of circles: 1 × 1015 cm−3 B, 2 × 1014 cm−3 donors, squares 4 × 1014 cm−3 P, 9 × 1013 cm−3 acceptors. Adapted from [721]
288
8 Transport
k EC − EF + AC e kT k EF − EV + AV , Sp = e kT
Sn = −
(8.75a) (8.75b)
where Ai are constants (I.31a) depending on the energy dependence of the density of states and the mobility. The sign of the thermopower tells whether conduction takes place above (negative sign) or below (positive sign) the Fermi level. If the Fermi level is fixed and both electrons and holes contribute (twoband conduction), the thermopower is (evaluating (I.32), b = σn /σ p and the gap center energy E M = (E C − E V )/2) k S= e
EF − EM AV − b AC 1 − b Eg + + 1 + b 2 kT kT 1+b
.
(8.76)
In the case of intrinsic conduction from (7.18) E F − E M = (kT /2) ln(NV /NC ). The thermoelectric power from some highly doped ntype silicon samples is depicted in Fig. 8.26a. At low temperature the (low) conductivity is due to conduction in a donor impurity band (cmp. Sect. 7.5.7). At high compensation of about 90 % (grey data points in Fig. 8.26a), the band is only 10 % filled and acts like a valence band with positive thermopower at sufficiently low temperature when the free carrier density is small. Without compensation, the thermopower remains negative since the almost completely filled impurity band acts conduction band like. The dependence of thermopower on doping has been simulated in [723] (Fig. 8.26); the
(b)
500
Si 0 500 1000 1500 2000 0
10
20
30
40
Temperature (K)
50
60
Thermoelectric power S ( V/K)
Thermoelectric power S (mV/K)
(a)
0 Si
500
1000
1014
1015
1016
1017
1018
1019
NDNA (cm3)
Fig. 8.26 (a) Thermoelectric power S of highly doped ntype silicon as a function of temperature. Circles are experimental data and dashed lines guides to the eyes. The approximate doping of the samples is white 2.7 × 1019 cm−3 As, grey 2.2 × 1018 cm−3 As, black 1.1 × 1018 cm−3 As and 1.0 × 1018 cm−3 B with ND − ND = 1.25 × 1017 cm−3 at room temperature. Adapted from [721]. (b) Thermopower of doped ntype silicon at room temperature as a function of doping concentration. Experimental data (symbols) from [721] and theory (solid line) from [723]
8.13 Coupled Heat and Charge Transport
289
decrease with increasing doping is mostly attributed to the reduced mobility due to ionized impurity scattering. The increase of thermopower at low temperatures is due to the phonondrag effect which is discussed for the samples from [721] in [724]. As a figure of merit for the production of thermoelectric power the Z T value is used, Z T = σ S 2 T /κ.
8.13.2 Peltier Effect In a semiconductor with a temperature difference at its ends a current flow will be allowed now (short circuit). The current leads via the charge transport also to a heat (or energy) transport. This effect is called the Peltier effect. The Peltier coefficient is negative (positive) for electrons (holes). The total amount of energy P that is transported consists of the generation term and the loss due to transport: P = j · Eˆ − ∇ · q.
(8.77)
With (8.71) and (8.72) we find P=
j·j + S j ·∇T − Π ∇ · q + κ ΔT. σ
(8.78)
The first term is Joule heating, the second term is Thomson heating. The third exists only when carriers are generated or when they recombine. The fourth term is the heat conduction. In the Thomson term S j ·∇T heat is generated in an ntype semiconductor if j and ∇T are in the same direction. This means that electrons that move from the hotter to the colder part transfer energy to the lattice. The effect can be used to construct a thermoelectric cooler, as shown in Fig. 8.27, that generates a temperature difference due to a current flow. For optimal performance σ should be large to prevent excess Joule heating and κ should be small such that the generated temperature difference is not rapidly equalized. Fig. 8.27 Schematic Peltier cooler. The heat sinks (grey) and the cold junction (black) on the left are metals that make ohmic contacts with the semiconductors. The current flow is such that electrons move through the ntype semiconductor from right to left
j heat sink
ntype T
heat sink
ptype j
Chapter 9
Optical Properties
Abstract After introduction of the complex dielectric function, reflection, diffraction are briefly discussed. The focus lies on absorption mechanisms; several transition types (direct and indirect bandband transitions, impurityrelated transitions, lattice absorption) are discussed including the effects of excitons, polaritons and high carrier density. Also the various effects of the presence of free carriers are given.
9.1 Spectral Regions and Overview The interaction of semiconductors with light is of decisive importance for photonic and optoelectronic devices as well as for the characterization of semiconductor properties. When light hits a semiconductor, reflection, transmission and absorption are considered, as for any dielectric material. The response of the semiconductor largely depends on the photon energy (or wavelength) of the light and various processes contribute to the dielectric function. An overview of the electromagnetic spectrum in the optical range is given in Table 9.1. The energy and wavelength of a photon are related by1 E = hν = hc/λ, i.e. 1240 . (9.1) E [eV] = λ [nm] In the infrared regime, energy is often measured in wave numbers (cm−1 ) for which the conversion 1 meV = 8.056 cm−1 holds.
1 The
more exact numerical value in (9.1) is 1239.84.
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_9
291
292
9 Optical Properties
Table 9.1 Spectral ranges with relevance to semiconductor optical properties Range Wavelengths Energies Deep ultraviolet Ultraviolet Visible Near infrared Midinfrared Far infrared THz region
80 µm
DUV UV VIS NIR MIR FIR THz
>5 eV 3–5 eV 1.6–3 eV 0.6–1.6 eV 60 meV–0.6 eV 1.6–60 meV n 1 . The polarization plane is defined by the surface normal and the kvector of the light (plane of incidence). The parallel (‘p’) polarized wave (TMwave, electric field vector oscillates in the plane) is shown as ‘↔’; perpendicular (‘s’) polarization (TEwave, electric field vector is perpendicular to plane) is depicted as ‘·’
9.3 Reflection and Diffraction
295
Fig. 9.2 Reflectance of the GaAs/vacuum interface (close to the band gap, n r = 3.347) for radiation from vacuum/air (left panel) and from the GaAs (right panel), respectively, as a function of incidence angle and polarization
When the reflected and the diffracted wave are perpendicular to each other, the reflectance of the ppolarized wave is zero. This angle is the Brewster angle φB , tan φB =
n2 . n1
(9.14)
If a wave has vertical incidence from vacuum on a medium with index of refraction n r , the reflectance is given (both polarizations are degenerate) as R=
nr − 1 nr + 1
2 .
(9.15)
For GaAs, the reflectance for vertical incidence is 29.2 %.
9.4 Absorption In the absorption process, energy is transferred from the electromagnetic field to the semiconductor. In the case of a linear absorption process, when the probability of light absorption is proportional to the incoming intensity, the decrease of intensity in the absorbing medium is exponential (Lambert–Beer’s law [725, 726]),2 I (x) = I (0) exp(−α x).
2 In
[726], the absorption coefficient μ was defined via I (d)/I (0) = μd , i.e. μ = exp −α.
(9.16)
296
9 Optical Properties
Fig. 9.3 Schematic absorption spectrum of a typical semiconductor. From [727]
The quantity α is the absorption coefficient, its reverse the absorption depth. The spectral dependence α(E), the absorption spectrum, contains the information of the possible absorption processes, their energy, momentum and angular momentum selection rules, and their oscillator strength. In Fig. 9.3 a schematic absorption spectrum of a semiconductor is depicted. The transition of electrons from the valence to the conduction band begins at the band gap energy. The band gaps of Si, Ge, GaAs, InP, InAs, InSb are in the IR, those of AlAs, GaP, AlP, InN in the VIS, those of GaN and ZnO in the UV, MgO and AlN are in the deep UV. The Coulomb correlation of electrons and holes leads to the formation of excitons that leads to absorption below the band gap. The typical exction binding energy is in the range of 1–100 meV (see Fig. 9.16). Optical transitions from valenceband electrons into donors and from electrons on acceptors into the conduction band lead to band–impurity absorption. In the region from 10–100 meV the interaction with lattice vibrations (phonons) leads to absorption if the phonons are infrared active. Further in the FIR lie transitions from impurities to the closest band edge (donor to conduction and acceptor to valence band). A continuous background is due to freecarrier absorption. If absorption is considered, the reflectance (9.15) needs to be modified. Using the complex index of refraction n ∗ = n r + iκ, it is given as
∗
2 2
n − 1 2
= (n r − 1) + κ . R =
∗
2 n +1 (n r + 1) + κ2
(9.17)
9.5 Electron–Photon Interaction
297
9.5 Electron–Photon Interaction The absorption process is quantum mechanically described by the coupling of electrons and photons. The process is described with timedependent perturbation theory. If Hem is the perturbation operator (electromagnetic field), the transition probability per time wfi for electrons from (unperturbed) state ‘i’ (initial) to state ‘f’ (final) is given (with certain approximations) by Fermi’s golden rule wfi (ω) =
2π
2 Hfi δ(E f − E i − ω),
(9.18)
where ω is the photon energy, E i (E f ) is the energy of the initial (final) state. Hfi is the matrix element
(9.19) Hfi = Ψf H Ψi , where Ψi (Ψf ) are the wavefunctions of the unperturbed initial (final) state. ˙ μH = ∇ × A, A is the vector potential for the electromagnetic field, i.e. E = −A, ∇ · A = 0 (Coulomb gauge). The Hamiltonian of an electron in the electromagnetic field is 1 (9.20) H= (k − qA)2 . 2m When terms in A2 are neglected (i.e. twophoton processes), the perturbation Hamiltonian is thus Hem = −
q i q Ap = A · ∇ ≈ q r · E. m m
(9.21)
The latter approximation is valid for small wavevectors of the electromagnetic wave and is termed the electric dipole approximation. In order to calculate the dielectric function of the semiconductor from its band structure we assume that A is weak and we can apply (9.18). The transition probability R for the photon absorption rate at photon energy ω is then given by3 2π R(ω) =
 cHem v 2 δ (E c (kc ) − E v (kv ) − ω) d3 kc d3 kv , kc
(9.22)
kv
with the Bloch functions c and v of the conduction and valence band, respectively, as given in (6.36b). The vector potential is written as A = Aˆe with a unit vector eˆ parallel to A. The amplitude is connected to the electricfield amplitude E via 3 Here we assume that the valenceband states are filled and the conductionband states are empty. If the conductionband states are filled and the valenceband states are empty, the rate is that of stimulated emission.
298
9 Optical Properties
A=−
E exp (i(qr − ωt)) + exp (−i(qr − ωt)) . 2ω
(9.23)
In the electricdipole approximation the momentum conservation q + kv = kc , q being the momentum of the light wave is approximated by kv = kc . The matrix element is then given by  cHem v 2 = with
2 e2 A2
cˆe · pv
, 2 m
(9.24)
2 1 c eˆ · pv
= pcv 2 = Mb2 , 3
(9.25)
and the momentum matrix element pcv given in (6.35). A kindependent matrix element pcv 2 is often used as an approximation. In Fig. 9.4 the matrix elements for valence to conduction band transitions in GaN are shown as a function of k. GaN
E c
60
20
40
10
20
Ec
C B A
2
pcv  (eV)
30
0 A
0
L M
A
H K
A
L M
A
H K
Fig. 9.4 Theoretical momentum matrix elements  pcv 2 along highsymmetry directions in the Brillouin zone (see Fig. 3.34d) for transitions between valence and conduction bands in GaN and light polarized perpendicular (left panel) and parallel (right panel) to the caxis. The transitions are A: Γ9 (A)→ Γ7c , B: Γ7 (B)→ Γ7c , C: Γ7 (C)→ Γ7c (see Fig. 6.38). Adapted from [728]
In terms of the electricfield amplitude E(ω) the transition probability is
2π e 2
E(ω)
2 2 p  δ (E c (k) − E v (k) − ω) d3 k. R(ω) = cv mω 2
k
(9.26)
9.5 Electron–Photon Interaction
299
If the integration over k is restricted to those values allowed in unit volume, the power that is lost from the field in unit volume is given by R ω, leaving a 1/E factor. The dielectric function = r + ii is given by 1 2π e 2 pcv 2 δ (E c (k) − E v (k) − ω) d3 k 4π0 m ω k e2 2 pcv 2 1 r = 1 + d3 k, 2 2 2 k 0 m ωcv m ωcv 1 − ω /ωcv i =
(9.27a) (9.27b)
with ωcv = E c (k)−E v (k). The second equation has been obtained via the Kramers– Kronig relations4 (see Appendix C). Comparison with (D.7) yields that the oscillator strength of the band–band absorption is given by 2 pcv 2 e2 , (9.28) f = 2 0 m ωcv m ωcv with Ncv =
2 pcv 2 m ωcv
(9.29)
being the classical ‘number’ of oscillators with the frequency ωcv .
9.6 Band–Band Transitions 9.6.1 Joint Density of States The strength of an allowed optical transitions between valence and conduction bands is proportional to the joint density of states (JDOS) Dj (E cv ) (cf. (6.59), (6.60) and (9.27a)) d2 S 1 , (9.30) Dj (E cv ) = 2 3 (2π/L) ∇ ˜ k E cv  S( E) where E cv is an abbreviation for E c (k) − E v (k) and d2 S is a surface element of the constant energy surface with E˜ = E cv . The spin is assumed to generate doubly degenerate bands and accounts for the prefactor 2. Singularities of the JDOS (vanHove singularities or critical points) appear where ∇k E cv vanishes. This occurs when the gradient for both bands is zero or when both bands are parallel. The latter generates particularly large JDOS because the condition is valid at many points in kspace. 4 The real and imaginary parts of the dielectric function are generally related to each other via the Kramers–Kronig relations.
300
9 Optical Properties
Table 9.3 Functional dependence of the joint density of states for critical points in 3, 2 and 1 dimensions Dim. Label Type Dj for E < E 0 Dj for E > E 0 √ 3D M0 Min. 0 E − E0 √ M1 Saddle C − E0 − E C √ Saddle C C − E − E0 M2 √ M3 Max. E0 − E 0 2D M0 Min. 0 C Saddle − ln(E 0 − E) − ln(E − E 0 ) M1 Max. C 0 M2 √ 1D M0 Min. 0 E − E0 √ M1 Max. E0 − E 0 E 0 denotes the energy (band separation) at the critical point, C stands for a constant value. The type of critical point is given (min.: minimum, saddle: saddle point, max.: maximum)
Generally, the (threedimensional) energy dispersion E(k) around a threedimensional critical point (here developed at k = 0) can be written as E(k) = E(0) +
2 ky2 2 kz2 2 kx2 + + . 2m x 2m y 2m z
(9.31)
The singularities are classified as M0 , M1 , M2 and M3 with the index being the number of masses m i in (9.31) that are negative. M0 (M3 ) describes a minimum (maximum) of the band separation. M1 and M2 are saddle points. For a twodimensional kspace there exist M0 , M1 and M2 points (minimum, saddle point and maximum, respectively). For a onedimensional kspace there exist M0 and M1 points (minimum and maximum, respectively). The functional dependence of the JDOS at the critical points is summarized in Table 9.3. The resulting shape of the dielectric function is visualized in Fig. 9.5.
9.6.2 Direct Transitions Transitions between states at the band edges at the Γ point are possible (Fig. 9.6). The k conservation requires (almost) vertical transitions in the E(k) diagram because the length of the light k vector, k = 2π/λ, is much smaller than the size of the Brillouin zone k ≤ π/a0 . The ratio of the lengths of the k vectors is of the order a0 /λ and typically about 10−3 for NIR wavelengths.
9.6 Band–Band Transitions
301
r
M0
M1
i
M2
M3
M0
M1
M2
M3
3D
M0
M1
M2
M0
M1
M2
2D
M0
M0
M1
M1
1D Fig. 9.5 Shape of the real (left panel) and imaginary (right panel) parts of the dielectric function in the vicinity of critical points in 3, 2 and 1 dimensions (for labels see Table 9.3). The dashed line in each graph indicates the energy position of the critical point E 0 . Adapted from [729]
(a)
(b) E
E
h h
E C =E V +Eg
ph,e ph,a
E C =E V +Eg h
EV
k
EV
kph
k
Fig. 9.6 (a) Direct optical transition and (b) indirect optical transitions between valence and conduction bands. The indirect transition involves a phonon with energy ωph (index a: phonon absorption, e: phonon emission) and wavevector kph
For isotropic parabolic bands the bandband transition energy versus wavevector relation is 2 1 1 + ∗ k2. (9.32) E cv (k) = E g + 2 m ∗e mh When the energy dependence of the matrix element is neglected, the absorption coefficient is determined by the corresponding squareroot joint density of states (M0 critical point): E − Eg α(E) ∝ (9.33) ≈ ∝ E − Eg. E
302
9 Optical Properties
The approximation is valid if the considered energy interval, e.g. around a band edge, is small. Absorption spectra of (Inx Ga1−x )2 O3 alloy thin films at room temperature are shown in Fig. 9.7a. The α2 versus photon energy plots shows a linear dependence with broadening and additional states at the band edge due to disorder effects. The extrapolation of the linear parts yields the absorption edge (Fig. 9.7b). Absorption spectra of GaAs are shown in Fig. 9.8a for photon energies close to the band gap at various temperatures. The rapid increase, typical for direct semiconductors, is obvious. In particular at low temperatures, however, the absorption lineshape close to the band gap is dominated by an excitonic feature, discussed in Sect. 9.6.6. Due to the increasing density of states, the absorption increases with the photon energy (Fig. 9.8c). At 1.85 eV there is a step in the absorption spectrum of GaAs due to the beginning of the contribution of transitions between the so hole band and the conduction band (see E 0 + Δ0 transition in Fig. 9.8e). When bands run in parallel, i.e. with the same separation, in the E(k) diagram, the absorption processes accumulate at the same transition energy. In this way higher peaks in the absorption spectrum due to the E 1 or E 0 transitions originate as indicated in the band structure in Fig. 9.8e. The selection rules for transitions from valence to conduction band must take into account the angular momentum and spin states of the wavefunctions. The optical transitions for circularly polarized light are shown in Fig. 9.9a, fulfilling the selection rule Δm j = ±1. A lifting of the energetic degeneracies of these states occurs, e.g. by magnetic fields or spatial confinement (cmp. Fig. 12.29). For twophoton absorption (Sect. 9.6.14), the selection rule is Δm j = ±2 as shown in Fig. 9.9b [732]. We note that in some materials the direct transition between certain bands is forbidden. An example is SnO2 where the direct transition from the topmost valence
(a)
(b)
Fig. 9.7 (a) Absorption spectra of (Inx Ga1−x )2 O3 alloy thin films on Al2 O3 , plotted as α2 versus photon energy. (b) Band edge determined from extrapolation of linear parts
9.6 Band–Band Transitions
303
(a) 4
1
1.2 1.1
GaAs
1.0 0.9 0.8 0.7 0.6
1.42
1.44
1.46
1.48
1.50
1.52
1.54
1.56
(c) GaAs
4
1
(b) 10
E0 +
0
5 E0
0
(d)
1.5
2.0
2.5
(e)
Fig. 9.8 (a) Absorption of GaAs close to the band gap at different temperatures. Adapted from [730]. (b) Highresolution absorption spectrum of highly pure GaAs at T = 1.2 K in the exciton region. Dashed line is theory without excitonic correlation. Adapted from [731]. (c) Absorption spectrum of GaAs at T = 21 K in the vicinity of the band gap. Adapted from [730]. (d) Complex dielectric function of GaAs at T = 300 K, dashed (solid) line real (imaginary) part of dielectric constant. Peak labels relate to transitions shown in part (e). (e) Band structure of GaAs with band gap transition (E 0 ) and higher transitions (E 0 + Δ0 , E 1 , E 1 + Δ1 , E 0 , and E 2 ) indicated
304
9 Optical Properties
(a)
(b)
mj
mj
3/2 hh
1/2
1/2
1/2 lh
1/2 lh
electrons
3/2 hh
holes
3/2 hh
1/2
1/2
1/2 lh
1/2 lh
3/2 hh
Fig. 9.9 Optical selection rules for band–band transitions in bulk material for (a) single photon transitions and (b) twophoton transitions (with photon energy equal to half the transition energy)
band into the lowest conduction band (at Γ ) is forbidden (cmp. Fig. 9.46). If the matrix element increases linearly with E − E g , the absorption coefficient varies like α(E) ∝ (E − E g )3/2 .
(9.34)
9.6.3 Indirect Transitions In an indirect band structure the missing k difference (across the Brillouin zone) between valence and conductionband state needs to be provided by a second quantum. A phonon can provide the necessary momentum and additionally contributes a small amount of energy ωph . There are several steps in the absorption spectrum due to various involved phonons (or combinations of them). At low temperature (T = 1.6 K, Fig. 9.10) phonons can only be generated and the absorption starts at energies above the band gap. At higher temperatures (typically above 40 K [733], Fig. 9.10), acoustical phonons assisting the optical absorption transition can also be absorbed from the crystal; in this case due to energy conservation the absorption starts already at an energy E g − ωph below the band gap. At even higher temperatures (>200 K, Fig. 9.10), also optical phonons can be absorbed. The perturbation calculation yields an absorption coefficient with a quadratic dependence on energy (9.35a) [734]. Essentially, for the absorption into a specific (empty) conduction band state (with squareroot density of states) various initial (filled) valence band states (also with squareroot density of states) are possible, making the probability depend on the product of the DOS and thus on the energy to the first power. Integrating over all energy states with energy separation E ± ωph , yields an E 2 dependence.5 Considering the temperature dependent population of 5A
flat optical phonon dispersion is assumed.
9.6 Band–Band Transitions
305
Absorption coefficient
(cm1/2)
8
GaP
296K 77K
LA e
6
TA e
TOe
1.6K
4 216K TA a 2
77K
EgX
LA a TOa
TAe
(LO+TA)a 0 2.15
2.18
LAa 2.21
LAe
2.24
2.27
TAa
2.30
2.33
2.36
2.39
2.42
Energy (eV)
√ Fig. 9.10 Absorption edge of GaP ( α vs. E) at various temperatures. The index ‘e’ (‘a’) indicates phonon emission (absorption) during the optical absorption process. The theoretical excitonic gap (E gX ) at T = 77 K is indicated. Adapted from [733]
the phonon density of states (Bose statistics, (E.3)) the absorption coefficients for transitions with phonon emission (αe ) and phonon absorption (αa ) are: αe (E) ∝
(E − (E g + ωph ))2 1 − exp(−ωph /kT )
(9.35a)
αa (E) ∝
(E − (E g − ωph ))2 . exp(ωph /kT ) − 1
(9.35b)
The twoparticle process is less probable than the direct absorption that only involves one photon. The strength of indirect absorption close to the band gap is about 10−3 smaller than for the direct transition. An 11parameter formula based on terms like (9.35a) can describe the room temperature absorption spectrum of silicon in the visible with a precision of a few percent [735]. The absorption spectra close to the absorption edge √ are shown for GaP (Fig. 9.10) and Si (Fig. 9.11a). According to (9.35a), the plot of α versus energy (Macfarlane– Roberts plot [736]) yields a straight line beyond the spectral region of phonon effects. The complicated form close to the (indirect) gap energy is due to the contribution of different phonons. The phonon energies found to contribute to the silicon absorption edge [737] agree with the TA and TO energy at the X minimum [738] (Fig. 9.11b). Also multiple phonons can contribute (Fig. 9.10). The momentum conservation can also be achieved by impurity scattering or electronelectron scattering [739]. We note also that the indirect semiconductors have an optical transition between Γ valence and conductionband states. However, this transition is at higher energies than the fundamental band gap, e.g. for Si (E g = 1.12 eV) at 3.4 eV (see Fig. 6.6a). In
306
9 Optical Properties
(a)
(b)
Fig. 9.11 (a) Absorption edge of Si at two different temperatures. Adapted from [737]. (b) Phonon energies in silicon along [001] obtained from neutron scattering (black unidentified, green TA, purple LA, blue LO, red TO). The vertical grey bar indicates the position of the conduction band minimum, the horizontal grey bars the energies of the phonons observed at the indirect optical absorption edge. The dark grey overlap areas indicate that TO and TA phonons contribute. Adapted from [738]
(a) E
(b) 1
104 10
3
10
2
10
1
10
0
10
1
10
2
Ge
7
L6
k 8
L
0.76 0.78 0.80 0.82 0.84 0.86 0.88 0.90
Fig. 9.12 (a) Scheme of indirect and direct optical transitions starting at the top of the valence band in Ge. Vertical solid lines represent the involved photon, the horizontal dashed line the involved phonon. (b) Experimental absorption spectrum of Ge (T = 20 K). Adapted from [737]
Fig. 9.12, the absorption scheme for indirect and direct absorbtion processes starting with an electron at the top of the valence band is shown together with an experimental absorption spectrum for Ge with the direct transition (Γ8 → Γ7 ) at 0.89 eV, 0.136 eV above the fundamental band gap. In Fig. 9.13, the absorption edge of BaTiO3 is shown. An indirect transition with an increase of (weak) absorption ∝ E 2 and an indirect gap of E i = 2.66 eV and a
9.6 Band–Band Transitions
307
1/2
k2
k
4
10
15
15
10
10
5
5
0 2.5
2.75
3.0
3.25
0 3.0
3.05
3.1
3.15
Fig. 9.13 Absorption of BaTiO3 at room temperature. Experimental data (circles) from [740] with fits (dashed lines) ∝ E 2 and ∝ E 1/2 , respectively
direct transition with an increase of (strong) absorption ∝ E 1/2 and a direct gap of E d = 3.05 eV are observed. These transitions could be due to holes at the M (indirect gap) and Γ (direct gap) points (cf. Sect. 6.3.11), respectively.
9.6.4 Urbach Tail Instead of the ideal (E − E g )1/2 dependence of the direct bandedge absorption, often an exponential tail is observed (see Fig. 9.14). This tail is called the Urbach tail [741] and follows the functional dependence (for E < E g ) α(E) ∝ exp
E − Eg E0
,
(9.36)
where E 0 is the characteristic width of the absorption edge, the socalled Urbach parameter. The Urbach tail is attributed to transitions between band tails below the band edges. Such tails can originate from disorder of the perfect crystal, e.g. from defects or doping, and the fluctuation of electronic energy bands due to lattice vibrations. The temperature dependence of the Urbach parameter E 0 is thus related to that of the band gap as discussed in [742, 743].
308
9 Optical Properties
(b)
(a) 10 4 1
GaAs 15
10 3
10 2 10 10
1
GaAs 10 0 1.3
1.4
1.5
1.6
1.7
5 0
500
1000
Fig. 9.14 (a) Experimental absorption spectrum (circles) of GaAs at room temperature on a semilogarithmic plot. The exponential tail below the band gap is called the Urbach tail (the dashdotted line corresponds to E 0 = 10.3 meV in (9.36)). The dashed line is the theoretical dependence from (9.33). Adapted from [744]. (b) Temperature dependence of Urbach parameter E 0 for two GaAs samples. Experimental data for undoped (solid circles) and Sidoped (n = 2 × 1018 cm−3 , empty circles) GaAs and theoretical fits (solid lines) with onephonon model. Adapted from [742]
9.6.5 Amorphous Semiconductors The sharp features in the dielectric function due to critical points in the band structure of crystalline semiconductors are washed out in amorphous material. As an example the spectra of the imaginary part of the dielectric function for crystalline (trigonal) and amorphous selenium are shown in Fig. 9.15.
Fig. 9.15 Imaginary part of the dielectric function of amorphous (solid line) and crystalline (trigonal) selenium (dashdotted lines for two different polarization directions). From [745]
Se
20
trigonal
2nk
15 Ec
10
5
amorphous 0
2
4
6
8
10
9.6 Band–Band Transitions
309
9.6.6 Excitons An electron in the conduction band and a hole in the valence band form a hydrogenlike state due to the mutual Coulomb interaction. Such a state is called an exciton. 2 K2 , where The centerofmass motion is separated and has a dispersion E = 2M M = m e + m h is the total mass and K is the centerofmass momentum K = ke + kh .
(9.37)
The relative motion yields hydrogenlike quantized states E n ∝ n −2 (n ≥ 1): E Xn = −
m 0 e4 1 m ∗r 1 , m 0 2r 2(4π0 )2 n 2
(9.38)
where m ∗r denotes the reduced effective mass m ∗−1 = m ∗−1 + m ∗−1 r e h . The third factor is the atomic Rydberg energy (13.6 eV). The exciton binding energy E Xb = −E X1 is −3 scaled by (m ∗ /m 0 ) −2 r ≈ 10 . A more detailed theory of excitons beyond the simple hydrogen model presented here, taking into account the valenceband structure, can be found in [746] for direct and [747] for indirect cubic and in [748] for wurtzite semiconductors. The exciton binding energies for various semiconductors are listed in Table 9.4 and shown in Fig. 9.16a versus the band gap. The radius of the exciton is rXn = n 2
m0 r aB , m ∗r
(9.39)
where aB = 0.053 nm denotes the hydrogen Bohr radius.6 The Bohr radius of the exciton is aX = rX1 (14.6 nm for GaAs, ∼2 nm for ZnO). The exciton moves with the centerofmass Kvector through the crystal. The complete dispersion is (see Fig. 9.16b)
b , see Sect. 9.6.10) binding energies in various bulk Table 9.4 Exciton (E Xb ) and biexciton (E XX semiconductors b (meV) b /E b Material E Xb (meV) E XX E XX X
GaAs GaAs QW ZnSe GaN CdS ZnS ZnO
4.2 9.2 17 25 27 37 59
2.0 3.5 5.6 5.4 8.0 15
0.22 0.21 0.22 0.20 0.22 0.25
Values for 10 nm GaAs/15 nm Al0.3 Ga0.7 As quantum well (QW) are taken from [749]
6 Cf. (7.20); an electron bound to a donor can be considered as an exciton with an infinite hole mass.
310
9 Optical Properties
(a)
(b)
Fig. 9.16 (a) Exciton binding energy versus band gap for various semiconductors. (b) Schematic dispersion of excitonic levels. The K vector refers to the centerofmass motion
E = E g + E Xn +
2 2 K . 2M
(9.40)
The oscillator strength of the exciton states decays ∝ n −3 . The absorption due to excitons is visible in Fig. 9.8a for GaAs at low temperatures. If inhomogeneities are present, typically only the n = 1 transition is seen. However, under special conditions also higher transitions of the exciton Rydberg series are seen (e.g. n = 2 and 3 in Fig. 9.8b). The exciton concept was introduced first for absorption in Cu2 O [750]. The J = 1/2 absorption spectrum (‘yellow series’) is shown in Fig. 9.17. In this particular
(a) 1PA (a.u.)
Fig. 9.17 Onephoton (top) and twophoton (bottom) absorption spectra of Cu2 O at T = 4.2 K. Arrows denote theoretical peak positions. Adapted from [752]
Cu2O
(b)
4 green
2.030
2.035
2.14
2.15
2.16
2.17
9.6 Band–Band Transitions
311
(a)
(b)
Oscillator strength (arb. units)
Optical density
En Eg (meV)
10
Energy (eV)
1
10
4
105 10
6
10
7
10
8
2
5
n 10
20
Fig. 9.18 (One photon) Absorption spectrum of Cu2 O (thickness 34 µm) at T = 1.2 K with transitions labelled n = 2 . . . 25. Adapted from [751]
material both the valence and conduction bands have s character, thus the 1s transition of the exciton is forbidden and the np transitions are observed in normal (onephoton) absorption. With twophoton absorption also the s (and d) transitions can be excited. On a piece of natural Cu2 O, the Rydberg series has been measured up to n = 25 [751] (Fig. 9.18a). The peak energy and the oscillator strength follow the n −2 (E Xb = 92 meV, E g = 2.17208 eV) and n −3 laws, respectively, expected from a hydrogen model (Fig. 9.18b). The deviation from the n −3 dependence for the oscillator strength at large n is due to interaction effects of excitons with large radius at finite exciton density. The scattering (unbound) states of the exciton [753] for E > E g contribute to absorption above the band gap. The factor by which the absorption spectrum is changed is called the Sommerfeld factor. For bulk material it is S(η) = η
exp(η) , sinh(η)
(9.41)
1/2 with η = π E bX /(E − E g ) . The change of the absorption spectrum due to the Coulomb correlation is shown in Fig. 9.19. There is a continuous absorption between the bound and unbound states. At the band gap there is a finite absorption (S(E → E g ) → ∞). The detail to which exciton peaks can be resolved depends on the spectral broadening.
312
(a)
(c)
9 Optical Properties
(b)
(d)
Fig. 9.19 Modification of the absorption edge of a direct transition by excitonic effects for different spectral (Lorentzian) broadening (∝ (E 2 + Γ 2 /4)−1 ), (a) Γ = 0.01E Xb , (b) Γ = 0.1E Xb , (c) Γ = E Xb . (d) is (c) in linear scale. Dashed lines are electron–hole plasma absorption according to (9.33) Fig. 9.20 Theoretical dependency (lines) for the the differences of the Cline and Aline as well as Bline and Aline exciton transition energies in GaN as a function of the caxis strain. Symbols are experimental data from [754]. Adapted from [468]
100
GaN
50
E CE A
0
50 0.2
EBE A
0.1
0
0.1 zz
0.2
9.6 Band–Band Transitions
313
Table 9.5 Phonon broadening parameters (FWHM) of various bulk semiconductors Material ωLO (meV) Γ0 (meV) γAC (µeV/K) γLO (meV) GaAs ZnSe GaN ZnO
36.8 30.5 92 33
0 1.9 10 1.2
4±2 0±7 15 ± 4 32 ± 26
16.8 ± 2 84 ± 8 408 ± 30 96 ± 24
Values from fits with (9.42) to experimental data for GaAs [759], ZnSe [757], GaN [756], ZnO [760] (phonon energy fitted) as shown in Fig. 9.22b
In Fig. 9.20 the energy separations of the A, B, and Cexcitons in GaN are shown [468]. Thus, the ordering of the valence bands depends on the strain state of the semiconductor.
9.6.7 Phonon Broadening The scattering with phonons and the related dephasing leads to homogeneous broadening Γhom of absorption (and recombination) lines. Acoustic and optical phonons contribute to the broadening according to the dependence [755] Γhom (T ) = Γ0 + γAC T + γLO
1 , exp(ωLO /kT ) − 1
(9.42)
where ωLO is the optical phonon energy and the last factor is the Bose function (E.24). Γ0 is a temperatureindependent contribution, Γ0 = Γ (T = 0). The increasing broadening with increasing temperature is obvious, e.g., in absorption spectra (Fig. 9.21a). In Fig. 9.21b experimental data for GaAs, ZnSe and GaN are assembled. The data have been fitted with (9.42); the resulting phonon broadening parameters are listed in Table 9.5.7 The optical transitions in polar semiconductors exhibit stronger coupling to optical phonons. The phonon coupling parameters from different measurements on GaN are discussed and compared in [758].
9.6.8 Exciton Polariton Electrons and holes are particles with spin 1/2. Thus, the exciton can form states with total spin S = 0 (paraexciton, singlet) and S = 1 (orthoexciton, triplet). The 7 Such parameter can be directly determined from spectroscopic broadening (as in [756]) or a timeresolved measurement of the decay of the coherent polarization (fourwave mixing) as in [757]. In the latter, the decay constant of the dephasing T2 is related to the decay constant τ of the FWMsignal by T2 = 2τ for homogeneous broadening. The Fourier transform of exp −t/(2τ ) is a Lorentzian of the type ∝ ((E − E 0 )2 + Γ 2 /4)−1 with Γ = 1/τ being the FWHM.
314
9 Optical Properties
(a)
(b)
Fig. 9.21 (a) Absorption spectra of GaN bulk (0.38 µm thick epilayer on sapphire) for various temperatures T = 100, 200, 300, 350, 400, 450, and 475 K. Adapted from [756]. (b) Homogeneous broadening as a function of temperature, symbols are experimental data, solid lines are fits, rf. Table 9.5
exchange interaction leads to a splitting of these states, the singlet being the energetically higher. The singlet state splits into the longitudinal and transverse exciton with respect to the orientation of the polarization carried by the Bloch functions and the centerofmass motion K of the exciton. Dipole transitions are only possible for singlet excitons (bright excitons). The triplet excitons couple only weakly to the electromagnetic field and are thus also called dark excitons. The coupling of these states to the electromagnetic field creates new quasiparticles, the exciton polaritons [761, 762]. The dielectric function of the exciton (with background dielectric constant b ) is (ω) = b 1 +
β β ∼ b 1 + , = 1 − (ω 2 /ωX )2 1 − (ω 2 /ωT )2 + K 2 /(M ωT ) (9.43)
where β is the oscillator strength and the energy is ωX = ωT + 2 K 2 /2M. ωT is the energy of the transverse exciton at K = 0. With this dispersion the wave dispersion must be fulfilled, i.e. c2 k 2 = ω 2 (ω),
(9.44)
where k is the kvector of the light that needs to be k = K due to momentum conservation. The dependence of the dielectric function on k is called spatial dispersion [763]. Generally, up to terms in k 2 it is written as (ω) = b 1 +
β . 1 − (ω 2 /ω0 )2 + D k 2
(9.45)
9.6 Band–Band Transitions
315
The term k 2 with curvature D (for the exciton polariton D = /(M ωT )) plays a role in particular when ωT2 − ω 2 = 0. For k = 0 even a cubic material is anisotropic. The dimensionless curvature Dˆ = Dk 2 should fulfill Dˆ = /(Mc) 1 in order to make k 4 terms unimportant. For exciton polaritons8 typically Dˆ = ωT /(m c2 ) ≈ 2 × 10−5 for ωT = 1 eV and m ∗ = 0.1.
Energy
(a)
(b)
UPB
L
EX T
EX
LPB
k
Fig. 9.22 (a) Schematic dispersion of exciton polaritons. The lower polariton branch (‘LPB’) is at small k photonlike, at large k excitonlike. The upper branch (‘UPB’) is excitonlike at small k and photonlike at larger k. The limit of the UPB for k → 0 is the energy of the longitudinal exciton. The dashed lines represent the pure exciton dispersions. (b) Theoretical effect of spatial dispersion on the reflectance at the fundamental exciton resonance at normal incidence for ZnSe material parameters (ωT = 2.8 eV, β = 1.0 × 10−3 and a background dielectric constant of b = 8.1, damping was set to Γ = 10−5 ωT ). The arrow denotes the position of ωL . The solid (dashed) line is with (without) spatial dispersion for Dˆ = 0.6 × 10−5 ( Dˆ = 0). Data from [763]
From (9.44) together with (9.45) two solutions result: 2ω 2 = c2 k 2 + (1 + β + Dk 2 )ω02
1/2 ± −4c2 k 2 (1 + Dk 2 )ω02 + (c2 k 2 + (1 + β + Dk 2 )ω02 )2 .
(9.46)
The two branches are shown schematically in Fig. 9.22a. Depending on the k value they have a photonic (linear dispersion) or excitonic (quadratic dispersion) character. The anticrossing behavior at k ≈ ωT /c (for ωT = 1 eV, k ≈ 0.5 × 10−5 cm−1 ) creates a bottleneck region in the lower polariton branch. This name stems from the small emission rate of acoustic phonons (i.e. cooling) in that region, as predicted in [764] and experimentally found, e.g. in CdS [765]. The polaritons decay into a 8 The dependence of the opticalphonon energies on k is typically too small to make spatial dispersion effects important. According to (5.19) Dˆ = − (a0 ωTO /4c)2 ≈ 4 × 10−11 for typical material parameters (lattice constant a0 = 0.5 nm, TO phonon frequency ωTO = 15 THz).
316
9 Optical Properties
photon when they hit the surface. The effect of the oscillator strength of the dispersion is shown in Fig. 9.23 for twoexciton resonance. In the case of several excitons (9.45) reads n βi . (9.47) (ω) = b 1 + 1 − (ω 2 /ω0,i )2 + Di k 2 i=1
(b)
(c)
3
3
3
2
2
2
1
1
1
Energy
(a)
0
0
1
2
3
4
5
0
0
1
2
k
3
k
4
5
0
0
1
2
3
4
5
k
Fig. 9.23 Schematic polariton dispersion for a twoexciton resonance (curvature of exciton dispersion greatly exaggerated, Dˆ = 10−2 ) at ωT,1 = 1 and ωT,2 = 1.5 for three different oscillator strengths (a) f = 10−3 , (b) f = 10−2 , (c) f = 10−1 . The dashed lines in (c) represent the pure exciton dispersions
For k = 0 either ω = 0 (lower polariton branch) or (ωL ) = 0. For the latter we find from (9.45) (9.48) ωL = 1 + β ωT . Therefore, the energy splitting ΔE LT , mostly denoted as ΔLT , between the L and Texciton energy given by ΔE LT = (ωL − ωT ) =
1 1 + β − 1 ωT ≈ β ωT 2
(9.49)
is proportional to the exciton oscillator strength (for experimental values see Table 9.6). We note that if (D.9) is used for the dielectric function, β in (9.49) needs to be replaced by β/b . The effect of spatial dispersion on the reflection at the fundamental exciton resonance is depicted in Fig. 9.22b. For nonnormal incidence an additional feature due to the longitudinal wave is observed for ppolarization [763]. For a detailed discussion additional effects due to anisotropy in wurtzite crystals, an exciton free layer at the semiconductor surface, additional boundary conditions and damping need to
9.6 Band–Band Transitions
317
Table 9.6 Exciton energy (low temperature), LT splitting and exciton polariton oscillator strength for various semiconductors CdS A CdS B ZnO A ZnO B ZnSe GaN A GaN B GaAs ωT ΔLT β
(eV) (meV) (10−3 )
2.5528 2.2 1.7
2.5681 1.4 1.1
3.3776 1.45 0.9
3.3856 5 3.0
2.8019 1.45 1.0
3.4771 1.06 0.6
3.4816 0.94 0.5
1.5153 0.08 0.11
Values for ZnO from [766], values for GaAs from [767], all other values from [768]
(a)
(b) 3.395
ZnO
Ec BL
GaN
5
3.390
BT B
5
6
3.380
AL
5
AT
5
3.375
A
1,2
0
10 5
20 1
0
5
10 5
15
1
Fig. 9.24 (a) Exciton polariton dispersion (k ⊥ c) of ZnO with experimental data (T = 1.8 K). Solid (dotted) lines are for polaritons with E c (E ⊥ c). The dashed lines refer to excitons. Adapted from [771]. (b) Exciton polariton dispersion (T = 2 K) in GaN (on sapphire) for E ⊥ c. Adapted from [772]
be considered [769, 770]. The polariton dispersions of ZnO and GaN are shown in Fig. 9.24.
9.6.9 BoundExciton Absorption Excitons can localize at impurities or inhomogeneities. Such excitons are called bound excitons. Here, the absorption due to such complexes is discussed. The recombination is discussed in Sect. 10.3.2. In GaP:N excitons are bound to isoelectronic
318
9 Optical Properties
Transmission
(a)
n=
12
3
4
5 67 8
NN1' NN1
NN2 NN3 BA
GaP:N
(b)
Fig. 9.25 (a) Transmission spectrum of GaP:N with a nitrogen concentration of about 1019 cm−3 at 1.6 K (thickness: 1.1 mm). n is indicated for the first eight transitions due to excitons bound to nitrogen pairs. NNn ’ indicate phonon replica. The ‘A’ line denotes the position of the transition due to excitons bound to a single nitrogen atom (observable for samples with low N doping). The ‘B’ line is forbidden and due to the J = 2 exciton. Adapted from [616]. (b) Absorption spectra of Ndoped (NN = 7 × 1018 cm−3 ) and intrinsic GaP (T = 2 K). Adapted from [612]
N impurities (substituting P), resulting in the ‘A’ line at 2.3171 eV (at T = 4.2 K).9 The absorption due to A excitons is well resolved in the spectrum of Fig. 9.25b. At sufficiently high nitrogen doping, there exist nitrogen pairs, i.e. a complex where a nitrogen impurity has a second nitrogen impurity in the vicinity. The pairs are labeled NNn . It was believed that the second nitrogen atom is in the nth shell around the first one. However, the proper level asignment is probably different in the view of modern theory [472]. Also clusters with more than two nitrogen atoms may exist. NN1 is a prominent level and relates to a N–Ga–N complex having 12 equivalent sites for the second N atom on the next neighbor anion site. The transitions due to excitons bound to NNn , as shown in Fig. 9.25a, give a series of lines (see Table 9.7) that fulfill limn→∞ NNn = A. Although GaP has an indirect band structure, the absorption coefficient of Nrelated transitions is large, about 105 cm−1 for a nitrogen doping 9 The A line is due to excitons with J = 1, resulting of coupling of the electron spin 1/2 with the hole angular momentum of 3/2. The Bline is a dipole forbidden line due to ‘dark’ excitons with J = 2.
9.6 Band–Band Transitions
319
Table 9.7 Index of nitrogen pairs NNn and energy separation ΔE of boundexciton transitions from the freeexciton line for n = 1 . . . 10 and the ‘A’ line n 1 2 3 4 5 6 7 8 9 10 ∞ (A) ΔE 143 (meV)
138
64
39
31
25
22
20
18
17
11
level of 1019 cm−3 .10 This is due to the fact that the electron spatially localized at the nitrogen isoelectronic trap (Sect. 7.7.9) has a sizeable k = 0component of its wavefunction (Fig. 7.41), leading to a large transition probability for Γ point holes with an oscillator strength of 0.09 [773].
9.6.10 Biexcitons Similar to two hydrogen atoms forming a hydrogen molecule, two excitons can also form a bound complex, the biexciton involving two electrons and two holes. The biexciton binding energy is defined as b = 2 E X − E XX . E XX
(9.50)
Biexcitons are binding in bulk material. Accordingly, the biexciton recombination or absorption occurs at lower energy than that of the exciton. Values of the biexciton binding energy are listed in Table 9.4 for various semiconductors. The ratio of biexciton and exciton binding energies is fairly constant about 0.2. In semiconductors with small exciton binding energy, such as GaAs, biexcitons are hard to observe in bulk material but show up in heterostructures that provide additional carrier confinement (see also Sect. 14.3.4). While the exciton density increases linearly with external excitation, the density of biexcitons increases quadratically.
9.6.11 Trions The complexes ‘eeh’ and ‘ehh’ are called trions. Also, the notation X− and X+ is common. X− is typically stable in bulk material but hard to observe. In quantum wells or dots, trions are easier to observe. In quantum dots excitons with higher charge, e.g. X2− , have also been observed (see Fig. 14.34).
10 Also
the recombination (Sect. 10.3.2) is efficient and allows green GaP:N and yellow GaAsP:N light emitting diodes.
320
9 Optical Properties
9.6.12 Band Gap Renormalization The band structure theory has been developed so far for small carrier densities. If the carrier density is large the interaction of free carriers has to be considered. The first step was exciton formation. However, at high temperatures (ionization) and at large carrier density (screening) the exciton is not stable. Exchange and correlation energy leads to a decrease of the optical absorption edge that is called band gap renormalization (BGR). An effect due to significant carrier density is to be expected when the density is of the order of the exciton volume, i.e. n ∼ aB−3 . For aB ∼ 15 nm (GaAs) this means n ∼ 3 × 1017 cm−3 . The dimensionless radius rs is defined via 4π 3 1 . rs = 3 n aB3
(9.51)
The sum of exchange and correlation energies E xc is found to be mostly independent of material parameters [774] (Fig. 9.26a) and follows the form E xc =
(a)
a + b rs , c + d rs + rs2
(b)
0
(9.52)
0
E xc (Ry)
1 Ge Si
2
5 3 CdS CdSe CdTe ZnO
4
10 0
5 1
rs
2
3
0
1
2
3
4
5
rs
Fig. 9.26 (a) Theoretical exchange and correlation energies in units of the exciton Rydberg energy as a function of the dimensionless variable rs for Ge, Si and a model system (with one isotropic conduction and valence band each). The solid line is a fit according to (9.52). Adapted from [774]. (b) Band gap renormalization in terms of the excitonic Rydberg for various II–VI semiconductors. Solid line is the relation according to (9.52), dashed line is the dependence predicted in [775] for T = 30 K. Data are compiled in [776]
9.6 Band–Band Transitions
1
1.2
5
Fig. 9.27 Absorption of GaAs (low temperature, T = 10 K) as a function of the electron–hole density n (theory). Adapted from [777]
321
GaAs
1.0 0.8 0.6
n=0 15 3 n=5 10 cm 16 3 n=3 10 cm 3 16 n=8 10 cm
0.4 0.2 0.0 0.2 1.490
1.495
1.500
with a = −4.8316, b = −5.0879, c = 0.0152 and d = 3.0426. Thus the density dependence of the band gap at small carrier density is ∝ n 1/3 . Experimental data for a number of II–VI semiconductors roughly follow such a dependence (Fig. 9.26b). In Fig. 9.27, a theoretical calculation of the absorption spectrum of bulk GaAs for various carrier densities (n = p) [777] is shown. With increasing density, the excitonic resonance broadens and vanishes. The shape approaches the electron–hole plasma shape. The absorption edge shifts to smaller energies. At high carrier density, the absorption becomes negative in a spectral range before absorption sets in. In this spectral region, the material exhibits gain and an incoming light wave is amplified (cmp. Sect. 10.2.6).
9.6.13 Electron–Hole Droplets At low temperature and high density, electron–hole pairs in Ge and Si can undergo a phase transition into a liquid state. This electron–hole liquid (EHL) was suggested in [778] and is a Fermi liquid exhibiting the high conductivity of a metal and the surface and density of a liquid. The condensation is due to exchange interaction and correlation. The formation is fostered by the band structure of Ge [779] and the long lifetime of carriers in the indirect band structure. In unstressed Ge typically a cloud of electron–hole droplets with diameter in the µm range exists. The phase diagram is shown in Fig. 9.28a. In suitably stressed Ge electron–hole droplets with several hundred µm diameter form around the point of maximum shear strain in inhomogeneously strained crystals, as shown in Fig. 9.28b. The pair density in such a liquid is of the order of 1017 cm−3 . We note that the metallic EHL state hinders observation of the Bose–Einstein condensation (BEC) of (bosonic) excitons. The lightexciton mass offers a high
322
9 Optical Properties
(a)
(b) screw
Ge
exp c
7
EHG
exp
Tc
sp
6
EHL
T (K)
5 4 3
EHL
2
EHL
1 0
0
0.5
1.0
1.5 17
2.0
2.5
3
(10 cm )
Fig. 9.28 (a) Temperature–density phase diagram of electrons and holes in Ge. The regions of electron–hole gas (EHG) and liquid (EHL) and the droplet phase are labeled. Solid line is theoretical calculation, symbols are experimental data from [780]. The dashdotted line denoted ρsp is the experimentally obtained temperature dependence of the liquid density due to singleparticle exp exp excitations. ρc and Tc denote the experimental critical density and temperature, respectively. Adapted from [781]. (b) Photographic image of radiative recombination (at 1.75 µm wavelength) from a 300µm diameter droplet of electron–hole liquid (EHL) in a stressed (001) Ge disk (diameter 4 mm, thickness 1.8 mm) at T = 2 K. The stress is applied from the top by a nylon screw along a 110 direction. Adapted from [782], reprinted with permission, © 1977 APS
condensation temperature in the 1 K range (compared to the mK range for atoms). Recent experiments with spatially indirect excitons in coupled quantum wells lead towards BEC [783, 784]. A sufficiently long lifetime ensures cooling of the excitons close to the lattice temperature. Another potential candidate for BEC are longliving excitons (msrange) in Cu2 O [785]. The condensation of polaritons (cf. Sect. 9.6.8) in microcavities to welldefined regions of kspace has been discussed in [786] and compared to bosonic condensation in bulk.
9.6.14 TwoPhoton Absorption So far, only absorption processes that involve one photon have been considered. The attenuation of the intensity I of a light beam (of frequency ω0 ) along the z direction can be written as dI (9.53) = −α I − β I 2 , dz
9.6 Band–Band Transitions
323
Fig. 9.29 Experimental twophoton absorption spectrum of GaAs (T = 4 K) (dots) plotted as a function of the difference of the doublephoton energy 2ω from the GaAs band edge E g . The solid line is a theoretical calculation, the dashed lines represent slopes with exponent 1/2 and 3/2, respectively. Adapted from [789]
GaAs 10
22
1/2
10
21
g
3/2
T
g
10
20
19
10
3
10
2
1
10
10
1
g
where α is due to the (linear) absorption coefficient (and possibly scattering) and β is the twophoton absorption coefficient. A twophoton process can occur in two steps, e.g. via a midgap level, which is not considered any further here. Here, we consider twophoton absorption (TPA) via the population of a state at 2ω0 higher energy than the initial state with a nonlinear optical process. The TPA coefficient is related to the nonlinear thirdorder electric dipole susceptibility tensor [787] χi jkl . Within the twoband approximation theory predicts [788] 3/2 . β ∝ 2 ω0 − E g
(9.54)
The exponent 3/2 is indeed found experimentally, as shown in Fig. 9.29 for GaAs. The strength of absorption depends on the relative orientation of the light polarization with respect to the main crystallographic directions, e.g. TPA for polarization along 110 is about 20 % larger than for the 100 orientation.
9.7 Impurity Absorption 9.7.1 Shallow Levels For charge carriers bound to shallow impurities long range Coulomb forces are most important and they exhibit a hydrogenlike term scheme En =
m∗ 1 1 × 13.6 eV, m 0 2r n 2
(9.55)
324
9 Optical Properties
(a)
5p0 4p±
0
±
3p± 4p0 3p0 2p±
(b)
...
2p0
h
ph
4p 3p
11.62
1s(E) 1s(T1)
1.33
2p
44.09 43.25 42.41 42.25 40.07 39.14 34.08
45.31
1s(A1)
h 1s
Fig. 9.30 (a) Term scheme of phosphorus donor in silicon, all energies in meV. After [791]. (b) Schematic sequence for photothermal ionization, here absorption of a photon with ω = E 3p − E 1s and subsequent absorption of a phonon with energy ωph ≥ E ∞ − E 3p
with the ionization limit E ∞ being the conduction (valence) band edge for donors (acceptors), respectively. They can be excited by light to the nearest band edge. Such absorption is typically in the FIR region and can be used for photodetectors in this wavelength regime. The optical absorption cross section of impurity absorption can be related to the carrier capture cross section [513, 514]. The actual transition energies can deviate from (9.55) due to deviation of the potential close to the impurity from the pure Coulomb potential. Such an effect is known as the chemical shift or central cell correction (cf. Sect. 7.5.5) and is characteristic of the particular impurity. In GaAs such shifts are small (∼100 µeV) [790]. The term scheme for P in Si is shown in Fig. 9.30a. The ground state (1s) is split because of a reduction of the tetrahedral symmetry due to intervalley coupling. The anisotropic mass at the Xvalley in Si causes the p states (and states with higher orbital momentum) to split into p0 and p± states. Such an effect is absent in a direct semiconductor with an isotropic conductionband minimum such as GaAs (Fig. 9.31). Optical transitions between the 1s and various p states can be directly observed in absorption, e.g. for Si:P in [792]. These transitions are also observed in photoconductivity because the missing energy to the ionization into the continuum is supplied by a phonon at finite temperature (photothermal ionization) (Fig. 9.30b) [791]. The
9.7 Impurity Absorption
(a)
325
5
4
6
(b)
7
Si 2p
GaAs
GaAs
1s3p0
2p0 Sn Pb 2p
illuminated
ED 3p 4p
0T
2s
1.9T 30
1s3p
2p
dark
3p 3p0
40
50 1
48
60
50
52 1
)
54
)
Fig. 9.31 (a) Farinfrared photoconductivity response (Lymantype s→p series) of not intentionally doped GaAs with residual donors Pb, Sn, and Si, NA = 2.6×1013 cm−3 , ND − NA = 8×1012 cm−3 . The upper (lower) curve is for a magnetic field of 0 (1.9) T. Measurement temperature is 4.2 K. (b) Photoconductive response of a (different) GaAs sample with the same impurities (ND = 1 × 1013 cm−3 ) with (upper curve) and without (lower curve) illumination with abovebandgap light (B = 1.9 T, T = 4.2 K). Adapted from [793] b
ED
1
GaAs:Te
500 3
ND (cm ) 2.1 1.0 6.7 1.0
0 0
50
16
10 1014 1015 1015
100 1
Fig. 9.32 Lowtemperature (T = 1.35 K) absorption spectra of highly doped ntype GaAs:Te with doping concentrations as labeled (circles ND = 2.1 × 1016 cm−3 , stars 6.7 × 1014 , triangles 1.0 × 1015 ). A sharp photoconductivity spectrum (in arbitrary units) from lowdoped GaAs:Te (crosses, ND = 1.0 × 1014 cm−3 ) is shown for comparison (cf. Fig. 9.31a). The energy of the 1s→2p transition and the donor binding energy (onset of continuum absorption) are indicated. Adapted from [794]
splitting of the 2p transition in Fig. 9.31a is the chemical shift due to different donors incorporated in the GaAs (Si, Sn, and Pb). Peak broadening is mostly due to Stark broadening due to neighboring charged impurities. The application of a magnetic field induces Zeemanlike splittings and increases the sharpness of the peaks. The peak width can be further increased by illuminating the sample with light having a
326
9 Optical Properties
higher energy than the band gap. The additional charge carriers neutralize charged impurities and allow higher resolution (Fig. 9.31b). In Fig. 9.32 absorption spectra of highly doped ntype GaAs are shown. For doping concentrations larger than the critical concentration of ∼1×1016 cm−3 (cf. Table 7.6) significant broadening is observed due to the formation of an impurity band.
9.7.2 Deep Levels The absorption of deep levels is typically in the infrared. In Fig. 9.33a the possible optical absorption processes involving the Fe levels in InP (cf. Sect. 7.7.8) during the charge transfer Fe3+ → Fe2+ are shown. These transitions and their fine structure (Fig. 9.33b) have been observed in calorimetric absorption spectroscopy (CAS) experiments [604]. In Fig. 9.34 the photoconductivity of is shown. The sharp peaks are due to transitions of interstitial, singly ionized Mg, Mg+ i [795]. Mg in Si is a double donor [575] (see Sect. 7.7.2). Above the ionization limit of about 256 meV, the peaks are replicated, shifted by the LO phonon energy of 59.1 meV. However, now they rather appear as dips. This behavior is typical for a discrete state interacting with a continuum, also called Fano resonance [796, 797] with its characteristic lineshape, going below the continuum level. The absorption spectra due to various deep acceptors in GaAs are compared in Fig. 9.35. The density of states in the band increases with k (proportional to √ E − E c ). The carrier on the impurity is strongly localized and described with a wave packet centered around Γ , its kcomponents decreasing with increasing k. Thus the maximum absorption will be at an intermediate kvalue and an associ
(a)
(b) EC
1.34 5
InP:Fe
T2
1.14
5
0.78
E
InP:Fe
TA
VB
0.25 0 Fe
3+
Fe
2+
EV
5
E
0.77 0.78
VB 5 T 2
1.14
1.15
Fig. 9.33 (a) Schematic band diagram of InP with levels of Fe impurities in the 3+ and 2+ charge states at low temperature. All energies are given in eV. The arrows denote the optical transition of a valenceband electron to the Fe center, Fe3+ + ω → Fe2+ + h. (b) Calorimetric absorption spectra (at T = 1.3 K) of InP:Fe, [Fe] = 5 × 1016 cm−3 . Part (b) adapted from [604]
9.7 Impurity Absorption
327
Fig. 9.34 Photocurrent spectrum of Si:Mg. Transitions are due to Mg+ i from its 1s state to excited states as labeled and indicated by vertical lines. CB denotes the conduction band edge (ionization limit). Above the CB edge (shaded area) phononassisted absorption occurs (Fano resonances). For comparison the absorption spectrum below CB is shown shifted by the phonon energy (dashed line). Above the plot, the transition mechanisms (photothermal ionization and Fano resonance) are schematically shown. Adapted from [795]
GaAs 2 2
Mn
17
Ag 1
Cu
Au
0.8 i
Fig. 9.35 Absorption spectra (σ = α/ p) due to various deep impurities in GaAs as labeled. The dashed line is a theoretical lineshape assuming a hole bound to a δpotential. The energy axis is scaled by the ionization energy. The kink for Mn at 3.5 E i ≈ 450 meV is due to the onset of absorption into the splitoff valence band. Adapted from [279]
0.6
0.4 1
2
3
4 i
328
9 Optical Properties
ated energy larger than the ionization energy E i (lowest transition to continuum at for k = 0). The lineshapes in Fig. 9.35 fit to a model with a δpotential (zero range model, neglecting long range Coulomb terms) [798] with maximum absorption close to 2 E i , 1/2 E (E − E i )3/2 α(E) ∝ i . (9.56) E3
9.8 Absorption in the Presence of Free Charge Carriers In the presence of charge carriers, various absorption processes can occur. First, the dissipative motion of carriers leads to infrared absorption, termed the free carrier absorption (Sect. 9.8.1). Filling of a band with carriers leads to a shift of the bandband absorption edge, the Burstein–Moss shift (Sect. 9.8.2). Besides the freecarrier absorption, free carriers present in the semiconductor can lead to further absorption processes with transition energies below the band gap. These processes are due to transitions within the band structure and can be • intervalence band transitions of holes (Sect. 9.8.3), • phononassisted intervalley transitions of electrons (Sect. 9.8.4), • phononassisted intraband transitions of electrons (Sect. 9.8.5).
9.8.1 FreeCarrier Absorption The absorption due to free carriers in the infrared spectral range (away from phonon resonances) can be described with the Drude model [799]. A timedependent electric field accelerates the charge carriers within a band. The excess energy is subsequently transferred to the lattice via scattering with phonons. A review of the effect of free carriers on optical properties can be found in [800]. In the relaxationtime approximation energy is relaxed with a time constant τ . Thus energy is absorbed from the electromagnetic wave and dissipated. Effectively, this process represents an intraband excitation. The complex conductivity (8.36) is given by σ ∗ = σr + iσi =
n e2 τ m∗
ωτ 1 +i 1 + ω2 τ 2 1 + ω2 τ 2
.
(9.57)
We note that a static magnetic field introduces birefringence as discussed in more detail in Sect. 13.2.2. The wave equation for the electric field is ¨ + σ ∗ μ0 E. ˙ ∇ 2 E = r 0 μ0 E
(9.58)
9.8 Absorption in the Presence of Free Charge Carriers
329
For a plane wave ∝ exp [i(kr − ωt)] the wavevector obeys ω k= c
r + i
σ∗ , 0 ω
(9.59)
where c = (0 μ0 )−1/2 is the velocity of light in vacuum, r is the background dielectric constant (for large ω). The part FC of the dielectric function due to free carriers is FC =
i σ∗ . 0 ω
(9.60)
The complex index of refraction is n∗ = nr + i κ =
σ∗ r + i . 0 ω
(9.61)
Taking the square of this equation yields τ2 σi n e2 = r − 0 ω 0 m ∗ 1 + ω 2 τ 2 2 τ σr ne . = 2 nr κ = ∗ 0 ω 0 ω m 1 + ω 2 τ 2
n 2r − κ2 = r + i
(9.62a) (9.62b)
The absorption coefficient is related to κ by (9.9). For the case of higher frequencies, i.e. ωτ 1, the absorption is α=
n e2 1 . 0 c n r m ∗ τ ω 2
(9.63)
The absorption decreases with increasing frequency like ω −r . The classical Drude treatment as followed here results in an exponent of r = 2. This is the case for neutral impurity scattering and also for small frequencies ω E F . A more detailed discussion of the energy dependence of freecarrier absorption can be found in [801]. Other exponents have been derived for scattering by acoustical phonons (r = 3/2), LO phonons (r = 5/2) and ionized impurities (r = 7/2). More detailed quantum mechanical treatments of freecarrier absorption in the presence of impurities and phonons can be found in [802, 803]. For semiconductors freecarrier absorption is particularly important in the midand farinfrared regions when carriers are present due to doping or thermal excitation. In Fig. 9.36a absorption spectra of ntype Ge for various doping concentrations are shown. The absorption coefficient in the transparency regime varies proportionally to λ2 ∝ ω −2 as predicted in (9.63). In Fig. 9.36a, the absorption can be seen to rise for photon energy above 0.7 eV due to absorption in the band structure. Electrons are
330
9 Optical Properties
excited from the valence band across the fundamental band gap into the conduction band (cmp. Sect. 9.6.3), which is an indirect transition in Ge. In Fig. 9.36b the absorption coefficient due to free carrier absorption at fixed wavelength is shown as a function of dopant concentration.11 The slope is slightly overlinear, indicating a weak dependence τ (n). A sublinear relation has been found for heavily pdoped GaAs [804]. The index of refraction is given by (also for ωτ 1) n 2r
ω 2 ne2 2r ωp 4 1 p 2 = r − + κ = 1 − + r 0 m ∗ ω 2 ω 4n 2r ω ω2 τ 2 ω 2 p ≈ r 1 − , ω
(9.64)
where ωp =
n e2 r 0 m ∗
(9.65)
(a)
(b)
Fig. 9.36 (a) Optical absorption spectra (at T = 4.2 K) of ntype Ge for various As dopant concentrations as labeled. The arrow denotes the band edge of undoped Ge, the vertical dashed line the energy for which the freecarrier absorption is measured in part (b). The inclined dashed line visualizes the slope ∝ λ2 . Curved dashed lines are guides to the eye. Adapted from [739]. (b) Freecarrier absorption at λ = 2.4 µm as determined from part (a) of the figure (blue squares) as a function of As dopant concentration. Additionally data at 300 K (red circles) from the same samples are included [739]. The dashed lines visualizes the slope ∝ ND1.25 11 Even
at low temperature, n ≈ ND since ND Nc (cf. [515] and Sect. 7.5.7).
9.8 Absorption in the Presence of Free Charge Carriers
(a)
331
(b) 2
1
0 1 1
0
2 0
1
/
0
2
1
2
k
p
Fig. 9.37 (a) Dielectric constant for plasmon oscillations. Shaded area represents region of attenuation (negative ). (b) Dispersion relation (k in units of ωp /c, ω in units of ωp ) in the presence of free carriers (9.67, for r = 1). Shaded area represents forbidden frequency range for propagating solutions. Dashed line is photon dispersion ω = ck Fig. 9.38 Plasma wavelength λp for ntype GaAs with various electron concentrations due to different doping levels. Filled circles: experimental values, dashed line: n −1/2 dependence; the deviation is due to nonparabolicity of the electron mass (cf. Fig. 9.50b). Data from [805]
is the plasma frequency. The approximation is valid for small absorption and when (ωτ )−2 can be neglected. A graphical representation is given in Fig. 9.37a. For coupling to electromagnetic waves (still ωτ 1) (ω) = r 1 −
ω 2 p
ω
=
c2 k 2 ω2
(9.66)
must be fulfilled. It follows that the dispersion relation in the presence of free carriers (Fig. 9.37b) is c2 k 2 . (9.67) ω 2 = ωp2 + r
332
9 Optical Properties
Fig. 9.39 Czochralskigrown Ga2 O3 crystals with different electron concentration, courtesy of Z. Galazka, IKZ Berlin
n 1016 cm3
18
n 10 cm
3
Ga2O3
For ω > ωp , > 0, thus waves can propagate. For ω < ωp , however, the dielectric constant is negative, i.e. < 0. For such frequencies waves are exponentially damped and cannot propagate or penetrate a layer. This effect can be used in a plasmon waveguide. The expected dependence of the plasmon wavelength on the carrier density λp = 2πc/ωp ∝ n −1/2 is depicted in Fig. 9.38 for GaAs. For semiconductors the plasmon frequency is in the midor farinfrared spectral region.12 The effect of freecarrier absorption is visualized in Fig. 9.39. The blue hue of the boule with the higher electron concentration is due to free carrier absorption in the long wavelength part of the visible spectrum.
9.8.2 Burstein–Moss Shift In the discussion so far it has been assumed that all target states in the conduction band are empty. In the presence of free carriers the absorption is modified by the • change of the distribution function • manybody effects (band gap renormalization) The latter is discussed in the next section. For a degenerate electron distribution all states close to the conductionband edge are populated. Thus a transition from the valence band cannot take place into such states. This shift of the absorption edge to higher energies is called the Burstein–Moss shift [806, 807]. Originally, the Burstein–Moss shift was evoked to explain the absorption shift in InSb with varying carrier concentration (Fig. 9.40). kconserving optical transitions between parabolic hole and electron bands have the dependence 2 k 2 2 k 2 2 k 2 + = E + , (9.68) E = Eg + g ∗ 2 m ∗e 2 mh 2 mr 12 The much higher freeelectron density in metals shifts the plasma frequency to the UV, explaining
the reflectivity of metals in the visible and their UV transparency.
9.8 Absorption in the Presence of Free Charge Carriers Fig. 9.40 Burstein–Moss effect at InSb (E g = 0.18 eV) at room temperature. Theoretical dependence and data points for intrinsic InSb and 5 × 1018 cm−3 ntype. Data from [806]
333
InSb
1
1.0 0.8
1.5
0.6
2
0.4
3 4 7
0.2
Eg
gap
1017
1018
1019 3
Fig. 9.41 Principle of Burstein–Moss shift. Left panel: Schematic band structure with completely filled electron states shown in grey. The kvector for the lowest photon energy optical absorption process is ˆ Right panel: indicated as k. Electron distribution function for a degenerate electron gas with Fermi level in the conduction band
E
E
EF EF 4kT EC
EV
k
fe
k
where m r is the reduced mass of electron and hole. About 4kT below the Fermi level all levels in the conduction band are populated (Fig. 9.41). Thus the k value at which the absorption starts is given as kˆ =
2 mr (E F − E C − 4kT ). 2
(9.69)
Besides the energy shift in the conduction band, the corresponding energy shift in the valence band k 2 /(2m h ) must be considered. Thus, the Burstein–Moss shift of the absorption edge is me . (9.70) ΔE = ω − E g = (E F − 4kT − E C ) 1 + mh
334 Fig. 9.42 Burstein–Moss effect for CdO. The linear fit is for E g = 2.22(8) eV and m r = 0.113(11) m e . The dashed lines indicate the confidence interval of ±0.08 eV. Adapted from [808]
9 Optical Properties 20
3
3.5
CdO 3.0
2.5
2.0 n2/3 (1013 cm2 )
The relation between n and the Fermi level is given by (7.6). If E F − E C kT −EC 3/2 . Using (7.8) for NC , the the Fermi integral can be approximated by √2π 23 EFkT Burstein–Moss shift can be written for this case as 2 2/3 me h 2 2/3 3 2/3 h ΔE = n n . (9.71) 1+ ≈ 0.97 8 me π mh 8 mr The n 2/3 dependence of the energy shift is found, e.g., for CdO13 with different carrier concentrations (due to different deposition temperature, no intentional doping) [808] and depicted in Fig. 9.42.
9.8.3 InterValenceband Transitions Transitions within the valence band can occur between three bands, i.e. lh→hh, so→hh, and so→lh, as schematically depicted in Fig. 9.43. Theoretical treatments have been given in [809, 810]. For GaAs, such intravalenceband absorption occurs at photon energies close to Δ0 as shown in Fig. 9.44a for ptype GaAs:Zn [811]. For ptype GaSb, the absorption coefficient below the fundamental band gap is found almost entirely due to intervalence band transitions, as shown in Fig. 9.44b for a hole concentration of p = 3.2 × 1016 cm−3 [812].
13 CdO
is an indirect semiconductor, the optical band gap is the energy of the direct transition at the Γ point. The indirect transitions involve holes from other points in the Brillouin zone (cmp. Fig. 6.10).
9.8 Absorption in the Presence of Free Charge Carriers
335
E
EV
k
lh
EV
hh
0
so Fig. 9.43 Schematic optical transitions within the valence band
(a)
(b)
1
400 1
GaAs:Zn
pGaSb
200 100 60 40 0
20 10
0.1
0.2
0.3
0.4
0.5
0.6
Fig. 9.44 (a) Optical absorption spectrum of GaAs:Zn with p = 2.7 × 1017 cm−3 at T = 84 K. The absorption above the splitoff energy Δ0 is due to the hh/lh → so process . Adapted from [811]. (a) Optical absorption coefficient of GaSb with p = 3.2 × 1016 cm−3 . Experimental data (solid line) and calculation of intervalence band contribution (squares). The free carrier contribution is less than 5 cm−1 in the considered spectral range. Adapted from [812]
9.8.4 InterValley Transitions Electrons at the conduction band minimum can undergo optical transitions to the same band at a different point of the Brillouin zone. Such intervalley transition, as sketched in Fig. 9.45a, is phononassisted to fulfill momentum conservation and occurs around the energy difference ΔE between the two valleys (cmp. Table 8.4). For InP with an electron concentration of n = 1.65 × 1018 cm−3 , below the fundamental band edge at 1.4 eV, an additional contribution starting around 0.8– 0.9 eV is found besides the free carrier absorption (Fig. 9.45b) [813]. Taking into account the filling of the bottom of the conduction band, an energy separation for the two valleys of ΔE = 0.90 ± 0.02 eV was found for various values of the electron
336
9 Optical Properties
(a)
(b) 10 2 nInP 1
E
10
1
10
0
E
k
10
1
10
2
0.2
0.4
0.6
0.8
1.0
1.2
1.4
X Fig. 9.45 (a) Schematic of intervalley conduction band transitions involving a photon (solid line arrow) and a phonon (dashed line arrow). (b) Optical absorption coefficient of InP with n = 1.65 × 1018 cm−3 . Experimental data (solid line) and calculation of intervalley band contribution (dashed line). The extrapolated free carrier contribution is shown as dashdotted line and the difference of experimental absorption and extrapolated free carrier contribution as circles. Adapted from [813]
concentrations. This energy corresponds to the energy difference of conduction band minima at Γ and X in InP. The lineshape of this absorption processes can be modeled and fits well the difference of measured absorption and extrapolated freecarrier absorption spectra. Transitions to the lower minimum at L (ΔE = 0.6 eV) are not observed, possibly masked by the freecarrier absorption.
9.8.5 IntraBand Transitions Phononassisted transitions within the lowest conduction band (not to a different valley), as indicated schematically in Fig. 9.46a for the SnO2 band structure [814], can cause absorption at photon energies below the fundamental absorption edge. Actually in SnO2 , the optical transition across the fundamental band gap is only weakly dipoleallowed and leads to small absorption coefficient below 100 cm−1 directly above the fundamental band gap of about 3.6 eV. The strong dipoleallowed transition with absorption coefficient around 105 cm−1 begins at about 4.3 eV and stems from electrons in a lower valence band [815]. The freecarrier absorption due to transitions within the lowest conduction band are calculated to start already at 2.8 eV (Fig. 9.46b) and thus can also impact transparency in the visible spectral range.
9.9 Lattice Absorption
337
(a) 9
(b) SnO2
SnO2 (1018 cm 2 )
6
3
0
3 X
Z
W
Fig. 9.46 (a) Band structure of SnO2 and absorption processes; the transition from the topmost valence band (dashed arrow) is forbidden. (b) Calculated freecarrier absorption (σ = α/n) for SnO2 . The solid and dashed lines are results including phononassisted transitions for two light polarizations. The dotted lines are fits of the Drude model to the infrared regime. Adapted from [814]
9.9 Lattice Absorption While there is no interaction of optical phonons and (infrared) light in Si and Ge due to crystal structure symmetry [816], strong effects are present for compound semiconductors. A review can be found in [817].
9.9.1 Dielectric Constant The dielectric constant (with damping parameter Γ ) in the vicinity of the optical phonon energies is given by (cf. (5.50))
2 − ω 2 − iωΓ ωLO (ω) = (∞) 2 ωTO − ω 2 − iωΓ
.
(9.72)
The dispersion relation (without damping) can be written as f (0) − (∞) = (∞) 1 + . (ω) = (∞) + 1 − (ω/ωLO )2 1 − (ω/ωLO )2 Thus the oscillator strength (compare with (D.10)) is f = LST relation (5.49) the oscillator strength is
(0)−(∞) . (∞)
(9.73) With the
338
9 Optical Properties
Fig. 9.47 Lattice absorption oscillator strength f from (9.74) for various elemental, III–V and II–VI semiconductors as a function of their ionicity f i (cf. Table 2.1). Dashed line is linear dependence on ionicity for similar (reduced) mass, dashdotted lines are guides to the eye for similar ionicity and varying mass
f =
2 2 − ωTO ωLO ωLO − ωTO ≈2 , 2 ωTO ωTO
(9.74)
and thus proportional to the splitting ΔLT = ωLO − ωTO between the longitudinal and transverse optical phonon frequency. The approximation in (9.74) is valid for ΔLT ωTO . The oscillator strength increases with the ionicity, i.e. the electronegativity difference of the atoms in the base (Fig. 9.47). Additionally, the oscillator strength depends on the reduced mass and the highfrequency polarizability; this can be seen, e.g., for the series of the Zn compounds that all have similar ionicity. For the series of the nitrides, the mass effect is small since the reduced mass is dominated by the light N mass.
9.9.2 Reststrahlenbande The absorption of electromagnetic radiation by optical phonons is governed by the dielectric function that has been derived in (9.72). For small damping, i.e. Γ ΔLT , the dielectric constant is negative between ωTO and ωLO . From r = n 2r −κ2 it follows that κ2 is much larger than n 2r . Therefore, the reflectance (9.17) will be close to 1. This energy range is the socalled reststrahlenbande. This term stems from multiple reflections in this wavelength regime that suppresses neighboring spectral regions and thus achieves a certain monochromatization in the farinfrared spectral region. Within the semiconductor the absorption is large in the reststrahlenbande (Fig. 9.48).
9.9 Lattice Absorption
339
Fig. 9.48 Farinfrared absorption of GaAs. In the region around 35 meV is the reststrahlenbande with high absorption due to optical phonons. Adapted from [146], based on [818]
GaAs 0
25
50
75
9.9.3 Polaritons The coupled propagation of phonons and electromagnetic radiation is related to the equation (without phonon damping) (ω) = (∞)
2 − ω2 ωLO 2 ωTO − ω 2
=
c2 k 2 . ω2
(9.75)
There are two branches of propagating waves (real k): 1 c2 k 2 2 + ωLO ± ω = 2 (∞) 2
2 2 2 2 1 c2 k 2 2 c k ωTO 2 + − . ωLO 4 (∞) (∞)
(9.76)
√ For k = 0 we find the√solutions ω = ωLO and ω = kc/ (0). For large k we find ω = ωTO and ω = kc/ (∞). These solutions are shown in Fig. 9.49. Both branches have a phonon and a photonlike part. The coupled state between the phonon and the photon field is called the (phonon) polariton.
Fig. 9.49 Dispersion of the polariton. The dotted line displays the dispersion for a purely imaginary wavevector with the absolute value k
340
9 Optical Properties
In the interval [ωTO , ωLO ] the wavevector is purely imaginary, i.e. k = ik˜ with ˜ For this case there is only one solution that is also depicted in Fig. 9.49, real k.
2 ˜2
1 c k 2 + ωLO ω2 = 2 (∞)
+
1
c2 k˜ 2 2 + ωLO 4 (∞)
2 +
2 c2 k˜ 2 ωTO (∞)
2 .
(9.77)
9.9.4 Phonon–Plasmon Coupling The coupling of phonons and plasmons in the spectral region of the reststrahlenbande leads to the development of two new branches, the longitudinal phonon plasmon modes (LPP+ and LPP−), in the common dispersion. The dielectric function is
ωp2 ω2 − ω2 − (ω) = (∞) 1 + LO 2 ω2 ωTO − ω 2
.
(9.78)
For (ω) = 0 for k = 0 (coupling to photons) the two solutions ωLPP+ and ωLPP− do not cross as a function of ωp (Fig. 9.50),
(a)
(b)
Fig. 9.50 (a) Frequency of the coupled longitudinalphonon plasmon (LPP) modes (lower (upper) polariton branch in blue (red)) as a function of the plasma frequency. Dashed line shows uncoupled plasmon frequency (ω = ωp ), grey area indicates spectral region between TO and LO modes. (b) Experimental data on the polariton energies in ntype GaAs with different carrier concentration ωp ∝ √ n m ∗ (9.65). Dashed (dashdotted) line is plasmon frequency ωp without (with) consideration of conduction band nonparabolicity (cf. Fig. 6.31b). Data from [805, 819]
9.9 Lattice Absorption
ωLPP± =
341
! 1 2 2 2 + ωp2 )2 − 4 ωTO ωp2 . ωLO + ωp2 ± (ωLO 2
(9.79)
For small plasma frequencies ωLPP+ = ωLO , i.e. the optical phonons couple to the electromagnetic field without change. Also ωLPP− = ωp . For large carrier density, i.e. ωp ωLO , we find ωLPP− = ωTO and ωLPP+ = ωp . Thus, the carriers have effectively screened the electric field of the phonon that had led to the increase of the TO to the LO frequency.
Chapter 10
Recombination
Les hommes discutent, la nature agit. Men argue, nature acts. Voltaire
Abstract The various mechanisms and statistics of carrier recombination in semiconductors including bandband, excitonic, bandimpurity (Shockley–Read–Hall kinetics) and Auger recombination are explained. Also recombination at extended defects and surfaces is treated. Using the diffusionrecombination theory, the onedimensional carrier profiles for typical situations in experiments and devices are derived.
10.1 Introduction In thermodynamic nonequilibrium excess charges can be present in the semiconductor. They can be created by carrier injection through contacts, an electron beam or the absorption of light with wavelength smaller than the band gap. After the external excitation is turned off, the semiconductor will return to the equilibrium state. The relaxation of carriers into energetically lower states (and energy release) is called recombination. The term stems from the electron recombining with the hole created after absorption of a photon. However, there are other recombination mechanisms. A dedicated textbook is [820]. In the simplest picture an excitation generates carriers with a rate G (carriers per unit volume and unit time). In the steady state (after all turnon effects) a constant excess charge n carrier density is present. Then the generation exactly compensates the recombination processes. The principle of detailed balance even says that each microscopic process is balanced by its reverse process. If the time constant of the latter is τ , n is given by n = G τ . This follows from the steadystate solution n˙ = 0 of n dn =G− . dt τ © Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_10
(10.1) 343
344
10 Recombination
In the literature two limiting cases have been discussed, the relaxation and the lifetime semiconductor, depending on the relation of two time constants. The one time constant τ0 is the relaxation time constant due to recombination as discussed in the following. The smaller τ0 is, the faster excited electrons and holes recombine and ‘disappear’. Fast lifetimes are typically present in direct semiconductors (compared to indirect ones), semiconductors with high defect density and amorphous semiconductors. The other time constant is τD = /σ, the dielectric relaxation time; it describes the transport of carriers due to mobility (and diffusion). Large dielectric relaxation times are present in semiconductors with high mobility (low defect density, small carrier mass), small τD typically for hopping conduction. The relaxation case is given for τ0 τD ; carriers will recombine quickly and it is hard to build up nonequilibrium carriers and separate them with an applied electric field. In the recombination case τD τ0 , nonequilibrium carriers can assume nonuniform distributions and an applied electrical field generates separate quasiFermi levels for electrons and holes1 (cmp. Sect. 7.6).
10.2 Band–Band Recombination The band–band recombination is the relaxation from an electron in the conduction band into the valence (the empty state there is the hole). In a direct semiconductor, electrons can make an optical transition between the bottom of the conduction band to the top of the valence band. In an indirect semiconductor, this process is only possible with the assistance of a phonon and is thus much less probable.
10.2.1 Spontaneous Emission We consider the spontaneous recombination of an electron of energy E e and a hole of energy E h (Fig. 10.1a). C(E e , E h ) is a constant proportional to the matrix element of the optical transition (cf. Sect. 9.5). The spontaneous recombination rate rsp at photon energy E ≥ E C − E V = E g is (assuming energy conservation, i.e. E = E e − E h , but without kconservation in a dense plasma [821]), rsp (E) =
∞
dE e EC
EV
−∞
dE h C(E e , E h )
× De (E e ) f e (E e ) Dh (E h ) f h (E h ) δ(E − E e + E h )
1 In
the relaxation case, the separation of quasiFermi levels is kT .
(10.2)
10.2 Band–Band Recombination
345
(a)
(b)
(c)
Ec E=h
Eg
E=h
E=h
E=h E=h
Ev
Fig. 10.1 Processes of band–band recombination: (a) spontaneous emission, (b) absorption and (c) stimulated emission. A full (empty) circle represents an occupied (unoccupied) electron state
=
E+E V
dE e C(E e , E e − E)
EC
× De (E e ) f e (E e ) Dh (E e − E) f h (E e − E), where f h denotes the hole occupation f h = 1 − f e . The lineshape of the band–band recombination with kconservation2 is proportional to the joint density of states (9.30) and the Fermi distribution function. At small excitation and at low doping it can be approximated by the Boltzmann distribution function and the lineshape is given as I (E) ∝
E E − E g exp − . kT
(10.3)
An experimental spectrum is shown in Fig. 10.2 together with a fit according to (10.3). The expected FWHM of the peak is 1.7954 kT , which is about 46 meV at T = 300 K. At low sample temperature, the temperature of the carrier gas is typically higher than the lattice temperature, depending on the cooling mechanisms (carrier–carrier scattering, optical phonon emission, acoustic phonon emission, recombination, . . .) and the excitation rate. The carrier temperature in GaAs, determined from the Boltzmann tail of spontaneous emission (photoluminescence) is depicted in Fig. 10.3 as a function of excitation density; clearly it increases with increasing excitation. The recombination rate in indirect semiconductors is small since the transition is phononassisted. For silicon, an internal quantum efficiency in the 10−6 range has been reported [824]. For germanium, the direct transition is energetically fairly close to the fundamental, indirect L–Γ band edge transition (Fig. 9.12).The energy difference can be reduced from its bulk value of 136 meV by tensile strain. Additionally, the direct transition can be favored by heavily ndoping and filling the L conduction band minimum states (see Sect. 9.8.2). In this case, direct recombination from
effects are neglected here, e.g. for temperatures kT E Xb . Such effects are discussed in Sect. 10.3.
2 Excitonic
346
10 Recombination
(b)
(a) 5
GaAs
4 3
E= 46meV
2
Eg= 1.423eV
1 0 1.35
1.40
1.45
1.50
1.55
Fig. 10.2 (a) Photoluminescence spectrum of an undoped LPEgrown epitaxial GaAs layer at room temperature and low cw (λ = 647 nm) excitation density (10 W/cm2 ). The solid line is a lineshape fit with (10.3) and E g = 1.423 eV and T = 293 K. (b) Room temperature, direct (eΓ – hΓ ) recombination from heavily ndoped (1019 cm−3 ) germanium (1 µm thick Ge layer on silicon (001)) with biaxial (thermal) tensile strain. The strainsplit valence band edge (Fig. 6.43) causes the e–hh and e–lh transitions (individual contributions with lineshape according to (10.3) shown as dashed lines) to occur at different energies. Adapted from [822] 0.08 GaAs 0.07
15
20
0.05 0.04
TC (K)
0.06
1/TC (K1)
Fig. 10.3 Carrier temperature TC in GaAs as a function of excitation density at a lattice temperature of 1.6 K. The dashed line is guide to the eyes, the solid line corresponds to an activation energy of 33 meV, similar to the GaAs optical phonon energy. Adapted from [823]
0.03 0.02 0.01 104
40
ntype ptype
103
102
101
100 1
Excitation density (arb. units)
the conduction band Γ minimum can be observed [822] and the effective energy difference has been lowered to about 100 meV.
10.2.2 Absorption A similar consideration is made for the absorption process (Fig. 10.1b). An electron is transferred upon light absorption from a valenceband state (occupied) to a conductionband state that must be empty. The coefficient is B1 . Also, the process
10.2 Band–Band Recombination
347
is proportional to the light intensity, represented by the density of occupied photon states Nph (E), rabs (E) =
E+E V
dE e B1 (E e , E e − E)
EC
× De (E e ) (1 − f e (E e )) Dh (E e − E) (1 − f h (E e − E)) Nph (E). (10.4)
10.2.3 Stimulated Emission In this case, an incoming photon ‘triggers’ the transition of an electron in the conduction band into an empty state in the valence band. The emitted photon is in phase with the initial photon (Fig. 10.1c). The rate is (with coefficient B2 ): rst (E) =
E+E V
dE e B2 (E e , E e − E)
EC
× De (E e ) f n (E e ) Dh (E e − E) f h (E e − E) Nph (E).
(10.5)
The photon density Nph at a given energy is given by Planck’s law and the Bose– Einstein distribution (Appendix E) Nph (E) = N0
1 . exp (E/kT ) − 1
(10.6)
The prefactor is the density of states of the electromagnetic field3 N0 (E) = 8 π E 2 (n r / hc)3 .
10.2.4 Net Recombination Rate In thermodynamical equilibrium the rates fulfill rsp (E) + rst (E) = rabs (E).
(10.7)
The population functions are Fermi functions with quasiFermi levels Fn and Fp . Since for absorption and stimulated emission the same quantummechanical matrix element is responsible, B1 = B2 . The detailed balance (10.7) yields E − (Fn − Fp ) −1 . C(E 1 , E 2 ) = B1 (E 1 , E 2 ) Nph exp kT
(10.8)
total number of photon states in vacuum between the frequencies zero and ν is N (ν) = 8πν 3 /(3c3 ). With ν = E/ h and N0 = dN (E)/dE and considering c → c/n r we obtain the given value for N0 . 3 The
348
10 Recombination
In thermodynamic equilibrium, i.e. Fn = Fp , C(E 1 , E 2 ) = N0 B1 (E 1 , E 2 ) = B.
(10.9)
If the constant B, the bimolecular recombination coefficient, is independent of the energy E, the integration for the net bimolecular recombination rate rB can be executed analytically and we find rB =
∞ Eg
rsp (E) + rst (E) − rabs (E) dE
Fn − Fp = B n p 1 − exp − kT
.
(10.10)
In thermodynamic equilibrium, of course, rB = 0. The recombination rate Bnp is then equal to the thermal generation rate G th G th = B n 0 p0 .
(10.11)
The bimolecular recombination rate typically used in Shockley–Read–Hall (SRH) [825, 826] kinetics is (10.12) rB = B (n p − n 0 p0 ). Values for the coefficient B are given in Table 10.1. In the case of carrier injection, np is larger than in thermodynamical equilibrium, i.e. n p > n 0 p0 , and the recombination rate is positive, i.e. light is emitted. If the carrier density is smaller than in thermodynamical equilibrium, e.g. in a depletion region, absorption is larger than emission. This effect is also known as ‘negative luminescence’ [827] and plays a role particularly at elevated temperatures and in the infrared spectral region.
Table 10.1 Bimolecular recombination coefficient at room temperature for a number of semiconductors Material B (cm3 /s) GaN GaAs AlAs InP InAs 4HSiC Si GaP
1.1 × 10−8 1.0 × 10−10 7.5 × 10−11 6.0 × 10−11 2.1 × 10−11 1.5 × 10−12 1.1 × 10−14 3.0 × 10−15
Data for GaN from [828], Si from [829], SiC from [830], other values from [831]
10.2 Band–Band Recombination
349
10.2.5 Recombination Dynamics The carrier densities n and p, are decomposed into the densities n 0 and p0 in thermodynamic equilibrium and the excesscarrier densities δn and δ p, respectively n = n 0 + δn p = p0 + δ p.
(10.13a) (10.13b)
Here, only neutral excitations are considered, i.e. δn = δ p. Obviously the time = ∂∂tδn , and correspondingly for the hole density. The equation derivative fulfills ∂n ∂t for the dynamics n˙ = p˙ = −Bnp + G th = −B (n p − n 0 p0 ) = −B (n p − n 2i )
(10.14)
can be written as ∂ δp = −B (n 0 δ p + p0 δn + δn δ p) . ∂t
(10.15)
The general solution of (10.15) is given by δ p(t) =
(n 0 + p0 ) δ p(0) . [n 0 + p0 + δ p(0)] exp [B t (n 0 + p0 )] − δ p(0)
(10.16)
In the following, we discuss some approximate solutions of (10.15). First, we treat the case of a small (neutral) excitation, i.e. δn = δ p n 0 , p0 . The dynamic equation is in this case ∂ δp = −B (n 0 + p0 ) δ p. ∂t
(10.17)
Then the decay of the excesscarrier density is exponential with a time constant (lifetime) τ given by 1 τ= . (10.18) B (n 0 + p0 )
350
10 Recombination
In an ntype semiconductor additionally n 0 p0 , and thus the minority carrier lifetime τ p is 1 τp = . (10.19) B n0 If the nonequilibrium carrier densities are large, i.e. n ≈ p n 0 , p0 , e.g. for strong injection, the kinetics obeys ∂ δp = −B (δ p)2 , ∂t
(10.20)
and the transient has the form δ p(t) =
δ p(0) , 1 + B t δ p(0)
(10.21)
where δ p(0) is the excess hole density at time t = 0. Such a decay is called hyperbolic and the recombination is bimolecular. The exponential decay time is formally τ −1 = Bδ p(t) and is thus time and density dependent. A detailed discussion of minority carrier lifetime is given in [832].
10.2.6 Lasing The net rate for stimulated emission and absorption is E − (Fn − Fp ) rst (E) − rabs (E) = 1 − exp kT E+E V × dE e B De (E e ) f e (E e ) Dh (E e − E) f h (E e − E) Nph (E). EC
(10.22) The net rate at photon energy E = ω is only larger than zero (i.e. dominating stimulated emission) when Fn − Fp > E ≥ E g .
(10.23)
When the difference of the quasiFermi levels is larger than the band gap, the carrier population is inverted, i.e. close to the band edges the conductionband states are more strongly populated with electrons than the valenceband states, as shown in Fig. 10.4. An incoming optical wave of energy E will then be net amplified by stimulated emission. Equation (10.23) is also called the thermodynamic laser condition. We note that lasing requires further conditions as discussed in Sect. 23.4.
10.3 Exciton Recombination Fig. 10.4 Chargecarrier distribution during inversion, necessary for lasing. Shaded areas are populated with electrons. A stimulated transition between an electron and a hole is indicated
351
E
Fn EC
EV Fp
D(E)
10.3 Exciton Recombination 10.3.1 Free Excitons The observation of freeexcitons is limited for semiconductors with a small exciton binding energies (such as in GaAs) to low temperatures. However, for large exciton binding energy, recombination from freeexcitons is observed even at room temperature, as shown in Fig. 10.5 for ZnO. A low temperature recombination spectrum of silicon is shown in Fig. 10.6. In pure silicon, phononassisted exciton recombination (cmp. Sect. 10.4) is observed involving acoustic (ITA ) and optical (ITO ) phonons. The weakly observed nophonon line (I0 ) is forbidden in perfect Si.
10.3.2 Bound Excitons Excitons can localize at impurities, defects or other potential fluctuations and subsequently recombine [834, 835]. Excitons can be bound to neutral or ionized donors and acceptors impurities [836]. Also they can be bound to isoelectronic impurities, the most prominent example being N in GaP [837] (cmp. Sect. 9.6.9). or isoelectronic clusters [838]. The recombination of excitons localized in quantum wells (Sect. 12.4) and quantum dots (Sect. 14.3.4) is discussed later.
352
10 Recombination
PL Intensity (arb. units)
ZnO
1
D0,X 3.20
3.25
3.30
3.35
XA 3.40
Energy (eV)
Fig. 10.5 Temperaturedependent luminescence spectra of a ZnO thin film (on sapphire). At low temperatures, the spectra are dominated by donorbound exciton transitions (Al0 , X)). The vertical dashed line indicates the lowtemperature position of the donorbound exciton transition (D0 , X). The curved dashed line visualizes the energy position of the freeexciton transition (XA ) that becomes dominant at room temperature
Fig. 10.6 Low temperature recombination spectra from silicon with low (solid lines) and sizeable (dashed line) phosphorus dopant concentration. Spectrum for NP = 2 × 1014 cm−3 (NP = 8 × 1016 cm−3 ) taken at 26 K (15 K). Transitions in pure Si are label with ‘I’, transitions involving P donors are labeled with ‘P’. Q indicates the dissociation energy of the bound exciton. Adapted from [833]
10.3 Exciton Recombination
353
Table 10.2 Localization energy Q (Q ∗ ) of excitons on selected impurities (ionized impurities, D+ or A− , respectively) in various semiconductors Host Donor Q (meV) Q ∗ (meV) Q ∗ /Q σ Reference GaAs GaN AlN CdS ZnSe
ZnO
EMD Zn EMD Mg Si Mg EMD Al Ga In Al Ga In
0.88 8.1 6.8 20 16 40 6.6 4.9 5.1 5.4 15.5 16.1 19.2
1.8 31.1 11.2
2.0 3.8 1.6
0.28 0.36
[840] [841] [842] [843] [843]
3.8 5.4 6.6 7.5 3.4 4.1 8.5
0.6 1.1 1.3 1.4 0.21 0.25 0.44
0.17 0.27
[844] [845, 846]
0.3
[847]
σ is the ratio of effective electron and hole (polaron) masses. EMD: effective mass donor
The transition energy ω of an exciton bound to a neutral impurity is ω = E g − E X b − Q,
(10.24)
where Q is the binding (or localization) energy of the exciton to the impurity. The binding energy of an exciton to an ionized impurity is denoted with Q ∗ . A transition involving an exciton bound to a neutral donor is denoted (D0 , X); correspondingly (D+ , X), also denoted as (h, D0 ), and (A0 , X). Values for donorbound excitons in various semiconductors are listed in Table 10.2. The (D0 , X) complex is stable for 0 < σ = m ∗e /m ∗h < 0.43 according to [839]. The (D+ , X) peak can occur on the lowor highenergy side of the (D0 , X) recombination. Whether Q ∗ < Q or Q ∗ > Q depends on σ being smaller or larger than 0.2, respectively [839], and is fulfilled for many semiconductors, e.g. GaAs, GaN, CdS, and ZnSe. Recombination in silicon due to excitons involving phosphorus donors is depicted in Fig. 10.6. The (D0 , X) transition in Si:P is labeled ‘P0 ’ (Q = 6 meV). Other Prelated transitions are discussed in [833]. In Si, the binding energy to the impurity is about one tenth of the binding energy of the impurity (Haynes’s rule [834, 848]), i.e. Q/E Db and Q/E Ab ≈ 0.1 (Fig. 10.7a). In GaP the approximate relations Q = 0.26E Db − 7 meV and Q = 0.056E Ab + 3 meV have been found [837]. For donors in ZnO, the relation Q = 0.365E Db − 3.8 meV holds (Fig. 10.7b) [849]. In Fig. 10.8, the recombination spectrum of GaAs:C is shown that exhibits recombination from excitons bound to the acceptor (carbon) and shallow donors. The exciton is more strongly bound to an ionized donor (D+ ) than to a neutral donor. Varying the concentration of a specific impurity and observing the corresponding change in the intensity of the (D0 , X) transition allows to identify the chemical species to which the exciton is bound. This can be achieved via the comparison of different samples or more elegantly by introducing radioactive isotopes. This is shown in
354
10 Recombination
(b)
(a) 20
Si In
15
10
Bi As Ga P Sb Al B
5
0
0
50
150
100
ED
b
200
(meV)
Fig. 10.7 Energy Q required to remove an exciton from a neutral impurity (10.24) as a function of the ionization energy E Db (open circles) or E Ab (solid circles) of the involved impurity in (a) silicon (experimental data from [848]) and (b) ZnO (experimental data from [849]
(A0,X)
GaAs:CAs
(h,D0) (D0,X) 0
(e,A )
0
(D0,A0 )
(h,D2s)
0
(D ,X)2s 20
1.49
1.50
1.51
1.52
Fig. 10.8 Photoluminescence spectrum (T = 2 K, D = 10 mW cm−2 ) of GaAs:CAs (NA = 1014 cm−3 ) with donor and acceptorrelated boundexciton recombination around 1.512 eV, (e, A0 ), (h, D0 ) and (D0 , A0 ) pair and freeexciton recombination. Adapted from [840]
Fig. 10.9 for In in ZnO; the (111 In0 , X) transition disappears with the characteristic time constant close to that (97 h) of the nuclear decay of 111 In into stable 111 Cd. However, in such experiments it should be considered that the decay product and accompanying highenergy radiation can create new electronic and structural defects, respectively.
10.3 Exciton Recombination
355
(a)
(b)
Fig. 10.9 (a) Lowtemperature photoluminescence spectrum of ZnO implanted with 111 In featuring the socalled I9 line. Spectra are recorded at various times after implantation as labeled. (b) Intensity of I9 line as a function of time. Adapted from [850]
(a)
(b) 0
(D ,X)
TES
D
exc.
EC
20
0
0
X
D* n=3 n=2
4
ED
40
n=1
1
1.510
1.515
EV
Fig. 10.10 (a) Photoluminescence spectrum (T = 1.5 K, D = 50 mW cm−2 ) of highpurity GaAs with two donors (Ge and Se/Sn). The lower spectrum has been excited 6 meV above the band gap, the upper spectrum has been resonantly excited with the laser set to the (D0 , X) transition and exhibits n = 2, 3, 4, and 5 TES transitions. α, β, γ denote excited (hole rotational) states of the (D0 , X) complex. Adapted from [852]. (b) Schematic representation of the n = 2 TES process, left initial, right final state
The peak labeled (D0 ,X)2s in Fig. 10.8 is called a twoelectron satellite (TES) [851]. Highresolution spectra of the TES in GaAs [506, 852] are shown in Fig. 10.10a. The TES recombination is a (D0 ,X) recombination that leaves the donor in an excited
356
10 Recombination
state as schematically shown in Fig. 10.10b. Therefore a hydrogenlike series with n = 2, 3, . . . is observed with energies n E TES
=E
(D0 ,X)
−
E Db
1 1− 2 n
.
(10.25)
The effect of isotope disorder on the sharpness and splitting of impurity states has been investigated in [853, 854]. The recombination of excitons bound to Al, Ga and In in natural silicon (92.23 % 28 Si, 4.67 % 29 Si, 3.10 % 30 Si) is split into three lines due to the valleyorbit splitting [855] of electron states at the band minimum (Fig. 10.11). Each of these (A0 , X) lines is split by 0.01 cm−1 for Si:Al due to a symmetry reduction of the 4fold degenerate A0 ground state, as observed in the presence of applied axial strain or an electric field. The comparison to spectra from enriched 28 Si shows that the observed splitting without external perturbation is due to isotope disorder that causes random strains and splits the A0 ground state into two doublets [854] (Fig. 10.11). Similarly, the (unsplit) phosphorusinduced (D0 , X) transition in enriched Si is found to be much sharper ( 0.03 the low temperature recombination peak is due to donorbound excitons. Adapted from [871]
broadening is obvious, causing a single peak for x > 0.03. The temperature dependence of the peak positions is shown in Fig. 10.17 for the same samples. For x = 0.005 the bound exciton (Aldonor) (D0 , X) and free exciton (XA ) recombination lines can still be resolved despite the inhomogeneous broadening of σ = 2.6 meV. At
10.3 Exciton Recombination
(a)
361
(b)
(c)
Fig. 10.17 Temperature dependence of the shift of energy position of (D0 , X) and XA photoluminescence peak in Mgx Zn1−x O alloys with three different Mgcontents, (a) x = 0.005, (b) x = 0.03, (c) x = 0.06. The energy positions are given relative to the low temperature position of the respective (D0 , X) peaks. Adapted from [860]
low temperature the luminescence intensity is dominated by (D0 , X) recombination, at room temperature by free exciton (XA ) recombination. Both peaks are present at low temperatures and exhibit a redshift with increasing temperatures due to the shrinking of the band gap (Fig. 10.17a). The (D0 , X) peak vanishes at about 180 K due to ionization of the excitons from the donors (Q ≈ 15 meV, similar as in pure ZnO). For larger Mgcontent of x = 0.03 the two peaks can still mostly be separated (σ = 6.0 meV). The (D0 , X) energy position shows a small dip (about 2 meV) due to exciton localization in the alloy disorder potential (arrow in Fig. 10.17b). At low temperatures excitons are frozen in local potential minima and have a nonthermal (nonBoltzmann) population. With increasing temperature they can overcome energy barriers and thermalize, leading to a shift of the recombination peak to lower energies. Further increase of temperature populates higher levels and leads to a shift of the recombination peak to higher energies. Superimposed is the redshift due to the band gap shrinkage. This socalled “S”shape effect of E(T ) is discussed in Sect. 12.4 in detail with regard to exciton localization in a quantum well disorder potential. For x = 0.06 only a single photoluminescence peak is observed for the alloy (σ = 8.5 meV). The (D0 , X) peak is the dominant for the Mgx Zn1−x O alloys at low temperatures even in the presence of large alloy broadening (Fig. 10.16b). The peak changes its nature from (D0 , X) at low temperatures to XA at room temperature. In between, first exciton thermalization (redshift) in the disorder potential and
362
10 Recombination
subsequently exciton ionization from the donors (blueshift, arrow in Fig. 10.17c) are observed [860]. Such exciton ionization from impurities has also been observed for AlGaN:Si [549, 872].
10.4 Phonon Replica The momentum selection rule for freeexciton recombination allows only excitons with K ≈ 0 (for K, cf. (9.37)) to recombine. The fine structure of this recombination is connected to polariton effects (cf. Sect. 9.6.8). Excitons with large K can recombine if a phonon or several phonons are involved [873] that provide the necessary momentum q = K1 −K2 , with K1 (K2 ) being the wave vector of the initial (intermediate) exciton state (Fig. 10.18). A socalled zerophonon line at energy E 0 is then accompanied by phonon replica below E 0 at integer multiples (at low temperature) of the (LO) phonon energy ωph E n = E 0 − n ωph . (10.31) Phonon replicas have been observed in many polar semiconductors such as CdS [874] and ZnSe [875]. A sequence of such phonon replica, as observed in GaN [876], is depicted in Fig. 10.19a. The lineshape of the nth phononassisted line is proportional to the exciton population at a given excess energy, which is proportional to the density of states and the Boltzmann distribution function [877]
Fig. 10.18 Schematic representation of 1 LO exciton scattering of an exciton at K = 0 to an intermediate state with K ≈ 0 and subsequent radiative decay. ω represents the phonon energy and E 1 the energy of the emitted photon
E
n=3 n=2 n=1
continuum
h
ph
E1
K
10.4 Phonon Replica
363
(a)
(b)
GaN
100 1LO 2LO
101 102
5LO
4LO
3LO
103
92meV
3.1
3.2
3.3
3.4
3.5
Fig. 10.19 (a) Photoluminescence spectrum of GaN (grown on SiC substrate) at T = 50 K. In addition to emission from free (FE) and bound (BE) excitons several phonon replica (labeled as 1LO– 5LO) are observed. Vertical dashed lines indicate energy positions of multiple LOphonon energies (ωLO = 92 meV) below the FE peak. Adapted from [876]. (b) Photoluminescence spectrum of 1LO phononassisted recombination peak at T = 103 K (from the data of Fig. 10.5). Data points (dots) and lineshape fit (solid line) according to (10.32) with the parameters L 1 = 0.9 and E 1 = 3.2955 eV (and background)
In (E ex ) ∝
E ex E ex exp − wn (E ex ). kT
(10.32)
Here, E ex represents the exciton kinetic energy. The factor wn (E ex ) accounts for the qdependence of the matrix element. It is typically expressed as Ln . wn (E ex ) ∝ E ex
(10.33)
Accordingly, as temperature dependent refinement of (10.31), the energy separation ΔE n of the energy of the peak maximum of phonon replica from E 0 is given by
1 kT. ΔE n = E n − E 0 = −n ωph + L n + 2
(10.34)
It is found theoretically that L 1 = 1 and L 2 = 0 [877]. These relations are approximately fulfilled for GaN [878]. A lineshape fit for the 1 LO phononassisted transition in ZnO is shown in Fig. 10.19b. In Fig. 10.20a the ‘green band’ emission of ZnO is shown as presented in [879]. This band is mostly attributed to a Cu impurity; recently, evidence has grown from isotope decay and annealing studies that it is related to the zinc vacancy [880] (Fig. 10.20b). The zero phonon line is followed by many replica with a maximum at about 6 LO phonons. The intensity I N of the N th replica is given by [881, 882] I N ∝ exp(−S)
SN , N!
(10.35)
364
10 Recombination
(a)
(b)
650
600
550
500
450
6 5
ZnO
7
4
8 3
9
2 1
2.0
2.2
2.4
2.6
2.8
Fig. 10.20 (a) Luminescence spectrum of ZnO in the visible. The arrow denotes the zerophonon line at 2.8590 eV. The numbers of the phonon replica are labeled. Adapted from [879]. (b) Luminescence spectra (solid lines) of a ZnO bulk crystal before (‘untreated’) and after annealing in O2 atmosphere at T = 1073 K. After annealing in Zn atmosphere at the same temperature, the green band disappears again (dashed line). From [880]
where S is the socalled Huang–Rhys parameter. In [880], a coupling parameter of S = 6.9 has been determined. Equation (10.35) is obtained from the consideration of transitions in the configuration diagram [881, 883] (Fig. 10.21), using the Born–Oppenheimer approximation. Here the electronic wavefunctions are separated from the vibrational wavefunctions, leading to the Franck–Condon principle, that optical transitions occur with the positions of the nuclei fixed and thus vertical in the configuration diagram Fig. 10.21. Assuming low temperatures, only the lowest state is (partially) occupied. The Huang– Rhys parameter, the average number of phonons involved in the transition, is related to the displacement δq = q1 − q0 of the two configurations S=
C δq 2 , 2 ωph
(10.36)
where C is the ‘spring constant’ of the parabola, C = d2 E/dq 2 . For small S 1, we are in the weak coupling regime and the zerophonon line is the strongest. In the strong coupling regime, S > 1, the maximum is (red) shifted from the zerophonon line. We note that in absorption, phonon replica occur on the highenergy side of the zerophonon absorption. For large S the peak intensities are close to a Gaussian. The correspondence of emission and absorption is nicely seen for excitons on isoelectronic oxygen traps in ZnTe [882]. The oxygen is on substitutional Te site. Up to seven phonon replica are visible in Fig. 10.22 around the zerophonon or Aline with a separation of about 26 meV, the optical phonon energy in ZnTe. The Huang–Rhys parameter is about 3–4. Other peaks are due to acoustic phonons.
10.5 SelfAbsorption
365
(a)
(b)
E
absorption
emission
S= 0
Sh E1
1
E
2
h
4 8
E0
q0
q1
q
ZPL
E
Fig. 10.21 (a) Configuration diagram of two states that differ in their configuration coordinate by δq = q1 − q0 . Both are coupled to phonons of energy ω. The absorption maximum (solid vertical line) and emission maximum (dashed vertical line) are shifted with respect to the zerophonon line (dotted vertical line) with energy E 1 − E 0 . The Huang–Rhys parameter is S ∼ 4. (b) Intensity of zerophonon line (‘ZPL’) and phonon replica (10.35) for emission and absorption processes with different values of the Huang–Rhys parameter S as labeled
Fig. 10.22 Photoluminescence (solid line) and absorption (dashed line) spectra of excitons bound to substitutional oxygen in ZnTe at T = 20 K. The energy position is relative to the Aline at 1.9860 eV. The vertical dashed lines have a separation of 25.9 meV. Adapted from [884]
10.5 SelfAbsorption Luminescence that is emitted within the semiconductor can be (re)absorbed before it may reach the surface and can leave the crystal. This effect is called selfabsorption. It is particularly strong for radiation with an energy where the absorption α(ω) is high, i.e. above the band gap of a direct semiconductor. Similarly to the penetration
366
10 Recombination
Fig. 10.23 Photoluminescence spectrum (at T = 55 K) from bulk ZnO excited homogeneously via twophoton excitation by a Qswitched ruby laser (pulse width 40 ns). Adapted from [885]
depth 1/α for radiation entering the crystal, emission approximately occurs only from a layer of such thickness. For typical values of α in the range of 105 cm−1 , the ‘skin’ of the semiconductor that emits light with energy above the band gap is 100 nm. For light at the low energy side of the band gap or with energy within the band gap (deep levels), the emission depth can be much larger. After reabsorption, the energy has another chance to relax nonradiatively, thus reducing the quantum efficiency. Alternatively it can be reemitted, either at the same energy or at a lower energy. Possibly several reabsorption processes occur before a photon eventually leaves the semiconductor (‘photon recycling’). Such processes are important in LED structures where photon extraction has to be optimized (Sect. 23.3.4). Emission on phonon replica (Sect. 10.4) is redshifted from the energy range of strong absorption and thus suffers no (or only little) selfabsorption. This can be seen from the spectrum of a thick ZnO crystal excited homogeneously (via twophoton absorption with a red Ruby laser), Fig. 10.23. The zero phonon line (at E X ), originating from the ≈100 nm skin of the samples and being by far the strongest in thin films (Fig. 10.5), is practically absent and emission on the phonon replica collected from the entire volume dominates the spectrum.
10.6 Donor–Acceptor Pair Transitions Optical transitions can occur between neutral donors and acceptors. The (spatially indirect) donor–acceptor pair (DAP) recombination is present in (partially) compensated semiconductors and follows the scheme D 0 A0 → D + A− eh → D + A− + γ, where γ is a photon with the energy ω. The energy of the emitted photon is given by ω = E g − E Db − E Ab +
1 e2 , 4π0 r R
(10.37)
10.6 Donor–Acceptor Pair Transitions 1.57 1.56 1.55 1.54 1.53 1.52 1.51 1.50 1.49 1.48 1.47 1.46 1.45 1.44 1.43 1.42 1.41 1.40
Zn O
367 C O
GaP
Cd O
15.5 meV
0
0.5
1.0
1.5
2.0
2.5
3.0
Fig. 10.24 Transition energies in GaP (T = 1.6 K) of the donor–acceptor recombination involving the deep oxygen donor and C, Zn, and Cd acceptors, respectively. The lines follow (10.37) for E gGaP = 2.339 eV, r = 11.1 and (E Db )O = 893 meV, (E Ab )C = 48.5 meV, (E Ab )Zn = 64 meV, and (E Ab )Cd = 96.5 meV. Predicted missing modes for GaP:C, O are labeled with ‘G’. Adapted from [886]
where R is the distance between the donor and the acceptor for a specific pair. Since R is discrete, the DAP recombination spectrum consists of several discrete lines. If the donor and acceptor occupy the same sublattice, e.g. O and C both substituting P √ sites in GaP, the spatial distance of the donor and acceptor is R(n) = a0 n/2, where a0 is the lattice constant and n is an integer. However, for certain ‘magic’ numbers n = 14, 30, 46, . . . no lattice points exist and therefore the corresponding lines are missing (labeled ‘G’ in Fig. 10.24). No such gaps exist in DA spectra where donors and acceptors occupy different sublattices, e.g. GaP:O,√ Zn (see also Fig. 10.24). In this case, the spatial separation is given by R(n) = a0 n/2 − 5/16. If significant broadening is present, the lines are washed out and a donor–acceptor pair band forms.
10.7 InnerImpurity Recombination The transitions of electrons between different states of an impurity level can be nonradiative or radiative. As an example, the radiative transition of electrons in the Fe2+ state in InP 5 T2 →5 E (Fig. 10.25) and its fine structure were observed first in [888] at around 0.35 eV.
368
10 Recombination
(b)
(a) 1.34
EC 5
InP:Fe
T2
1.14
5
0.78
InP:Fe 5
E
T2
5
E
0.25 0 Fe
3+
Fe
2+
EV
0.340
0.345
0.350
Fig. 10.25 (a) Schematic band diagram of InP with levels of Fe impurities in the 3+ and 2+ charge states at low temperature. All energies are given in eV. The arrow denotes the optical transition from an excited Fe2+ state to the Fe2+ ground state. (b) Photoluminescence spectrum (at T = 4.2 K) of InP:Fe sample with [Fe] = 5 × 1016 cm−3 . Part (b) adapted from [887]
10.8 Auger Recombination In competition with the radiative, bimolecular recombination is the Auger recombination (Fig. 10.26). In the Auger process, the energy that is released during the recombination of an electron and hole is not emitted with a photon but, instead, transferred to a third particle. This can be an electron (eeh, Fig. 10.26a) or a hole (hhe, Fig. 10.26b). The energy is eventually transferred nonradiatively from the hot third carrier via phonon emission to the lattice. The probability for such process is ∝ n 2 p if two electrons are involved and ∝ np 2 if two holes are involved. The Auger process is a threeparticle process and becomes likely for high carrier density, either through doping, in the presence of many excess carriers, or in semiconductors with small band gap. Auger recombination is the inverse of the impact ionization (cf. Sect. 8.4.4). Phononassisted Auger recombination relaxes the momentum conservation rule for the involved charge carriers at the cost of an additional particle being involved in the scattering process. It has been pointed out that this process is dominating in bulk material [889, 890] and quantum wells [891]. In thermodynamic equilibrium the rates for Auger recombination and thermal Auger generation must be equal, thus G th = Cn n 20 p0 + Cp n 0 p02 ,
(10.38)
where Cn and Cp denote the Auger recombination coefficients. The equation for the dynamics in the presence of excess carriers (if solely Auger recombination is present) is given as ∂ δn = G th − R = −Cn (n 2 p − n 20 p0 ) − Cp (n p 2 − n 0 p02 ). ∂t
(10.39)
10.8 Auger Recombination
(a)
e
369
E
(b)
Eg
e
E
Eg
lh
hh
lh
hh
k
k
Fig. 10.26 Schematic representation of Auger recombination. An electron recombines with a hole and transfers the energy to (a) another electron in the conduction band, (b) another electron in the valence band
The Auger recombination rate typically used in SRH kinetics is rAuger = (Cn n + Cp p) (np − n 0 p0 ) .
(10.40)
Typical values for the Auger recombination coefficients are given in Table 10.3. In Fig. 10.27a the electron lifetime in heavily pdoped InGaAs (lattice matched to InP) is shown [893]. It follows τn−1 = Cp NA2 as expected from (10.39) for ptype material. The Auger process in silicon has been discussed in detail [894]. In Fig. 10.27b experimental data for ntype and ptype Si are summarized. Auger theory can predict the lifetimes in ntype material. The predicted rate in ptype material is too small, thus a phononassisted process is evoked [894]. Table 10.3 Auger recombination coefficients for some semiconductors. Data for InSb from [892], SiC from [830], others from [831]
Material
Cn (cm6 /s)
Cp (cm6 /s)
4HSiC Si, Ge GaAs, InP InSb
5 × 10−31
2 × 10−31 9.9 × 10−32 3.0 × 10−30
2.8 × 10−31 5.0 × 10−30 1.2 × 10−26
370
10 Recombination
(a)
(b)
Fig. 10.27 (a) Experimental values of the electron lifetime in heavily pdoped InGaAs on InP at room temperature. The dashed lines show dependencies of Auger (∝ NA−2 , Cp = 8.1 × 10−29 cm−6 s−1 ) and bandband recombination (∝ NA−1 , B = 1.43 × 10−10 cm−3 s−1 ). Adapted from [893]. (b) Experimental Auger lifetimes in ptype (squares) and ntype (circles) silicon at 300 K. The dashed (solid) line is theory for ptype (ntype) material. Adapted from [894]
10.9 Band–Impurity Recombination A very important recombination process is the capture of carriers by impurities. This process is in competition with all other recombination processes, e.g. the radiative recombination and the Auger mechanism. The band–impurity recombination is the inverse process to the carrier release from impurities and intimately related to carriers statistics (Chap. 7). It is particularly important at low carrier densities, for high dopant concentration and in indirect semiconductors since for these the bimolecular recombination is slow. This process is generally considered to be nonradiative since no photons close to the band edge are emitted.4
10.9.1 Shockley–Read–Hall Kinetics The theory of capture on and recombination involving impurities is called Shockley– Read–Hall (SRH) kinetics [825]. An example of radiative band–impurity recombination (of the type shown in Fig. 10.28a) is shown in Fig. 10.8 (e, A0 ) recombination at the carbon acceptor in GaAs.
4 Depending
on the energetic depth of the trap, mid or far infrared photons can be emitted.
10.9 Band–Impurity Recombination
(a)
371
(b)
(c)
(d) EC Et
EV Fig. 10.28 Bandtoimpurity processes at an impurity with one level (left initial, right final state in each part): (a) electron capture (from conduction band), (b) electron emission (into conduction band), (c) hole capture (from valence band), (d) hole emission (into valence band). The arrows indicate the transition of the electron
We consider electron traps [895] (see Fig. 10.28) with a concentration Nt with an energy level E t . In thermodynamic equilibrium they have an electron population f t0 =
exp
1 Et −EF kT
+1
,
(10.41)
where f t is the nonequilibrium population of the trap. Then the capture rate rc is proportional to the unoccupied traps and the electron concentration, rc ∝ n Nt (1− f t ). The proportionality factor has the form vth σn , where vth is the thermal velocity √ vth = 3kT /m ∗ ≈ 107 cm/s and σn is the capture cross section that is of atomic scale, typically ∼10−15 cm2 . The capture cross section can be related to the optical absorption cross section [513, 514]. In order√ to make the following calculation more transparent, we put the effectivem 0 /m ∗ into σ in the following and thus have the same thermal velocity mass ratio √ vth = 3kT /m 0 for electrons and holes. The capture rate of electrons is rc = vth σn n Nt (1 − f t ).
(10.42)
The emission rate from filled traps is gc = en Nt f t ,
(10.43)
where en denotes the emission probability. In a similar way, the emission and capture rates for holes can be written: rv = vth σp p Nt f t gv = ep Nt (1 − f t ).
(10.44) (10.45)
372
10 Recombination
In thermodynamical equilibrium, capture and generation rates are equal, i.e. rc = gc and rv = gv . Thus, the emission probability is en = vth σn n 0 Using written as
1− f t0 f t0
= exp
1 − f t0 . f t0
(10.46)
Et −EF kT
, (7.10) and (7.11) the emission probabilities can be
en = vth σn n t ep = vth σp pt ,
(10.47) (10.48)
with
Et − EC kT Et − EV . pt = NV exp − kT
n t = NC exp
(10.49) (10.50)
We note that n t pt = n 0 p0 (cf. (7.15)). The temperature dependence of the thermal velocity is ∝ T 1/2 , the temperature dependence of the bandedge density of states is ∝ T 3/2 (7.8) and (7.9). Thus,the temperature dependence of the emission rate en is (apart from the exponential term) ∝ T 2 if σ is temperature independent. Charge conservation requires in nonequilibrium (and of course in equilibrium) rc − rv = gc − gv . From this we obtain the population of the trap in nonequilibrium: ft =
σ n n + σp p t . σn (n + n t ) + σp ( p + pt )
(10.51)
The recombination rate rb−i of the band–impurity recombination is then ∂δn ∂t = rc − gc
rb−i = −
=
σn σp vth Nt (n p − n 0 p0 ) . σn (n + n t ) + σp ( p + pt )
(10.52)
Using the ‘lifetimes’ τn 0 = (σn vth Nt )−1 τ p0 = (σp vth Nt )−1 ,
(10.53) (10.54)
10.9 Band–Impurity Recombination
373
this is typically written as rb−i =
1 (n p − n 0 p0 ) . τ p0 (n + n t ) + τn 0 ( p + pt )
(10.55)
For an ntype semiconductor the Fermi level is above E t and the traps are mostly full. Thus hole capture is the dominating process. The equation for the dynamics simplifies to p − p0 ∂δ p . (10.56) =− ∂t τ p0 Thus, an exponential decay with minoritycarrier lifetime τ p0 (or τn 0 for ptype material) occurs. A recombination center is most effective when it is close to the middle of the band gap (midgap level). The condition ∂rb−i /∂ E t = 0 leads to the trap energy E tmax with the maximum recombination rate being located at E tmax =
EC + EV σn N C − kT ln . 2 σp N V
(10.57)
The curvature ∂ 2 rb−i /∂ E t2 at E tmax is proportional to −(np − n 0 p0 ) and thus indeed is negative in the presence of excess carriers. However, the maximum can be fairly broad. The SRH kinetic presented here is valid for low densities of recombination centers. A more detailed discussion and a more general model can be found in [896]. A typical example for a recombination center is gold in silicon. The minority carrier lifetime decreases from 2 × 10−7 s to 2 × 10−10 s upon increase of the Au concentration from 1014 to 1017 cm−3 . The incorporation of recombination centers is an important measure for the design of highfrequency devices [897]. Due to importance in silicon technology the recombination properties of many metals in silicon have been investigated, in particular Fecontamination and the role of FeBcomplexes [898–900]. A reduction in minoritycarrier lifetime can also be achieved by irradiation with highenergy particles and the subsequent generation of point defects with energy levels at midgap. In Fig. 10.29 various data on minority carrier lifetime in silicon are compiled. Over some doping range, a dependence of the lifetime ∝ N −1 as in (10.53) prevails. For doping beyond the 1019 cm−3 range, Auger recombination (Sect. 10.8) with τ ∝ N −2 is dominant. A more detailed discussion can be found in [901, 902]. Generally the lifetimes are temperature dependent [903] as expected from (10.52).
374
10 Recombination
Fig. 10.29 Minority carrier lifetime at room temperature as a function of majority carrier concentration in ntype and ptype silicon. The dashed lines have the slopes N −1 and N −2 . Data from [902]
10.9.2 Multilevel Traps Traps with multiple levels in the band gap have generally similar but more complicated dynamics as compared to singlelevel traps. Lifetimes are an average over negatively and positively charged states of the trap.
10.10 ABC Model Summarizing the results on bandimpurity recombination (Sect. 10.9), bimolecular recombination (Sect. 10.2) and Auger recombination (Sect. 10.8), the total recombination rate R can be written simplified as R = A n + B n2 + C n3,
(10.58)
where A is the coefficient for the bandimpurity recombination, B the bimolecular recombination coefficient and C the Auger recombination coefficient; n denotes the carrier density. This model is known as the ‘ABC’ model. It can be refined separating effects of electrons and holes and including higher terms. Often such model is used to investigate recombination in devices as a function of injection, e.g. [904, 905]. The internal radiative quantum efficiency ηint is given by ratio of the radiative recombination rate and the total recombination rate, ηint =
B n2 Bn = . A n + B n2 + C n3 A + B n + C n2
(10.59)
10.11 Field Effect
375
10.11 Field Effect The emission of electrons from a trap is thermally activated with an ionization energy E i = E C − E t . If the trap is in a strong electric field E, the emission probability can change. An acceptorlike trap after removal of the electron is neutral and its potential is short range. A donor has a longrange Coulomb potential after ionization. In an electric field, these potentials are modified as visualized in Fig. 10.30. Various additional processes can now occur.
10.11.1 Thermally Activated Emission For the δlike potential the ionization energy remains unchanged. For the Coulomb potential the barrier in the field direction is lowered by
ΔE i = e
e √ E. π 0 r
(10.60)
The emission rate en is increased in the field by exp (ΔE i /kT ). This effect is called the Poole–Frenkel effect [906] and can be quite important. For silicon and E = 2 × 105 V/cm and ΔE i = 100 meV a 50fold increase of the emission rate at room temperature is expected. As an example the Poole–Frenkel effect for the − electron emission from (neutral) interstitial boron in silicon (B0i → B+ i + e ) is
(a)
(b)
Ei Ei
Fig. 10.30 Field effect at (a) a δlike potential and (b) a Coulomb potential
376
10 Recombination E (V/cm) 103
2 10
0
3
10
4
2 10
4
4 10
4
Si:B
1
Electron emission rate en (s )
Fig. 10.31 Field effect for electron emission from interstitial boron in silicon (T = 65 K). The filled circles represent experimental data from DLTS, the data point marked with an empty circle is from EPR (zero field). The line is a linear fit and extrapolation. Adapted from [907]
102
101
100 0
50
100
E
1/2
150 1/2
)
200
)
√ shown in Fig. 10.31, following the enhancement of en ∝ exp( E). The extrapolation to E = 0 agrees with the EPR result [241, 907].5
10.11.2 Direct Tunneling Carriers can tunnel from the trap level through the barrier in the field direction into the conduction band. This process is temperature independent. The transmission √ factor of a barrier is (in WKB approximation) proportional to exp[−(2/) 2m [V (x) − E] dE]. The emission probability for a triangular barrier is then √ 3/2 eE 4 2m ∗ E i en = √ ∗ exp − . 3e E 4 2m E i
(10.61)
In the case of a Coulomblike potential the argument of the exponent in (10.61) needs to be multiplied by a factor 1 − (ΔE i /E i )5/3 with ΔE i from (10.60).
10.11.3 Assisted Tunneling In a thermally assisted tunneling process the electron on the trap level is first excited to a virtual level E t + E ph by phonon absorption and then tunnels out of the trap 5 The
slope of the line in Fig. 10.31 is slightly smaller than expected from (10.60).
10.11 Field Effect
377
(photonassisted tunneling). From the energetically higher level the tunneling rate is higher. The probability is proportional to exp E ph /kT . The additional energy can also be supplied by a photon (photonassisted tunneling).
10.12 Recombination at Extended Defects 10.12.1 Surfaces A surface (cmp. Chap. 11) is typically a source of recombination, e.g. through midgap levels induced by the break of crystal symmetry. The recombination at surfaces is modeled as a recombination current js = −e S (n s − n 0 ),
(10.62)
where n s is the carrier density at the surface and S is the socalled surface recombination velocity. The surface recombination velocity for GaAs is shown in Fig. 10.32. For InP, if the surface Fermi level is pinned close to midgap, the surface recombination velocity increases from ∼5 × 103 cm/s for a doping level of n ∼ 3 × 1015 cm−3 to ∼106 cm/s for a doping level of n ∼ 3 × 1018 cm−3 [908]. For Si, the surface recombination rate depends on the treatment of the surface and lies in the range between 1–104 cm/s [911]. The SiSiO2 interface can exhibit S ≤ 0.5 cm/s. Timeresolved measurements and detailed modeling for Si have been reported in [911].
Fig. 10.32 Surface recombination velocity for GaAs as a function of ntype doping concentration. Different experimental points correspond to different surface treatment methods. Dashed line is a guide to the eye. Experimental data from [912]
107
GaAs 106
105
104 1015
1016
1017
1018 3
1019
378
10 Recombination
(a)
(b)
Fig. 10.33 (a) Minority carrier lifetime in (ptype) silicon as a function of grain boundary size. The dashed line has the slope ∝ A. Data from [916]. (b) Linescan of the electron beam induced current (EBIC) perpendicular to a single grain boundary in silicon. The arrow denotes the position of the grain boundary. Compiled from [917]
10.12.2 Grain Boundaries Grain boundaries can be a source of nonradiative recombination. This is technologically important for solar cells made from polycrystalline silicon (cf. Sect. 22.4.6). The grain boundary can be understood as an inner surface in the crystal. Modelling of recombination at a grain boundary can be done using an interface recombination velocity [913, 914] or considering deep traps [915]. The minority carrier lifetime decreases with decreasing grain boundary area A (Fig. 10.33a). The carrier loss at a grain boundary can be imaged directly via the efficiency of the collection of an electron beam induced current (EBIC) as shown in Fig. 10.33b. The minority carrier lifetime is only unaffected when the average distance √ to a grain boundary is much larger than the minority carrier diffusion length, A L D , otherwise the entire grain volume is subject to nonradiative recombination.
10.12.3 Dislocations Also dislocations typically act as recombination centers, sometimes called carrier sinks. In Fig. 10.34 it can be seen that the minority carrier lifetime depends on the dislocation density n d and follows a τ −1 ∝ n d law, as if each dislocation is a recombination center [918]. The nonradiative recombination makes dislocations appear as ‘dark line defects’ in luminescence imaging [919]. In [920] also the decrease of carrier lifetime around (misfit) dislocations has been imaged. The effect of dislocations on the radiative recombination efficiency depends on the diffusion length [920].
10.13 ExcessCarrier Profiles
379
Fig. 10.34 Inverse minority carrier lifetime in ntype silicon (40 cm), low resistivity Ge (3–5 cm) and high resistivity Ge (30–40 cm). Data from [918]
10.13 ExcessCarrier Profiles In this section, some typical excesscarrier profiles (in onedimensional geometry) are discussed that arise from certain excitation conditions. The excesscarrier density Δp (here holes in an ntype semiconductor, i.e. Δp = pn − pn0 ) is determined by the diffusion equation (cf. (8.64a)) Dp
∂ 2 Δp Δp = −G(x) + . 2 ∂x τp
(10.63)
10.13.1 Generation at Surface First, the generation of excess carriers in a semiinfinite piece of semiconductor shall occur only at the surface at x = 0. The generation is zero everywhere else and the excitation is incorporated via the boundary condition Δp(x = 0) = Δp0 . The general solution for the homogeneous equation (10.63), i.e. G = 0, is x x + C2 exp , Δp(x) = C1 exp − Lp Lp with the diffusion length L p = ∞) = 0 the solution is
(10.64)
Dp τp . Taking the boundary condition Δp(x →
x Δp(x) = Δp0 exp − Lp
.
(10.65)
380
10 Recombination
In order to connect Δp0 with the total generation rate per unit area G tot , we calculate
∞ Δp0 L p Dp Δp(x) dx = = Δp0 . (10.66) G tot = τp τp τp 0
10.13.2 Generation in the Bulk Now, a generation rate following (9.16), realistic for photodiodes and solar cells, is considered, (10.67) G(x) = G 0 exp (−α x) , i.e. due to light absorption with the (wavelengthdependent) absorption coefficient α. The total generation rate is G tot =
∞
G(x) dx =
0
G0 . α
(10.68)
The total generation rate is equal to the number of photons per second Φ0 that enter the semiconductor. The solution of (10.63) is the sum of the homogeneous solution (10.64) and a particular solution that is given by Δp(x) = C exp (−α x) .
(10.69)
The constant C is determined to be C=
G 0 τp . 1 − α2 L 2p
Therefore, the solution is G 0 τp x x exp (−α x) . Δp(x) = C1 exp − + C2 exp + Lp Lp 1 − α2 L 2p
(10.70)
(10.71)
Using again Δp(x → ∞) = 0 (leading to C2 = 0) and a recombination velocity S at the front surface, i.e. ∂Δp . (10.72) − e S Δp0 = −e Dp ∂x x=0
10.13 ExcessCarrier Profiles
(a)
381
(b)
Fig. 10.35 Excess carrier density profile (10.73) in (a) linear and (b) semilogarithmic plot for S = 0 and S = ∞. Other parameters are given in panel (a)
The solution is given as Δp(x) =
S + α Dp G 0 τp x exp − exp x) − . (−α 1 − α2 L 2p S + Dp /L p Lp
(10.73)
For vanishing surface recombination, S = 0, the solution is (Fig. 10.35) Δp(x) =
G 0 τp x exp − exp x) − α L . (−α p 1 − α2 L 2p Lp
(10.74)
For αL p 1, (10.65) is recovered. This dependence is the excesscarrier profile if the absorption is strong, which is a tendency for short wavelengths. The current at the surface, j (x = 0) ∝ ∇ Δp, is zero. In the case of very strong surface recombination, S → ∞, (10.73) becomes G 0 τp x exp (−α x) − exp − , Δp(x) = 1 − α2 L 2p Lp
(10.75)
with Δp(0) = 0 (Fig. 10.35). The current at the surface is (Dp τp = L 2p ) G0 Lp α Lp ∂Δp = −e = −e Φ0 . j (x = 0) = −e D ∂x x=0 1 + α Lp 1 + α Lp
(10.76)
Part II
Selected Topics
Chapter 11
Surfaces
Gott schuf das Volumen, der Teufel die Oberfläche. God created the bulk; surfaces were made by the devil. attributed to W. Pauli
Abstract The specifics of semiconductors surfaces, their symmetry, equilibrium crystal shape, reconstructions, steps and faceting are summarized, being important for epitaxy. Physical surface properties such as vibrational and electronic states are discussed.
11.1 Introduction Obviously every crystal has a surface all around it, connecting it to the surrounding world. This represents a brutal perturbation of the bulk periodicity with the consequence of a whole new world of physics at the surface. With regard to semiconductor technology, the surface properties are of large importance in a number of instances: • The crystal growth of semiconductors always occurs at a surface. This subject will be discussed in Chap. 12. • The surface is subject to interaction with the chemistry of the surrounding atmosphere. This is of essential importance for catalysis, e.g. oxidation of CO at noble metals or photocatalytic water splitting, e.g. using TiO2 , into oxygen and hydrogen [921, 922]. Photocatalysis is briefly discussed in Sect. 22.1. The interaction and reaction with the surrounding atmosphere can lead modifications of the semiconductor such as change of conductivity, e.g. in SnO2 , which can be used in the construction of gas detectors [923–925]. • Surface passivation and barriers, e.g. using photoresist, silicon oxides or nitrides, are often necessary in practical devices in order to avoid surface recombination (Sect. 10.12.1) or the interaction with atmospheric oxygen or water. But surface physics is interesting in its own right, investigating the properties of a complex mostly twodimensional system. ‘Pure’ surfaces are studied using © Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_11
385
386
11 Surfaces
crystals cleaved in ultrahigh vacuum or carefully prepared atomically clean surfaces. A special case are twodimensional materials, also termed atomic sheets, such as graphene; these will be discussed in Sect. 18.1. At the surface the atoms rearrange, compared to their bulk positions, vertically and laterally, also forming new bonds (surface reconstructions). The mechanical properties (surface phonons) and electronic properties (surface states) are different from the bulk modes. Detailed treatments of surface physics and its experimental methods can be found in [617, 926–928].
11.2 Surface Crystallography The surface symmetry, i.e. the twodimensional spatial periodicity of the constituent atoms, is described with the ten twodimensional point groups (Table B.1). The point symmetries are 1, 2, 3, 4, and 6fold rotational symmetry (Fig. 3.4) with or without mirror plane(s). The twodimensional point symmetries of popular substrate orientations are compiled in Table 11.1; the different symmetry of the first layer and the halfspace are notable. The combination of five 2D Bravais lattices (cmp. Sect. 3.3.4) with the 10 2D point groups leads to the 17 twodimensional space groups (wallpaper groups) [929]. For the treatment of surface in reciprocal space, the threedimensional kvector is split into the twodimensional component k parallel and the onedimensional component k⊥ perpendicular to the surface, k = k + k⊥ .
(11.1)
The three most important Brillouin zones in twodimensional kspace are depicted in Fig. 11.1. Often the special points of the 2D Brillouin zones are denoted with a bar over the letter. Table 11.1 Twodimensional point symmetries of common substrates with ideal lowindex surfaces
Crystal Rocksalt
Surface
(001) (110) (111) Diamond (001) (110) (111) Zincblende (001) (110) (111) Wurtzite (00.1) (10.1) (11.0)
1st layer 1st & 2nd layers Half space 4 mm 2 mm 6 mm 4 mm 2 mm 6 mm 4 mm 1m 6 mm 6 mm 2 mm 2 mm
4 mm 2 mm 3m 2 mm 2 mm 3m 2 mm 1m 3m 3m 2 mm 2 mm
4 mm 2 mm 3m 2 mm 2 mm 3m 2 mm 1m 3m 3m 1m 1m
11.3 Surface Energy
387
Fig. 11.1 Twodimensional Brillouin zones for (a) square, (b) rectangular and (c) hexagonal surface symmetry. Special points are labelled and the grey areas indicate the smallest irreducible area
(a)
(b) X'
M
(c) J'
M
K
M
J
X
11.3 Surface Energy The surface energy, more precisely the surface energy per area γ, is related to the work that is necessary to split a crystal in two parts. Such process will leave broken (‘dangling’) bonds. This energy will depend on the crystal orientation as is already clear from the fact that there are easy cleaving planes (Sect. 5.4.2). The surface energy will also depend on the surface reconstruction (see Sect. 11.4), i.e. the rearrangement of surface bonds and atoms. Generally, the reduction of the number of dangling bonds on a surface lowers its energy, while the distortion of bonds increases its energy.
Table 11.2 Surface energy (in J/m2 ) for various C, Si and Ge surfaces Material {111} {110} {100}
{311}
C Si Ge
8.34 2.12 1.61
8.12 1.82 1.32
7.48 2.04 1.51
9.72 2.39 1.71
Data from [930]
(a)
(b) 0)
(111)
(11
(110)
(111) (113) (001) (113)
1.02
3) (0
(11
(111)
/ (111)
(113)
(111 )
)
01
1.01 1.00 0.99 0.98
(111)
(110)
0.97 0.96 90
Si 60
30
0
30
60
90
Angle (degree)
Fig. 11.2 (a) Equilibrium crystal shape (cross section in 110 azimuth) of 1.06 µm diameter Si bulb at T = 1323 K with facet orientations as labelled. (b) Anisotropy of surface energy (relative to γ(111)) for Si, the dashed line is guide to the eyes. Adapted from [931]
388
11 Surfaces
The anisotropy of the surface energy for a given orientation hkl, γ(hkl), determines the equilibrium crystal shape (ECS) at a given temperature (below melting temperature). The crystallite is assumed to be of at least mesoscopic size such that energy effects due to edges and apexes can be neglected compared to the surface energy terms. As an example theoretically calculated surface energy values for covalent semiconductors are listed in Table 11.2. The equilibrium shape of silicon has been observed for µmsized bulbs as shown in Fig. 11.2a for T = 1323 K ; the experimental anisotropy of surface energy of silicon is shown in Fig. 11.2b.
11.4 Surface Reconstruction When in a Gedankenexperiment the bulk crystal is split such that a surface with defined orientation develops, many bonds are cut. These dangling bonds can be saturated with other atoms such as hydrogen. In particular under vacuum conditions, the dangling bonds will rearrange and form new bonds such as dimers along the surface, lowering the total energy. This surface reconstruction displays twodimensional periodicity of a surface unit cell. Since the forces from the splitaway halfspace are missing, the atomic planes will rearrange vertically1 and the surfacenear layers will exhibit slightly different lattice spacing than in bulk. In [932] the surface reconstructions of many semiconductors are reviewed. In Fig. 11.3a the rearrangement of surface atoms on GaAs(110) is depicted as an example. The anion is moved up, the cation moved down, preserving the bond length, rotating the bond by about γ = 30◦ for various III–V semiconductors [933] (Fig. 11.3b). The height difference of the top anion and cation Δ1 scales with the bulk lattice constant (Fig. 11.3c). The details are specific to materials and orientations. Different reconstructions occur for different thermodynamical conditions, some of them being metastable, as depicted for GaAs(100) in Fig. 11.4. Several different surface reconstructions can also be present simultaneously at a surface within different domains. The stable reconstruction of the Si(111) surface is the somewhat complicated 7×7 reconstruction which is schematically depicted in Fig. 11.5a as proposed in [936] (‘DAS’ dimeradatomstacking fault model). A STM image of this surface has been reported first in [937] and is depicted in Fig. 11.5b. Details of this surface are also recently a subject of interest [938].
1 Typically
the distance between the first and second layer is reduced, and the distance between the second and third layer a little bit increased.
11.4 Surface Reconstruction
(a) Ga As
389
ideal
reconstructed
(c) (b)
[110]
[100] Fig. 11.3 (a) Schematic drawing of the GaAs(110) surface after cutting bonds (‘ideal’) and actual atomic rearrangement with asymmetric dimer in the reconstructed state. Adapted from [934]. (b) Schematic of the III–V (110) surface relaxation red circles: anions, blue circles: cations) with bond rotation ω and atom shift Δ. (c) Experimental values for he relaxation Δ1 as shown in panel (b) for various semiconductors versus their bulk lattice constant a0 ; dashed line is straight line as guide to the eyes. Data from [933]
(a)
(b)
(4 2)
0.2 0.1 c(4 4)
Energy (eV)
[110] [110]
0 0.1 0.2 0.3 0.4
2(2 4)
mixed dimer
2(2 4)
(2 6)
GaAs(100) 0.5
Ga chemical potential
0
(eV)
Fig. 11.4 (a) Various reconstructions of the GaAs(100) surface. Filled (empty) circles represent As (Ga) atoms. Atom positions in the top two atomic layers are indicated by larger symbols. (b) The relative formation energy per (1 × 1) unit cell of various reconstructions as a function of the Ga chemical potential. Vertical dashed lines mark the approximate anion and cationrich limits of the thermodynamically allowed range of Δμ. Adapted from [935]
390
11 Surfaces
(a)
(b)
[110]
1nm
[112] [111]
Fig. 11.5 (a) Schematic drawing of the 7 × 7 reconstruction of Si(111) surface. The large grey circles represent adatoms, the small balck circles rest atoms. Adapted from [936] (b) STM image (empty states) of such surface. Adapted from [937]
11.5 Surface Morphology The surface reconstruction is related to the local atomic arrangement of the surface atoms. On larger length scales, surfaces can exhibit roughness in general and various specific morphologies, among them steps, step bunches, facets, hillocks or pits. When atomically flat terraces are separated by steps of equal heights, the surface is termed vicinal. The step height can be an atomic monolayer or more. The step edges can be straight, smoothly curved or rugged, depending on the formation energy of kinks. If the substrate surface is inclined by a small ‘offcut’ angle θ with respect to a low index plane, for a step height h the average terrace width L is given by L=
h h ≈ . tan θ θ
(11.2)
The Si(001) surface (under certain conditions) exhibits monoatomic steps between the Atype 1 × 2 and Btype 2 × 1 terraces [939]; clearly also the step edges between A–B and B–A are quite different, one being much rougher than the other (Fig. 11.6). The surface is thus a two domain surface, the symmetry of both A and Btype terraces being 2 mm, rotated by 90◦ against each other. A similar example is the Zn(00.1) surface. The found step height of the monoatomic steps is 0.27 nm and corresponds c/2 [940]. The terrace width is about 12 nm (Fig. 11.7a), yielding an offcut (11.2) of about 1.3◦ . The surface pattern shows triangular features in two orientations, rotated by 60◦ . The 3 m symmetry of the surface, although the first monolayer has 6 m point symmetry (Table 11.1), occurs in two domains rotated against each other by 60◦ . The LEED pattern from each individual terrace is expected to have threefold symmetry; the mixed character of the surface yields a sixfold pattern (Fig. 11.7b). Steps can gather and form step bunches with a height much larger than a monolayer (Fig. 11.8). Faceting of higher index planes occurs when it is energetically favorable to
11.5 Surface Morphology
391
Fig. 11.6 STM image of Si(001) surface with an offcut θ = 0.5◦ . Adapted from [939]
(a)
(b)
10nm Fig. 11.7 (a) STM images a ZnO(00.1) Oterminated surface, left (right) panel with zero (about 1.3◦ ) offcut, exhibiting monolayer step heights of 0.27 nm. (a) LEED pattern of such surface (recorded at 70 eV). Adapted from [940] Fig. 11.8 SEM image of the surface of a 4HSiC layer on [00.1]oriented substrate with 8◦ misorientation towards [11.0]. Adapted from [942]
5µm
392
11 Surfaces (114)
(113) (114)
100nm
(113)
10nm
Fig. 11.9 STM images of a silicon surface close to (113), 21.5◦ from (001) towards (111), i.e. (113)3.7◦ . Adapted from [943]
form alternating facets of low energy low index planes, for example Si(223) exhibits periodic ridges with (111) and (113) facets [941]. The faceting of a surface close to (113), exhibiting smooth (113) and rough (114) planes, is depicted in Fig. 11.9.
11.6 Surface Physical Properties 11.6.1 Surface Phonons As a model for surface vibrational states, the diatomic onedimensional chain model discussed in Sect. 5.2.2 can be modified to allow for a different surface spring constant Cs instead of C1 or C2 . Such model can be solved numerically for finite chain length. The bulk dispersion is found with an extra mode in the gap or above the maximum frequency for a range of values of Cs as depicted in Fig. 11.10. When the spring constant of the surface atom is smaller than the larger of the two spring constants C1 and C2 (in our model calculation C2 > C1 ), a state in the gap forms; for a surface spring constant larger than C2 , first the surface vibration lies within the optical bulk band and then forms a state above the maximum optical frequency ωm , given by (5.18).2 In order to display the dispersion of surface states together with the bulk band structure, the latter is projected to the surface k vector: E n (k) is considered as E n,k⊥ (k ) = E ν (k ), where ν = n, k⊥ is a new, continuous index. In the plot of E nsurf versus k , for each value of k a range of energies reflects the bulk band structure, as shown in Fig. 11.11 for GaAs. This concept pertains to phonon dispersion as well as to electronic states. appearance of states within the gap and above ωm resembles that of localized vibrational modes of substitutional masses (Sect. 5.2.6). 2 The
11.6 Surface Physical Properties
393 C2
M2=M1 , C2=2C1
Frequency (ωmax)
1.0
0.5
0.0
0
1
2
3
4
Csurface (C1)
Fig. 11.10 Onedimensional model calculation of surface vibrational state frequency (in units of the maximum bulk optical phonon frequency ωm ) as a function of the spring constant Csurface of the surface atom replacing C1 (blue curve) or C2 (black curves). As model parameters we use equal masses and C2 = 2 C1 (γ = 0.943 from (5.17)). The grey areas represent the energy range of the acoustic and optical phonon bulk bands 40
GaAs (110)
Energy (eV)
30
20
10
0 J‘
J
Fig. 11.11 Surface phonon dispersion for GaAs(110) (solid lines) with the surface projected bulk band structure (light grey area). The symboles are experimental data from two different methods. The dark grey areas at about 10 meV indicate regions where the A1 peak is present in the calculated scattering crosssection. Adapted from [933]
11.6.2 Surface Plasmons Freecarrier oscillations in the bulk had been discussed in Sect. 9.8.1. A surface plasmon is the quantum of a surfacebound plasma oscillation. Such effect has been discussed in [944] and reviewed in [945, 946]. A metal (or conductive semiconductor)
394
11 Surfaces
Fig. 11.12 Sketch of surface plasmon field distribution. Adapted from [947]
with dielectric constant according to (9.65) 1 = m = r (ωp /ω)2 and a dielectric (or vacuum) with 2 = d are assumed (Fig. 11.12). The surface plasmon (polariton) (SPP) is a wave localized at the surface with evanescent parts into the metal and the dielectric. The dispersion of the surface plasmon (polariton) is given by kSPP
ω = c
1 2 . 1 + 2
(11.3)
For large k, the limiting frequency is the SPP frequency (from 1 = 2 ) ωp ωSPP = √ < ωp , 1 + d /r
(11.4)
which √ is smaller than the plasma frequency. For a metal against vacuum, ωSPP = ωp / 2. The SPP dispersion for a ZnO:Ga/air interface is depicted in Fig. 11.13 for three different doping concentrations.
0.9 20
n=7.2 10 cm
ZnO:Ga
0.8
3
1.5
n=3.2 1020cm3
0.6
2
0.5 0.4
3
n=1.2 1020cm3
4
0.3
5 0.2 10
0.1 0
0
2
4
6 6
8 1
Wave vector (10 m )
Wavelength (µm)
0.7
Energy (eV)
Fig. 11.13 Surface plasmon polariton dispersion for ZnO:Ga/air for three different carrier concentrations as labelled, experimental data (symbols) and theory (lines). Adapted from [948]
11.6 Surface Physical Properties
395
11.6.3 Electronic Surface States The bulk band structure is given by the energy eigenvalues E n (k). The surface adds its own states E nsurf (k ), many of them in the gap. The calculation of gap states has been already briefly discussed in Sect. 6.2.3. The nature of bulk states is oscillatory in the bulk and exponentially decaying in the outside (Fig. 11.14a), the nature of surface states is localized at the surface and decaying both towards the bulk and the outside (Fig. 11.14b). A third type of states is a surface resonance which is oscillatory in the bulk and has enhanced probability at the surface, of course also decaying towards the outside (Fig. 11.14c); such states are surface related but energetically degenerate with states of the bulk band structure. Surface states for Si(100) in 2 × 1 reconstruction are shown in Fig. 11.15. The surface bands arise from (filled and unfilled) π and π ∗ orbitals from the dangling bonds on the threefoldcoordinated surface atoms [949]. A calculation for the ideal (unreconstructed) (100), (110) and (111) surfaces of Si, Ge and GaAs can be found in [950]. Further work on silicon surface states (clean and with adsorbates) is compiled in [951]. For a conventional insulating material (with gap) the states of conduction and valence band have defined s and ptype symmetry (cmp. Fig. 2.5) and the surface states can be populated with spin up and down electrons as is schematically drawn in Fig. 11.16a. Such ‘normal’ surface states are thus not spinpolarized. This has been shown, e.g., for the wellknown surface states of Si(111)(7 × 7) [952] in [953]. In a socalled topological insulator [954], a band inversion is present. In HgTelike materials, s and ptype bands are inverted at the Γ point (cmp. Sect. 6.9.4). In layered
Fig. 11.14 Schematic wavefunction versus coordinate for (a) bulk state in the vicinity of the surface (its position indicated by the vertical dashed line), (b) surface state and (c) surface resonance state
(a)
(b)
(c)
396
11 Surfaces Si(100)(2 1)
Energy (eV)
2.0
1.0
0
1.0 J
M
J‘
Surface wave vector
Fig. 11.15 Surface band structure of Si(100)(2 × 1), lines denote a theoretical quasiparticle calculation, symbols represent experimental data. The grey areas indicate the projected bulk band structure. Adapted from [949]
(a)
(b)
E
E
k
k
Fig. 11.16 (a) ‘Normal’ band structure with surface states, the valence band states are antisymmetric (‘−’) from pstates, the conduction band states are symmetric (‘+’) from sstates. The arrows denote the electron spin orientation of the states. (b) ‘Topological’ band structure with surface states crossing the gap and electrons in the two surface states having unique spin orientations
(orthorhombic) Bi2 Se3 like trichalcogenide materials two pz orbitals with opposite parity are inverted at the Γ point. Reasons for the band inversion are spinorbit interaction but also scalar relativistic effects and lattice distortions [955]. The spinorbit interaction is responsible for opening a gap; the associated surface states cross the band gap (Fig. 11.16b) and are spinpolarized (Fig. 11.16c) [956, 957]. A review of various systems is given in [958]. Charge transport in such spinpolarized surface states suffers no scattering (thus these states are called ‘topologically protected’) unless by a center that breaks time reversal symmetry (magnetic impurity). The
11.6 Surface Physical Properties
397
0.4 0.3
Bi2Se3
Energy (eV)
0.2 0.1 0 0.1 0.2 0.3
Fig. 11.17 Density of states for Bi2 Se3 (111) surface. Adapted from [957] M
K
Bi2Se3
0.1 surface states
0.2 Dirac point
0.3 0.4 0.01
0
0.01
ky (nm1)
(b)
K
0.01
0
0.01
kx (nm1)
M
Intensity (arb. units)
Energy (eV)
M
ARPES intensity (arb. units)
(a) EF=0
M
Bi2Se3
0.01
0
0.01
ky(nm)1
Fig. 11.18 (a) Angleresolved photoemission spectra from Bi2 Se3 (111) surface along two different kspace directions. The Fermi level is at energy zero. The blue dashed line indicates the angular scan displayed in panel (b). (b) Spinpolarized momentum distribution curve at a binding energy of −140 meV, measured along the k y direction. Adapted from [960]
more or less linear dispersion of these states forms a ‘Dirac cone’ (cmp. Sect. 18.1.2 for the band structure of graphene with six Dirac cones). Topological surface (or interface) states have been observed in various systems [958]. As an example we show data on bulk Bi2 Se3 [959] for which the surface states are found to cross the band gap (Figs. 11.17 and 11.18a) and spinpolarized measurements (Fig. 11.18b) show a strong spin polarization (about 50 %) of the two branches.
Chapter 12
Heterostructures
The interface is the device. H. Kroemer [961]
Abstract Heterostructures are the most important basis for modern devices and are covered regarding various aspects including heteroepitaxy on planar and patterned substrates, surfactants, heterostructure band lineup as well as energy levels and recombination in planar confined systems (quantum wells and twodimensional electron gases).
12.1 Introduction Heterostructures consist of (at least two) different materials. The geometry of the interfaces between the two materials can be complicated. The simplest case is a planar interface, i.e. a layered system. A metal–semiconductor junction is generally a heterostructure. However, we will use the term mostly for structures of various semiconductors. Most of the heterostructures discussed here are epitaxial, i.e. fabricated by the successive epitaxy of the various layers on a substrate. Another method to fabricate heterostructures of different (and dissimilar) materials is wafer bonding that is briefly discussed in Sect. 12.6. Many modern semiconductor devices rely on heterostructures, such as the heterobipolar transistor (HBT), the high electron mobility transistor (HEMT), lasers and nowadays also lightemitting diodes. Shockley had already considered heterostructures in his 1951 patent for pnjunctions. For the development and the realization of heterostructures H. Kroemer and Zh.I. Alferov were awarded the 2000 Physics Nobel Prize. The properties of charge carriers in layers that are part of heterostructures can be quite different from those in bulk material, e.g. extremely high mobility, high radiative recombination efficiency or novel states of matter, as revealed in the quantum Hall effects. © Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_12
399
400
12 Heterostructures
12.2 Heteroepitaxy 12.2.1 Growth Methods Since the thickness of layers in the active part of heterostructures has to be controlled to monolayer precision and the thickness of layers can go down to the single monolayer range, special growth methods have been developed [962–964]. Among these molecular beam epitaxy (MBE [965]), chemical vapor deposition (CVD [966, 967]) and metalorganic vapor phase epitaxy (MOVPE [968]) are the most common for Si, Ge, III–V and II–VI semiconductors. In particular, oxide semiconductors are also fabricated with pulsed laser deposition (PLD [969]). Liquid phase epitaxy (LPE [970]) used to be very important for the fabrication of LEDs but has lost its role largely to MOVPE. MBE is performed in an ultrahigh vacuum (UHV) chamber, pumped by getter pumps and cryoshrouds. The source materials are evaporated from effusion cells and directed towards the heated substrate. If the source materials are supplied as a gas stream, the method is called gassource MBE (GSMBE). If metalorganic compounds are used as precursors, the method is denoted as MOMBE. The atoms impinge on the substrate with thermal energy and are first physisorbed. After diffusion on the surface they either desorb or they are chemisorbed, i.e. incorporated into the crystal. In order to obtain high spatial homogeneity of material properties such as composition, thickness and doping, the substrate is rotated during deposition. During CVD and MOVPE the heated substrate is in a gaseous environment. The transport gas is typically H2 , N2 or O2 . Precursor materials are hydrides such as silane, germane, arsine or phosphine (SiH4 , GeH4 , AsH3 , PH3 ) and (for MOVPE) metalorganic compounds, such as, e.g. trimethylgallium (TMG). Due to the toxicity of the hydrides, alternative, i.e. lesstoxic and lessvolatile compounds are used, such as TBAs ((CH3 )3 CAsH2 ). The crystal growth occurs after pyrolysis and catalysis of the compounds close to or on the substrate surface. All remaining C and H atoms (and whatever else that is not incorporated into the crystal) leave the reactor and are neutralized and stopped in a scrubber. Insitu monitoring is of importance to obtain information about the growth process while it is underway. Using the information in a feedback loop it is possible to achieve insitu control of the process, e.g. for precise determination of growth rates or layer thickness. Techniques are RHEED (reflection highenergy electron diffraction) [971] (only for UHV systems) and RAS (reflection anisotropy spectroscopy) [972, 973].
12.2.2 Substrates Thinfilm epitaxy is mostly performed on wafers, i.e. thin circular slices of substrate material. The most common substrate materials are Si (currently up to 400 mm diameter [974, 975]), Ge (also up to 300 mm [976]), GaAs (up to 6 inch), InP (up to 4 inch)
12.2 Heteroepitaxy
401
and sapphire (up to 6 inch). Typical wafer thickness is 300–500 µm. Also, very thin, flexible Si wafers (8–10 µm) have been developed [977]. A wafer is cut from a large single cylindrical crystal that is fabricated with suitable growth techniques such as Czochralski (CZ) growth (1918) modified by Teal and Little [978, 979]. In CZ growth the crystal is pulled from a seed crystal out of a melt of previously polycrystalline, pure or doped material. All dislocations stop in the narrow neck between the seed and the main body of the cylinder. The diameter of the crystal is controlled by the pulling rate and the heating power. For the growth of III–V compound semiconductors liquid encapsulated CZ (LEC) growth has been developed to counteract the high volatility of the growthV component. During LEC growth the melt is completely covered with molten boric oxide (B2 O3 ). The keys to optimization of the crystal growth process are numerical modeling and computer control. In Fig. 12.1a,c a large CZ silicon crystal and a smaller LEC GaAs crystal (boule) are shown. Over time wafer size and ingot mass have increased remarkably (Fig. 12.1b). For details on other important fabrication methods for bulk crystals, including floatzone (FZ [980]) or vertical gradient freeze (VGF), we refer to the literature [981]. Significant expertise is necessary for cutting, grinding and polishing (lapping) wafers for epitaxy. For semiconductors, the wafer is marked with flats to indicate orientation and doping. In Fig. 12.2 the standard flats are shown for (100) and (111)oriented material. The primary (major) flat (OF, orientation flat) defines the crystallographic
(a)
(b)
(c)
Fig. 12.1 (a) Silicon single crystal for 300mm diameter wafers after opening of the crucible. From [982] with permission. (b) Historic development (first year of larger production) of silicon wafer diameter and ingot mass. Data from [975]. (c) GaAs single crystal (boule) for 4inch wafers and some cut and polished wafers
402
12 Heterostructures
S S P
P
S
P
P
Fig. 12.2 Schematic semiconductor wafer geometry for various orientations and doping with the primary (P) and secondary (S) flats indicated
(a)
(b)
(c)
Fig. 12.3 (a) AFM images of an asreceived ZnO wafer, exhibiting small terraces and nm deep ¯ wafers with vicinal surfaces after thermal treatment scratches from polishing. (b, c) Two ZnO (0001) (1000 ◦ C for 2 h in O2 ), exhibiting atomically flat terraces with c/2 monoatomic step heights. Two different substrates with different offcut (misorientation direction and angle) are shown. Adapted from [990]
orientation1 is longer than the secondary (minor) flat which defines the conductivity type (IF, identification flat). For a 4inch (100 mm) diameter wafer the OF is 32 and the IF 12 mm long. The front surface, on which the epitaxy is performed, typically undergoes an elaborate cleaning and polishing process. Silicon processes [981, 984] are based on the RCA cleaning procedure [985] and the related Shiraki etch [986] and can achieve clean, atomically flat surfaces [987]. IIIV semiconductors are typically prepared using a polishing etch [988, 989], often solutions containing bromine. It is possible to create compound semiconductor surfaces that exhibit large, essentially monoatomically flat terraces between individual surface steps. Polishing or other surface damage can also be removed prior to epitaxy with thermal (Fig. 12.3) or ion beam treatments. ¯ surface, in the ‘EJ’ definition, the primary the ‘US’ flat definition, the primary flat is the (011) ¯ flat is (01¯ 1).
1 In
12.2 Heteroepitaxy
403
(b) (a)
Fig. 12.4 Crosssectional TEM of MBEgrown Alx Ga1−x As/GaAs heterostructures for (a) x = 0.41 and (b) x = 1.0. Using an AlAs/GaAs superlattice an excellent flattening of substrate roughness is achieved. From [991]
One prerequisite for making highquality heterostructures with thin layers is a flat surface. Even if the polished substrate is not perfect, flat interfaces can be achieved with the growth of appropriate superlattice buffer layers (Fig. 12.4). Roughness can exist on all length scales and is typically investigated using atomic force microscopy scans. High throughput demands and the advent of multiwafer reactors make prior cleaning and etching procedures tedious. For this purpose, substrates for welldeveloped material systems are offered ‘epiready’. Epiready wafers are often covered with a very thin protective film that can be released using a thermal treatment at or below typical growth temperature in the growth reactor immediately prior to epitaxy. The protective film separates the polished semiconductor wafer from the ambient. Examples are a few monolayers of arsenic on GaAs or two monolayers GaN on SiC. However, the suitability of a purchased substrate may depend on the duration and conditions of its storage. A special case is the use of curved substrates which allow the study of growth on different crystal orientations in a continuous fashion. Such experiments have been performed using cylindrical substrates [992] and hemispherical crystals. For the latter homoepitaxy has been reported for Si [993, 994], SiC [995] or GaAs [996]. Also heteroepitaxy has been investigated, for example for GaP and GaAs on Ge [997] (cmp. Fig. 12.12). Using such curved substrates, the growth rate can be determined as a function of crystal orientation as shown for GaAs (on GaAs) in Fig. 12.5; large differences are found for (111)A and (111)B surfaces. For growth of silicon the variations with angle are much smaller in the range of 10 % [992].
12.2.3 Growth Modes The growth of a material A on a material B can occur via three fundamental growth modes (Fig. 12.6), the layerbylayer or Frankvan der Merwe (FvdM) growth mode [384], the island or VolmerWeber (VW) growth mode [998] and the
404
12 Heterostructures (110)
(111)B
(113)A (001) (113)B (111)A
(110)
140
GaAs
Growth rate (µm/h)
120 100 80 60 40 20 0
90
60
30
0
30
60
90
Angle (degree)
Fig. 12.5 Growth rate of GaAs in vapor phase transport at 725◦ as a function of crystal orientation. The dashed line is guide to the eyes. Adapted from [996]
(a)
(b)
(c)
Fig. 12.6 Schematic of the three different fundamental epitaxial growth modes
StranskiKrastanow (SK) growth mode [999]. In [999] the possibility of island formation on an initially flat heteroepitaxial surface was proposed for the growth of latticematched ionic crystals that have different charges. The term SK growth is now typically used in latticemismatched heteroepitaxy for the island formation (and related relaxation of strain energy, cmp. Fig. 14.26) on an initially twodimensional layer (wetting layer).2 Also growth of islands relaxed by misfit dislocations in strained heteroepitaxy has been termed SK growth [1000]. The growth mode is determined by the relation of the free energies (per area) of the surface σs , interface σi and film σf . Wetting of the substrate and growth of a coherent film (FvdMgrowth) occurs for σs > σ i + σ f .
(12.1)
If the inequality has the opposite sign, VolmerWeber or StranskiKrastanow growth occurs. Additionally the strain energy of the film must be considered. The SK growth 2 This
is the growth mode of selfassembled epitaxial quantum dots as discussed in Sect. 14.3.3.
12.2 Heteroepitaxy
405
Fig. 12.7 HRTEM cross section of the interface region of MOVPE grown hexagonal AlN on 6HSiC substrate. Adapted from [1004]
2HAlN
6HSiC 1nm
generally occurs when there is wetting of the substrate but layer strain is unfavorable and leads to islanding. Layerbylayer growth typically involves nucleation of twodimensional islands and ‘filling’ of the remaining monolayer before the next one is started. Another growth mode resulting in smooth epitaxial layers is stepflow growth where adatoms are incorporated mainly at step edges. A more detailed discussion can be found in [1001]. Further details on crystal growth can be found in [1002]. The nucleation and the initial film growth are important and determine the film quality. Several techniques have been developed to overcome common problems. A typical strategy is the growth of a lowtemperature nucleation layer.
12.2.4 Heterosubstrates If homosubstrates are not available or very expensive, semiconductors are grown on dissimilar substrates, e.g. (Al,Ga)N and ZnO on sapphire (Al2 O3 ) or SiC.3 In Fig. 12.7 the interface region of hexagonal AlN on 6HSiC (cmp. Fig. 3.28b) is shown. The change of crystallographic phase is obvious; the perfect atomic arrangement justifies the term ‘epitaxy’, literally meaning ‘order on top’. In many cases, the integration of III–V or II–VIbased semiconductors for optoelectronic applications on silicon for electronic devices is desirable, such as GaAs/Si, InP/Si, GaN/Si or the growth on economic substrates is attractive such as GaN/Al2 O3 and ZnO/Al2 O3 . For all such combinations the epitaxial relationship, i.e. the alignment of the crystallographic directions of both materials, which can have different space groups, has to be considered. Some examples for epitaxial relationships are given in Table 12.1. The epitaxial relation is determined by the energetically favorite formation of the interface and the early stages of growth.
3 For
ZnO, homosubstrates have recently been produced with 3inch diameter [1003].
406
12 Heterostructures
Table 12.1 Epitaxial relationship for various film/substrate combinations, ZnO (or GaN) on c, aand r sapphire and Si(111) ZnO Al2 O3 ZnO Al2 O3 ZnO Al2 O3 ZnO / GaN Si ¯ [00.1] [11.0] [10.2] [111] ¯ [00.1] [00.1] [00.1] [11.0] [11.0] [10.2] [00.1] [111] ¯ ¯ ¯ [01.0] [11.0] [00.1] [00.1] [01.1] –/ [21.0] [110] [11.0]
Fig. 12.8 Xray diffraction intensity from the asymmetric ZnO (10.4) (upper panel) and the sapphire (10.10) (lower panel) reflections as a function of the azimuthal sample orientation (rotation angle φ around the [00.1] axis). The peaks appear at different tilt angles ω due to an overall tilt of the mounted sample (dashed sinusoidal lines). The ZnO [00.1] axis is not tilted with respect to the sapphire [00.1] direction
Tilt
(deg)
0.4
=30°
0.2 0 0.2 0.4
ZnO (1 0.4)
Tilt
(deg)
0.4 0.2 0 0.2 0.4
Al2O3 (1 0.10)
180
90
0
180
90
(deg)
In Fig. 12.8, Xray diffraction data are shown from a ZnO layer on coriented sapphire. The hexagonal ZnO lattice is rotated by 30◦ with respect to the trigonal sapphire lattice. In the case of growth of ZnO on Si(111) an amorphous SiO2 layer can form at the interface such that the crystallographic information of the substrate is lost. The ZnO grains exhibit random inplane orientation (Fig. 12.9). If substrate and epilayer have different space groups, the formation of domains can occur [1006]. The twodimensional symmetries of various substrates are listed in Table 11.1. The group theoretical minimum number of domains NRD in dependence of the twodimensional symmetries of substrate and epilayer with rotational symmetries Cn and Cm , respectively, is given by [1007] NRD =
lcm(n, m) , m
(12.2)
12.2 Heteroepitaxy
407
(a)
(b)
(c)
Fig. 12.9 (a) Planview TEM image (inset: electron diffraction diagram averaged over several grains) of ZnO on Si(111).(b) Crosssectional TEM of the same sample. (c)Highresolution crosssectional image of the ZnO/SiO2 /Si interface region. Adapted from [1005]
where lcm denotes the least common multiple. The values are listed in Table 12.2 and visualized in Fig. 12.10. If the main symmetry axes of substrate and epilayer are not aligned, mirror domains appear. An example is the growth of GaN(00.1) on Ge(111), for which it has been reported that the major symmetry directions do not align exactly. There ¯ inis a 4◦ inplane rotation of the lattices with respect to the usual [11.0] [110] plane relationship [1008] (cmp. the exact alignment for GaN/Si(111) in Table 12.1).
408
12 Heterostructures
Table 12.2 Number of rotational (or mirror) domains NRD for all 2D point groups of substrate (G S ) (rows) and epilayer (G E ) (columns). When two numbers are given (xy), the first (second) number represents the number of domains if mirror symmetry planes of substrate and epilayer align (misalign). G S \G E 1 m 2 2 mm 3 3m 4 4 mm 6 6 mm 1 2 2 4 3 6 4 8 6 12
1 12 2 24 3 36 4 48 6 612
1 2 1 2 3 6 2 4 3 6
Fig. 12.10 Visualization of the minimum number of rotational domains for different substrate and epilayer symmetries according to Table 12.2
1 12 1 12 3 36 2 24 3 36
1 2 2 4 1 2 4 8 2 4
epi
1 m 2 2 mm 3 3m 4 4 mm 6 6 mm
1 12 2 24 1 12 4 48 2 24
2
1 2 1 2 3 6 1 2 3 6
3
1 12 1 12 3 36 1 12 3 36
4
1 2 1 2 1 2 2 4 1 2
1 12 1 12 1 12 2 24 1 12
6
sub 2
3
4
6
Due to 3 m mirror symmetry of the substrate, the misaligment is equivalent for clockwise and counterclockwise rotation. Therefore two domains with an angle of 8◦ occur (Fig. 12.11). Another wellknown domain effect in heteroepitaxy is the occurrence of antiphase domains of zincblende semiconductors (e.g. GaAs, GaP, InP,...) grown on Si(001) with monoatomic steps; such surface actually exhibits two kind of terraces (1 × 2 and 2 × 1 reconstructions) and is thus itself not homogeneous. The formation of antiphase domains can be avoided by using an offcut of the surface against the (001)planes promoting doubleatomic steps [1009]. In Fig. 12.12a the growth of GaP on a Ge
Fig. 12.11 Xray diffraction φscans of GaN(00.1)/Ge(111). Adapted from [1008]
409
Xray Intensity (arb. units)
12.2 Heteroepitaxy
GaN(10.1) Ge(220)
0
=8°
90
180
270
(degree)
hemisphere with [111]pole is depicted; spherical triangles meeting at the 100 poles can be seen. In a similar experiment GaAs was grown in a spherical depression in Ge(001) (Fig. 12.12b), allowing a more detailed look at the [001]pole. Close to the it, within an approximately square area, antiphase domains (cmp. Sect. 4.4.4) form. Along the connection lines between different 001poles, an antiphase domain boundary forms, microscopically broken up into domains [997]. Details of the initial deposition steps can determine the orientation in polar materials. GaN directly grown on cAl2 O3 grows with Nface orientation (see Fig. 3.19). The high surface mobility of Ga allows nitrogen to take its preferred position in the first atomic layer. Even under Garich conditions the N atoms can kickoff the Ga from its favorite site on the surface. If an AlN buffer is used the strong bond between Al and oxygen leads to an Al atomic layer at the interface and subsequent GaN grows with a Gaface [1010].
(a)
(b)
2mm 10µm
Fig. 12.12 The morphology of (a) GaP grown on a Ge hemisphere with [111]pole and (b) GaAs grown in a Ge(001) spherical depression. Adapted from [997]
410
12 Heterostructures
12.2.5 Patterned Substrates Using patterning of the substrate certain growth modes and crystallographic directions of the growth front can be evoked. ¯ growth of wurtzites, on a sapphire Returning to the discussion of [00.1] or [00.1] substrate with lateral AlN patterns, laterally orientationmodulated GaN can be grown (Fig. 12.13). At the juncture of the phases an inversion domain boundary forms [1011]. The defect density can be reduced in parts of the structure using epitaxial lateral overgrowth (ELO) [1013]. The defects thread only from the limited contact area of the layer with the substrate and the part of the layer away from the mask (‘wing’) is free of defects (Fig. 12.14). While the patterning of a mask may be cumbersome and require interruption of growth, the insitu deposition of a random SiN mask with small holes has been found beneficial in the epitaxy of GaN [1014]. GaN islands nucleate selectively in the mask openings (Fig. 12.15a). The nucleation and subsequent coalescence of islands (Fig. 12.15b) leads to defect annihilation and eventually again to a flat film (Fig. 12.15c). The reduction of defect density is evident (Fig. 12.15d) and leads to improved optical properties [1015].
(a)
(b)
(c)
(d)
Fig. 12.13 Side view of the heterointerfaces between AlN and coriented sapphire with nitrogen (a) and Al (b) being the first layer. Adapted from [1010]. (c) Phase image of piezoresponse force microscopy (PFM) of lateral polarity GaN heterostructure and (d) linescan of phase signal along white line in part (c). Adapted from [1012], part (c) reprinted with permission, © 2002 AIP
12.2 Heteroepitaxy
411
Fig. 12.14 SEM crosssectional image of GaN grown on a structured Si(111) substrate. The laterally grown wings extend about 2.5 µm over the grooves. The thickness of the GaN layer is 0.5 µm on the bottom of the grooves, while it is 1.4 µm on top of the ridges. Reprinted with permission from [1013], © 2001 AIP
(a)
(b)
(c)
(d) GaN
SiN mask
GaN
sapphire
Fig. 12.15 SEM images of GaN (a) growing through the openings of a random SiN mask, (b) laterally overgrowing the mask and coalescing and (c) eventually forming a flat film. Bar widths are 2, 1 and 10 µm. (d) Crosssection TEM image. Adapted from [1014]
Using patterned substrates with stripelike mesas and promoting the growth on a sidewall of the mesa, the direction of GaN growth front can be steered into a semipolar direction (cmp. Sect. 15.4.3). The rplane sapphire substrate with etched mesa stripes oriented along the [11.0] direction exposes [00.1]oriented sidewall facets on which the GaN grows along its caxis; The angle of 57.6◦ between the r and the cplanes of sapphire is very close to the angle (3.21c) of 58.4◦ between the GaN semipolar (11.2) and the (00.1) plane. The flat growth front represents a
412
12 Heterostructures
Fig. 12.16 SEM crosssectional image of MOVPE GaN grown on patterned rsapphire exposing a (11.2) growth front. Based on SEM image courtesy of F. Tendille
GaN
[11.2] C [00.1] [11.3] M [11.0]
R [11.2] C [00.1]
A [11.0]
rAl2O3
1 µm
(11.2) facet [1016] (Fig. 12.16). After coalescence of grains from various mesas, a flat (11.2) surface arises, allowing the reduction of various defects including basal stacking faults [1017, 1018].
12.2.6 Pseudomorphic Structures Heterostructures can generally be made from any sequence of materials. However a mismatch in lattice constant (or a different crystal structure) leads to strains and stresses that are of the order of 103 atmos for strains of 1 % (σ ∼ C, C ≈ 5 × 1010 Pa) as discussed in Sect. 5.3.3. The total strain energy is ∝ C2 . Above a critical thickness h c ∝ −1 (cf. Sect. 5.4.1) defects, e.g. misfit dislocations (relaxing strain with their edge components), are generated (Sect. 12.2.7). There are a number of semiconductor combinations that are lattice matched and thus can be grown with arbitrary thickness. Alx Ga1−x As is closely lattice matched to GaAs for all Al concentrations. See Fig. 6.21 for latticematched pairs, e.g. In0.53 Ga0.47 As/InP. Often, thin layers of latticemismatched materials with thickness smaller than the critical thickness are used. For many device applications the ability to grow pseudomorphic layers thicker than the critical layer thickness would be beneficial. The use of compliant substrates was proposed in [1019] to meet this demand. A recent review on compliant substrate technologies can be found in [393]. Schemes to accommodate part of the mismatch strain in the substrate include the use of cantilevered membranes, silicononinsulator, twist bonding, glass bonding or trenched substrates. In this sense also nanowhiskers (Sect. 14.2.3) represent a compliant substrate, enabling the growth of coherent (laterally confined) layers thicker than the critical thickness of a 2D layer (cmp. Fig. 14.9).
12.2 Heteroepitaxy
413
12.2.7 Plastic Relaxation Above the critical thickness, a film will relax plastically by forming misfit dislocations. The crosshatch pattern at the surface due to misfit dislocations is shown in Fig. 12.17. A TEM image of an array of misfit dislocations can be found in Fig. 5.33b. The strain relaxation in mismatched heteroepitaxy can be determined experimentally via the wafer curvature of the heterostructure (Sect. 5.3.5). Data for the thickness dependent relaxation (d) of In0.15 Ga0.85 As on GaAs (mismatch ≈1%) are shown in Fig. 12.18. Growth interruptions lead to larger relaxation at smaller thickness. Therefore relaxation at early times or small thickness (above h c ) is kinetically hindered, i.e., the available dislocation density and glide velocity are not sufficient to relieve the strain. At large thickness the strain does not go to zero (saturation regime) and the film remains in a metastable, incompletely relaxed state as discussed in more detail in [1020]. An extreme case of plastic relaxation is cracking (Sect. 4.4.1) which can occur for example in thick films during cooling due to the mismatch of the thermal expansion coefficients of substrate and epilayer (Fig. 12.19). Such cracking can be avoided by the introduction of suitable stressrelaxing layers and growth on predefined mesas [1021, 1022].
Fig. 12.17 Optical image of the surface of a supercritical, plastically relaxed Inx Ga1−x As film on GaAs. Image width is about 1 mm. The crosshatch pattern is due to misfit dislocations ¯ A along [110] and [110]. pseudomorphic layer would exhibit no contrast under the given conditions
414
12 Heterostructures
Fig. 12.18 Average film strain (measured insitu via substrate curvature) of In0.15 Ga0.85 As/GaAs grown at 450◦ C as a function of film thickness (determined from growth time × deposition rate). Relaxation for three different growth modes are shown (as labeled): continuous growth, employment of several growth interruptions (GRI) and GRI with annealing step (to 550◦ ). Adapted from [1020] Fig. 12.19 1 × 1 mm2 top view with a differential interference contrast microscope of a 1.3µm thick GaN layer grown on Si(111). Reproduced with permission from [1021], © 2000 IPAP
12.2.8 Surfactants The condition (12.1) allows layerbylayer growth (cf. Sect. 12.2.3), i.e. the substrate surface free energy is higher than the than the total of interface and film surface free energy. This makes wetting energetically favorable. For two elements A and B, one of them must have the lower surface free energy. If A can be grown on B in Frankvan der Merwe (or StranskiKrastanow) growth mode, then (12.1) does not hold for B on A and the growth will occur in VolmerWeber mode, i.e. with islands. This is a serious problem for the growth of embedded layers of the type A–B–A. If the embedded film grows well, the capping does not and vice versa.
12.2 Heteroepitaxy
(a)
415
(c)
(b)
Fig. 12.20 (a, b) 10 nm thick Ge layer on Si (100) deposited at room temperature with MBE and annealed up to 770◦ C without (a) and with (b) Sb surfactant. Adapted from [1030]. (c) Crosssection TEM image of a heterostructure of 70 monolayers germanium on Si (111), grown by MBE with Sb surfactant. The horizontal arrow labeled ‘I’ denotes the position of the interface. The arrows labeled ‘D1’ and ‘D2’ denote the positions of partial dislocations (cmp. Fig. 4.19). Adapted from [289]
In the case of Ge on Si, Ge has the lower surface free energy than Si. Ge grows on Si in StranskiKrastanow mode [1023] (Fig. 12.20a). Si grows both on Ge(001) and Ge/Si(001) in a VolmerWeber mode [1024] causing severe problems for the fabrication of Si/Ge/Si quantum wells or superlattices. A substantial modification of growth mode can be achieved by using a third element C as a capping layer, saturating surface bonds. It lowers the surface free energy of both materials A and B, thus favoring wetting of the substrate. Such element C is called surfactant (surfaceactive species) [1025, 1026]. Typical examples are As [1025] or Sb [289] on Si and Ge (Fig. 12.20b). Also the surfactant modifies defect nucleation and can lead to defectfree epitaxial Ge/Si layers (Fig. 12.20c). Surfactants have also been described for the growth of compound semiconductors, e.g. In [1027] or Sb [1028, 1029] for GaAs.
12.3 Energy Levels in Heterostructures 12.3.1 Band Lineup in Heterostructures In heterostructures, semiconductors with different band gaps are combined. The relative position of conduction and valence band (band alignment) is determined by the electron affinities χ as shown in Fig. 12.21. For a semiconductor, the electron affinity is the (positive) energy difference between vacuum level and conduction band edge. It can lead to different types of heterostructures. Early perspectives of semiconductor heterostructures are discussed in [1031].
12 Heterostructures
0
Si Ge SiC AlN GaN InN AlP GaP InP AlAs GaAs InAs AlSb GaSb In S b ZnO ZnS Cd S Zn S e Cd S e ZnTe CdTe Al2O3 Ga2O3 In2O3
416
1 2 Sm
3
Mg In Al Sn Au Ag
4 5 6 7 8 9
Fig. 12.21 Position of conduction and valenceband edges for a variety of semiconductors (relative to a common vacuum level at E = 0 eV). Based on values from [1032], for Al2 O3 (on InP) from [1033], for Ga2 O3 (on GaN) from [1034] for In2 O3 (on Si) from [1035, 1036]. On the right hand side the work functions of several metals are shown for comparison.
Evac
(a)
(b)
(c)
2
Electron energy
1
1
EC Eg1
2
2 1
Eg2
Eg2 Eg2
Eg1
EC,V Eg1
EV Spatial coordinate
Fig. 12.22 Position of band edges (band alignment) in (a) typeI, (b) typeII and (c) typeIII heterostructure.
In Fig. 12.22, the band alignment for typeI, typeII and typeIII heterostructures are shown. In the typeI structure (straddled band lineup) the lower conductionband edge and the higher valenceband edge are both in the material with smaller band gap. Thus, electrons and holes will localize there. In the typeII structure a staggered lineup is present and electrons and holes will localize in different materials. In the typeIII structure, also termed ‘broken gap’ structure, the conduction band of one material is below the valence band of the other material. The technologically most relevant are typeI structures. The design of heterostructures to fulfill a certain device functionality or to have certain physical properties is called ‘band gap engineering’.
12.3 Energy Levels in Heterostructures
(a)
417
(b)
(d)
(c)
(e)
Fig. 12.23 Heterostructures with different layer sequences (band gap engineering). (a) quantum well (QW), (b) multiple quantum well (MQW), (c) superlattice (SL), (d) singlebarrier tunneling structure, (e) doublebarrier tunneling structure
In a typeI heterostructure, the conduction and valenceband discontinuities are given, respectively, by ΔE C = χ1 − χ2 ΔE V = (χ1 + E g1 ) − (χ2 + E g2 ).
(12.3a) (12.3b)
Depending on the layer sequence of high and lowbandgap materials various configurations, as shown in Fig. 12.23 have obtained special names, such as single heterointerface, quantum well (QW), multiple quantum well (MQW), superlattice (SL). In the extreme case the layer is only one monolayer thick (Fig. 12.24) and the concept of layer and interface blurs. Such atomically precise layer sequences are mastered nowadays for a variety of material systems such as (Al,Ga)As/GaAs/InAs, InP/(In,Ga)As, Si/SiGe, ZnO/(Mg,Zn)O and also BaTiO3 /SrTiO3 . The abruptness of interfaces is determined by the epitaxial machine through the switching precision of the incoming material flux and fundamentally limited by segregation phenomena which can be modeled with a segregation coefficient [1037] (cmp. Sect. 4.2.4). As shown in Fig. 12.24c, In has the tendency to be carried into the following GaAs layer. A quantitative evaluation is possible using aberrationcorrected scanning transmission electron microscopy [1038].
12.3.2 Quantum Wells The energy in a single quantum well of thickness L z (along the growth direction z) can be calculated with the quantummechanical particleinabox model. In the envelope function approximation (Appendix H) the wavefunction is written as a product of the Bloch function and the envelope function χ(z). Ψ A,B (r) = exp (i k⊥ r) u nk (r) χn (z),
(12.4)
418
12 Heterostructures
(a)
InAs
(b)
(c)
Fig. 12.24 Ultrathin heterostructures: (a) Crosssectional TEM of a MOVPEgrown shortperiod superlattice (SPS) of InAs layers in GaAs1−x Nx ). In high resolution (right image), the individual rows of atoms can be seen. From [1039]. (b, c) Crosssection STM image of 2 ML InAs on GaAs; the segregation of In into the top layer is visible atom by atom. Adapted from [1040]
where ‘A’ and ‘B’ denote the two different materials. The envelope function χ fulfills, approximately, the onedimensional Schrödingertype equation, 2 ∂ 2 − ∗ 2 + Vc (z) χn (z) = E n χn (z), 2m ∂z
(12.5)
12.3 Energy Levels in Heterostructures
419
(a)
n=3
(b)
n=2 n=2
n=1
n=1
Lz
Lz
Fig. 12.25 Schematic energy levels and wavefunctions in a potential well with (a) infinite barriers, and (b) finite barrier height
where m ∗ denotes the effective mass. Vc is the confinement potential determined by the band discontinuities. Typically, Vc = 0 in the well and V0 > 0 outside in the barrier. E n are the resulting energy values of the quantized levels. In the case of infinite barriers (V0 → ∞, Fig. 12.25a) the boundary conditions χ(0) = χ(L z ) = 0 yield nπ 2 Lz nπ z , χn (z) = An sin Lz 2 En = 2m ∗
(12.6) (12.7)
where E n is called the confinement energy. For finite barrier height V0 (Fig. 12.25b) the calculation leads to a transcendental equation. The wavefunction tunnels into the barrier. While for infinite barrier height the lowest level diverges for L z → 0, for finite barrier height E 1 → V0 . A complication arises from the different effective mass in the well and barrier material. This is taken into account by forcing the continuity of χ and χ /m ∗ across the interfaces4 (‘BenDanielDuke’ boundary conditions [1042]). The Schrödinger equation and (semi)analytical solutions for special and numerical methods for
1 ∂χ 4 The kinetic energy term in (12.5) is written as 2 ∂ 2 ∂z m ∗ (z) ∂z
[1041].
for varying mass across the structure
420
12 Heterostructures
(a)
(b)
(c)
(d)
Fig. 12.26 Schematic representation of the development of hole levels in a quantum well: (a) degenerate bulk levels at Γ , (b) splitting at the subband edge (due to different quantized values of k z ), (c) inplane dispersion (mass reversal), (d) anticrossing behavior. Based on [991]
arbitrary potential distributions are discussed in [1043]. The application of k · p theory (Appendix G) to heterostructures is discussed in [1044]. The motion of carriers in the plane is still free and has a twodimensional dispersion. Thus, each quantized level contributes m ∗ /(π2 ) to the density of states at each subband edge E n . For holes, the situation is a little more complicated than for electrons (Fig. 12.26). First, the degeneracy of heavy and light holes is lifted since their mass enters the confinement energy. The effective hole masses along the z direction, i.e. those that enter (12.5), are 1 z = γ1 − 2 γ2 m hh 1 z = γ1 + 2 γ2 . m lh
(12.8a) (12.8b)
The light holes have the higher quantization energy. The angular momentum is quantized along the z direction. The transverse masses for the dispersion in the interface plane are 1 x y = γ1 + γ2 m hh 1 x y = γ1 − γ2 . m lh
(12.9a) (12.9b)
Now the heavy hole, i.e. the Jz = ± 23 state, has the smaller mass and the light hole (Jz = ± 21 ) the larger (Fig. 12.26c). However, this consideration is only an approximation since the lifting of degeneracy and the dispersion have to be treated on the same level. Higher terms of the perturbation calculation lead to band mixing and remove the band crossing that seems to originate from the situation at the Γ point. In reality, the bands show anticrossing behavior and are strongly deformed. The hole dispersion in a superlattice and the anticrossing behavior is shown in Fig. 12.27.
12.3 Energy Levels in Heterostructures Fig. 12.27 Hole dispersion in a 68ML GaAs/71 ML Al0.25 Ga0.75 As superlattice (numerical calculation). The double curves originate from a lifting of timereversal symmetry at k = 0. Reprinted with permission from [1045], © 1985 APS
421 0
hh1
GaAs/ AlGaAs
hh2
10
lh1
hh3
20
hh4 lh2
30
0.04
0.03
0.02
0.01
[110]
0
0.01 0.02
0.03 0.04
[100]
Fig. 12.28 Observed electron–hole transitions (energy difference to the first e–h transition from excitation spectroscopy) in GaAs/AlGaAs quantum wells of varying thickness. Symbols are experimental data, solid lines are theoretical model. Data from [1046]
Experimentally observed transition energies in quantum wells of varying thickness are shown in Fig. 12.28 and are in good agreement with the theoretical calculation. We note that for infinite barriers optical transitions are only allowed between confined electron and hole states with the same quantum number n. For finite barriers this selection rule becomes relaxed, and other transitions become partially allowed, e.g. e1 –hh3 . The optical matrix element from the Bloch part of the wavefunction, which was isotropic for (cubic) bulk material (9.25), is anisotropic for quantum wells. TE (TM) polarization is defined with the electromagnetic field in (perpendicular to) the plane of the quantum well (Fig. 12.29a). At the subband edge, i.e. for inplane wavevector k = 0 the matrix elements for the various polarizations and propagation
422
12 Heterostructures
(b)
mj
1/2
1/2
1/2
1/2
lh
lh
electrons
TM
(a)
TE mj
TE
3/2 hh
3/2
holes
hh
Fig. 12.29 (a) Directions of electricfield vector relative to the quantumwell plane for TE and TM polarization. (b) Optical selection rules for band–band transitions in a quantum well. If the (inplane averaged) relative strength of the e–hh transitions (solid lines) is 1, the relative strength of the TEpolarized e–lh transitions (dashed lines) is 1/3 and that of the TMpolarized e–lh transitions (dashdotted lines) is 4/3 Table 12.3 Squared momentum matrix elements cˆe · pv2 in a quantum well for various propagation directions in units of Mb2 . The quantumwell normal is along z
e–hh
e–lh
e–so
Propagation eˆ x (TE)
eˆ y (TE)
eˆ z (TM)
x y z x y z x y z
1/2 – 1/2 1/6 – 1/6 1/3 – 1/3
0 0 – 2/3 2/3 – 1/3 1/3 –
– 1/2 1/2 – 1/6 1/6 – 1/3 1/3
directions are given in Table 12.3. The matrix elements averaged over all inplane directions for TEpolarization are 3/2Mb2 (1/2Mb2 ) for the electron to heavy (light) hole transition. For TM polarization the values are 0 and 2Mb2 , respectively [1047]. The optical selection rules are shown in Fig. 12.29 (see Fig. 9.9 for bulk material). For propagation along the quantumwell plane, the ratio between the strength of the TE polarized e–hh and e–lh transitions is 3:1. The confinement potential squeezes charge carriers bound to impurities closer to the ion. Therefore, the binding energy increases as shown in Fig. 12.30. This behavior can be modeled theoretically with good precision. It makes a difference whether the impurity is located at the center or the interface of the quantum well. The confinement potential also squeezes electrons and holes in the exciton closer together and thus increases their Coulomb interaction. The binding energy of the quantumwell exciton is thus larger than in bulk material and depends on the well
12.3 Energy Levels in Heterostructures
423
GaAs/Al Ga As 40
35
30
25 0
5
10
15
20
25
30
35
Fig. 12.30 Experimental values for the acceptor binding energy in GaAs/Al0.3 Ga0.7 As quantum wells (solid circles) from [1048] as a function of well width. Solid line is theory (variational calculation) for the wellcenter acceptor including top four valence bands and finite barriers, dashed line is hydrogenlike model with infinite barrier height. Adapted from [1049]
(a)
(b) 15 Al0.4Ga 0.6 As/GaAs
InGaAs/ GaAs
10 9
10 8 mb m w , b mb mw , b= mb=mw , b mb=mw , b=
5 0
5
7
w w w
6
w
10
15
0
5
10
z
Fig. 12.31 (a) Theoretical (variational) calculation (solid line) of the heavyhole exciton binding energy versus QW thickness in a GaAs/Al0.4 Ga0.6 As quantum well (using also different approximations, other lines). Adapted from [1050]. (b) Experimental exciton binding energy in Inx Ga1−x As/GaAs quantum wells of different thickness. Circles: data and error bars from [1051], x unspecified, squares: data from [1052], x = 0.18
width (Fig. 12.31). In the simple hydrogenlike model with infinite barriers the exciton binding energy is 4 times the bulk binding energy in the limit L z → 0. In a realistic calculation the effect of different dielectric constants in the well and barrier (image charge effect) need to be considered.
424 Fig. 12.32 Band structure of a superlattice with a potential depth of 0.4 eV and well and barrier width w (L QW = L barr ). Adapted from [1053]
12 Heterostructures 0.45 0.40
E4 0.35 0.30 0.25
E3 0.20 0.15
E2
0.10 0.05
E1 0
0
1
2
3
4
5
6
7
8
9
10
12.3.3 Superlattices In a superlattice, the barrier thickness is so small that carriers can tunnel in neighboring wells or, in other terms, that there exists a significant wavefunction overlap between adjacent wells. This leads to a band structure (Fig. 12.32), similar to the Kronig–Penney model (Appendix F). For the superlattice the bands are called minibands, the gaps are called minigaps. The density of states does not make a step at the subband edge but follows an arccos function. The modification of the density of states, as seen in the absorption spectrum, are shown in Fig. 12.33 for 1, 2, 3 and 10 coupled wells.
12.3.4 Single Heterointerface Between Doped Materials We consider a single heterointerface between ndoped materials. As an example we take nAlGaAs/nGaAs (Fig. 12.34). First, we consider the materials without contact, forming a typeI structure. In thermodynamic equilibrium the system must have a constant Fermi level. Thus, charge is transferred from the region close to the interface from AlGaAs to GaAs. This results in the formation of a triangular potential well in the GaAs close to the interface. A twodimensional electron gas (2DEG) forms in this potential well (Fig. 12.35). The charge transfer in thermodynamic equilibrium adjusts the band bending and the charge density (quantized levels in the well) in such a way that they are selfconsistent. The Poisson equation and the Schrödinger equation are simultaneously fulfilled. Numerically, both equations are iteratively solved and the solution is altered until it is selfconsistent, i.e. it fulfills both equations.
12.3 Energy Levels in Heterostructures
425
Fig. 12.33 Absorption spectra of a single, double, triple and ten coupled quantum wells. Theoretically predicted transitions with heavy (light) holes are labeled with filled (empty) bars at their respective transition energies. Adapted from [1054] Fig. 12.34 Schematic formation of a triangular potential well in a nAlGaAs/nGaAs heterostructure, (a) before and (b) after equilibration of Fermi levels
(a) AlGaAs
(b) GaAs
Ec
Ec
Ev
Ev
If the region of the 2DEG is not doped, the electron gas exists without any dopant atoms and ionized impurity scattering no longer exists. This concept is called modulation doping. Mobilities up to 3.1 × 107 cm2 /Vs have been realized (Fig. 12.36). The theoretical limits of mobility in a 2DEG at modulationdoped AlGaAs/GaAs heterointerfaces are discussed in detail in [1056].
426
12 Heterostructures
Fig. 12.35 (a) Conductionband edge at a GaAs/Al0.3 Ga0.7 As heterointerface (T = 0 K) with two confined states at E 0 and E 1 marked with solid horizontal lines. In the GaAs channel there are 5 × 1011 cm−2 electrons. The barrier height is 300 meV, NDGaAs = 3 × 1014 cm−3 . The position of the Fermi level E F is at E = 0 and indicated with a dashdotted line. (b) Envelope wavefunctions φ0 and φ1 of the two confined states, dashdotted line: calculation without exchange and correlation for state at E 0 . Adapted from [1055] Fig. 12.36 Progress in the achievement of high electron mobility in GaAs, annotated with the technical innovation responsible for the improvement. Adapted from [1057]
12.4 Recombination in Quantum Wells
427
12.4 Recombination in Quantum Wells 12.4.1 Thickness Dependence The energy of exciton recombination in quantum wells is blueshifted with respect to that in bulk material due to the quantumconfinement energies of electrons and holes (Fig. 12.37). The electron–hole recombination lineshape in quantum wells is given by the product of the joint density of states and the Boltzmann function (when Boltzmann statistics apply). The JDOS is given by a step function (Heavyside function H (E)). E , (12.10) I (E) ∝ H (E − E 11 ) exp − kT
(a)
(b) AlGaAs QW1 AlGaAs
E
QW2
Ee2
GaAs AlGaAs
Ee1 EC
Eh1 Eh2
Egbarr
E11 E22 EV
(c) PLintensity(arbitraryunits)
Eg
QW2
QW1 AlGaAs *1000
1.5
1.6
1.7
1.8
1.9
Energy(eV)
Fig. 12.37 (a) Schematic energy diagram of a quantum well with confined electron (e1, e2) and hole (h1, h2) states and recombination between them at energies E 11 and E 22 . (b) Schematic sample structure with two GaAs/Alx Ga1−x As quantum wells with thicknesses 3 and 6 nm. (c) Photoluminescence spectrum (T = 300 K) of the structure from part (b). A small amount of barrier luminescence appears at 1.88 eV, according to x = 0.37 (cf. Fig. 6.19c)
428
12 Heterostructures
(b)
InGaAs/InP
T=80K
(a)
104 GaAs/AlGaAs
103
102
10
1
10
0
T=25K
E11
T=4.7K
1.50
1.55
1.60
1.65
1.70
0.82
0.84
0.86
0.88
0.90
0.92
Fig. 12.38 (a) Reflectance spectra at various temperatures from a 17 nm thick GaAs/Al0.3 Ga0.7 As quantum well. The inset shows the temperature dependence of the homogeneous linewidth. (b) LO phonon broadening parameter (FWHM) for various quantum well widths. Adapted from [1061]s
where E 11 = E g + E e1 + E h1 represents the energy of the E1–H1 subband edge as shown in Fig. 12.37. An experimental spectrum (Fig. 12.39a) shows that excitonic effects influence the recombination lineshape in a GaAs quantum well even at room temperature [1058]. The recombination decay constant of excitons decreases with decreasing well width, partly due to the increase of exciton binding energy as discussed in [1059].
12.4.2 Broadening Effects ManyBody Effects At high carrier densities when the electron (quasi) Fermi level is above the electron subband edge, the spectrum broadens and reflects the Fermi–Dirac distribution (Fig. 12.39b). At low temperatures a manybody effect, multiple electron– hole scattering with electrons at the Fermi edge, leads to an additional peak, termed Fermiedge singularity that is discussed in [1060]. Homogeneous Broadening The temperature dependence of the homogeneous broadening of quantum well luminescence has been investigated in [1061]. It follows the dependence of the broadening known from bulk material (Sect. 9.6.7) with similar values for the LO broadening parameter. In Fig. 12.38a the reflectance spectra for different temperatures of a 17 nm GaAs/Al0.3 Ga0.7 As QW are shown. The optical phonon broadening parameter for various well widths is shown in Fig. 12.38b and coincides with the bulk value.
12.4 Recombination in Quantum Wells
(a)
429
(b)
Fig. 12.39 (a) Photoluminescence spectrum of a 5nm GaAs/AlGaAs quantum well at T = 300 K. The solid (dashed) line is fit with (without) excitonic effects. The two peaks are due to transitions involving heavy and light holes. Adapted from [1058]. (b) Photoluminescence spectra at three different temperatures as labeled of a 10nm modulationdoped InGaAs/InP quantum well with an electron sheet density n s = 9.1 × 1011 cm−2 . The electron quasiFermi level is Fn − (E C + E e1 ) = 44.1 meV from the subband edge. The dashed line in the T = 80 K spectrum is the lineshape from JDOS and a Fermi–Dirac distribution without enhancement at the Fermi edge. Adapted from [1060]
The homogeneous broadening leads to excitons with inplane centerofmass wavevector K = 0 being allowed to recombine radiatively. This leads to a linear increase of exciton lifetime as demonstrated for GaAs quantum wells up to 50 K in [1059]. In [1062] all exciton wavevectors within the light cone are considered, explaining the linear increase of exciton lifetime in (nonpolar) ZnO quantum wells up to room temperature. Inhomogeneous Broadening Inhomogeneous broadening affects the recombination lineshape. Since the interfaces of the QW are not ideally flat, the exciton averages over different quantumwell thicknesses within its volume. Also, e.g. for the GaAs/AlGaAs system, the wavefunction in the (binary) quantum well tunnels into the barrier, the amount depending on the QW width, and there ‘sees’ the alloy broadening (see Sect. 10.3.3). The problem of exciton dynamics in a potential with random fluctuations has been treated in detail [1063, 1064]. A simplified picture is as follows: At low temperatures the excitons populate preferentially the potential minima. A simple lineshape5 of the QW absorption or joint density of states is given by a step function (cf. Table 9.2) at the QW band edge E 0 . The inhomogeneous broadening has a Gaussian probability distribution p(δ E) ∝ exp[−(δ E)2 /2σ 2 )] with δ E being the deviation from the QW band edge δ E = E − E 0 . The resulting lineshape is given by the convolution of the Gaussian
5 neglecting
excitonic enhancement.
430
12 Heterostructures
(a)
(b)
(c)
Fig. 12.40 (a) Recombination spectra (solid lines, scaled to same height) of a model quantum well for different temperatures as labeled and complete thermalization, dashed (dashdotted) line is unperturbed (inhomogeneously broadened by σ = 20 meV) shape of the QW absorption edge. The energy scale is relative to the energy position of the unperturbed QW absorption edge at E 0 . (b) Theoretical energy position and (c) linewidth of exciton recombination from a model disordered quantum well. The hightemperature limits are marked by arrows. Parts (b, c) adapted from [1063]
with the unperturbed absorption spectrum yielding an errorfunctionlike spectrum6 as shown in Fig. 12.40a. For complete thermalization the level population is given by the Boltzmann function. The recombination spectrum is given by the product of the absorption spectrum (or JDOS) and the Boltzmann function. It is (red) shifted with respect to E 0 by about7 σ2 ΔE(T ) = − = γ(T ) kT. (12.11) kT This shift between emission and absorption is also called the Stokes shift. √ z error function is defined as erf(x) = (2/ π) 0 exp −t 2 dt. 7 Formula (12.11) is exact for the product of a Gaussian and the Boltzmann function. 6 The
12.4 Recombination in Quantum Wells
431
Within their lifetime, limited at least by radiative recombination, the excitons are typically unable to reach the energy position required by the Boltzmann function, but only a local minimum. Thus, their thermalization may be incomplete due to insufficient lateral diffusion. This effect is particularly important at low temperatures when thermal emission into adjacent deeper potential minima is suppressed. In this case, the redshift is smaller than expected from (12.11). A numerical simulation [1063] yields such behavior of the energy position of the recombination line as shown in Fig. 12.40b. Simultaneously, the width of the recombination spectrum also exhibits a minimum (Fig. 12.40c). These findings are in agreement with experiments [1065, 1066]. An analytical model for temperature dependent exciton localization in the presence of disorder has been given in [1067], yielding a value 0 ≤ γ ≤ γ0 = (σ/kT )2 in (12.11). A potential fluctuation can localize an exciton laterally at low temperatures [1058] and behave like a quantum dot (cf. Sect. 14.3). Localized and delocalized excitons are separated by a boundary called the mobility edge [1068]. The transition between the two regimes is a Mott transition [1069]. Monolayer Growth Islands Under certain growth conditions, quantum wells with piecewise very flat interfaces can be fabricated. The thickness difference between such regions (with lateral extension in the µm range) is an integer monolayer. Accordingly, the recombination spectrum yields several, typically two or three, discrete lines (Fig. 12.41).
12.4.3 Quantum Confined Stark Effect The quantum confined Stark effect (QCSE, Sect. 13.1.2) in quantum wells shifts energy levels when electric fields are present along the width of the quantum well. A strong effect exists for pyro and piezoelectric material combinations such as caxis oriented (In,Ga)N/(Al,Ga)N [1070, 1071] or (Cd,Zn)O/(Mg,Zn)O [1072, 1073] quantum wells due to the builtin electric field (cf. Sect. 15.2). The QCSE induced redshift is larger in thicker quantum wells and goes beyond the bulk band gap of the quantum well material (Fig. 12.42b). Also the wavefunction overlap is reduced with increasing well width, leading to an increase of the radiative recombination lifetime as shown in Fig. 12.42. The pyroelectric field and the related modification of lifetime are absent in quantum wells grown on nonpolar directions such as [11.0] (Fig. 12.42a).
432
12 Heterostructures
Fig. 12.41 Photoluminescence spectrum (T = 2 K) (dots) of GaAs/AlGaAs quantum well grown by MBE with 120 s growth interruptions. Recombination is due to excitons in islands of 19, 18, and 17 monolayers (a0 /2) height. The solid line is a lineshape fit including lifetime broadening (Γ = 1.34 meV) and residual inhomogeneous broadening (σ = 0.04 meV) due to AlGaAs barrier alloy fluctuations. Note that the energy separation of the peaks is much larger than kT . The peak doublet structure is discussed in [1058]. Adapted from [1058]
(a)
(b)
Fig. 12.42 (a) Radiative lifetime of electronhole pairs in polar [00.1]oriented In0.2 Ga0.8 N/GaN (circles) and nonpolar [11.0]oriented GaN/Al0.2 Ga0.8 N (squares) quantum wells of varying thickness. Experimental data are shown in symbols. The solid line is the (scaled) theoretical dependence of the electronhole overlap for (In,Ga)N/GaN QWs. The dashed line is guide to the eyes. The arrow denotes the recombination time constant in bulk GaN. Adapted from [1074, 1075]. (b) Low temperature PL peak recombination energy (solid squares) for ZnO/Mg0.3 Zn0.7 O quantum wells for various well widths L z (barrier width L B = 5 nm). Dashed line indicates dependence for internal field of 0.9 MV/cm, horizontal dashed line indicates recombination energy in ZnO bulk. Carrier lifetime determined from PL (circles), dashed line is guide to the eyes. Adapted from [1073]
12.5 Isotope Superlattices
433
320 70
Gen/74Gen SL 70
LO1 LO3 LO5 70 LO7 74 LO1 74 LO3 74 LO5
310
70
Ge alloy
1
70 70
300
74
Ge
290
280
270
0
10
20
30
40
bulk
Fig. 12.43 Measured (full circles) and theoretical (solid lines) confined LO phonon energies in 70 Ge /74 Ge superlattices versus the layer thickness (number of monolayers) n. The dashed lines n n represent a calculation that considers intermixing at the interfaces. On the right, the energies of bulk modes for isotopically pure 70 Ge and 74 Ge are shown together with that of an 70 Ge0.5 70 Ge0.5 alloy. Adapted from [1076]
12.5 Isotope Superlattices A special type of heterostructure is the modulation of the isotope content. The first kind of heterostructures made like this were 70 Gen /74 Gen symmetric superlattices [1076]. Figure 12.43 shows phonon energies determined from Raman spectroscopy for various layer numbers n. The modes are classified by 70 LOm and 74 LOm denoting the material in which the amplitude is maximal and m being the number of maxima in that medium.8 Such modes are visualized in Fig. 12.44a for a 69 GaP16 /71 GaP16 superlattice. Theoretical mode energies as a function of the superlattice period are shown in Fig. 12.44b.
12.6 Wafer Bonding Wafer bonding is a fairly recently developed method to join different and dissimilar materials. Two wafers of the respective materials are put together face to face and are adequately fused. The idea is to not only ‘glue’ the wafers together with a sticky (and compliant) organic material, but to form strong atomic bonds between the two materials with possibly a perfect interface. In some cases, the interface needs to allow chargecarrier transport through it. Less stringent conditions need to be met for photon transport. 8 Only
modes with odd m are Ramanactive.
434
12 Heterostructures
Fig. 12.44 (a) Atomic displacements [Ga (filled dots) and P (open circles)] of oddindex LO modes in a 69 Ga16 P/71 Ga16 P superlattice unit cell. These modes have even parity with respect to midlayer planes, which are at atom numbers 16 and 48 in this example. The labels on the left identify the predominant character of the mode, those on the right give the relative Raman intensities with respect to that of the 69 LO1 mode. The tick marks on the vertical axis indicate zero displacement of the respective mode. (b) Upper panel: Energies and characters of oddindex LO phonon modes in GaP isotope SLs as calculated within the planar bond charge model for the case of ideal interfaces. 69 LO modes are shown as open symbols; 71 LO modes as full symbols. The shaded area marks m m n = 16 for which the atomic displacements of the modes are shown in part (a). Lower panel: Calculated intensities of the modes relative to that of the 69 LO1 phonon mode. Adapted from [335], reprinted with permission, © 1999 APS
(a)
(b)
Fig. 12.45 Highresolution TEM images of waferbonded (a) SiSi and (b) GaAsSi interfaces. White circles indicate the position of misfit dislocations. Part (a) reprinted from [1077], © 2003, with permission from Elsevier. Part (b) reprinted with permission from [1078], © 1998 AIP
12.6 Wafer Bonding
435
Mechanical deficiencies such as surface roughness, dust particles and the like must be avoided in the waferbonding process since they result in voids. Several methods have been developed for bonding various materials [1079, 1080]. Such processes are successful for large substrate sizes. With proper processing, ideal interfaces can be created, as shown in Fig. 12.45. Such structures, if made between a pdoped and a ndoped semiconductor, show diode characteristics.
Chapter 13
External Fields
Abstract The effects of external electric and magnetic fields on the electronic and optical properties of bulk materials and quantum wells are discussed including the Stark effect and quantumconfined Stark effect, the Hall effect and Quantized Hall Effects.
13.1 Electric Fields 13.1.1 Bulk Material The centerofmass motion of the exciton is not influenced by an electric field. The Hamilton operator for the relative motion of an electron–hole pair of reduced mass μ along z in the presence of an electric field E along the z direction is Δ − e E z. Hˆ = − 2μ 2
(13.1)
Here, the Coulomb interaction, leading to the formation of bound exciton states, is neglected. In the plane perpendicular to the field (here the z direction) the solutions for the relative motion are just plane waves. In the electric field the bands are tilted (Fig. 13.1), i.e. there is no longer an overall band gap. Accordingly, the wavefunctions are modified and have exponential tails in the energy gap.
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_13
437
438
13 External Fields
(b)
E=0
E 0 e2
e2
e1
e1
(a)
h
EC h
h
Eg h1
EV
h1 h2 h3 h4
h2 h3 h4
h5
h5
Fig. 13.1 Impact of an electric field on (a) bulk material (tilt of bands) and (b) a quantum well (quantum confined Stark effect, QCSE)
After separation of the motion in the (x,y) plane the Schrödinger equation for the motion in the z direction is −
2 d 2 − e E z − E z φ(z) = 0 , 2μ dz2
which is of the type
d2 f (ξ) − ξ f (ξ) = 0 , dξ 2
(13.2)
(13.3)
1/3 2 2 2 1/3 e E e E and the optoelectronic energy Θ = . The with ξ = EΘz − z 2μ 2 2μ solution of (13.3) is given by the Airy function Ai (cf. Fig. 13.2): √ φEz (ξ) =
eE Ai(ξ). Θ
(13.4)
The prefactor guaranties the orthonormality (with regard to the Ez ). The absorption spectrum is then given by α(ω, E) ∝
1√ Θ π Ai 2 (η) − η Ai2 (η) , ω
with η = (Eg − E)/Θ and Ai (x) = dAi(x)/dx.
(13.5)
13.1 Electric Fields
439
(a)
(b)1
0.4 0.5 0.2 0
0
0.5
0.2 0.4
1 10
8
6
4
2
0
2
4
10
8
6
4
2
0
2
4
Fig. 13.2 (a) Airy function Ai(x), (b) Ai’(x)
Optical transitions below the band gap become possible that are photonassisted tunneling processes. The belowbandgap transitions have the form of an exponential tail. Additionally, oscillations develop above the band gap, the socalled Franz– Keldysh oscillations (FKO) (Fig. 13.3a). The absorption spectrum scales with the optoelectronic energy Θ. The energy position of the FKO peaks En is periodic with (ν ∼ 0.5) 3/2 √ En − Eg ∝ (n − ν) E μ.
(13.6)
A nonperiodicity can indicate a nonparabolicity of the mass. For a given mass the electric field strength can be determined. Wellpronounced oscillations are only present for homogeneous fields. Experimental spectra show additionally the peaks due to excitonic correlation (Fig. 13.3b) at low field strength. At higher fields the FKO evolve and the amplitude of the excitonic peaks decreases because the excitons are ionized in the field.
13.1.2 Quantum Wells In a quantum well an electric field along the confinement direction (z direction) causes electrons and holes to shift their mean position to opposite interfaces (Fig. 13.1b). However, excitons are not ionized due to the electric field. With increasing field (for both field directions) the energy position of the absorption edge and the recombination energy is reduced. This is the quantum confined Stark effect (QCSE). Corresponding experimental data are shown in Fig. 13.4i–v. The shift depends quadratically on the electric field since the exciton has no permanent dipole moment (mirror symmetry of the quantum well). Thus, only the secondorder Stark effect is present (as for the hydrogen atom) in which the field first induces a dipole p = αE. This dipole interacts with the field with an energy E = −p· E = −αE2 . The carrier separation in opposite sides of the quantum well (Fig. 13.4b) leads to a reduced overlap of the electron and hole wavefunctions and subsequently to an increased recombination lifetime (see Fig. 12.42).
440
13 External Fields
(a)
(b) 30
0.10
ehh
25 20
1
(10 cm )
0.05
= (E) (0)
3
0 2
0.005
4
elh
15 0.3V 0.2V 0V 0.5V
10
0 3
0.005
5
5
InGaAs
2.0V 1
0.80
0.84
0 0.80
0.88
0.81
0.82
0.83
0.84
Fig. 13.3 (a) Theoretical absorption (top panel) with (solid line) and without (dashdotted line) electric field for a volume semiconductor (without Coulomb interaction) and theoretical change of absorption (bottom panel). (b) Experimental absorption spectra of InGaAs on InP at T = 15 K for various applied voltages as labeled. Adapted from [1081]
(a)
(b) AlGaAs/ GaAs
(ii)
(i)
AlGaAs/ GaAs
(iii)
(iii) (iv) (v)
(ii)
(i) 1.42
1.46
1.50
1.43
1.45
1.47
Fig. 13.4 Impact of electric fields on the absorption spectrum of n × (9.5 nm GaAs/9.8 nm Al0.32 Ga0.68 As) multiple quantum well structures. a Electric field along the [001] growth direction (n = 50), (i)–(v): E = 0, 0.6, 1.1, 1.5, and 2 × 105 V/cm. b Electric field within the interface plane (n = 60), (i–iii): E = 0, 1.1, and 2×105 V/cm. Adapted from [1082]
13.1 Electric Fields
441
If the field is within the quantumwell interface plane, the field leads to the ionization of excitons without shift of the energy position. The loss of the excitonic peak is visualized in the spectra in Fig. 13.4a–c.
13.2 Magnetic Fields In magnetic fields, electrons (or holes) perform a cyclotron motion with frequency ωc = eB/m∗ , i.e. a motion perpendicular to the magnetic field on a line of constant energy in kspace. This line is the intersection of a plane perpendicular to the magnetic field and the respective isoenergy surface in kspace. For semiconductors with anisotropic mass, such as Si and Ge, the quantum theory of cyclotron resonance has been given in [1083]. The physics of semiconductors in magnetic fields is covered in detail in [1084]. The ballistic cyclotron motion can only occur between two scattering events. Thus, a significantly long path along the cyclotron trajectory (classically speaking) and the connected magnetotransport properties are only possible when • ωc τ 1, i.e. when the average scattering time τ is sufficiently large. This requires high mobility. • the magnetic field is sufficiently strong and the temperature sufficiently low, i.e. ωc kT , such that thermal excitations do not scatter electrons between different Landau levels. • the cyclotron path is free of geometric obstructions. An external magnetic field also produces a splitting of the spin states. For the electron, the energy splitting ΔE is given by ΔE = ge∗ μB B ,
(13.7)
where B is the magneticfield amplitude and ge∗ the (effective) electron gfactor. This value differs from the freeelectron value in vacuum of ge = 2.0023 due to the presence of spinorbit interaction (see Sect. 13.2.3). Values for ge∗ at low carrier density and low temperatures are 2 for Si, 1.2 for InP and ZnSe, −1.65 for CdTe, −0.44 for GaAs, −15 in InAs, and −50 for InSb. In [1085] the temperature dependence of ge∗ in GaAs, InP and CdTe is also measured and discussed. The electron gfactor increases in thin GaAs/AlGaAs quantum wells [1086].
13.2.1 Hall Effect An electrical current along the x (longitudinal) direction in a perpendicular magnetic field B = (0, 0, B) along z causes an electric field Ey along the transverse (y) direction (Fig. 13.5). The charge accumulation is due to the Lorentz force. The related
442
13 External Fields
B
z y
v
x F
B w
I
VH Fig. 13.5 Scheme of the Halleffect geometry. The movement of one electron in the longitudinal electric current I is shown schematically. The coordinate system (x, y, z) and the directions of the magnetic field B, the drift velocity of an electron v and the resulting Lorentz force F are given. The transverse field Ey is given by VH /w Fig. 13.6 Hallbar geometry. The current I is driven by a source from contact 1 to 2. The Hall voltage is measured between contacts 3 and 4, the longitudinal voltage between 3 and 5
Vxx
5
3
I
Bz
Vxy =VH
1
4
2
I
6
transverse voltage is called the Hall voltage and the resistivity ρxy = Ey /jx the Hall resistivity [21, 24, 25]. Many aspects of the Hall effect are discussed in [1087]. For thinfilm samples typically Hall bars [1088] (see Fig. 13.6 and also Fig. 13.17, for a reasonable measurement of the Hall voltage the ratio of length and width of the Hall bar should be at least 3) or the vanderPauw geometry (Fig. 13.7) and method are used [1089–1091]. For band transport in the relaxation time approximation (Sect. 8.2), the steadystate equation of motion is m∗
v = q (E + v × B) . τ
(13.8)
We note that this equation of motion is also valid for holes, given the convention of Sect. 6.9.1, i.e. positive effective mass and charge. With the cyclotron frequency ωc = qB/m∗ the conductivity tensor is (j = qnv = σ E)
13.2 Magnetic Fields
443
(a)
(b)
(c)
(d)
(e)
Fig. 13.7 (a–d) Geometry for vanderPauw Hall measurements. (a) Best geometry (cloverleaf ), (b) acceptable square geometry with small contacts on the corners, (c,d) not recommended geometries with contacts on the edge centers or inside the square, respectively. (e) Current distribution, as visualized by lockin thermography [1092], in epitaxial ZnO layer on sapphire with Hall geometry as in part (b). Grey dashed line indicates the outline of the 10 × 10 mm2 substrate, grey areas indicate gold ohmic contacts
⎛
σ σxx = σyy σxy = −σyx σzz
⎞ σxx σxy 0 = ⎝ σyx σyy 0 ⎠ 0 0 σzz 1 1 = σ0 = σ0 2 2 1 + ωc τ 1 + μ2 B2 ωc τ μB = σ0 = σ0 1 + ωc2 τ 2 1 + μ2 B2 q2 n τ = σ0 = = q n μ. m∗
(13.9a) (13.9b) (13.9c) (13.9d)
Perpendicular to the magnetic field, the conductivity (σzz ) is given by (8.5). If only one type of carrier (charge q, density n) is considered, the condition jy = 0 leads to Ey = μB Ex and jx = σ0 Ex . The Hall coefficient is defined as RH = Ey /(jx B) or more precisely as ρxy RH = , (13.10) B where the resistivity tensor ρ is the inverse of the conductivity tensor σ, ⎛
⎞ ρxx ρxy 0 ρ = σ −1 = ⎝ ρyx ρyy 0 ⎠ 0 0 ρzz σxx ρxx = ρyy = 2 2 σxx + σxy
(13.11a) (13.11b)
444
13 External Fields
σxy 2 + σ2 σxx xy 1 1 ρzz = = . σzz σ0
ρxy = −ρyx =
(13.11c) (13.11d)
For a single type of carriers, the Hall coefficient is therefore given by RH =
μ 1 = . σ0 qn
(13.12)
It is negative (positive) for electron (hole) conduction. We note that electrons and holes are deflected in the same ydirection by the magnetic field and collect at the same electrode. Thus the Hall effect allows the determination of the carrier type and the carrier density.1 If both types of carriers are present simultaneously, the conductivity (twoband conduction) is given by the sum of electron and hole conductivity (8.11), σ = σe + σh .
(13.13)
The Hall constant (13.10) is then RH =
1 −n μ2e (1 + μ2h B2 ) + p μ2h (1 + μ2e B2 ) . 2 e n2 μ2e (1 + μh B2 ) − 2 n p μe μh (1 + μe μh B2 ) + p2 μ2h (1 + μ2e B2 ) (13.14)
Under the assumption of small magnetic fields,2 i.e. μB 1, the Hall coefficient is 1 RH = e
n p (−n + p) μ2e μ2h (μe − μh )2 2 −n μ2e + p μ2h + B + ··· . (−n μe + p μh )2 (−n μe + p μh )4 (13.15)
For small magnetic field this can be written as RH =
1 Using
1 p − n β2 , e (p − n β)2
(13.16)
the Hall effect, the net free charge carrier concentration is determined. We note that the concentration of fixed charges in semiconductors can be investigated by depletion layer spectroscopy (Sect. 21.2.4). 2 We note that for a mobility of 104 cm2 /Vs, μ−1 is a field of B = 1 T.
13.2 Magnetic Fields
445
with β = μe /μh < 0. For large magnetic fields, i.e. μB 1, the Hall coefficient is given by 1 1 RH = . (13.17) e p−n In Fig. 13.8, the absolute value of the Hall coefficient for InSb samples with different doping concentrations is shown. The pdoped samples exhibit a reverse of the sign of the Hall coefficient upon increase of temperature when intrinsic electrons contribute to the conductivity. The zero in RH occurs for n = p μ2h /μ2e = ni /β. For high temperatures, the Hall coefficient for n and pdoped samples is dominated by the electrons that have much higher mobility (Table 8.2). The simultaneous conduction in a band and an impurity band (cmp. Sect. 7.5.7) has been separated with a suitable model assuming two conduction channels for holes [1094] (Fig. 13.9). In the derivation of the (unipolar) Hall coefficient we had assumed that all carriers involved in the transport have the same properties, in particular that they are subject to the same scattering time. This assumption is generally not the case (cmp. Appendix I) and we need to operate with the ensemble average of the discussed
(a)
(b)
Fig. 13.8 (a) Conductivity and (b) absolute value of the Hall coefficient versus inverse temperature for four pdoped (A–D) and two ndoped (E, F) InSb samples. The doping levels are given in (a). Adapted from [1093]
446
13 External Fields
Fig. 13.9 Carrier densities in valence band (circles) and impurity band (triangles) from evaluating the Hall effect on GaAs doped with lithium (and annealed) taking into account two conduction channels. Adapted from [1094]
Temperature (K)
Hole concentration (cm3)
1018
200
100
70
50
GaAs:Li 1017
impurity band
1016 valence band 1015 5
10
15
20
1000/T (1/K)
quantities. The ensemble average of an energydependent quantity ζ(E) over the (electron) distribution function f (E) is denoted as ζ and is given as3 ζ =
ζ(e) f (E) dE . f (E) dE
(13.18)
In particular τ 2 is now different from τ 2 . Considering the equation j = σ E for the ensemble averaged current densities we find (for one type of carrier, cf. (13.12)) 1 (13.19) rH , RH = qn with the socalled Hall factor rH given by γ + ωc2 γ 2 τ
α= 1 + ωc2 τ 2 τ2 γ=
. 1 + ωc2 τ 2
rH =
α2
(13.20)
3 For this consideration it is assumed that the energy dependence is the decisive one. Generally, averaging may have to be performed over other degrees of freedom as well, such as the spin or, in the case of anisotropic bands, the orbital direction.
13.2 Magnetic Fields
447
The Hall factor depends on the scattering mechanisms and is of the order of 1. For large magnetic fields the Hall factor approaches 1. For small magnetic fields we have 1 τ 2
. (13.21) RH = q n τ 2 The mobility calculated from (cf. (13.9d)) σ0 RH is called the Hall mobility μH and is related to the mobility via μH = rH μ.
(13.22)
It is assumed so far that the free carrier density and mobility are homogeneous within the volume of current transport. Multilayer models can be fitted to experimental Hall data in order to account for different conduction channels in different layered parts of the sample [1095]. E.g., in a twolayer model, contributions from bulk and surface/interface conduction can be separated [1096–1098]. The magnetic field dependence of σ can be used in a general case to separate contributions of carriers with different density and mobility (including its sign) without assumptions and obtain the mobility spectrum s(μ) (MSA, mobility spectral analysis),
∞
1 dμ 1 + μ2 B2 −∞ ∞ μB s(μ) dμ, σxy = 1 + μ2 B2 −∞
σxx =
s(μ)
(13.23a) (13.23b)
as a generalization of (13.13), (13.9b) and (13.9c) [10991101]. Examples are the separation of electron conductivity in (GaAs) Γ  and (InAs) XMinima in a GaAs/AlGaAs/InAs double quantum well structures [1099] (Fig. 13.10a), substrate and 2DEG electron conductivity in AlGaN/GaN heterostructures [1102], and electrons and holes in an InAs/GaSb quantum well [1100] (Fig. 13.10b). In the case of hopping conduction (Sect. 8.7), the theory of Hall effect is more involved [1103, 1104]. If carriers are transported by hopping, generally, they may not be free to move as expected by (13.8) in response to the applied magnetic field and the Lorentz force. A Hall effect occurs only at the junction of three (or more) hopping sites [1103]. The sign of the experimentally determined Hall coefficient is often opposite to the one expected from the carrier type according to (13.12), e.g. as studied in aSi [1105, 1106]. The sign anomaly depends on intricacies such as the local site geometry and interference processes taking place among bonding and antibonding orbitals of various numbers as summarized in [1107].
448
13 External Fields
(b)105 AlAs/GaAs
104
electrons X
103
102
Conductivity (arb. units)
Conductivity (arb. units)
(a)105
104 holes 3D 10
10
10
3
10
3
2D 10
4
InAs/GaSb
electrons
2
2
10 5
10 4
2
10 3
10 2 10 2
10 3
10 4
2
Mobility (cm /Vs)
Mobility (cm /Vs)
Fig. 13.10 (a) Mobility spectrum of GaAs/AlGaAs/InAs double quantum well structure. Adapted from [1099]. (b) Mobility spectrum of InAs/GaSb quantum well structure. Adapted from [1100]
13.2.2 FreeCarrier Absorption The absorption of free carriers was treated in Sect. 9.8.1 without the presence of a static magnetic field. Solving (13.8) for a static magnetic field B = μ0 H with H = H (hx , hy , hz ) and a harmonic electric field E ∝ exp(−iωt) yields for the dielectric tensor (cf. (9.60)) i = σ, (13.24) 0 ω and by comparing to j = σ E = q n v, ⎡
⎛
⎞⎤−1 0 −hz hy (ω) = −ωp∗2 ⎣(ω 2 + i ω γ) 1 − i ωc ⎝ hz 0 −hx ⎠⎦ , −hy hx 0
(13.25)
where 1 denotes the (3 by 3) unity matrix and γ = 1/τ = q/(m∗ μ) is the damping parameter with μ representing the optical carrier mobility (in the nonisotropic case a tensor γ needs to be used). The (unscreened) plasma frequency is given by (cmp. (9.65)) ωp∗ =
n
e2 . 0 m∗
(13.26)
13.2 Magnetic Fields
449
The freecarrier cyclotron frequency is ωc = e
μ0 H . m∗
(13.27)
If the effective mass is treated as a tensor, 1/m∗ is replaced by m∗ −1 in (13.26) and (13.27). For zero magnetic field the classical Drude theory for one carrier species is recovered (cf. (9.62a)) ωp∗2 . (13.28) (ω) = − ω (ω + iγ) With the magnetic field perpendicular to the sample surface, i.e. B = μ0 (0, 0, H) the magnetooptic dielectric tensor simplifies to (cf. (13.9d)) (ω) = ˜xx = ˜zz = ˜xy =
⎞ ˜xx i˜xy 0 − 2 ⎝ −i˜xy ˜xx 0 ⎠ ω 0 0 ˜zz 1 + iγ/ω (1 + iγ/ω)2 − (ωc /ω)2 1 (1 + iγ/ω) ωc /ω . (1 + iγ/ω)2 − (ωc /ω)2 ωp∗2
⎛
(13.29a) (13.29b) (13.29c) (13.29d)
The inplane component xx provides information about ωp∗ and γ, i.e. two of the three parameters n, μ and m∗ are known. Additionally, the antisymmetric tensor component xy is linear in the cyclotron frequency and provides q/m∗ . This subtle but finite birefringence depends on the strength (and orientation) of the magnetic field and can be experimentally determined in the infrared using magnetoellipsometry [1108, 1109]. Such ‘optical Hall effect’ experiment allows the determination of the carrier density n, the mobility μ, the carrier mass4 m∗ and the sign of the carrier charge sgn(q) with optical means. The electrical Hall effect (Sect. 13.2.1) can reveal n, μ and sgn(q) but cannot reveal the carrier mass.
13.2.3 Energy Levels in Bulk Crystals In a 3D electron gas (the magnetic field is along z, i.e. B = B[0, 0, 1]) the motion in the (x, y) plane is described by Landau levels. Quantum mechanically they correspond to levels of a harmonic oscillator. The magnetic field has no impact on 4 We
note that mobility and effective mass defined and measured in this way may be referred to as ‘optical’. Other definitions and approaches to the mobility or effective mass may give different results.
450
13 External Fields
(a)
(b)
kz
h
B
c
n=0 n=1 n=... n=nm
ky
kx EF 0 1/2
3/2
5/2
7/2 E F
E
Fig. 13.11 3D electron gas in an external magnetic field. (a) Allowed states in kspace for magnetic field along the z direction. (b) Density of states (DOS) ρ versus energy (in units of ωc ). Dashed line is threedimensional DOS without magnetic field. Based on [991]
the motion of electrons along z, such that in this direction a free dispersion relation ∝ kz2 is present. The energy levels are given as 1 2 2 ωc + k . Enkz = n + 2 2m z
(13.30)
Thus, the states are on concentric cylinders in kspace (Fig. 13.11a). The populated states of the 3D electron gas (at 0 K) lie within the Fermi vector of length kF . For the 3D system the density of states at the Fermi energy is a square root function of the Fermi energy (6.67). In the presence of a magnetic field the density of states diverges every time that a new cylinder (with a onedimensional density of states, (6.75)) touches the Fermi surface at EF . In real systems, the divergence will be smoothed, however, a pronounced peak or the periodic nature of the density of states is often preserved. The period is given by the number nm of cyclotron orbits (Landau levels) within the Fermi surface. 1 (13.31) ωc = EF . nm + 2 If the number of carriers is constant, the density of states at the Fermi energy at varying magnetic field varies periodically with 1/B. From the conditions nm + 21 1 eBm1 = EF and nm + 1 + 21 eBm2 = EF with B12 = B11 + ΔB we find 1 e = ∗ . ΔB m EF
(13.32)
13.2 Magnetic Fields
451
This periodicity is used to determine experimentally, e.g., the properties of the Fermi surface in metals using the Shubnikov–de Haas oscillations (of the magnetoresistance) or the de Haas–van Alphén effect (oscillation of the magnetic susceptibility). Equation (13.30) needs to be extended to account for the splitting (13.7) of the Landau level due to the electron spin. According to [1110] the electron Landau level energy can be written as
1 En = n + 2
eB ± ge∗ (E) μB B , m∗ (E)
(13.33)
with energy dependent effective mass and gfactor 1 1 Eg (Eg + Δ0 ) 2 1 + = m∗ (E) m∗ (0) 3Eg + 2Δ0 E + Eg E + Eg + Δ0 Eg (Eg + Δ0 ) 1 1 − ge∗ (E) = ge∗ (0) Δ0 E + Eg E + Eg + Δ0
(13.34a) (13.34b)
The band edge value m∗ (0) of the effective mass is given by (6.39) and that of the gfactor by 2 Δ0 EP . (13.35) ge∗ (0) = 2 1 − 3 Eg (Eg + Δ0 ) For large spinorbit splitting, the value of the gfactor deviates strongly from 2 and becomes negative.
13.2.4 Energy Levels in a 2DEG In a 2D electron gas (2DEG), e.g. in a quantum well or a potential well at a modulationdoped heterointerface, a free motion in z is not possible and kz is quantized. The energy levels (for each 2D subband) are only given by the cyclotron energy (Fig. 13.12a). The density of states is a sequence of δlike peaks (Fig. 13.12b). Each peak contributes (degeneracy gˆ of a Landau level) a total number of gˆ =
eB h
(13.36)
states (per unit area without spin degeneracy and without the degeneracy of the band extremum). In reality, disorder effects lead to an inhomogeneous broadening of these peaks. The states in the tails of the peaks correspond to states that are localized in real space. Also, in a 2D system several physical properties exhibit an oscillatory behavior as a function of Fermi level, i.e. with varying electron number, and as a function of the magnetic field at fixed Fermi energy, i.e. at fixed electron number (Fig. 13.13).
452
13 External Fields
(a)
(b)
ky
h
c
kx n=0 n=1 n=2 E E1
EF(0)
E1+h c/2
EF(0)
Fig. 13.12 2D electron gas in an external magnetic field. (a) Allowed states in kspace. (b) Density of states (DOS) ρ versus energy. Dashed line is twodimensional DOS without magnetic field. Thick vertical lines: δlike DOS without broadening, curves: broadened DOS. Based on [991]
13.2.5 Shubnikov–de Haas Oscillations From the 2D density of states (per unit area including spin degeneracy) D2D (E) = m∗ /π2 the sheet density of electrons ns can be expressed as a function of the Fermi level (at T = 0 K without spin degeneracy) ns =
m∗ EF . 2π 2
(13.37)
Using (13.32) we thus find (without spin degeneracy, without valley degeneracy), that the period of 1/B is ∝ ns : 1 e 1 . (13.38) = ΔB h ns The carrier density of a 2DEG can therefore be determined from the oscillations of magnetoresistance, and is proportional to the density of states at the Fermi level (Shubnikov–de Haas effect). A corresponding measurement with varying field and fixed electron density is shown in Fig. 13.14. The periodicity with 1/B is obvious. Since only the component of the magnetic field perpendicular to the layer affects the (x, y) motion of the carriers, no effect is observed for the magnetic field parallel to the layer. In another experiment the carrier density was varied at constant field (Fig. 13.15). The electron density in an inversion layer in ptype silicon is (linearly) varied with the gate voltage of a MOS (metal–oxide–semiconductor) structure (inset in Fig. 13.15, for MOS diodes cf. Sect. 24.5). In this experiment, the Fermi level was shifted through the Landau levels. The equidistant peaks show that indeed each Landau level contributes the same number of states.
13.3 Quantum Hall Effect
453
Fig. 13.13 Oscillatory (theory, T = 6 K) behavior of a 2DEG (GaAs/AlGaAs) in a magnetic field: (a) Fermi level, (b) magnetization, (c) specific heat, (d) thermoelectric power. A Gaussian broadening of 0.5 meV was assumed. Adapted from [991, 1111]
(meV)
35
(a)
30
25
(b)
Magnetization
30 20 10 0 10 20 30
(c)
15
10
5
Thermoelectric
0
(d)
0.3 0.2 0.1 0 0
2
4
6
8
10
13.3 Quantum Hall Effect In high magnetic fields, at low temperatures and for highmobility, 2D electron gases exhibit a deviation from the classical behavior. We recall that the classical Hall effect (i.e. considering the Lorentz force, classical Drude theory), the generation of a field Ey perpendicular to a current flow jx (cf. Sect. 13.2.1), was described with the conductivity tensor σ (here, for the (x, y)plane only)
454
13 External Fields
Fig. 13.14 Shubnikov–de Haas oscillations at a modulationdoped AlGaAs/GaAs heterostructure with a 2DEG, n = 1.7 × 1017 cm−2 and μ = 11 400 cm2 /Vs. Data from [1112]
H
AlGaAs/GaAs
0
Fig. 13.15 Shubnikov–de Haas oscillations of a 2DEG at the (100) surface of ptype silicon (100 cm) at a magnetic field of 33 kOe and T = 1.34 K. The inset shows schematically the contact geometry. Data from [1113]
2
layers
4
6
8
60
80
100
oxide n+
n+ silicon
0
20
40
σ0 1 ωc τ σ= 1 + ωc2 τ 2 −ωc τ 1 1 →0 σxx = σ0 1 + ωc2 τ 2 ωc τ ne σxy = σ0 → , 2 2 1 + ωc τ B
(13.39a) (13.39b) (13.39c)
where σ0 is the zerofield conductivity σ0 = ne2 τ /m∗ (8.5). The arrows denote the limit for ωc τ → ∞, i.e. large fields. The resistivity tensor ρ = σ −1 is given by ρxx ρxy ρ= −ρxy ρxx σxx →0 ρxx = 2 2 σxx + σxy
(13.40a) (13.40b)
13.3 Quantum Hall Effect
455
ρxy =
−σxy B →− . 2 + σxy ne
2 σxx
(13.40c)
13.3.1 Integral QHE Experiments yield strong deviations from the linear behavior of the transverse resistivity ρxy = Ey /jx = BRH with the Hall coefficient RH = −1/(ne) with increasing magnetic field is observed at low temperatures for samples with high carrier mobility, i.e. ωc τ 1 (Fig. 13.16). In Fig. 13.17a,b, Hall bars are shown for 2DEGs in silicon metal–oxide–semiconductor fieldeffect transistor (SiMOSFET) electron inversion layers and at GaAs/AlGaAs heterostructures, respectively. The Hall resistivity exhibits extended Hall plateaus with resistivity values that are given by 1 h , (13.41) ρxy = i e2 i.e. integer fractions of the quantized resistance ρ0 = h/e2 =25812.807… , which is also called the vonKlitzing constant. In Fig. 13.16, a spin splitting is seen for the n = 1 Landau level (and a small one for the n = 2). We note that the topmost Hall
Fig. 13.16 Hall resistivity ρxy and longitudinal resistivity ρxx for a modulationdoped GaAs/AlGaAs heterostructure (n = 4 × 1011 cm−2 , μ = 8.6 × 104 cm2 /Vs) at 50 mK as a function of magnetic field (10 kG=1 T). The numbers refer to the quantum number and spin polarization of the Landau level involved. The inset shows schematically the Hall bar geometry, VL (VH ) denotes the longitudinal (Hall) voltage drop. Reprinted with permission from [1114], ©1982 APS
456
13 External Fields
Fig. 13.17 (a) Silicon MOS (metal–oxide–semiconductor) structure of K. v. Klitzing’s et al. original experiments. (b) GaAs/AlGaAs heterostructure sample grown with molecular beam epitaxy for QHE measurements, chip carrier and bond wires. Reprinted with permission from [1115]
plateau is due to the completely filled n = 0 Landau level; the resistance is ρ0 /2 due to the spin degeneracy of 2. The integral quantum Hall effect, first reported in [1116, 1117], and the value for ρ0 are found for a wide variety of samples and conditions regarding sample temperature, electron density or mobility of the 2DEG and the materials of the heterostructure. Within the plateau the resistivity is well defined within 10−7 or better up to 4 × 10−9 . A precise determination allows for a new normal for the unit Ohm [1118, 1119], being two orders of magnitude more precise than the realization in the SI system, e2 1 . At the same and an independent value for the finestructure constant α = c 4π0 time, the longitudinal resistivity, starting from the classical value for small magnetic fields, exhibits oscillations and eventually it is zero for the plateaus in ρxy . For ρxx values of 10−10 / have been measured, which corresponds to 10−16 /cm for bulk material, a value three orders of magnitude smaller than for any nonsuperconductor. The interpretation of the quantum Hall effect(s) is discussed in [1120] among many other treatises. The simplest explanation is that the conductivity is zero when a Landau level is completely filled and the next is completely empty, i.e. the Fermi level lies between them. The temperature is small, i.e. kT ωc , such that no scattering between Landau levels can occur. Thus no current, similar to a completely filled valence band, can flow. The sheet carrier density ns is given by counting the i filled Landau levels (degeneracy according to (13.36)) as ns = i
eB . h
(13.42)
13.3 Quantum Hall Effect
457
In the transverse direction energy dissipation takes place and the Hall resistivity ρxy = B/(ns e) takes the (scatteringfree) values given in (13.41). However, this argument is too simple as it will not explain the extension of the plateaus. As soon as the system has one electron more or less, the Fermi energy will (for a system with δlike density of states) be located in the upper or lower Landau level, respectively. Then, the longitudinal conductivity should no longer be zero and the Hall resistivity deviates from the integer fraction of ρ0 . Therefore (in the localization model) an inhomogeneous (Gaussian) broadening of the density of states is assumed. Additionally, the states in the tails of the distribution are considered nonconducting, i.e. localized, while those around the peak are considered conductive. This mobility edge is schematically shown in Fig. 13.18a–c. When the Fermi level crosses the density of states of the broadened Landau level (upon increase of the magnetic field), it first populates localized states and ρxx remains at zero. When the Fermi level crosses the delocalized, conducting states, the longitudinal conductivity shows a peak and the Hall conductivity increases from the plateau value by e2 /h to the next plateau. When the Fermi level lies within the upper nonconducting states, the Hall resistivity remains constant in the next plateau. For the sample in Fig. 13.16 it has been estimated that 95 % of the Landau level states are localized [1114]. In the localization model it is still astonishing that the samples exhibit the step of e2 /h in the conductivity as if all electrons on the Landau level contribute to conduction, cf. (13.42). According to the calculations in [1123] the Hall current lost by the localized states is compensated by an extra current by the extended states. The behavior of the electrons in the quantum Hall regime (‘quantum Hall liquid’) can be considered similar to that of an incompressible fluid where obstructions lead the fluid to move with increased velocity. Nevertheless, the single particle picture seems to be insufficient to model the IQHE. Another model for the explanation of the QHE, supported now with plenty of experimental evidence, is the edge state model where quantized onedimensional conductivity of edge channels, i.e. the presence of conductive channels along the sample boundaries, is evoked [1124]. Due to depletion at the boundary of the sample, the density of the 2DEG varies at the edge of the sample and ‘incompressible’ stripes develop for which ∂μ/∂ns → ∞. When the filling factor is far from an integer, the Hall voltage is found to vary linearly across the conductive channel and the current is thus homogeneous over the sample (Fig. 13.18d). In the Hall plateau, the Hall voltage is flat in the center of the channel and exhibits drops at the edges, indicating that the current flows along the boundary of the sample (edge current) [1122] in agreement with predictions from [1125]. Although the current pattern changes with varying magnetic field, the Hall resistivity remains at its quantized value. The most fundamental arguments for the explanation of the IQHE come from gauge invariance and the presence of a macroscopic quantum state of electrons and magnetic flux quanta [1126]. This model holds as long as there are any extended states at all.
458
13 External Fields
(d)
D(E)
(a)
xx
(b)
2
(c)
xy
e /h
0
1
Fig. 13.18 (a) Density of states D(E), (b) longitudinal conductivity σxx and (c) Hall conductivity σxy for a Landau level as a function of the filling factor μ = n/d, where n is the electron density and d the degeneracy of the level. In (a) the filling factor relates via the position of the Fermi level to an energy scale. The grey areas in (a) denote localized states. The slanted dashed line in (c) has a slope of ne/B. Adapted from [1121]. (d) Normalized Hall potential profile for different magnetic fields around filling factor ν = 2. The overall voltage drop corresponds to 20 mV. The insets show the sample geometry and transport data. The 2DEG is from a GaAs/Al0.33 Ga0.67 As modulationdoped heterostructure, ns = 4.3 × 1011 cm−2 , μ = 5 × 105 cm2 /Vs, T = 1.4 K. Adapted from [1122]
13.3.2 Fractional QHE For very low temperatures and in the extreme quantum limit, novel effects are observed when the kinetic energy of the electrons is smaller than their Coulomb interaction. New quantum Hall plateaus are observed at various fractional filling factors ν = p/q. We note that the effects of the fractional quantum Hall effect (FQHE) in Fig. 13.19 mostly arise for magnetic fields beyond the n = 1 IQHE plateau. The filling factor ν = n/(eB/h) is now interpreted as the number of electrons per magnetic flux quantum φ0 = h/e.
459
R xx
R xy (h/e 2)
13.3 Quantum Hall Effect
Fig. 13.19 Hall resistance Rxy and magnetoresistance Rxx of a twodimensional electron system (GaAs/AlGaAs heterostructure) of density n = 2.33 × 1011 cm−2 at a temperature of 85 mK, versus magnetic field B. Numbers identify the filling factor ν, which indicates the degree to which the sequence of Landau levels is filled with electrons. Plateaus are due to the integral (ν = i) quantum Hall effect (IQHE) and fractional (ν = p/q) quantum Hall effect (FQHE). Adapted from [1127], reprinted with permission, ©1990 AAAS
The effects of the FQHE cannot be explained by singleelectron physics. The plateaus at fractional fillings ν occur when the Fermi energy lies within a highly degenerate Landau (or spin) level and imply the presence of energy gaps due to manyparticle interaction and the result of correlated 2D electron motion in the magnetic field. A decisive role is played by the magnetic flux quanta. The presence of the magnetic field requires the manyelectron wavefunction to assume as many zeros per unit area as there are flux quanta penetrating√it. The decay of the wavefunction has a length scale of the magnetic length l0 = /(eB). Since the magnetic field implies a 2π phase shift around the zero, such an object is also termed a vortex, being the embodiment of the magnetic flux quanta in the electron system. Such a vortex represents a charge deficit (compared to a homogeneous charge distribution) and thus electrons and vortices attract each other. If a vortex and an electron are placed onto each other, considerable Coulomb energy is gained. At ν = 1/3, there are three times more vortices than there are electrons, each vortex representing a charge deficit of 1/3 e. Such a system is described with manyparticle wavefunctions, such as the Laughlin theory for ν = 1/q [1126] and novel quasiparticles called composite fermions[1128, 1129] for other fractional fillings. For further reading we refer readers to [1130]and references therein.
460
13 External Fields
(a)
(a)
(b)
(b)
Fig. 13.20 Weiss oscillations: (a) magnetoresistance and (b) Hall resistance of an antidot lattice (inset in (a)) with pattern (solid lines) and without pattern (dashed lines) at T = 1.5 K. (b) Schematic of the different orbits: (‘p’: pinned, ‘d’: drifting, ‘s’: scattered). Reprinted with permission from [1131], ©1991 APS
13.3.3 Weiss Oscillations In Fig. 13.20, measurements are shown for a Hall bar in which an array of antidots (in which no conduction is possible) has been introduced by dry etching. The antidot size is 50 nm (plus depletion layer) and the period is 300 nm. These obstructions for the cyclotron motion lead to a modification of the magnetotransport properties. Before etching of the antidot array the 2DEG has a mean free path length of 5–10 μm at 4 K for the mobility of ≈ 106 cm2 /Vs. At low magnetic fields there is a strong deviation of the Hall resistivity from the straight line to which the QHE levels converge. Similarly, ρxx shows a strong effect as well. These effects are related to commensurability effects between the antidot lattice and the cyclotron resonance path. When the cyclotron orbit is equal to the lattice period, electrons can fulfill a circular motion around one antidot (pinned orbit, Fig. 13.20b) that leads to a reduction of conductivity. At high fields, drifting orbits for which the cyclotron orbit is much smaller than the lattice period occur. At small fields, scattering orbits also contribute for which the cyclotron radius is large and the electron has antidots from time to time. Resonances in the Hall resistivity have been found due to pinned orbits enclosing 1, 2, 4, 9 or 21 antidots.
Chapter 14
Nanostructures
The principles of physics, as far as I can see, do not speak against the possibility of maneuvering things atom by atom. R.P. Feynman, 1959 [1132]
Abstract Onedimensional nanostructures (quantum wires) and zerodimensional ones (quantum dots) are discussed with regard to their various fabrication methods and the tunable physical properties in such systems. Main effects covered are the modified density of states, confined energy levels, (envelope) wavefunction symmetry and the resulting novel electrical and optical properties.
14.1 Introduction When the structural size of functional elements enters the size range of the de Broglie matter wavelength, the electronic and optical properties are dominated by quantummechanical effects. The most drastic impact can be seen from the density of states (Fig. 14.1). The quantization in a potential is ruled by the Schrödinger equation with appropriate boundary conditions. These are simplest if an infinite potential is assumed. For finite potentials, the wavefunction leaks out into the barrier. Besides making the calculation more complicated (and more realistic), this allows electronic coupling of nanostructures. Via the Coulomb interaction, a coupling is even given if there is no wavefunction overlap. In the following, we will discuss some of the fabrication techniques and properties of quantum wires (QWR) and quantum dots (QD). In particular for the latter, several textbooks can also be consulted [1133, 1134].
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_14
461
462
14 Nanostructures
Fig. 14.1 Schematic geometry and density of states for 3D, 2D, 1D and 0D electronic systems
14.2 Quantum Wires 14.2.1 VGroove Quantum Wires Quantum wires with high optical quality, i.e. high recombination efficiency and welldefined spectra, can be obtained by employing epitaxial growth on corrugated substrates. The technique is shown schematically in Fig. 14.2. A Vgroove is etched, using, e.g., an anisotropic wet chemical etch, into a GaAs substrate. The groove ¯ . Even when the etched pattern is not very sharp on the direction is along 110
14.2 Quantum Wires
463
Fig. 14.2 Schematic cross section of a GaAs/AlGaAs heterostructure grown on a channeled substrate, illustrating the concept of selfordered quantumwire fabrication. Adapted from [1135]
bottom, subsequent growth of AlGaAs sharpens the apex to a selflimited radius ρl of the order of 10 nm. The side facets of the groove are {111}A. Subsequent deposition of GaAs leads to a larger upper radius ρu > ρl of the heterostructure. The GaAs QWR formed in the bottom of the groove is thus crescentshaped as shown in Fig. 14.3. A thin GaAs layer also forms on the side facets (sidewall quantum well) and on the top of the ridges. Subsequent growth of AlGaAs leads to a resharpening of the Vgroove to the initial, selflimited value ρl . The complete resharpening after a sufficiently thick AlGaAs layer allows vertical stacking of crescentshaped QWRs of virtually identical size and shape, as shown in Fig. 14.4. In this sense, the selflimiting reduction of the radius of curvature and its recovery during barrierlayer growth leads to selfordering of QWR arrays whose structural parameters are determined solely by growth parameters. The lateral pitch of such wires can be down to 240 nm. Fig. 14.3 Transmission electron microscopy crosssectional image of a crescentshaped single GaAs/AlGaAs quantum wire. From [1136]
464
14 Nanostructures
Fig. 14.4 TEM crosssectional image of a vertical stack of identical GaAs/AlGaAs crescentshaped QWRs. From [1135]
To directly visualize the lateral modulation of the band gap, a lateral cathodoluminescence (CL) linescan perpendicular across the wire is displayed in Fig. 14.5. In Fig. 14.5a, the secondary electron (SE) image of the sample from Fig. 14.3 is shown in plan view. The top ridge is visible in the upper and lower parts of the figure, while in the middle the sidewalls with the QWR in the center are apparent. In Fig. 14.5b, the CL spectrum along a linescan perpendicular to the wire (as indicated by the white line in Fig. 14.5a) is displayed. The xaxis is now the emission wavelength, while the yaxis is the lateral position along the linescan. The CL intensity is given on a logarithmic scale to display the full dynamic range. The top QW shows almost no variation in band gap energy (λ = 725 nm); only directly at the edge close to the sidewall does a second peak at lower energy (λ = 745 nm) appear, indicating a thicker region there. The sidewall QW exhibits a recombination wavelength of 700 nm at the edge to the top QW, which gradually increases to about 730 nm at the center of the Vgroove. This directly visualizes a linear tapering of the sidewall QW from about 2.1 nm thickness at the edge to 3 nm in the center. The QWR luminescence itself appears at about 800 nm. After fast capture from the barrier into the QWs and, to a much smaller extent corresponding to its smaller volume, into the QWR, excess carrierswill diffuse into the QWR via the adjacent sidewall QW and the vertical QW. The tapering of the sidewall QW induces an additional drift current.
14.2 Quantum Wires
465
Fig. 14.5 (a) Planview SE image of single QWR (sample A), showing top and sidewall with QWR in the center. The white line indicates the position of the linescan on which the CL spectra linescan (b) has been taken at T = 5 K. The CL intensity is given on a logarithmic grey scale to display the full dynamic range as a function of wavelength and position along the white line in (a). From [1136]
14.2.2 CleavedEdge Overgrowth Quantum Wires Another method to create quantum wires of high structural perfection is cleavededge overgrowth (CEO) [1137], shown schematically in Fig. 14.6. First, a layered structure is grown (single or multiple quantum wells or superlattice). Then, a {110} facet is fabricated by cleaving (in vacuum) and epitaxy is continued on the cleaved facet. At the junctures of the {110} layer and the original quantum wells QWRs form. Due to their crosssectional form they are also called Tshaped QWRs. A second cleave and another growth step allow fabrication of CEO quantum dots [1138, 1139] (Fig. 14.6c).
14.2.3 Nanowhiskers Whiskers are primarily known as thin metal spikes and have been investigated in detail [1140]. Semiconductor whiskers can be considered as (fairly short) quantum wires. They have been reported for a number of materials, such as Si, GaAs, InP and ZnO [1141]. A field of ZnO whiskers is shown in Fig. 14.7. If heterostructures are
466
14 Nanostructures
(b) (c) (a)
(d)
50nm
QW cleavage plane
[001] QW
Fig. 14.6 Principle of CEO quantum wires and 2fold CEO quantum dots. Part (a) depicts a layered structure (quantum wells or superlattice, blue), (b) describes the growth on the cleaved facet used for fabrication of quantum wires. In (c) a second cleave and growth on top of the plane allows the fabrication of quantum dots. From [1138]. (d) Crosssectional TEM image of CEO GaAs/AlGaAs quantum wires. Two quantum wells (QW) and the QWR at their junction are labeled. The first epitaxy was from left to right. The second epitaxy step was on top of the cleavage plane (dashed line) in the upward direction. Adapted from [1139], reprinted with permission, ©1997 APS
incorporated along the whisker axis [1142], quantum dots or tunneling barriers can be created (Fig. 14.8). The nanocrystal can also act as a nanolaser [1143, 1144]. In ZnO nanowhiskers the conversion of mechanical energy into electrical energy has been demonstrated [1145] based on the piezoelectric effect (Sect. 15.4). The critical thickness h c in nanowire heterostructure is strongly modified from the 2D situation (Sect. 5.4.1). Based on the strain distribution of a misfitted slab in a cylindrical wire [1148] the dependence of critical thickness on the nanowhisker radius r was developed [1149, 1150]. For given misfit there is a critical radius rc for which h c is infinite for r < rc (Fig. 14.9).
14.2 Quantum Wires
467
(a)
(b)
Fig. 14.7 (a) Array of ZnO nanowhiskers on sapphire, fabricated using thermal evaporation. Adapted from [1146]. (b) Single, freestanding ZnO nanowire fabricated using PLD. Adapted from [1147] Fig. 14.8 TEM image of a part of an InAs whisker 40 nm in diameter that contains InP barriers. The zooms show sharp interfaces. On top of the whisker is a gold droplet from the socalled vapor–liquid–solid growth mechanism. The whisker axis is [001], the viewing direction is [110]. Adapted from [1142], reprinted with permission, ©2002 AIP
Au InAs InP InAs InP InAs
14.2.4 Nanobelts A number of beltshaped nanostructures has been reported [1141]. These are wirelike, i.e. very long in one dimension. The crosssection is rectangular with a high ¯ aspect ratio. In Fig. 14.10a ZnO nanobelts are shown. The wire direction is [21.0]. The large surface is (00.1), the thickness of the belt extends in [01.0]direction. High resolution transmission microscopy (Fig. 14.10b) shows that these structures are defectfree. The pyroelectric charges on the ZnO (0001) surfaces (Sect. 15.2) lead to the formation of open (Fig. 14.11c) spirals. Closed spirals (Fig. 14.11a) occur if
468
14 Nanostructures
Fig. 14.9 Critical radius rc above which an infinitely thick layer with misfit grows coherently on a cylindrical nanowire (relaxation by 60◦ dislocations, b = 0.4 nm, ν = 1/3). Adapted from [1150]
(a)
(b)
Fig. 14.10 (a) SEM image of an ensemble of ZnO nanobelts. (b) HRTEM image of a single ZnO nanobelt, viewing direction is [00.1]. The inset shows the diffraction pattern. Adapted from [1151]
the short dimension is along [00.1] and alternating charges become compensated in a ‘slinky’like ring (Fig. 14.11b).
14.2.5 Quantization in TwoDimensional Potential Wells The motion of carriers along the quantum wire is free. In the crosssectional plane the wavefunction is confined in two dimensions. The simplest case is for constant cross section along the wire. However, generally the cross section along the wire may change and therefore induce a potential variation along the wire. Such potential variation will impact the carrier motion along the longitudinal direction. Also, a twist of the wire along its axis is possible. In Fig. 14.12, the electron wavefunctions in a Vgroove GaAs/AlGaAs QWR are shown. Further properties of Vgroove QWRs have been reviewed in [1153].
14.2 Quantum Wires
(a)
469
(b)
(c)
Fig. 14.11 (a) Bright field and (b) dark field TEM image of a ZnO nanoring formed by the ‘slinky’like growth of a nanobelt. (c) SEM image of an open ZnO nanospiral. The insets in (a, c) show schematically the surface charge distribution. Adapted from [1152] Fig. 14.12 Electron wavefunctions (Ψ 2 on logarithmic grey scale) for the first three confined levels for the QWR of Fig. 14.3. From [1136]
n=1
n=2
n=3
In Fig. 14.13, the excitonic electron and hole wavefunctions are shown for a (strained) Tshaped QWR. In Fig. 14.14a the atomic structure of a very thin ZnO nanowhisker with a crosssection consisting of seven hexagonal unit cells is shown. The theoretical onedimensional band structure [1155] is shown in Fig. 14.14b together with the charge density of the lowest conduction band state (LUMO) and the highest valence band state (HOMO). The band gap is generally too small because of the LDA method used.1 In [1155] also the properties of nanowires with various diameters are compared. The HOMO at Γ lies only 80 meV above the top of valence band of bulk ZnO, and its position changes little with the wire diameter. It is mainly composed by surface oxygen 2p like dangling bonds (Fig. 14.14d). The LUMO (Fig. 14.14c) is delocalized in the whole nanowire, indicating that it is a bulk state. The delocalized LDA in [1155] yields E g = 0.63 eV for the bulk ZnO band gap; its experimental value is 3.4 eV. 1 The
470
14 Nanostructures
hh
e
(a)
[110]
[110]
[001]
(b) [110] [001] Fig. 14.13 (a) Threedimensional view of the electron and (heavy) hole part of the excitonic wavefunction in a 4 × 5 nm Tshaped In0.2 Ga0.8 As/GaAs QWR. The orbitals correspond to 70 % probability inside. (b) Cross section through the electron and hole orbitals in their center along the wire direction. Reprinted with permission from [1154], ©1998 APS
(b)
(a)
(c)
(d)
Fig. 14.14 (a) Atomic arrangement of a 1 nm wide ZnO nanowire. (b) Theoretical band structure and charge density of the (c) lowest conduction band and (d) highest valence band state. Adapted from [1155]
distribution is also responsible for the large dispersion of the LUMO from Γ to A. The energy of the LUMO increases substantially with decreasing diameter due to the radial confinement.
14.3 Quantum Dots
471
14.3 Quantum Dots 14.3.1 Quantization in ThreeDimensional Potential Wells The solutions for the ddimensional (d = 1, 2, or 3) harmonic oscillator, i.e. the eigenenergies for the Hamiltonian 1 p2 + m ω02 xi2 Hˆ = 2m 2 i=1 d
are given by
d En = n + 2
(14.1)
ω0 ,
(14.2)
with n = 0, 1, 2, . . . . More detailed treatments can be found in quantummechanics textbooks. Next, we discuss the problem of a particle in a centrosymmetric finite potential well with different masses m 1 in the dot and m 2 in the barrier. The Hamiltonian and the potential are given by 2 ∇ + V (r ) Hˆ = ∇ 2m −V0 , r ≤ R0 . V (r ) = 0 , r > R0
(14.3) (14.4)
The wavefunction can be separated into radial and angular components Ψ (r) = Rnlm (r ) Ylm (θ, φ), where Ylm are the spherical harmonic functions. For the ground state (n = 1) the angular momentum l is zero and the solution for the wavefunction (being regular at r = 0) is given by sin(k r ) R(r ) =
kr sin(k R0 ) k R0
, r ≤ R0 exp (−κ (r − R0 )) , r > R0
2 m 1 (V0 + E) 2 2 m 2 E . κ2 = − 2 k2 =
(14.5b) (14.5c)
From the boundary conditions that both R(r ) and interface at r = R0 , the transcendental equation k R0 cot (k R0 ) = 1 −
(14.5a)
1 ∂ R(r ) m ∂r
are continuous across the
m1 (1 + κ R0 ) m2
(14.6)
472
14 Nanostructures
is obtained. From this formula the energy of the single particle ground state in a spherical quantum dot can be determined. For a given radius, the potential needs a certain strength V0,min to confine at least one bound state; this condition can be written as V0,min =
π 2 2 8 m ∗ R02
(14.7)
for m 1 = m 2 = m ∗ . For a general angular momentum l, the wavefunctions are given by spherical Bessel functions jl in the dot and spherical Hankel functions h l in the barrier. Also, the transcendental equation for the energy of the first excited level can be given: k2 R2 . (14.8) k R0 cot (k R0 ) = 1 + m 2+2κ R +κ02 R 2 1 0 0 − 2 m2 1+κ R0 In the case of infinite barriers (V0 → ∞), the wavefunction vanishes outside the dot and is given by (normalized) Rnml (r ) =
2 jl (knl r ) , 3 j R0 l+1 (knl R0 )
(14.9)
where knl is the nth zero of the Bessel function jl , e.g. kn0 = nπ. With twodigit precision the lowest levels are determined by knl
l=0l=1l=2l=3 l=4l=5
n = 0 3.14 4.49 5.76 6.99 8.18 9.36 n = 1 6.28 7.73 9.10 10.42 n = 2 9.42
The (2l + 1) degenerate energy levels E nl are (V0 = ∞, m = m 1 ): E nl =
2 2 knl . 2m R02
(14.10)
The 1s, 1p, and 1d states have smaller eigenenergies than the 2 s state. A particularly simple solution is given for a cubic quantum dot of side length a0 and infinite potential barriers. One finds the levels E n x n y n z : Enx n y nz =
2 2 n 2x + n 2y + n 2z , π 2m a02
(14.11)
with n x , n y , n z = 1, 2, . . . . For a sphere, the separation between the ground and first excited state is E 1 − E 0 ≈ E 0 , for a cube and a twodimensional harmonic
14.3 Quantum Dots C0
473 C1
C2
C3
(a)
Electrons
V0
V1
V2
V3
(b)
V0
87.6%
V1
81.8%
V2
76.2%
V3
74.6%
V0
9.6%
V1
13.7%
V2
17.6%
V3
21.0%
V0
2.3%
V1
3.6%
V2
5.3%
V3
3.0%
(c) Holes
(d)
(e)
Fig. 14.15 Isosurface plots (25 % of maximum value) of the total probability densities (a, b) and valenceband projections (c)–(e) of bound electron (a) and hole (b)–(e) states in a model pyramidal InAs/GaAs quantum dot with base length b = 11.3 nm. The percentages are the integrals of the projections to the bulk heavy, light and splitoff hole bands, respectively, and the isosurfaces show the corresponding projection shapes. For each valenceband state the difference from 100 % is the
∞ integral −∞ ψs↑ 2 + ψs↓ 2 d3 r of the stype (conduction band) Bloch function projection (not shown). Reprinted with permission from [1159]
oscillator it is exactly E 0 . For a threedimensional harmonic oscillator this quantity is E 1 − E 0 = 2E 0 /3. For realistic quantum dots a full threedimensional simulation of strain, piezoelectric fields and the quantummechanical confinement must be performed [1156, 1157]. In Fig. 14.15, the lowest four electron and hole wavefunctions in a pyramidal InAs/GaAs quantum dot (for the strain distribution see Fig. 5.27 and for the piezoelectric fields see Fig. 15.16) are shown. The figure shows that the lowest hole states have dominantly heavyhole character and contain admixtures of the other hole bands. The wavefunction in such quantum dots can be imaged using scanning tunneling microscopy [1158].
14.3.2 Electrical and Transport Properties The classical electrostatic energy of a quantum dot with capacitance C that is capacitively coupled to a gate (Fig. 14.16) at a bias voltage Vg is given by
474
14 Nanostructures
(a)
(b)
VSD
acts
source
drain
gate VG
Fig. 14.16 (a) Schematic drawing of a quantum dot with tunnel contacts and gate electrode. (b) Realization with an inplane gate structure. The distance between ‘F’ and ‘C’ (gate electrode) is 1 µm. Electron transport occurs from a 2DEG between 3/F to 4/F through the quantum points contacts 1/3 and 2/4. Part (b) reprinted with permission from [1160]
E=
Q2 − Q α Vg , 2C
(14.12)
where α is a dimensionless factor relating the gate voltage to the potential of the island and Q is the charge of the island. Mathematically, minimum energy is reached for a charge Q min = α C Vg . However, the charge has to be an integer multiple of e, i.e. Q = N e. If Vg has a value, such that Q min /e = Nmin is an integer, the charge cannot fluctuate as long as the temperature is low enough, i.e. kT
e2 . 2C
(14.13)
Tunneling into or out of the dot is suppressed by the Coulomb barrier e2 /2C, and the conductance is very low. Analogously, the differential capacitance is small. This effect is called Coulomb blockade. Peaks in the tunneling current (Fig. 14.17b), conductivity (Fig. 14.17a) and the capacitance occur, when the gate voltage is such that the energies for N and N + 1 electrons are degenerate, i.e. Nmin = N + 21 . The expected level spacing is e α ΔVg =
e2 + Δ N , C
(14.14)
where Δ N denotes the change in lateral (kinetic) quantization energy for the added electron. e2 /C will be called the charging energy in the following. A variation of the source–drain voltage (for a given gate voltage) leads to a socalled Coulomb staircase since more and more channels of conductivity contribute to the current through the device (Fig. 14.18). Single electron tunneling (SET) is investigated with respect to metrology for a novel ampere standard [1118].
(a) 1.0
(b) 1.0 Current (nA)
475
2
14.3 Quantum Dots
0.5
0 0.6
0.55
0.5
0.5 0
0.5
0
1
1
SourceDrain Voltage VSD (mV)
G
Fig. 14.17 (a) Conductivity (Coulomb oscillations) and (b) current–voltage diagram at different gate voltages (Coulomb staircase, shifted vertically for better readability) of a tunnel junction with a quantum dot as in Fig. 14.16. Adapted from [1160]
(a)
(b)
(c)
(d)
(e)
(f)
Fig. 14.18 Chemical potentials of source and drain and of a quantum dot in between them. (a), (b), and (c) show the sequence for a variation of the gate voltage and visualize the origin of the Coulomb oscillations (see Fig. 14.17a). (d), (e) and (f) visualize a variation of the source–drain voltage and the origin of the Coulomb staircase (cf. Fig. 14.17b)
A lot of research so far has been done on lithographically defined systems where the lateral quantization energies are small and smaller than the Coulomb charging energy. In this case, periodic oscillations are observed, especially for large N . A deviation from periodic oscillations for small N and a characteristic shell structure (at N = 2, 6, 12) consistent with a harmonic oscillator model (ω0 ≈ 3 meV) has been reported for ≈500nm diameter mesas (Fig. 14.19b, c). In this structure, a small mesa has been etched and contacted (top contact, substrate back contact and side gate). The quantum dot consists of a 12nm In0.05 Ga0.95 As quantum well that is laterally constricted by the 500nm mesa and vertically confined due to 9 and 7.5nm thick Al0.22 Ga0.68 As barriers (Fig. 14.19a). By tuning the gate voltage, the number
476
14 Nanostructures
(b)
(c) (a)
Fig. 14.19 (a) Schematic sample geometry for sidegated In0.05 Ga0.95 As/Al0.22 Ga0.68 As diskshaped quantum dot. (b) Coulomb oscillations in the current versus gate voltage at B = 0 T observed for a D = 0.5 µm diskshaped dot. (c) Addition energy versus electron number for two different dots with D = 0.50 and 0.44 µm. Adapted from [1161]
of electrons can be varied within 0 and 40. Measurements are typically carried out at a sample temperature of 50 mK. In the sample shown in Fig. 14.20, selfassembled QDs are positioned in the channel under a splitgate structure. In a suitable structure, tunneling through a single QD is resolved. In small selfassembled quantum dots singleparticle level separations can be larger than or similar to the Coulomb charging energy. Classically, the capacitance for a metal sphere of radius R0 is given as C0 = 4π 0 r R0 ,
(14.15)
e.g. C0 ≈ 6 aF for R0 = 4 nm in GaAs, resulting in a charging energy of 26 meV. Quantum mechanically, the charging energy is given in firstorder perturbation theory by E 21 = 00Wee 00 =
Ψ02 (re1 ) Wee (re1 , re2 ) Ψ02 (re2 ) d3 re1 d3 re2 ,
(14.16)
14.3 Quantum Dots
477
Fig. 14.20 (a) Schematic layer sequence of epitaxial structure comprising a nAlGaAs/GaAs heterointerface with a twodimensional electron gas and a layer of InAs/GaAs quantum dots. (b) and (c) are corresponding band diagrams with no gate bias and gate voltage below the critical value, respectively. (d) Experimental dependence of drain current on gate voltage in a splitgate structure at a drain source voltage of 10 µV. Inset: Dependence of valley current on temperature (squares) with theoretical fit. Reprinted with permission from [1162], ©1997 AIP
where Wee denotes the Coulomb interaction of the two electrons and Ψ0 the ground state (single particle) electron wavefunction. The matrix element gives an upper bound for the charging energy since the wavefunctions will rearrange to lower their overlap and the repulsive Coulomb interaction. For lensshaped InAs/GaAs quantum dots with radius 25 nm a charging energy of about 30 meV has been predicted.
14.3.3 SelfAssembled Preparation The preparation methods for QDs split into topdown (lithography and etching ) and bottomup (selfassembly) methods. The latter achieve typically smaller sizes and require less effort (at least concerning the machinery). Artificial Patterning Using artificial patterning, based on lithography and etching (Fig. 14.21), quantum dots of arbitrary shape can be made (Fig. 14.22). Due to defects introduced by highenergy ions during reactive ion etching the quantum efficiency of such structures is very low when they are very small. Using wetchemical etching techniques the damage can be significantly lowered but not completely avoided. Since the QDs have to compete with other structures that can be made structurally perfect, this is not acceptable. Template Growth Template growth is another technique for the formation of nanostructures. Here, a mesoscopic structure is fabricated by conventional means. The nanostructure is created using sizereduction mechanisms, e.g. faceting, (Fig. 14.23). This method
478
14 Nanostructures
Fig. 14.21 Lithography and etching techniques for the fabrication of semiconductor structures
can potentially suffer from low template density, irregularities of the template, and problems of reproducibility. Colloids Another successful route to nanocrystals is the doping of glasses with subsequent annealing (color filters). When nanocrystals are prepared in a solgel process, the nanoparticles are present as a colloid in wet solution (Fig. 14.24). With the help of suitable stabilizing agents they are prevented from sticking to each other and can be handled in ensembles and also individually. Mismatched Epitaxy The selfassembly (or selforganization) relies on strained heterostructures that achieve energy minimization by island growth on a wetting layer (Stranski– Krastanow growth mode, see Sect. 12.2.3 and [1133]). Additional ordering mechanisms [1166, 1167] lead to ensembles that are homogeneous in size2 [1168] and shape [1169] (Fig. 14.25). 2 The ordering in size is remarkable. Typically Ostwald ripening (due to the Gibbs–Thomson effect; smaller droplets have larger vapor pressure and dissolve, larger droplets accordingly grow) occurs in an ensemble of droplets or nuclei. In the case of strained QDs, surface energy terms stabilize a certain QD size.
14.3 Quantum Dots
479
Fig. 14.22 Quantum dots of various shapes created by lithography and etching techniques. From [1163]
Fig. 14.23 (a) Schematic representation of growth on top of a predefined template, (b) crosssectional TEM of quantum dot formation at the apex. Reprinted with permission from [1164], ©1992 MRS
Fig. 14.24 CdSe colloidal nanoparticles. From [1165]
480
14 Nanostructures
Fig. 14.25 Selforganized formation of InGaAs/GaAs quantum dots during epitaxy. Left Planview and crosssectional transmission electron micrographs. Right Histogram of vertical and lateral size of the quantum dots. Reprinted with permission from [1170], ©1993 AIP
embedded vacuum
E strain
2.2
InAs
(eV/nm3)
GaAs
EQD E2D GaAs
QD
2D
GaAs
Barr
QD
0
Fig. 14.26 Distribution of strain energy for (left) uncapped island and (right) island embedded in host matrix. Numerical values are for InAs/GaAs
When a thin layer of a semiconductor is grown on top of a flat substrate with different lattice constant, the layer suffers a tetragonal distortion (Sect. 5.3.3). Strain can only relax along the growth direction (Fig. 14.26). If the strain energy is too large (highly strained layer or large thickness), plastic relaxation via dislocation formation occurs. If there is island geometry, strain can relax in all three directions and about 50 % more strain energy can relax, thus making this type of relaxation energetically favorable. When the island is embedded in the host matrix, the strain energy is similar to the 2D case and the matrix becomes strained (metastable state). When such QD layers are vertically stacked, the individual quantum dots grow on top of each other (Fig. 14.27) if the separation is not too large (Fig. 14.29). This effect is due to the effect of the underlying QD. In the case of InAs/GaAs (compressive strain), the buried QD stretches the surface above it (tensile surface strain). Thus, atoms impinging in the next QD layer find a smaller strain right on top of the buried
14.3 Quantum Dots
481
Fig. 14.27 Crosssectional TEM image of a stack of five layers of quantum dots. Due to strain effects, vertical arrangement is achieved Fig. 14.28 Crosssectional STM image of a stack of five InAs quantum dots in a GaAs matrix. Individual In atoms can be observed inbetween the wetting layers and the quantum dots. Each quantum dot layer was formed by growing 2.4 ML of InAs. The intended distance between the quantum dot layers was 10 nm. Image size is 55 × 55 nm2 . Reprinted with permission from [1171], ©2003 AIP
QDs. In STM images of the cross section through (XSTM) such a stack (Fig. 14.28) individual indium atoms are visible and the shape can be analyzed in detail [1171]. The vertical arrangement can lead to further ordering since a homogenization in lateral position takes place. If two QDs in the first layers are very close, their strain fields overlap and the second layer ‘sees’ only one QD. The lateral (inplane) ordering of the QDs with respect to each other occurs in square or hexagonal patterns and is mediated via strain interaction through the substrate. The interaction energy is fairly small, leading only to shortrange inplane order [1166] as shown in Fig. 14.30. The inplane ordering can be improved up to the point that regular one or twodimensional arrays form or individual quantum dots are placed on designated positions using directed selfassembly [1133]. Among others, dislocation networks buried under the growth surface of the nanostructure, surface patterning and modification have been used to direct the QD positioning.
482
14 Nanostructures
Fig. 14.29 Experimentally observed pairing probability in MBEgrown stacks of InAs/GaAs quantum dots as a function of the spacerlayer thickness. Data are taken from (a) (110) and (b) (1–10) crosssectional TEM images. The filled circles are fit to data from theory of correlated island formation under strain fields. Reprinted with permission from [1172], ©1995 APS
IonBeam Erosion During the erosion of a surface with lowenergy ion beam sputtering ordered patterns of dots appear [1173–1176]. Isotropic [1177] and hexagonal [1173, 1175] (Fig. 14.31) nearrange ordering has been observed. The pattern formation mechanism is based on the morphologydependent sputter yield and further mechanisms of mass redistribution [1178]. Also linear patterns have been reported [1179].
14.3.4 Optical Properties The optical properties of QDs are related to their electronic density of states. In particular, optical transitions are allowed only at discrete energies due to the zerodimensional density of states. Photoluminescence from a single QD is shown in Fig. 14.32. The δlike sharp transition is strictly true only in the limit of small carrier numbers (1 exciton per dot on average) since otherwise manybody effects come into play that can encompass recombination from charged excitons or multiexcitons. At very low excitation
14.3 Quantum Dots
483
Fig. 14.30 Lateral ordering of QD array. (d) Planview TEM of QD array on which the statistical evaluation is based. (a) Twodimensional histogram of QDs as a function of the nearestneighbor distance and direction, (b,c) projections of part (a). Solid lines in (b) and (c) are theory for square array with σ = 20 % deviation from ideal position. Adapted from [1133] and [1166]
(a)
(b)
Fig. 14.31 (a) AFM image of a Si (001) substrate after 960 min of ion sputtering (1.2 keV Ar+ , normal incidence). (b) Twodimensional autocorrelation function from a 400 × 400 nm2 area of image in part (a). Adapted from [1175]
density the recombination spectrum consists only of the oneexciton (X) line. With increasing excitation density small satellites on either side of the Xline develop that are attributed to charged excitons (trions) X+ and X− . On the lowenergy side, the biexciton (XX) appears. Eventually, the excited states are populated and
484
14 Nanostructures
Fig. 14.32 Optical emission spectra (T = 2.3 K) of a single InGaAs/GaAs quantum dot at different laser excitation levels P as labeled. The single exciton (X) and biexciton (XX) lines are indicated. Adapted from [1180]
a multitude of states contribute with rich fine structure. In bulk material the biexciton (Sect. 9.6.10) is typically a bound state, i.e. its recombination energy E XX is lower than that of the exciton E X . A similar situation is present in Fig. 14.32. It was pointed out in [1181] that in QDs the biexciton recombination energy can also be larger than the exciton recombination energy. In [1182] the modification of the QD confinement potential of InAs/GaAs QDs by annealing was reported. The exciton binding energy (E X E XX ) is tuned from positive (‘normal’) to negative values upon annealing (Fig. 14.33). The charging state of the exciton can be controlled in a fieldeffect structure. The recombination energy is modified due to Coulomb and exchange effects with the additional carriers. In chargetunable quantum dots [1183] and rings [1184] exciton emission has been observed in dependence of the number of additional electrons. The electron population can be controlled in a Schottkydiodelike structure through
14.3 Quantum Dots
485
Fig. 14.33 Biexciton binding energy determined for a single InAs/GaAs quantum dot for various annealing times. Data from [1182]
Fig. 14.34 Luminescence of charged excitons from a single quantum ring at T = 4.2 K versus the bias voltage with which the number of electrons in the quantum dot N is tuned from zero to N > 3. Adapted from [1184], reprinted with permission from Nature, ©2000 Macmillan Magazines Limited
the manipulation of the Fermi level with the bias voltage. At high negative bias all charge carriers tunnel out of the ring and no exciton emission is observed. A variation of the bias then leads to an average population with N = 1, 2, 3, . . . electrons. The recombination of additional laserexcited excitons depends (due to the Coulomb interaction) on the number of the electrons present (Fig. 14.34). The singly negatively charged exciton X− is also called a trion. The interaction of a spin with an exciton in a CdTe quantum dot has been observed in [1185]. If the CdTe quantum dot is pure, a single line arises. If the dot contains a single Mn atom, the exchange interaction of the exciton with the Mn S = 5/2 spin leads to a sixfold splitting of the exciton line (Fig. 14.35). In an external magnetic field a splitting into a total of twelve lines due to Zeeman effect at the Mn spin is observed.
486
14 Nanostructures
Fig. 14.35 Photoluminescence spectrum of a single CdTe/ZnSe quantum dot containing a single Mn atom (T = 5 K)
Fig. 14.36 Ensemble photoluminescence spectrum (T = 293 K, excitation density 500 W/cm2 ) of InAs/GaAs QDs
In a QD ensemble, optical transitions are inhomogeneously broadened due to fluctuations in the QD size and the size dependence of the confinement energies (Fig. 14.36). Interband transitions involving electrons and holes suffer from the variation of the electron and hole energies: ∂ Ee ∂ Eh + δL . (14.17) σ E ∝ ∂L ∂L
14.3 Quantum Dots
487
Fig. 14.37 Luminescence (under UV excitation) from flasks of colloidal CdTe quantum dots with increasing size (from left to right). From [1165]
A typical relative size inhomogeneity of σ L /L of 7 % leads to several tens of meV broadening. Additional to broadening due to different sizes fluctuations of the quantum dot shape can also play a role. The confinement effect leads to an increase of the recombination energy with decreasing quantumdot size. This effect is nicely demonstrated with colloidal quantum dots of different size as shown in Fig. 14.37.
Chapter 15
Polarized Semiconductors
Abstract In this chapter semiconductors with a spontaneous polarization and ferroelectric semiconductors are discussed. Also the effect of piezoelectricity is treated in some detail for zincblende and wurtzite materials.
15.1 Introduction Semiconductors can have an electric polarization. Such polarization can be induced by an external electric field (Fig. 15.1a). This phenomenon, i.e. that the semiconductor is dielectric, has been discussed already in Chap. 9. In this chapter, we discuss pyroelectricity, i.e. a spontaneous polarization without an external field (Fig. 15.1b), ferroelectricity,1 i.e. pyroelectricity with a hysteresis (Fig. 15.1c) and piezoelectricity, i.e. a polarization due to external stress.
15.2 Spontaneous Polarization The reason for a spontaneous polarization Psp (without external electric field) is the static, relative shift of positive and negative charges in the unit cell. For a slab of semiconductor material (thus ignoring depolarization effects present in other geometries), the polarization causes polarization charges located at the upper and lower surfaces (Fig. 15.2a). The polarization vector P points from the negative to the positive charge. The electric field due to the polarization charges has the opposite direction. In the absence of free charges, the Maxwell equation ∇ · D = 0 yields for piecewise constant fields at a planar interface (Fig. 15.2b) (D2 − D1 ) · n12 = 0 where n12 is the surface normal pointing from medium 1 to medium 2. Therefore, the polarization charge σP = 0 ∇ · E is given by 1 Ferromagnetic
semiconductors are discussed in Chap. 16. We note that there exist so called multiferroic materials that possess more than one ferroic property [1186, 1187]. © Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_15
489
490
15 Polarized Semiconductors
P
(a)
P
(b)
P
(c)
Psp
Psp
Psp=0 Eext
Eext
Eext
Fig. 15.1 Schematic representation of the polarization versus external electric field dependence for (a) dielectric, (b) pyroelectric and (c) ferroelectric semiconductors
(b) (a)
P1 P
P
P
n 12
E
P2 P
Fig. 15.2 (a) Surface polarization charges σP on a slab of semiconductor material with polarization. The electric field is given by E = −P/0 . (b) Polarization charge σP at an interface between two semiconductors with different polarization. In the depicted situation σ is negative
σP = −(P2 − P1 ) · n12 .
(15.1)
Polarization charges develop at interfaces where the polarization is discontinuous, e.g. an interface between two semiconductors with different spontaneous polarization. Vacuum (at a surface) represents a special case with P = 0. For cubic zincblende structure semiconductors, Psp is typically fairly small. The anisotropy of the wurtzite structure allows for sizeable effects (Fig. 15.3). The main cause is the nonideality of the cellinternal parameter u (cf. Sect. 3.4.5).
15.3 Ferroelectricity Ferroelectric semiconductors exhibit a spontaneous polarization in the ferroelectric phase and zero spontaneous polarization in the paraelectric phase. As a function of temperature, the ferroelectric material undergoes a phase transition from the hightemperature paraelectric phase into the ferroelectric phase. There can be further phase transitions between different ferroelectric phases that differ in the direction of the polarization. The literature until 1980 is summarized in [1189]. A more recent treatment can be found in [1190,1191]. PbTiO3 has perovskite structure (cf. Sect. 3.4.10). It exhibits a phase transition at TC = 490 ◦ C from the cubic into the (ferroelectric) tetragonal phase as shown in Fig. 15.4a. Mostly the cell symmetry changes, while the cell volume remains almost constant. A more complicated situation arises for BaTiO3 . At 120 ◦ C the transition
15.3 Ferroelectricity
491
0.04
0.02
BP
BP BSb BAs GaP
BSb
BAs
GaP
0
TlP 2HSiC
Psp (C/m 2 )
AlSb 2HSiC
0.02
AlAs
AlP AlAs TlP
0.04
AlP
BN
BN
GaN
InN
GaN
TlN
TlN
ZnO
InN ZnO
0.06
0.08 AlN
AlN
0.10
0.20 0.25
0.30
0.35
0.40
0.45
0.50
0.373
0.375
0.377
0.379
0.381
0.383
u
Fig. 15.3 Spontaneous polarization Psp for various semiconductors as a function of the lattice constant a (left) and the cellinternal parameter u (right). Based on [1188]
(a) 0.415 0.410
tetragonal
cubic PbTiO3
c
0.405
(b) 20 PS (102 C/m2)
0.400
(a c) 0.395
0.390
a=b
BaTiO3
15
10
5
Tc
0.385
0 200
150
100
50
0
50
100
150
T (°C)
Fig. 15.4 (a) Cell parameters of PbTiO3 as a function of temperature. Adapted from [1194]. (b) Phase transitions of BaTiO3 as a function of temperature. The spontaneous polarization PS points along 100, 110 and 111 in the tetragonal (C4v ), orthorhombic (C2v ) and trigonal (C3v , rhombohedral) phase, respectively. Adapted from [1195]
into the ferroelectric phase occurs (Fig. 15.4b) that is tetragonal with the polarization in the [100] direction. At −5 ◦ C and −90 ◦ C transitions occur into an orthorhombic and a rhombohedral (trigonal) phase, respectively. The largest polarization is caused by a displacement of the negatively (O) and positively (Ba, Ti) charged ions of the
492
15 Polarized Semiconductors 2
Ba
(a)
(b)
2
O
2
O
Ti
4
Fig. 15.5 (a) Crystal structure of BaTiO3 (see Fig. 3.26). (b) Schematic tetragonal deformation below the Curie temperature, generating a dipole moment
unit cell by δ ≈ 0.02 nm (Fig. 15.5). Such an origin of the spontaneous polarization is called a displacement transition.2
15.3.1 Materials A large class of ferroelectric semiconductors are of the type ABO3 , where A stands for a cation with larger ionic radius and B for an anion with smaller ionic radius. Many ferroelectrics have perovskite (CaTiO3 ) structure. They are A2+ B4+ O2− 3 , e.g. , e.g. (Li,Na,K) (Nb,Ta)O . Ferroelectrics can (Ba,Ca,Sr) (Zi,Zr)O3 or A1+ B5+ O2− 3 3 also be alloyed. Alloying in the B component yields, e.g. PbTix Zr1−x O3 also called PZT. PZT is widely used for piezoelectric actuators. Also, alloying in the A component is possible, e.g. Bax Sr1−x TiO3 . Another class of ferroelectrics are AV BVI CVII compounds, such as SbSI, SbSBr, SbSeI, BiSBr. These materials have a width of the forbidden band in the ∼2 eV VI range. A further class of ferroelectric semiconductors are AV 2 B3 compounds, such as Sb2 S3 .
15.3.2 Soft Phonon Mode The finite displacement of the sublattices in the ferroelectric means that the related lattice vibration has no restoring force. The displacement is, however, finite due to higherorder terms (anharmonicity). Thus, for T → TC ωTO → 0. Such a mode
2 The widely accepted model for such ferroelectric is that the basic displacement occurs into the 111direction at low temperature. The three higher symmetry phases at higher temperature are the result of 2 (orthorhombic), 4 (tetragonal) or 8 (cubic) allowed 111 orientations which make the macroscopically averaged polarization appear in 110 or 100direction or vanishing altogether, respectively [1192, 1193].
15.3 Ferroelectricity
(a)
493
SbSI
50
(b)
Ba
SrTiO3 BaTiO3
40 TC
KTaO3
30
TO
(cm1)
Sr TiO3
Ca Sr TiO3
20 CaTiO3
10 0 0
100
200
300
1000/(T
C
Fig. 15.6 (a) Decrease of the transverse phonon mode of SbSI close to the Curie temperature of TC = 288 K. The dashed curved line represents a T − TC 1/2 dependence. Adapted from [1196]. (b) Dielectric constant of various perovskites versus 1/(T − TC ) in the paraelectric phase (T > TC ). Adapted from [1197]
is called a soft phonon mode. The decrease of the phonon frequency is shown in Fig. 15.6a for SbSI. From the LST relation (5.49), it follows that the static dielectric function must increase strongly. The increase is ∝ (T − TC )−1 (Fig. 15.6b).
15.3.3 Phase Transition In the case of ferroelectrics, the order parameter for the Ginzburg–Landau theory of phase transitions is the spontaneous polarization P. The free energy F of the ferroelectric crystal is written in terms of the free energy of the paraelectric phase F0 and is expanded in powers of P (here up to P 6 ) as F = F0 +
1 1 1 α P 2 + β P 4 + γ P 6. 2 4 6
(15.2)
In this equation, we have neglected effects due to charge carriers, an external electric field or external stresses and we assume homogeneous polarization. In order to obtain a phase transition, it has to be assumed that α has a zero at a certain temperature TC and we assume (expanding only to the linear term) α = α0 (T − TC ).
(15.3)
SecondOrder Phase Transition For modeling a secondorder phase transition, we set γ = 0. Thus, the free energy has the form (Fig. 15.7a) F = F0 +
1 1 α P 2 + β P 4. 2 4
(15.4)
494
15 Polarized Semiconductors
(a)
(b) 60 50
PS (102 C/m2)
>0 Free energy
LiTaO3
=0
0 (α < 0) corresponds to the paraelectric (ferroelectric) phase. (b) Spontaneous polarization of LiTaO3 as a function of temperature exhibiting a secondorder phase transition. The dashed line is theory with suitable parameters. Adapted from [1198]
The equilibrium condition with regard to the free energy yields a minimum for ∂F = α P + β P3 = 0 ∂P ∂2 F = α + 3 β P2 > 0 . ∂ P2
(15.5a) (15.5b)
Equation (15.5a) yields two solutions. P = 0 corresponds to the paraelectric phase. P 2 = −α/β is the spontaneous polarization in the ferroelectric phase. The condition from (15.5b) yields that α > 0 in the paraelectric phase, while α < 0 in the ferroelectric phase. Also, β > 0 below the Curie temperature (β is assumed to be temperature independent in the following). Using (15.3), the polarization is given as (Fig. 15.7b) α0 (15.6) (T − TC ) . P2 = β Therefore, the entropy S = − ∂∂TF and the discontinuity ΔCp of the heat capacity ∂S Cp = T ∂T at the Curie point TC are given by p S = S0 + ΔCp =
α02 (T − TC ) β
α02 TC , β
(15.7a) (15.7b)
with S0 = − ∂∂TF0 being the entropy of the paraelectric phase. This behavior is in accordance with a secondorder phase transition with vanishing latent heat (continuous entropy) and a discontinuity of the heat capacity. The dielectric function in
15.3 Ferroelectricity
495
(a)
2
15
PS (10 C/m )
20
2
(b) 25
10 5
BaTiO3 0 20
30
40
50
60
70
80
90
100 110
Fig. 15.8 (a) Schematic plot of the free energy versus spontaneous polarization for a firstorder phase transition. The lowest curve is for α = 0, the others are for α > 0. (b) Spontaneous polarization in BaTiO3 as a function of temperature exhibiting a firstorder phase transition. The dashed line is a guide to the eye. Adapted from [1199]
the paraelectric phase is ∝ 1/α and in the ferroelectric phase ∝ −1/α. The latter relation is usually written as the Curie–Weiss law =
C . T − TC
(15.8)
FirstOrder Phase Transition When the P 6 term is included in (15.2) (γ = 0), a firstorder phase transition is modeled. However, in order to obtain something new, compared to the previous consideration, now β < 0 (and γ > 0) is necessary. The dependence of the free energy on P is schematically shown in Fig. 15.8a for various values of α. The condition ∂F = 0 yields ∂P α P + β P 3 + γ P 5 = 0, (15.9) with the solutions P = 0 and β P =− 2γ 2
1+
4αγ 1− 2 β
.
(15.10)
For a certain value of α, i.e. at a certain temperature T = T1 , the free energy is zero for P = 0 and also for another value P = P0 (second curve from the top in Fig. 15.8a). From the condition 1 1 1 α(T1 ) P02 + β P04 + γ P06 = 0, 2 4 6
(15.11)
496
15 Polarized Semiconductors
the values for P0 and α at the transition temperature T = T1 are given by 3 β 4 γ 3 β2 α(T1 ) = > 0. 16 γ P02 = −
(15.12a) (15.12b)
The schematic dependence of P at the phase transition temperature T1 is depicted in Fig. 15.8b. For T ≤ T1 the absolute minimum of the free energy is reached for finite polarization P > P0 . However, between F(P = 0) and the minimum of the free energy an energy barrier (second lowest curve in Fig. 15.8) is present for T close to T1 . The energy barrier disappears at the Curie–Weiss temperature T0 . At the phase transition temperature, the entropy has a discontinuity ΔS = α0 P02 ,
(15.13)
that corresponds to a latent heat ΔQ = T ΔS. Another property of the firstorder phase transition is the occurrence of hysteresis in the temperature interval between T1 and T0 1 β2 ΔT ≈ T1 − T0 = , (15.14) 4α0 γ in which an energy barrier is present to hinder the phase transition. For decreasing temperature, the system tends to remain in the paraelectric phase. For increasing temperature, the system tends to remain in the ferroelectric phase. Such behavior is observed for BaTiO3 , as shown in Fig. 15.4b.
15.3.4 Domains Similar to ferromagnets, ferroelectrics form domains with different polarization directions in order to minimize the total energy by minimizing the field energy outside the crystal. The polarization can have different orientations, 6 directions for P along < 100 > (tetragonal phase), 12 directions for P along < 110 > (orthorhombic phase) and 8 directions for P along < 111 > (rhombohedral phase). In Fig. 15.9, such domains are visualized for BaTiO3 . Due to the restricted geometry, domain formation in thin films is different from that in bulk material. Domains can also be artificially created by socalled poling. The ferroelectric semiconductor is heated to the paraelectric phase. With electrodes, appropriate electric fields are applied and the material is cooled. The polarization is then frozen in the ferroelectric phase. The domains of a periodically poled structure in LiNbO3 (PPLN) are shown in Fig. 15.10b. The nonlinear optical properties in such structures can be used for efficient second harmonic generation (SHG).
15.3 Ferroelectricity
497
Fig. 15.9 Ferroelectric domains in a BaTiO3 single crystal visualized by birefringence contrast. Reprinted with permission from [1200], © 1949 APS
(b)
(a)
PPLN
Fig. 15.10 (a) Scheme of PPLN (perodically poled lithium niobate), arrows denote the direction of spontaneous polarization. (b) Polarization microscopy image (vertical stripes are domains, horizontal dark lines are scratches)
15.3.5 Optical Properties The firstorder phase transition of BaTiO3 manifests itself also in a discontinuity of the band gap (Fig. 15.11). The coefficient ∂ E g /∂T for the temperature dependence of the band gap is also different in the para and ferroelectric phases.
498
15 Polarized Semiconductors
Fig. 15.11 Temperature dependence of the band gap in BaTiO3 (for polarized light with E ⊥ c). Experimental data from [1201]
15.4 Piezoelectricity 15.4.1 Piezoelectric Effect External stress causes atoms in the unit cell to shift with respect to each other. In certain directions, such a shift can lead to a polarization. Generally, all ferroelectric materials are piezoelectric. However, there are piezoelectric materials that are not ferroelectric, e.g. quartz, GaAs and GaN. Piezoelectricity can occur only when no center of inversion is present. Thus, e.g., GaAs is piezoelectric along < 111 >, but Si is not. Also, the cubic perovskite structure (in the paraelectric phase) is not piezoelectric. Generally, the piezoelectric polarization is related to the strains via the tensor eijk of the piezoelectric modules3 Pi = eijk jk .
(15.15)
15.4.2 Zincblende Crystals In zincblende semiconductors, the polarization (with respect to x = [100], y = [010], z = [001]) is due to shear strains only and is given as ⎛
⎞ yz Ppe = 2 e14 ⎝ x z ⎠ . x y
3 Another
formulation is used with parameters dijk and Pi = dijk σjk .
(15.16)
15.4 Piezoelectricity
499
Table 15.1 Piezoelectric coefficients (in C m−2 ) for various zincblende and wurtzite semiconductors Zincblende Wurtzite II–VI e14 e33 e31 e15 III–V e14 InSb InAs GaSb GaAs AlSb
−0.123 −0.078 −0.218 −0.277 −0.118
CdTe ZnSe ZnS ZnO GaN
0.054 0.049 0.254 0.69 0.375
CdSe CdS ZnS ZnO GaN AlN BeO
0.347 0.385 0.265 0.89 0.73 1.46 0.02
−0.16 −0.262 −0.238 −0.51 −0.49 −0.60 −0.02
−0.138 −0.183 −0.118 −0.45 −0.3 −0.48
Data from [690,1202,1205], for zbZnO from [1206], for zbGaN from [1207]
The values of e14 for various zincblende compound semiconductors are listed in Table 15.1. We note that the sign of e14 reverses from negative in cubic III–V to positive in cubic II–VI semiconductors. This nontrivial behavior involves strain effects on ionic and electronic polarization and ionicity as discussed in [163,1202]. The coefficient e33 , the equivalent to e14 in wurtzite semiconductors (see below), is positive for III–V and IIVI semiconductors. The strain in pseudomorphic heterostructures (cf. Sect. 5.3.3) can cause piezoelectric polarization in a piezoelectric semiconductor. In zincblende, the main effect is expected when the growth direction is along [111] and the strain has a purely shear character. In this case, the polarization is in the [111] direction, i.e. perpendicular to the interface (P⊥ ). For the [001] growth direction, no piezoelectric polarization is expected. For the [110] growth direction, the polarization is found to be parallel to the interface (P ). The situation is shown for various orientations of the growth direction in Fig. 15.12.
15.4.3 Wurtzite Crystals In wurtzite crystals, the piezoelectric polarization (with respect to x = [2–1.0], y = [01.0], z = [00.1]) is given by4 ⎛
⎞ 2 e15 x z ⎠. 2 e15 yz Ppe = ⎝ e31 (x x + yy ) + e33 zz
4 In
Voigt notation, Px = e15 e5 , Py = e15 e4 .
(15.17)
500
15 Polarized Semiconductors
Fig. 15.12 Threedimensional view of the (a) total, (b) longitudinal and (c) transverse polarization in uniaxially compressed GaAs. Adapted from [1203]. (d) Transverse polarization P (parallel to the interface) and (e) longitudinal electric field E ⊥ (perpendicular to the interface) in the InGaAs layer of a GaAs/In0.2 Ga0.8 As superlattice with joint inplane lattice constant (obtained from energy minimization, 1.4 % lattice mismatch, the InGaAs is under compressive and the GaAs under tensile strain). The layer thicknesses of the GaAs and InGaAs layers are identical. The quantities are shown for various orientations of the growth direction. The vector of the growth direction varies in the (01–1) plane (φ = π/4) with polar angle θ reaching from [100] (0◦ ) over [111] to [011] (90◦ ). Image (f) depicts the transverse polarization P (P⊥ = 0 in this geometry) for growth directions in the (001) plane (φ = 0). Parts (d, e, f) reprinted with permission from [1204], © 1988 AIP
15.4 Piezoelectricity
501
Fig. 15.13 Piezoelectric polarization Ppe in GaN (Gaface) versus inplane strain = (a − a0 )/a0 for biaxial, uniaxial and hydrostatic strain. The value of the spontaneous polarization Psp is indicated by an arrow. From [1209]
10
GaN Gaface
0
Px
biaxial
1
10
2
Psp
Ppe (C/m )
Py
Pz
uniaxial
2
10
Pz
3
10
Px Py
hydrostatic 4
10 0.10
0.08
0.06 0.04 0.02
0

Values for the piezoelectric coefficients of several wurtzite semiconductors5 are listed in Table 15.1. The polarization (along c) for biaxial strain in heteroepitaxy (5.73) on the [00.1] surface is C13 e33 , (15.18) Ppe = 2 e31 − C33 where = (a − a0 )/a0 is the inplane strain. The dependence of the magnitude for GaN on the inplane strain is shown in Fig. 15.13 together with the polarization for uniaxial stress along [00.1] and hydrostatic strain. In the latter two cases, the polarization is smaller. The difference of spontaneous polarization of the constituent materials in heterostructures and piezoelectric effects in strained quantum wells lead to quantum confined Stark effect (QCSE, Sect. 13.1.2). The spatial separation of electrons and holes leads to a larger radiative lifetime (Fig. 12.42) and thus reduced radiative recombination rate in the presence of nonradiative channels, an effect unwanted in light emitting diodes. In particular nitride based LEDs grown along the cdirection are ¯ prone to this effect. Therefore growth on nonpolar surfaces such as (1100) (mplane) ¯ (aplane) has been investigated [1210,1211]. However, crystal quality and (1120) for these growth planes seems limited. ¯ or (1122) ¯ [1212], with at An alternative route are ‘semipolar’ planes, e.g. (101¯ 1) ¯ least reduced polarization effects. The (1122)plane is tilted about 58◦ (for GaN) from the caxis, close to the theoretically predicted zero of the internal electric field for InGaN/GaN quantum wells [1213] (Fig. 15.14). Promising experimental results have ¯ been published on semipolar growth, especially for InGaN/GaN on (1122)oriented GaN substrates [1214].
5 If e 14
for a zincblende material is transformed to a coordinate√system along [111], the wurtzitelike √ piezoelectric constants are e33 = 2 e14 / 3 and e31 = −e14 / 3 [1208].
502
15 Polarized Semiconductors
(a)
(b)
Fig. 15.14 (a) Internal electric field and (b) transition probability for electronhole pairs in pseudomorphic Inx Ga1−x N/GaN quantum well (L w = 3 nm) for three different indium contents x as labeled. θ denotes the angle between the caxis and the normal of the interface plane (see inset). Based on [1213]
Fig. 15.15 (a) Electric field and (b) additional confinement potential for electrons due to piezoelectric charges for a strained In0.2 Ga0.8 As/GaAs quantum wire. Adapted from [1203]. (c) Piezoelectric charge density in a (111)oriented GaAs wire with hexagonal cross section. Adapted from [1215]
15.4 Piezoelectricity
(a)
charges
503
(b) (c)
42
42
(d)
25
21
Fig. 15.16 (a) Piezoelectric charges and (b)–(d) resulting Coulomb potential for InAs/GaAs quantum dot with base length b = 12 nm. (a) Isosurfaces corresponding to volume charges ±0.3 e nm−3 . (b) Isosurfaces for the Coulomb potential at ±30 meV. (c, d) Cross section through the Coulomb potential somewhat above the wetting layer in two different magnifications, (d) is a zoom into (c). The InAs/GaAs interface is visible in (d) due to the image charge effect. Parts (a) and (b) reprinted with permission from [367], © 1995 APS
15.4.4 Piezoelectric Effects in Nanostructures The strain distribution around zincblende strained quantum wires [1203], (111)oriented wires under torsion [1215] and epitaxial (embedded) quantum dots [367] contains shear components and thus generates piezoelectric fields. In Fig. 15.15a, b, the electric field and potential due to the piezoelectric charges are shown for a strained In0.2 Ga0.8 As/GaAs quantum wire. In Fig. 15.15c the threefold symmetric piezoelectric charge density within the crosssection of a (111)oriented GaAs wire under torsion (due to second order piezoelectricity) is depicted. In Fig. 15.16, the piezoelectric charges and potential are shown for the quantum dot from Fig. 5.27. The piezoelectric potential has quadrupole character and thus reduces the symmetry of the QD (to C2v ) [367].6 Piezoelectric effects are particularly important in wurtzite nanostructures [1216].
6 The
strain distribution has C2v symmetry for a squarebased pyramid for zincblende materials. The energy levels and wavefunctions are more strongly impacted by the piezoelectric effects than by the strain asymmetry [1156, 1157].
Chapter 16
Magnetic Semiconductors
Abstract Materials and properties of two types of semiconductors with spontaneous magnetization or ferromagnetic and paramagnetic properties are explained: Compound materials and diluted magnetic semiconductors. A short introduction to semiconductor spintronics covers the concepts of spin transistor and spin LED.
16.1 Introduction Magnetic semiconductors exhibit spontaneous magnetic order. Even ferromagnetism, important for spin polarization, as needed in spinelectronics (also called spintronics), can occur below the Curie temperature that is characteristic of the material. Magnetic semiconductors can be binary compounds such as EuTe (antiferromagnetic) or EuS (ferromagnetic). Another class of magnetic semiconductors contains paramagnetic ions in doping concentration (typically < 1021 cm−1 ) or alloy concentration x (typically x ≥ 0.1%). Such materials are termed diluted magnetic semiconductors (DMS). The incorporation of the magnetic atoms leads first to conventional alloy effects, such as the modification of the lattice constant, the carrier concentration or the band gap. The status of the field up to the mid1980s can be found in [1217, 1218], mostly focused on II–VI DMS. A review of work on III–V based materials for spintronics, mostly GaAs:Mn, can be found in [1219]. A 2003 review of wide band gap ferromagnetic semiconductors is given in [1220], a 2014 review of Mncontaining DMS in [1221].
16.2 Magnetic Semiconductors In a magnetic semiconductor, one sublattice is populated with paramagnetic ions. The first two ferromagnetic semiconductors discovered were CrBr3 [1222] in 1960 and EuO [1223] one year later. Europium monoxide has an ionic Eu2+ O2− character, such that the electronic configuration of europium is [Xe]4f7 5d0 6s0 and that of oxygen is 1s2 2s2 2p6 . Some properties of europium chalcogenides [1224] are summarized in Table 16.1. © Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_16
505
506
16 Magnetic Semiconductors
Table 16.1 Material properties of Eu chalcogenides Material E g (eV) Magnetic order EuO EuS EuSe
1.12 1.65 1.8
EuTe
2.00
FM FM AF FM AF
TC , TN (K) 69.3 16.6 4.6 2.8 9.6
‘FM’ (‘AF’) denotes ferromagnetic (antiferromagnetic) order. TC (TN ) denotes the Curie (Néel) temperature. Data collected in [1226]
EuO can be modeled as a Heisenberg ferromagnet with dominant nearest and nextnearest Eu–Eu interactions [1225]. The Heisenberg exchange parameters J1 and J2 for these four compounds are shown in Fig. 16.1. In the nearestneighbor interaction J1 a 4f electron is excited to the 5d band, experiences an exchange interaction with the 4f spin on a nearest neighbor and returns to the initial state. This mechanism generally leads to ferromagnetic exchange. The nextnearestneighbor interaction J2 is weakly ferromagnetic (EuO) or antiferromagnetic (EuS, EuSe, EuTe). In the superexchange process, electrons are transferred from the anionic p states to the 5d states of the Eu2+ cations, resulting in an antiferromagnetic coupling. Fig. 16.1 Heisenberg nearest (J1 , squares) and nextnearest (J2 , circles) exchange parameters (in units of J1,2 /kB ) for the Eu chalcogenides versus the Eu–anion distance. Dashed lines are guides to the eye. Experimental data from [1226]
16.3 Diluted Magnetic Semiconductors
507
16.3 Diluted Magnetic Semiconductors In Table 16.2, the transition metals and their electron configurations are summarized. The 3d transition metals are typically used for magnetic impurities in DMS due to their partially filled 3d shell. Due to Hund’s rule, the spins on the 3d shell are filled in parallel for the first five electrons up to half filling (in order to allow the electrons to get out of their way in real space). Thus, the atoms have a sizeable spin and a magnetic moment. The spin of Mn is S = 5/2. Most transition metals have a 4s2 configuration that makes them isovalent in II–VI compounds. We note that Zn has a complete 3d shell and thus no net spin. In Fig. 16.2, an overview of the crystallographic properties is given for Mnalloyed II–(Se, S, Te, O) based DMS [1227] (DMS with Se, S, and Te have been discussed in [1228]). As an example, the properties of Hg1−x Mnx Te are discussed. This alloy is semiconducting (positive band gap 0 ) for x > 0.075 and a zerogap material (negative interaction gap 0 ) for smaller Mn concentration (cf. Fig. 6.40). The transitions between the Γ6 and Γ8 bands can be determined with magnetoabsorption spectra in the infrared [1229]. In Fig. 16.3a, the magnetic field dependence of transition
Table 16.2 3d, 4d and 5d transition metals and their electron configurations Sc21 Ti22 V23 Cr 24 Mn25 Fe26 Co27 Ni28 2 3 5 5 6 7 3d 3d 3d 3d 3d 3d 3d 3d8 2 2 2 2 2 2 4s 4s 4s 4s 4s 4s 4s 4s2 Y39 Zr 40 Nb41 Mo42 Tc43 Ru44 Rh45 Pd46 4d 4d2 4d4 4d5 4d6 4d7 4d8 4d10 5s2 5s2 5s 5s 5s 5s 5s – La57 Hf 72 Ta73 W74 Re75 Os76 Ir 77 Pt 78 2 3 4 5 6 7 5d 5d 5d 5d 5d 5d 5d 5d9 2 2 2 2 2 2 2 6s 6s 6s 6s 6s 6s 6s 6s Note that Hf72 has an incompletely filled 4fshell with 4f14 Fig. 16.2 Diagrammatic VI overview of AII 1−x Mnx B alloys and their crystal structures. The bold lines indicate ranges of the molar fraction x for which homogeneous crystal phases form. ‘Hex’ and ‘Cub’ indicate wurtzite and zincblende, respectively. From [1227]
Cu29 3d10 4s Ag47 4d10 5s Au79 5d10 6s
Zn30 3d10 4s2 Cd48 4d10 5s2 Hg80 5d10 6s2
508
16 Magnetic Semiconductors
(b)
300
Hg1xMnxTe 200
(a)
(meV)
100
0
0
Hg1xMnxTe x=0.004
370 350
100
330 310
200
290 300
0
270
0
1
2
3
4
5
0
0.05
0.1
0.15
x Fig. 16.3 (a) Energies of Γ6 → Γ8 transitions versus magnetic field for Hg0.996 Mn0.004 Te at T = 2 K. Symbols are experimental values for two polarization directions as indicated. Numbers denote quantum numbers of transitions. Solid lines are theoretical fits. (b) Interaction gap versus Mn concentration for Hg1−x Mnx Te at T = 4.2 K. Various symbols represent data from different authors and methods. Dashed line is a guide to the eye. Adapted from [1229]
energies between different Landau levels is shown that can be extrapolated to yield the interaction gap. The interaction gap is shown in Fig. 16.3b as a function of the Mn concentration. For small Mn concentrations, the DMS behaves like a paramagnetic material. For larger concentrations, the Mn atoms have increasing probability to be directly neighbored by another Mn atom and suffer superexchange interaction (cf. (3.23b)). At a certain critical concentration xc , the cluster size becomes comparable with the size of the sample. If interaction up to the first, second or third neighbor are taken into account for a fcc lattice, the critical concentrations are given by xc = 0.195, 0.136, and 0.061, respectively [1230]. The nearestneighbor interaction between Mn atoms in such DMS as (Zn,Cd,Hg)Mn(S,Se,Te) was found to be antiferromagnetic,1 i.e. neighboring spins are aligned antiparallel. Due to frustration of antiferromagnetic longrange order on a fcc lattice, an antiferromagnetic spin glass forms. The transition temperature TC between the paramagnetic and spinglass phases of Hg1−x Mnx Te is shown in Fig. 16.4. In III–V compounds, the 3d transition metals represent an acceptor if incorporated on the site of the groupIII element as, e.g., in the much investigated compound Ga1−x Mnx As. This material will be used in the following to discuss some prop1 Such
superexchange leads to antiferromagnetic interaction if the bond angle is ‘close’ to 180◦ .
16.3 Diluted Magnetic Semiconductors Fig. 16.4 Magnetic phase diagram of Hg1−x Mnx Te, ‘P’ (‘SG’) denotes the paramagnetic (spin glass) phase. Various symbols represent data from different authors and methods. Dashed line is a guide to the eye. Adapted from [1229]
509 25
Hg1xMnxTe
TC (K)
20 15
P
10
SG 5 0
0.1
0.2
0.3
0.4
0.5
x
erties of magnetic semiconductors. It seems currently well understood and has a fairly high Curie temperature of TC ≈ 160 K. Ferromagnetism in a diluted magnetic semiconductor is believed to be caused by indirect exchange through itinerant charge carriers. The ferromagnetic coupling can be invoked by the Ruderman–Kittel– Kasuya–Yoshida (RKKY) interaction, i.e. the spins of the paramagnetic ions are aligned via interaction with the free carriers in the semiconductor. A related concept is the double exchange2 [1231–1233] in which carriers move in a narrow Mnderived dband (for dwave character see Fig. 7.16c). Such a mechanism was first invoked for PbSnMnTe [1234]. Later, ferromagnetism was discovered in InMnAs [1235] and GaMnAs [1236]. In (In,Ga)MnAs a Mn ion (spin up) spin polarizes the surrounding hole gas (spin down), which has been supplied from the Mn acceptors. This mechanism lowers the energy of the coupled system. The interaction H = −β N0 x S s
(16.1)
between the Mn dshell electrons (S = 5/2) and the plike free holes (s = 1/2) is facilitated by p–d hybridization of the Mn states. N0 denotes the concentration of cation sites in the A1−x Mnx B alloys. The coupling via electrons is much weaker (coupling coefficient α). The holes interact with the next Mn ion and polarize it (spin up), thus leading to ferromagnetic order. The ferromagnetic properties are evident from the hysteresis shown in Fig. 16.6a. Without the carrier gas such interaction is not present and the material is only paramagnetic. Theoretical results for the Curie temperature of various ptype semiconductors are shown in Fig. 16.5. Generally, the quest for higher Curie temperatures (well above room temperature) is underway and wide band gap materials such as GaN or ZnO doped with transition metals have shown some encouraging results. Mnsubstituted chalcopyrite semiconductors are analyzed theoretically in [1237] and are predicted to exhibit lessstable ferromagnetism than III–V semiconductors of comparable band gap. 2 This
model is also called the Zener model.
510
16 Magnetic Semiconductors
Fig. 16.5 Computed values of the Curie temperature TC for various ptype semiconductors plotted versus the band gap (dashed lines are guides to the eye). All materials contain 5 % Mn on the cation sublattice and a hole concentration of p = 3.5 × 1020 cm−3 . Values for TC taken from [1233]
The carrier density and thus magnetic properties in a DMS can be controlled in a spacecharge region (cf. Sect. 21.2.2) as demonstrated in [1238]. In Fig. 16.6, results are shown for hydrogen (deuterium) passivated GaMnAs that exhibits ferromagnetism as ‘asgrown’ thin film. The deuterium is incorporated in similar concentration as the Mn, assumes a backbond position (forming a H–As–Mn complex) and compensates the hole gas from the Mn (cf. Sect. 7.8). The lowtemperature conductivity drops nine orders of magnitude [1239]. Such material displays only paramagnetic behavior. An optimal Mn concentration for ferromagnetic Ga1−x Mnx As is around x = 0.05. For smaller Mn concentrations, the hole density is too small and the Curie
Fig. 16.6 Magnetization M versus magnetic field H for Ga0.963 Mn0.037 As at low temperature. (a) Comparison of asgrown (full squares) and deuterated (open circles) thin film with magnetic field in the layer plane at T = 20 K. (b) Magnetization of the deuterated sample at T = 2 K for larger magnetic fields. Solid line is Brillouin function for g = 2 and S = 5/2. Adapted from [1239]
16.3 Diluted Magnetic Semiconductors Fig. 16.7 Magnetization M versus magnetic field H for Zn0.935 Mn0.065 O thin film at T = 10 and 300 K. A hysteresis is obvious for both temperatures
511 0.08 Zn
Mn
10K
O
0.04 300K
0 0.04 0.08 7
3.5
0
3.5
7
temperature drops; for larger Mn concentrations, the structural properties of the alloy degrade (phase separation into GaAs and MnAs).3 Magnetic hysteresis has been found in nearly compensated Mndoped ZnO [1240, 1241] (Fig. 16.7). Such material is interesting due to its small spinorbit coupling. The exchange mechanism is under debate.
16.4 Spintronics Spintronics (as opposed to electronics) is an emerging field that uses the electron spin rather than its charge for transport, processing and storage of information. Prototype devices are the spin transistor and the spin LED. A crucial point is spin injection, i.e. the creation of (highly) spinpolarized currents. It remains to be seen whether spintronics can be developed to its theoretically envisioned potential and will play a commercially important role in the course of microelectronics. The spin degree of freedom also promises potential for quantum information processing due to its weak coupling to charge and phonons and the resulting long dephasing time. It shall be mentioned here that the magnetization alters also the ‘classical’ transport properties of the semiconductor. The Hall effect is modified strongly and reflects the magnetic hysteresis, also termed anomalous Hall effect (AHE).4 This effect was already discovered by Hall in 1881 for Ni and Co [1242]; a review of the AHE can be found in [1243]. Also the optical excitation of spinpolarized carriers in nonmagnetic materials causes AHE [1244].
3 MnAs is a ferromagnetic metal. MnAs clusters can be a problem since they create ferromagnetic properties but not in the way the DMS is supposed to work. 4 This use of the term ‘anomalous’ should be distinguished from the historical use of ‘anomalous’ Hall effect for the sign reversal of the Hall voltage for hole conductors.
512
16 Magnetic Semiconductors
source
gate
drain
Fig. 16.8 Scheme of spin transistor after the proposal of [1247]. Source and drain are ferromagnets with their magnetization shown schematically as arrows. The channel under the gate transports electrons whose spin rotates in the electric field under the gate
16.4.1 Spin Transistor In this device (for regular transistors cf. Chap. 24), spinpolarized electrons are injected from contact 1, transported through a channel and detected in contact 2. During the transport, the spin rotates (optimally by π) such that the electrons cannot enter contact 2 that has the same magnetization as contact 1 (Fig. 16.8). The spin rotation is caused by spinorbit interaction due to the electric field under the gate contact. This effect is called the Rashba effect and is purely relativistic [1245]. As channel material, a semiconductor with strong spinorbit coupling such as InAs or (In,Ga)Sb is preferable. However, the use of narrowgap semiconductors and the increase of spin scattering at elevated temperatures [1246] make the realization of such a transistor at room temperature difficult.
16.4.2 Spin LED In a spin LED (for LEDs see Sect. 23.3), the injection of spinpolarized carriers into the active layer leads to circularly polarized luminescence. The spin alignment can be achieved with semimagnetic semiconductors grown on top of the active layer or via spin injection from a ferromagnetic metal into the semiconductor (for metal–semiconductor junctions cf. Sect. 21.2). In Fig. 16.9a, a Fe/AlGaAs interface is shown. Ideally, the spinpolarized electrons from the ferromagnetic metal tunnel into the semiconductor and transfer to the recombination region. Subsequently, the emission is circularly polarized (Fig. 12.29b). The degree of circular polarization is Pσ =
Iσ+ − Iσ− , Iσ+ + Iσ−
(16.2)
with Iσ± being the intensity of the respective polarization. The degree of polarization depends on the magnetization of the metal. For the saturation magnetization of Fe, the maximum polarization is about 30 % at T = 4.5 K (Fig. 16.9b) [1248]. The interface
16.4 Spintronics
513 M Fe
(b)
(a)
Fe
Fe/ AlGaAs/ GaAs
AlGaAs (110)
[001]
Fig. 16.9 (a) Transmission electron microscopy image of the (110) cross section of the Fe/AlGaAs interface of a spin LED. The vertical lines in Fe are the (110) planes with 0.203 nm distance. (b) Magneticfield dependence of the circular polarization ratio Pσ at T = 4.5 K (16.2) (filled and empty circles) and the outofplane component of the Fefilm magnetization (dashed line, scaled to the maximum of Pσ ). Reproduced from [1249] by permission of the MRS Bulletin
and its structural nonideality of the interface presumably prevent the spin injection from being 100 % efficient [1249].
Chapter 17
Organic Semiconductors
Abstract An introduction to organic semiconductors, based on the sp2 bonding scheme is given, covering small organic molecules and polymers. Their electronic structure, doping schemes, as well as their particular transport and optical properties are covered.
17.1 Introduction Organic semiconductors are based on carbon compounds. The main structural difference from inorganic semiconductors is the bond based on sp2 hybridization (cf. Sect. 2.2.3) as present in benzene (and graphite). Diamond, although consisting of 100 % carbon, is not considered an organic semiconductor. We note that carbon can form further interesting structures based on sp2 bonds, such as carbon nanotubes (Sect. 18.2), (single or few layer) graphene sheets (Sect. 18.1) rolled up to form cylinders, or fullerenes, e.g. soccerballlike molecules such as C60 . In the 1980 Handbook on Semiconductors only a good ten pages were devoted to organic semiconductors [1250]. Now several textbooks are available [1251, 1252] for a much more detailed treatment than given here.
17.2 Materials 17.2.1 Small Organic Molecules, Polymers The prototype organic molecule is the benzene molecule with its ringlike structure (Fig. 2.8). There is a large number of organic, semiconducting molecules that differs by the number of benzene rings (Fig. 17.1), the substitution of carbon atoms by nitrogen or sulfur (Fig. 17.2a, b), the polymerization (Fig. 17.2c) or the substitution of hydrogen atoms by side groups (Fig. 17.2d). Since PPV is insoluble, typically derivatives
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_17
515
516
17 Organic Semiconductors
Fig. 17.1 Various organic compounds: 1: naphtalene, 2: anthracene, 3: tetracene, 4: pentacene, 5: pyrene, 6: perylene, 7: chrysene, 8: pyranthrene, 9: isoviolanthrene, 10: anthanthrene, 11: coronene, 12: ovalene, 13: violanthrene, 14: pterphenyl, 15: rubrene, 16: mdinaphthanthrene, 17: anthanthrone, 18: mdinaphthanthrone, 19: violanthrone, 20: pyranthrone, 21: isoviolanthrone
such as MEHPPV1 [1254] that are soluble in organic solvents are used. Compared to benzene, the substitution of one carbon atom by nitrogen (pyridine) represents doping with one electron. In Fig. 17.3, the most important building blocks of organic molecules are shown.
17.2.2 Organic Semiconductor Crystals Small organic molecules can crystallize into solids, socalled organic molecular crystals (OMC), due to vanderWaals interaction. In Fig. 17.4a, the monoclinic unit cell of an anthracene crystal [1255] is shown as an example. Also tetracene and 1 2ethoxy,5(2’ethylhexyloxy)1,4phenylene
vinylene.
17.2 Materials
517
(a)
(b)
(c)
(d)
(e)
(f) N
O
O
O
N
N
Al
Fig. 17.2 Organic compounds: (a) thiophene, (b) pyridine, (c) poly(pphenyl), (d) poly(pphenylvinyl), (e) Alq3 (tris(8hydroxyquinolate)aluminum) and (f) a threedimensional view of the Alq3 molecule. Part (f) reprinted with permission from [1253], © 1998 AIP Fig. 17.3 Building blocks of organic molecules, ‘R’=alkyl group, i.e. CH3 (methyl), CH3 CH2 (buthyl), . . .
R
RHC
H
alkane
CHR
alkene
O
R RC
CR
OH
carboxylic acid
O
alkyne
ester R
OR
aromatic
O
amide R
OH
alcohol
R
OR
ether
R
NHR O
O
R
ketone R
Cl R
acid chloride
NH 2
amine
NH
imine
N
nitrile
R O
RHC
aldehyde R
H
RC
518
17 Organic Semiconductors
(a)
(b)
Fig. 17.4 (a) Monoclinic unit cell (for size see Table 17.1) of anthracene crystal. (b) Two herringbone layers of pentacene in a projection onto the bc plane of the triclinic unit cell. Adapted from [1263] Table 17.1 Properties of oligoacene crystals Property Naphtalene Anthracene Melting point (◦ C) Crystal system a (nm) b (nm) c (nm) α (◦ ) β (◦ ) γ (◦ )
Tetracene
Pentacene
80
217
357
>300 ◦ C
Monoclinic 0.824 0.600 0.866 90 122.9 90
Monoclinic 0.856 0.604 1.116 90 124.7 90
Triclinic 0.798 0.614 1.357 101.3 113.2 87.5
Triclinic 0.793 0.614 1.603 101.9 112.6 85.8
Melting point and unit cell parameters. Data from [1256]
pentacene (Fig. 17.4b) have this layered ‘herringbone’ structure. A comparison of the unit cells of oligoacene crystals is given in Table 17.1. Crystal growth of single crystal OMC is achieved with a variety of methods, among them sublimation, Bridgman and Czochralskitype methods [1257, 1258], vapor phase growth [1259, 1260] or from solution [1261, 1262]. Single organic molecular crystals exhibit intrinsic material properties. The practical use of organic semiconductors involves thin films, e.g. in LEDs (OLED, Sect. 23.3.7) and transistors (OFET, Sect. 24.6.3). Thin films of organic molecules are typically disordered and their performance parameters are inferior to that of OMCs.
17.3 Electronic Structure
519
17.3 Electronic Structure The pz orbitals in benzene are partially filled and there is an energy gap between HOMO and LUMO (Fig. 2.11). A similar consideration is valid for polymers. The coupling of orbitals along the polymer chain leads to broadening of the π and π ∗ states into a (filled) valence and an (empty) conduction band, respectively (Fig. 17.5). The HOMO and LUMO positions of various organic semiconductors are shown in Fig. 17.6 relative to the vacuum level (cmp. Fig. 12.21 for inorganic semiconductors). The HOMO is also known as ionization energy (IE), the LUMO as electron affinity (EA). With layered organic semiconductors heterostructures can be built, e.g. to design recombination pathways (recombination layer, electron blocking layers (EBL) and hole blocking layers (HBL)). For electron injection and electron extraction (hole injection) contacts, metals with appropriate work function (in connection with a possible interface dipole layer) have to be used. More details on injection and extraction contacts to organic semiconductors are discussed in Sect. 21.2.7.
Fig. 17.5 Schematic band structure of a polymer originating from the states of the benzene molecule (see Fig. 2.11)
6 pz 18 sp2
Fig. 17.6 Position of HOMO and LUMO for a variety of organic semiconductors (relative to a common vacuum level at E = 0 eV). Based on values from [1264]. On the right hand side the work functions of several metals are shown for comparison
520
17 Organic Semiconductors
17.4 Doping The doping of organic semiconductors can be achieved by • partial oxidation or reduction of the organic molecule, • substitution of atoms in the organic molecule, • mixing of the matrix with ‘dopant’ molecules. The systematic shift of the Fermi level with dopant concentration has been reported in [1265]. Typically, the conductivity increases superlinearly with the doping concentration (Fig. 17.7a), an effect discussed in detail in [1266]. While the mobility remains constant, the thermal activation energy E a for carriers decreases with increasing doping (Fig. 17.7b) due to electrostatic interaction [515, 1267], an effect already discussed in Sect. 7.5.7. The activation energy in the dilute limit E a,0 is modified to (cmp. (7.53)) 1/3 (17.1) E a = E a,0 − β ND .
(a)
(b)
Fig. 17.7 (a) Conductivity (at 0.9 V/µm) versus dopant concentration ND for PPEEB films. Experimental data (circles) and fit (solid line) according to (17.1) with activation energy E a,0 = 0.23 eV and β = 6.5 × 10−8 eV cm (μ = 0.2 cm2 /Vs). Dashed line denotes linear relation between conductivity and ND . Adapted from [1268]. (b) Thermal activation energy E a of carriers (holes) in ZnPc:F4 TCNQ as a function of the molar dopant concentration. Adapted from [1265]
17.5 Transport Properties
521
17.5 Transport Properties Transport in organic semiconductors is characterized by • strong polaronic effects, • hopping conduction, • low mobility, low drift saturation velocity. The interaction of charges with lattice deformations leads to the formation of polarons [1269]. In organic materials these are often ‘small’, i.e. the extension of the deformation is on atomic scale. Such selftrapping of charges reduces their mobility. Two charges can share the same deformation (bipolaron) or oppositely charged polarons can attract (similar to an exciton). If these charges are on the same (neighboring) polymer chain, the polaron is called intrachain (interchain). The conductivity within a molecule, e.g. a long polymer chain, and the conductivity between different molecules have to be distinguished. The conduction between different molecules occurs via hopping. Typically, the conductivity is thermally activated according to Ea , (17.2) σ = σ0 exp − kT where E a is an energy of the order of 1 eV. Such activation also pertains to the mobility alone, e.g. E a = 0.48 eV for PPV [1270]. The maximum lowfield mobility of many crystalline organic semiconductors at room temperature is around 1 cm2 /Vs with a weak temperature dependence [1271]. Such mobility is much smaller than that of crystalline silicon and rather comparable to that of amorphous silicon. Improved purity and handling of organic semiconductors has allowed to achieve intrinsic material properties (Fig. 17.8). The mobility increases
Fig. 17.8 Historic development of the experimentally achieved mobility of organic semiconductors at room temperature
522
17 Organic Semiconductors
Fig. 17.9 Carrier velocity in ultrapure and highly perfect single crystals of (nconducting) perylene at T = 30 K and (pconducting) naphtalene at T = 4.3 K. For comparison electron (hole) velocity in silicon at room temperature is shown as solid (dashed) line. Adapted from [1258]
at low temperatures, e.g. below 100 K in naphtalene [1272]. This has been attributed to the freezeout of phonons and the transition from hopping to band transport. The drift velocity at higher fields shows saturation but the values, even at low temperature, are much smaller than in silicon (Fig. 17.9). An analytical model for the described main features of transport in organic semiconductors has been given in [1273].
17.6 Optical Properties Organic molecules can emit light efficiently and are thus useful for light emitters. For the photophysics of organic materials it is essential to recall the molecular physics of singlet and triplet states. In the singlet (triplet) state, the total spin quantum number of the unpaired electrons is S = 0 (S = 1). A simple energy scheme includes a ground state S0 and excited singlet (S1 ) and triplet (T1 ) states. The recombination transition S1 → S0 is allowed and its lifetime short. Such luminescence is termend ‘fluorescence’. Recombination from the triplet state is forbidden or at least very slow (‘phosphorescence’). As an example for a small organic molecule, the fluorescence lifetime of Alq3 is about 12 ns [1274]. The triplet lifetime is in the 10 µs range [1275]. Luminescence and absorption spectra of Alq3 are shown in Fig. 17.10. The luminescence peak is redshifted with respect to the absorption edge due to the FrankCondon principle (Fig. 10.21). The density of excited (empty) states of the Alq3 molecule is shown in Fig. 17.11 together with the orbitals associated with the four prominent states. The lowest orbital is the LUMO and leads to the visible luminescence of the Alq3 in the red. In Fig. 17.12a, the photoluminescence (PL) and absorption of a polymer, polythiophene are shown. The recombination is below the band gap of 2.1–2.3 eV on an excitonic level at 1.95 eV. There are several phonon replica whose separation of 180 meV corresponds to the C–C stretching mode. The PL excitation (PLE) spectrum
17.6 Optical Properties
523
Fig. 17.10 Luminescence and absorption spectra of Alq3 (vapordeposited 150 nm thin film on a quartz substrate) at room temperature. Adapted from [1276]
(a)
(b)
Fig. 17.11 (a) Projected density of states (for C, N, and O) of excited states in an Alq3 molecule. The origin of the energy axis is the HOMO level. (b) Orbitals for the four states labeled I–IV in (a). Reprinted with permission from [1253], © 1998 AIP
of polythiophene demonstrates that the PL at 1.83 eV can be excited via the exciton level. The theoretical band structure of polythiophene is shown in Fig. 17.13a. The Brillouin zone is onedimensional. The situation I corresponds to a single molecular chain, the situation II pertains to the chain embedded in a medium with a dielectric constant = 3. The predicted band gaps are 3.6 and 2.5 eV, respectively. The exciton binding energy is about 0.5 eV. The exciton is a Frenkel exciton that has a small extension and is localized. The high binding energy is favorable for radiative recombination since the exciton is stable at room temperature. For photovoltaic applications,
524
17 Organic Semiconductors
Fig. 17.12 Photoluminescence (PL) spectra at T = 20 and 300 K and absorption spectrum (green line) of polythiophene. The vertical dashed line denotes the detection energy (E det = 1.83 eV) of the PL excitation (PLE) spectrum (blue circles) (T = 20 K). Adapted from [1277]
Fig. 17.13 (a) Band structure of polythiophene (‘I’: naked chain, ‘II’: chain in a dielectric medium ( = 3)), (b) singleparticle energies and band gap, (c) exciton levels (‘E’: experimental values). Reprinted with permission from [1278], © 2002 APS
it is unfavorable since it has to be overcome in order to separate electrons and holes (after absorption). Generally, intrachain excitons (as here) and interchain excitons, where electron and the hole are localized on different chains, are distinguished.
17.6 Optical Properties
525
Collection of carriers in the ‘dark’ triplet state poses a problem limiting the quantum efficiency to 25 % in a simple model [1279]. Harvesting luminescence from all exciton states would yield significantly higher efficiencies than is possible in purely fluorescent materials (or devices). A successful route is the use of a phosphorescent guest material. Radiative transitions from triplet states become partially allowed when the excited singlet and triplet states are mixed. This is typically achieved in metalorganic molecules with heavy metal atoms, providing large spinorbit interaction effects [1280, 1281]. Most prominently Ru, Pt and Ircontaining compounds are used, e.g. fac tris(2phenylpyridine) iridium [Ir(ppy)3 ] in 4,4’N,N’dicarbazolebiphenyl [CBP] (Fig. 17.14a, b) [1282]. The luminescence spectrum of Ir(ppy)3 is shown in Fig. 17.14d. The radiative decay constant of the Ir(ppy)3 triplet state is about 800 ns and observable if energy transfer from the host triplet state is exotherm (ΔG = G G − G H < 0 [1275], see Fig. 17.15a) and fast. This is the case for CBP:Ir(ppy)3 (Fig. 17.15b), ΔG ≈ −0.2 eV. Actually, reverse transfer from Ir(ppy)3 to CBP seems responsible for some loss in luminescence efficiency and the decrease in phosphorescent lifetime from 800 to 400 ns. In the case of N,N’diphenylN,N’bis(3methylphenyl)[1,1’biphenyl]4,4’diamine
(a)
(b)
(c)
(d)
Fig. 17.14 Molecular structure of (a) Ir(ppy)3 , (b) CBP and (c) TDP (see text). (d) Electroluminescence spectra (at room temperature) of CBP:6 % Ir(ppy)3 , CBP:10 % Ir(ppy)3 /1 %DCM2 and CBP:2 %DCM2. Based on data from [1282, 1283]
526
17 Organic Semiconductors
[TDP] (Fig. 17.14c) host, the triplet energy transfer to the phosphorent Ir(ppy)3 guest is endotherm (ΔG ≈ +0.1 eV) and represents the rate limiting step [1275]. In this case the recombination of Ir(ppy)3 has a decay constant of about 15 µs (Fig. 17.15b). The thermal activation character is confirmed by even longer decay times at low
(a)
(b)
Fig. 17.15 (a) Schematic term diagram of host (TH ) and guest (TG ) triplet states. Straight arrows denote energy transfer between triplet states, wiggly arrows denote radiative transitions to the (singlet) ground state. (b) Electroluminescence transients (at room temperature, detected in the range 500–560 nm [cmp. Fig. 17.14b]) of CBP:6 % Ir(ppy)3 (τ ≈ 1 µs) and TDP:6 % Ir(ppy)3 (τ ≈ 15 µs). Insets: term schemes with arrow denoting the rate limiting step. Based on data from [1275]
(a)
(b)
Fig. 17.16 (a) Schematic term scheme of CBP:Ir(ppy)3 /DCM2 and energy transfer and recombination paths (cmp. spectrum in Fig. 17.14). The rate constants are shown for various processes, the rate limiting step is shown with a bold arrow. (b) Electroluminescence transients after 100 ns excitation pulse (grey area) of Ir(ppy)3 and DCM2 luminescence from CBP:10 % Ir(ppy)3 /1 % DCM2. Based on data from [1283]
17.6 Optical Properties
527
Fig. 17.17 Photoconductivity and absorption spectrum of anthracene
temperatures (τ ≈ 80 µs at T = 200 K) [1275]. Endothermic transfer allows to pump a blue guest phosphor without a blue host material. Further, subsequent Förster energy transfer [1284] from the guest triplet state to a fast and efficient singlet state (SD ) of a fluorescent dye is possible, e.g. from CBP:Ir(ppy)3 to DCM2 [1283]. The transient lifetime of pure DCM2 is about 1 ns. In a mixture of CBP:10 % Ir(ppy)3 /1 % DCM2 the luminescence of DCM2 appears with the same 100 ns decay constant as that of Ir(ppy)3 (Fig. 17.16b). This decay constant (rate limiting step, see Fig. 17.16a) corresponds to the energy transfer depleting the triplet state of Ir(ppy)3 to DCM2 and is much faster than the pure Ir(ppy)3 radiative lifetime. The photoconductivity of organic semiconductors is typically related to their absorption spectrum as shown for anthracene in Fig. 17.17.
Chapter 18
Graphene and Carbon Nanotubes
Abstract The phononic properties and the band structure of graphene and carbon nanotubes of different chirality are given and derived within elementary models. Also inorganic atomic sheets and nanotubes such as BN are briefly discussed.
18.1 Graphene 18.1.1 Structure Graphene is a single sheet of carbon atoms in hexagonal arrangement (Fig. 18.1). The carbon bond length is dC−C = 0.142 nm. It can be prepared from graphite via micromechanical cleavage, i.e. mechanical exfoliation (repeated peeling) of small mesas of highly oriented pyrolytic graphite [1285, 1286]. Graphite is a stacked arrangement of such graphene sheets (Fig. 18.2a) held together by vanderWaals forces as shown in Fig. 18.2b. The carbon atoms bond inplane via sp2 hybridization. Organic molecules such as, e.g., anthracene or coronene (Fig. 17.1) can be understood as molecularsize pieces of such twodimensional graphene sheet with hydrogen saturating the outside, broken bonds. In literature single layer graphene sheets (SLG) and fewlayer graphene (FLG) sheets are distinguished. Ideally such twodimensional crystal is infinitely extended, e.g. for band structure calculations. Real crystals have a boundary (surface) which is topologically a line or very thin sidewall. The mechanical properties of graphene are discussed in [1287]. The phonon dispersion of graphene is shown in Fig. 18.3. For the ZA and ZO modes the displacement is perpendicular to the graphene plane (outof plane modes).
18.1.2 Band Structure A single layer of graphene is a zerogap semiconductor (cf. Fig. 6.40) which shows a linear photonlike spectrum (18.1) E = k c∗ © Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_18
529
530
18 Graphene and Carbon Nanotubes
Fig. 18.1 Schematic atomic arrangement in graphene; the C–C bond length is dC−C = 0.142 nm. Several vectors for making carbon nanotubes (cf. Sect. 18.2) are shown
(a)
(b)
Fig. 18.2 (a) Schematic layer structure of graphite with bond length and layer distance labelled. (b) AFM image of graphene on oxidized silicon. The height of two areas relative to the background is labelled. Adapted from [1288]
around the Fermi energy at the K point (Fig. 18.4a). This point is also called Dirac point. The important bands close to the Fermi level stem from the πorbitals. The linear dispersion around the K point is similar to that of relativistic particles without rest mass. The electrons in graphene are of course not really massless, their velocity (6.31) being v = c∗ ≈ 106 m/s, about 300 times smaller than the speed of light [1290, 1291]. In the simplest tightbinding approximation, the band structure is given as
18.1 Graphene
531
Fig. 18.3 Phonon dispersion in graphene. Symbols are experimental data from various methods. Dashed lines is DFTLDA theory, solid lines GGA. Adapted from [1289]
√ 3a k y a kx a kx E(k) = ±T 1 + 4 cos cos + 4 cos2 , 2 2 2
(18.2)
where a is the lattice constant and T ≈ 3 eV is the nextneighbor hopping energy [1292]. In the meantime more elaborate tightbinding schemes have been reported [1293, 1294] as shown in Fig. 18.4b. The twodimensional band structure is visualized in Fig. 18.4c. Such band structure has been directly confirmed experimentally [1295] as shown in Fig. 18.5a–e. The distortion of the band structure with increasing electron concentration (Fig. 18.5e–h) from the conical bands is due to strong electron–electron, electron–phonon, and electron–plasmon coupling effects [1295]. The band structure of FLG has been theoretically analysed in [1296]. For bilayers experimental data on the band structure can be found in [1297]. Subtle differences exist for different stacking orders of the graphene sheets. Bulk graphite shows a semimetallic behavior with a band overlap of about 41 meV. For more than ten graphene layers the difference with the band overlap in bulk graphite is less than 10 %.
18.1.3 Electrical Properties The Shubnikovde Haas (SdH) oscillations from a graphene sheet exhibit a behavior [1291] 4e 1 1 , (18.3) = ΔB h nS which corresponds to (13.38) for a twodimensional electron system and a spinand valleydegeneracy1 of two. The cyclotron mass has been determined from the
1 Each
of the six valleys at the K points is shared by three Brillouin zones.
532
18 Graphene and Carbon Nanotubes
(a)
(b)
(c)
Fig. 18.4 (a) Band structure of graphene from first principles. (b) Threedimensional representation E(k x , k y ) of the πbands of graphene. (c) Band structure of graphene with only πbands shown, solid lines are abinitio calculation, dashed lines are calculated with tightbinding approximation. Adapted from [1294]
√ temperature dependence of the SdH oscillations to be proportional2 to n (Fig. 18.6). The cyclotron mass is generally related [1298] to the area S(E) = πk 2 in kspace of the orbits at the Fermi energy via mc =
2 ∂ S(E) 2π ∂ E
(18.4)
With the linear dispersion (18.1) we can write (18.4) as mc =
2 In
2 2π E E = 2. 2 2 2π c∗ c∗
a parabolic dispersion as in (13.37), the cyclotron mass is independent of n.
(18.5)
18.1 Graphene
533
(a)
(c)
(b)
(d)
(e)
(f)
(g)
(h)
Fig. 18.5 Experimental bandstructure of graphene (on (0001) 6HSiC) as determined from ARPES. (a) Energy distribution of states as a function of momentum along principal directions in the Brillouin zone. The singleorbital tightbinding model (18.2) with T = 2.82 eV is shown as solid lines. The Fermi level is shifted by 0.435 eV due to doping. (b) Constant energy map of the states at binding energy corresponding to the Dirac energy E D ; the boundary of the Brillouin Zone boundary is superimposed as dashed line. The arrow at the K point indicates the directions over which the data in (e–h) were acquired. (c, d) Constant energy maps at the Fermi energy (E F = E D + 0.45 eV) and E D − 1.5 eV, respectively. (e–h) Experimental energy bands along the line through the K point parallel to Γ –M direction as indicated in (b). The dashed lines are an extrapolation of the lower bands below the Dirac crossing energy, which are observed not to pass through the upper bands (above E D ), suggesting the kinked shape of the bands around E D . The sheet electron density is n S = 1.1, 1.5, 3.7, and 5.6 × 1013 cm−2 for (e)–(h), respectively, due to increased doping upon potassium adsorption. Adapted from [1295]
534
18 Graphene and Carbon Nanotubes
Fig. 18.6 Cyclotron mass in graphene as a function of the sheet electron concentration n S (negative values relate to hole concentration, E F < E D ). Adapted from [1291]
For the linear energy dispersion (18.1) the number of states up to energy E F is (with a degeneracy of 4) N (E F ) = 4
π kF2 4π E F2 = A , (2π/L)2 h 2 c∗2
(18.6)
where A is the system area. Therefore we have (at low temperature) with (18.5) nS =
4π E F2 ∝ m 2c , h 2 c∗2
(18.7)
as determined experimentally. Therefore the behavior of the SdH oscillations confirms the linear dispersion relation. The experimental value for the velocity is c∗ ≈ 106 m/s. From (18.7) the density of states (per area and energy) around the Dirac point increases linearly with energy, D(E) =
8π E. h 2 c∗2
(18.8)
The carrier density in a graphene sheet can be controlled via the field effect. The graphene is positioned on an insulator/semiconductor structure, typically SiO2 /Si (cf. Sect. 21.3). The carrier density is then related to the applied (gate) voltage Vg via (21.89) and (21.91), i.e. i Vg nS = , (18.9) ed where d is the thickness of the insulator and i its dielectric constant. By applying positive (negative) bias electron (holes) can be induced in the sheet. The electron and hole densities depend on the Fermi energies3
3 Here
we assume the linear dispersion for all thermally populated states.
18.1 Graphene
535
Fig. 18.7 Band structure of graphene with various positions of the Fermi energy E F in relation to the Dirac energy E D . States occupied with electrons are shown with in bold
nS = pS =
8π h 2 c∗2 8π h 2 c∗2
∞
ED ED −∞
E − ED dE 1 + exp [(E − E F )/kT ]
(18.10a)
−(E − E D ) dE 1 + exp [−(E − E F )/kT ]
(18.10b)
as visualized in Fig. 18.7. These relations cannot be inverted to obtain E F (n, p) analytically. The total charge carrier density is ρS = e( pS − n S ). The Hall effect (Fig. 18.8) shows the expected ambipolar dependence according to (13.16) which takes the form RH =
1 pS − n S e (n S + pS )2
(18.11)
for equal electron and hole mobilities.4 From Hall effect measurements the mobility has been determined to be about 104 cm2 /Vs, independent of temperature between 10 and 100 K, and the same for electrons and holes. This value, however, is much smaller than the inplane mobility of about 106 cm2 /Vs at 4.2 K in high quality samples of highly ordered pyrolithic graphite (HOPG) [1299]. In suspended graphene a mobility of 2.3 × 105 cm2 /Vs has been found, limited by finite sample size [1300]. Thus in graphene layers on a solid surface extrinsic effects such as charge traps, interfacial phonons, ripples or fabrication residue seem to limit the carrier mobility. The QHE has been observed in graphene [1291], reportedly up at room temperature [1301]. The plateaus (4e2 / h)(n + 1/2) correspond to unusual halfinteger filling, the first plateau occurring at 2e2 / h, as has been also suggested from theory, and related to the ‘pseudospin’. Another consequence of the Diraclike behavior of the fermions in graphene is the presence of finite maximum resistivsign, μh = −μe . For T = 0 and E F = E D , n S = pS = 0 and thus 1/RH should be zero. For finite temperatures there is always n S > 0 and pS > 0, even for E F = E D . Thus 1/RH ∝ 1/( pS − n S ) diverges at ρS = e( pS − n S ) = 0 with a change of sign.
4 Including
536
18 Graphene and Carbon Nanotubes
Fig. 18.8 Hall coefficient (T = 10 K) for a graphene sheet as a function of the free carrier sheet density ρS /e = pS − n S (positive values indicate ptype). Data shown as solid lines from [1291]
ity ρmax = h/4e2 = 6.45 k even at low temperature and E F = E D . It is due to the fact that localization effects, leading to insulating behavior, are strongly suppressed. Then each carrier keeps a mean free path in the order of its Fermi wavelength. The Klein paradox [1302, 1303], the efficient tunneling of Dirac particles through high and thick barriers seems accessible in transport experiments with graphene [1304].
18.1.4 Other TwoDimensional Crystals Twodimensional crystals have been reported also for other materials such as BN, MoS2 , NbSe2 , Bi2 Sr2 CaCu2 Ox [1286] or ZnO [1305]. The phonon spectra of graphene, BN and BC2 Nsheets are compared in Fig. 18.9. The spectrum of BC2 N is similar to the superposition of the C and BN spectra [1306].
18.2 Carbon Nanotubes 18.2.1 Structure A carbon nanotube (CNT) is a part of a graphene sheet rolled up to form a cylinder. They were first described as multiwalled nanotubes by Iijima [1307] in 1991 (Fig. 18.10b) and in their singlewalled form (Fig. 18.10a) in 1993 [1308]. Reviews can be found in [1293, 1309]. The chirality and diameter of a nanotube are uniquely described by the chiral vector (18.12) ch = n 1 a1 + n 2 a2 ≡ (n 1 , n 2 ),
18.2 Carbon Nanotubes
537
(a)
(b)
(c)
Fig. 18.9 (a) Crystal structure of BC2 N. (b) Brillouin zone of BC2 N (rectangle) and C, BN (hexagon). (c) Phonon dispersion of graphene (C) and BN and BC2 Nsheets. Adapted from [1306]
(a)
(b)
Fig. 18.10 (a) TEM image of singlewalled carbon nanotubes (SWNT). (b) TEM images of various multiwalled carbon nanotubes (MWNT). Adapted from [1307]
where a1 and a2 are the unit vectors of the graphene sheet. The chiral vector denotes two crystallographic equivalent sites which are brought together along the circumference of the nanotube. The possible vectors are visualized in Fig. 18.1 for −30◦ ≤ θ ≤ 0◦ . The fiber diameter is given by d=
a 2 ch  = n 1 + n 1 n 2 + n 22 , π π
(18.13)
538
18 Graphene and Carbon Nanotubes
(a)
(b)
(c)
Fig. 18.11 Structure of different types of carbon nanotubes that have similar diameter of 0.8 nm. (a) Armchair (6,6), (b) zigzag (8,0) and (c) chiral symmetry. Adapted from [1309]
Fig. 18.12 A chiral nanotube (chiral vector is (10,5), θ = −19.11◦ ) with hemispherical caps at both ends based on an icosahedral C140 fullerene. The tube diameter is 1.036 nm. Adapted from [1311]
√ with the graphene lattice constant a = 3 dC−C = 0.246 nm. Abinitio calculations show that the diameter becomes a function of the chiral angle below 0.8 nm; deviations from (18.13) are below 2 % for tube diameters d > 0.5 nm [1310]. The (n, 0) tubes (θ = 0) are termed ‘zigzag’ and an example is depicted in Fig. 18.11b. Nanotubes with θ = ± π/6, i.e. of the (n, n) (and (2n, −n)) type, are called ‘armchair’. All others are termed ‘chiral’. The extension along the wire axis is large compared to the diameter. The tip of a nanotube is part of a buckminsterfullerene type molecule (Fig. 18.12). When the nanotube if formed by rolling a single sheet of graphene (SLG), a singlewalled nanotube (SWNT) is formed. A FLG sheet creates a multiwalled nanotube (MWNT). For small number of layers they are called doublewalled, triplewalled and so forth. The mechanical strength of carbon nanotubes is very large. For SWNT Young’s moduli of 103 GPa have been found experimentally [1312] in agreement with theoretical predictions [1313].
18.2.2 Band Structure In carbon nanotubes there is some mixing of the π(2pz ) and σ(2s and 2pz ) carbon orbitals due to the radial curvature. This mixing is, however, small and can
18.2 Carbon Nanotubes
539
(a)
(b)
(c)
(d)
Fig. 18.13 (a) Brillouin zone of the graphene lattice (bold line) and allowed kvalues for a (6,6) armchair nanotube. (b) Band structure of a (6,6) carbon nanotube. Adapted from [1315]. (c) Brillouin zone of the graphene lattice (bold line) and allowed kvalues for a (6,0) zigzag carbon nanotube. In the lower part the real space structure is visualized. (d) Band structure of graphene (left) and a (6,6) nanotube (right). Adapted from [1316]
be neglected near the Fermi level [1314]. The band structure of a nanotube is mainly determined by zonefolding of the graphene band structure. The vector along the (infinitely extended) wire k z is continuous. The vector k⊥ around the nanotube is discrete with the periodic boundary condition ch · g⊥ = 2π m,
(18.14)
where m is an integer. The distance of allowed k⊥ values is (5.5) Δk⊥ =
2π 2 = . πd d
(18.15)
The character of the nanotube band structure depends on how the allowed kvalues lie relative to the graphene Brillouin zone and its band structure. This is visualized in Fig. 18.13. For the case of an armchair tube (n, n), as shown in Fig. 18.13a, the Kpoint of the graphene band structure always lies on an allowed kpoint. Therefore,
540
18 Graphene and Carbon Nanotubes
(a)
(c)
(b)
Fig. 18.14 (a, b) Brillouin zone of the graphene lattice (bold line) and allowed kvalues for a (a) (6,0) and a (b) (8,0) zigzag nanotube. (c) Band structures of a (12,0) metallic and (13,0) semiconducting armchair carbon nanotube. Adapted from [1315]
the nanotube is metallic, i.e. zerogap, as seen in the bandstructure in Fig. 18.13b. The Dirac point is between Γ and X. For a zigzag nanotube, the kspace is shown in Fig. 18.13c for a (6, 0) nanotube. The corresponding band structure for a (6, 0) nanotube is also metallic (Fig. 18.13d) with the Dirac point at the Γ point. In Fig. 18.14c the band structure of another metallic (12, 0) zigzag nanotube is shown. However, only for (3m, 0) the Kpoint is on an allowed state and thus the tube metallic. For the other cases, as shown for the kspace of a (8, 0) nanotube in Fig. 18.14b, this is not the case. The corresponding band structure (Fig. 18.14c for (13, 0)) has a gap and thus the nanotube is a semiconductor. Generally, the condition for a nanotube to be metallic is with an integer m n 1 − n 2 = 3 m.
(18.16)
There are two semiconducting ‘branches’ with ν = (n 1 −n 2 ) mod 3 = ±1. The tubes with ν = +1 have a small band gap, those with ν = −1 have a larger band gap.√ The density of states is a series of onedimensional DOS, proportional to E (6.75). It is compared in Fig. 18.15 for a metallic and a semiconducting nanotube. Within 1 eV from the Fermi energy the DOS can be expressed in an universal term [1317].
18.2 Carbon Nanotubes
541
Fig. 18.15 Density of states for a (9,0) metallic and (10,0) semiconducting zigzag carbon nanotube within the tightbinding approximation (18.2). The energy scale is given in units of the tightbinding parameter T ≈ 3 eV. The dashed lines are the DOS of graphene. Adapted from [1311]
18.2.3 Optical Properties Optical transitions occur with high probability between the vanHove singularities of the DOS. The theoretical absorption spectrum of a (10,0) nanotube is shown in Fig. 18.16. In an ensemble of nanotubes various types and sizes occur. The transition energies of all possible nanotubes sorted by diameter are assembled in the Kataura plot (Fig. 18.17a). Experimental data are shown in Fig. 18.17b. The two branches of semiconducting nanotubes ν = ±1 yield different transition energies. The overall dependence of the transition energy follows a 1/dlaw.
18.2.4 Other Anorganic Nanotubes Structures similar to carbon nanotubes have been reported for BN [1322, 1323]. A boron nitride nanotube is a cylindrically rolled part of a BN sheet. BN tubes are always semiconducting (Fig. 18.18) and have a band gap beyond 5 eV similar to hexagonal BN which is mostly independent on chirality and diameter [1324].
542
18 Graphene and Carbon Nanotubes
Fig. 18.16 Calculated absorption spectra for a (semiconducting) (10,0) carbon nanotube for parallel (solid line) and perpendicular (dotted line) polarization. The thick (thin) lines are calculated with (without) the matrix element included. Adapted from [1318]
(a)
(b)
Fig. 18.17 (a) Theoretical transition energies of semiconducting (filled symbols) and metallic (open symbols) carbon nanotubes as a function of tube diameter (Kataura plot). Energies are calculated from vanHove singularities in the JDOS within the thirdorder tightbinding approximation [1294]. (b) Experimental Kataura plot for the first two semiconducting (S, closed symbols) and the first metallic (M, open symbols) transition. Dashed lines connect the (nearto) armchair tubes; full lines connect tubes in a branch, ν = (n 1 − n 2 ) mod 3. Data from photoluminescence [1319] and resonant Raman scattering [1320]. Adapted from [1321]
Thus, while carbon nanotubes appear black since they absorb within 0–4 eV, BN is transparent (or white if scattering). For high energies larger than 10 eV C and BN tubes are quite similar since they are isoelectronic and the highlying unoccupied states are less sensitive to the difference in the nuclear charges than the states at and below the Fermi energy [1325].
18.2 Carbon Nanotubes
543
Fig. 18.18 Band structure and density of states (DOS) of C(3,3) and BN(3,3) nanotubes, calculated with DFTLDA. Adapted from [1325]
Chapter 19
Dielectric Structures
Abstract Dielectric structures, in particular periodic dielectric structures are treated. A general onedimensional model is developed describing Bragg mirrors. Examples for photonic band gap materials in one, two and three dimensions are given. Different types of dielectric cavities and microscopic resonators including Fabry–Pérot and whispering gallery resonators are treated. Quantum electrodynamic physical effects from light matter coupling such as Purcell effect and strong coupling are treated.
19.1 Photonic Band Gap Materials Layered structures of dielectric materials with different index of refraction are used as optical elements such as filters or reflection and antireflection coatings [1326]. In this section we discuss the use of such concepts in one, two and threedimensional photonic band gap materials.
19.1.1 Introduction A structure with a socalled photonic band gap (PBG) exhibits an energy range (color range) in which photons cannot propagate in any direction. In the photonic band gap, there are no optical modes, no spontaneous emission and no vacuum (zerofield) fluctuations. We recollect that spontaneous emission is not a necessary occurrence: Looking at Fermi’s golden rule (19.18) for the transition probability integrated over all final states 2π (19.1) M2 ρf (E), w(E) = we see that the decay rate depends on the density ρf of final states at energy E. In the case of spontaneous emission, this is the (vacuum) density Dem of electromagnetic
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_19
545
546
19 Dielectric Structures
Fig. 19.1 Right electromagnetic dispersion with a forbidden gap at the wavevector of the periodicity. Left Electronwave dispersion typical of a directgap semiconductor. When the photonic band gap straddles the electronic band gap, electron–hole recombination into photons is inhibited since the photons have no place to go (zero final density of states)
modes (per energy per volume) that varies ∝ ω 2 : Dem (E) =
8π E 2. (hc)3
(19.2)
In a homogeneous optical medium c must be replaced with c/n (cmp. Sect. 10.2.3). If the band gap of a PBG is tuned to the electronic gap of a semiconductor, the spontaneous emission, and also induced emission, can be suppressed. Thus, one mode has to be left by ‘doping’ the structure. In this mode all emission will disappear and an efficient singlemode (monochromatic) LED or ‘zerothreshold’ laser could be built. A schematic comparison of the band structure of electrons and photons is given in Fig. 19.1.
19.1.2 General 1D Scattering Theory The formation of a photonic band gap in a onedimensional dielectric can be calculated to a large extent analytically and thus with direct insight. Let n(x) be the spatially varying index of refraction (no losses or nonlinear optical effects). The onedimensional wave equation (Helmholtz equation) reads for the electric field E ω2 ∂ 2 E(x) 2 + n (x) E(x) = 0. ∂x 2 c2
(19.3)
19.1 Photonic Band Gap Materials
547
A comparison with a onedimensional Schrödinger equation ∂ 2 Ψ (x) 2m − 2 [V (x) − E] Ψ (x) = 0 ∂x 2
(19.4)
shows that the Helmholtz equation corresponds to the quantummechanical wave equation of zero external potential V and a spatially modulated mass, i.e. a case that is usually not considered. Let us consider now the amplitude ak of the k eigenvector. The eigenvalue is then ωk . The onedimensional mode density ρ(ω) (per energy and per unit length) is ρ(ω) =
dk , dω
(19.5)
which is the inverse of the group velocity. We follow onedimensional scattering theory as presented in [1327]. At this point we do not rely on any specific form of n(x) (Fig. 19.2a). The (complex) transmission coefficient t for any index structure is t = x + iy =
√
T exp(iφ),
(19.6)
(a) n 1
t
r
0 d
0
x
(b) n 1
tN ...
rN 0
(c) n
d
2d
3d
0 x
(N1)d Nd
d1 d2
n2
1
n1
rN
tN ...
0
d
2d
3d
0 (N1)d Nd
x
Fig. 19.2 1D scattering problem: (a) General scattering of an index of refraction distribution, (b) N period stack, (c) twolayer (quarterwave) stack
548
19 Dielectric Structures
where tan φ = y/x. φ is the total phase accumulated during propagation through the structure. It can be written as the product of the physical thickness of the structure d and the effective wave number k. Hence we have the dispersion relation d y d tan(kd) = . dω dω x
(19.7)
Evaluating the derivative we find d cos2 (kd)
y x − x y dk , = dω x2
(19.8)
where the prime denotes derivation with respect to ω. Using the relation cos2 θ = (1 + tan2 θ)−1 , we obtain the general expression ρ(ω) =
dk 1 y x − x y . = dω d x 2 + y2
(19.9)
19.1.3 Transmission of an NPeriod Potential Now, the behavior of N periods of a given index distribution n(x) within a thickness d of one period (Fig. 19.2b) is investigated. The scattering matrix M connects +the u intensity at x = 0 with that at x = d. We use the column vector u = u− containing the right and leftgoing waves (labeled ‘+’ and ‘−’, respectively), u ± = f ± exp(±ikx), u(0) = M u(d). (19.10) Using the boundary conditions u(0) = (1, r ) and u(d) = (t, 0), we find that M has the structure 1/t r ∗/t ∗ . (19.11) M= r/t 1/t ∗ The conservation of energy requires that det M = (1− R)/T = 1. The eigenvalue equation for M is (19.12) μ2 − 2μ Re(1/t) + 1 = 0. The two eigenvalues μ± are related by μ+ μ− = det M = 1. If we consider an infinite, periodic structure, we know from Bloch’s theorem that the eigenvector varies between unit cells only via a phase factor, i.e. μ = 1. Therefore, the eigenvalues can be written as (19.13) μ± = exp(±iβ),
19.1 Photonic Band Gap Materials
549
where β corresponds to the Bloch phase of a hypothetical infinite periodic structure. This phase β should not be confused with φ defined earlier, which is associated with the unit cell transmission. We find the condition Re(1/t) = cos β
(19.14)
for the Bloch phase. Since every matrix obeys its own eigenvalue equation, we have also (1 being the unity matrix) M2 − 2 M cos β + 1 = 0.
(19.15)
By induction one can show that the N period case has the scattering matrix MN = M
sin(N β) sin((N − 1)β) −1 . sin β sin β
(19.16)
The solution for the finite period case can be written in terms of the Bloch phase of the infinite potential. The transmission and reflection of the N period system are given by 1 sin(N β) sin((N − 1)β) 1 = − tn t sin β sin β rn r sin(N β) = . tn t sin β
(19.17a) (19.17b)
The transmission of intensity can be written as (T = t ∗ t) 1 sin2 (N β) =1+ TN sin2 β
1 −1 . T
(19.18)
Again, up to this point no specific distribution of the index of refraction within the unit cell has been specified. From (19.17a), a general formula for the mode density ρ N (ω) of the N stack can be obtained as [1327] 1 ρN = Nd
sin(2N β) 2 sin β
η +
ηξξ 1−ξ 2
cos2 (N β) + η 2
where ξ = x/T = cos β and η = y/T .
−
N ηξ 1−ξ 2
sin(N β) sin β
2 ,
(19.19)
550
19 Dielectric Structures
19.1.4 The QuarterWave Stack A quarterwave stack, also known as a Bragg mirror, exhibits a onedimensional photonic band gap. One period consists of two regions with thickness and index of refraction (d1 , n 1 ) and (d2 , n 2 ), respectively (Fig. 19.2c). In the quarterwave stack each region has an optical thickness of λ/4 (the wave accumulates in each region a phase of π/2) for a particular wavelength λ0 or (midgap) frequency ω0 . Thus, the condition reads λ0 π c . (19.20) = n 1 d1 = n 2 d2 = 4 2 ω0 Using the Fresnel formulas, the transmission of an arbitrary twolayer cell is t=
T12 exp(i( p + q)) , 1 + R12 exp(2iq)
(19.21)
where p = n 1 d1 ω/c and q = n 2 d2 ω/c are the phases accumulated in the two layers, respectively. The values of T12 and R12 are given as 4 n1 n2 (n 1 + n 2 )2 (n 1 − n 2 )2 = . (n 1 + n 2 )2
T12 =
(19.22a)
R12
(19.22b)
For the quarterwave stack ( p = q = π/2), we obtain for (19.21) t=
T12 exp(iπ ω) ˜ , 1 + R12 exp(iπ ω) ˜
(19.23)
where ω˜ = ω/ω0 is the frequency scaled to the midgap value. The transmission of a single twolayer cell is T =
1 − 2 R12
2 T12 , 2 cos(π ω) ˜ + R12
(19.24)
and the Bloch phase is given by cos(π ω) ˜ − R12 T12 sin(π ω) ˜ . η= T12
cos β = ξ =
(19.25a) (19.25b)
19.1 Photonic Band Gap Materials
551
(a)
(b)
Fig. 19.3 Quarterwave stack with indices of refraction (a) n 1 , n 2 = 1.0, 1.5 and (b) 1.0, 3.0. Solid lines dimensionless density of modes ρ N (19.19), dashed lines transmission TN (19.26) for two different numbers of pairs N = 5 (left panels) and 10 (right panels) versus the dimensionless frequency ω˜
For the N period quarterwave stack the transmission is given by TN =
1 + cos β . 1 + cos β + 2 (R12 /T12 ) sin2 (N β)
(19.26)
A band gap forms. Within the band gap, the density of modes is lowered, at the edges it is enhanced (Figs. 19.3 and 19.4). The transmission at midgap decreases 2N , where n i < n j . ∝ n i /n j In the limit of large N the complete width Δω˜ of the band gap is implicitly given by cos
n1 − n2 2 . Δω˜ = 1 − 2 2 n1 + n2
π
(19.27)
If n 1 − n 2  n 1 + n 2 , we find Δω˜ ≈
4 n 1 − n 2  . π n1 + n2
(19.28)
552
(a)
19 Dielectric Structures
(b)
Fig. 19.4 Quarterwave stack with indices of refraction n 1 , n 2 = 1.0, 1.5: (a) Transmission TN at midgap (ω˜ = 1, down triangles) and at the band edge (ω˜ = 1 − Δω/2, ˜ up triangles) versus number of pairs N . (b) Dimensionless density of modes ρ N at maximum near the band edge and at midgap versus number of pairs N
The principle of the quarterwave stack is scalable to frequencies other than visible light.1 In Fig. 19.5 the reflectance of various quarterwave stacks from yttriastabilized zirconia (YSZ [1328], high index material, Fig. 19.6a) and Al2 O3 are shown [1329]. The different design wavelengths have been achieved solely by varying the layer thicknesses. In Fig. 19.6b the three Bragg mirrors from Fig. 19.5 with N = 15.5 pairs are replotted in relative frequency units ω. ˜ The spectra look very similar; subtle differences in the width of the reflectance band are due to slightly larger index contrast at higher design energy (cmp. Fig. 19.6a). The width of the gap is approximately Δω˜ ≈ 0.18 in agreement with (19.28). As further example, a Mo/Si Bragg mirror with a period of 6.7 nm is shown in Fig. 19.7. Such a mirror works in the extreme UV and is used for soft Xray optics, possibly in advanced lithography systems. Dielectric thin films can also be designed for antireflection coatings, edge filters or pass and stop band filters as detailed in [1326].
19.1.5 Formation of a 3D Band Structure For other applications, e.g. waveguides with minimized footprint, 3D (or at least 2D) photonic band gap structures are needed. Details can be found in dedicated textbooks [1332–1334]. In [1335] planar, cylindrical and spherical Bragg mirrors are discussed.
1 This
is a general property of Maxwell’s equations which do not contain a specific length scale.
19.1 Photonic Band Gap Materials
553
Fig. 19.5 Reflectance of various Bragg mirrors from YSZ/Al2 O3 grown by pulsed laser deposition on sapphire. The different layer thicknesses result in the design energies 0.43 eV (N = 10.5, Rmax = 0.9812, red), 1.19 eV (N = 10.5, Rmax = 0.9779, orange), 2.11 eV (N = 15.5, Rmax = 0.99953, green), 3.39 eV (N = 15.5, Rmax = 0.99946, blue) and 4.54 eV (N = 15.5, Rmax = 0.99989, purple)
(a)
(b)
Fig. 19.6 (a) Index of refraction of YSZ and Al2 O3 as a function of photon energy. (b) Reflectance spectra of the 2.11 eV, 3.39 eV and 4.54 eV Bragg mirrors of Fig. 19.5 replotted as a function of the scaled frequency ω˜ = ω/ω0
Since we want a photonic band gap that is present for all directions of propagation, a Brillouin zone with a shape close to a sphere is preferable. Then, the main directions are at similar kvalues (Fig. 19.8). One of the best suited is the fcc lattice. Since the L point is centered at ≈14 % lower frequency than the X point, the forbidden gaps for different directions must be, however, sufficiently wide to create a forbidden frequency band overlapping at all points along the surface of the Brillouin zone. For example, the bcc lattice has a Brillouin zone that is less symmetric than that of the fcc lattice (see Fig. 3.34) and thus is less suited for the creation of an omnidirectional
554
(a)
19 Dielectric Structures
(b)
50nm
Mo Si
Si
Fig. 19.7 (a) Crosssectional TEM of Mo/Si superlattice with 2.7 nm Mo and 4.0 nm Si (period: 6.7 nm) on Si(001) substrate. From [1330]. (b) Reflection spectrum for a SL with period of 6.5 nm and 88.5◦ angle of incidence. Data points are shown as circles, the solid line is a fit with a period of 6.45 nm. Adapted from [1331]
kz
(a)
(b)
X W L
X
U X kx
ky
L
K
k L
X
Fig. 19.8 (a) The Brillouin zone of the fcc lattice. (b) Schematic forbidden gaps at the L and X points
photonic band gap. However, the photonic band gap must not arise above the first band, relaxing problems due to asymmetry of the Brillouin zone (cf. Table 19.1). Maxwell’s equations (zero charge density) for monochromatic waves ∝ exp(iωt) ∇ ·D = 0
μω H ∇ ×E = i c ω ∇ ×H = i D c ∇(μH) = 0 ,
(19.29a) (19.29b) (19.29c) (19.29d)
19.1 Photonic Band Gap Materials
555
Fig. 19.9 (a) Calculated photonic band gap structure of a fcc dielectric structure composed of air spheres in a dielectric background of refractive index n = 3.5. The filling ratio is 86 % air and 14 % dielectric material. Dotted and solid lines represent coupling to s and ppolarized light, respectively. Reprinted with permission from [1336], ©1990 APS. (b) Density of states for the band structure of part (a)
Fig. 19.10 (a) Calculated photonic band structure for a diamond dielectric structure consisting of overlapping air spheres in a dielectric material with n = 3.6. Filling ratio of air is 81 %. The frequency is given in units of c/a, a being the cubic lattice constant of the diamond lattice and c being the velocity of light. (b) Gaptomidgap frequency ratio for the diamond structure as a function of filling ratio for dielectric spheres n = 3.6 in air (solid circles) and air spheres in dielectric n. Optimal case: air spheres with 82 % filling ratio. Reprinted with permission from [1336], ©1990 APS
together with D(r) = (r)E(r) and μ = 1 they are combined into the wave equation ω2 ∇ × −1 (r) ∇ × H(r) + 2 H(r) = 0. c
(19.30)
This equation is numerically solved for planar waves with wavevector k. In the following, results are shown for various structures. In a fcc lattice of air spheres in a dielectric medium with n = 3.6 (a typical semiconductor), no band gap can be achieved (Fig. 19.9a), only a pseudogap (Fig. 19.9b) appears. In a diamond lattice (two fcc lattices shifted by 1/4 111), a complete photonic band gap is possible [1336] (Fig. 19.10). Recently, a periodic array of spirals (Fig. 19.11) has been predicted to exhibit a large photonic band gap [1337]. Glancingangle deposition [1338] (GLAD) is a way to realize such structures. Another method
556
19 Dielectric Structures
Fig. 19.11 (a) Tetragonal squarespiral photonic crystal. The crystal shown here has a solid filling fraction of 30 %. For clarity, spirals at the corners of the crystal are highlighted with a different shade and height. The tetragonal lattice is characterized by lattice constants a and b. The geometry of the square spiral is illustrated in the insets and is characterized by its width, L, cylinder radius, r , and pitch, c. The top left inset shows a single spiral coiling around four unit cells. (b) Band structure for the direct structure crystal characterized by [L, C, r ]=[1.6, 1.2, 0.14] and a spiral filling factor f spiral = 30 %. The lengths are given in units of a, the lattice constant. The width of the PBG is 15.2 % relative to the center frequency for background dielectric constant b = 1 and spiral dielectric constant s = 11.9. The positions of highsymmetry points are illustrated in the inset. Reprinted with permission from [1337], ©2001 AAAS. (c) Oblique and edge views of a tetragonal square spiral structure grown using the GLAD (glancingangle deposition) process. Reprinted with permission from [1338], ©2002 ACS
to fabricate structures with arbitrary geometry within a material is twophoton lithography or twophoton holography. Another path to PBG structures are socalled inverted opals. First, a closepacked structure of spheres, e.g. monodisperse silica spheres, is fabricated by sedimentation or selfassembly. The gaps are filled with a highindex medium and the template is subsequently removed, e.g. by etching or dissolving. The resulting structure is shown in Fig. 19.12a. Such a structure has a photonic band gap (Fig. 19.12b) if the refractive index is sufficiently high (>2.85) [1339].
19.1 Photonic Band Gap Materials
557
(b) (a) (i)
(ii)
(iii) (iv) (v)
(c)
Fig. 19.12 (a) Cartoon showing, in five steps, the fabrication of an inverse diamond structure with a full photonic band gap. First, (i) a mixed bodycentered cubic lattice is assembled (ii) after which the latex sublattice is removed; (iii) then the structure is sintered to a filling fraction of ∼50 % after that (iv) silicon or germanium infiltration takes place and finally (v) silica elimination. (b) Photonic band diagrams of (upper panel) a silicon/silica composite diamond opal and (lower panel) made of air spheres in silicon resulting from the removal of the silica spheres from the former. The filling fraction for silicon is 50 %. The inset shows the corresponding real space structures. Reprinted with permission from [1347], ©2001 AIP. (c) SEM images of internal facets of silicon inverse opal: (i) (110) facet, (ii) (111) facet. Adapted from [1348], reprinted with permission from Nature, ©2000 Macmillan Magazines Limited
The band gap in this case is between the 4th and 5th band. Table 19.1 offers a compilation of various PBG structures and their properties.
558
19 Dielectric Structures
Table 19.1 Various photonic band gap structures and some of their properties Name Crystal type n Δω˜ (%) Reference Diamond Yablonovite Woodpile Spirals Squarespirals Layered 3D Inverted scaffold Inverse opal Inverse hcp
Diamond fcc fc tetragonal sc Tetragonal bc orthorhombic sc fcc hcp
2 2 2 4 4 4 5 8 16
29 19 20 17 24 23 7 4.25 2.8
[1336] [1340] [1341] [1342] [1337] [1343] [1344] [1345] [1346]
The band gap is between the nth and (n + 1)th band, Δω˜ is given for air/silicon ( ≈ 12)
19.1.6 Disorder A real photonic band gap structure deviates from the ideal, perfectly periodic system by slight variations of the position and possibly also the size of the dielectric ‘atoms’. This is schematically shown in Fig. 19.13a. The difference between the real and ideal structure is a (bipolar) spatial distribution of Δ (r) which acts as a source of scattering and hence exponential attenuation of coherent beams propagating through photonic crystals over lengths l, named the ‘(extinction) mean free path’. After propagating over such distance l, a light beam is converted to a diffuse glow that corrupts the functionality of any photonic integrated circuit. Experimentally for opals a mean free path consistent with 5 % fabrication accuracy has been found (Fig. 19.13b). For such disorder and a lattice constant a ≈ λ, the mean free path is about only 10 wavelengths, l ≈ 10λ.
19.1.7 Defect Modes Similar to a perfect periodic atomic arrangement leading to the formation of the electronic band structure, a perfectly periodic dielectric structure leads to the photonic band structure. As we know from semiconductor physics, much of the interesting physics and numerous applications lie in defect modes, i.e. localized electronic states due to doping and recombination at such centers. The equivalent in PBG structures are point defects (one unit missing) or line defects (a line of units, straight, bend or with sharp angles, missing). Such defects create localized states, i.e. regions for light localization. In the case of line defects we deal with waveguides that can be conveniently designed and could help to reduce the size of photonic and optoelectronic integrated circuits.
19.1 Photonic Band Gap Materials
559
(a)
(b)
Fig. 19.13 (a) Schematic photonic band gap structure with perfect (upper left) and disordered (upper right) periodicity. In the lower left panel the disordered structure is overlayed with the ideal structure (red circles). In the lower right panel, the difference between ideal and disordered structure is shown. (b) Optical mean free path in an opal photonic band gap structure for various lattice constants. Solid line is theory for 5 % fabrication accuracy. Adapted from [1349]
1D Model We revisit our 1D scattering theory and create now a ‘defect’. A simple defect is the change of the width of the center n 2 region in a quarterwave stack. For the numerical example, we choose N = 11, n 1 = 1, n 2 = 2. In Fig. 19.14, the transmission curves are shown for the undisturbed quarterwave stack and the microcavity with n 2 d2center = 2λ0 /4 = λ0 /2. A highly transmissive mode at ω = ω0 arises that is quite sharp with Δω = 3 × 10−4 . Thus, the quality factor Q, also called the Qfactor or finesse, Q=
ω0 , Δω
(19.31)
with ω0 being the resonance frequency and Δω being the linewidth, is 3.3 × 103 in this case. If the thickness is varied (Fig. 19.15), the mode shifts away from the center. A similar scenario arises for higherorder nl /2cavities, e.g. n 2 d2center = 4λ0 /4 = λ0 (Fig. 19.16).
560
(a)
19 Dielectric Structures
(b)
Fig. 19.14 Defect mode in 1D photonic band gap: (a) Transmission of N = 11 quarterwave stack exhibiting a photonic band gap (n 1 = 1, n 2 = 2) (dashed line) and of microcavity (solid line) with center n 2 region of width λ0 /2 (instead of λ0 /4). (b) Relative width of mode is about 3 × 10−4 Fig. 19.15 Transmission of N = 11 quarterwave stack (n 1 = 1, n 2 = 2) with center n 2 region of widths 1.8 λ0 /4 (dashed line) and 2.2 λ0 /4 (solid line)
Fig. 19.16 Transmission of N = 11 quarterwave stack (n 1 = 1, n 2 = 2) with center n 2 regions of widths 3 λ0 /4 (solid line), 3.5 λ0 /4 (dashdotted line) and 4 λ0 /4 (dashed line)
19.1 Photonic Band Gap Materials
561
2D or 3D Defect Modes An example of 2D waveguiding is shown in Fig. 19.17. Point defects can be used for highfinesse wavelength filtering. Emitters surrounded by a photonic band gap material with a defect mode can emit into the defect mode only, leading to spectrally filtered, highly directional emission.
Fig. 19.17 2D photonic band gap waveguide structure. (a) Fabrication principle, (b) SEM image of the structure, (c) light guiding at a 90◦ bend. Reprinted with permission from [1350], ©2000 AIP
562
19 Dielectric Structures
19.1.8 Coupling to an Electronic Resonance In a verticalcavity surfaceemitting laser (cf. Sect. 23.4.14), an optical defect mode in a 1D dielectric structure is coupled to an electronic excitation, such as an exciton in a quantum well or dot. In the simplest picture, the oscillator must emit its radiation into the cavity mode since other modes do not exist in the Bragg band. Thus, the emission energy is given and fixed by the cavity mode. However, the photon mode (field oscillator) and the electronic oscillator form a coupled system that generally must be described using quantum electrodynamics. Energy is periodically exchanged between the two oscillators with the Rabi frequency. An analogous phenomenon is investigated in the field of atom–cavity interactions. A necessary condition for the observation of such an oscillation is that the radiation energy remains long enough in the cavity that can be expressed as [1351, 1352] (cf. (19.37)) α d 1 − R ≈ π/Q,
(19.32)
where α is the absorption coefficient of the electronic transition, d is the length of the absorbing medium, R is the reflectance of the cavity mirror and Q is the finesse of the cavity given in (19.31). This situation is called the strong coupling regime since it leads to anticrossing behavior of the cavity mode and electronic resonance. In the weak coupling regime for small absorption, the resonances cross (within their linewidth). For resonance, the emission intensity of the oscillator into the cavity mode is enhanced and its lifetime is reduced (Purcell effect), which is discussed in Sect. 19.2.2. The transmission T of a Fabry–Perot cavity with two (equal and lossless) mirrors of transmission Tm = 1 − Rm is given by T (ω) =
Tm2 exp (−2 L α(ω)) , 1 − Rm exp (i 2 n ∗ L ω/c)2
(19.33)
√ with the complex index of refraction n ∗ = n r + iκ = and α = 2ωκ/c (cf. (9.9)). For an empty cavity, i.e. a (small) background absorption αB and a background index of refraction n r = n B , the resonances occur when the phase shift 2n B Lω/c is an integer multiple of 2π, i.e. for ωm = m
πc , nB L
(19.34)
with m ≥ 1 being a natural number. In the vicinity of the resonance, i.e. for ω = ωm + δω, we can expand exp (2n B Lω/c) ≈ 1 + i2n B Lδω/c and obtain from (19.33) a Lorentzian for the transmission T (ω) ≈
(Tm /Rm )2 exp (2Lα(ω)) Tm2 exp (−2Lα(ω)) = . (δω)2 + γc2 1 − Rm (1 + i2n B L δω/c)2
(19.35)
19.1 Photonic Band Gap Materials
563
The frequency width (HWHM) γc of the emptycavity resonance is given by γc =
c 1 − R , R 2 nB L
(19.36)
where R = Rm exp (−2Lα). Thus, the decay rate (photon loss from the cavity) is proportional to Tm + αB L if both terms are small. The quality factor of the cavity resonance m is given by ωm mπ Q= ≈ . (19.37) 2 γc 1− R Now, the electronic resonance is put into the cavity leading to a change in the dielectric function to (cf. (D.11))
=
n 2B
f 1+ , 1 − (ω 2 + iωΓ )/ω02
(19.38)
where the index of refraction due to the electronic resonance is given by n(ω) = √ and (D.13a, b). For resonance of the cavity mode and the electronic oscillator, i.e. ωm = ω0 , the solution for the cavity resonance condition 2n r ωL/c = m2π is obtained, using (19.34), from n r (ω) = m
ωm πc = nB . ωL ω
(19.39)
A graphical solution (Fig. 19.18a) yields three intersections of the left and right hands of (19.39). The very high absorption at the central solution (ω = ω0 ) results in very low transmission. The other two solutions2 yield the frequencies of the coupled normal mode peaks. For f 1, we use (D.13a) in (19.39) and find for the splitting ±Ω0 /2 of the two modes (19.40) Ω02 = f ω02 − Γ 2 . This frequency is called the Rabi frequency. If the dielectric function of the oscillator is put into (19.33), the splitting is found to be Ω02 = f ω02 − (Γ − γc )2 .
(19.41)
A splitting will only be observable if Ω0 Γ, γc . If the two resonances ωc and ω0 are detuned by Δ = ωc − ω0 , the splitting Ω of the transmission peaks shows the typical anticrossing behavior of two coupled oscillators Ω 2 = Ω02 + Δ2 .
f > (Γ /ω0 )2 , i.e. in the strong coupling > 0. The absorption coefficient at ω0 must be larger than Γ n ∞ /c.
2 These solutions only occur for sufficient oscillator strength
regime where
Ω02
(19.42)
564
19 Dielectric Structures
(a)
(b)
20 15
GaAs/ AlGaAs
10 5 0 5 10 15 15 10
5
0
5
10
15
20
Fig. 19.18 (a) Graphical representation of (19.39) with the two solutions marked with circles for n ∞ = 1 (dashed line), f = 10−3 , Γ /ω0 = 10−2 and ω0 = ωm . (b) Reflectance peak positions (experimental data (circles) at T = 5 K) versus cavity detuning ωc − ω0 for a cavity with two GaAs/AlGaAs Bragg mirrors (24/33 pairs for the front/bottom mirror) and five embedded quantum wells whose resonances are closely matched. Solid lines are a theoretical fit according to (19.42) with Ω0 = 4.3 meV. The dashed lines show the electronic resonance ω0 and the cavity resonance ωc . Part (b) adapted from [1352]
In the experiment, typically the electronic resonance remains fixed at ω0 and the cavity resonance is detuned by variation of the cavity length across the wafer (Fig. 19.18b). A detailed theory of cavity polaritons is given in [1353]. The nonlinear optics of normal mode coupling in semiconductor microcavities is reviewed in [1354]. The inplane dispersion of the cavity polaritons depends on the coupling strength. First, the photon dispersion is given by 1/2 , E ph (k) = ω = c k = c k2 + k z2
(19.43)
where k is the inplane kvector and k z is given by the resonance condition, k z = ωm /c with (19.34), π . (19.44) kz = m nB L Thus the dispersion relation is no longer linear as for freely propagating light. For small k this leads to an (inplane) effective photon ‘rest mass’, applying (6.34), 1 ∂ 2 E ph 1 = . (19.45) m ∗ph 2 ∂k 2 We find m ∗ph =
kz ω(k = 0) . = c c2
(19.46)
19.1 Photonic Band Gap Materials
565
Fig. 19.19 Dispersion of cavity photon mode and electronic resonance at E el = 3.0 eV (dashed lines) and coupled modes (solid lines) for 2V = 40 meV
Now we assume the electronic oscillator to be in resonance with the photon dispersion at k = 0, i.e. E el = ω(k = 0). The electronic resonance shall have vanishing dispersion for simplicity since the exciton mass is much larger than (19.46). The eigenwert equation of the coupled system, resembling (6.57), is E − E ph V = 0, V E − E el
(19.47)
with two solutions, called the upper and lower cavity polariton branch, visualized in Fig. 19.19. Their splitting at k = 0 is 2V . Thus the coupling parameter V = Ω0 /2 corresponds [1353] to the Rabi frequency (19.40). Experimental values for the splitting of 3–15 meV in InAlGaAs based [1352, 1355–1358], 17–44 meV in CdZnTeSe based [1359], 6–60 meV in (Al,In,Ga)N based [1360–1364] and 78 meV in ZnO based [1365] microcavities were found. It is possible to condensate cavity polaritons in the minimum of the dispersion around k = 0 (Bose–Einstein condensation). In [1366] stimulated scattering and gain from cavity polaritons have been reported. Further details on cavity polaritons can be found in [1367, 1368].
19.2 Microscopic Resonators 19.2.1 Microdiscs A microdisc is a cylindrical resonator with a thickness d that is small compared to the radius R. It can be fabricated from semiconductors and semiconductor heterostructures using patterning and materialselective etching. With underetching a mostly freestanding disc can be made that resides on a post (Fig. 19.20). The coordinate system is (ρ, φ, z) with the z direction being perpendicular to the disc area. Typically, the disc is so thin that there is only one node along z. Solving the
566
19 Dielectric Structures
(a)
(b)
500nm 1µm Fig. 19.20 (a) Side view of a 3µm diameter disc containing one 10nm InGaAs quantum well between 20nm InGaAsP barriers standing on an InP pillar that has been selectively underetched using HCl. (b) Top view SEM image of a 5µm diameter InGaAsP microdisc. The pedestal shape is a rhombus due to anisotropic etching of the HCl. Adapted from [1369], reprinted with permission, ©1992 AIP
(a)
(b) 6
4
5 4 3 2 1 0 0.0
0.05
0.1
Fig. 19.21 (a) Field intensity for whispering gallery mode (10, 0) (TMpolarized) for a circle with 1 µm radius (shown as white line) and n = 1.5. The image size is 4 × 4 µm2 . (b) Theoretical quality factor of a 2µm InP microdisc as a function of the deformation parameter (19.49). The insets show (8,0) whispering gallery modes at a wavelength of 1.55 µm for n = 3.4. Part (b) adapted from [1372]
wave equation in this geometry [1370], the modes are characterized by two numbers (m, l). m describes the number of zeros along the azimuthal direction φ with the field amplitude being proportional to exp(±imφ). Thus, except for m = 0, the modes are simply degenerate. Modes with E z = 0 are called TE modes. This is the preferred polarization of emission. The number l denotes the number of zeros in the radial direction. Only for modes with m = 1, is the intensity nonzero on the axis, i.e. for ρ = 0. All other modes have vanishing intensity in the disc center. The light intensity in whispering gallery modes is preferentially concentrated along the circumference of the disc as shown in Fig. 19.21a. Since the light can only escape via evanescent waves, the light is well ‘captured’ in such a mode.
19.2 Microscopic Resonators
567
(a)
(b)
Fig. 19.22 Strong coupling of a single QD exciton (due to monolayer fluctuation in a 13 ML thick GaAs/Al0.33 Ga0.67 As QW) with a WGM in a microdisk of 2 µm diameter (inset). (a) Anticrossing of upper and lower peak for various temperatures. Symbols are data points, solid lines are theory considering coupling. The dashed (dashdotted line) is the expected temperature shift of the WGM mode (exciton energy). (b) Photoluminescence spectrum at the anticrossing point (T = 30 K). Experimental data (squares) and fit with two peaks (solid line). Adapted from [1373]
The Qfactor (19.31) is extremely high and takes values of several 104 . In order to couple light out of such a disc, deformed resonators, e.g. with a defect in the form of protrusions [1371], were devised. Deformed resonators are discussed in more detail in the next section. The strong coupling of a QD exciton to a whispering gallery mode is shown in Fig. 19.22 where anticrossing behavior is observed at low temperatures. Tuning is achieved by temperature variation. Behavior of a similar system in the weak coupling regime is shown in Fig. 19.24.
19.2.2 Purcell Effect According to Fermi’s golden rule (19.1), the probability of an optical transition depends on the density of available optical modes (final states). If the density of modes is enhanced compared to its vacuum value (19.2) at a resonance of an optical cavity, the lifetime of the electronic state decreases by the Purcell factor [1374] FP =
3 (λ/n)3 Q , 4π 2 V
(19.48)
568
19 Dielectric Structures
(a)
(b) 6 5
3
0
/
4
2 1 0
0
5
10
15
20
25
30
35
P
Fig. 19.23 (a) Micropillar with MBEgrown GaAs/AlAs DBRs and a cavity containing five layers of InAs quantum dots as indicated. The pillar has been prepared by reactive ion etching. Reprinted with permission from [1375], ©1998 APS. (b) Experimental decay time τ of onresonance quantum dot luminescence scaled by offresonance lifetime τ0 = 1.1 ns (close to lifetime in a QD in bulk) for a variety of micropillars with different Purcell factors FP . The error bars correspond to the measurement accuracy of the decay time (±70 ps), the dashed line is a guide to the eye. Adapted from [1375]
where n is the refractive index of the medium, Q is the quality factor of the cavity resonance and V is the effective mode volume.3 Experiments on the emission of quantum dots (that generally provide small absorption and thus allow for the weak coupling regime) in etched micropillars containing a microcavity (Fig. 19.23a) have shown that indeed the luminescence decay is faster for cavities with large Purcell factor (Fig. 19.23b) [1375]. The resonance of cavity mode and emitter leads to an enhanced emission intensity as shown in Fig. 19.24 for the exciton emission of a single quantum dot in a microdisc [1376].
19.2.3 Deformed Resonators The whispering gallery modes in circular (or spherical) cavities are longlived and emission goes into all angles. Light escape is based only on the exponentially slow 3V
is given by the spatial integral of the vacuum field intensity for the cavity mode, divided by its maximum value.
19.2 Microscopic Resonators
569
(a)
(b) QDX WGM
1.322
7 6
1.321
5 4
1.320
3 2
1.319
1 0
10
20
30
40
50
60
0 1.5
1.0
0.5
0.0
0.5
1.0
Fig. 19.24 (a) Temperature dependence of the energy positions of the whispering gallery mode (WGM) of a 5µm diameter AlGaAs/GaAs microdisc (Q = 6500) and the singleexciton resonance of a single InAs quantum dot contained within the disc. (b) Intensity of WGM mode as a function of the detuning E WGM − E QD−X from the QD single exciton resonance. The excitation density was 15 Wcm−2 for all data. Adapted from [1376]
process of evanescent leakage (neglecting disorder effects such as surface roughness). In order to overcome the isotropic light emission, the resonator needs to be deformed. This can be accomplished with an ellipsoidal shape, i.e. r (φ) = R [1 + cos φ] ,
(19.49)
where 1 + 2 is the aspect ratio of the ellipse. The increased radiation leads to a decrease of the Qfactor as shown in Fig. 19.21b. Also, a new decay process, refractive escape, becomes possible. A ray that is initially in a whispering gallery trajectory diffuses in phase space until finally an angle smaller than the critical angle for total reflection (9.11) is reached. The ray dynamics becomes partially chaotic [1377]. One other possible deformation of the circular disc geometry is a ‘flattened quadrupole’ as shown in Fig. 19.25a. This shape can be parameterized by a deformation parameter and the angledependent radius r (φ) given by 1/2 . r (φ) = R 1 + 2 cos2 (2φ)
(19.50)
For small deformation, the whispering gallery modes become chaotic and exhibit preferred emission along the long axis of the resonator (Fig. 19.25b). For larger deformations ( ≥ 0.14), a stronger and qualitatively different directionality occurs in the shape of a bowtie [1378] as shown in Fig. 19.25c. The optical laser power extracted from deformed resonators was found to increase exponentially with ; for = 0.2 it was 50 times larger than for the circular resonator. Another modification that can be applied to the microdisc in order to increase outcoupling of light, is the spiral resonator [1379] as shown in Fig. 19.26a. The radius is parameterized by
570
19 Dielectric Structures
Fig. 19.25 (a) SEM image of a quadrupolar cylinder laser with deformation parameter ≈ 0.16 on a sloped InP pedestal. The light grey area in the top view is the electrical contact. (b) Simulated nearfield intensity pattern of a chaotic whispering gallery mode for = 0.06 and n = 3.3. (c) Simulated nearfield intensity pattern of a bowtie mode for = 0.15. The length of the minor axis for (b) and (c) is 50 µm. Reprinted with permission from [1378], ©1998 AAAS
r (φ) = R 1 + φ . 2π
(19.51)
The experimental emission pattern is displayed in Fig. 19.26b. It exhibits a maximum along the direction of the tangent at the radius step. The simulated nearfield intensity of such an emission mode is shown in Fig. 19.26c. In a spiral laser, ray dynamics is also chaotic [1380].
19.2 Microscopic Resonators
571
Fig. 19.26 (a) SEM image of a microcavity disc laser diode with a disc radius of 50 µm. The pcontact ring electrode defines the areas through which carriers are injected into the microdisc and where stimulated emission can take place. (b) Radial distribution of the light output from the spiralshaped microdisc laser diode measured below and above threshold. The radius of the spiral microdisc was r0 = 250 µm and the deformation parameters were = 0.05 (grey) and = 0.10 (black). An emission beam at an angle of α = 0◦ corresponds to a direction normal to the notch surface as shown in the inset. Below the laser threshold, the emission pattern is essentially isotropic and independent of the deformation parameter. Above the threshold, directional emission is clearly observed with the emission direction at a tilt angle α ≈ 25◦ . The measured divergence angle of the farfield pattern is ∼ 75◦ for = 0.10 and ∼ 60◦ for = 0.05. Reprinted with permission from [1381], ©2004 AIP. (c) Simulated nearfield intensity pattern of an emission mode with nk R ≈ 200 for deformation = 0.10. Reprinted with permission from [1379], ©2003 AIP
19.2.4 Hexagonal Cavities Hexagonal cavities develop, e.g., in microcrystals of wurtzite semiconductors (with the caxis along the longitudinal axis of the pillar). In Fig. 19.27a, a ZnO tapered hexagonal resonator (needle) is shown. Whispering gallery modes modulate the
572
19 Dielectric Structures
Fig. 19.27 (a)–(c) SEM images of ZnO nanoneedle fabricated by pulsed laser deposition. (d) Schematic geometry of crosssectional plane. Ri (R) is the radius of the incircle (circumscribing circle). The circumference of the inscribed white hexagon, representing the path of a whispering gallery mode, has a length of 6Ri . (e) Twodimensional plot of spectra recorded along a linescan along the needle’s longitudinal axis. The left vertical axis shows the linescan position x, the right one refers to the respective needle diameter D. The spectral maxima, i.e. the measured WGM energies, appear as bright belts going from the bottom left corner to the right upper one. With decreasing diameter, all resonances shift systematically to higher energies. The white dots give theoretical TMresonance energy positions obtained from (19.52), white crosses give the same for TEpolarization. Reprinted with permission from [1382], ©2004 APS
intensity of the green ZnO luminescence [1382].4 In a simple planewave model, the resonance condition is given by
hc 6 2 (19.52) N + arctan β 3n − 4 , 6Ri = nE π
4 We
note that besides the green luminescence as in Fig. 10.20, an unstructured green band also occurs that is observed here. Its origin may be linked to the oxygen vacancy [1383].
19.2 Microscopic Resonators
573
Fig. 19.28 Simulated nearfield intensity pattern of modes in a cavity with hexagonal cross section (absolute value of electric field in linear grey scale): Modes (N = 4) with (a) symmetry −a and (b) mode 4+ (nomenclature from [1384]) for n = 2.1 and k R = 3.1553 − i0.0748. Modes (c) 26− and (d) 26+ for n = 1.466 and k R = 22.8725 − i0.1064. The displayed modes have a chiral pattern. Emission originates mostly from the corners. (e) Microphotoluminescence spectra of a single ZnO nanopillar. The three topmost curves are unpolarized. The curve labeled ‘bulk’ shows the unmodulated luminescence of the green luminescence in bulk. The line labeled ‘exp.’ shows the experimental µPL spectrum of the investigated nanopillar. The experimental spectra recorded for TM and TEpolarization, respectively, are shown in the lowest two curves. The curve labeled ‘theory’ displays the theoretical luminescence spectra. Dashed vertical lines are guides to the eye referring to the spectral position of the dominating WGMs. The inset shows a SEM image of the investigated pillar, the scale bar has a length of 500 nm. The dotted lines show the position of the edges of the hexagonal resonator obtained from topography contrast
(a)
(b)
(c)
Fig. 19.29 (a) Photoluminescence spectra of a ZnO microwire with hexagonal cross section for various pump power densities (lowest curve: D = 60 kW/cm2 , top curve: D = 250 kW/cm2 ) at T = 10 K. The inset shows the scanning electron microscopy image of a typical microwire (d = 6.40 µm). (b) Dependence of the emitted PL intensity of a selected lasing peak (denoted by an arrow in the spectrum in part (a)) on the excitation density D. Lines are guide to the eyes. (c) Dependence of the resonant energies on the interference order N for wires with different diameters as labeled on top of the graph. Lines are the predicted theoretical values calculated from (19.52) using diameter values obtained from SEM measurements; the symbols represent the experimentally observed peaks. Adapted from [1385]
574
19 Dielectric Structures
where Ri is the radius of the inner circle (Fig. 19.27d), n is the index of refraction, N is the mode number and β is given by βTM = 1/n (βTE = n) for TM (TE) polarization, respectively. Due to birefringence, n  (n ⊥ ) has to be used as the index of refraction for TM (TE) polarization. A N = 26 whispering gallery mode of a hexagonal resonator is shown in Fig. 19.28c, d. The 6fold symmetric emission stems from the edges of the hexagon. While whispering gallery resonators have typically mode numbers N 1, in such hexagonal resonators the whispering gallery modes could be followed down to N = 1 [1382] as shown in Fig. 19.27a, b, e. Under high optical pumping laser action occurs on the whispering gallery modes. The peak positions, close to the band gap in the spectral region of the electronhole plasma, follow (19.52) [1385], as shown for various diameters in Fig. 19.29. Pumping threshold even at room temperature is below 100 kW/cm2 [1386].
Chapter 20
Transparent Conductive Oxide Semiconductors
Many of the most important semiconductors are oxides. A.H Wilson, 1939 [65]
Abstract Typical materials in the class of transparent conductive oxides are mentioned. Their physical properties and the limits of conductivity versus transparency are discussed.
20.1 Introduction Transparent conductive oxides (TCO) are semiconductors that are simultaneous transparent and highly conductive. Therefore they can serve as transparent contacts, e.g. as a solar cell front contact or in display applications. The materials are typically fabricated in the form of thin films on glass, polymers or similar substrates and devices. The crystallographic structure is polycrystalline or amorphous. The first TCO investigated was CdO in pressed powder [1387] and thin film form [31]. The recent historic development of the resistivity of the most important TCO materials in the last 30 years is shown in Fig. 20.1. Further information on TCO films can be found in [1388–1390].
20.2 Materials Any widegap (E g > 3 eV) semiconductor that is conductive, e.g. due to intrinsic defects or by chemical impurities (doping), can be considered to be a TCO. Practically only a few, nontoxic materials that can be easily deposited are of importance. The first TCO application was heating of air plane windows. As always in semiconductor technology, price drives the suitability for applications. This in particular true for TCO applications since they include large area devices such as solar © Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_20
575
576
20 Transparent Conductive Oxide Semiconductors
Fig. 20.1 Historical development of the resistivity of doped ZnO (circles), In2 O3 (squares) and SnO2 (diamonds) TCO films. Adapted from [1390]
Fig. 20.2 Practical TCO materials
cells, displays and also large glass panes for electromagnetic shielding and architectural heat and IR transparency management. Therefore large quantities of TCO are needed. The popular ITO (indiumtinoxide) suffers from large indium price and potential indium scarcity, opening the field for aluminumdoped ZnO (ZAO) which is abundant. Possible other compounds including Cd are of no practical interest due to toxicity. Conductive GaN has not been considered due to its large processing temperatures. All practical TCO materials contain either Zn, Sn or In (Fig. 20.2). A number of TCO materials is reviewed in [1391]. TCO are mostly nconducting. Also pconducting TCOs have been reported, e.g. CuAlO2 delafossite [1392] with room temperature conductivity of σ = 1 S/cm, ZnIr2 O4 [1393] with σ = 2 S/cm and ZnCo2 O4 spinel [1394] with σ = 20 S/cm. However, there has been so far no report on a practical transparent highly conductive ptype electrode. The term ITO stands for a variety of Sndoped indium oxide (In2 O3 ) materials, the Sn content being typically in the 5–10 % range but not strictly defined. The crystal structure of In2 O3 [1395] is shown in Fig. 20.3. The effect of the replacement of indium by tin atoms in In2 O3 on mechanical, electrical and optical properties of ITO has been calculated in [1396] using DFT. In Fig. 20.4 the band structures of pure In2 O3 and (Sn0.065 In0.935 )2 O3 (one out of 16 indium atoms was replaced in the calculation) are compared [1397]. The fundamental band gap is slightly lowered, the high doping introduces a gigantic BursteinMoss shift. Additionally another band gap opens that splits the lowest conduction band. Also the conduction mechanism in amorphous oxides has been discussed [1398].
20.3 Properties
577
Fig. 20.3 The bixbyite crystal structure of indium oxide (In32 O48 ) showing one unit cell where the indium and oxygen atoms are represented by the full and empty circles, respectively. Adapted from [1396]
Fig. 20.4 Comparison of the band structure of In2 O3 (left) and (Sn0.065 In0.935 )2 O3 (right). The position of the Fermi level is for both cases at E = 0. Adapted from [1397]
20.3 Properties The best conductivity of TCOs is in the range of 10−4 cm for the specific resistivity. Such value is about three orders of magnitude smaller than that of metals. However, the TCO meanwhile is highly transparent in the visible region, while metals become transparent only in the UV region because of their high plasma frequency (cf. Sect. 9.8.1). The conduction mechanism in ZnO:Al is band transport in a highly doped semiconductor. The carrier concentration is typically around 1021 cm−3 . One of the best results is a (Hall) mobility of 47.6 cm2 /Vs, leading to a specific resistivity of 8.5 × 10−5 cm [1399]. The mobility is limited by (doping level dependent) ionized impurity scattering (Sect. 8.3.3) as shown in Fig. 20.5 for various films. A detailed discussion of ionized impurity scattering in doped ZnO films can be found in [1400].
578
20 Transparent Conductive Oxide Semiconductors
Fig. 20.5 Hall mobility for various ZnO:Al TCO thin films as a function of carrier (electron) concentration. The dashed line is the Brooks–Hering theory of ionized impurity scattering (taking into account nonparabolicity of the conduction band). The dashdotted line is mobility in the presence of grain boundaries, the solid line is combined theory. Symbols are experimental data from two sets of samples. Adapted from [1390]
Also the mobility is correlated (Fig. 20.6) with scattering at structural defects such as grain boundaries [1401] (cf. Fig. 8.5). We note that the carrier mobility in a (polycrystalline) TCO is not very different from that in highly doped (crystalline) silicon (Fig. 8.7). Conductivity and transparency are, however, linked. The high doping of the TCO leads to shifts in the band gap (renormalization and BursteinMoss shift), band tails and the like that can introduce absorption in the visible spectral region. Also the infrared transparency is related to the conductivity by free carrier absorption and the plasma edge (Sect. 9.8.1). With increasing carrier density, the plasma edge shifts into the visible spectral range (Fig. 20.7a), limiting the possible maximum carrier density to several 1021 cm−3 , the exact value depending on the carrier mass. In Fig. 20.7b the transparency spectra of two SnO2 films with different conductivity are compared. The higher conductivity due to larger carrier concentration leads to reduced IR
Fig. 20.6 Hall mobility of ZnO:Al films (of varying thickness) versus the crystallite size. Experimental data (from [1390]) are shown as symbols. The dashed line is a guide to the eyes
20.3 Properties
(a)
579
(b)
Fig. 20.7 (a) Absorption coefficient of ntype ZnO for various electron concentrations as labeled. Spectra synthesized from ellipsometric data of thin films. The visible spectral range is indicated. The contributing absorption processes are bandband transitions (BB), free carrier absorption (FC) and phononrelated absorption (Ph) as labeled. (b) Transparency versus wavelength spectra of two SnO2 films with different conductivity as labeled. Adapted from [1402]
transparency. Generally, the transmission of a TCO is limited by the band edge on the high energy side of the spectrum and the plasma edge on the low energy side of the spectrum. The limited carrier concentration due to the onset of free carrier absorption in the visible spectral range (∼3 × 1021 cm−3 ) and the limited mobility in the presence of such high impurity concentration (max. 50 cm2 /Vs) restrict the minimum resistivity of a TCO (or any transparent conductor) to about 4 × 10−5 cm [1403].
Part III
Applications
Chapter 21
Diodes
Abstract A thorough treatment of Schottky (metal–semiconductor) diodes, MIS (metal–insulator–semiconductor) diodes and (bipolar) pndiodes is given, focussing on suitable materials, the formation of space charge layers and the forward and reverse current–voltage characteristics. Applications of such devices based on their rectifying properties are discussed.
21.1 Introduction One of the simplest1 semiconductor devices is the diode. It is a socalled twoterminal device, i.e. a device with two leads. The most prominent property of a diode is the rectifying current–voltage (I–V ) characteristic. This function was initially realized with vacuum tubes (Fig. 21.1); a heated filament emits electrons that are transferred through vacuum to the anode if it is on a positive potential. The semiconductor diode technology led to a tremendous miniaturization, integration with other devices (in planar technology) and cost reduction. We distinguish2 unipolar diodes, for which the majority carriers cause the effects (e.g. metal–semiconductor diodes), and bipolar diodes in which minority carriers play the decisive role, e.g. in the pnjunction diode.
21.2 Metal–Semiconductor Contacts The metal–semiconductor contact was investigated in 1874 by F. Braun (see Sect. 1.1). For metal sulfides, e.g. CuFeS2 , he found nonohmic behavior. We remark here that we treat first metal–semiconductor contacts with rectifying properties. Later it becomes understandable that metal–semiconductor contacts can also be used as 1 The simplest device is a resistor made from a homogeneous piece of semiconductor, used, e.g., as a part of an integrated circuit or as a photoresistor as discussed in Sect. 22.2. 2 This distinction is not only made for diodes but also many other semiconductor devices such as transistors, see Chap. 24.
© Springer International Publishing Switzerland 2016 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, DOI 10.1007/9783319238807_21
583
584
21 Diodes
Fig. 21.1 (a) Schematic image of a vacuum diode. The electron current flows from the heated cathode to the anode when the latter is at a positive potential. (b) One of John A. Fleming’s first diode ‘valves’, 1904. (c) Commercial ‘tungar’ rectifier, around 1916 [1405]. (b, c) adapted from [1404]
ohmic contacts, i.e. contacts with a very small contact resistance. Rectifying metal– semiconductor contacts are also called Schottky diodes. A very important variation are metal–insulator–semiconductor diodes for which an insulator, mostly an oxide, is sandwiched between the metal and the semiconductor. Such diodes are treated in Sect. 21.3. Reviews on Schottky diodes can be found in [1406–1412].
21.2.1 Band Diagram in Equilibrium The metal and the semiconductor have generally different positions of the Fermi levels relative to the vacuum level. When the metal is in contact with the semiconductor, charges will flow in such a way that in thermodynamic equilibrium the Fermi level is constant throughout the structure.3 In the following we treat two limiting cases: The contact of a metal with a semiconductor without any surface states (Schottky–Mott model) and a contact where the semiconductor has a very high density of surface states (Bardeen model). The position of the Fermi level in the metal is given by the work function Wm that is shown in Fig. 21.2 for various metals (see also Table 21.1). A recent review of published values of metal work functions is given in [1413]. The work function reflects the atomic shell structure; minima of the work function exist for groupI elements. The work function is the energy difference between the vacuum level (an electron is at rest in an infinite distance from the metal surface) and the metal Fermi level (Wm > 0). Since the electron density in the metal conduction band is very high, 3 This
situation is similar to the heterostructure interface (Sect. 12.3.4), with the metal, however, having a very short screening length.
21.2 Metal–Semiconductor Contacts
585
7 Se
6
B
4 3
Cr Ge V Fe Ga Ti Sc Mn Cu Zn Be Mg Ca Al Si
Pd Ru Nb
Ag Te Sn
Rb Mo Sb Zr Cd In Y
Sr
Li
2
Pt
Co Ni As
C
5
K
Rb
Re
Au Hg W Bi Ir Ta Os Hf La Pb Tl Nd Gd
Tb Ce Ba Eu Sm Cs
Lu
U Th
1 0
0
10
20
30
40
50
60
70
80
90
Fig. 21.2 Work function Wm of various metals Table 21.1 Values of the work function Wm of various metals Z Element Wm (eV) Z Element Wm (eV) Z 3 4 5 6 12 13 14 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34
Li Be B C Mg Al Si K Ca Sc Ti V Cr Mn Fe Co Ni Cu Zn Ga Ge As Se
2.4 3.4 4.5 4.8 3.66 4.2 4.2 2.2 2.87 3.5 4.1 4.3 4.4 3.89 4.4 5.0 4.9 4.5 4.3 4.2 4.8 5.1 5.9
37 38 39 40 41 42 44 45 46 47 48 49 50 51 52 55 56 57 58 59 60 62 63
Rb Sr Y Zr Nb Mo Ru Rh Pd Ag Cd In Sn Sb Te Cs Ba La Ce Pr Nd Sm Eu
2.1 2.59 3.1 3.8 4.3 4.2 4.71 4.6 5.0 4.7 4.0 4.12 4.3 4.1 4.8 2.14 2.5 3.5 2.9 – 3.2 2.7 2.5
64 65 66 67 68 69 70 71 72 73 74 75 76 77 78 79 80 81 82 83 90 92
Element
Wm (eV)
Gd Tb Dy Ho Er Tm Yb Lu Hf Ta W Re Os Ir Pt Au Hg Tl Pb Bi Th U
3.1 3.0 – – – – – 3.3 3.9 4.1 4.55 5.0 4.8 4.6 5.3 4.8 4.49 3.8 4.0 4.4 3.5 3.6
586
21 Diodes
the position of the metal Fermi level does not change considerably when charge is exchanged between the metal and the semiconductor. Since in a semiconductor the Fermi level depends strongly on the doping and temperature it is not useful to characterize the material itself. For semiconductors the electron affinity χsc = Evac − EC > 0 is defined as the energy difference between the vacuum level and the conductionband edge (see Fig. 12.2). Ideal Band Structure When the metal and the semiconductor are not in contact (Fig. 21.3a), the metal is characterized by its work function Wm = Evac − EF and the semiconductor by its electron affinity χsc . First, we assume that Wm > χsc . For an ntype semiconductor, the energy difference between the Fermi level and the conduction band is denoted as − e Vn = EC − EF
(21.1)
being negative, Vn < 0, for nondegenerate semiconductors. Thus, the position of the semiconductor Fermi level is given as EF = Evac − χsc + e Vn .
(21.2)
If the metal and semiconductor are brought into contact the Fermi levels will equilibrate. For the case of Fig. 21.3 (EF,sc > EF,m ) electrons will flow from the semiconductor to the metal. The negative surface charge of the metal is compensated by a positive charge (due to D+ ) in the semiconductor in the vicinity of the surface. Eventually a (Schottky) barrier of height4 FBn FBn = Wm − χsc
(21.3)
forms at the interface. The subscript ‘n’ stands for the contact on an ntype semiconductor. Surface/interface effects such as nonmatching bonds, surface states, etc. are neglected at this point. In the semiconductor there exists a positively charged region that is called the depletion layer or spacecharge region [1414]. Its extension (w in Fig. 21.3b) and properties will be discussed in Sect. 21.2.2. The space charge region in the metal is very thin due to the small screening length. For a contact on a ptype semiconductor the barrier FBp (to the valence band) is (see Fig. 21.4d) (21.4) FBp = Eg − (Wm − χsc ). Between the surface of the metal and the bulk part of the semiconductor there is a potential drop FBn Wm − χsc Vbi = (21.5) + Vn = + Vn , e e
4 We
denote the energy barrier height with FB = −eφB .
21.2 Metal–Semiconductor Contacts
587
(a)
(b)
Fig. 21.3 Schematic band structure of a metal–semiconductor junction that is dominated by bulk properties of the semiconductor. (a) no contact, (b) metal and semiconductor in contact. w denotes the width of the depletion layer. Outside the depletion layer the semiconductor is neutral. FB,n denotes the Schottky barrier height, Vbi denotes the builtin voltage (here Vbi > 0)
which is termed the builtin potential (or diffusion voltage). The exact form of the voltage drop, the socalled band bending, will be discussed in Sect. 21.2.2. The surface index is defined as S=
∂FBn . ∂Wm
(21.6)
From the present consideration (21.3), the same semiconductor with metals of varying work function should result in S = 1. Band Structure in the Presence of Surface States Experimental data shown in Fig. 21.5a, however, show a different behavior with smaller slope. For GaAs, e.g., the barrier height is almost independent of the metal work function. Thus, a different model is needed for realistic Schottky diodes. A rule of thumb for the dominantly covalent semiconductors is that for ntype material the barrier height is 2/3 of the band gap and for ptype material 1/3 of the band gap, such that EC − EF ≈ 2Eg /3 (Fig. 21.5b). Only for ionic semiconductors S ≈ 1 holds (Fig. 21.5c) [1419]. If the semiconductor has a large density of states at its surface (1012 cm−2 ), there is a spacecharge region already without the metal [1420]. Surface traps are filled up to the Fermi level (Fig. 21.6a). The size of the band bending in the semiconductor will be denoted as FBn since it will turn out below as the Schottky barrier height. If the density of surface states is very high, the charge carriers moving from the semiconductor into the metal upon contact formation are accommodated in the surface states and the position of the Fermi level at the semiconductor surface changes only very little. Thus, the spacecharge region is not modified and it is identical to the surface depletion region. The Schottky barrier height is then given by the band bending at the (bare) semiconductor surface FBn (Fig. 21.6d) and does not depend on the metal work
588
21 Diodes
(a)
(d)
(b)
(e)
(c)
(f)
Fig. 21.4 Band structures of metal–semiconductor junctions for (a–c) an ntype semiconductor and (d–f) a ptype semiconductor (here FBp > 0). (b, e) in thermodynamic equilibrium, (a, d) with forward bias (V > 0), (c, f) with reverse bias (V < 0)
function at all (Bardeen model [1420]). For this limiting case we find for the surface index S = 0. For actual metal–semiconductor contacts the surface index S takes values between 0 and 1. A theory involving the semiconductor band structure and midgap (surface) states (MIGS) is needed [617, 1421]. For Si, the experimental result is S = 0.27; the corresponding density of surface states is Ds = 4 × 1013 cm−2 eV−1 .
21.2 Metal–Semiconductor Contacts
589
(a)
(b) 10
S=1 1.5
BN C
ECE F (meV)
S=0
FBn (eV)
GaP 1.0
GaAs
0.5
GaAs Si GaSb Ge
Ge
CdS
Si
1.0
SiC GaP AlAs BP AlSb
InP
InSb
0
3.0
4.0
5.0
W m (eV)
0.1 0.1
1.0
10
E g (meV)
(c)
Fig. 21.5 (a) Experimental Schottky barrier heights FBn versus metal work function Wm for various metal–semiconductor junctions as labeled. Dashed lines are guides to the eye, dashdotted lines indicate dependencies for S = 1 and S = 0. Data from [1415, 1416]. (b) EC − EF at the metal– semiconductor interface versus the band gap Eg for Au Schottky contacts on various semiconductors. The dashed line represents EC − EF = 2Eg /3. Data from [1417]. (c) Surface index S versus the electronegativity difference ΔX between the species of compound semiconductors. Dashed line is a guide to the eye. Data from [1416, 1418]
21.2.2 SpaceCharge Region The width w of the spacecharge region is calculated next. First, we make the socalled abrupt approximation. In this approximation (Schottky–Mott model), the charge density ρ in the spacecharge region (0 ≤ x ≤ w) is given by the doping, i.e. ρ = +eND . Outside the spacecharge region the semiconductor is neutral, i.e. ρ = 0 and the electric field is zero, i.e. dϕ/dx = 0. As further boundary conditions the potential at the interface is ϕ(0) = −Vbi < 0. The potential drop in the spacecharge region is determined by the onedimensional Poisson equation
590
21 Diodes
(a)
(b)
Fig. 21.6 Schematic band structure of a metal–semiconductor junction that is dominated by surface properties of the semiconductor. (a) No contact; due to pinning of the Fermi level at surface states of the semiconductor, a depletionlayer of width w is already present. (b) Metal and semiconductor in contact
d2 ϕ ρ =− , 2 dx s
(21.7)
where s = r 0 is the static dielectric constant of the semiconductor. Using the ansatz ϕ(x) = ϕ0 + ϕ1 x + ϕ2 x 2 we find ϕ(x) = −Vbi +
e ND s
w0 x −
1 2 x , 2
(21.8)
w0 being the depletion layer width at zero bias. The spatial dependence E(x) of the electric field strength is E(x) = −
e ND e ND (w0 − x) = Em + x, s s
(21.9)
with the maximum field strength Em = −eND w0 /s at x = 0. From the condition ϕ(w0 ) = 0 we obtain w0 as 2 s w0 = Vbi . (21.10) eND The charge density and the potential in the abrupt approximation are shown in Fig. 21.7 for GaAs material parameters. Beyond the abrupt approximation, the thermal distribution of the majority carriers must be treated with more care. The dependence of the charge density ρ = e(ND+ − n) on the potential ϕ (within the Boltzmann approximation) is (β = e/kT ) ρ = e ND 1 − exp (β ϕ) .
(21.11)
21.2 Metal–Semiconductor Contacts
591
(a)
(b)
Fig. 21.7 (a) Potential ϕ and (b) charge density ρ across the depletion layer of a Schottky nGaAs diode. Calculation parameters are s = 12.5 0 , Vbi − Vext = 2 V (small reverse bias), ND = 1 × 1016 cm−3 , T = 300 K. Abrupt approximation is shown as solid lines, exact (numerical) calculation as dashdotted line. Dashed line in (a) indicates depletion layer width w0 in the abrupt approximation
The actual charge density and the potential, obtained from a numerical solution of (21.7), are shown in Fig. 21.7 in comparison with the abrupt approximation. Clearly, at the Schottky depletion layer width w0 , the charge varies continuously and the potential does not drop to zero. We note that for the depletion layer ϕ ≤ 0 and n ≤ ND . The charge difference Δρ (due to the tail of the thermal distribution of the majority charge carriers in the depletion layer) between the real distribution (21.11) to the abrupt approximation model with constant charge density (ρ0 = eND ) in the depletion layer is Δρ(x) = ρ(x) − ρ0 = −e ND exp (β ϕ(x)) .
(21.12)
The integration of Δρ over the depletion layer yields that the voltage drop Vbi across the depletion layer needs to be corrected by ΔV Δϕ = 0
w0
x 0
−Δρ(x ) 1 dx dx = 1 − exp(−β Vbi ) ≈ β −1 . s β
(21.13)
The approximation is valid for βVbi 1. Therefore, (21.10) is corrected to w0 =
2 s
Vbi − β −1 . e ND
(21.14)
When a potential difference Vext is applied externally to the diode, (21.14) is modified by the change in the interface boundary condition, ϕ(0) = −Vbi + Vext . The band structure is shown schematically in Fig. 21.4a for a forward bias and in Fig. 21.4c for a reverse bias. Therefore, we obtain for the depletionlayer width
592
21 Diodes
(within the abrupt approximation) w(Vext ) =
2 s
Vbi − Vext − β −1 . e ND
(21.15)
Now we can also give explicitly the value of the maximum electric field Em (at x = 0)
2 e ND
Vbi − Vext − β −1 s 2
=− Vbi − Vext − β −1 . w
Em = −
(21.16)
We note that so far the barrier height is independent of the applied bias voltage. In the next section, it is shown that this is actually not the case. An alternative approach to solve the Poisson equation is to consider the field as a function of the potential, E(φ). Then,
and
dE dE 2 = 2E , dφ dφ
(21.17)
dE dE dx dE 1 d2 φ 1 = =− =− 2 . dφ dx dφ dx E dx E
(21.18)
Combining these two equations and using (21.7) and (21.11) we find dE 2 2 e ND (1 − exp(β φ)). =− dφ s
(21.19)
The integration of this equation yields with the boundary condition E(φ = 0) = 0, 2 e ND E (φ) = − s 2
1 exp(β φ) + φ− β β
.
(21.20)
At the interface φ(x = 0) = −(Vbi − V ), and for sufficient voltage drop in the semiconductor exp β φ 1, and therefore (21.16) for Em is recovered without using the abrupt approximation or its correction (21.13).5 Without approximation,
5 The functional integration method is limited to bijective potentials φ(x), i.e. strictly monotonously falling or rising potentials [1422] and thus covers monotonously varying doping density within the depletion layer.
21.2 Metal–Semiconductor Contacts
Em = −
2 e ND s
593
Vbi − Vext −
1 1 − exp(−β(Vbi − Vext )) . β
(21.21)
21.2.3 Schottky Effect The barrier height is reduced by the imagecharge effect that has been neglected so far. This effect has been worked out for metals by Schottky [1423] and has been adapted to semiconductors [1424, 1425]. An electron (charge q = −e) at position x in the semiconductor is facing a metal surface. The metal surface is at zero position (Fig. 21.8a). The potential distribution of the free charge is modified since the metal surface is an equipotential surface. The potential distribution outside the metal is identical to that if an image charge −q were located at −x. This image charge exerts a force (image force Fif ) on the electron Fif = −
q2 , 16 π s x 2
(21.22)
where s is the relative dielectric constant of the semiconductor. In order to bring an electron to x from infinity the work Eif Eif =
(a)
x
∞
Fif dx = −
q2 16 π s x
(21.23)
(b)
xm 1 if
FB0
FB
V=Vbi /2
B0
eVbi FBn
0
V=0
1
V=Vbi
EC EF
EF w
0
1
2 0
)
Fig. 21.8 (a) Energy of a particle with respect to the metal surface (dashed line), conduction band in semiconductor depletion layer (dashdotted line) and combined effect (solid line). The image charge energy lowers the potential barrier FB0 by the amount ΔFBif to FBn . (b) Conduction band on the semiconductor side of a metal–semiconductor junction at various bias voltages (V = 0, +Vbi /2, and −Vbi as labeled) taking into account the Schottky effect. The width of the depletion layer is indicated with a short vertical dashed line. The barrier height without Schottky effect is FB0 . The dashed line is the situation without Schottky effect for zero bias
594
21 Diodes
is needed. This image potential energy is shown in Fig. 21.8a. The total energy Etot (solid line in Fig. 21.8a) of the electron in the presence of an electric field E is given by Etot = q E x −
q2 . 16 π s x
(21.24)
We note that the divergence at x = 0 stems from the continuum idealization of the problem. It can be removed by shifting the position of the image charge slightly against the interface or by using an extended charge [1050]. The maximum of this function (dEtot /dx = 0) is at xm xm =
e . 16 π s E
(21.25)
The energy barrier (21.3) (without image charge effect now labeled as FB0 ) is reduced by ΔFB given by eE = 2 e E xm . 4π s
ΔFBif = e
(21.26)
With the field in the vicinity of the interface given by Em from (21.16), the barrier reduction is6 3 1/4 e ND
−1 ΔFBif = e V − V − β . (21.27) bi ext 8 π 2 3s For s = 0 (vacuum) and a field strength of 105 V/cm the maximum position is at xm = 6 nm and the barrier reduction is ΔFBif = 0.12 eV. For 107 V/cm, xm = 1 nm and ΔFBif = 1.2 eV. For semiconductors with r ∼ 10 the effect is smaller (Fig. 21.9). The Schottky effect depends on the bias voltage as visualized in Fig. 21.8b and therefore the barrier height depends on the applied bias voltage.
21.2.4 Capacitance The total space charge Q (per unit area) in the semiconductor is (V = Vext ) Q(V ) = e ND w =
2 e ND s Vbi − V − β −1 .
(21.28)
and depends on the external voltage. term 3s is technically s 2d where d is the imageforce dielectric constant. d is equal to s if the transit time of an electron from the metal to the maximum of the potential energy is sufficiently long to build up the dielectric polarization of the semiconductor [1406].
6 The
21.2 Metal–Semiconductor Contacts
595
Fig. 21.9 Electricfield dependence of the image charge lowering of the Schottky barrier. Dashdotted line is for vacuum dielectric constant, dashed line is (21.26) for r = 12. Adapted from [1426]
For measurement of the depletion layer capacitance first the external dc bias voltage V is set which defines the extension of the depletion layer. The (differential) capacitance is probed by an ac voltage with small amplitude δV V . First we assume that the ac frequency ω is small compared to characteristic time constants of the electrically active impurities (quasistatic capacitance) and discuss the bias dependence C(V ). Following we discuss the frequency and temperature dependence of the capacitance7 C(ω, T ), in particular when the measurement frequency is in the range of the (temperature dependent) electron capture or emission rate (10.42, 10.43). Bias Dependence From (21.28) the capacitance C = dQ/dV  (per unit area) of the space charge region is given by e ND s s = .
(21.29) C= w 2 Vbi − V − β −1 Equation (21.29) can also be written as
2 Vbi − V − β −1 1 = . C2 e ND s
(21.30)
If 1/C 2 is measured as a function of the bias voltage (C–V spectroscopy), it should be linearly dependent on the bias voltage if the doping concentration is homogeneous (Fig. 21.10a). The doping concentration can be determined from the slope via ND = −
7 Probing
2 e s
d dV
1 C2
−1
,
(21.31)
the capacitance as a function of the ac frequency is called admittance spectroscopy.
596
21 Diodes
(a)
(b)
Fig. 21.10 (a) Capacitance C (dashed line) and 1/C 2 (solid line) versus bias voltage dependence for an Au/GaAs Schottky diode (2µm MOVPEgrown GaAs:Si on a nGaAs substrate) at room temperature. From the extrapolation to 1/C 2 = 0 and (21.30) we obtain Vbi = 804 ±3 mV. (b) Donor concentration (ND = 4.8 × 1016 cm−3 ) determined via (21.31) from the 1/C 2 plot versus the depletion layer width (calculated using (21.29))
(see Fig. 21.10b) and the builtin voltage Vbi from the extrapolation to V = V such that 1/C 2 = 0, Vbi = V + kT /e. Using (21.5) the Schottky barrier height can be determined from this [1427] via FBn = e V − e Vn + kT − ΔFBif ,
(21.32)
where ΔFBif is the barrier lowering (21.27) due to the image force effect between the flatband and the zerobias cases. We note that for inhomogeneous doping the depth profile of the doping can be determined by C–V spectroscopy. The 1/C 2 versus bias curve is then no longer a straight line and exhibits a varying slope. ND (w) is evaluated according to (21.31) using w = s /C from (21.29) [1428], 2 s =− w= C e s
ND
d dV
1 C2
−1
,
(21.33)
Using functional integration, the capacitance of a depletion layer can be expressed in terms of ϕ(0) = Vbi − V without explicit knowledge of the potential ϕ(x) [1422].8 In the approximation eϕ(0) kT we obtain for homogeneous doping as refinement of (21.29) e ND s , (21.34) C= 2 Vbi − V − β −1 Nn0D − ln Nn0D
8 This
is valid as long as ϕ(x) is strictly monotonous.
21.2 Metal–Semiconductor Contacts
597
where n0 is the electron concentration in the neutral region. Within this general treatment, the validity of (21.31) has been confirmed. Also, C does not diverge in the flatband case, for V → Vbi , as for the abrupt approximation but exhibits a maximum [1422]. At a given bias voltage, the charge (ionized donors or acceptors) at the boundary of the spacecharge region is tested by the capacitance measurement. However, this principle works only if the depth of the spacecharge region actually changes with the bias voltage. The method can therefore not be directly applied to such systems like δdoped layers or quantum wells. Frequency and Temperature Dependence The release of carriers from (and capture on) a donor occurs with a characteristic emission rate gc (10.43) (capture rate rc ). This is true similarly for acceptors. Therefore, the capacitance depends on the sampling frequency (Fig. 21.11a). If the capacitance is probed with a frequency much smaller than the release rate, the system appears to be in equilibrium and has the (quasi)static capacitance C0 . If the probe frequency is much higher, the system cannot follow and the donor does not contribute to the capacitance. The characteristic frequency fˆ at the turning point of C(f ) is [895] (21.35) 2π fˆ = 2 gc ,
(a)
(b)
Fig. 21.11 (a) Capacitance versus probing frequency f for a Pd/ZnO Schottky diode (zero bias) at T = 85 K. Theoretical dependence (solid line) and experimental data (circles). (b) Capacitance of the same diode as a function of temperature (thermal admittance spectroscopy, TAS) for four different probing frequencies f =10, 50, 100 and 316 kHz (ac amplitude 50 mV). Arrows denote the release of carriers from four different defect levels, two shallow ones and the wellknown defects E1 and E3 [655, 1432]. The inset shows the contribution of the E1 defect, indicated by a rectangle in the main graph, in more detail. Symbols are experimental data, lines are fit with fourlevel model (E1: ED = 116 meV, E3: ED = 330 meV) [1433]
598
21 Diodes
with corrections of the simple factor of 2 discussed in [1429]. Since the emission rate depends exponentially on temperature, for a given frequency the capacitance depends on temperature [1430]. This is shown in Fig. 21.11b for ZnO which exhibits several donor levels. At low temperature shallow levels release their carriers, at higher temperature the deeper levels start to contribute. The DX center in AlGaAs (see Sect. 7.7.6) has been investigated in [1431] with this technique.
21.2.5 Current–Voltage Characteristic The current transport through a metal–semiconductor junction is dominated by the majority charge carriers, i.e. electrons (holes) in the case of an ntype (ptype) semiconductor, respectively. In Fig. 21.12, the possible transport mechanisms are visualized for an ntype semiconductor. Thermionic emission ‘above’ the barrier involves the hot electrons from the thermal distribution and will be important at least at high temperatures. Tunneling ‘through’ the barrier will be important for thin barriers, i.e. at high doping −1/2 (w ∝ ND , cf. (21.15)). ‘Pure’ tunneling for electrons close to the (quasi) Fermi level, also called field emission, and thermionic field emission, i.e. tunneling of electrons with higher energies, are distinguished. Also, recombination in the depletion layer and hole injection from the metal are possible. The transport of electrons above the barrier can be described with diffusion theory [1434, 1435] or thermionicemission theory [1436]. A detailed treatment can be found in [1437, 1438]. In both cases the barrier height is large compared to kT . For thermionic emission (typically relevant for semiconductors with high mobility) the current is limited by the emission process and an equilibrium (constant electron quasiFermi level) is established throughout the depletion layer and ballistic transport is considered. In diffusion theory (for low mobility) a thermal equilibrium between metal and semiconductor electrons is established in the interface plane and the current is limited by diffusion and drift in the depletion region.
Fig. 21.12 Transport mechanisms at metal–semiconductor junctions. (1) Thermionic emission (‘above’ the barrier) (2) tunneling (‘through’ the barrier), (3) recombination in the depletion layer, (4) hole injection from metal
(1) (2) (3) (4) EF
eV
EC EF
EV
21.2 Metal–Semiconductor Contacts
599
Thermionic Emission The current density per unit area js→m of electrons that flow from the semiconductor into the metal is due to the hot electrons from the thermal distribution function ∞ js→m = (−e) vx dn. (21.36) EF +FBn
The integral starts at the lowest possible energy, the top of the Schottky barrier (no tunneling allowed in this model!). The electron density dn in a small energy interval dE is dn = D(E) f (E) dE. (21.37) For a bulk semiconductor density of states (6.67) and the Boltzmann distribution (FB kT ) 1 dn = 2π 2
2m∗ 2
3/2 E − EF E − EC exp − dE. kT
(21.38)
For a given energy E, the carrier velocity v is determined by E = EC + Thus we obtain
1 ∗ 2 m v . 2
(21.39)
E − EC = v m∗ /2
(21.40)
dE = m∗ v dv.
(21.41)
and
Also, with (21.39) and (21.1), 1 ∗ 2 m v − e Vn . 2
(21.42)
m∗ v 2 exp (βVn ) exp − 4π v 2 dv. 2 kT
(21.43)
E − EF = (E − EC ) + (EC − EF ) = Therefore we write (21.38) as dn = 2
m∗ h
3
Then the onedimensional integral over 4πv 2 dv is converted into a threefold integral over dvx dvy dvz . Integration over all velocities in y and z directions yields a factor 2π kT /m∗ . The integration over vx runs from the minimum velocity vmin,x necessary to pass the barrier,
600
21 Diodes
2 m∗ vmin,x m∗ vx2 kT exp − vx dvx = ∗ exp − , 2 kT m 2 kT vmin,x ∞
(21.44)
with the minimum velocity determined by 1 ∗ 2 m vmin,x = e (Vbi − V ). 2
(21.45)
Thus the current density is given as, using (21.5), 4πe m∗ k 2 2 T exp (−β(Vbi − Vn )) exp (βV ) h3 FBn ∗ 2 = A T exp − exp (βV ) , kT
js→m =
(21.46)
with A∗ being the Richardson constant given by A∗ =
4πe m∗ kB2 e NC v¯ = , 3 h 4T 2
(21.47)
where v¯ is the average thermal velocity in the semiconductor. A∗ for electrons in vacuum is 120 A cm−2 K−2 . A similar result is obtained for the thermionic emission of electrons from a metal (overcoming the work function) into vacuum. If the bias is changed, the current from the semiconductor to the metal increases in the forward direction because the energy difference between the quasiFermi level and the top of the barrier is reduced. The current is reduced for reverse bias. The barrier from the metal into the semiconductor remains constant (except for the Schottky effect whose impact on the current–voltage characteristic is discussed next). Therefore the current jm→s from the metal into the semiconductor is constant and can be obtained from the condition j = js→m + jm→s = 0 for zero bias. Therefore the current–voltage characteristic in the thermionicemission model is
FBn exp (βV ) − 1 j = A T exp − kT = js exp (βV ) − 1 . ∗
2
The prefactor
FBn js = A T exp − kT ∗
2
(21.48)
(21.49)
is called the saturation current density. The saturation current increases with increasing temperature. The dependence (21.48) represents the ideal diode characteristic and is plotted in Fig. 21.13.
21.2 Metal–Semiconductor Contacts
601
(a)
(b)
Fig. 21.13 Ideal diode I–V characteristics I = Is (exp(eV /kT ) − 1) (a) in linear plot and (b) semilogarithmic plot
The temperature dependence of the saturation current js can be written as
js ln T2
= ln A∗ −
FBn kT
(21.50)
by transforming (21.49). The plot of ln js /T 2 to versus 1/T is called a Richardson plot and allows the barrier height and the Richardson constant to be determined from a linear fit (Fig. 21.14b). Ideality Factor If the Schottky (image force) effect, i.e. the change of barrier height with bias voltage, is considered, the semilogarithmic slope of the forward I–V characteristic is no longer V0−1 = e/kT but can be expressed as V0−1 = e/nkT , n being a dimensionless parameter termed the ideality factor,9 j = js n is given by
eV exp n kT
−1 .
1 ∂FB 1 ∂FB −1 ≈1+ . n= 1− e ∂V e ∂V
(21.51)
(21.52)
The ideality factor due to the image force effect nif (using (21.27) and the image force barrier lowering ΔFBif,0 at zero bias) [1439] is
9 Obviously
n = 1 for the ideal characteristic (21.48). Otherwise n ≥ 1.
602
21 Diodes
(a)
(b)
1
2
2 s
2
2
n
AgOx /ZnO
s,f
FB
2
2
FBf
FBf
AgOx /ZnO
1000/T (K1)
Fig. 21.14 Temperature dependent behavior of an AgOx /ZnO Schottky diode. (a) I–V characteristics. Inset depicts extracted parameters, ideality factor n, barrier height FB and flatband barrier height FBf (21.54). (b) Richardson plots for the extracted barrier height and the calculated flatband barrier height with linear fit. Adapted from [1440]
nif = 1 +
ΔFBif,0 xm =1+ . 4 e Vbi w0
(21.53)
Typical values are smaller than 1.03. For GaAs and ND = 1017 cm−3 , n = 1.02. With regard to V0 and its temperature dependence, we refer also to Fig. 21.17 and the related discussion. In Fig. 21.14a the temperature dependence of the I–V characteristic of an almost ideal ZnO Schottky diode [1440] is depicted. The extracted barrier height is almost independent of temperature as it should be. Also the ideality factor is rather small (about 1.1) and also independent of temperature. The Richardson plot Fig. 21.14b according to (21.50) for this diode is a straight line. The extracted constant A∗ = (10 ± 6) A cm−2 K−2 is reasonably close to the theoretical value of 32 A cm−2 K−2 (using m∗ = 0.32). In order to gain a barrier height independent from nonidealities, in [1441] the flatband barrier height FBf is discussed which is calculated from the diode parameters via kT NC f ln FB = n FB − (n − 1) , (21.54) e ND assuming all donors are ionized (otherwise ND shall be replaced by the electron density n, not to be confused here with the ideality factor). Accordingly, the saturation current density (21.49) is rewritten as js,f
Ff = A T exp − B kT ∗
2
(21.55)
21.2 Metal–Semiconductor Contacts
603
Laterally Inhomogeneous Barrier The increase of the ideality factor due to a spatially inhomogeneous barrier height has been proposed early on [1439, 1442–1446]. The barrier height FBn (y, z) across the contact area is typically assumed to have a Gaussian probability distribution [1447] p(FBn ) with a mean value F¯ Bn and a standard deviation σF , It turns out that the barrier C responsible for the capacitance, and thus the diffusion voltage determined height FBn C = F¯ Bn . The barrier by C–V spectroscopy, is given by the spatial average, i.e. FBn j height FBn determining the current–voltage characteristics (cf. (21.48)) via FBn exp − p(FBn ) dFBn j = A∗ T 2 exp (βV ) − 1 kT j FBn ∗ 2 exp (βV ) − 1 = A T exp − kT is given by
σ2 j FBn = F¯ Bn − F . 2 kT
(21.56)
(21.57)
Thus, the barrier height determined from the current–voltage characteristic underestimates the spatial average of the barrier height.10 The Richardson plot (21.50) is now modified (and is nonlinear in 1/T ) to
js ln T2
= ln A∗ −
FBn σF2 . + kT 2 k2 T 2
(21.58)
In [1448] the barrier nonuniformity due to the random distribution and discreteness of impurity charges in the depletion region is evaluated. This mechanism, yielding increasing barrier inhomogeneity for larger doping, represent a fundamental limit to the ideality of a Schottky diode. If the distribution of barrier heights is discrete, at low voltages the current will first flow at certain spots with low barrier (‘hot spots’). This leads to kinks in the I–V characteristics as found for SiC [1449] or ZnO [1450] (Fig. 21.15). Temperature Dependence Figure 21.16a shows the temperaturedependent I–V characteristics of a Pd/ZnO Schottky diode. A straightforward evaluation according to (21.48) results in a barrier height of about 700 meV and a Richardson constant that is orders of magnitude smaller than the theoretical value of 32 A K−2 cm−2 (for me∗ = 0.27). A fit of the temperaturedependent data with (21.57), as shown in Fig. 21.16b, results in F¯ Bn = 1.1 eV, in agreement with the (temperatureindependent) value obtained from CV spectroscopy, and σF = 0.13 eV [1451]. 10 This
phenomenon is similar to the redshift of luminescence lines (Stokes shift) due to thermalization in the presence of disorder, see Sect. 12.4.
604
21 Diodes
(a) (b)
(c)
1µm
Fig. 21.15 (a) I–V characteristic of ZnO Schottky diode (solid line) with fits due to regions with three different barrier heights (dashed lines). (b) Thermography image at bias of 1 V. The white square marks the area where one hot spot was investigated in detail. (c) SEM image of FIB prepared cross section of a defect (Al2 O3 particle) causing the lowest barrier hot spots, inset plane view of such defect before preparation. Adapted from [1450]
The temperature dependence of the ideality factor n is given by [1452] n=
1 , 1 − ρ2 + ρ3 /(2kT )
(21.59)
where ρ2 (ρ3 ) is the (temperatureindependent) proportionality coefficient of the bias dependence of the mean barrier height (standard deviation), i.e. 1 e 1 ρ3 = e
ρ2 =
∂ F¯ Bn ∂V ∂ σF2 . ∂V
(21.60a) (21.60b)
The fit of 1/n − 1 versus 1/T in Fig. 21.16c yields ρ2 = −0.025 and ρ3 = −0.028 eV for the ZnO diodes under investigation. The forward I–V characteristic of an Au/GaAs Schottky diode reported in [1453, 1454] is shown in Fig. 21.17a at various temperatures. The current amplitude decreases with decreasing temperature due to the temperature dependence of the saturation current (21.48). Also, the slope V0−1 of the characteristic j = js exp(V /V0 ) varies with temperature. Looking at the temperature dependence of V0 , it is described as V0 = k(T + T0 )/e rather than with an ideality factor n in the form of V0 = nkT /e.
21.2 Metal–Semiconductor Contacts
605
(a) 10
T= 293K
3
Pd/ZnO
210K
10 5
103
10
7
105 106 107
10 8 10
T=293K
104
10 6
jd (Acm2)
jd (Acm2)
10 4
3
2
1
0
1
9
0.0
0.2
0.4
(b)
0.6
0.8
(c) 0.15 2.0
0.2 n
1.8
1/n1
0.25
1.6 1.4
0.3
1.2 200
0.35
250 T (K)
0.4 0.45 0.5 0.55 3.0
3.5
4.0
4.5
5.0
1/T (1000/K) Fig. 21.16 (a) Forward I–V characteristic of Pd/ZnO Schottky diodes for various temperatures. Diode temperatures are 210, 220, 230, 240, 250, 260, 270, and 293 K. The inset shows the current j density versus voltage for 293 K on a semilogarithmic scale. (b) Effective barrier height FBn versus the inverse temperature. The solid line is a linear fit according to (21.57) yielding the standard deviation σF = 0.13 eV and the mean barrier height F¯ Bn = 1.1 eV. (c) Plot of 1/n − 1 versus the inverse temperature. The solid line is a linear fit of the data yielding the voltage deformation coefficients ρ2 = −0.025 and ρ3 = −0.028 eV. The inset shows the experimentally determined n factors and the n factors calculated from (21.59) using the voltagedeformation coefficients obtained from the linear fit (dashed line). Adapted from [1451]
606
21 Diodes
(a)
(b) 40
Au/ GaAs V0 (meV)
30 0
k e
0
20
k V0= e T
10
0
0
10
20
30
Fig. 21.17 (a) Forward I–V characteristic of Au/GaAs diode for various temperatures. (b) Temperature dependence of the voltage V0 . The experimental data are fitted with T0 = 45 ± 8 K. Adapted from [1453]
In other words, the ideality factor follows a temperature dependence n = 1 + T0 /T . In view of (21.59), such behavior means for small T0 that n ≈ 1/(1 − T0 /T ) and thus ρ2 = 0 and ρ3 = 2kT0 . For T0 = 45 K, ρ3 is 0.008 eV, which is a fairly small value. Thus, the temperature behavior of the diode is due to the narrowing of the Gaussian distribution of barrier height with bias voltage [1447]. Correlation of Barrier Height and Ideality Factor In a set of similar diodes with varying magnitude of barrier inhomogeneities, it is found that the effective barrier height and the ideality factor correlate [1454]. The extrapolation to n = nif yields the limit of the barrier height for a homogeneous barrier (Fig. 21.18). For silicon, it is found that the surface orientation has a minor influence on the Schottky barrier height (Fig. 21.18b) for an unreconstructed surface. The presence of a reconstruction lowers the barrier height11 (Fig. 21.18a).
11 Reconstructions
are accompanied by redistributions of the valence charge with respect to the undisturbed bulk (Sect. 11.4). The subsequent extra interface dipoles alter the barrier heights of reconstructed interfaces [1455].
21.2 Metal–Semiconductor Contacts
607
(a)
(b)
Fig. 21.18 (a) Effective barrier height versus ideality factor for Ag/nSi Schottky diodes prepared on Si(111) surface with (7 × 7) reconstruction or unreconstructed (1 × 1) as labeled. The more ideal (1 × 1) surface exhibits the higher barrier. The dashed lines are linear fits. (b) Effective barrier height versus ideality factor for Au/nSi Schottky diodes prepared on HFdipped (1 × 1) unreconstructed (001) and (111) surfaces. The dashed lines are linear fits and extrapolation to n = nif . Both surface orientations exhibit the same extrapolated homogeneous barrier height. Based on data compiled in [1455]
Diffusion Theory In diffusion theory the current density is considered in the presence of a carrierdensity and electricfield gradient. In the Boltzmann approximation the electron current is given by (8.59a). In stationary equilibrium the current density is constant, i.e. independent of x. Assuming that the carrier density has its equilibrium values at x = 0 and x = w, we find after integration and using (21.8)
FBn j = −e μn NC Em exp − kT = js exp (βV ) − 1 .
exp (βV ) − 1
(21.61)
Therefore, also in this case the ideal diode characteristic is obtained, however, with a different saturation current. The ideality factor in diffusion theory is n = 1.06 (for FBn 15 kT ) [1409]. Combined Theory A combination of both theories [1456] considers both mechanisms to be in series. The current can then be expressed as j=
FBn eNC vr exp − exp (βV ) − 1 1 + vr /vD kT
(21.62a)
608
21 Diodes
= A∗∗ T 2 exp (βV ) − 1 = js exp (βV ) − 1 .
(21.62b)
Here vr = v/4 ¯ is a ‘recombination velocity’ [1457] at the top of the barrier according to j = vr (n − n0 ), n0 being the equilibrium electron density at the top of the barrier and v¯ is the average thermal velocity in the semiconductor. vD is an effective diffusion velocity describing the transport of electrons from the edge of the depletion layer (x = w) to the top of the barrier (x = xm ). It is defined as vD−1
=
w xm
−e FBn − EC (x) exp − dx. μn kT kT
(21.63)
In [1456] μn has been assumed to be independent of the electric field. This assumption is potentially not realistic. If vD vr , thermionic theory applies and we obtain (21.48). The case vr vD ∼ μn Em relates to diffusion theory and we recover (21.61). The constant A∗∗ in (21.62b) is called the effective Richardson constant. Its calculated dependence on the electric field is shown in Fig. 21.19 for Si. At room temperature for most Ge, Si and GaAs Schottky diodes the thermionic emission of majority carriers is the dominating process. The effect of lateral barrier height inhomogeneity in a diffusion model has been discussed in [1458]. Tunneling Current At high doping the width of the depletion layer becomes small and tunneling processes become more probable. Also at low temperatures, when thermionic emission is very small, tunneling processes can dominate the transport between metal and semiconductor. One process is tunneling of electrons close to the Fermi level of
140
Si
120
electrons
100 2
Fig. 21.19 Calculated effective Richardson constant A∗∗ as a function of the electric field for a metal–Si diode at T = 300 K for a (ntype or ptype) doping of 1016 cm−3 . Adapted from [1459]
80 60 40
holes 20 0 5
10
20
50
100
200
500
21.2 Metal–Semiconductor Contacts
609
the semiconductor. This process is called field emission (F) and is at least important for degenerate semiconductors at very low temperatures. If the temperature is raised, electrons are excited to higher energies where they encounter a thinner barrier. The tradeoff between thermal energy and barrier width selects an electron energy Em above the conductionband edge for which the current is largest. This process is known as thermionic field emission (TF). For very high temperatures enough carriers can overcome the barrier completely and we are back in the thermionic emission regime. The validity of the two regimes is shown in Fig. 21.20 for Au/GaAs Schottky diodes as a function of doping concentration (ntype) and temperature. In the fieldemission regime the forward current is given by [1409] j = js exp
eV E00
,
(21.64)
with the characteristic energy parameter E00 given by E00 The saturation current is
e = 2
ND . m∗ s
FBn js ∝ exp − E00
(21.65)
.
(21.66)
In Fig. 21.21, the forward characteristic of a highly doped Au/Si is shown. The experimental value of E00 = 29 meV agrees well with the theoretical expectation of E00 = 29.5 meV. In the reverse direction the I–V characteristic under field emission is given by [1409]
12 10
kT (meV)
Fig. 21.20 Calculated conditions for thermionic field (‘TF’), field (‘F’) and thermionic (‘TE’) emission in a Au/GaAs Schottky diode as a function of temperature and doping concentration. Adapted from [1409]
Au/GaAs
8
TE
6
TF
4 2 0 1015
F 1016
1017 3
ND (cm )
1018
610
21 Diodes
(a) 10
3
104 10
5
(b)
106 00
8
109 10
log10
10
j VbiV
107
Au/Si ND=8 1018 cm3
10
3
10
4
10
5
10
6
10
7
10
8
10
9
10
0
0.2
0.4
0
0.6
0.5
(VbiV)
1.0 1/2
(eV
1/2
1.5
)
Fig. 21.21 (a) Forward and (b) reverse I–V characteristic of a Au/Si Schottky diode at 77 K. The doping concentration of the Si was ND = 8 × 1018 cm−3 . Adapted from [1409]
3/2 4π e m∗ 2 e (Vbi − V ) 2 FBn . j= E00 exp − √ h3 FBn 3E00 e(Vbi − V )
(21.67)
From Fig. 21.21b, a barrier height of 0.79 eV is deduced. In the TFemission regime the current–voltage characteristic is given by
eV j = js exp E0 with
E00 E0 = E00 coth kT
,
(21.68)
,
(21.69)
where E00 is given by (21.65). The energy for maximum TF emission Em is given by Em = e(Vbi − V )/ cosh2 (E00 /kT ). The cothdependence of E0 is shown in Fig. 21.22 for an Au/GaAs diode. A Schottky diode can suffer from nonideality such as series and parallel ohmic resistance [1452]. These effects are discussed in some detail below for pndiodes in Sect. 21.4.4 and apply similarly to Schottky diodes.
21.2 Metal–Semiconductor Contacts
611
Fig. 21.22 Temperature dependence of E0 of an Au/GaAs diode with ND = 5 × 1017 cm−3 . The solid line is the theoretical dependence for thermionic emission according to (21.69) with ND = 6.5 × 1017 cm−3 and m∗ = 0.07. Adapted from [1409]
Au/GaAs 17 3 ND=5 10 cm
40
E 0 (meV)
30
20
E 00 10
0
0
10
20
30
40
kT (meV)
21.2.6 Ohmic Contacts Although an ohmic contact does not have a diode characteristic, it can be understood from the previous remarks. An ohmic contact will have a small contact resistance for both current directions. The voltage drop across the contact will be small compared to the voltage drop in the active layer (somewhere else). Details on electric contacts can be found in [1460]. The contact resistance Rc is defined as the differential resistance at V = 0 Rc =
∂I ∂V
−1 V =0
.
(21.70)
At low doping, the transport is dominated by thermionic emission (21.48). In this case Rc is given by k FBn Rc = exp . (21.71) e A∗ T kT A small barrier height (Fig. 21.23a) will lead to small contact resistance. A negative Schottky barrier height, i.e. Wm < Evac − EF for a ntype semiconductor, leads to an accumulation layer without a barrier for carrier transport (Fig. 21.23b). For high doping Rc is determined by the tunneling current (Fig. 21.23c) and is proportional to FBn . (21.72) Rc ∝ exp E00 The contact resistance decreases exponentially with the doping. A theoretical calculation and experimental data are compared in Fig. 21.24 for contacts on Si.
612
21 Diodes
(a)
(b)
(c)
Fig. 21.23 Schematic conditions for the formation of an Ohmic contact, (a) low barrier height, (b) accumulation layer (c) high doping (thin depletion layer)
10
10
4
cm2)
106
10
2
Rc (
Fig. 21.24 Theoretical and experimental values of specific contact resistances at T = 300 K for Al/nSi [1461] and PtSi/nSi [1462] contacts as a function of donor concentration. Solid lines are theoretical dependencies for different values of the barrier height as labeled. Adapted from [500]
10
0
20
ND (cm3)
19
1018
10
1017
Pt/Si Al/Si =0.85V
B
10
2
10
4
0.60V
0.40V
106 0
5
10
ND
(10 cm )
30
The three mechanisms, low barrier height, accumulation layer and high doping, for the formation of Ohmic contacts are summarized schematically in Fig. 21.23. Ohmic contacts on wide band gap semiconductors are difficult, since metals with sufficiently small (large) work function for contacting ntype (ptype) material are mostly not available. Although Schottky contact devices have their place in semiconductor technology, Ohmic contacts are indispensable for almost all devices.12 Ohmic contacts are typically prepared by evaporating a contact metal containing the doping material for the semiconductor, e.g. Au/Zn for a contact on ptype GaAs [1463] and Au/Ge for a contact [1464] on ntype GaAs. The contact is alloyed around 400–500 ◦ C (see Fig. 21.25) above the eutectic temperature of Teu = 360 ◦ C (for Au/Ge) to form a
12 Also
a Schottky diode has an Ohmic back contact.
21.2 Metal–Semiconductor Contacts
613
Fig. 21.25 Specific contact resistance for Ni/AuGe on ntype epitaxial GaAs for varying alloying temperatures (2 min). Arrow at Teu denotes the eutectic temperature of AuGe. Adapted from [1468]
eutectic liquid in which the dopant can quickly diffuse. When the eutectic liquid cools it forms a solid, a highly doped semiconductor layer underneath the metal. The liquidphase reactions can lead to inhomogeneous contacts. On ntype GaAs Pd/Ge/Au contacts have been reported to have superior structural quality [1465]. Ohmic contacts for a number of different semiconductors are reviewed in [1466, 1467].
21.2.7 Metal Contacts to Organic Semiconductors Also, for organic semiconductors the metal contact plays a vital role, either for carrier injection or for manipulation of the spacecharge region. The position of the Fermi level has been determined for various organic semiconductors as shown in Fig. 21.26. These data have been obtained from measurements on metal–semiconductor–metal structures (MSM, see also Sect. 22.3.5) as shown in Fig. 21.27a. The thin (50 nm) organic layer is fully depleted, thus the builtin field inside the semiconductor is constant. The builtin field is measured by applying an external dc bias and finding the external potential at which the electroabsorption signal vanishes. Figure 21.27b shows the measured electroabsorption signal ΔT /T (relative change of transmission T ) and the optical density of an MEHPPV film as a function of photon energy for an Al/MEHPPV/Al structure. The exciton absorption peak is found at 2.25 eV. The bias
614 Fig. 21.26 Measured Fermi energies EF (labeled data in eV) and the work functions Wm of various metals contacting (a) pentacene, (b) Alq3 and (c) MEHPPV. EC (EV ) denotes the energy position of the electron (hole) polaron. Measured data for EF for MEHPPV from [1470], other from [1471]. Data for Wm from Table 21.1
21 Diodes
(a) vacuum level Wm
Pentacene EC 2.4
EF
Ca 2.9
3.0 Ca
Al 4.3 Au 4.8 Pt 5.3
4.3 Al 4.8 Au,Pt
EV 4.9
(b) vacuum level Wm Sm Ca Mg Al Cu Au Pt
2.7 2.9 3.7 4.3 4.6 4.8 5.3
Alq3
EF
EC 3.0 3.6 4.0 4.6 5.2 5.6
Sm,Ca,Mg Al Cu Au Pt
EV 6.0
(c) vacuum level Wm Sm 2.7 Ca 2.9 Al,Ag Cu Au Pt
4.3 4.6 4.8 5.3
MEHPPV EC 2.90
EV 5.30
EF 3.0 Sm,Ca 4.3 4.6 5.1 5.2
Al,Ag Cu Au Pt
at which the builtin field vanishes can then be determined for various other metals in metal/MEHPPV/Al structures. Figure 21.26 summarizes such results for various metals and three organic semiconductors. The plot of the Fermi level position versus the metal work function (Fig. 21.27d, e) shows that the metals investigated do not introduce interface states in the singleparticle gap that pin the Schottky barrier (see Fig. 21.5 for inorganic semiconductors). An electron trap, such as C60 in MEHPPV, can pin the Fermi level of the ncontact metal and leads to a change of the builtin potential [1469].
21.3 Metal–Insulator–Semiconductor Diodes
615
(a) met
glass
(c)
(b) 2
CaAl
0.3
1
SmAl
0.2
0.5
3
0
AlAl
1 0.1
2 3 2.0
2.2
2.4
2.6
0.0
AuAl
0.0 2.0
1.0
0.0
1.0
2.0
(e)
(d)
0.0
0.0
E F (eV)
Ca Sm
1.0
E F (eV)
1.0
0.4

T/T (103)
3
Al
1.0 Cu
2.0
1.0
Al
Pt
Ag
Au
Au
1.0
0.0
1.0
3.0
2.0
W m (eV)
1.0
0.0
Wm (eV)
Fig. 21.27 (a) Schematic MSM structure with organic semiconductor (sc.) on transparent glass substrate. Metal 1 is thin and semitransparent. Thickness of organic semiconductor (polymer or small molecules) is about 50 nm. (b) Electroabsorption spectra of Al/MEHPPV/Al structure at four dc bias voltages (solid lines) and optical density spectrum (dashed line). (c) Magnitude of the electroabsorption response at 2.1 eV as a function of bias for metal/MEHPPV/Al structures. (d, e) Calculated (solid lines) and experimental (points) potential difference across (d) metal/MEHPPV/Al structures and (e) metal/MEHPPV/Ca structures as a function of the workfunction difference of the contacts. Parts (b)–(e) adapted from [1470]
21.3 Metal–Insulator–Semiconductor Diodes In a metal–insulator–semiconductor (MIS) diode an insulator is sandwiched between the metal and the semiconductor. Subsequently, a MIS contact has zero dc conductance. The semiconductor typically has an ohmic back contact. As insulator, often the oxide of the respective semiconductor, is used. In particular SiO2 on Si has been technologically advanced (Fig. 21.28). In the latter case, the diode is called a MOS (metal–oxide–semiconductor) diode. This structure has great importance for
616
21 Diodes
Fig. 21.28 Highresolution transmission electron microscopy image of a 1.6nm thick gate oxide between polySi (cf. Sect. 24.5.4) and crystalline Si. From [1472]
polySi
Si
the investigation of semiconductor surfaces and overwhelming importance for semiconductor technology (planar integration of electronic circuits, CMOS technology). Also, CCDs (Sect. 22.3.8) are based on MIS diodes.
21.3.1 Band Diagram for Ideal MIS Diode An ideal MIS diode has to fulfill the following three conditions: (i) (as shown in Fig. 21.29) without external bias the energy difference φms between the work function of the metal and the semiconductor Eg ± e ΨB (21.73) φms = Wm − χsc + 2
(a)
(b)
Fig. 21.29 Band diagram of an ideal MIS diode with (a) n and (b) ptype semiconductor at external bias V = 0. The insulator (‘i’) thickness is d as labeled. The dashdotted line represents the intrinsic Fermi level Ei
21.3 Metal–Insulator–Semiconductor Diodes
617
is zero (φms = 0). The ‘+’ (‘−’) sign in (21.73) applies to a ptype, Fig. 21.29b (ntype, Fig. 21.29a) semiconductor. ΨB is the potential difference between the intrinsic and actual Fermi level, ΨB = Ei − EF /e > 0. (ii) The only charges present are those in the semiconductor and the opposite charge is on the metal surface close to the insulator. (iii) There is no dc current between the metal and the semiconductor, i.e. the conductivity of the insulator is zero. The quantity ΨB (Fig. 21.31) is given as (for a ptype material, using (7.18), the high temperature approximation (7.30) and (7.15))
EC + EV NA kT NV + ln − EV − kT ln 2 2 NC NV Eg NA NA = + kT ln √ = kT ln . (21.74) 2 ni NC NV
e ΨB = Ei − EF =
When an ideal MIS diode is biased, three general cases—accumulation, depletion and inversion—can occur (Fig. 21.30). We discuss these first for the ptype semiconductor. Figure 21.30d shows the accumulation case for a negative voltage at the metal.13 Part of the voltage drops across the insulator, the rest across the semiconductor. The valence band is bent upwards towards the Fermi level. The quasiFermi level in the semiconductor, however, is constant since no dc current flows.14 Since the chargecarrier (hole) density depends exponentially on the energy separation EF − EV , a charge accumulation (of holes) occurs in the (ptype) semiconductor in the vicinity of the interface to the insulator. In Fig. 21.30e the depletion case is shown. Now a moderate reverse voltage, i.e. a positive bias to the metal, is applied. A depletion of majority charge carriers occurs in the semiconductor close to the insulator. The quasiFermi level in the semiconductor remains beneath the intrinsic level (Ei ≈ EC + Eg /2), i.e. the semiconductor remains ptype everywhere. If the voltage is increased further to large values, the quasiFermi level intersects the intrinsic level and lies above Ei close to the insulator (Fig. 21.30f). In this region, the electron concentration becomes larger than the hole concentration and we have the inversion case. The inversion is called ‘weak’ if the Fermi level is still close to Ei . The inversion is called ‘strong’ when the Fermi level lies close to the conductionband edge.
13 This
poling is a forward bias of the respective Schottky diode since the positive pole is at the ptype semiconductor. 14 We note that in order to reach the situations shown in Fig. 21.30 from the zero bias case of Fig. 21.29, a current must have flowed since charge carriers are redistributed. Figure 21.30 depicts the stationary equilibrium after transient voltage switchon effects have subsided. The time, however, that is needed in order to reach such stationary equilibrium from zero bias (thermal equilibrium) may be very long (e.g. days, cf. Sect. 22.3.8).
618
21 Diodes
(a)
(d)
(b)
(e)
(c)
(f)
Fig. 21.30 Band diagram of ideal MIS diodes with (a–c) ntype and (d–f) ptype semiconductors for V = 0 in stationary equilibrium for the cases (a, d) accumulation, (b, e) depletion and (c, f) inversion
21.3 Metal–Insulator–Semiconductor Diodes Fig. 21.31 Band diagram at the surface of a ptype semiconductor of a MIS diode. Accumulation occurs for Ψs < 0, depletion for Ψs > 0 and inversion (as shown here) for Ψs > ΨB > 0
619 insulator
semiconductor EC
e
S
e
B
Ei EF EV
The corresponding phenomena occur for ntype semiconductors for the opposite signs of the voltage with electron accumulation and depletion. In the inversion case, p > n close to the insulator (Fig. 21.30a–c).
21.3.2 SpaceCharge Region Now we calculate the charge and electric field distribution in an ideal MIS diode, following the treatment in [1473]. We introduce the potential Ψ that measures the separation of the intrinsic bulk Fermi level and the actual intrinsic level Ei , i.e. −eΨ (x) = Ei (x) − Ei (x → ∞) (see Fig. 21.31). Its value at the surface is termed Ψs , the surface potential. The value is positive, i.e. Ψs > 0, if the intrinsic Fermi level at the surface is below the bulk Fermi level. The electron and hole concentrations are given (for a ptype semiconductor) as np = np0 exp(βΨ ) pp = pp0 exp(−βΨ ),
(21.75a) (21.75b)
where np0 (pp0 ) are the bulk electron (hole) concentrations, respectively, and β = e/kT > 0. Therefore, the net free charge is given by np − pp = np0 exp(βΨ ) − pp0 exp(−βΨ ).
(21.76)
The electron and hole concentrations at the surface are denoted with an index ‘s’ and are given by15 ns = np0 exp(βΨs ) ps = pp0 exp(−βΨs ).
15 Ψ s
(21.77a) (21.77b)
represents the voltage drop across the semiconductor that will be discussed in more detail in Sect. 21.3.3. In this sense, Ψs for the MIS diode is related to Vbi − V for the Schottky contact.
620
21 Diodes
We use the Poisson equation
d2 Ψ dx 2
= − ρs with the charge given by
ρ(x) = e p(x) − n(x) + ND+ (x) − NA− (x) .
(21.78)
As boundary condition we employ that far away from the surface (for x → ∞) there is charge neutrality (cf. (7.41)), i.e. np0 − pp0 = ND+ − NA− ,
(21.79)
and that Ψ = 0. We note that ND+ − NA− must be constant throughout the completely ionized, homogeneous semiconductor. Therefore (21.79) (but not charge neutrality) holds everywhere in the semiconductor. Using (21.76) the Poisson equation reads e ∂2Ψ pp0 exp(−βΨ ) − 1 − np0 exp(βΨ ) − 1 . =− 2 ∂x s
(21.80)
The Poisson equation is integrated and with the notations
np exp(−βΨ ) + βΨ − 1 + 0 exp(βΨ ) − βΨ − 1 pp0 s kT s = , LD = e2 pp0 e β pp0
F(Ψ ) =
(21.81a) (21.81b)
with LD being the Debye length for holes, the electric field can be written as E=−
√ ∂Ψ 2 kT F(Ψ ). =± ∂x e LD
(21.82)
The positive (negative) sign is for Ψ > 0 (Ψ < 0), respectively. At the surface, Ψs will be taken as the value for Ψ . The total charge Qs per unit area creating the surface field √ 2 kT ∂Ψ =± F(Ψs ) (21.83) Es = − ∂x x=0 e LD is given by Gauss’s law as Qs = −s Es . The dependence of the spacecharge density from the surface potential16 is depicted in Fig. 21.32. When Ψs is negative, F is dominated by the first term in (21.81a) and the space charge is positive (accumulation) and proportional to Qs ∝ exp(βΨ /2). For Ψs = 0 the (ideal) MIS diode is under flatband condition and the space charge is zero. For Ψs > 0 the space charge is negative. For 0 < Ψs ≤ ΨB note that we discuss the spacecharge region now only with regard to Ψs , the voltage drop across the semiconductor, and the dependence of Ψs on the bias of the diode will be discussed in the next section.
16 We
21.3 Metal–Insulator–Semiconductor Diodes
621
Fig. 21.32 Dependence of the space charge on the surface potential Ψs for ptype silicon with NA = 4 × 1015 cm−3 at T = 300 K. The flatband condition is present for Ψs = 0, strong inversion for Ψs > 2 ΨB
the space charge is due to ionized√ impurities (depletion) and F is dominated by the second term in (21.81a), i.e. Ψs ∝√ Ψs . For ΨB ≤ Ψs ≤ 2 ΨB the diode is in the weak inversion regime and still Ψs ∝ Ψs . Eventually the dominating term of the second bracket in (21.81a) f1 = np0 /pp0 exp(βΨ ) = (ni /NA )2 exp(βΨ ) becomes comparable and exponentially larger than the dominating term of the first bracket f2 = βΨ . Solving f1 = f2 for Ψ = γ ΨB yields the equation (NA /ni )γ−2 = γ ln(NA /ni ) and a value γ larger than and close17 to 2. Thus for Ψs > Ψsinv ≈ 2 ΨB (using (21.74)), Ψsinv ≈
2 kT NA ln , e ni
(21.84)
strong inversion starts and the space charge is given as Qs ∝ − exp(βΨ/2). For the case of strong inversion the band diagram is shown in Fig. 21.33 together with the charge, field and potential. The total voltage drop V across the MIS diode is (21.85) V = Vi + Ψs , with Vi being the voltage drop across the insulator. In the case of inversion, the charge (per unit area) in the spacecharge region Qs = Qd + Qn 17 For
NA /ni = 104 , 106 and 108 , we find γ = 2.33, 2.25 and 2.20, respectively.
(21.86)
622 Fig. 21.33 Ideal MIS diode at inversion: (a) band diagram, (b) charge distribution, (c) electric field and (d) potential
21 Diodes
(a) metal insulator
semiconductor
Vi EC
e
e
S
B
Ei EF EV
V>0
inversion region
(b) Qm
depletion region
neutral region
(x)
0
w
d
x
eNA Qn
(c) Qm /
i
x d
(d)
0
w
(x) V Vi s
x d
0
w
is composed of the depletion charge (ionized acceptors) Qd = −e w NA ,
(21.87)
with w being the width of the depletion region, and the inversion charge Qn , which is present only close to the interface. The metal surface carries the opposite charge Qm = −Qs
(21.88)
due to global charge neutrality. The insulator itself does not contribute charges in the case of an ideal MIS diode.
21.3 Metal–Insulator–Semiconductor Diodes
623
21.3.3 Capacitance The insulator represents a capacitor with the dielectric constant i and a thickness d. Therefore, the capacitance is i (21.89) Ci = . d Between the charges −Qs and Qs the field strength Ei in the insulator is Ei =
Qs  . i
(21.90)
The voltage drop Vi across the insulator is given by Vi = Ei d =
Qs  . Ci
(21.91)
The total capacitance C of the MIS diode is given by the insulator capacitance in series with the capacitance Cd of the depletion layer C=
Ci Cd . Ci + Cd
(21.92)
The capacitance of the spacecharge region varies with the applied bias (Fig. 21.34). For forward bias (accumulation), the capacitance of the spacecharge region is high. Therefore, the total capacitance of the MIS diode is given by the insulator capacitance C ≈ Ci . When the voltage is reduced, the capacitance of the spacecharge region drops to Cd = s /LD for the flatband case (Ψs = 0). For a high reverse voltage, the semiconductor is inverted at the surface and the spacecharge region capacitance is high again. In this case, the total capacitance is given by C ≈ Ci again. The previous consideration assumes that the charge density in the semiconductor can follow changes of the bias sufficiently fast.18 The inversion charge must disappear via recombination that is limited by the recombination time constant τ . For frequencies around τ −1 or faster, the charge in the inversion layer cannot follow and the capacitance of the semiconductor is given by the value Cd ∼ = s /wm . wm (Fig. 21.35) is the maximum depletionlayer width present at the beginning of inversion (cf. (21.10) and (21.84)) wm ∼ =
18 Typically,
2 s inv Ψ = e NA s
4 s kT NA ln . e2 NA ni
(21.93)
a dc bias voltage V is set and the capacitance is sampled with a small ac voltage of amplitude ΔV , with δV V .
624
21 Diodes
(a)
(b) 10Hz
1.0
1.0
Ci
Ci
Ci
1.0
CFB
0.8
(i)
0.8
=
s
B
=2
s
Cmin Cmin '
0.4
C/C i
C/C i
capacitance
0.6
B
0.2
0.6
V
0
Vmin VT
Cmin '
0.2
(iii)
VT
breakdown
0
103Hz 104Hz 5 10 Hz
0.6
0.4
(ii)
102Hz
0.8
=0
s
0 4
+V
2
0
2
4
Fig. 21.34 (a) Schematic dependence of the capacitance of a MIS diode on the bias for (i) low frequencies, (ii) high frequencies and (iii) deep depletion. (b) Highfrequency capacitance of a Si/SiO2 diode. The inset shows the frequency dependence. Adapted from [1474] Fig. 21.35 Maximum width of the depletion layer wm (21.93) at room temperature for deep depletion for GaAs, Si and Ge diodes as a function of bulk doping level
10
1
wm (µm)
GaAs 10
0
10
1
10
2
10
Si Ge
14
10
15
10
16
10
17
10
18
N B (cm3)
For further increased voltage (into the inversion regime), the electric field is screened by the inversion charge and the width of the depletion layer remains constant. Therefore, the total capacitance in the inversion regime is given by C∼ =
i . d + wm i /s
(21.94)
21.3.4 Nonideal MIS Diode In a real, i.e. nonideal, MIS diode, the difference φms in the work functions of the metal and semiconductor (cf. (21.73)) is no longer zero. Therefore, the capacitance
21.3 Metal–Insulator–Semiconductor Diodes
625
versus voltage relation is shifted with respect to the ideal MIS diode characteristic by the flatband voltage shift VFB VFB = φms −
Qox . Ci
(21.95)
Additionally, the flatband voltage can be shifted by charges Qox in the oxide that have been neglected so far. Such charges can be trapped, i.e. fixed with regard to their spatial position, or mobile, e.g. ionic charges such as sodium. For Al as metal (φm = 4.1 eV) and ntype Si (φs = 4.35 eV), the flatband voltage shift is φms = −0.25 V, as shown schematically in Fig. 21.36a for zero bias. VFB is split into 0.2 eV and 0.05 eV for the oxide and the silicon, respectively. In Fig. 21.36b, the dependence of φms on the doping, conductivity type and metal is shown for various SiO2 –Si MIS diodes. An AuSiO2 –Si diode with ptype Si and NA ≈ 1015 cm−3 fulfills the condition of an ideal MIS diode with regard to φms = 0. Al
(a)
SiO2
nSi
(b)
Evac
0.2eV
1.0
EC
i
Au/nS
0.6
p + po
lySi/p
0.4
(V)
0.2 ms
0.05eV
4.1eV 3.2eV
5.25eV
0.8
EC EF
i/nSi
+ S p poly
Au/pS
i
0
Al/nSi
0.2
i/nSi
9.0eV
0.4
+ S n poly
0.6 0.8
EV
1.0
Si
Al/pSi n + po lySi/p
Si
14
10
15
10
16
10
17
10
18
10
NB (cm3)
Fig. 21.36 (a) Schematic band diagram of an Al–SiO2 –Si (ntype) diode with 50 nm oxide thickness and ND = 1016 cm−3 for zero bias. Based on data from [1475]. (b) Difference of work functions φms for SiO2 –Si MIS diodes and various doping levels and electrode materials (Al, Au and polycrystalline Si). The square represents the situation depicted in panel (a). Based on data from [1476]
626
21 Diodes
21.4 Bipolar Diodes A large class of diodes is based on pnjunctions. In a homo pnjunction an ndoped region is next to a pdoped region of the same semiconductor. Such a device is called bipolar. At the junction a depletion region forms. The transport properties are determined by the minority carriers. An important variation is the pindiode in which an intrinsic (or lowly doped) region is between the doped region (Sect. 21.5.8). If the differently doped regions belong to different semiconductor materials, the diode is a he